This book discusses the spectral properties of solid-state laser materials, including emission and absorption of light,

*309*
*76*
*10MB*

*English*
*Pages 486
[468]*
*Year 2020*

- Author / Uploaded
- Zundu Luo
- Yidong Huang

*Table of contents : PrefaceAbout This BookContentsAbout the Authors1 Energy Level of Free Ions 1.1 Energy Levels of the Single Electron in Atoms (Free Ions) 1.2 General Properties of Energy Level in Multi-electron of Free Ions 1.3 Energy Levels of Free Transition-Metal Ions 1.4 Energy Levels of Free Rare Earth Ions 1.5 Theory of Interactions in Rare Earth Ions References2 Group Theory and Quantum Theory 2.1 Mathematical Description of the Symmetry 2.2 Basic Conception of the Group 2.3 Theory of Group Representations 2.4 Direct Product Group and Direct Product Representation 2.5 Sketches of the Group in Spectroscopy 2.5.1 Finite Group 2.5.2 Permutation Group 2.5.3 Continuous Groups 2.6 Point Group and Their Representation 2.7 Symmetry and Quantum Theory of the Ions in Solids 2.8 Full Rotation Group and Angular Momentum Theory 2.9 Irreducible Tensor Operators and the Calculation of Matrix Elements References3 Rare Earth Ions in Materials 3.1 Crystal Field on the Active Ions 3.2 Energy Level Splitting of the Rare Earth Ions 3.3 Crystal Field Quantum Number 3.4 Group Chain Scheme Method in Crystal Field Analysis References4 Theory of Radiative Transition 4.1 Interactions Between Active Ions and Radiation 4.2 Probability of Emission and Absorption Processes 4.3 Selection Rules for Radiative Transition 4.3.1 Selection Rules for Radiative Transition of Free Ions and Atoms 4.3.2 Selection Rules for Radiative Transition of Ions in Materials References5 Spectroscopic Parameter and Their Calculation 5.1 Absorption Coefficient, Absorption (Emission) Cross-Section, and Oscillator Strength 5.2 Analysis of the Absorption Coefficients of Anisotropic Crystal 5.3 Judd–Ofelt Approximation and Related Parameter 5.4 Spectroscopic Parameter Calculation of Rare Earth Ion in Crystal 5.5 Hypersensitive Transitions References6 Phonon and Spectral Line 6.1 Quantization of Lattice Vibration—Phonon 6.2 Phonon Emission and Absorption in the Optical Transition 6.3 Main Mechanisms of the Thermal Spectral Line Broadening and Shifting 6.4 The Contribution of Single-Phonon Absorption (Emission) to the Spectral Linewidth 6.5 The Contribution of Phonon Raman Scattering to the Spectral Linewidth 6.6 Calculation of the Thermal Shifting of Spectral Lines 6.7 Examples for the Calculation of Thermal Spectral Line Broadening and Shifting References7 Energy Levels and Spectroscopic Properties of Transition Metal Ions 7.1 Energy Levels and Spectral Properties of 3d1 Electron System 7.2 Energy Levels and Spectral Properties of 3d2 Electron System 7.3 Energy Levels and Spectral Properties of 3d3 Electronic System 7.4 Relative Intensity Analysis of R Line in Ruby Polarized Absorption Spectrum 7.5 Estimation of Trivalent Chromium Ion Spectral Parameters in Solid-State Laser Materials References8 Non-radiative Transition Inside Ions 8.1 Introduction of Non-radiative Transition Matrix Elements 8.2 Promoting Mode and Accepting Mode in Non-radiative Transition Process 8.3 Non-radiative Transition Probability for Weak Coupling Systems 8.4 Parallelism Between Non-radiative Transition Probability and Radiative Transition Probability 8.5 Temperature Dependence of Non-radiative Transition Probability in Weak Coupling Systems 8.5.1 Experimental 8.6 Non-radiative Transition in Strong Coupling Systems 8.7 Nonlinear Theory of Non-radiative Transition 8.8 Stimulated Non-radiative Transition References9 Energy Transfer and Migration Between Ions 9.1 Theory of Resonant Energy Transfer 9.2 Phonon-Assisted Energy Transfer Between Ions 9.3 Statistical Theory of Energy Transfer Between Ions 9.4 Energy Migration Between Ions 9.5 Characteristics of Concentration Dependent Fluorescence Quenching for Self-activated Laser Crystals References10 Laser and Physical Properties of Materials 10.1 Brief Introduction of Solid-State Laser Principle 10.2 Quality Factor of Solid-State Laser Materials 10.3 Relationship Between Laser Threshold and Chemical Composition of Host Materials 10.4 Thermo-Mechanical and Thermo-Optical Properties of Solid-State Laser Materials 10.5 Laser Damage and Nonlinear Optical Properties References11 Nonlinear Optical Properties of Laser Crystals and Their Applications 11.1 Second-Order Nonlinear Optical Effect of Crystal 11.2 Relationship Between Fundamental and Second Harmonic Waves in SFD Laser Crystal 11.3 Nonlinear Optical Coupling Equation of SFD Laser 11.4 Self Sum-Frequency Mixing Effect in Nonlinear Laser Crystal 11.5 Stimulated Raman Scattering Effect of Laser Crystal References12 Apparent Crystal Field Model of Laser Glass and Its Application 12.1 Structure and Spectral Characteristics of Glasses 12.2 Apparent Crystal Field Hamiltonian for Rare Earth Ions in Non-crystal Host 12.3 Crystal Field Level Analysis for Er3+ Ions in Three Typical Glasses ReferencesAppendix A Character Tables for Point-Symmetry GroupAppendix B Correlation Table of Group–SubgroupAppendix C Multiplication Tables for Some Point GroupsAppendix D Squared Reduced-Matrix Elements of Unit Operator for J → J′ Transition in Rare Earth IonsAppendix E 3jm Factors for Some Group ChainsAppendix F Clebsch-Gordan Coefficients of the Cubic Point Group with Trigonal BasesAppendix G Integral Numerical Value Associated with the Thermal Effect of the SpectraIndex*

Springer Series in Materials Science 289

Zundu Luo Yidong Huang

Physics of SolidState Laser Materials

Springer Series in Materials Science Volume 289

Series Editors Robert Hull, Center for Materials, Devices, and Integrated Systems, Rensselaer Polytechnic Institute, Troy, NY, USA Chennupati Jagadish, Research School of Physical, Australian National University, Canberra, ACT, Australia Yoshiyuki Kawazoe, Center for Computational Materials, Tohoku University, Sendai, Japan Jamie Kruzic, School of Mechanical & Manufacturing Engineering, UNSW Sydney, Sydney, NSW, Australia Richard M. Osgood, Department of Electrical Engineering, Columbia University, New York, USA Jürgen Parisi, Universität Oldenburg, Oldenburg, Germany Udo W. Pohl, Institute of Solid State Physics, Technical University of Berlin, Berlin, Germany Tae-Yeon Seong, Department of Materials Science & Engineering, Korea University, Seoul, Korea (Republic of) Shin-ichi Uchida, Electronics and Manufacturing, National Institute of Advanced Industrial Science and Technology, Tsukuba, Ibaraki, Japan Zhiming M. Wang, Institute of Fundamental and Frontier Sciences - Electronic, University of Electronic Science and Technology of China, Chengdu, China

The Springer Series in Materials Science covers the complete spectrum of materials research and technology, including fundamental principles, physical properties, materials theory and design. Recognizing the increasing importance of materials science in future device technologies, the book titles in this series reflect the state-of-the-art in understanding and controlling the structure and properties of all important classes of materials.

More information about this series at http://www.springer.com/series/856

Zundu Luo Yidong Huang •

Physics of Solid-State Laser Materials

123

Zundu Luo Fujian Institute of Research on the Structure of Matter Chinese Academy of Sciences Fuzhou, Fujian, China

Yidong Huang Fujian Institute of Research on the Structure of Matter Chinese Academy of Sciences Fuzhou, Fujian, China

ISSN 0933-033X ISSN 2196-2812 (electronic) Springer Series in Materials Science ISBN 978-981-32-9667-1 ISBN 978-981-32-9668-8 (eBook) https://doi.org/10.1007/978-981-32-9668-8 Jointly published with Science Press The print edition is not for sale in China (Mainland). Customers from China (Mainland) please order the print book from: Science Press. ISBN of the Co-Publisher’s edition: 978-7-03-064678-1 © Science Press and Springer Nature Singapore Pte Ltd. 2020 This work is subject to copyright. All rights are reserved by the Publishers, whether the whole or part of the material is concerned, speciﬁcally the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microﬁlms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a speciﬁc statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. The publishers, the authors, and the editors are safe to assume that the advice and information in this book are believed to be true and accurate at the date of publication. Neither the publishers nor the authors or the editors give a warranty, express or implied, with respect to the material contained herein or for any errors or omissions that may have been made. The publishers remain neutral with regard to jurisdictional claims in published maps and institutional afﬁliations. This Springer imprint is published by the registered company Springer Nature Singapore Pte Ltd. The registered company address is: 152 Beach Road, #21-01/04 Gateway East, Singapore 189721, Singapore

Preface

Solid-state laser systems are compact, easy to use, easy to tune, and have good beam quality; they have unique advantages comparing with lasers of gas, liquid, and other media so that have a very wide and important application in many ﬁelds. Therefore, it is necessary to search for suitable materials according to different performance requirements. This requires the material researchers deeply grasp the physical knowledge about the main performance of solid-state laser materials. Many excellent monographs have been published in this ﬁeld; however, we feel necessary to update them by including new published literatures as well as our own research work. The subject of this book is spectroscopic principle of rare earth ions and transition metal ions doped in solid. In addition to many general principles of spectroscopy and calculation methods, to determine the symmetry of the energy level, a unique group chain method is introduced, while a method from traditional crystal ﬁeld theory based on a comprehensive crystal ﬁeld quantum number table is also described. The stimulated non-radiative transition theory and the apparent crystal ﬁeld model introduced by us are discussed. Comparing with many published books, this book has the following advantages. That is, it derives all the calculation formulas from the ﬁrst principles of physics instead of direct citation in some books, so that readers can understand the physics insight clearly and exploit them correctly in their own work. Furthermore, readers could develop related formulas by themselves, which have not been given in this book, following the method provided in this book. We hope this book will provide useful references for researchers in solid-state laser materials, luminescent materials, solid-state spectroscopy, and laser science and technology, as well as senior undergraduates and postgraduates having basis knowledge of optics, quantum mechanics, spectroscopy, and condensed matter physics. The focus of this book is on the physical fundamentals. The spectral, laser, and physical properties of the materials mentioned in the book are just scales and claws, especially without reference to the rapidly developing and widely used ceramic laser materials and new activated ions such as bismuth in recent years. On the other hand, many excellent research works of peer experts have not been quoted. It is v

vi

Preface

unavoidable that there are mistakes or omissions in the book, and readers are welcome to criticize and correct them. We express gratitude to the Fujian Institute of Research on the Structure of Matter, Chinese Academy of Sciences, the Key Laboratory of Research on Chemistry and Physics of Optoelectronic Materials, Chinese Academy of Sciences, and the National Natural Science Foundation of China for their support and funding, also appreciate the help from editor Zhou Han of China Science Publishing House and editors of Springer Nature Press. Fuzhou, China

Zundu Luo Yidong Huang

About This Book

This book discusses in detail the spectral properties of solid-state laser materials, including emission and absorption of light, the law of radiative and non-radiative transitions, the selection rule of optical transition, and the calculation methods for the spectral parameters. To determine the symmetry of the energy level, a unique group chain method is introduced, while a method from traditional crystal ﬁeld theory based on a comprehensive crystal ﬁeld quantum number table is also described. The research works of the authors on this ﬁeld, especially the stimulated non-radiative transition theory and the apparent crystal ﬁeld model, are introduced. As such, the book provides essential tools for researchers and graduate students in the ﬁelds of solid spectroscopy and solid laser material physics, while also offering a valuable reference guide for instructors and advanced students of physics.

vii

Contents

1

2

3

Energy Level of Free Ions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Energy Levels of the Single Electron in Atoms (Free Ions) . 1.2 General Properties of Energy Level in Multi-electron of Free Ions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3 Energy Levels of Free Transition-Metal Ions . . . . . . . . . . . 1.4 Energy Levels of Free Rare Earth Ions . . . . . . . . . . . . . . . . 1.5 Theory of Interactions in Rare Earth Ions . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

... ...

1 1

. . . . .

. . . . .

. . . . .

7 11 15 24 29

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

31 31 33 36 40 41 41 43 46 48 52 55

..... .....

61 67

Rare Earth Ions in Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Crystal Field on the Active Ions . . . . . . . . . . . . . . . . . . . . . . . 3.2 Energy Level Splitting of the Rare Earth Ions . . . . . . . . . . . . .

69 69 72

Group Theory and Quantum Theory . . . . . . . . . . . . . . . . . . 2.1 Mathematical Description of the Symmetry . . . . . . . . . . 2.2 Basic Conception of the Group . . . . . . . . . . . . . . . . . . . 2.3 Theory of Group Representations . . . . . . . . . . . . . . . . . . 2.4 Direct Product Group and Direct Product Representation 2.5 Sketches of the Group in Spectroscopy . . . . . . . . . . . . . 2.5.1 Finite Group . . . . . . . . . . . . . . . . . . . . . . . . . . 2.5.2 Permutation Group . . . . . . . . . . . . . . . . . . . . . . 2.5.3 Continuous Groups . . . . . . . . . . . . . . . . . . . . . . 2.6 Point Group and Their Representation . . . . . . . . . . . . . . 2.7 Symmetry and Quantum Theory of the Ions in Solids . . . 2.8 Full Rotation Group and Angular Momentum Theory . . . 2.9 Irreducible Tensor Operators and the Calculation of Matrix Elements . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

ix

x

Contents

3.3 Crystal Field Quantum Number . . . . . . . . . . . . . . . . . . . . . . . . 81 3.4 Group Chain Scheme Method in Crystal Field Analysis . . . . . . 90 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 101 4

5

6

7

Theory of Radiative Transition . . . . . . . . . . . . . . . . . . 4.1 Interactions Between Active Ions and Radiation . . 4.2 Probability of Emission and Absorption Processes 4.3 Selection Rules for Radiative Transition . . . . . . . . 4.3.1 Selection Rules for Radiative Transition of Free Ions and Atoms . . . . . . . . . . . . . 4.3.2 Selection Rules for Radiative Transition of Ions in Materials . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

103 103 107 115

. . . . . . . . . . 115 . . . . . . . . . . 116 . . . . . . . . . . 123

Spectroscopic Parameter and Their Calculation . . . . . . . . 5.1 Absorption Coefﬁcient, Absorption (Emission) Cross-Section, and Oscillator Strength . . . . . . . . . . . . 5.2 Analysis of the Absorption Coefﬁcients of Anisotropic Crystal . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3 Judd–Ofelt Approximation and Related Parameter . . . 5.4 Spectroscopic Parameter Calculation of Rare Earth Ion in Crystal . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5 Hypersensitive Transitions . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . 125 . . . . . . . 125 . . . . . . . 132 . . . . . . . 136 . . . . . . . 145 . . . . . . . 156 . . . . . . . 158

Phonon and Spectral Line . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1 Quantization of Lattice Vibration—Phonon . . . . . . . . . . . . . 6.2 Phonon Emission and Absorption in the Optical Transition . . 6.3 Main Mechanisms of the Thermal Spectral Line Broadening and Shifting . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 The Contribution of Single-Phonon Absorption (Emission) to the Spectral Linewidth . . . . . . . . . . . . . . . . . . . . . . . . . . 6.5 The Contribution of Phonon Raman Scattering to the Spectral Linewidth . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6 Calculation of the Thermal Shifting of Spectral Lines . . . . . . 6.7 Examples for the Calculation of Thermal Spectral Line Broadening and Shifting . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . 161 . . 161 . . 170 . . 181 . . 183 . . 187 . . 192 . . 196 . . 201

Energy Levels and Spectroscopic Properties of Transition Metal Ions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 203 7.1 Energy Levels and Spectral Properties of 3d1 Electron System . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 204 7.2 Energy Levels and Spectral Properties of 3d2 Electron System . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 210

Contents

xi

Energy Levels and Spectral Properties of 3d3 Electronic System . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.4 Relative Intensity Analysis of R Line in Ruby Polarized Absorption Spectrum . . . . . . . . . . . . . . . . . . . . . . . . . 7.5 Estimation of Trivalent Chromium Ion Spectral Parameters in Solid-State Laser Materials . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

7.3

8

9

. . . . . . 219 . . . . . . 228 . . . . . . 232 . . . . . . 238

Non-radiative Transition Inside Ions . . . . . . . . . . . . . . . . . . . 8.1 Introduction of Non-radiative Transition Matrix Elements 8.2 Promoting Mode and Accepting Mode in Non-radiative Transition Process . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.3 Non-radiative Transition Probability for Weak Coupling Systems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.4 Parallelism Between Non-radiative Transition Probability and Radiative Transition Probability . . . . . . . . . . . . . . . 8.5 Temperature Dependence of Non-radiative Transition Probability in Weak Coupling Systems . . . . . . . . . . . . . 8.5.1 Experimental . . . . . . . . . . . . . . . . . . . . . . . . . . 8.6 Non-radiative Transition in Strong Coupling Systems . . . 8.7 Nonlinear Theory of Non-radiative Transition . . . . . . . . . 8.8 Stimulated Non-radiative Transition . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Energy Transfer and Migration Between Ions . . . . . . . 9.1 Theory of Resonant Energy Transfer . . . . . . . . . . . 9.2 Phonon-Assisted Energy Transfer Between Ions . . . 9.3 Statistical Theory of Energy Transfer Between Ions 9.4 Energy Migration Between Ions . . . . . . . . . . . . . . . 9.5 Characteristics of Concentration Dependent Fluorescence Quenching for Self-activated Laser Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

10 Laser 10.1 10.2 10.3

. . . . .

. . . . .

. . . . .

. . . . .

. . . . . 241 . . . . . 242 . . . . . 246 . . . . . 248 . . . . . 254 . . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

256 256 258 265 268 274

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

277 278 282 287 290

. . . . . . . . . 303 . . . . . . . . . 306

and Physical Properties of Materials . . . . . . . . . . . Brief Introduction of Solid-State Laser Principle . . . . Quality Factor of Solid-State Laser Materials . . . . . . Relationship Between Laser Threshold and Chemical Composition of Host Materials . . . . . . . . . . . . . . . . 10.4 Thermo-Mechanical and Thermo-Optical Properties of Solid-State Laser Materials . . . . . . . . . . . . . . . . . 10.5 Laser Damage and Nonlinear Optical Properties . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . 309 . . . . . . . . 309 . . . . . . . . 316 . . . . . . . . 318 . . . . . . . . 322 . . . . . . . . 337 . . . . . . . . 342

xii

Contents

11 Nonlinear Optical Properties of Laser Crystals and Their Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.1 Second-Order Nonlinear Optical Effect of Crystal . . . . . . . 11.2 Relationship Between Fundamental and Second Harmonic Waves in SFD Laser Crystal . . . . . . . . . . . . . . . . . . . . . . 11.3 Nonlinear Optical Coupling Equation of SFD Laser . . . . . 11.4 Self Sum-Frequency Mixing Effect in Nonlinear Laser Crystal . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.5 Stimulated Raman Scattering Effect of Laser Crystal . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12 Apparent Crystal Field Model of Laser Glass and Its Application . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.1 Structure and Spectral Characteristics of Glasses . . . 12.2 Apparent Crystal Field Hamiltonian for Rare Earth Ions in Non-crystal Host . . . . . . . . . . . . . . . . . . . . 12.3 Crystal Field Level Analysis for Er3+ Ions in Three Typical Glasses . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . 345 . . . . 347 . . . . 354 . . . . 359 . . . . 366 . . . . 374 . . . . 383

. . . . . . . . . 385 . . . . . . . . . 386 . . . . . . . . . 391 . . . . . . . . . 399 . . . . . . . . . 412

Appendix A: Character Tables for Point-Symmetry Group . . . . . . . . . . 415 Appendix B: Correlation Table of Group–Subgroup . . . . . . . . . . . . . . . . 421 Appendix C: Multiplication Tables for Some Point Groups . . . . . . . . . . 425 Appendix D: Squared Reduced-Matrix Elements of Unit Operator for J ! J′ Transition in Rare Earth Ions . . . . . . . . . . . . . . 427 Appendix E: 3jm Factors for Some Group Chains . . . . . . . . . . . . . . . . . . 453 Appendix F: Clebsch-Gordan Coefﬁcients of the Cubic Point Group with Trigonal Bases . . . . . . . . . . . . . . . . . . . . . . . . . 459 Appendix G: Integral Numerical Value Associated with the Thermal Effect of the Spectra . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 463 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 467

About the Authors

Zundu Luo is a professor at Fujian Institute of Research on the Structure of Matter (FIRSM), Chinese Academy of Sciences. He has been working in the ﬁeld of spectroscopic physics and laser crystal research since 1965, serving as the leading scientist of the research group of new laser crystal materials from 1982 to 2003. He has published more than 100 articles in SCI indexed journals and has been awarded the Second Class Prize of China’s National Science and Technology Progress and the First Class Prize of Scientiﬁc and Technological Progress of Chinese Academy of Sciences. Yidong Huang got his Ph.D. from Strathclyde University in 1997. He became a professor at Fujian Institute of Research on the Structure of Matter (FIRSM), Chinese Academy of Sciences in 1999. He is currently a member of the council of Chinese Optical Society. His research interests include laser and luminescence properties of rare earth and transition metal ions in solids; new laser and non-linear crystals, laser glasses, solid luminescence materials, and related devices. He has been working in the ﬁeld of laser crystal and solid state laser since 1987, as the leading scientist of the research group of laser crystal and solid state laser from 2004. He has published more than 200 articles in SCI indexed journals, and owns more than 20 patents. As a partner, he got one Second Class Prize of China’s national science and technology progress and one First Class Prize of scientiﬁc and technological progress of Chinese Academy of Sciences.

xiii

Chapter 1

Energy Level of Free Ions

Most of the solid-state laser materials consist of insulators doped with a small amount of rare earth ion or transition-metal ion (optically active ions, which will be simply called active ions in all the discussions of this book). The spectra of all these materials have very close relationship with the energy level structure of free ion (atom) and the transition rules between these energy levels. Therefore, the basic knowledge of the atomic spectroscopy is very important for the investigation of laser materials. There are many good reference books in this ﬁeld, for example, Herzberg [1], Condon and Shortley [2], Slater [3], and Condon and Odabasi [4]. In this chapter, only some basic knowledge necessary to the discussion in this book will be covered. The books mentioned can be referred for further understanding.

1.1

Energy Levels of the Single Electron in Atoms (Free Ions)

In the hydrogen atom as well as hydrogen-like atoms, for example, He+, Li2+, Be3+, and so on, there is only one electron around a nucleus with positive charge. The spectroscopy of single electron atoms is the only problem which can be dealt with by quantum mechanics strictly. However, it is the most important background for the analysis of the other problems of atomic spectroscopy. The quantum mechanics is used to analyze hydrogen atom and hydrogen-like atoms and solve a Schrödinger equation for a charged particle in a central electric ﬁeld. Its Hamiltonian can be written as H ¼ H0 þ Hso þ HZ þ other small terms

ð1:1Þ

where H0 is the Hamiltonian describing the interaction of the electron with the nucleus. Hso is the spin–orbital interaction Hamiltonian © Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8_1

1

2

1 Energy Level of Free Ions

Hso ¼ nðrÞl s

ð1:2Þ

where n(r) is the coefﬁcient of the spin–orbital coupling, l ¼ r p denotes the orbital vector operator of the electron, and s is the spin vector operator of the electron. The spin–orbital interaction is actually a relativistic effect. Besides, the other relativistic effects will not be considered here. HZ is the interaction Hamiltonian of the atoms in external magnetic ﬁeld. If the magnetic induction of external magnetic ﬁeld is represented by B, then HZ can be written as HZ ¼

e sB me

ð1:3Þ

where e denotes the electric charge of electron and me is the mass of electron. The general method to deal with the above problem in quantum mechanics is to consider at ﬁrst the main term in the Hamiltonian and then introduce the small terms as a perturbation. Without magnetic ﬁeld and spin–orbital interaction, we have H ¼ H0 ¼

2 2 2 2 h Ze2 h @ 2 @ 2 l 2 h Ze2 ¼ r þ þ 2 2 r @r 2me 4pe0 r 2me @r 2me r 4pe0 r ð1:4Þ

In spherical coordinate system, the components of the orbital angular momentum operator can be written as @ @ lx ¼ ih sin / þ cot h cos / @h @/ @ @ ly ¼ ih cos / cot h sin / @h @/ @ lz ¼ ih @/ Therefore 1 @ @ 1 @2 sin h l ¼ h þ 2 sin h @h @h sin h @/2

2

2

ð1:5Þ

The properties of the angular momentum operator will be discussed later in more detail. The solution of the Schrödinger equation should be presented at ﬁrst. The steady-state Schrödinger equation is expressed as h2 1 @ 1 @ @ 1 @2 Ze2 2 @ r sin h w ¼ Ew þ þ w @r r 2 sin h @h @h r 2 sin h @/2 2me r 2 @r 4pe0 r ð1:6Þ

1.1 Energy Levels of the Single Electron in Atoms (Free Ions)

3

The wave function W can be solved by means of variable separation method. One should ﬁrst separate the radial part and angular part as wðr; h; /Þ ¼ RðrÞY ðh; /Þ Then substituting into (1.6), we obtain 1 d 2me r 2 Ze2 1 1 @ @Y 1 @2Y 2 dR r sin h Eþ þ þ 2 ¼ R dr dr Y sin h @h @h 4pe0 r sin h @/2 h2 ð1:7Þ One can see in the above equation that the terms in the left-hand side depend only on the radial coordinate r, while those in the right-hand side depend only on the angular variables h and /. The validity of the equation means that both sides should be equal to a constant k. In this way, one equation of the variable r is obtained as 1 d 2me Ze2 k 2 dR r Eþ þ 2 R¼0 r 2 dr dr r 4pe0 r h2

ð1:8Þ

The other equation of angular variables h and / will be 1 @ @Y 1 @2Y sin h þ kY ¼ 0 þ 2 sin h @h @h sin h @/2

ð1:9Þ

Suppose Yðh; /Þ ¼ HðhÞUð/Þ, then the equation for angular variables can be further separated as d2 Uð/Þ þ m2 Uð/Þ ¼ 0 d/2

ð1:10Þ

with solution of Uð/Þ ¼ ð2pÞ1=2 expðim/Þ and m ¼ 0; 1; 2; . . .. The other equation is 1 d dHðhÞ m2 sin h þ k 2 HðhÞ ¼ 0 sin h dh dh sin h

ð1:11Þ

Let n ¼ cos h, then d dH m2 ð1 n2 Þ þ k H¼0 dn dn 1 n2

ð1:12Þ

This is the associated Legendre equation. Solution of this equation is valid in the range of 1 n 1, and the constant k can only be k ¼ lðl þ 1Þ, l = 0, 1, 2, 3, …, and jmj l. Its solution is

4

1 Energy Level of Free Ions

HðhÞ ¼ ð1Þðm þ jmjÞ=2

ð2l þ 1Þðl jmjÞ! 1=2 ðlÞ Pjmj ðcos hÞ 2ðl þ jmjÞ!

ð1:13Þ

Therefore YmðlÞ ðh; /Þ ¼ ð2pÞ1=2 ð1Þðm þ jmjÞ=2

ð2l þ 1Þðl jmjÞ! 1=2 ðlÞ Pjmj ðcos hÞ expðim/Þ 2ðl þ jmjÞ! ð1:14Þ

The spherical harmonic function Ylm ðh; /Þ, designated by quantum numbers l and m, is orthogonal and normalized, that is Z2p Zp 0

ðl0 Þ

Ym0 ðh; /ÞYmðlÞ ðh; /Þ sin hdhd/ ¼ dl0 l dm0 m

ð1:15Þ

0

For the problem of single electron in hydrogen atom, the equation for radial variable can be solved and expressed by Laguerre polynomials as l 2Zr þ1 Rnl ðrÞ ¼ Nnl expðZr=na1 Þ L2l ð1:16Þ n þ 1 ð2Zr=na1 Þ na1 where the constant of normalization Nnl is ( )1=2 2Z 3 ðn l 1Þ! Nnl ¼ na1 2n½ðn þ lÞ!3

ð1:17Þ

where a1 is the ﬁrst Bohr radius of the hydrogen atoms a1 ¼

4pe0 h2 me e2

Integer n called principal quantum number should satisfy n l þ 1 and the energy eigenvalues will be given by En ¼

Z 2 e2 m e Z 2 e4 ¼ 2 4pe0 2a1 n 2ð4pe0 Þ2 n2 h2

ð1:18Þ

Here SI unit system is used. Changing to CGS unit system, the electron charge e should be multiplied by a factor of (4pe0)1/2. It can be seen from (1.18) that the energy of single electron in the hydrogen and hydrogen-like atoms only depends on the principal quantum number n, if the spin– orbit interaction and other relativistic effects are neglected. Thus the states with different angular momentum and spin momentum quantum number but the same

1.1 Energy Levels of the Single Electron in Atoms (Free Ions)

5

principal quantum number have the same energy, which correspond to the degeneracy of the electronic states. The degree of the degeneracy f is found to be f ¼2

n1 X

ð2l þ 1Þ ¼ 2n2

ð1:19Þ

l¼0

Note that (1.4) shows the Hamiltonian without perturbation and possesses coordinates inversion symmetry, that is, the Hamiltonian is invariant with respect to the transformation of r ! r. In the spherical coordinate system, it corresponds to the transformations of r!r, h ! p h; / ! p þ /. If the inversion operator Pi is introduced, then Pi f ðrÞ ¼ f ðrÞ It is easy to show that [H0, Pi] = 0. Then, by a basic principle of quantum mechanics, the eigenstates of H0 are also the eigenstates of Pi. In this way, the eigenstates can be classiﬁed as even parity states and odd parity states. It can be demonstrated that Ylm ðp h; p þ /Þ ¼ ð1Þl Ylm ðh; /Þ

ð1:20Þ

namely Pi jnlmi ¼ ð1Þl jnlmi where l if even or odd corresponds to even or odd parity state, respectively. The energy correction by the spin–orbit interaction effect is DEls ¼

Z 4 m e e 4 a2 jðj þ 1Þ lðl þ 1Þ sðs þ 1Þ 2 3 1 2 ð4pe0 Þ 2h n l l þ 2 ðl þ 1Þ 2

ð1:21Þ

where a = 1/137 is the ﬁne structure constant and j is the total angular momentum quantum number involving the spin–orbital interaction. By calculating the energy correction due to relativistic effect of mass but not the other relativistic effects, Summerﬁeld obtained the following result DErel ¼

Z 4 m e e 4 a2 ð4pe0 Þ2 2h2 n4

n 3 l þ 12 4

! ð1:22Þ

Dirac established a relativistic equation of the electron in 1928, taking into account simultaneously the spin–orbital interaction and the other relativistic effects, and he obtained

6

1 Energy Level of Free Ions

Z 2 e2 Z 4 e 2 a2 1 3 Enj ¼ 2 ð4pe0 Þ 2a1 n ð4pe0 Þ 2a1 n3 j þ 12 4n

! ð1:23Þ

Owing to the fact that a2 = 5 10−5, the corrections introduced by the spin–orbital interaction and the relativistic effect of mass are very small and have a magnitude of 10−1 – 10−2 cm−1. There is one kind of atoms, in which the electrons are like that in the hydrogen atom. For example, the atoms of alkali metal, such as Li, Na, and K, have one valence electron with very weak coupling to its atomic core. The atomic cores have the electronic structure like those of the inert gases He, Ne, and Ar. The energy eigenvalue of the valence electron without the effect of spin–orbital interaction has a similar expression as that of the hydrogen atom 0 Enl ¼

Z 2 e2 ð4pe0 Þ 2a1 n 2

ð1:24Þ

where the principal quantum number n is replaced by effective quantum number n* and n ¼ n D. The quantum defect D has only a slight variation with the change of principal quantum number n. However, it decreases obviously even if the angular momentum quantum number has only a slight increase. It can be seen that the energy eigenvalue Enl depends not only on n but also on l. If the spin–orbital effect is also taken into account, one has 0 Enljs ¼ Enl

Z 4 me e4 a2 jðj þ 1Þ lðl þ 1Þ sðs þ 1Þ 2 2 3 1 2 ð4pe0 Þ 2h n l l þ 2 ðl þ 1Þ ð1:25Þ

where the effective charge Z ¼ Z r and r is the shielding constant. It means that the effect of interaction of the valence electron studied with the electrons of ﬁlled shell in the atom is to reduce the effect of nucleus charge. The spin–orbital interaction is proportional to Z4 and so the splitting of yellow D line of sodium is only 17.2 cm−1 while the corresponding value for the main line system of cesium atom reaches 554 cm−1. The basic but most useful result of the theory of single electron atom is that an electronic state is labeled by a principal quantum number n, an orbital angular momentum quantum number, a magnetic quantum number m, and a spin quantum number s. This is the basis for the discussion of multi-electron problems. Characters s, p, d, f, h, i, k, l, m, n, o, q … are used to denote l = 0, 1, 2, 3, 4, 5, 6, 7, 8, 9, 10, 11, 12 … in spectroscopy.

1.2 General Properties of Energy Level in Multi-electron of Free Ions

1.2

7

General Properties of Energy Level in Multi-electron of Free Ions

Multi-electron systems are complicate systems in quantum mechanics. The atoms can be treated as N electrons with mass me and charge −e moving around a nucleus with inﬁnite mass and charge of +Ze and other electrons in the atom. The non-relativistic Hamiltonian without spin–orbital interaction is N 2 N X X pi Ze2 e2 H¼ þ 2me 4pe0 ri 4pe0 ri;j i¼1 i [ j¼1

ð1:26Þ

The second term in the above expression involves variable ri,j, the distance between electron i and electron j; therefore, it is impossible to use the method of variable separation. Furthermore, this term is large enough and so perturbation method cannot be used. It is impossible to solve its energy level structure strictly and analytically. Fortunately, just like many other problems in quantum mechanics, this problem can be solved by approximate method neglecting less important interactions. Among these, the central ﬁeld approximation is the most important one; it assumes that each electron moves independently in the ﬁeld of nucleus and the central ﬁeld is made up of spherically averaged potential ﬁelds of the other electrons described by a function U(ri)/e. The non-spherical part of the electronic interactions is treated as a perturbation, so the approximated Hamiltonian can be expressed as H0 ¼

N 2 X pi þ Uðri Þ 2me i¼1

ð1:27Þ

Then Schrödinger equation will be N X h2 r2i þ Uðri Þ w ¼ E 0 w 2me i¼1

ð1:28Þ

Obviously, the N variables ri in the above equation can be separated, that is the wave function and eigenvalue can be expressed as w¼

N Y i¼1

wi ðki Þ; E0 ¼

N X

E 0 ð ki Þ

ð1:29Þ

i¼1

where ni ; li ; mi are simply represented by ki . For different variables ri, the equations have the same form. Thus the subscript i can be eliminated

8

1 Energy Level of Free Ions

2 2 h r þ UðrÞ wðkÞ ¼ E 0 wðkÞ 2me

ð1:30Þ

The difference between the above equation and that of the hydrogen atom is the potential function and so there is a difference in the radial wave function but the wave functions of the angular part are the same. The wave function can still be written as wðkÞ ¼ Rnl ðrÞYðmlÞ ðh; /Þ

ð1:31Þ

The energy E0 ðkÞ is degenerated for different quantum number m. Taking into account the electron spin, the wave function w(k) should be multiplied by a spin wave function a or b, which corresponds respectively to ms = +1/2 or ms = −1/2. According to Pauli exclusion principle, no two electrons can have the same set of four quantum numbers n, l, m, and ms simultaneously. As a result, the mathematic expression for the wave functions must be a determinant. For example, the wave function for three electrons will be w1 ðk1 Þa1 1=2 0 w ¼ ð3!Þ w2 ðk1 Þa2 w ðk1 Þa3 3

w1 ðk2 Þb1 w2 ðk2 Þb2 w3 ðk2 Þb3

w1 ðk2 Þa1 w2 ðk2 Þa2 w3 ðk2 Þa3

ð1:32Þ

and can be simpliﬁed as w0 ¼

þ þ þ k1 k2 k3

ð1:33Þ

where + is used to denote spin function a, and − denotes the spin function b. In an atom, there are at most 2(2l + 1) electrons that can simultaneously have the same n and l, and a completely ﬁlled electron shell is in which all the states with given n, l, m, and ms are occupied. From expressions of (1.20) and (1.29), it can be shown that the parity of P multi-electron system is Ni¼1 li , odd of this summation corresponds to a odd parity state and even of this summation corresponds to a even parity state, because each term in the determinant has the following relation Y

Rnl ðri ÞYmðlÞ ðh

P

p; p þ /i Þ ¼ ð1Þ

li Y

i

i

Rnl ðri ÞYmðlÞ ðh; ui Þ

i

therefore

P PW ¼ ð1Þ

i

li

W

There is also an important simpliﬁcation in the studies of the multi-electron problem of atoms (ions), that is, neglecting the effect of completely ﬁlled electron shells. In these

1.2 General Properties of Energy Level in Multi-electron of Free Ions

9

shells, the total angular momentum and spin momentum of the electrons are equal to zero and so their effect is the same on the electrons of different energy states in the partially ﬁlled shells. Therefore, in the discussion of the energy level splitting of the multi-electron system, the effect of the completely ﬁlled shells is not necessary to be taken into account. For example, the electronic conﬁguration of Nd3+ ions is 1s22s22p63s23p63d104s24p64d105s25p64f3. If the completely ﬁlled electron shells are not considered, only three 4f electrons should be taken into account. In this way, the work of the energy level calculation will be greatly reduced. However, even in this situation, the number of the energy levels is still very large. In the 4f3 conﬁguration, l = 3, −3 m 3, and ms ¼ 12. There are 14 states with the same n and l but different m and ms. Then, the three f electrons can occupy any of the 14 states. Therefore, taking into account of the spin, the total number of 14! states will be ð143Þ!3! ¼ 364. The quantum numbers n and l are all equal to 4 and 3, respectively; thus it is enough to use only quantum number m and ms to designate the energy state as {3+2+1+}, {3+−3+1+}, {0−−1−−3+}, and so on. Even in this case, there are 364 364 = 132, 496 matrix elements to be calculated, if one wants to study their energy levels. Fortunately, the symmetry of the system can be used to simplify the calculation of energy levels. In the free atoms, the continuous group and angular momentum theory can be used, and for the electrons of ions in the crystals, one can use the point group theory, which will be discussed in next chapter. First, we would like to mention the formation of spectral terms, their symbols, and the Hund rule for determining the ground states. By the interaction of electron orbital magnetic moment with spin magnetic moment, the energy levels of each electronic conﬁguration will be split into a series of energy level sets designated by a total spin quantum number S and a total orbital angular momentum quantum number L. Each energy level set contains (2S + 1) (2L + 1) states. Such energy level set is called spectral term using symbol 2S+1L. The interaction between orbital momentum and spin momentum is called the coupling of orbital angular momentum with spin angular momentum. There are four models of coupling in the atomic spectroscopy theory, that is, LS coupling (Russell–Saunders coupling), jj coupling, pair coupling (Racah coupling), and intermediate coupling. These depend on the relative magnitude between the Coulomb and the spin–orbital interactions. Generally speaking, the spin–orbit interaction has a magnetic origin and will be rapidly intensiﬁed as the atomic number Z increased. Calculated by the hydrogen wave function, spin–orbit coupling coefﬁcients can be expressed as [5] nnl ¼

e2 h2 Z4 2m2 e2 a21 n3 l l þ 12 ðl þ 1Þ

The spin–orbit splitting of sodium D line is 17.2 cm−1 while that of the cesium atom’s main line reaches 554 cm−1. For the rare earth ions, the spin–orbit coupling coefﬁcients of Tm3+ ions are more than three times higher than that of the Pr3+ ions. On the other hand, the spin–spin interaction is basically independent of Z. This phenomenon is

10

1 Energy Level of Free Ions

obvious which resulted from the nature of the spin–spin interaction, because it is a direct interaction between two electrons and so is not affected by the nucleus ﬁeld. Therefore, for the atoms with smaller atomic number Z, the magnitude of spin–spin interaction is larger than that of spin–orbital interaction. In this case, the spin momenta si of all the electrons will be coupled by exchange interaction to form a total spin angular momentum S. Similarly, the orbital momenta li of all the electrons will also be coupled by Coulomb interaction to form a total orbital angular momentum L. Finally, the total spin angular momentum S couples with the total orbital angular momentum L. This is so-called LS coupling. However, for the atoms with very large atomic number, and especially for their excited states, the couplings between the spin angular momentum and the orbital angular momentum of the same electron are stronger than the spin–spin couplings between different electrons. Therefore, the orbital angular momentum li couples with the spin angular momentum si of the same electron to form a total angular momentum ji of the electron, then ji of all the electrons will couple to form the total angular momentum J of the whole system. This is so-called jj coupling. LS coupling is the most commonly used model. For transition-metal ions, and especially their ground spectral terms, the LS coupling model can be used. This model can also be used in the ﬁrst approximation problems of rare earth ion in which the electrostatic interaction between different 4f electrons and the spin–orbit interaction have the same order of magnitudes. According to this model, the states can be designated by 2S+1LJ. The calculation of the state energies is to solve the eigenvalue problem of Hamiltonian involving all interactions in the atom and so the complicated and tedious work should be done. However, the qualitative rules are helpful to understand the energy level structure. Hund rule is one of the well-known qualitative rules, which has the following guidelines: (1) The spectral terms (or states) with the largest S values have the lowest energy values among all the spectral terms of an electron conﬁguration. Among these terms, those with the highest L values have the lowest energy values. (2) For the spectral terms in a conﬁguration with a number of electrons equal to or greater than that of the half-ﬁlled shell, the larger the J value, the lower is the energy. On the other hand, if the number of electrons is less than that of the half-ﬁlled shell, then the smaller the J values, the lower is the energy. Hund rule is very convenient to determine the ground state of an electronic conﬁguration. Taking the example of the trivalent rare earth ion Nd3+ mentioned above, its electronic conﬁguration (4f3) belongs to the case of an electron number lower than that of a half-ﬁlled shell. The total spin of three electrons can be 3/2 in maximum, and the maximum L is 6. According to the second guideline of Hund rule, the energy of state with J = 9/2 will be the lowest one. Therefore, the ground states should be 4I9/2. The trivalent erbium ions have electronic conﬁguration 4f11 and have the same spectral terms and states as those for the 4f3 conﬁguration. However, its electron number is greater than that of the half-ﬁlled shell and so the larger the J, the lower is the energy. Then its ground state should be 4I15/2.

1.2 General Properties of Energy Level in Multi-electron of Free Ions

11

In the case of LS coupling, the energy separation of the energy levels with different total angular quantum number J in the same spectral term 2S+1L has a rule called Landé interval rule. It can be expressed as DEJ DEJ1 ¼ AðLSÞJ, where the constant A(LS) depends on the value of LS and their signs determine whether the electron shell is half-ﬁlled or less than half-ﬁlled (the electron number in the shell q 2l + 1, A(LS) > 0) or greater than half-ﬁlled (the electron number in the shell q > 2l + 1, A(LS) < 0). This rule can be demonstrated as follows. Owing to the fact that the splitting of the energy levels with different total angular quantum number J in the same spectral term 2S+1L is the effect of spin–orbit interaction and proportional to L S, this energy separation can be written as DEJ ¼ C ðLSÞL S: Because of J¼L þ S; jJ j2 ¼ jLj2 þ jSj2 þ 2L S and so LS¼

h2 1 2 jJ j jLj2 jSj2 ¼ ½J ðJ þ 1Þ LðL þ 1Þ SðS þ 1Þ 2 2

DEJ ðSLÞ DEJ1 ðSLÞ ¼ CðLS2 Þh ½J ðJ þ 1Þ J ðJ 1Þ ¼ AðLSÞJ where AðLSÞ ¼ CðLSÞh2 . However, as will be pointed out in the next section, the energy separation of different J in the same spectral term 2S+1L will not follow strictly the Landé interval rule in the case of intermediate-coupling approximation. It should be pointed out that besides the above-mentioned interaction, the electrons in the atoms also have smaller inter-conﬁguration interaction, Coulomb and spin–orbit-correlated interaction, spin–spin interaction as well as spin–other orbital interaction. We will introduce simply these interactions and their effects in energy level calculation of rare earth ions in Sect. 1.5. 2

1.3

Energy Levels of Free Transition-Metal Ions

The transition-metal group discussed here is also called ﬁrst transition group and has partially ﬁlled electron shell 3dq (q < 10). The LS coupling is suitable for the electrons in this group especially for their ground conﬁguration. The spectral terms in 3dq conﬁguration are listed in Table 1.1. For the 3dq with q > 3, two quantum Table 1.1 Spectral terms of dq electronic conﬁguration [17] Conﬁguration 1

d, d2, d3, d4, d5

9

d d8 d7 d6

Spectral term 2

D1 S, 2 1 P, 1 2 S, 2 1 S,

1 1 1

D1, 1G1, 3P1, 3F1 D2, 2F1, 2G1, 2H1, 4P1, 4F1 1 2 1 1 1 2 1 1 3 2 3 1 3 2 3 1 3 1 5 1 D, F, G, I, P, D, F, G, H, D 2 1 2 3 2 2 2 2 2 1 2 1 4 1 4 1 4 1 4 1 6 1 P, D, F, G, H, I, P, D, F, G, S 2

12

1 Energy Level of Free Ions

Table 1.2 Classiﬁcation of the spectral terms in d3, d4, and d5 conﬁguration according to the reducing branching rule of the group chain U ð10Þ SU ð2Þ U ð5Þ SU ð2Þ SOð5Þ SU ð2Þ SOð3Þ Conﬁguration

U(10)

SU(2) ⊗ U(5)

SU(2) ⊗ SO(5)

SU(2) ⊗ SO(3)

d3(d7)

[13]

2

2

2

[2, 1]

4

d4(d6)

[14]

[1, 1] [2, 2]

1

3

[211]

5

d

5

5

[1 ]

[1] [2, 2, 1]

2

4

[2, 1, 1, 1]

(1, 2 (2, 4 (1, 1 (0, 1 (2, 1 (2, 3 (1, 3 (2, 5 (1, 2 (1, 2 (2, 2 (2, 4 (1, 4 (2, 6 (0,

0) 1) 1) 0) 0) 2) 1) 1) 0) 0) 1) 2) 1) 0) 0)

D P, 2D, 4 P, 4F 1 S 1 D, 1G 1 S, 1D, 3 P, 3F 3 P, 3D, 5 D 2 D 2 P, 2D, 2 S, 2D, 4 P, 4F 4 D, 4G 6 S 2

2

F, 2G, 2H

1

F, 1G, 1I

3

F, 3G, 3H

2

F, 2G, 2H F, 2G, 2I

2

numbers L and S cannot completely discriminate different spectral terms. The right superscript of the spectral term’s symbol in Table 1.1 denotes the number of spectral terms with the same quantum numbers L and S. Different spectral terms with the same quantum numbers L and S should be discriminated by different irreducible representation symbol of group chain. By using different irreducible representation symbol in the continuous group chain U ð10Þ SUð2Þ Uð5Þ SUð2Þ SOð5Þ SUð2Þ SOð3Þ, different spectral terms of this conﬁguration can be completely discriminated. The spectral terms of three 3dq conﬁgurations with q = 3, 4, and 5 according to irreducible representation branch of above group chain are listed in Table 1.2. The q values for unﬁlled electron shell 3dq (q < 10) are listed in Table 1.3. Owing to the fact that 3dq is an outer shell, the crystal ﬁeld interaction is of the same order of magnitude as the electron–electron Coulomb interaction (about 104 cm−1). However, it is much stronger than that of the spin–orbital interaction (about 102 cm−1). Therefore, energy levels of these ions are strongly affected by the electrostatic ﬁeld and the vibration of lattice ions. The energy level structure is very different for different host materials. It will be discussed later in a single chapter. Only the main features of the free iron group ions will be introduced here. Slater-Condon parameters Fk were used to describe the electrostatic interaction but now they are usually replaced by Racah parameters A, B, and C. The relations between these two kinds of parameters are:

1.3 Energy Levels of Free Transition-Metal Ions Table 1.3 Electronic conﬁgurations of iron group ions

13

Ion

q

Ti3+, V4+ V3+ V2+, Cr3+, Mn4+ Mn3+ Mn2+, Fe3+ Fe2+, Co3+ Co2+ Ni2+ Cu2+

1 2 3 4 5 6 7 8 9

A ¼ F0 49F4 B ¼ F2 5F4 C ¼ 35F4 The energies of the spectral terms of the conﬁgurations d2, d3, d4, and d5 can be expressed and some of them are listed in Table 1.4. Parameter A contributes the same energy to all the spectral terms in the same conﬁguration. Parameters B and C can be calculated by radial wave functions Rnl using some kinds of theoretical model or ﬁtted in comparison to experimental energy levels. The crystal ﬁeld energy is generally higher than that of the spin– orbital interaction for this group of ions and so the spin–orbital splitting should be calculated after the crystal ﬁeld energy calculation. Table 1.5 shows the experienced parameters of B, C, B/C, and spin–orbital coupling coefﬁcient. It can be seen from Table 1.5 that electron Coulomb interaction is indeed larger than that of the spin–orbital interaction for d electrons. Racah parameters for the same conﬁguration increased with atomic number due to the fact that the increasing of nuclear charge will cause decrease of the radius of d electron shell and ﬁnally result in a stronger electron Coulomb interaction. On the other hand, the spin– orbital coupling coefﬁcient of Cu2+ with atomic number 29 is about ﬁve times that of the Ti3+ with atomic number 22, and more than that it increases with Z4 as pointed out in Sect. 1.3. Table 1.4 Spectral term energy expression of 3dq conﬁguration [17] d2

d3

3

4

F = 3A−15B

3

4

P = 3A

1

G = A + 4B + 2C

2

H = 2P = 3A−6B + 3C

1

D = A − 3B + 2C

2

G = 3A − 11B + 3C

1

2

F = 3A + 9B + 3C

F = A−8B P = A + 7B

S = A + 14B + 7C

= 3A + 5B + 5C ± (193B2 + 8BC + 4C2)1/2 2D

(continued)

14

1 Energy Level of Free Ions

Table 1.4 (continued) d2

d3

4

d5

D = 6A − 21B

6

S = 10A − 35B

H = 6A − 17B + 4C

4

G = 10A − 25B + 5C

G = 6A − 12B + 4C

4

F = 10A − 13B + 7C

F = 6A − 5B + 5.5C ± 1.5(68B2 + 4BC + C2)1/2

4

D = 10A − 18B + 5C

3

D = 6A − 5B + 4C

4

P = 10A − 28B + 7C

3P = 6A − 5B + 5.5C ± 0.5(912B2 − 24BC + 9C2)1/2

2

I = 10A − 24B + 8C

d 5 3 3 3

I = 6A − 15B + 6C

1

2

H = 10A − 22B + 10C G = 10A − 13B + 8C

1G

= 6A − 5B + 3.5C ± 0.5(708B2 − 12BC + 9C2)1/2

2

1F

= 6A + 6C

2

G′ = 10A + 3B + 10C

1D

= 6A + 9B + 3.5C ± 1.5(144B2 + 8BC + C2)1/2

2

F = 10A − 9B + 8C

1S = 6A + 10B + 10C ± 2(193B2 + 8BC + 4C2)1/2

2

F′ = 10A − 25B + 10C

2

D′ = 10A−4B + 10C

= 10A−3B + 11C ± 3(57B2+ 2BC + C2)1/2

2D 2

P = 10A + 20B + 10C

2

S = 10A − 3B + 8C

Table 1.5 Racah parameters and spin–orbital coupling coefﬁcient for d electron (in unit of cm−1) [18] Ion (conﬁguration) Ti3+(3d1) V4+(3d1) Ti2+(3d2) V3+(3d2) Cr4+(3d2) V2+(3d3) Cr3+(3d3) Mn4+(3d3) Cr2+(3d4) Mn3+(3d4) Fe4+(3d4) Mn2+(3d5) Fe3+(3d5) Fe2+(3d6) Co3+(3d6) Co2+(3d7) Ni3+(3d7) Ni2+(3d8) Cu2+(3d9)

B

718 861 1039 766 918 1064 830 965 1144 960 1015 1058 1065 971 1115 1041 1238

C

B/C

2629 4165 4238 2855 3850

3.66 4.84 4.08 3.73 4.19

3430 3675 4459 3325 4800 3901 5120 4366 5450 4831 4659

4.13 3.81 3.90 3.46 4.73 3.69 4.81 4.50 4.89 4.64 3.76

n 154 248 121 209 327 167 273 402 230 352 514 347 410 533 649 829

1.4 Energy Levels of Free Rare Earth Ions

1.4

15

Energy Levels of Free Rare Earth Ions

Generally, lanthanide elements (from lanthanum Z = 57 to lutetium Z = 71), scandium (Z = 21), and yttrium (Z = 39) are referred to as rare earth elements. Except scandium and yttrium, they have similar electron shell structure, that is, the divalent and trivalent ions all have partially ﬁlled electron shell structure 4f q (q = 1–13). The 4f electrons of these elements are not in the outer shell but are shielded by the electron shell 5s25p6, so even in the host materials, their energy level structure and spectra have similar features compared to those of the free ions. From another point of view, it has been shown by photoelectron emission experiments that the position of 4f q states in trivalent rare earth compounds is lower than the top of their valence band by about 5 eV. So, for low 4f q energy levels, the free ion character can be well maintained. This property can also be explained by the energies of different interactions. The order of magnitude of electron Coulomb interaction is 104 cm−1, while the spin–orbital and crystal ﬁeld interactions are in the orders of 103 and 102 cm−1, respectively. Using the language of quantum mechanics, the wave functions of free rare earth ions are very good zero-order wave functions for the ions in materials. Therefore, having some knowledge about the free ion’s wave functions would be helpful for the further study of their spectroscopic properties in laser materials. In a good enough approximation, the principal quantum number n and the orbital angular momentum quantum number l can be still used to describe this multi-electron system, although the radial wave functions of the rare earth ions are different from those of hydrogen atom and the interaction between conﬁgurations cannot be neglected. In Table 1.6, 2S+1Ln represents that the spectral terms of 2S+1L appear n times. The J values corresponding to the different possible states are not shown in the table. They can be obtained from L and S as follows: J ¼ L S; L S þ 1; . . .; L þ S. For example, the spectral term 4D has S = 3/2, L = 2, and J can be: 1/2, 3/2, 5/2, 7/2, that is, giving rise to states 4 D1=2 ;4 D3=2 ;4 D5=2 ;4 D7=2 . When the number of electrons is large, quantum number LS are insufﬁcient to classify different spectral terms completely. Spectral terms with the same LS number can appear up to ten times. Therefore, in order to provide a full classiﬁcation of the states in fq conﬁguration, the group representation theory should be used. The continuous group, ﬁrst used by Racah, was introduced by Judd to classify the states of fq conﬁguration by a group chain of SUð2Þ Uð7Þ SUð2Þ SOð7Þ SUð2Þ G2 SUð2Þ SOð3Þ [4]. It is enough for readers to understand that in Table 1.7, [k1, k2, …] is another expression for the total spin quantum number S; on the other hand, (w1, w2, w3) and (u1, u2) are quantum numbers in

16

1 Energy Level of Free Ions

Table 1.6 Allowed spectral terms for f electrons f1, f13

2 1

f2, f12 f3, f11 f4, f10 f5, f9

1 1 1

f6, f8 f7

F

S , D1, 1G1, 1I1, 3P1, 3F1, 3H1

2 1 2

P , D2, 2F2, 2G2, 2H2, 2I1, 2K1, 2L1, 4S1, 4D1, 4F1, 4G1, 4I1

1 2 1

S , D4, 1F1, 1G4, 1H2, 1I3, 1K1, 1L2, 1N1, 3P3, 3D2, 3F4, 3G3, 3H4, 3I2, 3K2, 3L1, 3M1, S , D1, 5F1, 5G1, 5I1 2 4 2 5 2 7 2 6 2 7 2 5 2 5 2 3 2 2 2 1 2 1 4 1 4 2 4 3 4 4 4 4 4 3 4 3 P, D, F, G, H, I, K, L, M, N, O, S, P, D, F, G, H, I, 4 2 4 1 4 1 6 1 6 1 6 1 K, L, M, P, F, H 1 4 1 1 1 6 1 4 1 8 1 4 1 7 1 3 1 4 1 2 1 2 1 1 3 6 3 5 3 9 3 7 3 9 3 6 S, P, D, F, G, H, I, K, L, M, N, Q, P, D, F, G, H, I, 3 6 3 3 3 3 3 1 3 1 5 1 5 1 5 3 5 2 5 3 5 2 5 2 5 1 5 1 7 1 K, L, M, N, O, S, P, D, F, G, H, I, K, L, F 2 2 2 5 2 7 2 10 2 10 2 9 2 9 2 7 2 5 2 4 2 2 2 1 2 1 4 2 4 2 4 6 4 5 4 7 S, P, D, F , G , H, I, K, L, M, N, O, Q, S, P, D, F, G, 4 5 4 5 4 3 4 3 4 1 4 1 6 1 6 1 6 1 6 1 6 1 6 1 8 1 H, I, K, L, M, N, P, D, F, G, H, I, S 5 1 5

addition to the LS. With these quantum numbers, one can completely differentiate all states with the same LS quantum number. For more knowledge one can refer to books on theory of atomic spectroscopy [4, 6]. Table 1.7 contains the example for two rare earth conﬁgurations. Three coupling models have been mentioned in the previous discussion, but not the intermediate-coupling model. However, it should be pointed out that although in the ﬁrst-order approximation the LS coupling model can be used to deal with the energy level analysis of rare earth ions, the spin–orbital Hamiltonian cannot be neglected. The wave functions of LS coupling model were used as the ﬁrst-order approximation wave functions to calculate eigenvalues and eigenfunctions of the Hamiltonian H0 + Hs0. The eigenfunctions obtained in this way are called intermediate-coupling wave functions. Some of these wave functions, expressed as wave functions of LS coupling model for lower spectral terms in the rare earth ions in laser materials, are listed in Table 1.8. In this table, wð2S þ 1 LJ Þ refers to intermediate-coupling wave functions and uð2S þ 1 LJ Þ denotes the LS coupling wave functions. Some small terms have been neglected. It can be seen from Table 1.8 that in the intermediate-coupling wave functions the spin quantum number difference between the main wave functions and the mixed wave functions is DS ¼ 1. The reason is when the difference of spin quantum number between two wave functions is larger or smaller than 1, the matrix element of the spin–orbital interaction operator between them is equal to zero, so that there is no spin–orbital mixing. The matrix element of the spin–orbital interaction operator can be expressed by the formula (2–106) of Wyboune [7]. In Chap. 4, it will be shown that the transition between the two energy levels with different spin

1.4 Energy Levels of Free Rare Earth Ions

17

Table 1.7 Classiﬁcation of the spectral terms in f3 and f4 conﬁguration according to the reducing branching rule of the group chain SU ð2Þ U ð7Þ SU ð2Þ SOð7Þ SU ð2Þ G2 SU ð2Þ SOð3Þ Conﬁguration

SU(2) ⊗ U(7)

SU(2) ⊗ SO(7)

SU(2) ⊗ G2

SU(2) ⊗ SO(3)

f3(f11)

2

2

(1, 0, 0)

2

(1, 0)

2

F

2

2

(2, 1, 0)

2

(1, 1)

2

P, 2H

2

2

(2, 1, 0)

2

(2, 0)

2

D, 2G, 2I

2

2

D2, 2F, 2G, 2H, 2K, 2L

[2, 1] [2, 1] [2, 1]

(2, 1, 0)

2

(2, 1)

2

4

(1, 1, 1)

4

(0, 0)

4

S

4

4

(1, 1, 1)

4

(1, 0)

4

F

4

4

(1, 1, 1)

4

(2, 0)

4

D, 4G, 4I

1

1

(0, 0, 0)

1

(0, 0)

1

S

1

1

(2, 0, 0)

1

(2, 0)

1

D, 1G, 1I

(2, 2, 0)

1

(2, 0)

1

D, 1G, 1I

(2, 2, 0)

1

(2, 1)

1

D, 1F, 1G, 1H, 1K, 1L S, 1D, 1G, 1H, 1I, 1L, 1N

[2, 1]

4

3

[1 ] [13] [13]

f4(f10)

[22] [22]

1

2

1

1

2

1

1

2

1

[2 ] [2 ] [2 ]

3

2

[2, 1 ]

3

[2, 12]

3

2

[2, 1 ]

3

[2, 12]

(2, 2, 0)

1

(2, 2)

1

3

(1, 1, 0)

3

(1, 0)

3

F

3

(1, 1, 0)

3

(1, 1)

3

P, 3H

3

(2, 1, 1)

3

(1, 0)

3

F

3

(2, 1, 1)

3

(1, 1)

3

P, 3H

(2, 1, 1)

3

(2, 0)

3

D, 3G, 3I

(2, 1, 1)

3

(2, 1)

3

D, 3F, 3G, 3H, 3K, 3L P, 3F, 3G, 3H, 3I, 3K, 3M

3

2

3

3

2

3

3

2

3

[2, 1 ] [2, 1 ]

(2, 1, 1)

3

(3, 0)

3

5

(1, 1, 1)

5

(0, 0)

5

S

5

5

(1, 1, 1)

5

(1, 0)

5

F

5

5

(1, 1, 1)

5

(2, 0)

5

D, 5G, 5I

[2, 1 ]

5

4

[1 ] [14] [14]

quantum number is forbidden except due to the effect of intermediate coupling, the transition forbidden is partially released. However, for the so-called double-spin flip transition with DS ¼ 2, the forbidden rule is strictly established. Figure 1.1 shows that the radii of 5s and 5p shells are larger than that of 4f shell. However, the quantum defect D decreases with orbital angular momentum l, 5 Dð5sÞ\5 Dð5pÞ\4 Dð4f Þ; so that the energy of 4f electron is higher than those of 5s and 5p electrons and the electrons will ﬁrst ﬁll 5s and 5p shells and then the 4f shell. Therefore, the 4f electrons are in the inner shell with outer ﬁlled 5s and 5p shells to shield the interactions of the host materials. So for low 4fq energy levels, the free ion character can be maintained certainly. In a good enough approximation, the principal quantum number n and the orbital angular momentum quantum number l can be still used to describe this multi-electron system in the host materials, although the radial wave functions of the rare earth ions are different from those of hydrogen atom and the interaction between conﬁgurations cannot be neglected.

18

1 Energy Level of Free Ions

Table 1.8 Some of the intermediate-coupling wave functions of rare earth ions Ion Nd3+ [19]

Er3+ [20]

Ho3+ [21]

Tm3+ [20]

Intermediate-coupling wave functions w 4 I9=2 ¼ 0:9839u 4 I9=2 0:1672u ð210Þð21Þ2 H9=2 þ 0:0580u ð210Þð11Þ2 H9=2 w 4 I11=2 ¼ 0:9945u 4 I11=2 þ 0:0369u ð210Þð11Þ2 H11=2 0:0964u ð210Þð21Þ2 H11=2 w 4 I13=2 ¼ 0:9975u 4 I13=2 0:066u 2 K13=2 4 4 2 w I15=2 ¼ 0:9927u I15=2 þ 0:1201u K15=2 wð4 F3=2 Þ ¼ 0:9685uð4 F3=2 Þ 0:0563u 4 S3=2 þ 0:2268u ð210Þð20Þ2 D3=2 0:0622u 2 P3=2 0:0577u ð210Þð21Þ2 D3=2 w 4 I15=2 ¼ 0:9852u 4 I15=2 0:1708u 2 K15=2 4 4 2 w I13=2 ¼ 0:9955u I13=2 þ 0:0896u K13=2 w 4 I11=2 ¼ 0:9125u 4 I11=2 þ 0:1094uð4 G11=2 Þ þ 0:0631u 2 I11=2 þ 0:3740u ð210Þð21Þ2 H11=2 0:1073u ð210Þð11Þ2 H11=2 w 4 I9=2 ¼ 0:7322u 4 I9=2 þ 0:2765uðð210Þð20Þ2 G9=2 Þ 0:2204uðð210Þð21Þ2 G9=2 Þ þ 0:1953u ð210Þð11Þ2 H9=2 0:4125u ð210Þð21Þ2 H9=2 þ 0:3611uð4 F9=2 Þ w 4 S3=2 ¼ 0:8371u 4 S3=2 0:4196u 2 P3=2 0:2666u ð210Þð20Þ2 D3=2 þ 0:2237uð4 F3=2 Þ w 5 I8 ¼ 0:967u 5 I8 w 5 I7 ¼ 0:965u 5 I7 5 w I6 ¼ 0:976u 5 I6 w 5 I5 ¼ 0:952u 5 I5 5 5 w I4 ¼ 0:948u I4 w 5 S2 ¼ 0:841u 5 S2 þ 0:377u ð210Þð11Þ3 P2 w 5 F5 ¼ 0:896u 5 F5 0:315u ð211Þð21Þ3 P2 w 5 F4 ¼ 0:959u 5 F4 w 5 F3 ¼ 0:951u 5 F3 w 5 F2 ¼ 0:794u 5 F2 0:383u 5 S2 þ 0:345u ð211Þð21Þ3 D2 w 5 F1 ¼ 0:892u 5 F1 0:384u ð211Þð21Þ3 D1 wð3 P0 Þ ¼ 0:9718uð3 P0 Þ 0:2354uð1 S0 Þ wð 3 P 1 Þ ¼ uð 3 P 1 Þ wð3 P2 Þ ¼ 0:7693uð3 P2 Þ 0:1984uð3 F2 Þ 0:607uð1 D2 Þ wð1 S0 Þ ¼ 0:9718uð1 S0 Þ þ 0:2354uð3 P0 Þ wð3 F2 Þ ¼ 0:8769uð3 F2 Þ 0:1374uð3 P2 Þ 0:4606uð1 D2 Þ wð 3 F 3 Þ ¼ uð 3 F 3 Þ wð3 H4 Þ ¼ 0:5282uð3 F4 Þ þ 0:7713uð3 H4 Þ 0:3549uð1 G4 Þ wð3 F4 Þ ¼ 0:787uð3 F4 Þ 0:2883uð3 H4 Þ þ 0:5454uð1 G4 Þ wð3 H5 Þ ¼ uð3 H5 Þ wð3 H6 Þ ¼ 0:9956uð3 H6 Þ þ 0:0931uð1 I6 Þ wð1 D2 Þ ¼ 0:6473uð1 D2 Þ þ 0:623uð3 P2 Þ þ 0:4378uð3 F2 Þ

(continued)

1.4 Energy Levels of Free Rare Earth Ions Table 1.8 (continued) Ion

Intermediate-coupling wave functions wð1 G4 Þ ¼ 0:7594uð1 G4 Þ þ 0:5674uð3 H4 Þ 0:3182uð3 F4 Þ wð1 I6 Þ ¼ 0:9956uð1 I6 Þ 0:0931uð2 H6 Þ

Pr

3+

[20]

wð3 P0 Þ ¼ 0:996uð3 P0 Þ þ 0:0876uð1 S0 Þ wð 3 P 1 Þ ¼ uð 3 P 1 Þ wð3 P2 Þ ¼ 0:9592uð3 P2 Þ þ 0:2812uð1 D2 Þ wð3 F2 Þ ¼ 0:989uð3 F2 Þ þ 0:1475uð1 D2 Þ wð 3 F 3 Þ ¼ uð 3 F 3 Þ wð3 F4 Þ ¼ 0:8544uð3 F4 Þ þ 0:1035uð3 H4 Þ 0:5092uð1 G4 Þ wð3 H4 Þ ¼ 0:9878uð3 H4 Þ þ 0:1534uð1 G4 Þ wð3 H5 Þ ¼ uð3 H5 Þ wð3 H6 Þ ¼ 0:9985uð3 H6 Þ þ 0:0541uð1 I6 Þ wð1 S0 Þ ¼ 0:9962uð1 S0 Þ þ 0:0876uð3 P0 Þ wð1 D2 Þ ¼ 0:9483uð1 D2 Þ þ 0:2823uð3 P2 Þ þ 0:1452uð3 F2 Þ wð1 G4 Þ ¼ 0:8469uð1 G4 Þ 0:1167uð3 H4 Þ þ 0:5188uð3 F4 Þ wð1 I6 Þ ¼ 0:9956uð1 I6 Þ 0:0931uð3 H6 Þ

Fig. 1.1 Outer electron shell distribution of rare earth ions

19

20

1 Energy Level of Free Ions

The lower energy levels of 4f11 conﬁgurations of free Er3+ ion and this ion in ﬁve kinds of host crystals, including LaF3, are listed in Table 1.9. One can see from this table the differences of a given energy level for free Er3+ ion and that this ion in different crystals is generally less than 100 cm−1; only in few cases is about 200 cm−1. Therefore, in the discussion of an energy level position in different hosts, their position in LaF3 crystal can be seen as a good reference. Figure 1.2 shows the energy levels of 13 rare earth ions. This diagram has been frequently referred to in the literature. It can give us a general idea of the energy level positions for all the rare earth ions and help us in the analysis of an unknown spectrum and determines which energy levels are involved in the spectrum. From this diagram, if one considers the Gd3+ ion as a center, it can be seen that the Hund rule is really available and any spectral terms of a rare earth ion in the left hand position can be found in another rare earth ion in the corresponding right hand position. However, for the same spectral term 2S+1L, the lower 2S+1LJ levels in the left-hand side correspond to the higher 2S+1LJ levels in the corresponding right-hand side. It should also be noted that the energy separations between different spectral terms 2S+1L and different 2S+1 LJ levels in the same spectral term are larger for the rare earth ions in the right-hand side of Gd3+ ion. It is due to the fact that the Coulomb interaction between electrons and the spin–orbital interaction are stronger for the rare earth ions in the right-hand side, because of the effect of lanthanide contraction and the spin– orbital coupling coefﬁcient is greater for ions of larger atomic number. This tendency can be clearly seen from Fig. 1.3 which shows that the Slater parameter Fk and spin–orbital coupling coefﬁcient f increase with 4f electron number. In order to investigate the energy levels of rare earth ions, one should also know the separation between ground conﬁguration and excited conﬁgurations. This is because the excited conﬁgurations have important effects on the ground conﬁguration, which will be discussed in the following. Figure 1.4 is a schematic diagram Table 1.9 Level energies for the free Er3+ ion and that in ﬁve host crystals (unit of cm−1) Levels

Free ion [22]

LaF3 [22]

LaCl3 [23]

Cs3Lu2Cl9 [13]

Y2O3 [22]

Y3Al5O12 [24]

4

0 6,485 10,123 12,345 15,182 18,299 19,010 20,494 22,181 22,453 24,475 26,376 27,319

0 6,480 10,123 12,350 15,235 18,353 – 20,492 22,161 22,494 24,526 26,368 27,412

0 6,482 10,112 12,352 15,177 18,290 – 20,407 22,066 22,407 24,453 26,257 –

0 6,465 10,078 12,300 15,091 18,142 18,944 20,292 21,939 22,301 24,339 26,116 27,097

0 6,458 10,073 12,287 15,071 18,072 18,931 20,276 21,894 22,207 24,304 26,074 –

0 6,470 10,090 12,312 15,129 18,166 18,980 20,348 21,992 22,370 24,368 26,166 –

I15/2 I13/2 4 I11/2 4 I9/2 4 F9/2 4 S3/2 2 H11/2 4 F7/2 4 F5/2 4 F3/2 2 H9/2 4 G11/2 2 G9/2 4

1.4 Energy Levels of Free Rare Earth Ions

Ce3+

Pr3+

Nd3+

Pm3+

Sm3+

Eu3+

21

Gd3+

Tb3+

Dy3+

Ho3+

Er3+

Tm3+ Yb3+

Fig. 1.2 Energy levels of trivalent rare earth ions

for the separation between 4f electron and some of the excited shells of divalent and trivalent rare earth ions [8]. Figs. 1.5 and 1.6 are relations between two lowest conﬁgurations for the trivalent rare earth ions and divalent rare earth ions, respectively.

22 Fig. 1.3 Relation between Slater parameter Fk as well as spin-orbital coupling coefﬁcient f and the electron number determined by experiments on crystals of LaF3 and LaCl3 [16]

Fig. 1.4 Schematic diagrams for the separation between 4f electron and some of the excited shells of the divalent and trivalent rare earth ions [8]

1 Energy Level of Free Ions

1.4 Energy Levels of Free Rare Earth Ions

Fig. 1.5 Relation between two lowest conﬁgurations of the trivalent rare earth ions [8]

23

24

1 Energy Level of Free Ions

Fig. 1.6 Schematic diagrams for the separation between two lowest conﬁgurations of the divalent rare earth ions [8]

1.5

Theory of Interactions in Rare Earth Ions

By the end of this chapter, we would like to return to the subject of a series of interactions in rare earth ions and introduce their effects on the energy level positions. To investigate the energy levels of multi-electron system, a very good example is the application of continuous group in spectroscopy. In this ﬁeld, Racah in 1940s [9] and Judd in 1950s [6] have performed outstanding works. From the Hamiltonians used to describe the different interactions in the atoms and the wave functions classiﬁed by Lie group representations, by means of the tensor operator method established at that time, a series of interaction energies were calculated. We would like to introduce the parameter method that can describe all these interactions but not involving too much mathematics. The number of parameters introduced is the minimum necessary to describe all the interactions. For example, among the parameters tk used to describe conﬁguration interactions, the effect of t1 and t5 can be embodied by the electrostatic Coulomb interaction parameters and so they are omitted.

1.5 Theory of Interactions in Rare Earth Ions

25

As presented previously, Coulomb interaction and spin–orbit interaction can be taken into account by constructing intermediate-coupling wave functions. The other method generally adopted is to describe these two interactions by related parameters. The Coulomb interaction in (1.26) is considered individually as Hee ¼

n X

e2 4pe0 ri;j i [ j¼1

ð1:34Þ

By applying the following expanded expression k 1 4p X r\ ¼ Y ðkÞ ðhi ; ui ÞYqðkÞ hj ; uj k rij 2k þ 1 kq r [þ 1 q

ð1:35Þ

and CqðkÞ ð^r Þ

4p 2k þ 1

¼

1=2

YqðkÞ ðh; /Þ

for 4fq electronic conﬁguration, Hee becomes X

Hee ¼

F k fk ¼

X

Fk f k

ð1:36Þ

C ðkÞ ðiÞ C ðkÞ ðjÞjaLSi

ð1:37aÞ

k ¼ 0;2;4;6

k ¼ 0;2;4;6

where fk ¼ haLSj

X i[j

e2 F ¼ 2pe0

Z1 Z1

k

0

0

rk R24f ðri ÞR24f rj k \ dri drj r [þ 1

ð1:37bÞ

where Fk is called Slater parameter, and another parameter introduced by Condon and Shortley is Fk. The relations between them can be written as Fk ¼ Dk Fk

ð1:38Þ

where Dk are Condon-Shortley factors, for 4f electrons D0 ¼ 1; D2 ¼ 225; D4 ¼ 1089; D6 ¼ 184041=25 Coulomb interaction can also be described by Racah parameters E0, E1, E2, E3 and expressed as

26

1 Energy Level of Free Ions

Hee ¼

X

E k ek

ð1:39Þ

k¼0;1;2;3

The matrix elements of ek can be found in the well-known tables provided by Nielson and Koster [10], f k and ek have the following relations e0 ¼ f 0 ¼ qðq 1Þ 9 1 2 1 4 1 6 f þ f þ f e1 ¼ f 0 þ 7 42 77 462 143 2 130 4 35 6 f f þ f e2 ¼ 42 77 462 11 4 4 7 6 f f e3 ¼ f 2 þ 42 77 462

ð1:40Þ

where q is the number of electrons in the conﬁguration 4fq. The relations between Racah parameters and Slater parameters are E 0 ¼ F0 10F2 33F4 286F6 70F2 þ 231F4 þ 2002F6 E1 ¼ 9 F2 3F4 þ 7F6 2 E ¼ 9 5F þ 6F 2 4 91F6 E3 ¼ 3

ð1:41Þ

7E0 þ 9E 1 7 E1 þ 143E 2 þ 11E 3 F2 ¼ 42 E1 130E2 þ 4E 3 F4 ¼ 77 1 E þ 35E 2 7E 3 F6 ¼ 462

ð1:42Þ

or F0 ¼

The spin–orbital interaction of the whole atom system can then be obtained by simply summing (1.2) over all the electrons Hso ¼

n X

nðri Þli si

i¼1

Integrating over radial variable, it can be expressed as

ð1:43Þ

1.5 Theory of Interactions in Rare Earth Ions

27

Hso ¼ f4f Aso where f4f ¼

R1

ð1:44Þ

R24f ðrÞnðrÞdr. Aso is the angular operator of spin–orbit interaction

0

and can be expressed as pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ L þ S0 þ J Aso ðnlÞ ¼ ð1 Þ ð

2l þ 1Þðl þ 1ÞldJJ 0 dMM 0 D E L S J sLSV ð11Þ s0 L0 S0 0 0 S L 1 Reduced matrix elements of tensor operator V(11) can be found in [10]. Considering 4fq conﬁguration, the calculation of energy levels may have errors up to several hundreds of cm−1 compared with the experimental results, if only the above two interactions are included. The reason for this error is the Coulomb interaction between ground and excited conﬁgurations that has not been taken into account. This interaction can be divided into two kinds, that is, two-body and three-body interactions. Two-body interaction is written as Hcc1 ¼ aLðL þ 1Þ þ bGðG2 Þ þ cGðR7 Þ

ð1:45Þ

where a, b, c are ﬁtting parameters, G(G2) and G(R7) are Casimir operators for Lie group G2 and R7 with eigenvalues to be found from Tables 2.6 and 2.7 in [7]. The three-body interaction should be considered for conﬁgurations having three or more electrons and it has the following expression introduced by Judd [11] Hcc2 ¼

X

T i ti

ð1:46Þ

i

where i = 2, 3, 4, 6, 7, 8, Ti and ti are ﬁtting parameters and operators, respectively. The operators transformed according to the irreducible representations of group G2 and R7, also called three-body operators and can be found in [7]. Four-body or many-body interactions can be introduced in the same way, but without substantive effect on the energy level positions. Besides spin–orbital interaction expressed by fnl, the magnet interactions of spin–spin and the spin angular momentum with the orbital angular momentum of other electrons can be expressed as Hss þ soo ¼

X

M h mh

ð1:47Þ

h ¼ 0;2;4

where mh are effective operators and Mh are relative Marvin integral being written as follows

28

1 Energy Level of Free Ions

Mh ¼

a2 4

ZZ

rh R24f ðri ÞR24f rj h þi 3 dri drj rj ri [ rj

ð1:48Þ

In order to improve the ﬁtting of f electron spectroscopic data, it is necessary to introduce three two-body operators to take into account weaker electrostatic and spin–orbit-correlated interactions, expressed as Hcc3 ¼

X

ð1:49Þ

Pk pk

k ¼ 2;4;6

Pk are parameters while pk are two-electron operators depending on the spin angular momentum and can be found in [12]. Considering all the interactions introduced, the total Hamiltonian of the rare earth ions can be written as X X H¼ F k fk þ f4f Aso þ aLðL þ 1Þ þ bGðG2 Þ þ cGðR7 Þ þ T i ti k¼2;4;6

þ

X

k ¼ 2;4;6

P k pk þ

X

i¼2;3;4;6;7;8

M h mh

h ¼ 0;2;4

ð1:50Þ In this way, the E0, E1, E2, E3, (F0, F2, F4, F6); f; a, b, c; Ti (i = 2, 3, 4, 6, 7, 8); pk (k = 2, 4, 6); and mk (h = 0, 4, 6), 20 parameters can have a full description of the energy levels of free rare earth ions. It should be pointed out that compared to the electrostatic Coulomb interaction between electrons and the spin–orbit interaction, the conﬁguration and the relativistic magnetic interactions are much weaker. Moreover, we have Hcc1 [ Hcc2 [ Hcc3 Hss þ soo Among all the 20 parameters in (1.50), four parameters should be subjected to the Hartree-Fock restriction [13] M 0 ¼ 1:78M 2 ¼ 2:63M 4 P2 ¼ 1:33P4 ¼ 2P6 Therefore, there are only 16 independent parameters. After ﬁtting to the experimental energy level data, the values of these parameters for Er3+ ions in three crystal hosts are listed in Table 1.10. The relative parameters for Nd3+ in NdAl3 (BO3)4 (NAB) crystal can be found in [14]. It can be seen that these parameters are not only different for different host but are different for different sites in the same host. As pointed out by Marshall and Stuart [15], when a free ion placed in crystal (or liquid), its wave function will expand into crystal (or liquid). These kinds of expansion will produce the screen of 4f electron by the overlap electron cloud of 4f electron and its ligands, and ﬁnally

1.5 Theory of Interactions in Rare Earth Ions Table 1.10 Atomic parameters for Er3+ ions in three crystal hosts (units in cm−1)

29

Parameters

LaCl3 [22]

Cs3Lu2Cl9 [23]

Y3Al5O12 [13]

F2 F4 F6 f a b c T2 T3 T4 T6 T7 T8 P2 M0

98,260 69,793 48,114 2362 17.4 −638 2061 426 48 22 −305 289 353 416 4.2

97,940 69,850 49,850 2366 17.1 −647 1747 299 45 36 −312 213 352 539 4.2

99,333 70,581 49,207 2368 17.6 −612 1698 599 38 69 −362 323 505 478 3.6

result in the decrease of effective nuclear charge. Therefore, Slater parameters and spin–orbital coupling coefﬁcient ﬁtting by crystal spectral data will be less than those of free ions. These kinds of wave function expansion obviously will be different for different media so that the parameters ﬁtting by spectral data of different media have some difference. However, the difference of all the 16 parameters for different hosts in general is within a range of 1%. It is clearly shown in Table 1.10 that all the atomic parameters for rare earth ions in different hosts have nearly the same values. Fitting with so many parameters is complicated but the results after ﬁtting have not substantially improved, so for the practical problems of laser materials in which the gravity center of the spectral terms are non-essential, the atomic parameters can refer to those of other hosts and ﬁtting only the crystal parameters is enough.

References 1. G. Herzberg, Atomic Spectra and Atomic Structure (Dover Publication, New York, 1944) 2. E.U. Condon, G.H. Shortley, The Theory of Atomic Spectra (Cambridge University Press, New York, 1935) 3. J.C. Slater, Quantum Theory of Atomic Structure (McGraw-Hill Book Company, New York, 1960) 4. E.U. Condon, H. Odabasi, Atomic Structure (Cambridge University Press, London, 1980) 5. R.C. Powell, Physics of Solid-State Laser Materials (Springer, New York Inc, New York, 1998) 6. B.R. Judd, Operator Techniques in Atomic Spectroscopy (McGraw-Hill Book Company, New York, 1963)

30

1 Energy Level of Free Ions

7. B.G. Wybourne, Spectroscopic Properties of Rare Earths (Interscience Publishers, New York, 1965) 8. G.H. Dieke, Spectra and Energy Levels of Rare Earth Ions in Crystals (Interscience Publishers, New York, 1968) 9. G. Racah, Phys. Rev., 61, 186 (1942); 62, 438 (1942); 63, 367 (1943); 76, 1352 (1949) 10. C.W. Nielson, G.F. Koster, Spectroscopic Coefﬁcients for pn, dn and fn Conﬁgurations (MIT Press, Massachusetts, 1964) 11. B.R. Judd, Phys. Rev. 141, 4 (1966) 12. B.R. Judd, H.M. Crosswhite, H. Crosswhite, Phys. Rev. 169, 130 (1968) 13. S.R. Luthi, H.U. Gudel, H.U. Hehlen et al., Phys. Rev. B 57, 15229 (1998) 14. C. Cascales, C. Zaldo, U. Caldino, Garcia Sole J. Luo Z.D., J. Phys. Condens. Matter 13, 8071 (2001) 15. W. Marshall, R. Stuart, Phys. Rev. 123, 2048 (1961) 16. L. Guokui, J. Bernard (eds.), Spectroscopic of Rare Earths in Optical Materials (Springer, Berlin Heidelberg New York, 2005) 17. J.S. Grifﬁth, The Theory of Transition-Metal (Cambridge University Press, London, 1961) 18. B. Henderson, R.H. Bartram, Crystal-Field Engineering of Solid-State Laser Materials (Cambridge University Press, Cambridge, 2000) 19. B.G. Wybourne, J. Chem. Phys. 34, 279 (1961) 20. R. Pappalardo, J. Lumin. 14, 159 (1976) 21. K. Rajnak, W.F. Krupke, J. Chem. Phys. 46, 3532 (1967) 22. S. Hufner, Optical Spectra of Transparent Rare Earth Compounds (Academic Press, New York, 1978) 23. K.W. Kramer, H.U. Gudel, R.N. Schwartz, Phys. Rev. B 56, 13830 (1997) 24. J.B. Gruber, J.R. Quagliano, M.F. Reid et al., Phys. Rev. B 48, 15561 (1993)

Chapter 2

Group Theory and Quantum Theory

The electron–electron interaction, electron–nucleus interaction as well as the orbit– orbit, orbit–spin, spin–spin couplings, and the other complicate interactions of electrons in free ions have been discussed in Chap. 1. However, the whole system of the free ion containing all the electrons in it can be seen as a spherical symmetry system. This is due to the fact that the space of the free ion is isotropic in a good enough approximation. If the ion is placed in a solid material, this space isotropy will be generally destroyed by the interactions between the ions and the environment. The energy of the electrons in different states will be different because the interactions are different for different relative positions (relative distance or angle) between the electrons of ion studied and the lattice ions. This also means the elimination of energy level degeneracy of the free ions. It can be seen that the symmetry of the interactions plays a very important role in the determination of the electron energy states. Therefore, some knowledge of group theory and related quantum theory should be introduced before a detailed discussion of the electron energy level.

2.1

Mathematical Description of the Symmetry

Let us consider a simple cubic lattice; the ion distribution is shown in Fig. 2.1. In this special situation, the cube shown can represent the distribution of the ions in space. Therefore, one can ﬁnd out about the local symmetry of the crystal by investigating only the ion’s distribution in this cube. Obviously, if the cube is rotated around an axis passing through the centers of opposite faces, such as a axis, by 90°, 180°, or 270°, the distribution of the ions in the cube and in the whole lattice will not be changed. This is to say that a is one of the symmetry axis. Moreover, because the angle rotated around this axis is an integral multiple of 2p/4, it is called fourth-order axis and denoted by C4. Similarly, the b and c axes which pass through the centers of the other two sets of opposite faces are also fourth-order © Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8_2

31

32

2 Group Theory and Quantum Theory

g

Fig. 2.1 Distribution of ions in a simple cubic lattice

a

d

f

e c

b

axes. On the other hand, if the cube is rotated 120° or 240° around the axes passing through the opposite corners of the cube, that is, axes d, e, f, and g then the ion’s distribution has no variation. It is to say that d, e, f, and g are third-order axes and denoted by C3. In the same way, six axes passing through the midpoints of opposite edges of the cube are second-order axes and denoted by C2. It means that the conﬁguration will not be changed by the rotation of 180°. Besides, the inversion through the center of the cube and the reflection on the planes rh perpendicular to the fourth-order axes or rv passing through each pair of opposite edges are also symmetry elements of the cube. It should be noted that most of symmetry axes and symmetry planes include not only one symmetry element. For example, the three fourth-order axes include rotations of 90°, 180°, and 270°, that is, nine symmetry elements C4(3), C42 ð3Þ, and C43 ð3Þ. Similarly, four third-order axes include eight symmetry elements C3(4) and C32 ð4Þ coming from rotations of 120° and 240°, respectively. The ﬁgures inside the brackets indicate the number of symmetry elements. On the other hand, the combination (product) of two symmetry elements will generate a new symmetry element. For example, the combination of fourth-order axes and the symmetry planes generate fourth-order rotation–reflection axes S4(6), and the combination of third-order axes and the symmetry planes generate eight sixth-order rotation–reflection axes S6(8). Therefore, including the identity element E, there are all together 48 symmetry elements divided into ten classes in this symmetry group: E; C2 ð6Þ; C3 ; C32 ð8Þ; C4 ; C43 ð6Þ; C42 ð3Þ; I; rv ð6Þ; rh ð3Þ; S6 ; S56 ð8Þ; S4 ; S34 ð6Þ It can be found that a symmetry element in one class can be transformed into a symmetry element in the same class by combining with some symmetry element in other class. For example, eight symmetry elements C3 and C32 can be transformed into each other by C4 and C2, as well as C4 and C43 can be transformed into each other by C2. On the other hand, C4 axes with different orientations can be

2.1 Mathematical Description of the Symmetry

33

transformed into each other by C3 and so on. The symmetry axes in the same class rotate with the same angle; the difference is only the orientation of axes. Therefore, one can say that the symmetry elements in the same class are equivalent. We will see it more clearly later and ﬁnd that any two successive transformations always can be replaced by one single transformation and any transformation always has a corresponding inverse transformation. In mathematical language, these 48 elements constitute a symmetry group denoted by Oh. The group theory is a mathematical tool to investigate the symmetry of a system and the effects of this symmetry on the characteristics of the system. Almost all the characteristics of the micro-systems have very close relations with its symmetry and so group theory is a powerful tool in dealing with these problems. This is the main reason why we will introduce the basic knowledge of group theory in the following.

2.2

Basic Conception of the Group

By considering every symmetry element as an element of a group, from the example given above, one can see that the elements of a group have the following properties: (1) The product of any two elements, which is deﬁned as two successive transformations, is also an element of the group. (2) Each group includes an identity element E which satisﬁes (AE) = (EA) for any element A in the group. (3) For any element A in the group, there is an inverse element A−1 in the same group satisfying AA−1 = E. (4) For the multiplication of elements, the associative law is valid AðBC Þ ¼ ðABÞC. The last property cannot be directly seen from the example given. This is because the multiplication table of those group elements still has not been given. It is complicate to make the multiplication table for such a group of 48 elements. However, we can discuss it by using a simple example related to the symmetry elements of a regular triangle. These symmetry elements constitute a group denoted by C3v. From Fig. 2.2, it can be seen that this group has the following elements: (1) Unit operation (identity transformation) E; (2) Clockwise rotation through 120° around z-axis: C3; (3) Counter-clockwise rotation through 120° or clockwise rotations through 240° around z-axis: C32 ; (4) Reflection about plane Z1: r1; (5) Reflection about plane Z2: r2; (6) Reflection about plane Z3: r3. It is easy to see that these elements satisfy multiplication table (Table 2.1). It can be seen from this table that the association law ðC3 r1 Þr2 ¼ r3 r2 ¼ C32 ¼ C3 ðr1 r2 Þ is satisﬁed. On the other hand, r1r2 = C3, but r2 r1 ¼ C32 , so the product is different for different orders of the multiplication. The elements r1 and r2 are said to be non-commutative. If all the elements of a group are commutative, then the group is called Abelian.

34

2 Group Theory and Quantum Theory

Fig. 2.2 Symmetry elements in a regular triangle

Table 2.1 Multiplication table of C3v group

E

C3

C32

r1

r2

r3

E

E

C3

C32

r1

r2

r3

C3

C3

E

r3

r1

r2

C32 r1

C32 r1

C32 E

C3

r2

r3

r1

r2

r3

E

C3

r2

r2

r3

r1

C32

E

C32 C3

r3

r3

r1

r2

C3

C32

E

One can introduce the concept of the class by investigating this simple group. By applying the above multiplication table, one has: 1 1 C31 ¼ C32 ; ðC32 Þ1 ¼ C3 ; r1 1 ¼ r1 ; r2 ¼ r2 ; r3 ¼ r3

and so 1 2 1 EC3 E ¼ C3 ; C31 C3 C3 ¼ C3 ; C32 C3 C32 ¼ C3 ; r1 1 C3 r1 ¼ C3 ; r2 C3 r2 2 1 2 ¼ C3 ; r3 C3 r3 ¼ C3 ; Similarly, when A in G-1AG is replaced by C32 , G being all the elements in the group, the results obtained are still C3 and C32 . G-1AG is called the conjugate of A. According to the deﬁnition of group theory, if some elements in a group are conjugate to each other, then these elements form a class in the group. Obviously, C3 and C32 form a class in the group C3v. It can also be shown that r1, r2, and r3 form another class. If two symmetry operations belong to the same class, then one operation is replaced by the other in a new coordinate system. For example, in the case considered, one can rotate the triangle counter-clockwise of 120°; then the operation r1 in the rotated system is equal to the operation r2 in the old system. Any group can be decomposed into non-overlapping classes, which cover all the elements of the group. For an Abelian group, G-1AG = AG-1G = A, and so each of the group element forms a class. We would like to introduce here the concept of order. The number of elements in a group is the order of the group. If an element A in the group has relation An = E,

2.2 Basic Conception of the Group

35

then n is called the order of element A. When B and A are in the same class, then we have: n Bn ¼ G1 AG ¼ G1 AGG1 AGG1 . . .G ¼ G1 An G ¼ G1 EG ¼ G1 G ¼ E It means that the elements in the same class have the same order. Another important concept in the group theory is the subgroup. If one set of the elements H of a group G has all the four properties of the group mentioned above, then H is a subgroup of the group G. For example, suppose E, C3, C32 is a subgroup of group C3v, then all the products and the inverse of these elements are in the subgroup. Note that C33 ¼ E and so all the elements in the subgroup can be expressed as some integer power of one element of this subgroup. If all the elements in a group are integer power of a given element, then this group is cyclic. Therefore, the above-mentioned subgroup is a cyclic group with order 3. Group C3v has ﬁve subgroups as follows: fEg; fE; r1 g; fE; r2 g; fE; r3 g; E; C3 ; C32 It is useful to point out without proof that if the order of a group is a prime number, then this group is a cyclic group. The order of subgroup {E, C3, C32 } is 3, so that it is a cyclic group. If the subgroup H in the group G is self-conjugated to any element g in group G, that is, g−1H g = H, then subgroup H is called an invariant subgroup of the group G. The subgroup {E, C3, C32 } satisﬁes this condition and is an invariant subgroup of the group C3v. Factor group is another important concept in the group theory. In order to introduce this concept, it is necessary to mention about coset. If H is a subgroup of a group G, then from an element g in G but not in H, one can form a set of elements as follows gH ¼ fgha jha 2 H g It is deﬁned as the left coset of H. The right coset of H can be formed similarly Hg ¼ fha gjha 2 H g Obviously, if H is an invariant subgroup, then the left coset should be equal to the right coset and it is not necessary to distinguish between the left and the right coset. In this case, if one considers H as an element of the group, then all the cosets of H are also the elements of the group. The new group formed in this way is called a factor group and denoted by G/H. For example, for invariant subgroup H ¼ fE; C3 ; C32 g in C3v, H and {r1, r2, r3} constitute a factor group of order two.

36

2.3

2 Group Theory and Quantum Theory

Theory of Group Representations

The representation of a group is a method to embody the concept of the group elements. It relates the abstract group elements to the concrete symmetry operations and is an important way for the application of the group theory to spectroscopy. Abstractly, if any set of elements can be in correspondence with the elements of the group and if the same multiplication table can be applied, then this set of elements is a representation of the group. There are two kinds of correspondence in group theory, one is homomorphism, and the other is isomorphism. If the set of elements G′ and the set of elements G (a group) have the same multiplication table and the following correspondence relation: A ! A01 ; A02 . . .A0i ; B ! B01 ; B02 . . .B0i ; AB ! A01 B01 ; A02 B02 ; . . .; A0i B0i where A, B,… are elements of G and A01 ; B01 ; A02 ; B02 ; . . . are elements of G′, then G is said to be homomorphism to G′. If there is a one-to-one correspondence, then G is said to be isomorphism to G′. Obviously, isomorphism is also homomorphism, but homomorphism is not necessarily isomorphism. Two isomorphic groups have completely the same structure and have not any difference from the point of view of group theory. The aforementioned symmetry elements of a regular triangle and the following matrices are two isomorphic groups. E, r3 ¼

p12ﬃﬃ 23

1 0

0 1 0 1 ; r1 , ; r2 ¼ pﬃﬃ32 1 0 1 2 pﬃﬃ

23 1 2

p12ﬃﬃ ; C3 ¼ 23

pﬃﬃ 3 2 1 2

; C32 ¼

pﬃﬃ 3 2 1 2 1 pﬃﬃ2 3 2

; pﬃﬃ

23 12

It is a general way to use matrices in the linear space to represent a group. The transformations in the n-dimensional space Vn form a group designated by G. If one chooses a set of base functions for Vn, then each transformation will be represented by an n n matrix. The set of matrices representing the linear transformation will form a matrix representation of G and the base functions are said to form the bases of the representation. The matrix representation of G: M(A), M(B), M(C), … have a one-to-one correspondence with elements A, B, C, … of G and they are multiplied according to the same multiplication table AB ¼ C ! MðAÞMðBÞ ¼ MðCÞ;

AA1 ¼ E ! MðAÞMðAÞ1 ¼ MðEÞ

The representation matrices depend, in general, on the bases chosen for Vn. From linear algebra one knows that the matrices are transformed according to M 0 ðBÞ ¼ S1 M ðBÞSM 0 ð AÞ ¼ S1 M ð AÞS, and so on, when the bases transform by S. These kinds of transformations are deﬁned as similarity transformation. It is easy to show that M′ also forms a representation of the group G

2.3 Theory of Group Representations

37

M 0 ðAÞM 0 ðBÞ ¼ S1 MðAÞSS1 MðBÞS ¼ S1 MðAÞMðBÞS ¼ S1 MðABÞS ¼ M 0 ðABÞ Two representations which differ only by a similarity transformation are said to be equivalent. It should be pointed out that many linear transformations in physics keep the inner product of two vectors invariant. It is to say that for any two vectors x and y, the following equation is always valid: ðMx; MyÞ ¼ ðx; yÞ This transformation M is a unitary transformation and the transformation matrix of the unitary matrix satisﬁes M þ M ¼ MM þ ¼ 1 where M+ is transposed complex conjugate of matrix M. It can be shown [1] that for a ﬁnite group, every representation is equivalent to a unitary representation. If a matrix M can be expressed as M1 ðRÞ 0 MðRÞ ¼ ð2:1Þ 0 M2 ðRÞ and it is also written as MðRÞ ¼ M1 ðRÞ M2 ðRÞ

ð2:2Þ

then the matrix M is said to be reducible representation. In some cases, M1(R) and M2(R) can still be written into above direct summation further. When the matrix M cannot be reduced, then it is said to be an irreducible representation. A series of properties of the irreducible representation are very important in the application of group theory. Some orthogonal relations are given here without proof. If Ma(R) and Mb(R) are two irreducible representations for the group G, then their matrix elements have the following relation X R

Ma ðRÞik Mb ðRÞlj ¼

go dab dil dkj na

ð2:3Þ

where go is the order of group G and na is the dimension of irreducible representation. If irreducible representation a is non-equivalent to irreducible representation b, then dab = 0. Equation (2.3) can be introduced by Shur lemma [1, 2]. Matrices of an irreducible representation are dependent on the choice of basis. However, the summation of diagonal matrix elements—the trace of the matrix (called the character of irreducible representation in group theory)—is independent of P the basis chosen. It is easy to show in mathematics that the character vðRÞ ¼ i M ð RÞii does not change in the transformation of the coordinate. If

38

2 Group Theory and Quantum Theory

M 0 ðRÞ ¼ S1 MðRÞS then v0 ðRÞ ¼ ¼

X i X mn

X X ðS1 MSÞii ¼ ðS1 Þim Mmn Sni ¼ ðSS1 Þnm Mmn mn i imn X ¼ Mmm ¼ vðRÞ

M 0 ðRÞii ¼ dmn Mmn

X

m

Obviously, any two elements A and B in the same class can be written as A = S−1BS, and so the group elements in the same class have the same character. Two non-equivalent irreducible representations have different characters. Let k = i and l = j, then (2.3) becomes X

Ma ðRÞii Mb ðRÞjj ¼

R

go dab dij na

ð2:4Þ

Summing over i and j in the above equation, then X

va ðRÞ vb ðRÞ ¼ go dab

ð2:5Þ

R

Owing to the fact that the characters of the elements belonging to the same class are the same, if there are hi elements in a class Ci, then the summation over the elements of the group can be changed to the summation over the classes of the group. If there are r classes in the group, then r X

hi va ðCi Þ vb ðCi Þ ¼ go dab

ð2:6Þ

i¼1

By using orthogonal relation (2.5), one can obtain the number of times li that a particular irreducible representation appears in any reducible representation. One has vðRÞ ¼

X

li vi ðRÞ

i

and li ¼

1X vðRÞ vi ðRÞ go R

In addition, if a representation is irreducible, then

ð2:7Þ

2.3 Theory of Group Representations

X

39

vðRÞ vðRÞ ¼ go

R

because X

vðRÞ vðRÞ ¼

R

X

li vi ðRÞlj vj ðRÞ ¼ go

Rij

X

li lj dij ¼ go

ij

X

l2i

i

If the representation is irreducible, then v(R) cannot be decomposed into a sum of P several terms, that is, the only solution is l1 = 1, and so i l2i ¼ 1. By means of (2.3) and (2.6), the following two important properties of irreducible representation can also be introduced: (a) The sum of the squares of the dimensions of all irreducible representations is equal to the order of the group. (b) The number of different irreducible representations is equal to the number of classes in the group. The ﬁrst property can be shown by (2.3). Suppose Ma(R)ik forms a go-dimensional vector (the group element R has go elements, it constitutes a go-dimensional space). This vector is orthogonal, according to (2.3), to all other go-dimensional vectors formed by Ma(R)lj. There are n2a such orthogonal vectors. Besides, there are n2b and n2c vectors formed by Mb(R) and Mc(R), respectively, and all these vectors are P 2 orthogonal to each other. The total number of orthogonal vectors is ni and it is i

obviously equal to g0, and so X

n2i ¼ g0

i

The second property can be demonstrated by rewriting (2.6) as r X i¼1

where va ðCi Þ

va ðCi Þ

1=2 1=2 hi hi vb ðCi Þ ¼ dab g0 g0

ð2:8Þ

1=2 hi g0

can be considered as an r-dimensional vector (there are r

classes in the group). Equation (2.8) means that the vectors formed by nonequivalent irreducible representations are orthogonal. If the number of non-equivalent irreducible representations is n, then n = r, because the orthogonal vector in an r-dimensional space is r. These two properties are very useful in determining the character table of irreducible representations.

40

2.4

2 Group Theory and Quantum Theory

Direct Product Group and Direct Product Representation

One way to construct a complicate group from simple groups is to form a product group. If one has two groups G1 and G2 G1 ¼ E1 ; A1 ; B1 ; C1 . . . G2 ¼ E2 ; A2 ; B2 ; C2 . . . then all the products R1R2 between the elements of the two groups are commutative R1 R2 ¼ R2 R1 If R1 and R2 are represented by matrix M(R1) and matrix M(R2), respectively, then the direct product G1 ⊗ G2 is represented by matrices M(R1) ⊗ M(R2) with g1g2 g1g2 elements. Obviously, their characters have the following relation vðG1 G2 Þ ¼ vðG1 Þ vðG2 Þ

ð2:9Þ

As an example to construct a complex group from simple groups, we will discuss the construction of D3h from D3 and C1h. The group C1h contains only a unit element and a symmetry plane, while the group D3 includes a unit element, a third-order axis, and a second-order axis perpendicular to the third-order axis. Another two second-order axes will be generated by the third-order axis. Their characters tables are Tables 2.2, 2.3. The characters table of D3h = D3 ⊗ C1h is (Table 2.4). Similarly, other groups can also be formed by direct product, such as C4h ¼ C4 Ci ; C6h ¼ C6 Ci , S6 ¼ C3 Ci ; D3d ¼ D3 Ci , D2h ¼ D2 Ci ; D4h ¼ D4 Ci , D6h ¼ D6 Ci ; Oh ¼ O Ci ; Th ¼ T Ci . The direct product representation for a group can be formed from two different irreducible representations of the same group. The character of the direct product representation can be easily shown as the product of two characters of the related irreducible representations, that is vðcÞ ¼ vða bÞ ¼ vðaÞ vðbÞ

ð2:10Þ

This direct product representation is generally reducible and the numbers of irreducible representation contained can be calculated by the above-mentioned Table 2.2 Characters table of C1h group

C1h

E

rh

A′ A″

1 1

1 −1

2.4 Direct Product Group and Direct Product Representation

41

Table 2.3 Characters table of D3 group D3

E

2C3

3C2′

A1 A2 E

1 1 2

1 1 −1

1 −1 0

Table 2.4 Characters table of D3h group D3h = D3 ⊗ C1h

E

rh

2C3

2S3 (rh)C3

3C20

3rv ðrh C20 Þ

A01 ðA0 A1 Þ A02 ðA0 A2 Þ A001 ðA00 A1 Þ A002 ðA00 A2 Þ 0 0

1 1 1 1 2 2

1 1 −1 −1 2 −2

1 1 1 1 −1 −1

1 1 −1 −1 −1 1

1 −1 1 −1 0 0

1 −1 −1 1 0 0

E ðA EÞ E 00 ðA00 EÞ

orthogonal relations. If one uses Cabc to express the number of c irreducible representation contained in the direct product representation a ⊗ b, then Cabc ¼

1X v ðRÞ va ðRÞvb ðRÞ g0 R c

ð2:11Þ

To investigate the properties of a quantum system, the wave functions of the system are always expressed as products of those of the subsystems. For example, electronic wave function is a product of orbital wave functions and spin wave functions, and multi-electron wave function is a product of single-electron wave functions. A representation for a system can be expressed as a product of those of its subsystems. If the ﬁrst function belongs to representation a and the second one belongs to representation b, then the product function belongs to the representation a ⊗ b. In the application of group theory, we often express the direct product wave function as a linear combination of wave functions belonging to different irreducible representations. For this purpose we use the Clebsch-Gordan coefﬁcients (C-G coefﬁcients) as the combination coefﬁcients. They will be discussed in detail later.

2.5 2.5.1

Sketches of the Group in Spectroscopy Finite Group

Finite group is the group with ﬁnite number of elements; among this, the point group and the space group are most frequently used in physics.

42

2 Group Theory and Quantum Theory

1. Point group and space group Point groups have been mentioned many times in the above discussion, which is a symmetry group of ﬁnite bodies having at least one point ﬁxed. In crystal, point group is the set of symmetry elements of lattice points and will be discussed in a separate section. Space group is the symmetry group of conﬁguration in space. Crystallographic space group includes all the symmetry elements in crystal and can describe the symmetry of whole crystal lattice. Symmetry elements of space group can be expressed by {a|n}, where {e|0} is identity element and {a|0} is symmetry operation for some ﬁxed point, that is, the symmetry operation of point group while {e|n} is symmetry operation of pure translation group. Multiplication is deﬁned as fajngfbjn0 g ¼ fabjan0 þ ng, and the inverse element is fajng1 fa1 j a1 ng, owing to the fact that fajngfajng1 ¼ fajngfa1 j a1 ng ¼ faa1 j aa1 n þ ng ¼ fej0g. It can be easily demonstrated that the associative law of multiplication is also valid and the four criteria of groups are all satisﬁed. Because of the limit of lattice translation symmetry, the point group {a|0} in crystal can only be one of 32 kinds of point group, and conversely, by the limit of {a|0}, {e|n} should belong to one of 14 kinds of Bravias lattice. The 32 point groups combine with 14 Bravias lattices and form 230 space groups, which include 73 symmorphic space groups and 157 non-symmorphic space groups and can be divided into seven crystallographic systems. The symmorphic space groups are composed of all the symmetry elements of one translation group and one point group, while the non-symmorphic space groups include screw axis (a rotation through an angle u about symmetry axis followed by a fractional lattice vector translation along this axis) and glide reflection plane (a plane reflection followed by a fractional lattice vector translation parallel to this plane). The translation lattice vector may not necessarily be a Bravias lattice vector. The point groups, Bravias lattices, and the number of space group for seven crystallographic systems are listed in Table 2.5. It should be noted that a crystal belonging to a certain space group of a certain crystallographic system does not mean that all the lattice points have the point symmetry belonging to that crystallographic systems. For example, the laser 3+ crystal YAG (Y3Al5O12) belongs to space group Ia3d (O10 h ), but the trivalent Y 3+ ions occupy site A with point symmetry of D2, and the trivalent Al ions occupy two kinds of sites. Among these the site B has point symmetry of S6 and the site C has point symmetry of S4, but the point symmetry of divalent anion O2− is S2. The possible lattice point symmetry of the entire space group can be found in books or data compilation of crystallography. Space group is an important theoretical tool for crystallography and solid-state physics, especially the band theory of the solid and lattice vibration spectroscopy. This book is mainly concerned with the energy levels of local optical centers and transition between these energy levels; therefore, the knowledge of space group has only a brief introduction.

2.5 Sketches of the Group in Spectroscopy

43

Table 2.5 Point groups, Bravias lattices, and number of space group for seven crystallographic systems Crystal system

Point group

Bravias lattice

Number of space group

Triclinic Monoclinic

C1, S2 C2, C1h, C2h

Simple triclinic Simple and end-centered monoclinic

Orthorhombic

D2, C2v, D2h

Tetragonal

C4, S4, C4h, D4, C4v, D2d, D4h

Simple, end-centered, body-centered, and face-centered orthorhombic Simple and body-centered tetragonal

Trigonal

C3, S6, D3, C3v, D3d

Simple trigonal

Hexagonal

C6, C3h, C6h, D6, C6v, D3h, D6h

Simple hexagonal

Cubic

T, Th, O, Td, Oh

Simple, body-centered and face-centered cubic

Symmorphic 2 Symmorphic 6, non-symmorphic 7 Symmorphic 13, non-symmorphic 46 Symmorphic 16, non-symmorphic 52 Symmorphic 13, non-symmorphic 12 Symmorphic 8, non-symmorphic 19 Symmorphic 15, non-symmorphic 21

2.5.2

Permutation Group

Permutation symmetry is the symmetry of quantum system consisting of identical particles. For example, in the 3dq and 4fq conﬁguration of transition-metal ion and rare earth ion, the q electrons in these systems have permutation symmetry. Therefore, the permutation group has important application in the spectroscopy of these ions. Permutation group with n elements is usually denoted by Sn. In order to differentiate from symbol of relate point group, the symbol of permutation group is adopted as follows Pn ¼

1 a1

... ...

2 a2

n an

where Pn denotes the permutation of 1 by a1, 2 by a2…, n by an. The order of two permutation product PP′ is deﬁned from the right to the left, for example

1 2

2 1

3 3

1 2

2 3

3 1

¼

1 1

2 3

3 2

44

2 Group Theory and Quantum Theory

and the product of P′P is

1 2

2 3

3 1

1 2

2 1

3 3

1 3

¼

2 2

3 1

This result shows that the permutation does not satisfy the commutative law but it is easy to show that the associative law is valid and other requirements of group are all satisﬁed. The identity element is Pð0Þ n ¼

a1 a1

a2 a2

. . . an . . . an

b1 a1

b2 a2

... ...

a2 b2

. . . an . . . bn

If Pn ¼

bn an

then the inverse element will be P1 n

¼

a1 b1

because the P1 n satisﬁes the following expression Pn P1 n

¼

b1 a1

b2 a2

¼ Pð0Þ n

. . . bn . . . an

a1 b1

... ...

a2 b2

an bn

¼

a1 a1

a2 a2

... ...

an an

The group element number of permutation Pn is n!, that is, the order of group Pn is n! Any permutation can be resolved into cycles which affect only a smaller ﬁxed number of elements; for example, a P8 can be resolved as follows

1 2 2 3

3 1

4 5

5 6 4 7

7 6

8 8

¼ ð123Þð45Þð67Þð8Þ

The cycles in the right-hand side of the above expression have no common symbols. Permutations with same cycle structure belong to the same class of the group. Cycle structure can be written as ðmÞ ¼ ð1m1 ; 2m2 ; . . .; nmn Þ It expresses that the cycle structure of permutation has m1 1-cycle (unchanged), m2 2-cycles (transposition), …, mn n-cycles. The length of all the cycles satisﬁes

2.5 Sketches of the Group in Spectroscopy n X

45

imi ¼ n

i¼1

The number of permutation group Pn with cycle structure (m) can be expressed as NðmÞ ¼

n! 1m1 m1 !2m2 m2 !. . .nmn mn !

For example, the 4-symbol permutation group P4 can be divided into ﬁve classes and have altogether 4! = 24 elements: ð0Þ

1. Identity element P4 ¼ ð1Þð2Þð3Þð4Þ—NðmÞ ¼ 14! 4 4! ¼ 1 2. (123)(4), (132)(4), (124)(3), (142)(3), (134)(2), (143)(2), (234)(1), (243)(1) 4! —NðmÞ ¼ 11 1!3 1 1! ¼ 8 3. (12)(34), (13)(24), (14)(23)—NðmÞ ¼ 24! 2 2! ¼ 3 4. (12)(3)(4), (13)(2)(4), (14)(2)(3), (23)(1)(4), (24)(1)(3), (34)(1)(2) 4! —NðmÞ ¼ 12 12 1 2! ¼ 6 5. (1234), (1243), (1324), (1324), (1423), (1432)—NðmÞ ¼ 44! 1 1! ¼ 6 The class of Pn can generally be expressed by using partition [k] = [k1k1…kn], where k1 ¼ v 1 þ v 2 þ þ v n k2 ¼ v 2 þ v 3 þ þ v n . . .. . .. . .. . .. . .. . .. . . k n ¼ mn Because mi is a positive number, so k1 k2 kn 0, and also k1 þ k2 þ þ kn ¼ n. The possible class number of Pn is determined by the number of partition. Group theory uses Young diagrams to express partition ½k ¼ ½k1 k1 . . .kn , where there are k1 cells in the ﬁrst row and k2 cells in the second row, and so on. For example, for S4, its ﬁrst class can be written as [1111] = [14], the second class [31], the third class [22] [22], the fourth class [211] [212], and the ﬁfth class [4]. Their Young diagrams shown follow from left to right for the ﬁrst to ﬁfth class. It should be pointed out that there is a requirement that no lower row can be longer than upper row.

When the symbols of 1, 2, 3, 4 are placed into the Young diagram, one can obtain a table called Young tableau. If the numbers in a Young tableau are arranged

46

2 Group Theory and Quantum Theory

so that they increase from left to right and from top to bottom, the tableau is called a standard Young tableau. For example, the partition [212] has three standard Young tableaux as follows

1

2

1

3

1

3

2

2

4

4

3

4

It can be demonstrated that the number of standard Young tableau can be generated from a given Young diagram which is equal to the dimensions of the corresponding irreducible representation. For example, the dimension of partition [212] is 3 due to the fact that it has the above three standard Young tableaux. The method of using Young tableau to introduce the characters of irreducible representation can be referred from the books of group theory [1]. By Cayley theorem, any n order group isomorphism with one subgroup of permutation group Pn and the irreducible representation of unitary group U(n) and special unitary group SU(n), which have important application in physics, can be obtained by using irreducible representation of Pn. Therefore, permutation group is very important not only in mathematics but also in physics.

2.5.3

Continuous Groups

The groups in which elements can be labeled by continuously varying parameters are called as continuous groups. They have inﬁnite elements. It can be found in linear algebra that n dimension vector can be transformed by the following relation y ¼ Ax;

z¼By

) z ¼ Cx;

C ¼ BA

where A, B, and C are matrices of n line and n row. It is easy to show that the transformation matrices form a group due to the fact that the unit matrix I corresponds to the identity element, the product of two transformation matrices is in this matrix set, and the transformation of vector y into vector x satisﬁes the inverse transformation relation A−1A = I, as well as the associative law of multiplication is valid. Rotation group SO(3) which transforms one vector into another vector in three-dimensional space is the simplest example, in which the rotation angle is expressed as Euler angle. a, b, c obviously can be continuously varied, that is, it has inﬁnite number. If the angle parameters of matrix A are a, b, c, matrix B are a1, b1, c1, and matrix C are a2, b2, c2, then the angle parameters of matrix C can be expressed by those of matrices A and B; for example,

2.5 Sketches of the Group in Spectroscopy

47

sinb2 ¼ sinbcosa1 cosb1 þ cosbðcoscsinb1 sincsina1 cosb1 Þ Continuous groups commonly used in spectroscopy are: Groups of U(n) and SU(n)—n n unitary matrix set constitutes the n dimension unitary group U(n), where the condition of a matrix A to be a unitary will be X X A þ A¼I; i:e:ðA þ AÞij ¼ ðA þ Þik Akj ¼ Aki Akj ¼ dij k

k

(Matrix A+ is the conjugate transposed matrix of matrix A) It has n2 independent real parameters. On the other hand, all the n n unitary matrices with determinant equal to +1 constitute special unitary group SU(n) having n2 − 1 independent real parameters. Group O(n) and SO(n)—n n real orthogonal matrices constitute an n dimension real orthogonal group O(n), where the matrix A satisﬁes X X At A ¼ I; i:e:ðAt AÞij ¼ ðAt Þik Akj ¼ Aki Akj ¼ dij k

k

(Matrix At is the transposed matrix of matrix A) Its group elements are described by n(n − 1)/2 independent real parameters. Among the O(n) groups, the nn real orthogonal matrices with their determinants equal to +1 constitute the n dimension special real orthogonal group SO(n). Group O(n) is deﬁned in real number ﬁeld but group U(n) is deﬁned in complex number ﬁeld so that group O(n) is the subgroup of group U(n). The group SO(n) is a special group of the group O(n), and it is certainly a subgroup of group O(n). On the other hand, group O(n) is a subgroup of the group U(n) and SU(n) is a subgroup of U(n) group with determinant equal to +1; therefore, the group SO(n) is the common subgroup of groups O(n) and SU(n). One example of the application of continuous group in spectroscopy is that mentioned in Chap. 1 about the classiﬁcation of the spectral terms of nlq conﬁguration. By introducing high-order continuous group U(4l + 1) (group SO(3) is its subgroup), one can use different irreducible representation of following group chain Uð4l þ 1Þ SUð2l þ 1Þ SUð2Þ SOð2l þ 1Þ SUð2Þ SOð3Þ SUð2Þ to distinguish spectral different terms which have the same quantum number LS. The properties of permutation group and Young tableau can be used in the reduction of irreducible representation along the group chain because there is close connection between permutation group P(n) and unitary group U(n). The theory of continuous group and its application in atomic spectroscopy can be referred to the books of [1, 3].

48

2.6

2 Group Theory and Quantum Theory

Point Group and Their Representation

The symmetry properties of the energy levels and the energy level splitting of the ions (rare earth or transition-metal ions) in crystal are determined by symmetry of the surrounding lattice ions. This is the point symmetry around the positions where the active ions are located. These points remain ﬁxed when any symmetry transformation of the crystal is applied and so are the intersections of all the rotation axes and all the reflection planes, because two successive rotations of the body about two non-intersecting axes or two reflections in two planes without a common point result in a translation of the body. Symmetry operations in fact can be divided into three different fundamental kinds: rotation around an axis, reflection in a plane, and translations in certain direction. The third operation has not relation to the problems discussed in this book, and so we are not concerned with it. Before going to enumerate all the point symmetry groups, it is necessary to discuss the common features of the symmetry operations of rotations around an axis: (1) If a group includes element Rg which takes the axis a to axis b, then the symmetry elements rotating around the axis a and axis b through the same angle are conjugated, that is

Rb ¼ Rg Ra R1 g

ð2:12Þ

We can explain this formula in the following way: the operation RgRaR−1 g takes the axis b to axis a followed by rotating around the axis a through an angle u and then rotating from axis a to axis b at last. The ﬁnal result of this operation is a rotation around axis b through an angle u. Therefore, the operations which rotate around different axes through the same angle are conjugate elements belonging to the same class of the group. (2) If there is a 2-order axis perpendicular to the n-order axis Cn in a group, then Ckn and C-k n will belong to the same class. If the axis Cn lies on a plane rv, then k Cn ¼ rv Cnk ðrv Þ1 , because the symmetry plane rv changed the direction of rotation and so Ckn and C-k n belong to the same class. However, if there is a plane rh perpendicular to the Cn axis, which changes the rotation direction and at the same time reverses the direction of the axis, then Ckn and C-k n belong to different classes. (3) Many point groups are direct products of simple point group G (does not include inversion i) and the group of symmetry center I containing only unit element e and inversion i. One half of the direct product G ⊗ I is the original group G and the other elements are the elements of G multiplied by inversion element i. The inversion element i commutes with the elements of G, so the direct product contains two times the elements of group G. Therefore, the number of class of direct product group G ⊗ i is two times that of the group G;

2.6 Point Group and Their Representation

49

and each class C of the group G corresponds to two classes C and C ⊗ i. The new irreducible representations produced have the same number and dimension as those of the group G. This property makes it very simple to construct the character table of direct product group. There are two kinds of point groups: proper and improper rotations. The so-called improper rotation means a rotation about some axis followed by a reflection through a plane or followed by an inversion through the origin. First kind of point group (1) Cn Groups Cyclic groups of n order. It is a group of rotations about an axis of n order. Each one of its n elements forms a class itself and can be generated by any element in the group. Group C1 contains only the identical transformation E and without any symmetry. All the irreducible representations are of one-dimension. In a crystal there are only ﬁve kinds of rotation groups: C1, C2, C3, C4, and C6. (2) Dn Groups These groups are produced by adding a 2-order axis perpendicular to n-order axis Cn. By the action of Cn rotation, further n − 1 2-order axes are generated. Including n horizontal 2-order axis intersecting at angles p/n, there are altogether 2n elements. The number of classes is different for n is odd and n is even. If n is odd (n = 2p + 1), all the 2-order axes can be transformed to each other by Cn, and so they are in the same class. The rotations of clockwise Cn and those of counter-clockwise Cn are conjugate, because of the existence of perpendicular 2-order axes. Therefore, besides the identity element E = Cnn, 2p rotations form p classes and so there are p + 2 classes. If n is even (n = 2p), all the 2-order axes can not be arrived separately by Cn and so they are divided into two classes. The other elements in this group form p + 1 classes, that is, the identity element E forms one class and C2p is divided into p classes, because rotations of clockwise and those of counter-clockwise are conjugate. In this case, there are p + 3 classes. For example, there are three classes in D3 and ﬁve classes in D4. According to the properties of the irreducible representation illustrated in Sect. 2.4, because 22 + 12 + 12 = 6, there are two one-dimensional irreducible representations and one two-dimensional irreducible representation in group D3. For group D4, owing to the fact that 22 + 12 + 12 + 12 + 12 = 8, there are four one-dimensional irreducible representations and one two-dimensional irreducible representation. By means of orthogonal relations, it is easy to obtain their characters tables. (3) Tetrahedral Group T This group is formed by all the symmetry axes of a tetrahedron, that is, three 2-order axes passing through two midpoints of opposite edges and four 3-order axes passing through the vertices of the tetrahedron. Three 2-order axes are equivalent by rotating the 3-order axes, and four 3-order axes are also equivalent by rotating the

50

2 Group Theory and Quantum Theory

2-order axes. Therefore, there are 12 elements divided into four classes: E; three 2-order axes C2, four 3-order axes C3, four 3-order axes C32. Considering that 32 + 12 + 12 + 12 = 12, there are one three-dimensional irreducible representation and three one-dimensional irreducible representations. (4) Octahedron Group O The symmetry axes of a octahedron contain three 4-order axes passing through the centers of opposite faces, four 3-order axes which are body diagonal, and six 2-order axes passing through the midpoints of opposite edges. All the axes of the same order are equivalent. There are 24 elements divided into following ﬁve classes: E; 6 rotations C4 and C34; 3 rotations C24; 8 rotations C3 and C23; and 6 rotations C2. Because 32 + 32 + 22 + 12 + 12 = 24, there are two threedimensional irreducible representations, one two-dimensional irreducible representation and two one-dimensional irreducible representations. Second kind of point group (1) Cnv Groups The structure of groups Cnv is very similar to that of the groups Dn, so long as one replaces the 2-order axes perpendicular to Cn to a vertical plane rv passing through Cn. It is also a 2n order group containing n rotations about the axis of n order and n vertical reflections plane rv. When n is odd (n = 2p + 1), it has p + 2 classes, but has p + 3 classes when n is even (n = 2p). Therefore, the irreducible representation number is the same as that of the group Dn and its character table is listed together with that of group Dn. (2) Cnh Groups These groups are obtained by adding a perpendicular plane rh to Cn and have 2n elements: n rotations Ckn and n rotation–reflections Cknrh, with k = 1, 2, 3, …, n. All the elements are commutative and so is a Abelian group. The number of class is equal to the number of elements. If n is even, it includes symmetry inversion: p C2p rh ¼ C2 rh ¼ i. The simplest group C1h Cs contains only elements E and rh. (3) S2n Groups These are 2n order rotation–reflection cyclic groups. S2 Ci contains only identity 2p þ 1 and inversion elements. If 2n = 4p + 2, owing to the fact that S4p þ 2 ¼ C2 rh ¼ Ci , it includes symmetry center. These kind of groups are S2 and S6, and can be written as S4p þ 2 ¼ C2p þ 1 Ci . The number of classes is equal to the order of the group and all their irreducible representations are of one-dimension. Representation E of S4 is not a real two-dimensional representation but two one-dimensional representations (C3 and C4) merged into one.

2.6 Point Group and Their Representation

51

(4) Dnh Groups The 4n elements in these groups are obtained by adding to Dn a horizontal reflection plane rh perpendicular to the n-order symmetry axis. A 2-order axis and the plane rh passing through it will produce vertical plane rv perpendicular to the reflection plane rh. Besides the original 2n elements of group Dn, there are n reflection planes rv and n rotation–reflection elements Cknrh. Owing to the fact that rh is commutative with all the other group elements, group Dnh can be expressed as Dnh ¼ Dn Cs , where Cs is a group that contains only two elements E and rh. If n is even, then Dnh includes symmetry center and D2ph ¼ D2p Ci . The number of classes for groups Dnh is twice the number in the group Dn, while half of its classes are the same as those of Dn. The other classes can be obtained by multiplying these by rh. When n is odd, then all the rv planes belong to one class. When n is even, the rv planes belong to two classes. The rotation–reflections Cknrh and C−k n rh are conjugated in pair. The number of irreducible representations is twice the number in the group Dn, so the number of one-dimension and two-dimension representations is also twice the number in the group Dn. (5) Dnd Groups The other way to add the reflection plane to Dn is to draw vertical planes through the axis of the n-order axis and midway between each adjacent pair of horizontal 2-order axes. Another n − 1 similar planes are produced by the rotation of the norder axis. Therefore, these groups also contain 4n elements. Besides the original 2n elements of group Dn, there are n reflection planes rd, n rotation–reflection axes, þ1 like S2k ; k ¼ 1; 2; 3; . . .; n 1. It can be shown that 2n ð2k þ 1Þ

þ 1 1 2k þ 1 1 2k þ 1 1 rd S2k rd ¼ rd rh C2n rd ¼ rh rd C2n rd ¼ rh C2n 2n

ð2k þ 1Þ

¼ S2n

;

It means that the rotation–reflection axes are conjugated in pairs. When n is even n = 2p. The identity element E forms the ﬁrst class and p times the rotation C2p around n-order axis Cp2p = C2 forms the second class. The 2p second-order rotations around horizontal axis, which are equivalent by the n-order axis rotation, constitute the third class, and the 2p reflection planes rd constitute the fourth class. The rotation around n-order axis (for k = 1, 2, 3, …, p – 1) in which Ck2p and C-k 2p are conjugated constitute p-1 classes in pairs. Finally, the rotation–reflection axes S2k+1 and S-(2k+1) constitute 2n 2n p classes in pairs. Therefore, when n is even n = 2p, there are 2p + 3 classes. When n is odd, n = 2p + 1, there are horizontal 2-order axes perpendicular to the vertical plane and so a symmetry center Ci is produced. Therefore, D2p þ 1;d ¼ D2p þ 1 Ci and D2p+1,d has 2p + 4 classes, because D2p+1 has p + 2 classes and the class number of direct product of D2p+1 ⊗ Ci is twice the number in the group D2p+1. Their irreducible representations can be deduced by those of the groups D2p+1. (6) Group Oh It is the cubic group introduced previously.

52

2 Group Theory and Quantum Theory

(7) Group Td This group is formed by all the symmetry elements of a tetrahedron. It can be obtained by adding to the group T a reflection plane passing through one 2-order and two 3-order axes. In this way, the 2-order axes become 4-order rotation– reflection axes. All the 24 elements are divided into ﬁve classes: E, 8 rotations C3 and C23, 6 reflection planes, 6 rotation–reflection axes, and 3 rotations. It has the same irreducible representations as that of the group O. (8) Group Th This group is obtained by adding to the group T a symmetry center i: Th ¼ T Ci . The appearance of i produces three reflection planes mutually perpendicular to each other, because i = C2rh. On the other hand, by means of S6 ¼ C3 Ci , 6-order rotation–reflection axis is presented. Thus, 24 elements of this group are divided into eight classes, which has the number double that of the group T, and so the number of irreducible representations. Noteworthily, owing to the restriction of the translations, axes of 5-order and those higher than 6-order cannot exist and hence there are only 32 point groups in the crystal. They are: Cn ; Cnh ðn ¼ 1; 2; 3; 4; 6Þ Cnm ; Dn ; Dnh ðn ¼ 2; 3; 4; 6Þ S2n ðn ¼ 1; 2; 3Þ; Dnd ðn ¼ 2; 3Þ O; Oh ; T; Th ; Td

10 groups 12 groups 5 groups 5 groups

Among these 32 point groups, there are 11 point groups, which include symmetry center: S2 Ci ; S6 ; C2h ; C4h ; C6h ; D3d ; D2h ; D4h ; D6h ; Oh ; Th The irreducible representations of these 11 groups are divided into even representations g and odd representations u.

2.7

Symmetry and Quantum Theory of the Ions in Solids

We will turn to the topic of the energy levels of the active ions in solids. Owing to the fact that this problem is greatly dependent on the symmetry around the ions, we should deal with it by associating the group theory with quantum mechanics. Let us consider the relation between Schrödinger equation and the representation of symmetry transformation groups. If the ion is in a symmetry position represented by a group G = {Gi}, then under the action of an group element Gi, the wave functions of the system, that is, the eigenfunctions of the Hamiltonian operator should not have any change. Consider the Schrödinger equation

2.7 Symmetry and Quantum Theory of the Ions in Solids

Hw ¼ Ew

53

ð2:13Þ

In order to express the transformation of the wave function, the following two equations can be used 0 G1 i wðxÞ ¼ wðx Þ ¼ wðGi xÞ

ð2:14Þ

0 Gi wðx0 Þ ¼ wðxÞ ¼ w G1 i x

ð2:15Þ

These two equations show that the transformation of the system by the operation Gi is the same as to keep the system invariant but to transform the coordinate system by G−1 i . On the other hand, the linear algebra tells us that a real orthogonal transformation, which keeps the distance of two points invariant, is a unitary transformation (remember that the eigenfunctions of the Hamiltonian operator in quantum mechanics are orthogonal and normalized). Transforming uðxÞ ¼ HðxÞwðxÞ by means of (2.14) and (2.15), the following can be obtained 1 G1 i uðxÞ ¼ H ðGi xÞwðGi xÞ ¼ H ðGi xÞGi wðxÞ

Multiplying both sides of above equation from the left by Gi, one can obtain 1 uðxÞ ¼ Gi H ðGi xÞG1 i wðxÞðGi Gi ¼ 1 has been usedÞ:

Comparing with the original formula uðxÞ ¼ HðxÞwðxÞ, the following result is obvious HðxÞ ¼ Gi H ðGi xÞG1 i : Note that the Hamiltonian should be invariant because the system is invariant under the transformation, that is, HðxÞ ¼ H ðGi xÞ; therefore HðxÞGi ¼ Gi HðxÞ

ð2:16Þ

Operating Gi on both sides of (2.13) and using (2.16), then HðxÞGi wðxÞ ¼ Gi HðxÞwðxÞ ¼ Gi EwðxÞ ¼ E ðGi wðxÞÞ

ð2:17Þ

It shows that the wave functions belong to the same energy eigenvalue before and after the transformation. If the energy eigenvalue E has degeneracy g, that is, there are g wave functions wj belonging to the same energy eigenvalue E, Giwj should be a linear combination of g wave functions wj according to (2.17)

54

2 Group Theory and Quantum Theory

Gi wj ¼

g X

M ðGi Þlj wl

ð2:18Þ

l¼1

Operating with another group element, one can obtain a similar result Gk wj ¼

g X

MðGk Þlj wl

l¼1

Each group element in {Gi} has a corresponding matrix M{Gi}, and for the joint operation of product GiGk, one has Gi Gk wj ¼

g X l¼1

MðGk Þlj Gi wl ¼

g X

MðGk Þlj MðGi Þml wm ¼

l;m¼1

g X

MðGi Gk Þmj wm

m¼1

P Formula MðGi Gk Þmj ¼ gl¼1 MðGi Þml MðGk Þlj shows that the matrix for the group element product is equal to the product of the matrices of group elements. The existence of identity element and inverse element can also be demonstrated. Therefore, these matrices form a representation of the group G, and the related wave functions form the bases. It can be shown that the representation formed by the degeneracy bases is irreducible and its dimension is equal to g. Certainly, the accidental degeneracy and Kramers degeneracy should be excluded. After establishing the relation between irreducible representation and the degeneracy of energy levels, one can go back to the problem of free ions. Obviously, the free ions possess spherical symmetry: the symmetry group is three-dimensional rotation group R3 (SO(3)). The representation of the R3 group, as will be discussed in the following, can be reduced to a series of irreducible representations labeled by angular momentum quantum numbers J: DJ1 ; DJ2 ; . . .; DJi ; . . . The dimension of DJi is 2Ji+ 1, the degeneracy of the spectral term with angular momentum J. The eigen wave functions of free ions (the wave functions of the spectral terms) constitute the bases of the irreducible representations. The active ions in crystals have interactions with the surrounding ions and a lower symmetry perturbation potential should be added to the Hamiltonian with spherical symmetry. Then, the crystal ﬁeld potential has symmetry group G which is a subgroup of R3. The representations originally irreducible in R3 are now reducible and they can be split into two or more irreducible representations. For example,

2.7 Symmetry and Quantum Theory of the Ions in Solids

DJi ¼ Cð1Þ ðg1 Þ þ Cð2Þ ðg2 Þ

55

ð2:19Þ

then, it is said that the spectral term Ji is split into two levels with degeneracy g1 and g2. Having this general understanding, the next step is to realize a detailed method for the calculation of energy level splitting. In order to achieve this goal, one should have more knowledge of group theory and the theory of angular momentum as well as the application of the group theory to the calculation of matrix elements.

2.8

Full Rotation Group and Angular Momentum Theory

Full rotation group, that is, spherical symmetry group, is the symmetry group of free ions. It can be seen from previous analysis that the free ion’s wave functions constitute the bases of the irreducible representations of this group. On the other hand, these functions are also eigenfunctions of angular momentum. The essence of this relation is that the angular momentum operator is in fact a rotation operator. This can be clearly seen from the following analysis. Consider the transformation of a wave function wðx; y; zÞ after rotation around z axis wðx0 ; y0 ; z0 Þ ¼ Rwðx; y; zÞ If one rotates around z axis through an angle a, then according to the familiar formula x0 ¼ x cos a þ y sin a y0 ¼ x sin a þ y cos a z0 ¼ z Substituting a = du into this equation, then x0 ¼ x þ ydu y0 ¼ xdu þ y z0 ¼ z Because du is a very small angle, the following relations can be used: cosðduÞ ¼ 1; sinðduÞ ¼ du: Therefore

56

2 Group Theory and Quantum Theory

wðx0 ; y0 ; z0 Þ ¼ wðx þ ydu; y xdu; zÞ Expanding this formula into Taylor series @ @ wðx0 ; y0 ; z0 Þ ¼ wðx; y; zÞ þ du y x wðx; y; zÞ @x @y and using the angular momentum operator in quantum mechanics @ @ @ Jz ¼ ih x y ¼ i h @y @x @u We have Rðd/Þwðx; y; zÞ ¼ ð1 id/Jz =hÞwðx; y; zÞ ¼ expðid/Jz = hÞwðx; y; zÞ Rotating z axis through a ﬁnite angle u, then Rð/Þwðx; y; zÞ ¼ expði/Jz =hÞwðx; y; zÞ The electronic eigenfuctions of free ion constitute the bases of the irreducible representations of group R3. It can be seen from Chap. 1 that they are spherical harmonic functions Yjm ðh; uÞ jjmi We also have Jz jjmi ¼ mhjjmi

ð2:20Þ

Therefore, the 2j + 1 functions with m = −j, −j + 1, −j + 2, …, j − 2, j − 1, j under the symmetry operation of rotation through an angle u around z axis is a diagonal matrix with diagonal matrix elements eiju ; eiðj1Þu ; eiðj2Þu ; . . .; eiðj2Þu ; eiðj1Þu ; eiju Obviously, the character of the operation matrix (irreducible representations of group R3) is vðuÞ ¼

m¼j X m¼j

eimu ¼

sinðj þ 1=2Þu sinðu=2Þ

ð2:21Þ

When u = 0 or 2p, it should be calculated by the ratio of differential quotient and the result is vð0Þ ¼ 2j þ 1; vð2pÞ ¼ 2j þ 1 for j is an integer and vð2pÞ ¼ ð2j þ 1Þ for j is a half-integer.

2.8 Full Rotation Group and Angular Momentum Theory

57

Equation (2.21) will be used frequently to solve the problem of energy level splitting by crystal ﬁeld. It should be noted that when j is a half-integer, so j + 1/2 is an integer, then by (2.21) vðu þ 2pÞ ¼

sinðj þ 1=2Þu sinðj þ 1=2Þu sinðj þ 1=2Þu ¼ ¼ ¼ vðuÞ ð2:22Þ sinðu=2Þ sinðu=2 þ pÞ sinðu=2Þ

Therefore, for the half-integer j we have a double-valued character. In order to cope with this situation, a new group element E will be introduced, which represents a rotation of 2p and now the identity element E is the rotation of 4p. The augmented group contains twice as many elements as the original one and is call the double group. Besides the original elements G1, G2, …, Gn, there are new elements G1 , G2 ; . . .; Gn in the double group, which have the relation of Gi ¼ EGi . The irreducible representation of the double group can be divided into two parts, one is called single-valued representation, in which Gi and Gi have the same representation, and the other one is called double-valued representation, in which v Gi ¼ vðGi Þ. It should be noted that by using (2.21) and (2.22) to reduce the irreducible representation from higher symmetry to lower symmetry, the angle u for symmetry center and reflection mirror is taken to be p. For rotation–reflection axis S3, u = p/3, and for rotation–reflection axis S4 and S6, u should be p/2 and p/3, respectively. Now let us consider the coupling between two angular momenta, which can be different momenta of the same electron (e.g. one spin momentum and one orbital momentum) or the same kind of momentum for different electrons. In quantum mechanics, the zero-order wave function of an interaction system is the product of the wave functions of its subsystems. By using the language of group representation, the basis space describing the interaction system is the direct product of the basis spaces describing the subsystems. The direct product space is generally reducible, that is, it can be reduced to the sum of a series of subspaces. By a linear transformation, one can express the direct product space as the direct sum of a series of subspace orthogonal to each other. If the wave functions of two angular momenta are jj1 m1 i and jj2 m2 i, respectively, their direct product space can be transformed to irreducible space of the basis jj1 j2 jmi by the following linear transformation jj1 j2 jmi ¼

X

jj1 m1 j2 m2 ihj1 m1 j2 m2 jj1 j2 jmi

ð1:23Þ

m1 m2

The coefﬁcients hj1 m1 j2 m2 jj1 j2 jmi are called vector-coupling coefﬁcients. In order to write it in a more symmetric form, Wigner introduced the so-called 3-j symbols deﬁned as

j1 m1

j2 m2

j3 m3

¼ ð1Þj1 j2 m3 ð2j3 þ 1Þ1=2 hj1 m1 j2 m2 j j1 j2 j3 m3 i

ð2:24Þ

58

2 Group Theory and Quantum Theory

They have the following symmetric properties: The even permutation of the columns is symmetry

j1 m1

j2 m2

j3 m3

¼

j3 m3

j2 m2

j1 m1

¼

j1 m1

j3 m3

j2 m2

ð2:25Þ

The odd permutation of the columns involves a multiplying factor of ð1Þj1 þ j2 þ j3

j3 m3

j2 m2

j1 m1

¼

j1 m1

j2 m2

¼ ð1Þj1 þ j2 þ j3

j3 m 3

¼

j1 m1

j1 m1

j2 m2

j3 m3

j3 m 3

j2 m2

ð2:26Þ

and

j2 m2

j1 m1

j3 m3

¼ ð1Þ

j1 þ j2 þ j3

j1 m1

j2 m2

j3 m3

ð2:27Þ

The 3-j symbols also have the following orthogonal properties: X j3 ;m3

j ð2j3 þ 1Þ 1 m1

X j 1 m 1 m m 1

j2 m2

2

j3 m3

j2 m2

j3 m3

j2 m2

j1 m1

j03 m03

¼ d m1 m01 d m2 m02

ð2:28Þ

¼ ð2j3 þ 1Þ1 d j3 j03 d m3 m03

ð2:29Þ

j2 m02

j1 m01

j3 m3

Introducing by (2.29), it can be shown X j1 m1 m m m 1

2

3

j2 m2

j3 m3

2 ¼1

The values of 3-j symbols can be calculated by formula (e.g. Equations (2.1– 2.20) provided by Judd in reference [3]), and they can also be found from tables (e.g. Rotenberg et al. “The 3-j and 6-j symbols” [4]) or calculated by means of computer programs [5]. Two useful simple formulas are

j1 0

j2 0

j3 0

j m

j m

¼ ð1ÞJ=2

1 0

¼ ð1Þjm

m ½ð2j þ 1Þðj þ 1Þj 1=2

ðJ 2j1 Þ!ðJ 2j2 Þ!ðJ 2j3 Þ! ðJ þ 1Þ!

1=2

ð2:30Þ

J ! J 2 J j j ! 1 2 ! 2 j3 ! 2 2

J

ð2:31Þ

2.8 Full Rotation Group and Angular Momentum Theory

59

When 2j + 1 is even, (2.30) is not valid. In (2.31) J = j1 + j2 + j3, when J is odd, this 3-j symbol is equal to zero. It is the result obtained by (2.27). Some more formulas for the calculation of 3-j symbols in special cases can be found from the book of Rotenberg et al. [4] or directly calculated by a computer program [5]. There is an important property of the 3-j symbols that should be mentioned, that is, the triangle condition of 3-j symbols. It means that 3-j symbols will be zero unless three j are satisﬁed by the triangle condition j1 þ j2 j3 jj1 j2 j. On the other hand, the 3-j symbols vanish unless m1 + m2 + m3 = 0. We should also mention briefly some of the properties of 6-j and 9-j symbols, which are used in the wave functions calculations for the coupling of three and four angular momenta. For the coupling of three angular momenta, the ways for j1, j2, j3 coupling in pair can be different. For example, it can be (j1j2)j12j3J or j1(j2j3)j23J, that is, j1j2 couple at ﬁrst and then couple with j3, or j2j3 couple at ﬁrst and then couple with j1. The wave functions of reducible space obtained by different coupling ways can be transformed by jðj1 j2 Þj12 j3 JM i ¼

X

hðj1 j2 Þj12 j3 J j j1 ðj2 j3 Þj23 J ijj1 ðj2 j3 Þj23 JM i

ð2:32Þ

j23

and the 6-j symbols are deﬁned as

j1 j3

j2 J

j12 j23

¼ ð1Þj1 þ j2 þ j3 þ J ½ð2j12 þ 1Þð2j23 þ 1Þ 1=2 hðj1 j2 Þj12 j3 J j j1 ðj2 j3 Þj23 J i

ð2:33Þ The values of 6-j symbols can also be found from tables [4]. However, in these tables, only the values of some 6-j symbols are listed. Values of other 6-j symbols can be found by their symmetry properties. Each 6-j symbol can be seen as a regular tetrahedron with 6j vectors as its six edges and so it has the symmetry of a regular tetrahedron. Its symmetry properties can be expressed as: the 6-j symbol is invariant under any permutation of the columns and is also invariant under an interchange of the upper and lower arguments in any two columns or exchange of any two columns:

j1 j4

j2 j5

j3 j6

¼

j4 j1

j5 j2

j3 j6

¼

j2 j5

j1 j4

j3 j6

ð2:34Þ

The aforementioned four planes of the regular tetrahedron are triangles and the value of 6-j symbol will be zero unless the following triangle conditions are satisﬁed

60

2 Group Theory and Quantum Theory

Dðj1 j2 j3 Þ; Dðj1 j5 j6 Þ; Dðj4 j5 j3 ÞDðj2 j4 j6 Þ That means, for example, j1 þ j2 j3 jj1 j2 j In addition, the 6-j symbols have the following orthogonal relation: X

ð2j3 þ 1Þð2j6 þ 1Þ

j6

j1 j4

j2 j5

j3 j6

j1 j4

j2 j5

j03 j6

¼ d j3 j03

ð2:35Þ

One can ﬁnd the values of 6-j symbols and many useful calculation formulas in the book written by Rotenberg et al. [4]. The 9-j symbols are used to correlate different coupling ways for four angular momenta. For example, in the relation between jðj1 j2 Þj12 ðj3 j4 Þj34 J i and jðj1 j3 Þj13 ðj2 j4 Þj24 J i, the following coefﬁcients can be used in the transformation jðj1 j2 Þj12 ðj3 j4 Þj34 JM i ¼

X

hðj1 j2 Þj12 ðj3 j4 Þj34 J j ðj1 j3 Þj13 ðj2 j4 Þj24 J ijðj1 j3 Þj13 ðj2 j4 Þj24 JM i

j13 j24

ð2:36Þ The above coefﬁcients can be expressed as 9-j symbols by hðj1 j2 Þj12 ðj3 j4 Þj34 J j ðj1 j3 Þj13 ðj2 j4 Þj24 J i

8 > < j1 1=2 j3 ¼ ½ð2j12 þ 1Þð2j34 þ 1Þð2j13 þ 1Þð2j24 þ 1Þ > : j13

j2 j4 j24

9 j12 > = j34 > ; J

ð2:37Þ

We will not use 9-j symbols directly in this book and so would like to mention only two formulas, which are useful in the calculation of matrix elements 8 > < j11 j21 > : j31

9 j13 > = X j j21 j22 j23 j31 j12 j13 j32 j33 11 j23 ¼ > m21 m22 m23 m31 m32 m33 ; all m m11 m12 m13 j33 j11 j12 j22 j13 j23 j33 j21 j31 j32 m11 m21 m31 m12 m22 m32 m13 m23 m33

j12 j22 j32

ð2:38Þ 8 < j1 j : 30 j

j2 j4 j0

9 j= 1=2 j1 j2 þ j3 þ j þ j0 0 j ¼ ð1Þ ½ð2j þ 1Þð2j þ 1Þ j4 ; 0

j2 j3

j j0

ð2:39Þ

2.9 Irreducible Tensor Operators and the Calculation of Matrix Elements

2.9

61

Irreducible Tensor Operators and the Calculation of Matrix Elements

The calculation of matrix elements and energy levels are the most basis calculations in the theory of crystal spectroscopy. It is an important problem to use group theory and the theory of angular momentum in these calculations. This problem will be discussed in this section. The transformation characteristics of the angular momentum eigenfunctions under rotation groups have been investigated in the last section. The wave function spaces of the interacting systems have also been correlated with the representation spaces of the direct product of the rotation group. Obviously, if the operators are classiﬁed according to the transformation properties of the angular momentum eigenfunctions, that is to say, let the operators constitute the bases of the irreducible representation space of the rotational group; undoubtedly, we can make full use of the symmetry properties of the system and a series of formulas developed by group theory to simplify the computation of various matrix elements in spectroscopy, which is the reason for the introduction of irreducible tensor operators. By means of these transformation properties, one can deﬁne irreducible tensor operators: irreducible tensor operators are operators forming the bases of the irreducible representation of the rotation group. They satisfy the following relation in mathematics Rða; b; cÞTqðkÞ R1 ða; b; cÞ ¼

X q0

ðk Þ ðk Þ

Tq0 Rq0 q ða; b; cÞ

ð2:40Þ

Practically, (2.40) is the same as the transformation of angular momentum eigenfunctions under rotation expressed as follows Rða; b; cÞjkqi ¼

X q0

ðk Þ

jkq0 iRq0 q ða; b; cÞ

To view it at a different angle, irreducible tensor operators TqðkÞ have the same transformation properties under operation of rotation group as those of angular momentum eigenfunctions jkqi. Therefore, under the action of angular momentum —rotation operator, TqðkÞ and jkqi should have the same transformation, that is Jz jk; qi ¼ qjk; qi J jk; qi ¼ ½k ðk þ 1Þ qðq 1Þ 1=2 jk; qi h i Jz ; TqðkÞ ¼ qTqðkÞ

ð2:41aÞ

62

2 Group Theory and Quantum Theory

h i ðk Þ J ; TqðkÞ ¼ ½kðk þ 1Þ qðq 1Þ 1=2 Tq 1

ð2:41bÞ

Equations (2.40) and (2.41a, 2.41b) can be seen as the mathematical deﬁnition of irreducible tensor operator, in which Jz is the z component of angular momentum and J± are the shift operators which raise and lower the component q of angular momentum k, respectively. Having introduced the irreducible tensor operators, the calculation of matrix elements becomes very easy, because the transformation property of the product of operators and the wave functions can be easily obtained. In order to calculate matrix elements, it is necessary to know Wigner-Eckart theorem ﬁrst. The physics idea for the introduction of this theorem has been mentioned above. If one would like to calculate matrix elements ha0 j0 m0 jTqðkÞ jajmi, the ﬁrst step is to investigate the transformation property of TqðkÞ jajmi. According to the result discussed previously, it is transformed as the vectors in the direct product space RðkÞ RðjÞ , or one can say that TqðkÞ jajmi with all the different k and j are the bases of the direct product space RðkÞ RðjÞ . Reducing the reducible space, the basis can be written as jbJM i. By means of the angular momentum coupling method discussed previously, these vectors can be written as a linear combination of the bases in the direct product space RðkÞ RðjÞ (remember that the transformation property of the operators and the bases of wave function space is the same) jbJM i ¼

X

hkqjm j kjJM iTqðkÞ jajmi

ð2:42Þ

qm

One can make an inverse transformation by using the orthogonal property of the coefﬁcients TqðkÞ jajmi ¼

X

hkqjm j kjJM ijbJM i

JM

Multiplying both sides of this equation by ha0 j0 m0 j, then E X D a0 j0 m0 TqðkÞ ajm ¼ hkqjm j kjJM iha0 j0 m0 j bJM i JM

By using orthogonal property of angular momentum eigenfunctions, it can be shown that ha0 j0 m0 jbJM i is zero except J = j′, M = m′ and its values is independent 0 0 ðkÞ of m′. It is denoted as a j T aj and called irreducible matrix element, that is D E ha0 j0 m0 j bJM i ¼ a0 j0 T ðkÞ aj dJj0 dMm0

2.9 Irreducible Tensor Operators and the Calculation of Matrix Elements

63

then D

E D E a0 j0 m0 TqðkÞ ajm ¼ hkqjm j kjj0 m0 i a0 j0 T ðkÞ aj

This is so-called Wigner-Eckart theorem (W-E theorem). Writing the coefﬁcients in the form of 3-j symbols, then 0 E D j j0 m0 0 0 0 ðk Þ a j m Tq ajm ¼ ð1Þ m0

k q

j m

D E a0 j0 T ðkÞ aj

ð2:43aÞ

According to the deﬁnition (2.24) of 3-j symbol, the expression (2.43a) should be 0 E D 0 j a0 j0 m0 TqðkÞ ajm ¼ ð1Þkj þ m ð2j0 þ 1Þ1=2 m0

k q

j m

D

E a0 j0 T ðkÞ aj ð2:43bÞ

However, many authors adopt (2.43a) as the expression of W-E theorem. The reduced matrix elements of the two different formulas are different. On the other hand, the W-E theorem for point group can be expressed as hC1 c1 jOðcCÞ jC2 c2 i ¼ ðCÞ1=2 hC1 c1 jC2 c2 CcihC1 j OðCÞ jC2 i

ð2:43cÞ

where hC1 c1 jC2 c2 Cci is Clebsch-Gordan coefﬁcients (C-G coefﬁcients) of point group, C and c denote irreducible representation of point group and the component of that irreducible representation, respectively, and (C) is the dimension of irreducible representation C. C-G coefﬁcients of triangle basis can be found in Appendix F. Using this theorem, we can save a lot of time in the calculation of matrix elements, because with only one of the reduced matrix element a0 j0 T ðkÞ aji, all the (2j + 1)(2k + 1)(2j′ + 1) matrix elements can be calculated. Furthermore, by the properties of the 3-j symbols, some of the matrix elements are equal to zero and without calculation. We will use it frequently in the calculation of the energy level and transition probability. As an example, we would like to prove a useful formula for the calculation of energy level and transition probability. Many spectroscopic problems involved orbital and spin variables. If these two kinds of angular momentum are denoted by j1 and j2, respectively, by using (2.21), a general coupling state (basis hJM j of direct product space) can be expressed as a linear combination of the direct products of two subspace bases hj1 m1 j and hj2 m2 j as follows

64

2 Group Theory and Quantum Theory

hj1 j2 JM j ¼

X m1 m2

j hj1 m1 j2 m2 j 1 m1

J ð2J þ 1Þ1=2 ð1Þj1 j2 þ M M

j2 m2

ðK Þ

Similarly, a tensor operator TQ ð1; 2Þ of a direct product space ℜ(KQ) can be expressed as the following linear combination of tensor operators Tqðk1 1 Þ ð1Þ and Tqðk2 2 Þ ð2Þ of subspaces ℜ(k1q1) and ℜ(k2q2) ðK Þ TQ ð1; 2Þ

¼

X

Tqðk1 1 Þ ð1ÞTqðk2 2 Þ ð2Þ

q1 q2

k1 q1

k2 q2

K ð2K þ 1Þ1=2 ð1Þk1 k2 þ Q Q ð2:44aÞ

The formula for a point group can be expressed as follows h i X TcðCÞ ¼ Tcð1C1 Þ Tcð2C2 Þ ¼ Tcð1C1 Þ Tcð2C2 Þ hC1 C2 c1 c2 jCci

ð2:44bÞ

c1 c2

Equation (2.44b) is practically a general formula for the direct product of two irreducible tensors. If a point group irreducible representation C replaced by an angular momentum quantum number K, a component c of C replaced by Q and the C-G coefﬁcients of the point group replaced by 3-j symbol then formula (2.44a) can be obtained. The reduced matrix element expression of (2.44a) can be obtained as follows: The left side of (2.44a) can be expressed as ðK Þ hj1 j2 JM jTQ ð1; 2Þ j01 j02 J 0 M 0 ¼ ð1ÞJM

J M

K Q

J0 M0

D E j1 j2 J T ðK Þ ð1; 2Þj01 j02 J 0 ð2:44cÞ

By using the detailed expansion of the wave functions hj1 j2 JM j and j01 j02 J 0 M 0 , the summation of the right side of (2.44a) can be expressed as X XX

0

m1 m2 m01 m02 q1 q2

0

0

ð1Þk1 k2 þ Q þ 2j1 þ M þ j1 j2 þ M m1 m2

j1

k1

j01

m1

q1

m01

j2

k2

j02

m2

q2

m02

j1 m1

j2 m2

J M

j01

j02

m01

m02

J0 M

0

k1

k2

K

q1

q2

Q

D E 1=2 ½ð2J þ 1Þð2J 0 þ 1Þð2K þ 1Þ j1 T ðk1 Þ ð1Þj01 j2 kT ðk2 Þ ð2Þkj02

ð2:44dÞ J K J0 Multiply the right side of (2.44a) and (2.44d) by ð1ÞJM and M Q M 0 P . Take the orthogonal property of the 3-j symbol into account and sum over MM 0 Q

change the order of the column and row in the 3-j symbol. Eliminate the phase factors by means of Eqs. (2.26), (2.28), and (2.38), and then comparing both sides of the obtained equation, it can be shown that

2.9 Irreducible Tensor Operators and the Calculation of Matrix Elements

D

E j1 j2 J T ðK Þ ð1; 2Þj01 j02 J 0

8 > < j1 1=2 j2 ¼ ½ð2J þ 1Þð2J 0 þ 1Þð2K þ 1Þ > : J

j01 j02 J0

65

9 k1 > =D

ED E j1 T ðk1 Þ ð1Þj01 j2 T ðk2 Þ ð2Þj02 k2 > ; K ð2:45Þ

Relation (2.45) is a very useful formula in spectroscopy. If the discussion only concerns the matrix elements of “the ﬁrst part” operator T ðk1 Þ ð1Þ of the state jj1 j2 J i, this formula can be further simpliﬁed. Let T ðk2 Þ ð2Þ ¼ I, that is, unit operator, then k2 = 0, j2 = j′2, and K = k1, using (2.39) and noting that in this case one has D E j2 T ðk2 Þ ð2Þj02 ¼ ð2j2 þ 1Þ1=2 dj2 j02 the following expression can be obtained D

E 0 1=2 j1 j2 J T ðk1 Þ ð1Þj01 j02 J 0 ¼ ð1Þj1 þ j2 þ J þ k1 ½ð2J þ 1Þð2J 0 þ 1Þ

J j01

J0 j1

k1 j2

D

E j1 T ðk1 Þ ð1Þj01 dj2 j02

ð2:46Þ If we are concerned about the matrix elements of “the second part” operator T ð2Þ, then let T ðk1 Þ ð1Þ ¼ I, and k1 = 0, j1 = j′1, K = k2. By using (2.39) once again, the following expression can be obtained similarly ðk2 Þ

D

E 0 1=2 j1 j2 J T ðk2 Þ ð2Þj01 j02 J 0 ¼ ð1Þj1 þ j2 þ J þ k2 ½ð2J þ 1Þð2J 0 þ 1Þ

J j02

J0 j2

k2 j1

D

E j2 T ðk2 Þ ð2Þj02 dj1 j01

ð2:47Þ Although (2.45) can be used to calculate the matrix elements of a two-electron system, the previous discussion is about the matrix elements of single electron. Most of the problems in spectroscopy are concerned with multi-electron, and so the calculation of multi-electron matrix elements should be introduced. It should be pointed out that to construct the wave functions of a multi-electron system and calculate their matrix elements, the coefﬁcients of fractional parentage should be introduced. We would not go so far in mathematics but only make use of the unit operator of multi-electron, which has appropriate direct reading tables. Two operators AðqkÞ and OðqkÞ with the same transformation property obviously have the relation 0 D E D E j k j j0 m0 0 0 0 ðk Þ a0 j0 T ðkÞ aj a j m Tq ajm ¼ ð1Þ 0 q m m

66

2 Group Theory and Quantum Theory

TqðkÞ can be AðqkÞ or OðqkÞ . In this way E D E a0 j 0 D AðkÞ aj 0 0 0 ðk Þ 0 0 0 ðk Þ a j m Aq ajm ¼ a j m Oq ajm 0 0 ðkÞ ha j kO kaji

ð2:48Þ

In case OðqkÞ is a unit operator, (2.48) shows that any operator can be expressed as a unit operator multiplied by a certain value. The unit operator for a single electron is denoted by uðqkÞ ðiÞ, then its reduced matrix element will be D a0 j0 uðkÞ aji ¼ daa0 djj0 P and for multi-electron system UqðkÞ ¼ i uðqkÞ ðiÞ, the summation being over all the electrons. The related 6-j symbols and the coefﬁcients of fractional parentage are used to determine their irreducible matrix elements. Nielson and Koster [6] have given the tables for the irreducible matrix elements of the unit operator for the conﬁgurations of pn ; d n ; f n . We show now an example of the irreducible matrix elements of unit operators. The crystal ﬁeld potential energy of rare earth ions in crystal can be expressed as X V¼ Bkq CqðkÞ ð2:49Þ k;q

P where multi-electron operators CqðkÞ ¼ i CqðkÞ ðhi ; ui Þ are related to the spherical

1=2 YqðkÞ ðhi ; ui Þ and Bkq are the so-called harmonics functions by CqðkÞ ðhi ; ui Þ ¼ 2k4pþ 1 crystal ﬁeld parameters. By means of a relation like (2.48), it is obvious that ED X D E Bkq f n SLJM UqðkÞ f n S0 L0 J 0 M 0 f C ðkÞ f ð2:50Þ hf n SLJM jV jf n S0 L0 J 0 M 0 i ¼ kq

According to the formulas given above, one has D E J ðkÞ n 0 0 0 0 JM n f SLJM Uq f S L J M ¼ ð1Þ M

k J0 q M0

D E f n SLJ U ðkÞ f n S0 L0 J 0 ð2:51Þ

f n SLJ U ðkÞ f n S0 L0 J 0 can be obtained by using (2.46). Remember that the crystal ﬁeld potential is an orbital operator

2.9 Irreducible Tensor Operators and the Calculation of Matrix Elements D

E 0 1=2 f n SLJ U ðkÞ f n S0 L0 J 0 ¼ ð1ÞS þ L þ J þ k ½ð2J þ 1Þð2J 0 þ 1Þ

J L0

J0 L

k S

67

D

E f n SLU ðkÞ f n SL0 dSS0

ð2:52Þ where f n SLJ U ðkÞ f n SL0 J 0 can be found in the tables published by Kamiskii [7], which involves the data of all high-lying 2S+1LJ states (part of these data can be found in Appendix D of this book). On the other hand, we have ðkÞ l1 1=2 l1 hl1 j C jl2 i ¼ ð1Þ ½ð2l1 þ 1Þð2l2 þ 1Þ 0

k 0

l2 0

ð2:53Þ

For f electron it is D E 3 3C ðkÞ 3 ¼ ð1Þ3 7 0

k 0

3 0

The 3-j symbols in (2.53) are easy to be calculated by (2.31).

References 1. M. Hamermesh, Group Theory and Its Application to Physical Problems (Addison—Wesley Publishing Company, INC, London, 1962) 2. M. Tinkham, Group Theory and Quantum Mechanics (McGraw-Hill Book Company, New York, 1964) 3. B.R. Judd, Operator Techniques in Atomic Spectroscopy (McGraw-Hill Book Company, New York, 1963) 4. M. Rotenberg, R. Bivins, N. Metropolis, J.K. Wooton, The 3-j and 6-j Symbols, Technology Press, MIT (Mass, Cambridge, 1959) 5. D.J. Newman, N.G. Betty, Crystal Field Handbook (Cambridge, University Press, Cambridge, 2000) 6. C.W. Nielson, G.F. Koster, Spectroscopic Coefﬁcients for the pn, dn, and fn Conﬁguration, MIT Press (Mass, Cambridge, 1963) 7. A.A. Kaminskii, Crystalline Lasers: Physical Processes and Operating Schemes (CRC Press, Boca Raton, 1996)

Chapter 3

Rare Earth Ions in Materials

3.1

Crystal Field on the Active Ions

The crystal ﬁeld potential matrix element has been briefly mentioned in the last chapter. We should study it in much more detail, because it is a central problem in the energy level calculation of solid-state laser materials. First, it is necessary to have a general idea about the physical mechanisms of crystal ﬁeld. In free ions, there are electron–nucleus Coulomb interaction, electron– electron Coulomb interaction, orbital–spin interaction, and electron–electromagnetic ﬁeld interaction. Besides, the electrons in the active ions in a medium have complex interactions with the lattice ions in the environment that can be described by crystal ﬁelds. It includes at least the following interaction mechanisms [1, 2]: (1) Overlap and exchange interaction of electric charge distribution; (2) Covalence interaction; (3) Point charge Coulomb interaction; (4) Dispersing charge Coulomb interaction; (5) Dipole polarization interaction; (6) Quadrupolar polarization interaction; (7) Charge penetration interaction. In the case of rare earth ions, some authors claim that the ﬁrst two interactions make dominant contribution to the crystal ﬁeld [2]. Nevertheless, if the molecular dynamics simulation (MDS) method is used to determine the actual position of ligands, the calculation results of energy levels and electric-dipole transition intensities are satisfactory even only the point charge contribution is taken into account [3]. Thus the Hamiltonian for the electrons of active ions in crystals can be written as H ¼ Hen þ Hee þ Hso þ Hc þ Hext

ð3:1Þ

where Hen is the electron–nucleus interaction Hamiltonian, Hso denotes the spin– orbit interaction, Hc represents the crystal ﬁeld interaction Hamiltonian, and Hext is the interaction Hamiltonian with external ﬁeld. The last interaction will not be discussed in this book and the ﬁrst three interactions have been dealt with in Chap. 1. The main objective of this chapter is to discuss the crystal ﬁeld interaction © Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8_3

69

70

3 Rare Earth Ions in Materials

represented by Hc. The property of the system, especially the energy level structure, depends on the magnitude of the perturbation Hc. If Hc is smaller than Hen + Hee as well as Hso, then the energy levels are similar to those of the free ions. Thus we can use eigenfunctions of the free ions as zero-order wave functions to ﬁnd the crystal ﬁeld energy level splitting of the state 2S+1LJ. If the magnitude of Hc is the same as or even larger than that of Hso, then one should consider the interaction of Hc before that of the Hso. The characteristics of the energy level are reflected by the symmetry of the crystal ﬁeld and its point group irreducible representation. We now show the orders of magnitude of various interactions for transition metal ions and rare earth ions (in unit of wave number cm−1).

Iron group Rare earth

Hen

Hee

Hso

Hc

105 105

104 104

102 103

104 102

In order to solve the problem of the energy level splitting for the active ions in the materials, besides to treat crystal ﬁeld interaction as a perturbation, the following two approximations should be assumed: (1) The interactions between the electrons of neighbor active ions can be neglected; (2) The interactions between the electrons of the same active ions can be neglected. The ﬁrst approximation is correct for the active ions in the insulated laser materials. Solid laser materials (excluding semiconductors) doped with a small amount of rare earth or transition ions as the luminescent centers are in this category. The second approximation, that is, single-electron approximation, has been proved to provide good enough calculation results for energy levels. Certainly, there are a series of published papers on the correlative crystal ﬁeld [4–6]. The readers interested in the effects of the correlative crystal ﬁeld can refer to those papers. Indeed, the effects of lattice vibration on the energy levels cannot be neglected. However, we will discuss the effect of the crystal ﬁeld in a static lattice ﬁrst and then deal with the effects of lattice vibration. On the other hand, for a general purpose, we will not calculate the crystal ﬁeld splitting of different mechanisms separately, but use a phenomenological parameter method to summarize all the splitting effects caused by different mechanisms. Equation (2.48) is a general expression and valid not only for rare earth ions but also for transition-metal ions, because spherical harmonic functions CqðkÞ are orthogonal basis functions in a completed space and any function can be expanded by these functions. The expanded coefﬁcients Bkq are the so-called crystal ﬁeld parameters in general crystal ﬁeld theory. By using electrostatic model, one can obtain an expression of parameter Bkq. Classically, it is supposed that the charge distribution among lattice ions in the environment will not overlap with that of the

3.1 Crystal Field on the Active Ions

71

electrons in the active ions and so can comply with Laplace equation. Thus the crystal ﬁeld potential can be written as Hc ¼

XZ

ds

i

eqðRÞ j R ri j

where the summation is over the electrons at different position ri, and q(R) is the external charge distribution density. The related potential should be integrated over all the crystal. On the other hand, jR ri j1 can be expanded as jR ri j1 ¼

1 X rhk

P ðcos xi Þ kþ1 k k¼0 ri

where xi is the angle between the radius vector of external charge described by spherical coordinates R, H, U and the radius vector of the electron described by spherical coordinates ri, hi, /i in the active ion. r< and r> is the shorter and longer between R and ri, respectively. On the other hand, Pk ðcos xi Þ ¼

k X

ð1Þq

q¼k

¼

k X

4p Y k;q ðH; UÞY kq ðhi ; ui Þk 2k þ 1

ðk Þ ð1Þq Cq ðH; UÞCqðkÞ ðhi ; ui Þ

q¼k

If Hc is written as Hc ¼

X

Bkq

X

CqðkÞ ðhi ; /i Þ

ð3:2Þ

i

kq

then Z Bkq

¼ e

ð1Þ

q

rhk k qðRÞCq ðH; UÞ k þ 1 ri

ð3:3Þ

ds

Neglecting the electron overlapping effect as well as the exchanging and covalent ones between electrons in adjacent ions, one always has jRjijri j; then Z Bkq ¼ e

ð1Þ

q

ðk Þ qðRÞCq ðH; UÞ

rik

Rk þ 1

" ds ¼ e

Z ds

# ðk Þ ð1Þq qðRÞCq ðH; UÞ Rk þ 1

rik

ð3:4Þ

72

3 Rare Earth Ions in Materials

In the calculation of energy level splitting caused by the crystal ﬁeld, the crystal ﬁeld Hamiltonian has been integrated over electronic wave functions so that the crystal ﬁeld parameter can be expressed as Z Bkq ¼ e

ds

ðk Þ ð1Þq qðRÞCq ðH; UÞ k r k þ 1 R

ð3:5Þ

where k r ¼

Z1 drR24f ðr Þr 2

ð3:6Þ

0

In (3.6), R4f is electronic radial wave function. It should be noted that both (3.2) and (2.49) are universally valid, but the detailed expression of Bkq, that is, (3.5) is only valid under a special assumption of electrostatic model. There is a factor lC ðkÞ li in the matrix elements of crystal ﬁeld potential. Therefore, according to (2.49) and the triangle condition of 3-j symbol or the triangle rule of the angular momentum coupling, for transition-metal ions l = 2, one need to consider only 0 k 4, and for rare earth ions l = 3, then 0 k 6 should be satisﬁed. For the crystal ﬁeld splitting, the energy levels concerned all have the same parity, and k can only be even. The symmetry group of the active ions will also impose restrictions on the number of crystal ﬁeld parameters. The energy level structure has a big difference between the rare earth ions and the transition metal ions and so we would like to discuss only the former case in this chapter. The energy level structure of the transition metal ions will be discussed in Chap. 7.

3.2

Energy Level Splitting of the Rare Earth Ions

It was mentioned in the previous section that the crystal ﬁeld action on the rare earth ions in materials could be seen as a perturbation on the free ions. Hence, in order to calculate the energy level splitting of the rare earth ions, one can use the wave functions (more accurately, it should be intermediate-coupling wave functions) of free ions as the zero-order approximate wave functions. According to the crystal ﬁeld, wave functions are expanded as the bases of irreducible representation of rotation group or those of point group, and the method of crystal ﬁeld can be divided into two classes. In the ﬁrst class, that is the traditional crystal ﬁeld method, the basis functions used are the bases of rotation group irreducible representation. This traditional crystal ﬁeld method can be further divided into two kinds. The ﬁrst kind uses the Hamiltonian expansion (3.2) or (2.49) and, by means of the calculation method introduced in the last chapter, we can calculate matrix elements

3.2 Energy Level Splitting of the Rare Earth Ions

73

between energy levels and then solve the secular equation. The second kind of traditional crystal ﬁeld method is different from the ﬁrst only in the bases used. They are the eigenfunctions of equivalent angular momentum operators and so this method is called equivalent operator method. If Hc is expressed as X X Hc ¼ Akm Pkm ðri Þ ð3:7Þ km

i

The following replacement is usually carried out X

X X P2m ðri Þ ! aJ r 2 O2m ; P4m ðri Þ ! bJ r 4 O4m ; P6m ðri Þ ! cJ r 6 O6m

i

i

i

ð3:8Þ The equivalent operators Okm are obtained by replacing x, y, z in Pkm(r) (k = 2, 4, 6) by Jx, Jy, Jz. The matrix elements of the polynomial Pkm(r) and equivalent operator Okm can be found in Hufner’s book (1978) [7]. In order to correctly calculate the equivalent operator factors aJ, bJ, cJ, the intermediate-coupling approach should be considered [8, 9]. For most of the rare earth ions, these factors can also be found directly from tables [9]. This method has the advantage of direct and simple, but it cannot take into account of the mixing effect of free ion state’s functions belonging to different J values (J mixing effect). If the crystal ﬁeld is very strong, this effect can introduce a big error in the calculations of energy levels. By using the above two methods, the number of crystal ﬁeld parameters should be determined by the restrictions of the point symmetry at the site of active ions, that is, by the symmetry conditions and some of the parameters will be zero. In the following we will introduce the method for obtaining the crystal ﬁeld parameters in different point symmetry conditions. In the case of rare earth ions, as having been pointed out, 0 k 6, (3.2) can be written as Hc ¼

6 X k X ðk Þ Bkq CqðkÞ þ Bk;q Cq

ð3:9Þ

k¼0 q¼0

Note that writing in this form the terms with q = 0 have been repeatedly calculated and so the extra term should be eliminated. Bkq is usually a complex number and can be written as Bkq = RBkq + iIBkq, with real part RBkq and imaginary part IBkq. In order to ensure that the crystal ﬁeld potential is a real number, the real and imaginary parts of the crystal ﬁeld parameters should satisfy the following relations: RBkq ¼ ð1Þq RBkq ; IBkq ¼ ð1Þq þ 1 IBkq

ð3:10Þ

74

3 Rare Earth Ions in Materials

In the introduction of (3.10), the following relations have been used

1=2 4p q ðk qÞ! ðk Þ Cq ¼ r k Pkq ðcoshÞeiqu Ykq ðh; uÞ ¼ ð1Þ 2k þ 1 ðk þ qÞ! It can be shown1 1

The associated Legendre polynomial is deﬁned as Pkq ðcoshÞ Pkq ð xÞ ¼

ð1 x2 Þ 2k k!

q=2

k dk þ q 1 x2 where x ¼ cos h dxk þ q

in which þq k kX dk þ q 2 x 1 ¼ dxk þ q r¼0

where

kþq r

kþq r

dr dk þ qr ðx 1Þk k þ qr ðx þ 1Þk dxr dx

qÞ! r!ððkkþþqr Þ!

k þ qr Because ddxk þ qr ðx þ 1Þk ¼ 0 when r < q, after differential we have

k k X dk þ q 2 x 1 ¼ dxk þ q r¼q

kþq r

k! k! ðx 1Þkr ðx þ 1Þrq ðkr Þ! ðr qÞ!

r in the above expressions is a summing index, and one can make a replacement r ¼ r 0 þ q; then the expression changes into kþq

kq k X dk þ q 2 x 1 ¼ dxk þ q r 0 ¼0

!

0 k! k! ðx 1Þkqr 0 ðx þ 1Þr ðk q r 0 Þ! r! ! kq kq q X 0 0 ðk þ qÞ! 2 k! k! ðx 1Þkr 0 ðx þ 1Þr þ q x 1 ¼ 0 Þ! 0 ð ð þ q Þ! ðk qÞ! k r r 0 r r ¼0

r0 þ q

¼ ð1Þq

Pkq ð xÞ ¼

ð1 x2 Þ 2k k!

¼ ð1Þq

q=2

q dkq 2 k ðk þ qÞ! 2 x 1 x 1 dxkq ðk qÞ!

k ð1 x2 Þ dk þ q 1 x2 ¼ dxk þ q 2k k!

ðk þ qÞ! ð1 x2 Þ ðk qÞ! 2k k!

q=2

q=2

ð1Þq

q dkq 2 k ðk þ qÞ! 2 x 1 x 1 ðk qÞ! dxkq

dkq ðk þ qÞ! Pkq ð xÞ 1 x2 ¼ ð1Þq ðk qÞ! dxkq

Therefore Pkq ðcoshÞ ¼ ð1Þq

ðk þ qÞ! Pkq ðcoshÞ ðk qÞ!

3.2 Energy Level Splitting of the Rare Earth Ions

Pkq ðcoshÞ ¼ ð1Þq

75

ðk þ qÞ! Pkq ðcoshÞ ðk qÞ!

so that

CqðkÞ

ðk Þ ¼ ð1Þq Cq

Therefore, we have the following expression Hc ¼

6 X k n X

h i h io ðk Þ ðk Þ RBkq CqðkÞ þ ð1Þq Cq þ iIBk;q CqðkÞ þ ð1Þq þ 1 Cq

k¼0 q¼0

6 X k X

kq Vkq þ V

ð3:11Þ

k¼0 q¼0

We name the coefﬁcient Nkq as þ qÞ! Nkq ¼ ð1Þ2q ððkkq Þ! 1=2

Vkq ¼ Nkq r k Pkq ðcoshÞcos q/RBkq kq ¼ N 1=2 r k Pkq ðcoshÞsin q/IBkq V kq

From the above expression of Pkq ðcoshÞ; we have Pkq ½cosðp hÞ ¼ Pkq ðcoshÞ ¼ ð1Þk þ q Pkq ðcoshÞ and 2q=n e2piq=n ¼ epi ¼ ð1Þ2q=n In this way we can introduce the restriction condition of crystal parameters under the symmetry operation as shown in Table 3.1 given by Sachs [10]. As two examples, we will investigate the cases of point groups D3 and D3d. The point group D3 consists of three classes, that is, E, C3, and U2 (C2 axis which is perpendicular to the principal axis). We ﬁrst study the real crystal ﬁeld components. It can be seen from Table 3.1 that the invariance requirements are: (I) q = 3m; (II) k + 2q/3 + q = 2m. By requirement (I), it is necessary that q is an integer multiple of 3 and can only be 0, 3, 6 and so on. For even k, in order to satisfy the requirement (II), 2q/3 + q should be even. It is easy to see that in this case q should be

kq V None

kq invariance requirement V

ð1Þk þ q Vkq k + q = 2m

ð1Þ n Vkq q = nm 2q

2q

(p − h, /)

(h, / + 2p/n)

rh

kq kq ð1Þk þ q V ð1Þ n V k + q = 2m q = nm a n is the order of rotation and m is an integer, 0, 1, 2, …

ðh; /Þ Vkq None

(h, /) ! Vkq invariance requirement

Symmetry operation E Cn

kq V Vkq ¼ 0

(h, −/) Vkq None

rv

q

kq ð1Þn þ 1 V q = n(2m − 1)

q

ð1Þn Vkq q = 2nm

(h, −/ + p/n)

rd ðnÞa

2q

kq ð1Þk þ n þ 1 þ q V k + 2q/n + q = 2m − 1

2q

ð1Þk þ n þ q Vkq k + 2q/n + q = 2m

(p−h, − / + 2p/n)

U2 ðnÞa

Table 3.1 Invariance requirements for the crystal ﬁeld components under typical point group operations (m = 0, 1 …) [10] Sn

2q

kq ð1Þk þ n þ q V k + 2q/n + q = 2m

2q

ð1Þk þ n þ q Vkq k + 2q/n + q = 2m

(p − h, / + 2p/n)

76 3 Rare Earth Ions in Materials

3.2 Energy Level Splitting of the Rare Earth Ions

77

an integer multiple of 6 and can be written as q = 6m, which satisfy the requirement (I) as well; for odd k, in order to satisfy the requirement (II), 2q/3 + q should be odd and can be 3, 9, 15, …, which also satisfy requirement (I) and can be written as q = 6m − 3. Secondly, for the imaginary part of crystal ﬁeld parameters the invariance requirements are: (I) q = 3m; (II) k + 2q/3 + q + 1 = 2m. It is easy to ﬁnd the conditions for the non-zero crystal ﬁeld components: for even k, q = 6m − 3, for odd k, q = 6m. In this chapter, we will only concern with energy level splitting and discuss only the effects of even components of crystal ﬁeld. For the rare earth ions, as has been pointed out, even k can only be 2, 4, and 6. Therefore, in case of D3 point group symmetry, the real crystal ﬁeld components will be Vk0 (k = 2, 4, 6) and V66 corresponding to crystal ﬁeld parameters Bk0 (k = 2, 4, 6) and B66. On the other hand, the imaginary components of crystal ﬁeld parameters are: IB43 and IB63. In the following table it is simply written as B43 and B63. The point group D3d is the direct product of D3 and Ci S2. The crystal ﬁeld invariance requirements for D3d are those for D3 plus that for S2, which is k + 2q = 2m. It practically requires that k should be an even number. Therefore, as far as the even crystal ﬁeld is concerned, the crystal ﬁeld parameters are the same for the cases D3d and D3. The even crystal ﬁeld parameters for 32 point groups are shown in Table 3.2. Table 3.2 Even crystal ﬁeld parameters for 32 point groups Point group

Crystal ﬁeld parameters

Point group

Crystal ﬁeld parameters

C1, Ci

All Bkq except Bk0 (k = 2, 4, 6) are real, others are complex Bk0 (k = 2, 4, 6) are real, B22, B4q(q = 2, 4), B6q (q = 2, 4, 6) are complex

C3, S6(C3i) D2, C2v, D2h C6, C3h C6h C6v, D3h, D6h D6 D3 D3d

Bk0 (k = 2, 4, 6) are real, B43, B63, and B66 are complex Bk0 (k = 2, 4, 6), B22, B4q (q = 2, 4) and B6q (q = 2, 4, 6) are all real Bk0 (k = 2, 4, 6) are real, B66 is complex

C2, Cs(C1h), C2h C4, S4 C4h

Bk0 (k = 2, 4, 6) are real, B44 and B64 are complex

D4, C4v D2d, D4h

Bk0 (k = 2, 4, 6), B44, B64 are all real

T, O Td, Oh, Th

Bk0 (k = 4, 6), B44, and B64 are all real, and only two independent parameters. In qﬃﬃ ﬃ B , B64 ¼ 27B60 this case: B44 ¼ p5ﬃﬃﬃ 70 40

C3v

Bk0 (k = 2, 4, 6), B66 are all real

Bk0 (k = 2, 4, 6) and B66 are all real, B43, B63 are imaginary

Bk0 (k = 2, 4, 6), B43, B63, B66 are all real Note All the complex numbers have both imaginary and real parts, and they include two parameters

78

3 Rare Earth Ions in Materials

Table 3.3 Ratio of crystal ﬁeld parameters used in the two traditional crystal ﬁeld methods

k

Q

Bkq Akq r k

2 2

0 2

2 pﬃﬃﬃ 6 3

4 4

0 2

4

3

4

4

8 pﬃﬃﬃﬃﬃ 2 10 5 pﬃﬃﬃﬃﬃ 2 35 35 pﬃﬃﬃﬃﬃ 4 70 35

6 6

0 2

6

3

6

4

6

6

16 pﬃﬃﬃﬃﬃﬃﬃﬃ 16 105 105 pﬃﬃﬃﬃﬃﬃﬃﬃ 8 105 105 pﬃﬃﬃﬃﬃ 8 14 21 pﬃﬃﬃﬃﬃﬃﬃﬃ 16 231 231

The basic functions having the same k and q values in the two traditional crystal ﬁeld methods are different by a constant factor and so do their crystal ﬁeld parameters. The ratio between their crystal ﬁeld parameters is listed in Table 3.3. The energy level splitting of rare earth ions in a crystal ﬁeld can be obtained by using the method introduced in the last chapter, and the results are listed in Table 3.4. It can be seen that the energy level of even number electronic system has no Kramers degeneracy. When the site symmetry of rare earth ions belongs to 8point groups of triclinic, monoclinic, and rhombic crystal systems, the energy level of even number electronic system has no any degeneracy; but if their site symmetry is higher, the degeneracy of some energy levels is completely removed while the others remain twofold or threefold degeneracy, as shown in the following table. For the odd number electronic system, the crystal ﬁeld energy level number are all equal to J + 1/2, and each crystal ﬁeld energy level has only twofold Kramers degeneracy, except for the site symmetry of rare earth ion belongs to 5 cubic point groups. All the crystal ﬁeld energy levels of rare earth ion site in the 5 cubic symmetric point group position still have twofold Kramers degeneracy while some of the crystal ﬁeld energy levels have both the twofold crystal ﬁeld degeneracy and twofold Kramers degeneracy, thus form the fourfold degeneracy energy levels. The values of x and y in Table 3.4 are obtained by the relations J ¼ x þ 6k and J ¼ y þ 3k (k = 0, 1, 2, …). The square bracket in this table indicates that in case an integer number is obtained this integer should be taken, but if a non-integer number is obtained, then the next smaller integer number should be taken. x

012345

y

1/2 3/2 5/2

u1(x) u2(x)

100110 001011

u(y)

1

0

1

3.2 Energy Level Splitting of the Rare Earth Ions

79

Table 3.4 The relationship between the energy level splitting and the symmetry of crystal ﬁeld [7] Symmetry/Total angular momentum Triclinic C1, Ci Monoclinic Cs, C2, C2h Rhombic C2v, D2, D2h Trigonal C3, S6, C3v, D3, D3d HexagonalC3h, C6, C6h, D3h, C6v, D6, D6h Tetragonal S4, C4, C4h, D2d, C4v, D4, D4h Cubic T, Th, Td, O, Oh

J: 0, 1, 2, 3, 4, 5,

…

1, 3, 5, 7, 9, 11, …,

1, 1, 1, 3, 3, 3, 0, 1, 2, 2, 3, 4,

…, …,

1, 1, 3, 3, 5, 5, …, 0, 1, 1, 2, 2, 3, …, 1, 0, 0, 1, 1, 0, …, 0, 0, 1, 0, 1, 1, …, 0, 1, 1, 2, 2, 3, …, Symmetry/Total angular momentum J: 1/2, 3/2, 5/2, 7/2, 9/2, 27 point group except cubic 1, 2, 3, 4, 5, 1, 0, 1, 2, 1, Cubic T, Th, Td, O, Oh 0, 1, 1, 1, 2, Note p is the degeneracy of the level and functions u(x1), u(x2),

P 2J + 1

1

2[J/3] + 1 [(2J − 1)/3] + 1

1 2

2[J/2] + 1 1 [(J + 1)/2] 2 1 u1(x) + [J/6] 2 u2(x) + [J/6] [(J + 1)/2] 3 11/2, …, 2J + 1 P 6, …, J + 1/2 2 2, …, u(y) + [J/3] 2 2, …, [(J + (3/2))/3] 4 and u(y) are given as follows

The research work on the crystal ﬁeld of rare earth ions has two approaches. The ﬁrst is by calculating the crystal ﬁeld parameters through ﬁtting values of energy level splitting obtained from spectroscopy experiments to the eigenvalues of crystal ﬁeld Hamiltonian. The second is by calculating the crystal ﬁeld parameters using some kind of theoretical models. The second approach is not really a successful example, although many scientists have done a lot of work and proposed several kinds of theoretical models. This is because the crystal ﬁeld effect is a complicated effect involving many mechanisms. However, the calculation results of the simple point charge model considering the shielding effect can be used as staring values for crystal ﬁeld ﬁtting. If the crystal ﬁeld parameters of the point charge model are denoted by B0kq , then the reasonable starting values for the crystal ﬁeld ﬁtting can be expressed as Bkq and Bkq ¼ ð1 rk ÞB0kq . The value of r2 is about 0.8, r4 and r6 are about 0.1 [11], and some recent calculation even shows that r2 approaches 0.9 [2]. The crystal ﬁeld ﬁtting is generally divided into the following steps: 1. Estimate initial values of the crystal ﬁeld parameters; 2. Construct the energy matrix using estimated or referenced crystal ﬁeld parameters; 3. The estimation eigenvalues of the energy level are obtained by diagonalization of the matrix; 4. Establish a one-to-one correspondence between the experimental and calculated level positions; 5. Keep the eigenvector of the energy matrix ﬁxed and determine the crystal ﬁeld parameter values to minimize the mean square deviation between the experiment and the calculation energy levels; 6. Substitute the crystal ﬁeld parameters obtained in the ﬁfth step to the second step, and repeat second to ﬁfth step until the difference of calculated and experimental energy levels reaches the minimum. By using ﬁtting method, crystal ﬁeld analyses have been carried out for many crystals doped with rare earth ions and there is a large number of data of energy

80

3 Rare Earth Ions in Materials

Table 3.5 Crystal ﬁeld parameters of trivalent rare earth ions in yttrium aluminum garnet crystals [12] R3+

B20

B21

B40

B42

B44

B60

B62

B64

B66

Nd Nd Sm Sm Eu Tb Dy Dy Dy Er Er

514 424 502 599 627 461 492 504 502 424 401

129 101 95 −356 56 165 89 72 73 82 53

−363 −191 800 394 −344 −169 −60 −71 −77 −288 −107

−2005 −2108 −1542 −1464 −1611 −1720 −1743 −1737 −1771 −1522 −1591

−950 −1082 −1003 −212 −817 −900 −852 −895 −906 −899 −717

−1702 −1784 −1386 −315 −1437 −1324 −1140 −1171 −1164 −1122 −1021

−763 −681 −650 −481 −608 −621 −434 −454 −446 −303 −349

837 868 917 684 600 599 557 576 552 492 538

−718 −641 −542 −633 −632 −561 −462 −425 −432 −322 −404

Table 3.6 Crystal ﬁeld parameters of trivalent rare earth ions in yttrium lithium fluoride [12]

R3+

B20

B40

B44

B60

RB64

IB64

Pr Pr Nd Nd Nd Nd Dy Ho Er Er Er Er Tm Tm Yb

489 485 441 480 502 401 330 410 400 314 190 380 359 333 281

−1043 −1061 −906 −973 −962 −1088 −704 −615 −692 −625 −1184 −640 −608 −648 −556

1242 1296 1115 1119 1105 1230 937 819 925 982 858 975 844 867 569

−42 −57.5 −26.3 −60.6 −27.4 30 −70.4 −27.9 −21.3 −32.4 −44.8 −36.8 −173 −141 −106

1213 1186 1073 1051 1019 1074 609 677 610 584 295 599 629 623 840

22.5 0 20.6 49.0 35 0 92.7 32.8 149 171 0 99.8 0 3 953

level and crystal ﬁeld parameter in the literature. For example, in the Morrison and Leavitt’s work [12], the energy level and crystal ﬁeld parameter data for rare earth ions in 26 crystals are reported. Many data of a series of rare earth ions in different laser crystals can be found in Kaminskii’s books [13, 14]. In Tables 3.5 and 3.6, data for two typical laser crystals are listed. It can be seen from these tables that different rare earth ions have nearly the same crystal ﬁeld parameters. It should be pointed out that the two methods mentioned above have a common disadvantage, that is, their crystal ﬁeld Hamiltonian and related eigenfunctions are expanded in terms of basis functions of the rotation group and so the site symmetry

3.2 Energy Level Splitting of the Rare Earth Ions

81

properties of the electronic wave function cannot be directly determined. This increases the indeﬁniteness and the amount of work in identiﬁcation of the spectral lines. There are two methods to remedy this limitation. One is to introduce crystal ﬁeld quantum number which is related to irreducible representation of point group. By using the ﬁxed relationship between the crystal ﬁeld quantum number and the magnetic quantum number, the irreducible representation of the electronic wave function can be determined. The second way is to expand the crystal ﬁeld Hamiltonian and related eigenfunctions in terms of the basis functions of point group. By the second method, the crystal ﬁeld Hamiltonian and the eigenfunctions are designated by a series of irreducible representations of the group-chain with the symmetry reduced step by step. This method is hereby called group-chain scheme of crystal ﬁeld analysis.

3.3

Crystal Field Quantum Number

In the study of crystal electronic energy level, Hellwege in 1948 [15] introduced crystal ﬁeld quantum number according to the following fundamental expression: M ¼ lð mod qÞ ) M ¼ l þ kq;

k ¼ 0; 1; 2; . . .

The value of q is the order of highest symmetry axis of international point group symbol or the crystal system, that is, triclinic q = 1; monoclinic and rhombic q = 2; trigonal q = 3; tetragonal q = 4; hexagonal q = 6, for example C2(2), Cs(m), D2(222), C2v(mm2), D2h(2/m)—q = 2; C3v(3m), D3(32)—q = 3; 6m2), D4(422), C4v(4mm), S4(4), D2d(4m2)—q = 4; D6(622), C6v(6mm), D3h( C3h(6)—q = 6. For an odd number electronic system, from the M composition of the wave function, the crystal ﬁeld quantum number l can be determined and then the point group irreducible representation can be found, because in this case one l value corresponds to one irreducible representation. Therefore, by means of crystal ﬁeld quantum number, one can judge the irreducible representation character of energy level after their wave function is calculated by usual crystal ﬁeld analysis. However, for an even number electronic system, it happens for many point groups, only one crystal ﬁeld quantum number l cannot completely determine the irreducible representation of the wave function, that is, one l value corresponds to two different irreducible representations and the wave function should be completely characterized by crystal ﬁeld quantum number l and m. According to the deﬁnition of Hellwege [15], the wave function transforms as w(−x, y,−z) = eipmw(x, y, z) by the rotation around y axis through an angle p, on the other hand, the reflection in the plane xz equal to the rotation around y axis through an angle p plus the inversion through the symmetry center, that is, one has the relation w(x, −y, z) = eipmIw(x, y, z), where I is the parity of the wave function. For the even electronic system I = +1 so that one also has wðx; y; zÞ ¼ eipv wðx; y; zÞ: Therefore, for Cnv point group and Dn point group, the same crystal ﬁeld quantum numbers can be used to describe the relation between

82

3 Rare Earth Ions in Materials

the wave function and the irreducible representation. In this case, S = eipm in [15]. On the other hand, because D2h = D2 ⊗ Ci, the relation between the quantum number of wave function and the irreducible representation for point group D2h is similar to that of the point group D2; the only difference is that the group D2h has both even irreducible representation C+i and odd irreducible representation C−i . The crystal ﬁeld quantum number l for an even number electronic system and the crystal ﬁeld quantum number l, m for an odd number electronic system with wave functions of JZ M are listed in the following to supplement the deﬁciency of many books in this ﬁeld. 1. C2, Cs point groups q = 2. See Tables 3.7 and 3.8. Table 3.7 Correspondence of crystal ﬁeld quantum numbers and irreducible representations with magnetic quantum number M of wave function and energy level number N for odd number electronic system l ¼ 1=2 (C3, C4 conjugate forming a twofold degeneracy energy level) J M ±1/2 ±1/2, 3/2 ±5/2, ±1/2, 3/2 ±5/2, ±1/2, 3/2, 7/2 ±9/2, ±5/2, ±1/2, 3/2, 7/2 ±9/2, ±5/2, ±1/2, 3/2, 7/2, 11/2 ±13/2, ±9/2, ±5/2, ±1/2, 3/2, 7/2, 11/2 ±13/2, ±9/2, ±5/2, ±1/2, 3/2, 7/2, 11/2, 15/2

1/2 3/2 5/2 7/2 9/2 11/2 13/2 15/2

N 1 2 3 4 5 6 7 8

Table 3.8 Correspondence of crystal ﬁeld quantum numbers and irreducible representations with magnetic quantum number M of wave function and energy level number N for even number electronic system C1—l ¼ 0; C2—l ¼ 1 J l M 0 1 2 3 4

0 0 1 0 1 0 1 0 1

0 0 −1, −2, −1, −2, −3, −4, −3,

+1 0, +2 +1 0, +2 −1, +1, 3 −2, 0, +2, +4 −1, +1, 3

N

J

l

M

1 1 2 3 2 3 4 5 4

5

0 1 0 1 0 1 0 1

−4, −5, −6, −5, −6, −7, −8, −7,

6 7 8

N −2, −3, −4, −3, −4, −5, −6, −5,

0, +2, +4 −1, +1, +3, +5 −2, 0, +2, +4, +6 −1, +1, +3, +5 −2, 0, +2, +4, +6 −3, −1, +1, +3, +5, +7 −4, −2, 0, +2, +4, +6, +8 −3, −1, +1, +3, +5, +7

5 6 7 6 7 8 9 8

3.3 Crystal Field Quantum Number

83

2. D2, C2v point groups q = 2. See Tables 3.9 and 3.10. Table 3.9 Correspondence of crystal ﬁeld quantum numbers and irreducible representations with magnetic quantum number M of wave function and energy level number N for odd number electronic system l ¼ 1=2 (C5) J M

N

±1/2 ±1/2, 3/2 ±5/2, ±1/2, 3/2 ±5/2, ±1/2, 3/2, 7/2 ±9/2, ±5/2, ±1/2, 3/2, 7/2 ±9/2, ±5/2, ±1/2, 3/2, 7/2, 11/2 ±13/2, ±9/2, ±5/2, ±1/2, 3/2, 7/2, 11/2 ±13/2, ±9/2, ±5/2, ±1/2, 3/2, 7/2, 11/2, 15/2

1/2 3/2 5/2 7/2 9/2 11/2 13/2 15/2

1 2 3 4 5 6 7 8

Table 3.10 Correspondence of crystal ﬁeld quantum numbers and irreducible representations with magnetic quantum number M of wave function and energy level number N for even number electronic system C1—l ¼ 0, m = 0; C3—l ¼ 0, m = 1; C2—l ¼ 1, m = 0; C4—l ¼ 1, m = 1 J l m M N J l m M 0 1

2

3

4

0 0 1 1 0 0 1 1 0 0 1

0 1 0 1 0 1 0 1 0 1 0

0 0 −1, −1, −2, −2, −1, −1, −2, −2, −3,

0 0 1 1 0 0 1 1 0 0 1

0 1 0 1 0 1 0 1 0 1 0

1

1

−3, −1, +1, +3

2

1

1

0

0

3

0

1

−4, −2, 0, +2, +4 −4, −2, +2, +4

0

0

2

0

1

1

0

−3, −1, +1, +3

2

1

0

1

1

−3, −1, +1, +3

2

1

1

+1 +1 0, 2 +2 +1 +1 +2 0, +2 −1, +1, 3

1 1 1 1 2 1 1 1 1 2 2

5

6

7

8

−4, −2, +2, +4 −4, −2, 0, +2, +4 −5, −3, −1, +1, +3, +5 −5, −3, −1, +1, +3, +5 −6, −4, −2, 0, +2, +4, +6 −6, −4, −2, +2, +4, +6 −5, −3, −1, +1, +3, +5 −5, −3, −1, +1, +3, +5 −6, −4, −2, +2, +4, +6 −6, −4, −2, 0, +2, +4, +6 −7, −5, −3, −1, +1, +3, +5, +7 −7, −5, −3, −1, +1, +3, +5, +7 −8, −6, −4, −2, 0, +2, +4, +6, +8 −8, −6, −4, −2, +2, +4, +6, +8 −7, −5, −3, −1, +1, +3, +5, +7 −7, −5, −3, −1, +1, +3, +5, +7

N 2 3 3 3 4 3 3 3 3 4 4 4 5 4 4 4

84

3 Rare Earth Ions in Materials

In Table 3.10 there are some cases where two different l, m sets (corresponding to two wave functions with two different irreducible representations) have the same M component set. For example, if J = 2, two wave functions constituted by the same M = −1 and M = +1 component set corresponds to two different irreducible representations C2 ðl ¼ 1; v ¼ 0Þ and C4 ðl ¼ 1; v ¼ 1Þ: It means that this component set forms two linear combinations of u(2, −1) and u(2, 1) corresponding to two irreducible representations C2 and C4. One can ﬁnd out their irreducible representation according to their transformation character. For the D2 point group, the wave function u(J, M) transformed by U2 is U2 uðJ; MÞ ¼ ð1ÞJ þ M uðJ; MÞ (because U2 Y MM ðh; uÞ ¼ Y JM ðp h; p uÞÞ: In this example one has 1 1 1 1 w1 ¼ pﬃﬃﬃ uð2; 1Þ þ pﬃﬃﬃ uð2; 1Þ; w2 ¼ pﬃﬃﬃ uð2; 1Þ pﬃﬃﬃ uð2; 1Þ 2 2 2 2 In this case U2 uð2; 1Þ ¼ uð2; 1Þ; U2 uð2; 1Þ ¼ uð2; 1Þ; therefore, U2 w1 ¼ w1 and U2 w2 ¼ w2 . By the character table D2 point group in Appendix B, it can be decided that w1 has irreducible representation C4, that is l ¼ 1; m = 1, on the other hand, w2 has irreducible representation C2, that is l ¼ 1; m = 0. 3. C3v, D3 point groups q = 3. See Tables 3.11 and 3.12. Table 3.11 Correspondence of crystal ﬁeld quantum numbers and irreducible representations with magnetic quantum number M of wave function and energy level number N for odd number electronic system J

l ¼ 1=2 (C4) M

l ¼ 3=2 (C5,C6) M

1/2 3/2 5/2 7/2 9/2 11/2 13/2 15/2

±1/2 ±1/2 5/2, ±1/2 5/2, ±1/2, ±7/2 5/2, ±1/2, ±7/2 11/2, 5/2, ±1/2, ±7/2 11/2, 5/2, ±1/2, ±7/2, ±13/2 11/2, 5/2, ±1/2, ±7/2, ±13/2

±3/2 ±3/2 ±3/2 ±3/2, ±3/2, ±3/2, ±3/2,

±9/2 ±9/2 ±9/2 ±9/2, ±15/2

N 1 2 3 4 5 6 7 8

3.3 Crystal Field Quantum Number

85

Table 3.12 Correspondence of crystal ﬁeld quantum numbers and irreducible representations with magnetic quantum number M of wave function and energy level number N for even number electronic system C1—l ¼ 0, m = 0; C2—l ¼ 0, m = 1; C3—l ¼ 1 J l m M N J l

m

M

N

0 1

0 1

−3, +3 −3, 0, +3 5, 2, ±1, ±4 −6, −3, 0, +3, +6 −6, −3, +3, +6 5, 2, ±1, ±4 −6, −3, +3, +6 −6, −3, 0, +3, +6 5, 2, ±1, ±4, ±7 −6, −3, 0, +3+6 −6, −3, +3+6 8, 5, 2, ±1, ±4, ±7

1 2 4 3 2 4 2 3 5 3 2 6

2 3

4

0 0 ±1 0 ±1 0 0 ±1 0

0 1 0 0 1 0 1

±1

0 0 ±1 0 2, ±1 −3, +3 −3, 0, +3 2, ±1 −3, 0, +3 −3, +3 2, ±1, ±4

1 1 1 1 2 1 2 2 2 1 3

5

6

7

8

0 0 ±1 0 0 ±1 0 0 ±1 0 0 ±1

0 1 0 1 0 1

4. D4, C4v, D2d, S4 point groups q = 4. See Tables 3.13 and 3.14. Table 3.13 Correspondence of crystal ﬁeld quantum numbers and irreducible representations with magnetic quantum number M of wave function and energy level number N for odd number electronic system J

l ¼ 1=2 (D4, C4v, D2d − C6; S4 − C5, C6)) M

l ¼ 3=2 (D4, C4v, D2d − C7; S4−C7, C8) M

1/2 3/2 5/2 7/2 9/2 11/2 13/2 15/2

±1/2 ±1/2 ±1/2 ±1/2, ±9/2, ±9/2, ±9/2, ±9/2,

±3/2 ±3/2, 5/2 ±3/2, 5/2 ±3/2, 5/2 ±11/2, ±3/2, 5/2 ±11/2, ±3/2, 5/2, 13/2 ±11/2, ±3/2, 5/2, 13/2

7/2 ±1/2, ±1/2, ±1/2, ±1/2,

7/2 7/2 7/2 7/2, 15/2

N

1 2 3 4 5 6 7 8

86

3 Rare Earth Ions in Materials

Table 3.14 Correspondence of crystal ﬁeld quantum numbers and irreducible representations with magnetic quantum number M of wave function and energy level number N for even number electronic system C1—l ¼ 0, m = 0; C2—l ¼ 0, m = 1; C3—l ¼ 2, m = 0; C4—l ¼ 2, m = 1; C5—l ¼ 1 For point group S4, only one crystal ﬁeld quantum numberl is enough. In this case m = 0 and m = 1 has no difference, C1—l ¼ 0; C2—l ¼ 2; C3—l ¼ 1; C4—l ¼ 1 J

l

m

M

N

J

l

m

M

N

0

0

0

0

1

5

0

0

−4, +4

1

1

0

1

0

1

0

1

±1

1

±1

±1 2

0

0

±1

3

2 3

0

1

2

0

−2, +2

1

±1

1

2

1

−2, +2

1

2

0

−2, +2

1

0

0

−4, 0, +4

2

2

1

−2, +2

1

0

1

−4, +4

1

0

1

0

1

±1

3, ±1, ±5

3

3, ±1

2

2

0

−6, −2, +2, +6

2

2

0

−2, +2

1

2

1

−6, −2, +2, +6

2

2

1

−2, +2

1

0

0

−4, +4

1

0

1

−4, 0, +4

2

7, 3, ±1, ±5

4

±1

4

−4, 0, +4 3, ±1, ±5

6

7

0

0

−4, 0, +4

2

±1

0

1

−4, +4

1

2

0

−6, −2, +2, +6

2

3, ±1

2

2

1

−6, −2, +2, +6

2

0

0

−8, −4, 0, +4, +8

3

0

1

−8, −4, +4, +8

2

±1 2

0

−2, +2

1

2

1

−2, +2

1

8

±1

7, 3, ±1, ±5

4

2

0

−6, −2, +2, +6

2

2

1

−6, −2, +2, +6

2

Note The energy level number N in the above table is for point group D4, C4v and D2d. C1 energy level of D2d corresponds to C1 energy level of S4, C5 energy level of D2d split into C3 and C4 energy levels of S4. C3 and C4 energy levels of D2d correspond to C2 of S4. The determination of the irreducible representation for the wave function having same M component set can be done by transformation property

5. D6, C6v, D3h, C3 point groups q = 6. See Tables 3.15 and 3.16. Table 3.15 Correspondence of crystal ﬁeld quantum numbers and irreducible representations with magnetic quantum number M of wave function and energy level number N for odd number electronic system J

l ¼ 1=2 (D6, C6v, D3h − C7; C3h − C7, C8) M

1/2

±1/2

3/2

±1/2

l ¼ 3=2 (D6, C6v, D3h − C9; C3h − C11, C12) M

l ¼ 5=2 (D6, C6v, D3h − C8; C3h − C9, C10) M

N

1 ±3/2

2

5/2

±1/2

±3/2

±5/2

3

7/2

±1/2

±3/2

±5/2, 7/2

4

9/2

±1/2

±3/2, 9/2

±5/2, 7/2

5

(continued)

3.3 Crystal Field Quantum Number

87

Table 3.15 (continued) J

l ¼ 1=2 (D6, C6v, D3h − C7; C3h − C7, C8) M

l ¼ 3=2 (D6, C6v, D3h − C9; C3h − C11, C12) M

l ¼ 5=2 (D6, C6v, D3h − C8; C3h − C9, C10) M

N

11/ 2

±1/2, 11/2

±3/2, 9/2

±5/2, 7/2

6

13/ 2

±1/2, 11/2, ±13/2

±3/2, 9/2

±5/2, 7/2

7

15/ 2

±1/2, 11/2±13/2

±15/2, ±3/2, 9/2

±5/2, 7/2

8

Note In literature [6] the l value of ﬁrst column should be exchanged with that of its second column. In literature [16], l ¼ 3=2 and l ¼ 5=2 were mistakenly corresponded to C8 and C9 of D3h, respectively

Table 3.16 Correspondence of crystal ﬁeld quantum numbers and irreducible representations with magnetic quantum number M of wave function and energy level number N for even number electronic system D6, C6v, D3h: C1 ! l ¼ 0; m ¼ 0; C2 ! l ¼ 0; v ¼ 1; C3 ! l ¼ 3; v ¼ 1; C4 ! l ¼ 3; v ¼ 0 C5 ! l ¼ 1 twofold degeneracy level; C6 ! l ¼ 2 twofold degeneracy level C3h; C1 ! l ¼ 0, m is not necessary; C5 and C6 ! l ¼ 1 are two conjugate levels, C3 and C2 ! l ¼ 2 are also two conjugate levels; C4 ! l ¼ 3, m is not necessary J

l

m

M

N

J

l

m

M

N

0

0

0

0

1

5

0

1

0

1

0

1

1

±1 2

3

1

±1

5, ±1

2

1

±2

±2, 4

2 1

0

1

3

1

−3, +3

±1

±1

1

3

0

−3, +3

1

±2

±2

1

0

0

−6, 0, +6

2

0

1

0

1

±1

1

±1

0

0

0

1

±1 ±2

4

0 ±1

6

−6, +6

1

5, ±1

2

±2

1

±2

4, ±2

2

3

1

−3, +3

1

3

1

−3, +3

1

3

0

−3, +3

1

3

0

−3, +3

1

0

0

0

1

0

0

−6, +6

1

1

7

±1

±1

1

0

±2

4, ±2

2

±1

+6, 0, −6

2

5, ±1, ±7

3

3

1

−3, +3

1

±2

4, ±2

2

3

0

−3, +3

1

3

1

−3, +3

1

3

0

−3, +3

1

0

0

−6, 0, +6

2

0

1

+6−6

1

5, ±1, ±7

3

8

±1

4, ±2, ±8

3

3

±2 1

−3, +3

1

3

0

−3, +3

1

The determination of the irreducible representation for the wave functions having same M component sets corresponding to different l and m can be made by the transformation properties under the symmetry operation

88

3 Rare Earth Ions in Materials

The crystal ﬁeld quantum number and the Butler symbol [17] of irreducible representation have a corresponding relationship. For the example of point group C3v and D3, in the case of an even electronic system, l can be 0 and ±1. The energy levels with crystal ﬁeld quantum number l ¼ 0; m = 0 and 1 belong to representations C1 and C2. They are two one-dimensional irreducible representations corresponding to two single energy levels and both have the same quantum number l ¼ 0 but different m. Butler used “0” and ‘~0’ to discriminate them. The energy level of l ¼ 1 belongs to representation C3 and is denoted as “1” by Butler to indicate its twofold degeneracy property. In the case of an odd electronic system, l can only be ±1/2 and ±1/3. The energy levels of l ¼ 1=2 belong to representation C4. A single number “1/2” was used by Butler to not only correspond crystal ﬁeld quantum number but also indicate its twofold degeneracy property. On the other hand, for the energy levels C5 and C6 of l ¼ 3=2; Butler used “3/2” and “−3/2” to indicate that these original two single energy levels are accidental degeneracy to become a twofold degeneracy level. By the typical crystal ﬁeld analysis method, the introduction of crystal ﬁeld quantum number has two advantages: First, by means of crystal ﬁeld quantum number, the order of secular equation can be reduced in the solution of energy level and wave function, because different crystal ﬁeld quantum numbers correspond to different irreducible representations between which the matrix elements of crystal ﬁeld Hamiltonian are zero. For example, if the site symmetry is D3 then to solve the secular equation for energy level with J = 11/2, by means of crystal ﬁeld quantum number in Table 3.11, it can be divided into one 4-order equation with M = 11/2, 5/2, ±1/2, ±7/2 and two 2-order equation with M = ±3/2, ±9/2, while their degeneracy is clear. Secondly, by means of crystal ﬁeld quantum number, the irreducible representation character of wave functions solved in the crystal ﬁeld analysis can be determined and so it is easy to obtain the information data of polarization properties of the emission and absorption spectra between different energy levels. Here is an example of NdAl3(BO3)4 (NAB) crystal. By the typical crystal ﬁeld analysis method, the wave functions of two crystal ﬁeld energy levels of multiplet 4F3/2 and ﬁve crystal ﬁeld energy levels of multiplet 4I9/2 are as follows [18] (all the energy levels are twofold degeneracy):

3.3 Crystal Field Quantum Number 4

89

F3=2 ð1Þ w1 ¼ j1=2i w2 ¼ j1=2i

4

F3=2 ð2Þ w1 ¼ 0:7071ij3=2i 0:7071j 3=2i w2 ¼ 0:7071j3=2i 0:7071ij 3=2i

4

I9=2 ð1Þ w1 ¼ 0:6578j7=2i 0:5706j1=2i 0:4916j 5=2i w2 ¼ 0:6578j 7=2i 0:5706j 1=2i þ 0:4916j5=2i

4

I9=2 ð2Þ w1 ¼ ð0:1575 0:5796iÞj9=2i þ ð0:1575i þ 0:5796Þj 9j2i þ ð0:3576 0:1070iÞj3=2i þ ð þ 0:3576i 0:1070Þj 3=2i w2 ¼ ð0:1575 0:5796iÞj 9=2i þ ð0:1575i þ 0:5796Þj9j2i þ ð0:3576 0:1070iÞ 3=2i þ ð þ 0:3576i 0:1070Þj3=2i 4

I9=2 ð3Þ w1 ¼ ð0:3694 0:0536iÞj9=2i þ ð0:3694i þ 0:0536Þj 9=2i þ ð0:2404 0:5504iÞj3=2i þ ð0:2404i þ 0:5504Þj 3=2i w2 ¼ ð0:3694 0:0536iÞj 9=2i þ ð0:3694i þ 0:0536Þj9=2i þ ð0:2404 0:5504iÞ 3=2i þ ð0:2404i þ 0:5504Þj3=2i

4

I9=2 ð4Þ w1 ¼ 0:9390j7=2i 0:1755j1=2i 0:2957j 5=2i w2 ¼ 0:9390j 7=2i 0:1755j 1=2i 0:2957j5=2i

4

I9=2 ð5Þ w1 ¼ 0:1746j7=2i 0:9842j1=2i þ 0:0295j 5=2i w2 ¼ 0:1746j 7=2i 0:9842j 1=2i þ 0:0295j5=2i

Above are the linear compositions of wave functions with the same total angular momentum quantum number J but different magnetic quantum number M (quantum number J is omitted). From Table 3.11, it can be determined that the crystal ﬁeld quantum number of 4F3/2(1) is l ¼ 1=2; corresponding to irreducible representation C4; the crystal ﬁeld quantum number of 4F3/2(2) is l ¼ 3=2; corresponding to irreducible representations C5, C6; on the other hand, crystal ﬁeld quantum number of energy levels 4I9/2(1), 4I9/2(4), and 4I9/2(5) is l ¼ 1=2 corresponding to irreducible representation C4, while the crystal ﬁeld quantum number of 4I9/2(2) and 4 I9/2(3) is l ¼ 3=2 corresponding to irreducible representations C5, C6. By the irreducible representation correlation of SO3 ! O ! D3 in Appendix B, it can be seen that multiplet J = 3/2 is decomposed into one energy level of irreducible representation C4 and one energy level of irreducible representations C5, C6, while multiplet J = 9/2 decomposed into three energy levels of irreducible representation C4 and two energy levels of irreducible representations C5, C6. This is the same as the result obtained from the wave functions of literature [19] by using crystal ﬁeld quantum number method. (The precise point symmetry of Nd3+ ions in NAB crystal is C2, but in a good enough approximation, it can be described by point group D3 [19].)

90

3 Rare Earth Ions in Materials

In the NAB crystal, the wave functions and crystal ﬁeld quantum numbers as well as their irreducible representations for two crystals ﬁeld energy levels of 4 I11/2(2) and 4I11/2(3) among six energy levels of multiplet 4I11/2 are listed as follows [18] 4

I11=2 ð2Þ w1 ¼ 0:8434j7=2i þ 0:0965j1=2i 0:4182j 5=2i 0:3234j 11=2i w2 ¼ 0:8434j 7=2i þ 0:0965j 1=2i 0:4182j5=2i 0:3234j11=2i l ¼ 1=2 C4 4

I11=2 ð3Þ w1 ¼ ð0:0413 0:6617iÞj9=2i þ ð0:6617 þ 0:0413iÞj 9=2i þ ð0:1651 0:1822iÞj3=2i þ ð0:1822 þ 0:1651iÞj 3=2i w2 ¼ ð0:0413 0:6617iÞ 9=2 [ þ ð0:6617 þ 0:0413iÞj9=2i þ ð0:1651 0:1822iÞj 3=2i þ ð0:1822 þ 0:1651iÞj3=2i ¼ 3=2 C5 ; C6

By using the relation between the crystal ﬁeld quantum number and the magnetic quantum number M of wave function component, the following results can be obtained from the literature [18]: energy levels 4I11/2(1) and 4I11/2(4) both belong to irreducible representation C4; energy level 4I11/2(5) belongs to irreducible representations C5, C6, and energy level 4I11/2(6) also belongs to C4. In Chap. 4, this information will be used to determine the polarization of emission line. It should be pointed out that the irreducible representations of above energy levels are mostly the same as those of Cascales [20] and Jaque [21] obtained by the analysis of NAB crystal spectral lines. The only difference is in energy levels 4 I9/2(3), 4I9/2(4), 4I11/2(2), and 4I11/2(3). One possible reason for this inconsistency is that the D3 point group symmetry of Nd3+ ions in NAB crystal is only an approximation. There is C2 symmetry component in its crystal ﬁeld [18]. In this situation, r and p polarization transitions are all permitted. This will affect the results of energy level irreducible representations determined by the polarization character of spectral lines. It is for this reason, the irreducible representations of energy levels obtained by spectral data of Nd3+:YAl3(BO3)4 (NYAB) crystal, in which Nd3+ ions occupy precisely the D3 symmetry positions [22] has some difference with that of NAB crystal [21].

3.4

Group Chain Scheme Method in Crystal Field Analysis

The main idea of this method is to use a series of irreducible representations of a group–subgroup chain to designate the crystal ﬁeld wave functions and potential Hamiltonian. If the active ions occupy a G group symmetry position, then from SO3

3.4 Group Chain Scheme Method in Crystal Field Analysis

91

(or O3) to G, the group chain will be SO3 (or O3) H1 H2 H3 G. According to the difference in the group G, one can choose the ﬁrst group as SO3 or O3. For example, if G is group D3 then one should select SO3 as the ﬁrst group of the group chain, because group D3 is a subgroup of group O and group O is a subgroup of group SO3, but if G is group D2d then one should select O3 as the ﬁrst group of the group chain, because group D2d is a subgroup of group Td, group Td is a subgroup of group Oh, and group Oh is a subgroup of group O3. In the case of crystal Nd3+:YAl3(BO3)4, Nd3+ ions occupy D3 symmetry positions then the group chain will be SO3 O D3. One can use w(J, l, m, k, n) to describe the energy levels of a multiplet with angular momentum J split by the crystal ﬁeld, where l denotes the irreducible representation (irresp.) of ﬁrst subgroup H1 in the ﬁrst symmetry sub-chain SO3 H1 and m denotes the irresp. of the subgroup H2 in the second symmetry sub-chain H1 H2 reduced from l irreducible representation of H1. k and n have similar meanings. The crystal ﬁeld potential Hamiltonian can be written as Hc ¼

X k;l;m;k;n

k Vl;m;k;n ¼

X

ðk Þ

k Cl;m;k;n bl;m;k;n

ð3:10Þ

k;l;m;k;n

k where Cl;m;k;n denote the crystal ﬁeld parameters in the group chain scheme and ðk Þ

bl;m;k;n are the basic vectors. k For rare earth ions, k = 2, 4, 6. All the Vl;m;k;n terms should belong to the identity irresp. of group G, because the crystal ﬁeld potential must be invariant under the transformation of rare earth position point group. The method for writing down (3.10) for rare earth ions is to reduce k ¼ 2; 4 and 6 along the group chain SO3

H1 H2 H3 G and to ﬁnd all the channels for reaching the identity representations of group G (decomposition of group O3 to point group, the angular momentum quantum number divided into even parity J+ and odd parity J−, for the crystal ﬁeld energy level calculations, only involve the even parity J+. It should be pointed out that the group chain can have different length for different symmetry condition; the higher the site symmetry of the active ion, the shorter the length of group chain. There are a series of tables in Butler’s book [17] which provide a powerful tool to carry out this work. A simple example is given here to show how to use the tables for the purpose of writing down crystal ﬁeld potential Hamiltonian and their eigenfunctions. According to Butler [17], the notations of irreducible representations are different from those generally used. The irreducible representations of the wave functions, crystal ﬁeld parameters, and coupling coefﬁcient as well as those in Appendices 2, 3, and 5 will be denoted by the subscripts of related Beth’s notations in this book. Here, for example, we show the comparison between them in groups O and D3:

92

3 Rare Earth Ions in Materials

Group O

Group D3

Mulliken Bethe Butler

A1 C1 0

A2 C2 ~0

E C3 2

T1 C4 1

T2 C5 ~ 1

E′ C6

E″ C7

U′ C8

1 2

~ 1 2

3 2

This book

1

2

3

4

5

6

7

8

Mulliken Bethe Butler

A1 C1 0

A2 C2 ~0

E C3 1

E′ C4

E″ C5

C6

1 2

3 2

32

This book

1

2

3

4

5

6

Let’s consider the group chain scheme analysis of crystal ﬁeld energy levels of the ground multiplet 4I9/2 of Nd3+ ions occupying the D3 symmetry positions. The ﬁrst step is to investigate the ﬁrst section SO3 O of the group chain. From the table of branching rule of SO3 ! O section (Chap. 12 in Butler’s book [17] or Appendix B of this book), one can ﬁnd that the representation of 9/2 of SO3 group can be reduced into one 6(C6) and two 8(C8) representations. By using the branching rule for the O ! D3 section or related irreducible representation reduction tables, it can be found that the 6(C6) representation of group O corresponds to the 4(C4) representation of group D3. On the other hand, the 8(C8) representation of group O can be reduced to 4(C4) ⊕ 5(C5) ⊕ 6(C6) representations of group D3. In this way, the resolution of the multiplet 4I9/2 can be written as follows (note that in order to distinguish the difference between two 8(C8) representations of group O, the subscripts 0 and 1 are used to write it as 80(C80) and 81(C81)) 4 I9=2 ! 4 I9=2 64 4 I9=2 80 4 4 I9=2 80 5 4 I9=2 80 6 4 I9=2 81 4 4 I9=2 81 5 4 I9=2 81 6 ð3:11Þ That is, it splits into seven states. Among these states those corresponding to the representation 4 of group D3 have twofold degeneracy and those corresponding to representations 5 and 6 of group D3 have also twofold degeneracy, although each of them has only one-dimensional representations, but these two irreducible representations are conjugated and constitute a twofold degeneracy energy level. Therefore, the multiplet 4I9/2 will be split into ﬁve sub-states by the crystal ﬁeld with D3 point group symmetry. The wave functions of other energy states can also be introduced in the same way. The results are given in the paper published by the authors [18]. Generally, the crystal ﬁeld wave function can be expressed as W¼

X a;a1 ;a2 ;a3 ;a4

Caa1 a2 a3 a4 jaa1 a2 a3 a4 i

ð3:12Þ

Let’s consider the expression for the crystal ﬁeld Hamiltonian. It can be shown by the branching rule or by the related irresp. reduction tables that the irresp. for k = 2 in SO3 group will be reduced to two irresps. 3 ⊕ 5 of group O, but irresp. for

3.4 Group Chain Scheme Method in Crystal Field Analysis

93

k = 4 will be reduced to four irresps 1 ⊕ 2 ⊕ 3 ⊕ 5 of group O. On the other hand, the irresp. for k = 6 of SO3 group will be reduced to six irresps. 1 ⊕ 2 ⊕ 3 ⊕ 4 ⊕ 50 ⊕ 51 of group O. It can be found that only irresp. 1 and 5 of group O can be reduced to the identity irresp. 1 of group D3. The possible ways leading to identity irresp. 1 of group D3 can be shown as follows 2 ! 5 ! 1; 4 ! 1; 4 ! 5 ! 1; 6 ! 1 ! 1; 6 ! 50 ! 1; 6 ! 51 ! 1 It must be noted that k = 6 has two representations 5 of group O, and so two subscripts 0 and 1 should be used to distinguish them. In this way, the crystal ﬁeld Hamiltonian can be written as ð2Þ

ð4Þ

ð4Þ

ð6Þ

ð6Þ

ð6Þ

Hc ¼ C52 b5 þ C14 b1 þ C54 b5 þ C16 b1 þ C560 b50 þ C561 b51

ð3:13Þ

where bðlkÞ denotes the related unit vectors. In (3.13) the subscript 1 used to denote identity representation of D3 has been omitted. On comparing with Table 3.2, it can be seen that the number of parameters in (3.13) is the same as that for the traditional crystal ﬁeld theory, that is, there are six parameters. By observing the branching rule, it can be seen, for the even crystal ﬁeld potential, that the even representations of groups Oh and Td have one-to-one correspondence and Oh ! D3d, Td ! C3v, and O ! D3 all have the same table of branching rule. Therefore, one can write the six parameter expression of the crystal ﬁeld potential for point group of D3d and C3v similar to that of D3. The same method can be used to perform the analysis for other point groups. The crystal ﬁeld parameters for the 32 point symmetry groups are listed in Table 3.17. The numbers of above crystal ﬁeld parameters in the group chain scheme are the same as those of Table 3.2 for traditional crystal ﬁeld scheme. In the case of cubic system O, Oh, and Td, among the four parameters of the traditional crystal ﬁeld scheme, there are two relations shown previously, and so only two independent parameters, and the same is shown in Table 3.17. Note that in the above table, owing to the fact that the crystal ﬁeld potential with even parity is discussed, the crystal ﬁeld parameters concerned only with even parity and so the superscript + used to denote even parity is omitted. Having the expression for the crystal ﬁeld Hamiltonian and its eigenfunctions, the following work is to calculate the matrix elements. In order to do this calculation, the Wigner–Eckart theorem within the group chain scheme should be used. A simple introduction of this theorem is given here. For a more detailed discussion, one can refer to the book published by Butler [17] and Piepho and Schatz [23]. The Wigner–Eckart theorem has been given in (2.43). Expression of this theorem used in group chain scheme analysis will be introduced in the following. Similar to (2.43c), the expression of Wigner–Eckart theorem for point group can be expressed as

94

3 Rare Earth Ions in Materials

Table 3.17 Crystal ﬁeld parameters in the group chain scheme Crystalline system

Group

Crystal ﬁeld parameters

Subscript point group

Triclinic

C1

2 2 2 2 2 4 4 C3111 ; C5431 ; C3311 ; C5522 ; C5542 ; C1111 ; C4231

O ! D 4 ! D 2 ! C2

4 4 4 4 4 4 4 C3111 ; C3311 ; C5431 ; C5522 ; C5542 ; C4522 ; C4542 6 6 6 6 6 C1111 ; C3111 ; C3311 ; C4231 ; C560 431 ; C561 431 ; C2311

Monoclinic

C1

6 6 C560 522 ; C561 522 ; C560 542 ; C561 542 ; C4522 ; C4542 The same as above

Oh ! D4h ! D2h ! C2h

C2

2 2 2 4 4 4 4 C311 ; C543 ; C331 ; C111 ; C423 ; C311 ; C331

O ! D4 ! D2

4 6 6 6 6 C543 ; C111 ; C311 ; C331 ; C423 ; C560 43 ; C561 43

C2h Cs

6 C231 The same as above 2 2 2 4 4 4 C3111 ; C5431 ; C3311 ; C1111 ; C4231 ; C3111 ;

Oh ! D4h ! D2h

4 4 6 6 6 6 C3311 ; C5431 ; C1111 ; C3111 ; C3311 ; C4231 ; 6 C560 431 ; C561 431 ; C2311

Oh ! D4h ! D2h ! C2h

Orthorhombic

D2 D2h C2v

2 2 4 4 4 6 6 6 6 C31 ; C33 ; C11 ; C31 ; C33 ; C11 ; C31 ; C33 ; C23 The same as above 2 2 4 4 4 6 6 6 6 ; C333 ; C111 ; C331 ; C333 ; C111 ; C331 ; C333 ; C223 ; C331

O ! D4 O h ! Th Oh ! Td ! D2d

Triangular

D3 D3d C3v

C52 ; C14 ; C54 ; C16 ; C560 ; C561 The same as above 2 4 4 6 ; C11 ; C55 ; C11 ; C560 5 ; C561 5 C55 2 4 4 4 6 6 6 C51 ; C11 ; C51 ; C42 C11 ; C560 1 ; C561 1 ; C21 ; C42

O

C3 C3i Tetragonal

D4 D4h D2d C4v C4 C4h S4

2 4 4 4 6 6 6 C54 ; C11 ; C54 ; C44 C11 ; C560 4 ; C561 4 ; C21 ; C44

Oh O h ! Td O ! D3 O h ! Th

2 4 4 6 6 C33 ; C11 ; C33 ; C11 ; C33 ; C32 ; C14 ; C34 ; C16 ; C36 ; The same as above 2 4 4 6 6 ; C11 ; C31 ; C11 ; C31 ; C31 2 4 4 4 6 6 6 C31 ; C11 ; C31 ; C42 ; C11 ; C31 ; C42 The same as above 2 4 4 4 6 6 6 ; C111 ; C331 ; C442 ; C111 ; C331 ; C442 C331

O Oh O h ! Td Oh ! D4h O ! D4 Oh ! D4h Oh ! Td ! D2d

Hexagonal

D6 D6h C6v, D3h C6 C6h C3h

C12 ; C14 ; C16 ; C66 The same as above 2 4 6 6 ; C11 ; C11 ; C61 C11 2 4 6 6 6 C11 ; C11 ; C11 ; C61 ; C62 The same as above 2 4 6 6 6 ; C111 ; C111 ; C611 ; C622 C111

D∞ D∞h D∞h ! D6h D∞ ! D6 D∞h ! D6h

Cubic

T Th O Td, Oh

C14 ; C16 ; C26 The same as above C14 ; C16 The same as above

O Oh O Oh

D∞h ! D6h ! D3h

3.4 Group Chain Scheme Method in Crystal Field Analysis

D

E a a ð f Þ aaT/ bb ¼ a a

f /

95

D E aT ð f Þ b

b b

ð3:14Þ

For the cases in which the same irreducible representation appears r times, there are r different coefﬁcients, we have D where

E X a a ð f Þ aaT/ bb ¼ a a r b b

f /

b b

r D

E aT ð f Þ b

ð3:15Þ

a a

f /

b b1 b2 b3

1 rG c G a c1 C C 1 ¼ a1 c2 A G2 c3 Cn

refers to the 3jm coefﬁcients corresponding to the 3j coef a ﬁcients of the rotation group and called 2jm coefﬁcient corresponding to the a j coefﬁcient of ð1Þjm of the rotation group. It can be shown [17] that for m the group chain G G1 G2 Cn, the 3jm coefﬁcients can be reduced as following product 0

a B a1 B @ a2 a3

b b1

c c1

rG G1

a1 a2

b1 b2

c1 c2

G1 G2

a2 a3

b2 b3

c2 c3

G2 Cn

ð3:16Þ

G2 a2 b2 c 2 also is the 3jm a 3 b 3 c 3 Cn coefﬁcients, because the Abelian groups Cn are all one dimension. Therefore, the 3jm coefﬁcients for a group chain are equal to the product of 3jm factors of all the sections of the chain, no matter how long is the group chain. On the other hand, there is a factorization relation for the 2jm coefﬁcients, and so one has where for the group chain G2 Cn, 3jm factor

E ðk Þ aa1 a2 a3 Tf1 f2 f3 bb1 b2 b3 G G1 G2 X a a1 a2 a ¼ a1 a1 G1 a2 G2 a3 G3 r

D

f f1

b b1

rG r1 G 1

a1 a2

f1 f2

b1 b2

r1 G1 r2 G2

a2

f2

b2

a3

f3

b3

r2 G 2 D

EG aT ðkÞ b r

G3

ð3:17Þ Applying this theorem to the calculation of the matrix elements of the crystal ﬁeld Hamiltonian, and substituting into (3.10), we can obtain

96

3 Rare Earth Ions in Materials

haa1 a2 a3 a4 kHc kbb1 b2 b3 b4 i G G1 G2 G3 X a k b rG a a1 a2 a3 k ¼ Clmn a1 l b1 r1 G1 a1 G1 a2 G2 a3 G3 a4 Cn krr1 r2 r3 a1 l b1 r1 G1 a2 m b2 r2 G2 a3 n b3 r3 G3 D ðkÞ E a b b a2 m b2 r2 G2 a3 n b3 r3 G3 a4 0 b4

ð3:18Þ

where abk b is an irreducible matrix element of basis vector in the representation space of rotation group for a multi-electronic system. According to the previous description of the method of multi-electron unit vector (referred to the discussion of (2.48) to (2.49)), one has ED D E D E abðkÞ b ¼ f n SLaU ðkÞ f n SL0 b 3CðkÞ 3

ð3:19Þ

All the matrix elements can be obtained by using (3.18) and (3.19) as well as the tables in the books of Butler [17] or Piepho and Schatz [23]. As an example, it can be used to the calculation of the energy levels of Nd3+ ions in crystal YAl3(BO3)4, which have symmetry of point group D3. Let’s consider the multiplet 4F3/2. From the branching rule of SO3 ! O reduction, it can be seen that J = 3/2 corresponds to the irresp. 8 of group O. By the branching rule of O ! D3 reduction, the irresp. 8 of group O corresponds to the irresps. 4 ⊕ 5 ⊕ 6 of group D3. Therefore, the multiplet 4F3/2 will be reduced to three states with wave functions j3=2; 8; 4i, j3=2; 8; 5i, and j3=2; 8; 6i. One can omit the common ﬁrst label and write them as j8; 4i, j8; 5i, and j8; 6i. Equation (3.18) becomes 1 h3=2 a1 a2 jHc j3=2 b1 b2 i ¼ pﬃﬃﬃﬃﬃﬃﬃ ja2 j

3=2 a1

SO3 O

a1 a2

O X 3= 2 a1 D3 k

k 3=2 l b1

SO3 O

a1 a2

l b1 0 b2

O D3

D E Clk 3=2bðk Þ 3=2

ð3:20Þ The dimension factor ja2 j introduced in (3.20) is due to the fact that the group D3 includes irreducible representation higher than one dimension. Actually, if the calculation is to go down to the component of related irresps. (i.e. to multiply a 3jm coefﬁcients or a 3jm factor of D ! C3), the result will be the same. It can be seen by the branching rule of SO3 ! O and O ! D3 reductions that 2jm factors in (3.20) are all equal to +1. Obviously, the 3jm factor table for SO3 ! O reduction shows that only when k = 2 the ﬁrst 3jm factor in (3.20) has non-zero value. On the other hand, by (3.13), one knows that the only term remain ð2Þ is that including the factor of C5

3.4 Group Chain Scheme Method in Crystal Field Analysis

D E 3= 84Hc 3= 84 ¼ p1ﬃﬃﬃ 3=2 2 2 2 2 8 5

3= 2 8

SO3 O

8 4

97

5 8 1 4

O D3

D E C52 3=2bð2Þ 3=2 ð3:21Þ

Note the irresps. C4 of D3 group is a two-dimensional representation. In the tables of the 3jm factors for SO3 ! O reduction, one can see the following line (can be found in Appendix E or table of Butler [17]): pﬃﬃﬃ.pﬃﬃﬃ 3= 2 0000 þ 3 5 8

3= 2 8

2 5

Behind the 3jm symbol, there are four “0” in the same line. The ﬁrst number indicates the repeat number of the subgroup, and number 0 means there is no repetition of the subgroup. The number in the second, third, and fourth positions indicate the repeat number of the branches, and number 0 means there is no repetition of the branches. The symbol + indicates that the 3jm factor will not change sign under the exchange of columns while the symbol − indicates that the 3jm factor will change sign under the exchange of columns. Therefore

3= 2 2 8 5

3= 2 8

SO3

¼

O

2 5

3= 3= 2 2 8 8

SO3

pﬃﬃﬃ.pﬃﬃﬃ ¼ 3 5

O

Similarly, from the table of 3jm factors for O ! D3 reduction, it can be found that

8 4

5 1

8 4

O

¼

D3

5 1

8 8 4 4

O ¼ 1

.pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 23

D3

Substituting into (3.21), the following can be obtained D E D E 1 3= 84Hc 3= 84 ¼ p1ﬃﬃﬃ p1ﬃﬃﬃﬃﬃ C 2 3= bð2Þ 3= ¼ p ﬃﬃﬃ C2 U ð2Þ C5ð2Þ ð3:22Þ 5 2 2 2 2 10 2 2 5 Similarly D

!SO3 E 3= 2 3= E 8 5 8 O ð2Þ D3 1 2 2 3= 85Hc 3= 85 ¼ pﬃﬃﬃ C5 =2bð2Þ 3=2 2 2 6 1 5 D3 2 8 5 8 O pﬃﬃﬃ 3 1 1 ð2Þ ð2Þ ¼ pﬃﬃﬃ pﬃﬃﬃ C2 U ð2Þ C5 ¼ pﬃﬃﬃ C2 U ð2Þ C5 2 3 5 2 5 ð3:23Þ

98

D

3 Rare Earth Ions in Materials

!SO3 E 3 3 E 8 5 8 O ð2Þ D3 3= 86Hc 3= 86 ¼ p1ﬃﬃﬃ =2 2 =2 bð2Þ 3= C = 2 2 2 2 5 1 6 D3 5 2 8 5 8 O p ﬃﬃ ﬃ 3 1 1 ð2Þ ð2Þ ¼ pﬃﬃﬃ pﬃﬃﬃ C2 U ð2Þ C5 ¼ pﬃﬃﬃ C2 U ð2Þ C5 2 3 5 2 5 ð3:24Þ

In the above equation the fact that in D2 group irresp. 5 and irresp. 6 are conjugated to each other has been taken into account and the formulas for Ck and U ðkÞ (in the above equation k = 2, J = 3/2) are D D E E Ck 4f C ðkÞ 4f ; U ðkÞ 4f ; 4 FJ U ðkÞ 4f ; 4 FJ The table of the 3jm factors for O ! D3 reduction shows that all the non-diagonal matrix elements between different crystal ﬁeld states of this multiplet are zero. More calculation should be done for the states with higher angular momentum numbers but the method is the same. Let’s look at the example of J ¼ 9=2: Their energy levels have been given in (3.11) and as a calculation example one of the off-diagonal matrix elements is calculated in the following !SO3

E 6 5 80 O 2 D9 C = bð2Þ 9=2 4 1 4 D3 5 2 O !SO3 9= 4 9= E 6 5 8 0 O 4 D9 1 2 2 C = bð4Þ 9=2 þ pﬃﬃﬃ 4 1 4 D3 5 2 2 6 5 80 O !SO3 9= 9= E 6 50 80 O 6 D9 1 2 6 2 = bð6Þ 9=2 þ pﬃﬃﬃ C 4 1 4 D 3 50 2 2 6 50 80 O !SO3 9= 9= E 6 51 80 O 6 D9 1 2 2 6 þ pﬃﬃﬃ C = bð6Þ 9=2 4 1 4 D 3 51 2 2 6 51 80 O pﬃﬃﬃ D E D E 1 1 1 19 1 2 ¼ pﬃﬃﬃ ð pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃÞ pﬃﬃﬃ C52 9=2bð2Þ 9=2 þ pﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃ C54 9=2bð4Þ 9=2 2 3 2 3 3 11 2 3 5 11 13 pﬃﬃﬃ pﬃﬃﬃ D E D E 2 1 1 1 2 6 1 þ pﬃﬃﬃ ð pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃÞ pﬃﬃﬃ C560 9=2bð6Þ 9=2 þ pﬃﬃﬃ ð pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃÞ pﬃﬃﬃ C561 9=2bð6Þ 9=2 2 3 2 5 11 13 3 3 5 13 1 19 1 2 ¼ pﬃﬃﬃﬃﬃ C2 U ð2Þ C52 þ pﬃﬃﬃﬃﬃﬃﬃﬃ C4 U ð4Þ C54 pﬃﬃﬃﬃﬃ C6 U ð6Þ C560 pﬃﬃﬃﬃﬃﬃﬃﬃ C6 U ð6Þ C561 5 143 3 11 6 715 3 65

E 9= 64Hc 9= 80 4 ¼ p1ﬃﬃﬃ 2 2 2

D

9= 2 2 6 5

9= 2 80

ð3:25Þ The matrix elements for other J values can be found in the literature [18]. The crystal ﬁeld and energy level analysis for Nd3+:YVO4 crystal (in which Nd3+ ions occupy D2d point group position) by group chain method can be found in the author’s paper [24]. After obtaining the matrix elements, one can use exactly the same method as that used in the traditional crystal ﬁeld scheme to solve the secular equations. However, it is necessary to use the point charge model to calculate the starting values of crystal ﬁeld parameters in the traditional crystal ﬁeld scheme and then obtain those

3.4 Group Chain Scheme Method in Crystal Field Analysis

99

parameters in the group chain scheme. The relations between these two sets of crystal ﬁeld parameters can be introduced as follows. The crystal ﬁeld parameters in the traditional crystal ﬁeld scheme are the expanded coefﬁcients of the crystal ﬁeld Hamiltonian in terms of the irreducible representation basis functions of the full-rotation group. At the same time, the crystal ﬁeld parameters in the group-chain scheme are those expanded in terms of the irreducible representation basis functions of the point symmetry group. Therefore, it is easy to obtain their relations by the relation between the two kinds of basis functions X X ðk Þ kÞ Hc ¼ Cl;m;k;n bðl;m;k;n ¼ Bkq CqðkÞ kq

k;l;m;k;n

CqðkÞ

¼

1= 2 4p Y kq 2k þ 1

ð3:26Þ

Using the following relation between spherical harmonic function and the basis function of SO3 group [17] rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2k þ 1 1=2 k ð2k 1Þð2k 3Þð2k 5Þ r Y kq ¼ jkqi 4p k! 1= 2 4p ðk Þ Cq ¼ Y kq 2k þ 1 that is CqðkÞ

¼

4p 2k þ 1

1= 2

rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ð2k 1Þð2k 3Þð2k 5Þ Ykq ¼ r jkqi k! k

and ðk Þ blmkn

rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ð2k 1Þð2k 3Þð2k 5Þ ¼ jklmkni k!

We obtain X k;lmkn

ðk Þ k Clmkn blmkn

rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ð2k 1Þð2k 3Þð2k 5Þ ¼ Clmkn jklmkni k! k;lmkn rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ð2k 1Þð2k 3Þð2k 5Þ X ¼ Bkq jkqi k! kq X

k

ð3:27Þ

100

3 Rare Earth Ions in Materials

Hence the relation between the two basis functions can be written as X ak0 q0 jk 0 q0 i j k 0 l 0 m 0 n0 i ¼ k 0 q0

The conjugate of the above formula will be X akþ0 q0 hk 0 q0 j hk0 l0 m0 n0 j ¼

ð3:28Þ

k 0 q0

Multiply the left-hand side and right-hand side of the second equation of (3.27) with left side and right side of (3.28), respectively, and apply the orthogonal and normalized relation, then the following can be shown k Clmkn ¼

X

akq Bkq

ð3:29Þ

kq

The following relation is satisﬁed by the two sets of crystal parameters X X ^ k Þ2 ¼ ðC ðBkq Þ2 lmkn klmkn

ð3:30Þ

kq

because the two sets of basis functions are transformed by orthogonal transformation and the length of the vector is invariable by this transformation. Equation (3.29) is the crystal ﬁeld parameters in the group chain scheme. By using this equation the relation between the two kinds of crystal parameters for the crystal ﬁeld with D3 point group symmetry will be C52 ¼ B20 1 pﬃﬃﬃﬃﬃ 2 pﬃﬃﬃﬃﬃ 21B40 30B43 C14 ¼ 9 9 2 pﬃﬃﬃﬃﬃ 1 pﬃﬃﬃﬃﬃ 15B40 þ 42B43 C54 ¼ 9 9 4 pﬃﬃﬃ 2 pﬃﬃﬃﬃﬃﬃﬃﬃ 1 pﬃﬃﬃﬃﬃﬃﬃﬃ 2B60 þ 105B63 462B66 C16 ¼ 9 27 rﬃﬃﬃﬃﬃ 27 1 pﬃﬃﬃﬃﬃﬃﬃﬃ 5 462B63 þ 2 C560 ¼ B66 21 21 7 8 pﬃﬃﬃﬃﬃﬃﬃﬃ 8 pﬃﬃﬃﬃﬃﬃﬃﬃ 210B63 231B66 C561 ¼ B60 þ 9 189 189

ð3:31Þ

Noting that in D3 point group, Bkq ¼ Bk;q , it is easy to show that (3.31) satisﬁed by the invariant relation (3.30). By using the group chain scheme, a series of problems in crystal spectroscopy, including relative intensities of emission spectra in crystal, J mixing effect and up-conversion emission have been studied by the authors [18, 25–32]. The calculated

3.4 Group Chain Scheme Method in Crystal Field Analysis

101

results are in good agreement with the experimental data. In Chap. 12, this method is used to deal with spectroscopy problems of the rare earth ions in glasses; hence one can see that an incisive knowledge on their spectroscopic properties can be obtained.

References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32.

D.J. Newman, Adv. Phys. 20, 197 (1971) D.J. Newman, B. Ng, Crystal Field Handbook (Cambridge University Press, 2000) M. Klintenberg, S. Edvardsson, J.O. Thomas, Phys., Rev. B 55, 10369 (1997) B.R. Judd, Phys. Rev. Let. 39, 242 (1977) B. Ng, D.J. Newman, J. Chem. Phys. 87, 7086, 7110 (1987) E. Rukmini, C.K. Jayasankar, M.F. Reid, J. Phys. Condens. Matter 6, 5919 (1994) S. Hufner, Optical Spectra of Transparent Rare Earth Compounds (Academic Press, New York, 1978) B.R. Judd, Proc. Phys. Soc. (London) A227, 552 (1955) G.H. Dieke, Spectra and Energy Levels of Rare Earth Ions in Crystals (Interscience, New York, 1968) M. Sachs, Solid State Theory (McGraw-Hill Book Company, New York, 1963) D. Sengupta, J.O. Artman, Phys. Rev. B 1, 2986 (1970) C.A. Morrison, R.P. Leavitt, Handbook on the Physics and Chemistry of Rare Earths, vol. 5, ed. by K.A. Gschneidner Jr., L. Eyring (North-Holland Publishing Company, 1982) A.A. Kaminskii, Laser Crystals, their Physics and Properties (Springer, Heidelberg, 1981 and 1990) A.A. Kaminskii, Crystalline Lasers: Physical Processes and Operating Schemes (CRC Press, Boca Raton, 1996) K.H. Hellwege, Ann. Phys. 4, 95 (1948) G.K. Liu, B. Jacquier, Spectroscopic Properties of Rare Earths in Optical Materials (Tsinghua University Press and Springer, Berlin Heidelberg, 2005) P.H. Butler, Point Group Symmetry Application: Method and Tables (Plenum, New York, 1981) Z.D. Luo, Y.D. Huang, J. Phys. Condens. Matter 5, 6949 (1993) A. Benayas, D. Jaque, S.J. Gacia et al., J. Phys. Condens. Matter 19, 24640 (2007) C. Cascales, C. Zaldo, U.J. Caldino, J. Phys. Condens. Matter 13, 8071 (2001) D. Jaque, O. Enguitia, U.J. Caldino, J. Appl. Phys. 90, 561 (2001) D. Jaque, J. Capmany, Z.D. Luo, J. Phys. Condens. Matter 9, 9715 (1997) S.B. Piepho, P.N. Schatz, Group Theory in Spectroscopy with Applications to Magnetic Circular Dichroism (Wiley, New York, 1983) Y.D. Huang, Z.D. Luo, J. Phys. Condens. Matter 6, 3737 (1994) X.Y. Chen, Z.D. Luo, J. Phys. Condens. Matter 8, 2571 (1996) X.Y. Chen, Z.D. Luo, Acta Physica Sinica (in Chinese) 46, 181 (1997) X.Y. Chen, Z.D. Luo, J. Phys. Condens. Matter 9, 4197 (1997) X.Y. Chen, Z.D. Luo, Chinese J. Struct. Chem. 6, 358 (1997) X.Y. Chen, Z.D. Luo, J. Phys. Condens. Matter 9, 7981 (1997) X.Y. Chen, Z.D. Luo, J. Phys. Condens. Matter 10, 5147 (1998) X.Y. Chen, Z.D. Luo, Acta Physica Sinica (in Chinese) 7, 773 (1998) X.Y. Chen, Z.D. Luo, Acta Physica Sinica (in Chinese) 8, 607 (1999)

Chapter 4

Theory of Radiative Transition

Light emission and absorption are the main processes to be discussed in spectroscopy and laser physics, while absorption coefﬁcient, emission and absorption cross-sections, and oscillator strength are fundamental in the investigation of solid-state laser materials. Therefore, in order to have a deep understanding of these processes and calculate correctly all the spectral and laser parameters, it is necessary to study and systematically analyze these processes from the ﬁrst principles of electrodynamics and quantum mechanics as well as to discuss the selection rule and polarization character of radiative transition by symmetry property of the energy levels.

4.1

Interactions Between Active Ions and Radiation

The active ions in solid materials have interactions with electromagnetic ﬁeld, besides those with lattice ions and lattice vibrations. These interactions are the physical mechanisms of various performances of solid-state laser. In this chapter, we will discuss the interaction of active ions with radiation ﬁeld and introduce the formulas for calculating the emission and absorption probabilities and other important spectral parameters. In order to deal with both stimulated and spontaneous emissions, quantum theory should be used, because spontaneous emission cannot be accounted for by the classical or semi-classical theory. As it is well known from quantum theory, the photon þ creation operators aka and photon annihilation operators aka are used to describe radiation ﬁeld. These operators satisfy the following commutation relations [1] þ þ aka ; akþ0 a0 ¼ dk;k0 daa0 ; ½aka ; ak0 a0 ¼ 0; aka ; ak 0 a 0 ¼ 0

© Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8_4

ð4:1Þ

103

104

4 Theory of Radiative Transition

where a denotes the polarization state of the photon with energy hxk and momentum hk. The creation and annihilation operators have the following eigenvalues in the photon-number representation jnka i þ aka jnka i ¼

pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃ þ nka þ 1jnka þ 1ia_ a ; aka jnka i ¼ nka jnka 1i; aka aka jnka i ¼ nka jnka ð4:2Þ

In this representation, if the vector potential A of the ﬁeld is expressed as the following expression A¼

X 2phc2 1=2 xk Ve

ka

þ ea ðkÞ aka ðtÞeikr þ aka ðtÞeikr

ð4:3Þ

then the ﬁeld energy can be expressed as the sum of all the photons, where þ þ ixk t ðtÞ ¼ aka e aka ðtÞ ¼ aka eixk t ; aka

ð4:4Þ

where ea ðkÞ, in which a = 1, 2, is the unit vector used to represent the polarization direction of the photons, c is the velocity of the photons in vacuum, e refers to the dielectric constant of the solid material, and V denotes the volume occupied by the radiation ﬁeld. According to electromagnetic dynamics [2] E¼

1 @A c @t

ð4:5aÞ

and then one can obtain X 2phxk 1=2 1 @A þ ¼i E¼ ea ðkÞ aka ðtÞeikr aka ðtÞeikr c @t Ve ka By using the following relations Z

0

eiðkk Þr ds ¼ Vdkk0

and ea ðkÞ ea0 ðkÞ ¼ daa0

ð4:5bÞ

4.1 Interactions Between Active Ions and Radiation

105

Noting that the polarization vectors are perpendicular to vector k representing the direction of the light wave, that is, e1 ðkÞ k ¼ e2 ðkÞ k ¼ 0, then the energy Hamiltonian of the ﬁeld can be written as Hph ¼

Z X e 1 þ hxk aka aka þ E2 ds ¼ 4p 2 ka

ð4:6Þ

þ where aka aka represents the operator of the photon number. Equation (4.6) shows that the energy of each photon mode is equal to the number of photon multiplied by the energy of a single photon plus zero ﬁeld energy, and the total energy of the whole ﬁeld is the sum of the energy of all the photons. This is a well-known physical reality. Obviously, (4.3) can be used to obtain a correct result and so it is justiﬁed. Next, the interaction Hamiltonian between the radiation ﬁeld and the electron without spin will be introduced. For the case studied, the electric potential (scalar potential) can be assumed to be zero. It can be shown that if the interaction Hamiltonian is written in the form:

H¼

1 eA 2 p 2m c

ð4:7Þ

where p is the momentum of the electron with mass m, then the Newtonian equations for the electron in the ﬁeld can be introduced correctly. According to Hamiltonian equations in mechanics, one has [3] d @H d @H r¼ ; p ¼ dt @p dt @r where r is the vector of electronic coordinate. There are six equations here, from which the equations for the component x are: d @H d @H x¼ ; px ¼ dt @px dt @x By substituting (4.7) in the above equation, we obtain d 1 e x¼ px A x dt m c

ð4:8aÞ

d 1 e r¼ p A dt m c

ð4:8bÞ

Obviously, its vector form is

106

4 Theory of Radiative Transition

On the other hand, by (4.7) and x component of the second Hamiltonian equation d 1 e e @A px ¼ p A dt m c c @x

ð4:9Þ

Differentiating (4.8a) and using (4.9) and (4.8b), one obtains m

d2 x d ed dr e @A e d Ax ¼ Ax ¼ px dt2 dt c dt dt c @x c dt

ð4:10Þ

Owing to the fact that Ax = Ax(x, y, z, t), the total differential of the last term in the above equation can be expressed as dAx @Ax dx @Ax dy @Ax dz @Ax þ þ þ ¼ dt @x dt @y dt @z dt @t Therefore, (4.10) becomes m

d 2 x e dy @Ay @Ax dz @Ax @Az [email protected] Ax ¼ 2 dt c dt @x dt @z c @t @y @x

ð4:11Þ

By means of the well-known electromagnetic dynamics equation [2] B¼rA

E¼

1 @A c @t

It is easy to show, by (4.11), that m

d2 x e ¼ eEx þ ðv BÞx 2 dt c

ð4:12Þ

The right-hand side of the above equation is the x component of the Lorentz force, and so the formula (4.12) corresponds to the x component of the Newtonian equation for the electron in the radiation ﬁeld. Therefore, the interaction Hamiltonian of (4.7) is justiﬁed. Expanding formula (4.7), one has 1 eA 2 1 2 e e2 2 p p ðp A þ A pÞ þ ¼ A 2m c 2m 2mc 2mc2 If the term having the factor A2 is neglected, then the interaction Hamiltonian can be written as

4.1 Interactions Between Active Ions and Radiation

Hi ¼

107

e ðp A þ A pÞ 2mc

Expressing p as ihr and remembering that r A ¼ 0, it can be shown that p A ¼ A p ihr A ¼ A p Therefore e e X 2ph 1=2 þ pA¼ Hi ¼ ea ðkÞ p½aka ðtÞeikr þ aka ðtÞeikr mc m ka Vxk e

ð4:13Þ

where p is an operator acting on the electronic wave functions while the creation and annihilation operators are photon operators acting on photon wave functions.

4.2

Probability of Emission and Absorption Processes

In the last section, the mechanism of the interaction between electron and radiation ﬁeld is discussed and the formula for the interaction Hamiltonian has been introduced. The emission and absorption processes and the formulas of their transition probability will be discussed and derived in this section. The Hamiltonian Hi, a time-dependent perturbation operator, causes transitions between different electronic energy levels. According to time-dependent perturbation theory [4], transition probability can be calculated by using the following formula Wif ¼

2p 2p jhijHi jf ij2 qðxk Þ 2 Mif2 qðxk Þ 2 h h

ð4:14Þ

where the ﬁnal state of the radiation ﬁeld has state density qðxk Þ. Let us suppose that the radiation ﬁeld is limited in a cube with volume V = L3, then the k vector in (4.13) should satisfy the following equations obtained by period conditions kx ¼

2pnx 2pny 2pnz ; ky ¼ ; kz ¼ L L L

where each set of nx, ny, nz represents a state. Thus the number of states between k and k + dk will be qðkÞdk ¼ dnx dny dnz ¼

V V dkx dky dkz ¼ 3 k 2 dkdXk 8p3 8p

where dXk is the inﬁnitesimal solid angle in the direction k. By using k = x/c, the above expression can be written as

108

4 Theory of Radiative Transition

qðxk Þdxk ¼

V x2 dxk dXk 8p3 c3 k

Therefore qðxk Þ ¼

V x2 dXk 8p3 c3 k

ð4:15Þ

where c is the velocity of light; it should be replaced by c/n in solid materials. In the process of absorbing a photon and jumping to the ﬁnal state, the radiation ﬁeld has one photon less in the initial state. Expressing the wave function than that of initial state as i [ ¼ uei [ nk [ , then that of the ﬁnal state is f [ ¼ uef [ nk 1 [ . If the ion emits a photon, the wave function of initial e state will be ji [ ¼ jui [ jnk [ and that of the ﬁnal state can be expressed as e f [ ¼ uf [ nk þ 1, where uei and uef are electronic wave functions for the initial

and ﬁnal states, respectively. If one calculates the matrix elements of photon operators at ﬁrst, then the electronic transition matrix element for the emission process will be +

1=2 * X e 2ph M if ¼ ðnk þ 1Þ uef ea ðkÞ pi eikri uei i m Vxk e

ð4:16Þ

For the absorption process it is +

1=2 * X e 2ph e ikri e nk uf ea ðkÞ pi e M if ¼ ui i m Vxk e

ð4:17Þ

In these two expressions, the summations are over all the involved electrons. It can be seen from expression (4.16) that even if there is no radiation ﬁeld present before emission, that is, nk = 0, the transition matrix elements for emission are different from zero. It gives rise to spontaneous emission. The other term proportional to nk presenting the photon number in the radiation ﬁeld describes the stimulated emission. In order to carry out a detailed calculation, it is necessary to expand eikri . One can estimate the order of magnitude of kri at ﬁrst. The electronic coordinate ri is in the range of an ion radius of 10−8 cm, and the light wavelength k is in the range of 10−4–10− 5 cm, so we have k ri ¼

2pa 103 : k

Thus it is enough to keep only the ﬁrst and second terms in the expansion of eikri

4.2 Probability of Emission and Absorption Processes

eikri ¼ 1 þ ik ri ; eikri ¼ 1 ik ri

109

ð4:18Þ

The ﬁrst term corresponds to the electric-dipole transition. The transition probability per unit time for the stimulated absorption and emission of a photon with frequency xk can be expressed as + 2 * XZ X x3k e e dX n u u e ðkÞ er Pk ðabs:Þ ¼ Pk ðst:em:Þ ¼ k k a i f i 2phc3 e a¼1;2 i ð4:19Þ The transition probability for spontaneous emission can be expressed as +2 * Z X x3k X e e u dX Pk ðsp:em:Þ ¼ u e ðkÞ er k i i f a 2phc3 e a¼1;2 i

ð4:20Þ

In the deduction of expressions (4.19) and (4.20), the Poisson equation in quantum mechanics r_ ¼ hi ½H; r [1] has been used; therefore D E im D E D E im ½H; r; uef jpjuei ¼ Efe Eie uef jrjuei ¼ imxk uef jrjuei h h P In expressions (4.19) and (4.20), i eri is electric-dipole of the electronic system and so the corresponding transition is referred to as the electric-dipole transition. The unit polarization vectors e1(k) and e2(k) are perpendicular to each other and perpendicular to the photon propagate direction k and so one can discuss the problem in a coordinate system constituting by these three vectors. If the angle between radius ri of the electron i and the photon propagating direction k is hi while the angle between the projection of radius ri on the plane e1(k)–e2(k) and the polarization vector e1(k) is ui, then we have X X X ea eri ¼ eri ðsinhi cos/i þ sinhi sin/i Þ p ¼ m_r ¼

a¼1;2

i

i

Owing to the fact that the angles between the photon propagating direction k and the radius ri of different electron positions are independent of each other and can assume any different values, then the expressions (4.19) and (4.20) should be integrated over dX ¼ sinhdhd/. The integral of the term of cosuisinui over ui is zero. Therefore, the probabilities of stimulated and spontaneous electric-dipole emissions can be written, respectively, as

110

4 Theory of Radiative Transition

Pk ðst:em:Þ ¼

X x3k nk 3 2phc e i

x3k X Pk ðsp:em:Þ ¼ 2phc3 e i

Z

Z

D 2 sin2 hi dX uef ri uei D 2 sin2 hi dX uef ri uei

In the processes of emission and absorption, the electrons with different subscript i are independent and the inﬁnitesimal solid angle all have the same expression dX ¼ sin hdhdu, and so for the spontaneous electric-dipole emission we have Z Z D 2 x3k X 2p p 3 e e Pk ðsp:em:Þ ¼ sin hdhdu uf ri ui 3 2phc e i 0 0 2 4x3k X D e e ¼ e uf ri ui 3hc3 e i

ð4:21Þ

In the case of isotropic space, we have D

E D E D E D E uef jxi juei ¼ uef jyi juei ¼ uef jzi juei ¼ uef jri juei

The spontaneous transition probability for emission light polarized in any direction will be the same. In the general cases, the spontaneous transition probability for emission light polarized in any direction should be calculated according to the Theorem on the Total Probability [5]. By this theorem, if any event B occurs by the ways of A1, A2, A3,…, An having probability of p(A1), p(A2), p(A3), …, p(An), respectively, then the probability of event B to take place by using any of the above-mentioned ways can be calculated by: PðBÞ ¼

X

pðAi ÞpðAi jBÞ

i

where p(Ai|B) is the probability of event B occurred by the way of Ai, and p(Ai) is the probability of the way of Ai. The above summation should be changed to an integral in the case of continuous variables. Applying it to the isotropic solid material, considering that the probability of polarization direction in dXp is dXp/4p, the probability of spontaneous electric-dipole emission with polarization in any direction becomes: Z E2 1 4x3k X D e e Pk ¼ e uf jri jui dXp ð4:22Þ 4p 3hc3 e i

4.2 Probability of Emission and Absorption Processes

111

D E2 4x3 P The result is 3hc3ke e uef jri juei , because the space is isotropic. It can be shown i

that in this case E2 4x3 X D E2 4x3k X D e k Pk ¼ e uf jxi juei ¼ e uef jyi juei 3hc3 e i 3hc3 e i 2 E 4x3k X D e e ¼ e u z j ju i f i 3hc3 e i This result has been obtained previously. It leads to the conclusion that in isotropic solid materials, the electric-dipole spontaneous emission with polarization in any direction has the same transition probability as that with polarization along x, y, or z axis. This conclusion seems to be obvious; it is in fact the result of the theorem on the total probability. Understanding of this point is very important for the calculation of the transition probabilities in the case of anisotropic crystal. In the case of anisotropic crystal, the spontaneous emission probability for the transition emitting the light polarized in the direction of X, Y, and Z of crystallo physics axes can be written, respectively, as PðXÞ ðsp:em:Þ, PðYÞ ðsp:em:Þ, and PðZÞ ðsp:em:Þ. For the sake of convenience, S(i, f) is used to represent the sum of the electric-dipole moment matrix element square in the above formula. The probability of electric-dipole transition polarizing along a certain direction q is written as PðqÞ ðsp:em:Þ ¼

4x3k e2 ðqÞ S ði; f Þ 3hc3 e

ð4:23Þ

The theorem on the total probability gives the total spontaneous emission probability Pðsp:em:Þ ¼ pðXÞPðXÞ ðsp:em:Þ þ pðYÞPðYÞ ðsp:em:Þ þ pðZÞPðZÞ ðsp:em:Þ i ð4:24aÞ 1h ¼ PðXÞ ðsp:em:Þ þ PðYÞ ðsp:em:Þ þ PðZÞ ðsp:em:Þ 3 For an uniaxial crystal Pðsp:em:Þ ¼ pðpÞPðpÞ ðsp:em:Þ þ pðrÞPðrÞ ðsp:em:Þ 1 2 ¼ PðpÞ ðsp:em:Þ þ PðrÞ ðsp:em:Þ 3 3

ð4:24bÞ

Note: Dealing with the transition in the solid material, the correction factor introduced by the refractive index should be included, and this will be discussed later. Obviously, by using (4.24a, 4.24b), the error of over estimation in the transition probability as well as the Judd–Ofelt parameters can be avoided.

112

4 Theory of Radiative Transition

The related expressions for magnetic-dipole and electric-quadrupole transitions will be briefly discussed the related electric-dipole matrix element is D now. Suppose E

equal to zero, that is, uef jrjuei ¼ 0, assume the single electron approximation at the same time. Referring to formula (4.16), the expression of matrix element in (4.18) will be D

D E E uef e peikr uei ¼ i uef jðk rÞðe pÞjuei

ð4:25Þ

where ea(k) has been represented by e, for the sake of convenience. In order to understand their transition mechanisms (kr) (ep) is separated into two parts X X ðk rÞðe pÞ ¼ k i r i e j pj ¼ k i e j r i pj i;j

i;j

1X

1X ¼ k i e j r i pj r j pi þ k i e j r i pj þ r j pi 2 i;j 2 i;j X

1 1 k i e j r i pj þ r j pi ¼ ð k eÞ l þ 2 2 i;j

1 1X ¼ e ðk lÞ þ k i e j r i pj þ r j pi 2 2 i;j

ð4:26Þ

where i and j are used to denote three components of related vectors and l = r p is the orbital angular momentum operator. Similar to the transformation of the matrix elements of p to that of r in the introduction of formulas (4.19) and (4.20), the matrix element of the second term in (4.26) can be transformed into D D E E uef ri pj þ rj pi uei ¼ imxk uef ri rj uei

ð4:27Þ

Therefore D E E imx D E 1D k uef jðe rÞðk rÞjuei uef jðk rÞðe pÞjuei ¼ uef je ðk lÞjuei þ 2 2 ð4:28Þ Substituting (4.28) into (4.16), the spontaneous emission matrix element in single electron approximation can be expressed as Mif ¼

E mx D E

e 2ph 1=2 i D e k uf je ðk lÞjuei þ uef jðe rÞðk rÞjuei ð4:29Þ m Vxk e 2 2

The ﬁrst and the second terms in (4.29) correspond to the magnetic-dipole transition and the electric-quadrupole transition, respectively. Based on the above relations,

4.2 Probability of Emission and Absorption Processes

113

the more common Hamiltonians of the magnetic-dipole and the electric-quadrupole transitions can be obtained by using (4.13). Hmd ¼ i

X 2phxk 1=2

Ve ka ðik M md Þ

aka ea ðkÞ ðik M md Þ þ i

X 2p hxk 1=2 ka

Ve

þ aka ea ðkÞ

ð4:30Þ and Heq ¼

X phx3 1=2

k aka ðea ðkÞ erÞðik rÞ 2 Ve 2c ka X phx3 1=2 þ k þ aka ðea ðkÞ erÞðik rÞ 2 Ve 2c ka

ð4:31Þ

While introducing the above equations, unit vector ik in k direction and k ¼ xck ik has been used and the magnetic-dipole of electron is expressed as follows by including spin magnetic-dipole moment of electrons Msp = (e/mc)s M md ¼

eh ðL þ 2SÞ: 2mc

By using formulas (4.30) and (4.31), the probabilities of magnetic-dipole transition and electric-quadrupole transition can be obtained, respectively. The probability of spontaneous magnetic-dipole transition is given by Pmd sp:em: ¼

2 4x3k M h i md if 3 3hc e

ð4:32aÞ

while the probabilities of stimulated emission and absorption of magnetic-dipole transition are given, respectively, by md Pmd st:em: ¼ Pab: ¼

2 4x3k nk M h i md if 3hc3 e

ð4:32bÞ

Obviously, the magnetic-dipole and electric-quadrupole transition probabilities are much lower than that of the electric-dipole transition, when all the transitions are allowed by selection rules. A simple comparison of the order of magnitude can give us a general idea. For the free ions and atoms, the magnetic-dipole transition probability will be about 10−5–10−6 times of that of electric-dipole transitions, while the corresponding ﬁgures for electric-quadrupole transition will be only 10−7–10−8. The situation in solid-state laser materials is different. Owing to the fact that many transitions in the materials are observed within the same electronic

114

4 Theory of Radiative Transition

conﬁguration, the electric-dipole transitions are forbidden in zero-order approximation and allowed only if there is a perturbation caused by odd-parity crystal ﬁeld or lattice vibration which mix some wave function components with different parity into the wave functions of the initial and/or ﬁnal states of the transitions. Therefore, the transition probability is determined by the odd-parity perturbation. Without this kind of perturbation, the transitions between states with the same parity can only be magnetic-dipole or electric-quadrupole type. The relationship between the probability of the electric-dipole transition and the symmetry of the active ions can be divided into three kinds [6]: I. The active ions occupy position with symmetry of the following 11 point groups: S2 Ci ; S6 ; C2h ; C4h ; C6h ; D3d ; D2h ; D4h ; D6h ; Oh ; Th In these cases, the electric-dipole transition is forbidden. Weak electric-dipole transition can still be introduced by odd-parity lattice vibration mode. The intensity of phonon-assisted forced electric-dipole transition is proportional to the reduced temperature T/Tm (Tm is the melting temperature of the crystal in Kelvin scale). At the same temperature T, the lower the melting temperature Tm, the higher is the transition intensity. By this reason, at room temperature, rather strong fluorescence can be observed in some crystals with low melting temperature, but in the crystals with high melting temperature any fluorescence cannot be seen. The associated spectral line is called the phonon sideband, and at the location of one phonon energy away from the zero phonon line. II. The active ions occupy position with symmetry of the following 18 point groups:

C1 ; C2 ; C1h ; D2 ; C2v ; C4 ; S4 ; D4 ; C4v ; D2d ; C3v ; C6 ; D6 ; C6v ; D3h ; T; Td ; O In these cases, some pairs of nearest neighbor ion still have or nearly have inversion symmetry centered on active ions, although the electric-dipole transitions induced by crystal ﬁeld and forced by lattice vibration are all allowed, and the wave function admixture with different parity generally is not large enough and the electric-dipole transition is generally not strong enough, except in the case where some pairs of nearest neighbor ion have a large deviation from the inversion symmetry. III. The active ions occupy position with symmetry of the following three point groups: C3 ; D3 ; C3h In these cases, the wave function with different parity has larger admixture and so has higher electric-dipole transition rate.

4.2 Probability of Emission and Absorption Processes

115

It should be noted that for the active ion, the intensity of electric-dipole transition depends not only on its site symmetry but also on the number of nearest neighbor anions deviating from the inversion symmetry as well as their deviating magnitude. The selection rules for the transition will be given in the next section.

4.3

Selection Rules for Radiative Transition

In principle, if the related matrix element for a transition is non-zero, then the transition can take place. According to this principle, the selection rules for electric-dipole, magnetic-dipole, and electric-quadrupole transitions will be introduced. The results can be easily obtained by using the group theory. The discussion in this chapter does not involve complex coupling coefﬁcients. The notation of the point group irreducible representation still uses the Bethe’s notation.

4.3.1

Selection Rules for Radiative Transition of Free Ions and Atoms

According to the group theory, the transition matrix element is a physical quantity measuring the probability of transition so that it is invariant in a symmetry transformation; therefore, it must belong to the identity representation of the symmetry group. The total angular momentum quantum number J is a good quantum number for atoms and free ions. By Chap. 2 we know that the initial state i and the ﬁnal state f belong to the representations DJi and DJf of the full-rotation group, respectively. In the case of an electric-dipole transition, the electric-dipole is a vector belonging to D1 [7]. The non-zero transition matrix element requires that the product of DJi D1 includes DJf . It is easy to obtain that DJi D1 ¼ DJi þ 1 DJi DJi 1 . Therefore, the selection rule for the electric-dipole transitions is DJ = 0, ±1. It should be pointed out that when Ji = 0, Jf can only be equal to 1 and so the Ji = 0 ! Jf = 0 transition is forbidden. On the other hand, the parity of ﬁnal state should be different from that of the initial state, because the parity of electric-dipole is odd. In the case of weak spin–orbit coupling, Russell-Saunders approximation is good enough and so L and S are good quantum numbers. In this case, the electric-dipole moment operator belongs to representation D1 (L = 1, S = 0), and the initial state belongs to DLi DS but the ﬁnal state belongs to DLf DS . Obviously, we have the following selection rules. DS = 0, DL = 0, ±1, the parity should be changed in the transition but Li = 0 ! Lf = 0 is forbidden.

116

4 Theory of Radiative Transition

For the magnetic-dipole transitions, remembering that magnetic-dipole moment is an axial vector, which belongs to representation D1g (having even parity), one can obtain their selection rules by using the same method: DJ = 0, ±1; the parity should not be changed in the transition while Ji = 0 ! Jf = 0 is forbidden. When Russell-Saunders approximation is reasonable, we have the following selection rules: DS ¼ 0; DL ¼ 0; 1 but Li ¼ 0 ! Lf ¼ 0 is forbidden while it is relaxed by intermediate coupling; the parity should not be changed in the transition. Finally, for electric-quadrupole transition, the electric-quadrupole moment is a second-order tensor belonging to representation D2g. According to tables of representation product, one has: When Ji 2 DJi D2 ¼ DJi þ 2 DJi þ 1 DJi DJi 1 DJi 2 When Ji = 1 DJi D2 ¼ D3 D2 D1 When Ji = 0 DJi D2 ¼ D2 Therefore, the selection rules for an electric-quadrupole transition are: DJ ¼ 0; 1; 2; the parity should not be changed in the transition but Ji = 0 ! Jf = 0, 1 and Ji = 1 ! Jf = 0 are forbidden. For Russell-Saunders coupling, DS = 0, DL = 0, ±1, ±2; the parity should not be changed in the transition but Li = 0 ! Lf = 0, 1 and Li = 1 ! Lf = 0 are forbidden.

4.3.2

Selection Rules for Radiative Transition of Ions in Materials

In materials, quantum numbers J, L, and S of active ions are not really good quantum numbers due to the action of crystal ﬁeld. The good quantum numbers are the irreducible representations of active ion’s site symmetry group. Therefore, transition selection rules should be those involving their irreducible representations.

4.3 Selection Rules for Radiative Transition

117

Certainly, when the crystal ﬁeld strength is weak enough, the selection rules for free ions still have weak limitation. As it has been pointed out previously, the crystal ﬁeld interaction of transition-metal ions is stronger than that of the spin– orbit interaction, and so the energy levels of transition-metal ions should be denoted ﬁrst by the related irreducible representation but not the atomic quantum number J, L, and S. Remembering that the electric-dipole has the same irreducible representations as that of a polar vector (the radius of the electron), but the magnetic-dipole moment can be expressed as a vector product of two polar vectors, and the transition selection rules can be introduced easily by applying the tables of the irreducible representation product. Although the crystal ﬁeld interaction of rare earth ions in a material is weaker than their spin–orbit coupling and the quantum numbers J, L, and S can be still used to describe their energy levels, the odd parity crystal ﬁeld interaction has its effect on the electric-dipole transition. Therefore, in this case the selection rules for free ions will not be valid except that of DS = 0. It can be shown that the following selection rules are valid: Dl = ±1, DS = 0, DL 2l, DJ 2l (for rare earth ions l = 3), DJ = 2, 4, 6, if J = 0i or Jf= 0. The forbidden rule of Ji = 0 ! Jf = 0 transition is generally valid except the special cases in which Judd–Ofelt parameter X0 6¼ 0. This will be demonstrated in Chap. 5. Obviously, the electric-dipole transitions inside 4fn conﬁguration (Dl = 0) are forbidden in the strict sense but this forbidden rule is partly broken by the odd parity perturbation. When the spin–orbit coupling is strong, selection rules on L and S cannot be used. However, if J is still a good quantum number, the selection rule of DJ 2l is still valid. For example, in most of solids and liquids, it is difﬁcult to observe the 6H15/2 ! 6F1/2 transition of Dy3+ ions, although it is easy to observe the 6 H15/2 ! 6F3/2 transitions. Nevertheless, the selection rules related to the irreducible representations of the site symmetry of active ions are strictly valid. The irreducible representation D1u of the electric-dipole moment of full-rotational group can be reduced to the irreducible representations of the site symmetry of active ions as: D1u ¼

X

Pj

j

If the ﬁnal state is denoted by JSCf and the initial state by jJSCi i, then the P selection rule is: Ci C f j Pj , that is, the product of the irreducible representation of the initial state Ci with the complex conjugate irreducible representation of ﬁnal state C f should include the irreducible representation of the dipole P moment operator j Pj . For a uniaxial crystal, the p spectra have selection rules different from those of the r spectra, because the irreducible representations of p and r dipole moments are different. Let us take Nd3+:YVO4 as an example to explain how to use group theory to introduce the selection rule. Nd3+ ions in this crystal occupy D2d point

118

4 Theory of Radiative Transition

group positions; in this group all the irreducible representations are real and so C f ¼ Cf . The electric-dipole moment can be reduced to the following irreducible representations according to branching rule by Butler’s book [8] as well as the table in Appendix B. P1u ðSO3 Þ ¼ C5 ðD2d Þ C4 ðD2d Þ Among these representations, it can be seen by Appendix A that the one-dimensional C4(D2d) corresponds to the z component of the electric-dipole moment and the two-dimensional C5(D2d) corresponds to the x, y components of the electric-dipole moment. If one has Ci ⊗ C4 = Cf ⊕ , then the polarization direction of emission or absorption spectral lines will be along the z direction, that is, the p polarization transition is allowed. If one has Ci ⊗ C5 = Cf ⊕ , then the polarization direction of emission or absorption spectral lines will be along the x, y directions, that is, the r polarization transition will be allowed. For the crystal Nd3+:YVO4, the crystal ﬁeld wave functions with D2d point symmetry were given in reference [9]. For the fluorescence spectra corresponding to the transition 4F3/2 ! 4 I11/2, one of the spectra denoted by b ! a means transition from b level of 4F3/2 to a level of 4I11/2. These two levels belong to the irreducible representation C7. By using the table of irreducible representation product (Appendix C or reference [10]), it is easy to obtain C7 C5 ¼ C7 C6 ; C7 C4 ¼ C6 Obviously, the second product does not include irreducible representation C7 of the ﬁnal state. Therefore, the emission spectral line can only be r polarization. For some other transitions, the above two direct products of irreducible representations can include irreducible representations of the ﬁnal state. Thus, the emission or absorption spectral line can be both r and p polarizations. What kind of polarization can be observed in a particular situation should be determined by their relative strengths and this problem will be introduced later. The selection rules for transitions of active ions in materials can be tabulated as in the work of Wybourne [11] for the case of electric-dipole transitions in the D3h symmetry system which has even number of electrons (Table 4.1). For a system with odd number of electrons, similar selection rules can be obtained. However, double-value representations were introduced to match the Table 4.1 Selection rule of electric-dipole transition in the D3h symmetry system having even number of electrons

Irresp. of the level

C1

C2

C3

C4

C5

C6

C1 C2 C3 C4 C5 C6

– – – p – r

– – p – – r

– p – – r –

p – – – r –

– – r r r p

r r – – p r

4.3 Selection Rules for Radiative Transition

119

situations of the half-integer J. In this case, electric-dipole moment belongs to C4 (p-polarization) and C6 (r-polarization) and all the energy levels belong to C7, C8, and C9 representations. According to the table of representation product, it is easy to see that: C7 C4 ¼ C8 ; C8 C4 ¼ C7 ; C9 C4 ¼ C9 ; C9 C7 ¼ C9 C8 ¼ C5 C6 C7 C6 ¼ C8 C9 ; C8 C6 ¼ C7 C9 ; C9 C6 ¼ C7 C8 ; C9 C9 ¼ C1 C2 C3 C4 Therefore, one has the Table 4.2. Selection rules for other point group symmetry systems can be obtained in a similar way. We show here some examples for laser crystals. The rare earth ions occupy D2d, S4, and D3 positions in YVO4, LiYF4, and YAl3(BO3)4 crystals, respectively. It should be noted that some of the irreducible representations of the point groups D3 and S4 are complex representations, and to determine the selection rule the conjugate irreducible representation of ﬁnal state must be used. For example, the electric-dipole transition C3 ! C4 of S4 position because the z component of the electric-dipole moment belongs to irreducible representation C2 and C3 ⊗ (C4)* = C2 and that the electric-dipole transition C3 ! C4 is p polarized. According to the same method, the electrical-dipole transition rules of even and odd electronic systems are listed in Table 4.3 for the positions with point symmetries of D2d, S4, and D3. From the wave functions, crystal ﬁeld quantum numbers, and their corresponding irreducible representations of point group D3 for Nd3+:NAB crystal quoted in Chap. 3, it can be seen that the polarization character of 22 spectral lines produced by the transitions from 4F3/2(1, 2) to 4I9/2(1, 2 … 5) and 4I11/2(1, 2 … 6) are all the same as those calculated in the literature [12] by relating intensity of emission spectra (see Tables 2–5 of that paper). Especially, two transition lines which have been observed by Winzer [13] in his laser experiment: irreducible representations of energy levels 4F3/2(1) and 4I11/2(2) are C4 and that for energy level 4I11/2(3) is C5,6. According to Table 4.3, the light emitted by the transition of 4 F3/2(1) ! 4I11/2(2) can be r or p polarization, but the light emitted by the transition of 4F3/2(1) ! 4I11/2(3) can only be r polarization. These are in agreement with the calculation results of Table 2 of paper [12] and fully conﬁrmed by the laser experiment of Winzer [13]. Winzer used two Nd3+:NAB crystal plates with two different orientations. The surface of ﬁrst crystal plate was perpendicular to the optic axis while the direction of pumping light and laser light were parallel to the optical axis. On the other hand, the surface of second crystal plate was parallel to the Table 4.2 Selection rule of electric-dipole transition in the D3h symmetry system having odd number of electrons

Irresp. of the level

C7

C8

C9

C7 C8 C9

– rp r

rp – r

r r p

120 Table 4.3 Selection rule of electric-dipole transition in the D2d, S4, and D3 symmetry systems

4 Theory of Radiative Transition D2d

C1

C2

C3

C4

C5

C1 C2 C3 C4 C5 C6 C7 S4

– – – p r

– – p – r

– p – – r

p – – – r

r r r r p

C1 C2 C3 C4 C5 C6 C7 C8 D3 C1 C2 C3 C4 C5 C6

C1

C2

C3

C4

– p r r

p – r r

r r – p

r r p –

C1

C2

C3

– p r

p – r

r r rp

C5

– r p r C4

rp r r

C6

C7

r rp C6 C7

r – r p

rp r C8

p p – r

r r r –

C5

C6

r – p

r p –

optical axis while the direction of pumping light and laser light were perpendicular to the optic axis. From the ﬁrst crystal plate, r polarization laser emission at wavelength 1065.5 nm corresponding to the transition of 4F3/2(1) ! 4I11/2(3) was observed, while from the second crystal plate, r polarization as well as p polarization laser emission at wavelength 1063.8 nm corresponding to the transition of 4 F3/2(1) ! 4I11/2(2) also were observed. Finally, some problems about magnetic-dipole selection rules should be mentioned. This kind of transition is allowed within the same conﬁguration. The probability of magnetic-dipole transition is proportional to the following square of matrix element hw jL þ 2Sw 2 i f In the case that the related quantum numbers are approximately good quantum numbers, the selection rules for free ions are mention previously.

4.3 Selection Rules for Radiative Transition

121

However, the total transition probability between multiplets is distributed into different crystal ﬁeld levels by the interaction of crystal ﬁeld and their selection rule should be introduced by the group theory method. For example in the uniaxial crystal, in case of magnetic-dipole transition, it is generally necessary to measure three kinds of polarization spectra: a spectrum, the light transmits along optic axis c with E⊥c, H⊥c; r spectrum, the light transmits perpendicular to optic axis c with E⊥c, H//c, and p spectrum, the light transmits perpendicular to optic axis c with E//c, H⊥c. L = r p is an axial vector and so the transformation property of Lx, Ly, and Lz is the same as that of Rx, Ry, and Rz. In case of E⊥c or H⊥c, the condition of electric-dipole transition and magnetic-dipole transition is Ci CRx;y C f ¼ Ci Cx;y C f C1 In case of E//c or H//c, the condition of electric-dipole transition and magnetic-dipole transition is Ci CRz C f ¼ Ci Cz C f C1 If the rare earth ions occupy position with D3 point group, by the irreducible representation character table of group D3 in Appendix A, it can be seen that Rx, Ry and x, y belong to irreducible representation C3 while Rz and z belong irreducible representation C2. Therefore, in case of E⊥c or H⊥c the condition of electric-dipole transition and magnetic-dipole transition is Ci C3 C f C1 On the other hand, in case of E//c or H//c, the condition of electric-dipole transition and magnetic-dipole transition is Ci C2 C f C1 First, to see transition C4,C4, it can be found from Appendix C that the related irreducible representation product is (note that C4 is a real irreducible representation) C4 C3 C4 C1

C4 C2 C4 C1

Therefore, no matter E//c or E⊥c and H//c or H⊥c, C4,C4 can have electric-dipole and magnetic-dipole transitions. It means that the a,r, and p polarized spectra between different energy C4 levels can be observed and these three kinds of spectra all have electric-dipole and magnetic-dipole transition components.

122

4 Theory of Radiative Transition

Next to see the transition of C4,C5,6. Here C5 and C5 are conjugate to each other and constitute a doubly degenerate level and so written as C5,6 C4 C3 C5;6 C1 ; C4 C2 C5;6 62 C1 Therefore, between C4 and C5,6 we can have electric-dipole transition with E⊥c and magnetic-dipole transition with H⊥c. It means that between these two kinds of energy levels, the a, r, and p polarized spectra can be observed but the r polarized spectrum only has the component of electric-dipole transition and the p polarized spectrum only has the component of magnetic-dipole transition. Last to see the transition of C5,6,C5,6, one has C5;6 C2 C5;6 ¼ C1 ; C5;6 C3 C5;6 62 C1 By using the above discussion method, it can be shown that between two energy levels C5,6, the p and r polarized spectra can be observed, but p polarized spectrum only has the component of electric-dipole transition and r polarized spectrum only has the component of magnetic-dipole transition. The selection rule can be summarized in the Table 4.4. When rare earth ion occupies a position with other point group, their transition selection rules can be introduced by the similar method. It should be noted that Table 4.4 only shows the polarization character between crystal ﬁeld levels. The precondition for magnetic-dipole transition is the related transition should be allowed by magnetic-dipole selection rule between related multiplets. Because the intensity of electric-quadrupole transition is very weak, we would not discuss their transition selection rule. Actually, it is easy to use similar method to introduce their transition selection rule so long as one knows that the components of quadrupole moment transform as those of x2, y2, z2, xy, yz, and zx, then ﬁnd out the irreducible representation of these functions from character table of irreducible representation.

Table 4.4 Selection rule for rare earth ion occupy D3 point group position Irresp. of the energy level

C4

C5,6

C4 C5,6

a(ed.,md.), r(ed.,md.), p(ed., md.) a(ed., md.), r(ed.), p(md.)

a(ed., md.), r(ed.), p(md.) p(ed.), r(md.)

References

123

References 1. A.S. Davydov, Quantum Mechanics, 2nd edn. (Pergamon Press, Oxford, 1976) 2. L.D. Landau, E.M. Lifshitz, Field Theory (Pergamon Press, Oxford, 1958) 3. H. Goldstein, Classical Mechanics (Addison-Wesley Publishing Company, Inc., Third Printing, 1953) 4. W. Heitler, The Quantum Theory of Radiation (Clarendon Press, Oxford, 1954) 5. I.N. Broushtein, K.A. Semendyayev, Handbook of Mathematics (Van Nostrand Reinhold Company, New York, 1985) 6. P. Hong, S.R. Shinn, Matter. Res. Bull. 11, 461 (1976) 7. M. Tinkham, Group Theory and Quantum Mechanics (McGraw-Hill Inc., New York, 1964) 8. P.H. Butler, Point Group Symmetry Application Method & Tables (Plenum Press, New York, 1981) 9. Z.D. Luo, Y.D. Huang, J. Phys, Condens. Matter. 6, 3737 (1994) 10. G.F. Koster, J.O. Dimmock, R.G. Wheeler, et al. Properties of Thirty-Two Point Group (M.I. T. Press, Massachusetts, 1963) 11. B.G. Wybourne, Spectroscopic Properties of Rare Earths (Wiley, New York, 1965) 12. Y.D. Huang, Z.D. Luo, J. Phys.: Condens. Matter 5, 1581 (1993) 13. G. Winzer, P.C. Mocke, W.W. Krcehler, IEEE J. Quant. Elect. QE, 14(840) (1978)

Chapter 5

Spectroscopic Parameter and Their Calculation

5.1

Absorption Coefﬁcient, Absorption (Emission) Cross-Section, and Oscillator Strength

In the studies of spectroscopic properties of crystals and non-crystalline solid materials, the physical parameters normally used are absorption coefﬁcient, absorption (emission) cross-section, and oscillator strength but not the transition probability. We would like to discuss their physical meaning and calculation formulas while only deal with particular calculation problems of trivalent rare earth ion in this chapter. The calculation of spectroscopic parameters for transition metal ion is put into Chap. 7. In the previous discussion on transition probability, it was assumed that the electric ﬁeld acting on the electrons was the electric ﬁeld of external radiation ﬁeld. This is in fact only valid in vacuum. In solid materials, if radiation electric ﬁeld is denoted by E, and the local ﬁeld of electron is denoted by Eloc, then the transition matrix elements, which involve the electric ﬁeld acting on the electrons, should be multiplied by a factor of Eloc/E and the transition probabilities should be multiplied by a factor of (Eloc/E)2. This factor has different expressions for different local symmetries. In cases of high symmetry, it can be shown that its form is [(n2 + 2)/3]2 (where n is refractive index of the solid material). This correction factor is also used in low symmetry situations now. On the other hand, the velocity of light in the materiel should be c/n. Therefore, from (4.19) and (4.20), the electric-dipole absorption (stimulated emission) and spontaneous emission probabilities will become: Ped k ðabs:Þ ¼ Pk ðst:em:Þ ¼

2 4x3k n n2 þ 2 nk jlj2 3hc3 3

© Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8_5

ð5:1Þ

125

126

5 Spectroscopic Parameter and Their Calculation

Ped k ðsp:em:Þ ¼

2 4x3k n n2 þ 2 jlj2 3hc3 3

ð5:2Þ

where e = n2 has been used in obtaining the above formulas. The spontaneous emission probability is usually denoted by A and given by Aed ¼

2 4x3k n n2 þ 2 jlj2 3 3hc3

ð5:2aÞ

By similar introduction, replacing the refractive index correction factor (n2 + 2)2/ 9n by n, it can be shown that the probability of spontaneous magnetic-dipole emission is Amd ¼

4x3k n3 md 2 M 3hc3

ð5:2bÞ

Integrations over the solid angle have been made in obtaining these formulas and l is used to denote the electric-dipole matrix element. M md is used to denote the magnetic-dipole matrix element. In order to express the transition probabilities of absorption and stimulated emission, photon number nk is usually replaced by photon energy density d(xk) or light intensity I(xk). One can obtain their relation in the following discussion. The energy of photon ﬁeld per unit volume is photon energy density d(xk) integrated over frequency xk. It can also be expressed as the k integral of two times the product of photon energy, photon number, and wave vector density (there are two polarization directions belonging to each particular direction of k). Therefore one has Z

2 dðxk Þdxk ¼ V

Z hxk

1 nk þ qðkÞdk 2

By using qðkÞdk ¼

V Vx2k n3 4pk 2 dk ¼ dxk 3 8p 2p2 c3

we ﬁnally have dðxk Þ ¼

hx3k n3 nk p2 c3

5.1 Absorption Coefﬁcient, Absorption (Emission) Cross-Section …

127

and nk ¼

p 2 c3 dðxk Þ hx3k n3

Substituting (5.3) into (5.1), the following can be obtained 2 4p2 n2 þ 2 ed Ped ðabs:Þ ¼ P ðst:em:Þ ¼ dðxk Þjlj2 k k 3 3h2 n2

ð5:3Þ

ð5:4Þ

By using Iðxk Þ ¼ nc dðxk Þ; formula (5.4) changes into Ped k ðabs:Þ

¼

Ped k ðst:em:Þ

2 4p2 n2 þ 2 ¼ 2 jlj2 Iðxk Þ 3 3h nc

ð5:5aÞ

Similarly md Pmd k ðabs:Þ ¼ Pk ðst:em:Þ ¼

4p2 n md 2 Iðxk Þ M 3h2 c

ð5:5bÞ

Let us consider a light beam passing through a system with two energy levels E1 1 and E2 along x direction (E2 and E1 satisfying xk ¼ E2 E h ). N2 and N1 are the particle densities of the high and low energy levels having degeneracy g1 and g2, respectively. The electron in the low energy level absorbs light and go up to the high energy level; at the same time, the electron in the high energy level emits light and go down to the low energy level. Therefore, in the calculation of light absorption, the contributions from two kinds of transition must be considered. Pk(1n, 2m) is used to denote the transition probability from the nth degenerate state in level 1 to the mth degenerate state in level 2 and the transition probability from the mth degenerate state in level 2 to the nth degenerate state in level 1 is expressed by Pk(2m, 1n). m and n are used to denote the degenerate states of high and low levels, respectively. Therefore, the total transition probability of the level 1 into level 2 should be averaged over all the initial degenerate states of level 1 and summed over all the ﬁnal degenerate states of level 2. In this calculation, the spontaneous emission has been neglected, because it is very weak compared to the stimulated emission. Thus W12 ¼

1 X Pk ð1n ; 2m Þ g1 1n ;2m

ð5:6Þ

Similarly, the total transition probability from level 2 to level 1 is W21 ¼

1 X Pk ð2m ; 1n Þ g2 1 ;2 n

m

ð5:7Þ

128

5 Spectroscopic Parameter and Their Calculation

According to (5.1) or (5.5a, 5.5b), Pk (2m, 1n) = Pk (1n, 2m), therefore g1 W12 ¼ g2 W21

ð5:8Þ

By means of the results obtained, it can be seen that because of the absorption, the light passing through a solid material will be attenuated. Its intensity change in a distance dx can be expressed as g2 dIðxk Þ ¼ ðN1 W12 N2 W21 Þhxk dx ¼ N1 N2 W12 hxk dx g1 " # 2 2 4p2 ðn2 þ 2Þ N1 X l1n 2m xk gðxk Þ Iðxk Þdx ¼ 3hc 9ng1 1n ;2m

ð5:9Þ

jed ðxk ÞIðxk Þdx where g(xk) is introduced to take into account the absorption line shape and the value of g1N2/g2 has been neglected, because particle number in the excited state is much smaller than that in the ground state. Hence the intensity variation by passing through the media for distance x can be expressed as Iðxk Þ ¼ I0 ðxk Þejðxk Þx

ð5:10Þ

where j(xk) is the absorption coefﬁcient deﬁned as follows jed ðxk Þ ¼

2 4p2 ðn2 þ 2Þ2 N1 X l1n 2m xk gðxk Þ 3hc 9ng1 1 ;2

ð5:11aÞ

4p2 n N1 X md 2 M 12 xk gðxk Þ 3hc g1 1 ;2

ð5:11bÞ

n

m

Similarly jmd ðxk Þ ¼

n

m

The line shape factor g(xk) is normalized according to Z gðxk Þdxk ¼ 1 If one uses wavelength as variable, it should be noted that Z Z Z 2pc gðxk Þdxk ¼ gðxk Þdkk ¼ gðkk Þdkk ¼ 1 k2k n

5.1 Absorption Coefﬁcient, Absorption (Emission) Cross-Section …

129

so that gðxk Þ ¼

k2k n gðkk Þ 2pc

R The result of jðkk Þdkk should be ! Z Z 2 2 2 2pc kk n 4p2 n ðn2 þ 2Þ N1 X ed j ðkk Þdkk ¼ gðkk Þdkk l1n 2m 2pc 3hc kk n 9ng1 1 2 n m

3

2 8p k ðn þ 2Þ N1 X ¼ l1n 2m 3hc 9ng1 1 ;2 2

2

n

m

Similarly ! Z Z 2 2 X k n 4p n N 2 1 k M md 2pc gðkk Þdkk jmd ðkk Þdkk ¼ 12 2pc 3hc g1 1 2 kk n n m

8p3 kk nN1 X md 2 ¼ M 12 3hcg1 1 1 ;2 n

ð5:12aÞ

ð5:12bÞ

m

R where the average wavelength can be expressed as k ¼ kk gðkk Þdkk . Equations (5.12a) and (5.12b) are widely applied in spectroscopic calculations. v = (n2 + 2)2/9n was introduced as a correction factor by refractive index of the solid material in the literature (e.g. [1]). Therefore ! Z 2 N1 8p3 k X ed v j ðkk Þdkk ¼ l ð5:13Þ g1 3hc 1n ;2m 1n 2m The absorption cross-section and emission cross-section are often used to express absorption rate and emission rate in spectroscopy. Absorption cross-section is deﬁned as the quotient of the absorption coefﬁcient divided by the number of absorption centers per unit volume. Therefore, the absorption cross-section r12(xk) and r12(kk) as the functions of xk and kk, respectively, can be expressed as 2 4p2 xk X red v l1n 2m gðxk Þ ð5:14aÞ 12 ðxk Þ ¼ 3hcg1 1 ;2 n

rmd 12 ðxk Þ ¼

m

4p2 xk n X md 2 M 12 gðxk Þ 3hcg1 1 ;2 n

Z red 12 ðkk Þdkk

¼

ð5:14bÞ

m

2 8p3 k X v l1n 2m 3hcg1 1 2 n m

! ð5:15aÞ

130

5 Spectroscopic Parameter and Their Calculation

Z rmd 12 ðkk Þdkk

8p3 kn X md 2 M 12 3hcg1 1 2

¼

! ð5:15bÞ

n m

The oscillator strength of certain transition in spectroscopy can be deﬁned as the ratio of the power emitted or absorbed by the transition to the power emitted or absorbed by a classical oscillator. The power emitted or absorbed by a classical oscillator can be introduced from the following discussion. Let us discuss the oscillator strength of electric-dipole transition ﬁrst. By using classical radiation theory, the movement equation for an electric-dipole oscillator can be written as m€x þ Rx_ þ Gx ¼ eEx eixt

ð5:16Þ

The second and the third terms in the above equation are the resistant force and the restoring force of the free oscillator, respectively. The term on the right-hand side of the equation represents the driving force of the radiation ﬁeld, where x_ denotes the ﬁrst-order derivative dx/dt and €x is the second-order derivative d2x/dt2. Assuming that without the driving force of external electric ﬁeld, the vibrational frequency of the free oscillator is x0. The solution of (5.16) should be x0 eðc=2Þt cosðx0 t bÞ = (the general solution of the homogeneous equation) plus eEx cosðxtaÞ m 1=2 (c = R/m) (the special solution of the inhomogeneous ðx20 x2 Þ2 þ c2 x2 equation). The work done by the radiation ﬁeld driving force F(x) = eExeixt moving a distant dx is dw = F(x)dx = F(x)(dx/dt)dt. If F(x) is calculated by the left side of (5.16), then the power done by radiation ﬁeld driving force for all the frequency x will be Z1 Z1 dw _ P¼ ðm€x þ Rx_ þ GxÞxdx dx ¼ dt 0

0

Substituting the solution of x into above equation and using the approximate relations: x0 x, x2 − x20 2x(x0 − x), and noting that the time averages of both €xx_ and xx _ are zero and the free oscillation component of x decays to zero quickly, one can obtain Z1 P¼ 0

e2 Ex2 c Rx_ dx ¼ 8m 2

Z1

dx 2

0

ðx0 xÞ þ c2 =4

¼

2pe2 Ex2 8m

where c = R/m has been taken in the above equation. Taking into account the time-averaged energy density of the radiation ﬁeld qx ¼ Ex2 =8p and the radiation intensity IðxÞ ¼ cqx , the following relationship between the average absorption

5.1 Absorption Coefﬁcient, Absorption (Emission) Cross-Section …

131

power of a classical oscillator in the vacuum and the intensity of the radiation ﬁeld can be obtained P¼

2p2 e2 IðxÞ mc

ð5:17Þ

According to the deﬁnition, the power absorbed by the transition of an electron hxW12 must be equal to the product of absorption oscillator strength f12 multiplied by P and the factor of line shape gL ðxk Þ; then for the electric-dipole absorption process P hxk n;k Pk ð1n ; 2m Þ 2p2 e2 ed Iðxk Þf12 gL ðxk Þ ¼ hxW12 ¼ g1 mc " # 2 2 4p2 ðn2 þ 2Þ X ¼ l xk gðxk Þ Iðxk Þ 3hc 9ng1 1 ;2 1n 2m n

m

Equation (5.5a) has been used in the derivation of above equation. Therefore, the ed absorption oscillator strength f12 of the electric-dipole is expressed as ed ¼ f12

2 2 m ðn2 þ 2Þ2 X xk l1n 2m 2 3he g1 9n 1 ;2 n

ð5:18aÞ

m

ed Similarly, the emission oscillator strength f21 of the electric-dipole transition is expressed as

ed ¼ f21

2 2 2 m ðn2 þ 2Þ X x l2n 1m k 2 3he g2 9n 1 ;2 n

ð5:18bÞ

m

According to the same discussion method, remember that the refractive index correction factor (n2 + 2)2/9n should be replaced by n and the electric-dipole matrix element replaced by the magnetic coupling matrix element. The absorption oscilmd of the magnetic-dipole transition is expressed as lator strength f12 md f12 ¼

X 2 m M md 2 x n k 12 3he2 g1 1 ;2 n

ð5:18cÞ

m

md The corresponding emission oscillator strength f21 of the magnetic-dipole transition is expressed as md ¼ f21

X 2 m M md 2 xk n 21 2 3he g2 2;1 m

ð5:18dÞ

132

5 Spectroscopic Parameter and Their Calculation

ed The absorption oscillator strength f12 of electric-dipole transition for the trivalent rare earth ions in solids is in the order of magnitude 10−5–10−6 and for the divalent rare earth ions, it can reach the order of magnitude 10−2–10−3, nearly the same as that for the transition in 3dn conﬁgurations of transition-metal ions. One can see another deﬁnition of the absorption oscillator strength in the literature as follows ed f12 ¼

X 2 m l 2 xk 1n 2m 2 3he g1 1 ;2 n

ð5:19Þ

m

It gives the ratio of the power of the absorption to that of the classical oscillator, if the transition concerned is taking place in the vacuum. Obviously, the deﬁnition what we adopted can describe the actual situation for the transition occur in material and is much more reasonable. It is also the same as that given by Judd [2] and other classical literature [3].

5.2

Analysis of the Absorption Coefﬁcients of Anisotropic Crystal

Consider the general situation of biaxial crystals. If the absorption coefﬁcients of the crystal for the light polarized in the direction of crystal physical axes X, Y, and Z are denoted by jX, jY, and jZ, respectively, the absorption coefﬁcients for the light polarized in any direction can be calculated by the following way. Suppose the light is polarized in the direction with angle variables h and u in the spherical coordinate system constituted by crystal physical axes X, Y, and Z, then the electric ﬁeld E of the light has projections of Esinhcosu, Esinhsinu, and Ecosh in the directions of coordinate axes X, Y, and Z, respectively. Obviously, the light intensity of the component polarized in the directions of X, Y, and Z will be I0sin2hcos2u, I0sin2hsin2u, and I0cos2h, respectively. After the light pass through a crystal with thickness L, the intensity I of the transmitted light will be I ðh; uÞ ¼ I0 sin2 h cos2 u exp jðxÞ L þ I0 sin2 h sin2 u exp jðyÞ L þ I0 cos2 h exp jðzÞ L

I ðh; uÞ=I0 ¼ sin2 h cos2 u exp jðxÞ L þ sin2 h sin2 u exp jðyÞ L þ cos2 h exp jðzÞ L

where jðxÞ , jðyÞ , jðzÞ are the absorption coefﬁcients of the crystal for the light polarized in the direction of the axes X, Y, and Z, respectively. It can be demonstrated that the absorption coefﬁcients of the crystal for the light with wavelength k can be calculated by

5.2 Analysis of the Absorption Coefﬁcients of Anisotropic Crystal

133

1 I ðh; uÞ jðk; h; uÞ ¼ lim ln jL!0 L I0 ðxÞ 2 2 ¼ j ðkÞ sin h cos u þ jðyÞ ðkÞ sin2 h sin2 u þ jðzÞ ðkÞ cos2 h

ð5:20Þ

In a uniaxial crystal, the absorption coefﬁcients for the light polarized in X and Y directions are equal and denoted by jr and the absorption coefﬁcient for the light polarized in Z direction is denoted by jp, then jðk; h; uÞ ¼ jðrÞ ðkÞ sin2 h þ jðpÞ ðkÞ cos2 h

ð5:21Þ

If the unit vector of the electric ﬁeld E is denoted by e, and the unit vectors of X, Y, and Z axes are denoted by x, y, and z, respectively, then (5.20) can be expressed as jðe; kÞ jðxÞ ðkÞðe xÞ2 þ jðyÞ ðkÞðe yÞ2 þ jðzÞ ðkÞðe zÞ2

ð5:20aÞ

It is known from Born and Wolf [4] that an unpolarized light transmitting in the direction of h′, u′ with intensity I0 can be considered as two lights polarized in the direction perpendicular to the direction of h′, u′ with intensity I0/2. If these two polarized light beams pass through a uniaxial crystal with thickness L, the intensity of the transmitted light can be expressed as h i 1 h i 1 It ðk; h0 ; u0 Þ ¼ sin2 h0 I0 exp jðpÞ L þ 1 þ cos2 h0 I0 exp jðrÞ L 2 2 where h′ is the angle between the incident light I0 (i.e. the normal direction of the crystal) and the optic c axis (i.e. the direction of the crystal physical Z axis). The absorption coefﬁcient can be expressed as h i 1 h i

1 1 jðk; h0 ; u0 Þ ¼ lim ln sin2 h0 exp jðpÞ ðkÞL þ 1 þ cos2 h0 exp jðrÞ L jL!0 L 2 2

ð5:22Þ This expression is the same as that obtained by Lomheim and Deshazer [11]. Physically, j(k, h′,u′) should be obtained in the condition of jL 1. Satisfying this condition then one has 1 1 jðk; h0 ; u0 Þ jðpÞ sin2 h0 þ jðrÞ 1 þ cos2 h0 2 2

ð5:23Þ

Note that the angle parameters h′, u′ are different from h, u. The expression (5.23) can also be obtained by (5.21): According to the method mentioned above, an unpolarized light with intensity I0 and transmitting in the direction of h′, u′ can be decomposed into two lights of intensity I0/2 with

134

5 Spectroscopic Parameter and Their Calculation

polarization direction h1 = h′ + p/2, u1 = u′ and h2 = p/2, u2 = u′ + p/2, respectively. Then by (5.21) one can obtain 1 ðrÞ j ðkÞsin2 ðh0 þ p=2Þ þ jðpÞ ðkÞcos2 ðh0 þ p=2Þ 2 1 ðrÞ j ðkÞsin2 ðp=2Þ þ jðpÞ ðkÞcos2 ðp=2Þ þ 2 jðrÞ ðkÞ 1 ðrÞ j ðkÞcos2 h0 þ jðpÞ ðkÞsin2 h0 þ ¼ 2 2 1 ðpÞ 1 ðrÞ 2 0 2 0 ¼ j ðkÞsin h þ j ðkÞð1 þ cos h Þ 2 2

jðk; h0 ; u0 Þ ¼

Clearly, for a biaxial crystal, calculated by (5.20), we can show 1 4p

Z

Z Z Z 1 1 1 jðk; h; uÞdX dk ¼ jðxÞ dk þ jðyÞ dk þ jðzÞ dk 3 3 3 1 ðXÞ C þ CðYÞ þ CðZÞ ¼ 3 ð5:24Þ

Z

CdX ¼

1 4p

Z

where C is the integral of the absorption coefﬁcient over the wavelength range and is usually called absorbance. For uniaxial crystal, one has 1 4p

Z

Z CdX ¼

1 4p

Z

Z Z 1 2 ðpÞ jðk; h; uÞdX dk ¼ j dk þ jðrÞ dk 3 3

1 2 ¼ CðpÞ þ CðrÞ 3 3

ð5:25Þ

The probability of spontaneous transition polarized in q direction can be expressed as PðqÞ ðsp:em:Þ ¼

8pcn2 ðqÞ C 3k4 N1

8pcn2 ðXÞ ðYÞ ðZÞ C þ C þ C 3k4 N1 8pcn2 1 ðpÞ 2 ðrÞ C þ C Pðsp:em:Þ ¼ 4 3 k N1 3

Pðsp:em:Þ ¼

ð5:26Þ ð5:27Þ ð5:28Þ

One of the author’s paper [5] has shown that if one cannot measure polarized absorbance data but would like to obtain effective J–O parameters, then the total integrated absorbance resulting from unpolarized integrated absorbance data measured by three thin crystal slice mutual perpendicularly cutting from an arbitrary orientation crystal cube is a good approach to the space integrated averaged

5.2 Analysis of the Absorption Coefﬁcients of Anisotropic Crystal

135

absorbance required by (5.24) and (5.25). This can also be generally demonstrated by (5.20a). Suppose three unpolarized light beams are input in three mutually perpendicular directions of e1, e2, and e3, respectively, then by using the method mentioned above, an unpolarized light of intensity I0 can be decomposed into two polarized lights of intensity I0/2 with polarization directions perpendicular to each other, in the condition of jL 1. According to (5.20a), the absorption coefﬁcients in these three directions can be calculated by 1 ðe2 xÞ2 jðxÞ þ ðe2 yÞ2 jðyÞ þ ðe2 zÞ2 jz j1 jðe1 Þ 2 1 ðe3 xÞ2 jðxÞ þ ðe3 yÞ2 jðyÞ þ ðe3 zÞ2 jz þ 2 1 ðe1 xÞ2 jðxÞ þ ðe1 yÞ2 jðyÞ þ ðe1 zÞ2 jðzÞ j2 jðe2 Þ 2 1 ðe3 xÞ2 jðxÞ þ ðe3 yÞ2 jðyÞ þ ðe3 zÞ2 jðzÞ þ 2 1 ðe1 xÞ2 jðxÞ þ ðe1 yÞ2 jðyÞ þ ðe1 zÞ2 jðzÞ j3 jðe3 Þ 2 1 ðe2 xÞ2 jðxÞ þ ðe2 yÞ2 jðyÞ þ ðe2 zÞ2 jðzÞ þ 2 Taking e1, e2, and e3 as three axes of the coordinate system, the transformation of the XYZ coordinate system into the e1e2e3 coordinate system is a real orthogonal transformation with constant vector length. Remember that x, y, z are unit vectors in the XYZ coordinate system, so that X i¼1;2;3

ðei xÞ2 ¼ jxj2 ¼ 1;

X

ðei yÞ2 ¼ jyj2 ¼ 1;

i¼1;2;3

X

ðei zÞ2 ¼ jzj2 ¼ 1

i¼1;2;3

Apply these three relations, then one can obtain jð1Þ þ jð2Þ þ jð3Þ jðxÞ þ jðyÞ þ jðzÞ On integration over the wavelength, it is shown that Cð1Þ þ Cð2Þ þ CðZÞ CðXÞ þ CðYÞ þ CðZÞ

ð5:29Þ

Obviously, when one cannot measure the polarized absorption spectra of anisotropic crystals, it is possible to use the above method and formulas (5.27) and (5.28) to calculate the probability of spontaneous emission and radiative lifetime. It should be emphasized once again that in order to obtain a precise result the condition jL 1 should be satisﬁed.

136

5.3

5 Spectroscopic Parameter and Their Calculation

Judd–Ofelt Approximation and Related Parameter

In the studies of spectroscopic properties of rare earth ions, the intensity parameter method introduced by Judd [2] and Ofelt [6] has become a popular and useful method, especially the Judd–Ofelt three-parameter method, although it involves many approximations. In this section, the Judd-Ofelt three-parameter method will be introduced. By using this method, radiative lifetime, quantum efﬁciency, emission cross-section, and absorption cross-section of laser and luminescent materials can be calculated (see, e.g., [7]). From the discussion previously given, it can be seen that the spontaneous electric-dipole emission polarized in the direction eq from an energy level with degeneracy g2 has a probability of ¼ PedðqÞ sp

2 2 64p4 m3 n n2 þ 2 huf jeq Pjui i 3 3hc g2 3

ð5:30Þ

where P denotes the electric-dipole moment P ¼ e

X

ri

ð5:31Þ

i

If one uses spherical tensors Cq1 to express electronic radius r, then eq P ¼ e

X ri Cq1 Dð1Þ q i

i

ð5:32Þ

where q can be −1, 0, and +1, for uniaxial crystal, q = 0 corresponds to p polarization and q = ±1 corresponds to r polarization. Similar to (5.14a), the integral of the absorption coefﬁcient can be written as Z jedðqÞ ðxÞdx ¼

2 2 4p2 e2 xN 1 1 ð1Þ 4p2 xN v uf eq Pjui i ¼ v uf Dq jui i ð5:33Þ 3hcg1 3 hcg1

The problem now is how to calculate the above matrix elements. For the rare earth ions, electric-dipole transition between levels of the same 4fn conﬁguration is forbidden originally. The method of Judd and Ofelt is based on the consideration that the wave function of another conﬁguration with different parity can mix into the transition involving initial and ﬁnal state wave functions and then the electric-dipole transition matrix element will be non-zero. This admixture is produced by the interactions of odd parity, namely odd crystal ﬁeld potential and odd crystal vibrational mode. If one denotes the odd crystal ﬁeld potential as Vod, then the perturbed wave functions expanded to ﬁrst-order terms of Vod are given by

5.3 Judd–Ofelt Approximation and Related Parameter

ui ¼ uðf n Ji Mi Þ

137

X hf n Ji Mi jVod juðnlÞi uðnlÞ E ðf n Ji Mi Þ EðuðnlÞÞ uðnlÞ

ð5:34Þ

where u(nl) are the wave functions with parity different from those of the 4f n conﬁguration (the most important is the 4f n−15d conﬁguration). An expression for uf can be written in the same way. The odd parity crystal ﬁeld potential Vod can be expressed as Vod ¼

X

ðtÞ Btp DðtÞ p ; Dp ¼

X rit CpðtÞ

t;p

i

ðt is an odd numberÞ

i

In this way, the matrix element of the electric-dipole transition in a particular polarization direction q can be expressed as D

D E ð1Þ n n E uðnlÞ D f J M V h j juðnlÞ i X q f Jf Mf i i od uf Dð1Þ q ui ¼ Eðf n Ji Mi Þ EðuðnlÞÞ uðnlÞ D E ð1Þ X f n Ji Mi Dq uðnlÞ uðnlÞjVod jf n Jf Mf E f n Jf Mf EðuðnlÞÞ uðnlÞ

ð5:35Þ

It can be shown that [2] XD

E ED n f n Ji Mi Dð1Þ uðnlÞDðtÞ q uðnlÞ p f Jf Mf

uðnlÞ

¼

X

ð1Þp þ q Btp ð2k þ 1Þ

1

k

q p q k D n ðkÞ ðtÞ n lC 3ihf Ji Mi jUp þ q f Jf Mf

t p

1

k

t

3

l

3

D h3jr jlih3jr t jli 3C ð1Þ li

ð5:36Þ In order to calculate the above matrix element, three approximations have to be introduced. First, it is assumed that the states of u(nl) are degenerate with respect to all the quantum numbers except nl. This is a rather rough assumption because, for example, if the intermediate states are those of 4f n−15d conﬁguration, the energy range of this conﬁguration is from 50,000 cm−1 to at least 100,000 cm−1. Hence this approximation will introduce considerable errors in the ﬁnal result. The second approximation is Eðf n Jf Mf Þ EðuðnlÞÞ ¼ Eðf n Ji Mi Þ EðuðnlÞÞ

ð5:37Þ

This is also a very rough approximation, because the errors introduced by taking, for example, a transition from a initial state at about 20,000 cm−1 higher than the ground state to the ﬁnal ground state, the center of the intermediate 4f n−15d

138

5 Spectroscopic Parameter and Their Calculation

conﬁguration state assumed to be at 75,000 cm−1, the difference of E(f nJfMf) − E(u(nl)) and E(f nJiMi) − E(u(nl)) can be larger than 20%. However, it makes possible to combine the two summations in P (5.35) into one term and neglect all details of the intermediate states, by using uðnlÞ juðnlÞihuðnlÞj ¼ 1. The third approximation is that all the crystal ﬁeld energy levels of the initial and ﬁnal multiplets have the same population. However, the different crystal ﬁeld energy level is in fact populated according to the Boltzmann distribution. On the other hand, from the property of 3-j symbol explained in Chap. 2, one has

1 q

k p q

t p

¼ ð1Þ

1þkþt

t p

k p q

1 q

ð5:38Þ

Therefore, only when k is even, the two parts of (5.35) do not counteract each other, because t is an odd number and 1 + t + k should be even. From the tangle condition of 6-j symbol in (5.36) it can be seen that k should satisfy 0 k 6, so that k = 2, 4, and 6. Further calculation of (5.35) can be found in the papers of Judd and Ofelt [2, 6] as well as the books on the angular momentum theory and irreducible tensor method [8, 9]. The ﬁnal result is simply introduced in the following. Owing to the fact that the J–O three-parameter method is used to calculate the electric-dipole transition probability of multiplet to multiplet, the probability should be summed over different crystal ﬁeld levels within the same multiplet. Assuming the same population in all the crystal ﬁeld levels of the same multiplet, it can be shown that the square of transition matrix element in (5.33) can be expressed as E2 E 2 X ðqÞ D ðkÞ D SðqÞ Ji ! Jf ¼ Jf Dð1Þ ¼ X ½aSLJ U ð5:39Þ ½aSLJ J i q f i k k¼2;4;6

D E 2 The square of reduced matrix element ½aSLJ f U ðkÞ ½aSLJ i can be calculated by intermediate approximation wave functions or found from the tables in ðqÞ Kaminskii’s book (Ref. 7 of Chap. 2). The J–O parameters Xk are determined by the spectroscopic experimental method, because the odd crystal ﬁeld potential and odd lattice vibrational mode contributions are difﬁcult to be calculated theoretically. Combining (5.33) with (5.39) and remembering that the degeneracy of the initial state is 2 Ji + 1, it gives:

5.3 Judd–Ofelt Approximation and Related Parameter

CðqÞ

139

2 2 E 2 3 2 nq þ 2 X ðqÞ D ke N 8p 1 ¼ jðqÞ ðkÞdk ¼ Xk ½aSLJ f U ðkÞ ½aSLJ i 2Ji þ 1 3hc 9nq k¼2;4;6 2 2 ke2 nq þ 2 N1 8p3 ¼ SðqÞ ðJi ! Jf Þ 2Ji þ 1 3hc 9nq Z

ð5:40Þ where CðqÞ is referred to as absorbance of polarization q, then the experimental line strength S becomes 2Ji þ 1 3hc 9n CðqÞ ð5:41Þ SðqÞ ðJi ! Jf Þ ¼ 3 2 2 N1 8p ke ðn þ 2Þ2 By using the determined experimental line strength CðqÞ , Sq ðJi ! Jf Þ can be calðqÞ

culated by (5.41) and then Xk can be obtained by the ﬁtting method according to (5.39). It should be reminded that the J–O parameters are used for the electric-dipole transition of rare earth ions. The magnetic-dipole transition probability between some pairs of energy levels of some rare earth ions can reach an order of magnitude comparable with that of electric-dipole transition. For example, the 4I15/2 ! 4I13/2 transition of Er3+ ions and the 4I8 ! 4I7 transition of Ho3+ ions. The experimental spectra include the contribution of the magnetic-dipole transition, and how to correctly calculate J–O parameters in this case, which will be explained in the next section. Now it is possible to demonstrate the selection rule of electric-dipole transition about quantum number JLS for rare earth ion in materials, which has been mentioned in Sect. 4.3. As has been demonstrated above, the k should be 2, 4, and 6. On the other hand, the 0 reduced

matrix element of unit operator in (5.39) includes a J J k 6-j symbol (see (2.52)). From its triangle condition, it can be seen L0 L S that the transition allowed for DJ 6, DL 6 and in case of J or J′ = 0, only DJ = 2, 4, 6 is allowed. J = 0 $ J′ = 0 is forbidden except in the case of the matrix element of zero-order unit tensor operator U(0) exist, which will be discussed later, while by the dSS′ factor in (2.52) DS = 0 should be satisﬁed. The interaction between different multiplets with different J values resulted from even parity crystal ﬁeld, that is J mixing effect, has not been taken into account in the above calculation. Include this J mixing effect, and then the square of reduced matrix element of unit tensor operator should be replaced by the following expression [10, 13]

140

5 Spectroscopic Parameter and Their Calculation

D E2 D E2 ðkÞ ðkÞ ½aSLJ f Ueff ½aSLJ i Wf Jf Ueff Wi Ji 2 0 X X a Wf Jf ; Wf Jf0 a Wi Ji ; W0i Ji0 2 ð5:42Þ ¼ 2Jf0 þ 1 2Ji0 þ 1 W0 J 0 W0 J 0 f f

i i

D E2 W0f Jf0 U ðkÞ W0i Ji0

The coefﬁcients |a(WJ, W′J′)|2/(2 J′+1) is the J mixing coefﬁcients that take into account the mixing of multiplets W′J′ and WJ. The summation of above equation involves all the multiplet W′J′, which is near to the multiplet WJ, and the multiplet WJ itself. When W′J′ 6¼WJ, one has 0 0

2

jaðWJ; W J Þj ¼

X k¼2:4;6

S2k

ðkÞ 0 0 2 WJ U W J ½EðWJÞ EðW0 J 0 Þ

2

In case of W′J′ = WJ, the J mixing coefﬁcients should be calculated by 2

3 X jaðWJ; W0 J 0 Þj2 5 jaðWJ; W J Þj ¼ ð2J þ 1Þ41 2J 0 þ 1 0 0 0 0

2

w J 6¼wJ

The key for the calculation of J mixing coefﬁcients is the calculation of crystal ﬁeld strength coefﬁcient S2k , which should be calculated by means of the data of crystal ﬁeld energy level, because S2k is obtained by the following expression D2 ðWJÞ ¼

X 2 1 X 1 2 ½EðWJnÞ EðWJÞ ¼ S2k hWJ U ðkÞ WJi 2J þ 1 n 2J þ 1 k¼2;4;6

where E(WJn) is nth crystal ﬁeld energy level of multiplet WJ and EðWJÞ is the center of all these energy levels. The practical work of laser material research is not always necessary to determine precisely the crystal ﬁeld energy level position of the multiplets obtained by low temperature spectral measurement. Therefore, it is impossible to use the above equations to calculate line strength S including J mixing effect. However, this effect works only in the case that the strength of even crystal ﬁeld is strong enough and the energy interval between different multiplets is small. For the Nd3+:YVO4 crystal, the RMF error of the absorption intensity parameter S of the 4I9/2 multiplet measure at 300 K, taking into account the J mixing effect only to reduce its value from 0.152 to 0.147 [13]. Certainly, with J mixing effect some of the forbidden magnetic-dipole transition can have certain intensity. Although Judd [2] and Ofelt [6] neither take into account the effect of wave function mixing by ligand wave functions with different parity nor the mixing

5.3 Judd–Ofelt Approximation and Related Parameter

141

contributions of electron-electron Coulomb interaction with spin-orbital interaction in higher approximation, (5.39) is a generally applicable equation. During the past 40 years, after considering all the above mixing effects as well as the dynamic interaction, electron correlation interaction, and relativistic effect, and calculating the second and third-order approximation terms, the (5.39) is still correct. The odd k term introduced by mass polarization effect is small and it has its influence only in the case that the transition is forbidden by standard selection rule; for example, the transition from the multiplet of J = 0 to those odd number J in Eu3+ ions [14]. Other odd k term is very small. After the spectral measurement, the data of absorbance can be calculated from absorption bands. Usually the number of absorbance data obtained is larger than that of Xk (k = 1, 2, 3). The reduced matrix elements of unit operator can be found directly from the literature or calculated by intermediate-coupling wave function and the data are given in the table of literature [15]. (Some of these usually used in laser materials can be found in Appendix D.) By means of (5.41), several equations can be listed and then the ﬁxing method is used to calculate the J–O parameters. As pointed out in Sect. 5.2, for the anisotropic crystals, the absorbance in different direction is usually different, which corresponds to different strength parameter. For a biaxial crystal, there are three kinds of absorption spectra with polarization direction parallel to X, Y, and Z crystallophysics axes and for a uniaxial crystal there are p spectrum with polarization direction parallel to the optics axis and r spectrum with polarization direction perpendicular to the optics axis. Using (Y) (Z) (p) (r) the data of these spectra—X(X) k , Xk , and Xk —Xk and Xk can be calculated and then the emission probability in different polarization directions can be obtained. However, it should be noted that in the evaluation of radiative lifetime, the theorem on the total probability should be used, otherwise the calculated transition probability will have a deviation of three times to the actual value [16–18]. If the transition probability for q polarization is Pq, the total transition probabilities P should be P¼

1 X ðqÞ P 3 q

ð5:43Þ

and so in the general calculation, Xk should be Xk ¼

1 X ðqÞ X 3 q k

ð5:44Þ

When one uses (4.23) to calculate spontaneous transition probability in any polarization direction, the integral of the absorbing line strength is related to the integral of the absorbance over all the solid angle. Thus by (5.40) we have,

142

5 Spectroscopic Parameter and Their Calculation

1 4p

Z

2J þ 1 3hc 9n 1 SðJ ! J ÞdXp ¼ N 8p3 k ðn2 þ 2Þ2 4p 0

Z ð5:45Þ

CdX

where the choice of coordinates is arbitrary, the variables of the integral in the left-hand side can be in the polarization direction hp, up and the variables of the integral in the right-hand side can be in the light beam direction h, u. Both integrals are integrated over solid angle 4p. Kaminskii [17] discussed the relation between fluorescence branching ratio and the ratio of X ¼ X4 =X6 for Nd3+ ions. The ratios of fluorescence branching for the transitions 4F3/2 ! 4I9/2, 4I11/2, 4I13/2, and 4I15/2 can be obtained by the curves given. They can also be obtained by the following relations given by Lomheim et al. [11] b0:9 lm ¼ ð0:319X þ 0:077Þ=; b1:06 lm ¼ ð0:105X þ 0:287Þ=A; b1:3 lm ¼ 0:09=A; b1:8 lm ¼ 0:002=A; A ¼ 0:425X þ 0:457 The following relationship between the X value and the cell parameter a0 of garnet crystal can be obtained X ¼ La0 ð1 þ CDa0 Þ þ 0:128 where Da0 is the difference of lattice parameter a0 between the discussed crystal and the lutetium aluminum garnet crystal. For the neodymium-doped rare earth garnet, one has L = 8.04 10−3 nm−4, C = 10.1 nm−1. The calculated results of ﬁve neodymium-doped garnets are as follows: Crystal

Lu3Al5O12

Y3Al5O12

Lu3Ga5O12

Y3Ga5O12

Gd3Ga5O12

a0 (nm) Experimental value of X Calculated value of X

1.1915 0.29

1.201 0.30

1.2183 0.35

1.2777 0.38

1.2376 0.41

0.29

0.31

0.35

0.38

0.40

In many cases, (5.39) gives us a satisfactory analysis of experimental results. However, negative values of X2 have been found for some ions, for example Pr3+, and it is contradictory to the theory of Judd and Ofelt. Occasionally, two sets of parameters are needed; one used to analyze the transitions between low energy states, and the other used to analyze the transitions between high energy states. This problem comes from the approximate hypotheses mentioned above in the derivation of (5.39), of which the influence of the second hypotheses may be the largest. To deal with this problem, (5.39) should be modiﬁed to [12].

5.3 Judd–Ofelt Approximation and Related Parameter

X

S Ji ! Jf ¼

k¼1;2;3;4;5;6

"

143

#2 1 1 k þ ð1Þ n E ðf n Ji Þ EðuðnlÞÞ E f Jf E ðuðnlÞÞ

E 2 ½E ðf n Þ E ðuðnlÞÞ 2 D Xk ½aSLJ f U ðkÞ ½aSLJ i 4 ð5:46aÞ

where the strength parameters with k = 1, 3, 5 have been taken into account. However, this modiﬁcation is still in the theoretical scheme of Judd and Ofelt three-parameter method. By using this expression of S(Ji ! Jf), the problem of negative X2 values can be solved but the difference between experiment and calculated results is still large. In order to reduce the error, the authors of paper [12] adopted a method called normalized method. By using their method, in the least-square ﬁtting the root-mean square deviation is calculated not by PN RMSDS ¼

i¼1

cal Sexp i Si N3

2 !1=2 ð5:46bÞ

but by 0

11=2 cal 2 PN Sexp i Si exp Si B i¼1 C RMSDS ¼ @ A N3

ð5:46cÞ

Dunina [20] took into account the non-orthogonal wave function and obtained another expression of line strength S D E 2 X EJ þ EJf 2E 4f 2 S Ji ! Jf ¼ Xk ½aSLJ f U ðkÞ ½aSLJ i 1 þ i 4f 2 E4f 4d E k¼2;4;6 ð5:46dÞ where E4f 4d is the lowest 4f5d conﬁguration energy level position of Pr3+ ion and 4f 2 is the average energy level position of 4f2 conﬁguration. However, by (5.46b) E and (5.46d) we can solve the problem of negative X2 but the relative error is still large. If one uses (5.46c) and (5.46d) to evaluate J–O parameters, not only the problem of negative X2 can be solved but also the relative error can be reduced. This situation can be seen in the crystal Pr3+:GdCOB [21] and Pr3+:LaB3O6 [22]. A problem in the calculation of spectral intensity parameter must be mentioned. It is the existing parameter X0. Although the matrix element of zero-order unit tensor operator U(0) does not appear in the table published by Nielson and Koster [15], Piepho and Schatz [23] have given its expression

144

5 Spectroscopic Parameter and Their Calculation

D E ln SLU ð0Þ ln S0 L0 ¼ dLL0 dSS0 nð2L þ 1Þ1=2 ð2l þ 1Þ1=2

ð5:47Þ

It can be seen that this matrix element exists only in the case that the quantum numbers L and S of initial and ﬁnal states are equal to each other. On the other hand, it can be seen by (5.36), when k = 0, the triangle condition of 3-j symbol requires t = 1, so that only in case B1p 6¼ 0 the matrix element U(0) is non-zero. When the ions are at a position symmetry of point group G, the condition of B1p 6¼ 0 is that the irreducible representation 1− of group O3 resolves to the irreducible representations of group G that includes the identity representation C1. From the correlation table in Appendix B, it can be seen that one-order odd crystal ﬁeld component appeared only in the following ten point groups: Cs, C1, C2, C3, C4, C6, C2v, C3v, C4v, and C6v. Moreover, because of (5.47), the effect of X0 should be considered only in the case that the intermediate-coupling interaction is strong and both the initial and ﬁnal multiplets have a larger proportion of the same LS intermediate-coupling wave function. One example is Eu3+:LaF3 crystal, in which Eu3+ ions occupy C2 point group position. The transitions of 5D0 ! 7F0, 5D1 ! 7 F1, and 5D2 ! 7F2 all have the contribution of X0. Among these, the transition of 5 D0 ! 7F0 only results from the effect of X0. By the ﬁtting of spectral data, it can be found that in this sample X0 is smaller than X2 and X4 by two orders of magnitude, while smaller than X6 by one order of magnitude [24]. The three-parameter method of Judd-Ofelt can only be used in the calculation of spectroscopic parameters for multiplet-to-multiplet transitions. However, nowadays, the rare earth spectroscopic measurement, especially those performed at low temperature, can give us well-resolved spectral lines of the transitions between crystal ﬁeld levels. In order to evaluate this kind of ﬁne structure spectral lines, an all-parameter method should be used. The primary all-parameter method was introduced by Axe in 1963 [25]. It adopts Bktp Atp Ytk as parameters, where k = 2, 4, 6 and t is limited to be k ± 1, p can be 0, ±1, ±2, …, ±t (the number depends on the symmetry of the crystal ﬁeld.). Newman [26] pointed out that Axe’s method is not generally applicable, because it is assumed that the single-electron approximation and the overlapping approximation should be satisﬁed by the interactions between rare earth ions and their ligands. It does assume that all of the RE-L interactions are cylindrical and independent of each other. If these conditions are not satisﬁed, then new parameters should be added. In fact, the restriction on t will be lost, and let it can be equal to k. Reid and Richardson developed and applied the all-parameter method in a series of papers [27–31]. According to their method, electric-dipole line strength for a transition from wi to wf can be written as Si!f

X Xk ¼ Bktp l ktp lq

1 q

E2 D t ðkÞ k1 þ p þ q 1=2 ð1Þ ð2t þ 1Þ wi Ul wf p ð5:48Þ

5.3 Judd–Ofelt Approximation and Related Parameter

where

k l

1 q

t p

145

is the 3-j symbol and the unit tensor matrix element ðkÞ hwi jUl wf can be expressed as the product of 3-j symbol and reduced tensor

matrix elements wi U ðkÞ wf by using Wigner–Eckart theorem. The numbers of the parameters Bktp can reach 81 in general cases, where k = 2, 4, 6, and t is limited to be k and k ± 1, while p can be 0, ±1, ±2, …, ±t. Considering the crystal ﬁeld symmetry restrictions, these numbers can be reduced differently in different symmetry situations. If the rare earth ions occupy point group O positions, there are only two parameters while for the point group D2d it should be 10. In case of a lower symmetry, the parameters increase rapidly. For the point groups D3 and D2, there are 12 and 18 parameters, respectively. In order to evaluate the line strength with so many parameters, one should have low temperature spectral data with high-enough resolution. Burdick et al. [32] used the data of 97 well-resolved absorption spectral lines of Nd3+:YAG crystal at 10 K to calculate 18 parameters Bktp of D2 symmetry. Stefan et al. [33] used this method for the line strength evaluation of Er3+:Cs3Lu2Cl9 crystal. They measured the polarization absorption spectra at 10 and 16 K as well as the up-conversion fluorescence and excitation spectra at 4.2 K and used data of 95 spectral lines to calculate 12 parameters Bktp in C3v symmetry. The obtained parameters were used to evaluate the line strengths and to simulate the absorption and emission lines not observed previously. It should be mentioned that to calculate the transitions between crystal ﬁeld levels, there is a method introduced by the authors with parameters much less than those of the all-parameter method [34–36]. The relative line strengths and line to line transition possibilities were calculated for NdAl3(BO3)4, Nd3+:YVO4, and Nd3+:YAl3 (BO3)4 crystals as well as Er3+:LiYF4 crystal [37]. In the latter case, the excited-state absorption (ESA) spectra have also been calculated with rather good results by using data from ground state absorption measurements.

5.4

Spectroscopic Parameter Calculation of Rare Earth Ion in Crystal

Let us discuss a two energy level system in a closed cavity. Its low level has N1 population, g1 degeneracy with energy E1 and its high level has N2 population, g2 degeneracy with energy E2. According to Boltzmann distribution law, we have N 2 g2 E2 E1 ¼ exp N 1 g1 kB T

ð5:49Þ

When this system interacts with a radiation ﬁeld having frequency satisfying x ¼ ðE2 E1 Þ=h, the electrons in the high level have spontaneous and stimulated emission and those in the low level have stimulated absorption. The up and down

146

5 Spectroscopic Parameter and Their Calculation

transitions will be ﬁnally in equilibrium. From the earlier discussion, it can be seen that the probabilities of stimulated emission and absorption are proportional to the energy density of the radiation ﬁeld (it can be written as Bijd(x)), but the spontaneous emission probability is independent of the radiation ﬁeld. Hence one has the following relation dðxÞðN1 B12 N2 B21 Þ ¼ N2 A21

ð5:50Þ

By using (5.49) and (5.50), d(x) becomes dðxÞ ¼

N2 A21 A21 ¼ ðN1 B12 N2 B21 Þ B12 gg12 expð hx=kB T Þ B21

ð5:51Þ

According to Plank formula, the energy density of the radiation ﬁeld in a closed cavity is dðxÞ ¼

hx3 n3 1 2 3 p c expðhx=kB T Þ 1

ð5:52Þ

By comparing (5.51) with (5.52) and by using relation g1B12 = g2B21 similar to (5.8), one obtains a relation between the Einstein coefﬁcients B21 ¼

2 2 2 p2 c3 4p2 n þ 2 X A ¼ l2n ;1m 21 2 3 3 2 3 hx n 3h n g2 n;m

ð5:53aÞ

Obviously, the expression of B12 is B12 ¼

2 2 2 4p2 n þ 2 X l1m ;2n 2 2 3 3h n g1 n;m

ð5:53bÞ

By using (5.2), (5.30), (5.39) and the formula taking into account the average over initial states and summation over ﬁnal states as expressed by (5.7), at the same time referring to formula (5.53a, 5.53b), Einstein coefﬁcient B can be written as 2 2 4p2 e2 n þ2 B ðJi ! Jf Þ ¼ 2 2 Sed ðJi ! Jf Þ 3 3h n ð2Ji þ 1Þ ed

ð5:54aÞ

Similarly, the corresponding relation for magnetic-dipole transition can be obtained as follows Bmd ðJi ! Jf Þ ¼

4p2 e2 Smd ðJi ! Jf Þ 3h2 ð2Ji þ 1Þ

ð5:54bÞ

5.4 Spectroscopic Parameter Calculation of Rare Earth Ion in Crystal

147

It can also be shown that the spontaneous transition probabilities of electric-dipole transition can be expressed as 2 2 4 2 n n þ 2 q q 64p e AedðqÞ ðJi ! Jf Þ ¼ SedðqÞ ðJi ! Jf Þ 9 3hð2Ji þ 1Þk3 ¼ 8:047 109 ðcm=sÞ 2 E2 nq n2q þ 2 X ðqÞ D ðkÞ U ½aSLJ X ½ aSLJ f i k ð2J þ 1Þk3

ð5:55Þ

k¼2;4;6

The magnetic-dipole transition between multiplets in the same conﬁguration is allowed and different from the electric-dipole transition aroused by odd parity perturbation which is independent of the structure of the host. Its difference in different hosts resulted from the variation of free ion parameters produced by the nephelauxetic effect, or the influence of J mixing effect can be neglected [38]. Therefore, the magnetic-dipole transition probability in different hosts can be considered as the same. The oscillator strength in vacuum for magnetic-dipole transition fmd can be found in the literature [38], then Smd can be calculated by the following expression Smd ¼

3hð2Ji þ 1Þk fmd ¼ 9:2189 1012 ðcmÞð2Ji þ 1Þ kfmd 8p2 mc

ð5:56Þ

where Smd can also be expressed as Smd ¼

h 4pmc

2 E2 h½aSLJ i kL þ 2Sk½aSLJ f

ð5:57Þ

Smd in (5.57) is the result of summation over crystal ﬁeld energy levels of the multiplet and so is independent of the wave functions of crystal ﬁeld energy levels. If one discusses the transition between two crystal ﬁeld energy levels, then the line strength will be dependent on the wave functions of crystal ﬁeld energy levels and so is dependent on the point group symmetry of the ions in the host. Its transition selection rule is described in Chap. 4. The transition rate of spontaneous emission can be expressed as 8p2 e2 n2 md 64p4 e2 Amd Ji ! Jf ¼ f Ji ! Jf ¼ n3 Smd 2 mck 3hð2Ji þ 1Þ k3 ¼ 7:242 1010 ðcm=sÞ E2 X n2 h ½aSLJ C ½aSL k L þ 2S k½aSLJ C ½aSL i j f f ð2J þ 1Þ k3 ½aSL i ½aSL j

ð5:58Þ

148

5 Spectroscopic Parameter and Their Calculation

The square of matrix elements in the above equation can be calculated as follows: When Jf = Ji − 1 E2 h½aSLJ i kL þ 2Sk½aSLJ f ih i91=2 8h 2 2 2 2 < ðSi þ Li þ 1Þ Ji Ji ðLi Si Þ = ¼ d ai af d Si Sf d Li Lf : ; 4Ji when Jf = Ji= J jh½aSL J kL þ 2Sk½a0 S0 L0 J 0 ij ¼ dða; a0 ÞdðS; S0 ÞdðL; L0 Þ ð2J þ 1Þ 1=2 ½3JðJ þ 1Þ þ SðS þ 1Þ LðL þ 1Þ 4JðJ þ 1Þ E2 h½aSLJ i kL þ 2Sk½aSLJ f ¼ dðai af ÞdðSi Sf ÞdðLi Lf Þ ð2Ji þ 1Þ ½3Ji ðJi þ 1Þ þ Si ðSi þ 1Þ Li ðLi þ 1Þ 4Ji ðJi þ 1Þ

when Jf= Ji+ 1 E2 h½aSLJ i kL þ 2Sk½aSLJ f ih i9 8h < ðSi þ Li þ 1Þ2 ðJi þ 1Þ2 ðJi þ 1Þ2 ðLi Si Þ2 = ¼ dðai af ÞdðSi Sf ÞdðLi Lf Þ : ; 4ðJi þ 1Þ where C([aSL]i) and C([aSL]f) are the coefﬁcients of the intermediate-coupling wave functions for initial and ﬁnal multiplets, respectively. The total transition rates in case of both the electric-dipole and the magnetic-dipole transitions are allowed will be AðJi ! Jf Þ ¼ Aed ðJi ! Jf Þ þ Amd ðJi ! Jf Þ For uniaxial crystals 1 2 AðJi ! Jf Þ ¼ AðpÞ ðJi ! Jf Þ þ AðrÞ ðJi ! Jf Þ 3 3

5.4 Spectroscopic Parameter Calculation of Rare Earth Ion in Crystal

149

For biaxial crystals 1 1 1 AðJi ! Jf Þ ¼ AðxÞ ðJi ! Jf Þ þ AðyÞ ðJi ! Jf Þ þ AðzÞ ðJi ! Jf Þ 3 3 3 The oscillator strength of electric-dipole transition will be expressed as f edðqÞ ðJi ! Jf Þ ¼

8p2 mc ðn2 þ 2Þ 9n k 3hð2Ji þ 1Þ

X

2

D E2 ðqÞ Xk ½aSLJ f U ðkÞ ½aSLJ i

k¼2;4;6

¼ 1:205 1010 ðcm1 Þ

E2 ðn2 þ 2Þ2 X ðqÞ D Xk ½aSLJ f U ðkÞ ½aSLJ i nð2Ji þ 1Þk k¼2;4;6

ð5:59aÞ The oscillator strength of magnetic-dipole transition will be expressed as f md ðJi ! Jf Þ ¼

nh 6mcð2Ji þ 1Þk E 2 X C ½aSL i C ½aSL j h½aSLJ i kL þ 2Sk½aSLJ f ½aSL i ½aSL j

¼ nfmd ðJi ! Jf Þ

ð5:59bÞ

The total oscillator strength is f ðJ ! J 0 Þ ¼ f ed ðJ ! J 0 Þ þ f md ðJ ! J 0 Þ For uniaxial crystals 1 2 f ðJ ! J 0 Þ ¼ f ðpÞ ðJ ! J 0 Þ þ f ðrÞ ðJ ! J 0 Þ 3 3 For biaxial crystals 1 1 1 f ðJ ! J 0 Þ ¼ f ðxÞ ðJ ! J 0 Þ þ f ðyÞ ðJ ! J 0 Þ þ f ðzÞ ðJ ! J 0 Þ 3 3 3 Note that the above equations can be used to calculate absorption and emission oscillator strengths but the degeneracy degree of initial states and the average wave lengths should correspond to the absorption spectrum and emission spectrum, respectively. In uniaxial or biaxial crystals, the magnetic-dipole transition is also polarized. In the J–O parameter calculation of different polarization direction, the magnetic-dipole oscillator strength that should be subtracted is not the total oscillator strength of magnetic-dipole transition with all the polarization directions as

150

5 Spectroscopic Parameter and Their Calculation

expressed in (5.59b). Taking uniaxial crystals as an example, it is necessary to measure three different polarization spectra, the a, r, and p spectra, as mentioned in Chap. 4. If fmd is the total oscillator strength of the magnetic-dipole transition in vacuum, fmd expresses the total oscillator strength of magnetic-dipole transition between two multiplets in the crystals, then fmd = nfmd. One has the following relation 2 md 1 md þ fH==c f md ¼ fH?c 3 3 md md where fH?c and fH==c are the oscillator strengths of magnetic-dipole transition when the magnetic ﬁeld perpendicular and parallel to the c axis, respectively. From the r ðrÞ spectrum measurement, the oscillator strength fexp can be expressed as ðrÞ md fexp ¼ f edðrÞ þ fH==c ðpÞ

From the p spectrum measurement, the oscillator strength fexp can be expressed as ðpÞ md fexp ¼ f edðpÞ þ fH?c

Similarly, in addition to the p polarized oscillator strength of electric-dipole transition, it includes the oscillator strength oscillator strength of magnetic-dipole transition with magnetic ﬁeld perpendicular to the optical axis. The physical md md and fH==c cannot be obtained by calculation or direct measurequantities of fH?c ment. In order to obtain data of fed(r) and fed(p), the a spectrum should be measured, because ðaÞ md fexp ¼ f edðrÞ þ fH?c

Therefore 2 ðaÞ 1 ðrÞ þ fexp f md f edðrÞ ¼ fexp 3 3 h i 1 ðrÞ ðpÞ ðaÞ f edðpÞ ¼ fexp þ fexp fexp f md 3 2 1 1 ðaÞ 1 ðrÞ 1 ðpÞ f ed ¼ f edðrÞ þ f edðpÞ ¼ fexp þ fexp þ fexp f md 3 3 3 3 3

ð5:60aÞ ð5:60bÞ ð5:60cÞ

The oscillator strength expressed in the above equations should be used in the ðqÞ calculation of J–O parameters. The absorption oscillator strength fexpðabsÞ can be calculated by using the following expression

5.4 Spectroscopic Parameter Calculation of Rare Earth Ion in Crystal

ðqÞ

fexpðabsÞ ¼

mc2 pe2 k2abs N1

Z

jðqÞ ðkÞdk ¼

1:106 1012 ðcm1 Þ k2 N1 abs

Z

151

jðqÞ ðkÞdk

ð5:61Þ

As shown by (5.43), the effective J–O parameters for biaxial and uniaxial crystals should be written as Xk ¼

1 ðXÞ ðYÞ ðZÞ Xk þ Xk þ Xk 3

1 ðpÞ 2 ðrÞ Xk ¼ Xk þ Xk 3 3

ð5:62aÞ ð5:62bÞ

The emission cross-section can be introduced as follows: the emission cross-section r21 and the absorption cross-section r12 are related in a familiar way as that of (5.8), and so the emission cross-section r21 has the following expression edðqÞ

edðqÞ

r21 ðxk Þ ¼ r12 ðxk Þ ¼

g1 g2

E 4p2 xk e2 ðn2 þ 2Þ2 X ðqÞ D Xk ½aSLJ 1 U ðkÞ ½aSLJ 2 gðxk Þ 3hcð2J2 þ 1Þ 9nq k¼2;4;6 ð5:63aÞ

md rmd 21 ðxk Þ ¼ r12 ðxk Þ

g1 4p2 xk e2 n md S ðJ2 ! J1 Þgðxk Þ ¼ g2 3hcð2J2 þ 1Þ

ð5:63bÞ

It should be noted that (5.63a, 5.63b) can only be used in absorption and emission between two very sharp energy levels. In the solid laser materials, transitions related to absorption and emission bands usually occur between two multiplets constituted by sublevels Ei with degeneracy gi and sublevels Ej with degeneracy gj, respectively. In the calculation of both absorption and emission cross-sections the fact that the ions are distributed according to Boltzmann law in the related sublevels of multiplets should be taken into account. In other words, the absorption and emission cross-sections should be averaged over different levels with average weight of gj eej =kB T and gi eei =kB T for the high and low multiplet, respectively, and then the cross-sections can be expressed as P ji

rem ðxÞ ¼ P

gj eej =kB T rji j

P ji rabs ðxÞ ¼ P

gj eej =kB T

gi eei =kB T rij i

gi eei =kB T

ð5:64aÞ

ð5:64bÞ

152

5 Spectroscopic Parameter and Their Calculation

The energies of the high and low multiplets, calculated from the bottom of each multiplet, are denoted by ej and ei, respectively. If we change the zero point of energy level to calculate from the ground state, then the following relation should be used ej ¼ Ej EZL ;

ei ¼ Ei ;

Ej Ei ¼ hx;

ej ei ¼ hx EZL

and then X ji

gj eej =kB T rji ¼

X

gj eðej ei Þ=kB T eei rji ¼ exp½ðEZL hxÞ=kB T

ji

¼ exp½ðEZL hxÞ=kB T

X

X

gj eei =kB T rji

ji

gi e

ei =kB T

rij

ji

The relation girij = gjrji has been used in the last step of the above equation. By means of (5.64a) and (5.64b), the following expressions can be obtained. Zl exp½ðEZL hxÞ=kB T Zu

ð5:65aÞ

Zl exp½ðEZL hc=kÞ=kB T Zu

ð5:65bÞ

rem ðxÞ ¼ rabs ðxÞ rem ðkÞ ¼ rabs ðkÞ

For anisotropic crystals, the absorption and emission cross-sections in q polarization direction have the following relations ðqÞ

Zl exp½ðEZL hxÞ=kB T Zu

ð5:65cÞ

Zl exp½ðEZL hc=kÞ=kB T Zu

ð5:65dÞ

rðqÞ em ðxÞ ¼ rabs ðxÞ ðqÞ

rðqÞ em ðkÞ ¼ rabs ðkÞ

The above absorption and emission cross-sections includeP the contributions from both of the electric and magnetic transitions. Where Z ¼ t gt expðet =kB T Þ, Zu denotes the function for high multiplet with t = j and Zl denotes the function for low one with t = i. The noreciprocity introduced by electron–phonon interaction [40] has not been taken into account in the discussion. In order to use (5.65a, 5.65b, 5.65c, 5.65d) to calculate emission cross-section, it is necessary to have the data of crystal ﬁeld energy levels of the high and low multiplets, which can only be obtained from the low temperature spectra. However, the Zl/Zu in (5.65a, 5.65b, 5.65c, 5.65d) and then emission cross-section can also be calculated from the absorption spectrum and the radiative lifetime by using the formula introduced as follows. By (5.5a, 5.5b) and (5.14a, 5.14b), it can be shown that the electric and magnetic transitions have the same relation as the probability of spontaneous dipole transition with the emission cross-section. The related formulas for anisotropic crystal are as follows

5.4 Spectroscopic Parameter Calculation of Rare Earth Ion in Crystal

rðqÞ em ðxÞ ¼

p2 c2 ðqÞ A gðxÞ x2 n2 21

rðqÞ em ðmÞ ¼

153

c2 k4 ðqÞ ðqÞ ðqÞ A gðkÞ A gðmÞ r ðkÞ ¼ em 8pm2 n2 21 8pn2 c 21 ð5:66Þ

Integrated over x then Z

2 rðqÞ em ðxÞx dx ¼

p2 c2 ðqÞ A n2 21

Two sides of (5.65c) multiplied by x2 and integrated over x, by using above equation, it can be shown that ðqÞ

Zl =Zu ¼

p2 c2 expðEZL =kB T ÞA21

R ðqÞ n2 rem ðxÞx2 expð hx=kB T Þdx

therefore rðqÞ em ¼

ðqÞ

R

ðqÞ

ðqÞ

p2 c2 rabs ðxÞA21

n2 rabs ðxÞx2 expð hx=kB T Þdx

ð5:67aÞ

Change the variable from x to k, then rðqÞ em ðkÞ ¼

ðqÞ

1 expðhc=ðkkB TÞÞA21 ðqÞ r ðkÞ R 8pn2 c rðqÞ ðkÞk4 expðhc=ðkkB TÞÞdk abs abs

ð5:67bÞ

In the calculation of the emission cross-section, (5.65a, 5.65b, 5.65c, 5.65d) and (5.67a, 5.67b) are usually referred to as reciprocity method. The emission cross-section can also be calculated directly by the data of fluorescence spectra, it is called Fuchtbauer-Ladenburg equation, which will be introduced in the following. The spontaneous transition probability from a high multiplet 2 to a low multiplet 1, with wavelength k, can be expressed as ðqÞ

A21 ðkÞ ¼

X ji

hc ðqÞ fj Aji d Ej Ei k

ð5:68Þ

In the above equation, the indexes of j and i are used to denote the crystal ﬁeld energy levels of multiplets 2 and 1, respectively. fj is the Boltzmann distribution factor of the ions in high multiplet 2. Substituting (5.68) into the third equation of (5.66), one obtains

154

5 Spectroscopic Parameter and Their Calculation

rðqÞ em ðkÞ ¼

k4 X ðqÞ hc f A d E E gðkÞ j j i ji k 8pn2q c ji

ð5:69Þ

If the sensitivity of the fluorescence detective system is G and the ion number of the high multiplet is Nu, then the total detected fluorescence intensity polarized in q direction will be I

ðqÞ

ðkÞ ¼ GNu

X

ðqÞ fj Aji d

ji

hc hc Ej Ei gðkÞ k k

ð5:70Þ

The total photon number in the spectrum polarized in q direction can be expressed as Z

1 hc

ðqÞ

kI ðqÞ ðkÞdk ¼ GNu A21

spectrum 2!1 so that Z

ðqÞ

GNu ¼

kIðkÞdk=hcA21

ð5:71Þ

spectrum 2!1 By substituting (5.71) into (5.70) and comparing with (5.69), one can obtain the following expression referred to as Fuchtbauer-Ladenburg (F-L) equation ﬁnally. rðqÞ em ðkÞ ¼

ðqÞ

k5 A21 I ðqÞ ðkÞ R kI ðqÞ ðkÞdk 8pn2q c spectrum 2!1

ð5:72Þ

If the variable is chosen to be the frequency, then the corresponding expression is rðqÞ em ðmÞ ¼

ðqÞ

c2 A21 Iq ðmÞ R Iq ðmÞ

8pn2q m3

spectrum 2!1

m

dm

ð5:73Þ

5.4 Spectroscopic Parameter Calculation of Rare Earth Ion in Crystal

155

For the cubic crystals and the glasses, the emission cross-section of active ions can be calculated by the following formulas using fluorescence lifetime sf, fluorescence branching ratio b, and fluorescence quantum efﬁciency η rem ðkÞ ¼

bgk5 IðkÞ R ; 8pn2 csf kIðkÞdk

rem ðmÞ ¼

spectrum 2!1

bgc2 IðmÞ R 8pn2 sf m3 spectrum 2!1

IðmÞ m dm

These expressions are the same as those introduced by Aull [40] but without the Boltzmann distribution factor fj appearing in the denominators. It should be noted that these expressions are based on the supposition that the sensitivity of the detection is the same for the whole fluorescence spectrum of the transition between the two multiplets. It is also useful to mention the fact that in order to measure the fluorescence lifetime accurately, it is necessary to eliminate the effect of radiation trapping, especially for the three-level system or quasi-three-level system like that of Yb3+ ions, in which this effect is more signiﬁcant [41]. In these cases in order to reduce the error of fluorescence lifetime measurement, it is usual to use powder sample with the grain diameter about 100 lm immersing in a liquid having refractive index near that of the sample. In this way, the internal reflection of the fluorescent light by the powder grains can be reduced so that the effect of radiation trapping is partially eliminated. The calculation of radiative lifetime for Yb3+ ions should be mentioned. For this ion, it is impossible to use absorption spectral data to calculate J–O parameter and then calculate transition probability. In this case, radiative lifetime is usually calculated by emission cross-section obtained by means of F-L formula or reciprocity method. By integrating both sides of the second equation of (5.66) over wavelength, then for the transition from multiplet Ji to multiplet Jj, one has 8pn2 c A ðJi ! Jj Þ ¼ k4 ðqÞ

Z

ðqÞ

rJi !Jj ðkÞdk

ð5:74Þ

The transition probabilities for uniaxial and biaxial crystals should be calculated using the following formulas, respectively 1 2 AðJi ! Jf Þ ¼ AðpÞ ðJi ! Jf Þ þ AðrÞ ðJi ! Jf Þ 3 3 1 ðxÞ 1 ðyÞ 1 AðJi ! Jf Þ ¼ A ðJi ! Jf Þ þ A ðJi ! Jf Þ þ AðzÞ ðJi ! Jf Þ 3 3 3 Finally, the radiative lifetime sr and fluorescence branching ratio bij can be calculated by the following expressions, respectively

156

5 Spectroscopic Parameter and Their Calculation

sr ðJi Þ ¼ P

5.5

1 ; AðJ i ! Jj Þ Jj

AðJi ! Jj Þ bij ¼ P Jj AðJi ! Jj Þ

ð5:75Þ

Hypersensitive Transitions

Just as pointed out earlier, the 4f electrons of rare earth ions are shielded by its outside ﬁlled shell 5s25p6, so that the transition intensities between different energy levels for trivalent rare earth ion are not much affected by its host. The dipole transition intensity of a particular transition channel for a rare earth ion in different hosts does not vary more than a factor of 2–3. However, a few transition channels are very sensitive to the environment of rare earth ion; these are so-called hypersensitive transition. All known hypersensitive transitions obey the selection rules of DS = 0, |DL| 2, |DJ| 2. These selection rules are the same as those of electric-quadrupole transition, but their intensity is several order magnitude larger than that of electric-quadrupole transition; therefore, it is also called pseudo-quadrupole transition. Hypersensitive transition channels of six rare earth ions commonly used in laser materials are shown in Table 5.1. Among these, some transitions do not obey the selection rule DS = 0 seemingly, however, their intermediate-coupling wave function does include the component satisfying this selection rule. For example, the intermediate-coupling wave function of 1G4 of the Tm3+ ion includes 31.8% 3F4 wave function and 56.7% 3H4 wave function which have the spin quantum number the same as that of the energy level 3H6. Among these hypersensitive transition channels, the 3F4–3H6 transition of Tm3+ ion is the channel for 2 lm laser which has important applications; the study on the relation between its transition probability and the composition as well as the structure of the hosts has important signiﬁcance. Regarding the hypersensitive transition mechanism, different authors have different opinions. Judd [42] considered that this transition is associated with large value of U(2) matrix element. The line strength S of electric-dipole transition

Table 5.1 Hypersensitive transition channels of six rare earth ions commonly used in laser materials Ion

Transition channel

Wave number (cm−1)

Ion

Pr3+ Nd3+ Ho3+

3

F2–3H4 G5/2–4I9/2 5 G6–5I8 3 H6–5I8 6 F11/2–6H15/2

4950 17200 22150 27700 7550

Er3+

Dy3+

4

Transition channel

Wave number (cm−1)

G11/2–4I15/2 H11/2–4I15/2 3 F4–3H6 3 H4–3H6 1 G4–3H6

26400 19200 5600 12550 21050

4

2

Tm3+

5.5 Hypersensitive Transitions

157

includes the reduced matrix element of unit operator U(k) as shown in (5.39) and the expression of this matrix element can be seen in (2.52) as J 0 hf n SLJ jU ðkÞ jf n S0 L0 J 0 i ¼ ð1ÞS þ L þ J þ k ½ð2J þ 1Þð2J 0 þ 1Þ 0 L

J0 L

k hf n SLjU ðkÞ jf n S0 L0 idSS0 S

where the d function and the triangle condition of 6-j symbol for k = 2 require that DS = 0, |DL| 2, and |DJ| 2 should be satisﬁed. This is just the selection rules of hypersensitive transition. Therefore, the hypersensitive transition not only demands a large reduced matrix element of unit operator U(2) but also a large J–O parameter X2. The contributions of odd crystal ﬁeld and odd lattice vibration to the J–O parameter Xk and Xk′ are expressed as [2] Xk ¼ ð2k þ 1Þ

X 2 Btp N2 ðt; kÞð2t þ 1Þ1 ; X0

k

tp

¼ ð2k þ 1Þ

X tp

@Btp 2 2 2 N ðt; kÞð2t þ 1Þ1 jhnjQjn0 ij qðnÞ @Q

where Nðt; kÞ is a factor that depends only on the atomic parameters, Btp(t = 1, 3, 5) is the odd parity crystal parameters and n and n′ are lattice vibration quantum numbers of initial and ﬁnal states, respectively, and q(n) is lattice vibration state density. It can be shown that the expression of J–O parameter Xk includes the following 3-j symbol as a factor

1 q

k p q

t p

Then by the triangle condition of 3-j symbol it can be shown that for X2(k = 2)6¼0, 3 t 1 should be satisﬁed, that is the quantity of X2 is determined by the odd crystal ﬁeld parameters B1p and B3p. From the data of N(t, k) obtained by Krupke [1] calculated using free ion wave function, it can be seen that in order to have X2 larger than X4 and X6, a large one-order crystal ﬁeld component B1p is necessary. The study of Krupke [1] has shown that X2 is mainly produced by the odd crystal ﬁeld potential, while for the X4 and X6, the contribution of odd vibrational modes accounts for a large proportion. Therefore, it is reasonable to consider that the one-order crystal ﬁeld potential is the important micro-mechanism of hypersensitive transition. The point group of crystal having crystal ﬁeld component B1p is the same as the situation of reduced matrix element U(0); that is the following ten point groups: Cs, C1, C2, C3, C4, C6, C2v, C3v, C4v, and C6v. Thereafter many authors proposed other mechanisms, among those like inhomogeneous dielectric model, ligand-polarization model and covalence model, and so on. However, these models cannot be uniﬁed to interpret hypersensitive transition phenomena in different dielectrics. For example, according to ligand polarization model, [43] the hypersensitive transition can occur when active ions occupy D3h point group position, but

158

5 Spectroscopic Parameter and Their Calculation

Krupke [1] showed that the rare earth ion in LaF3 crystal occupy D3h point group position; its X2 value is much smaller than those of X4 and X6, while Nd3+ in Y2O3 crystal occupy C2 position—one of symmetry positions having crystal ﬁeld component B1p; its 4G5/2 ! 4I9/2 transition intensity is 12 times that in LaF3 crystal. Meanwhile for other non-hypersensitive transition channel, the transition intensity of Nd3+:Y2O3 is only two times that of Nd3+:LaF3. It suggests that the hypersensitive transition of Nd3+ ions does not occur in D3h point group position. Recently, Russian authors [44–46] studied the Nd3+, Tm3+, Ho3+, and Dy3+ ions in YAG and GGG garnet crystals in which the ions can only occupy D2 position and the Ca3(NbGa)5O12 garnet crystal in which the ions can occupy C2, C2v, and C1 positions as well as the Y2O3 and KGd (WO4)2 crystals in which the ions occupy C2 position. They measured the oscillator strength and calculated the J–O parameters of related hypersensitive transition channels. Their experimental results support the B1p crystal ﬁeld component model. The intensity of hypersensitive transition has obvious relationship with the bond length and coordination number between the rare earth ion and their ligands [47]. The shorter the bond length and the higher the coordination number, the stronger is the hypersensitive transition. For example, the intensities of hypersensitive transition for Nd3 in three oxide crystals vary according to the sequence of YAG < YAP < Y2O3.

References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21.

W.F. Krupke, Phys. Rev. 145, 325 (1966) B.R. Judd, Phys. Rev. 127, 750 (1962) L.J.F. Broer, G.J. Gortter, J. Hoogschagen, Physica 11, 231 (1945) M. Born, E. Wolf, Principle of Optics, 5th edn. (Pergamon Press, Oxford, 1975) Z.D. Luo, X.Y. Chen, T.J. Zhao, Opt. Commun. 134, 415 (1997) G.S. Ofelt, J. Chem. Phys. 37, 511 (1962) X.Y. Chen, Z.D. Luo, J. Phys. Condens. Matter 13, 1171 (2001) B.R. Judd, Operator Techniques in Atomic Spectroscopy (McGraw-Hill Inc., New York, 1963) A.R. Edmonds, Angular Momentum in Quantum Mechanics (Princeton University Press, Princeton, 1957) S.D. Xia, Y.M. Chen, Sci. Sin. (Series A) 28, 950–974 (1985) T.S. Lomheim, L.G. Deshazer, Opt. Commun. 24, 89 (1978) P. Goldner, F. Auzel, J. Appl. Phys. 79, 7972 (1996) X.Y. Chen, Z.D. Luo, Chinese J. Struct. Chem. 16, 358 (1997) L. Smentek, B.G. Wybourne, B.A. Hess Jr., J. Alloys Comp. 323–324, 645 (2001) C.W. Nielson, G.F. Koster, Spectroscopic coefﬁcients for the pn, dn and fn conﬁgurations (M. I. T. Press, Cambridge, Massachusetts, 1963) H. Dai, O.M. Stafsudd, J. Phys. Chem. Solids 52, 367 (1991) H. Dai, O.M. Stafsudd, B. Dunn, Appl. Opt. 30, 4330 (1991) A. Brinier, W. Ych, F. Pz et al., J. Appl. Phys. 98, 123528 (2005) A.A. Kaminskii, L. Li, Phys. Stat. Sol (A), 26, 593 (196) W.T. Dunina, A.A. Kaminskii, A.A. Kornienko et al., Sov. Phys. Solid State 32, 289 (1990) A. Brinier, I.V. Kityk, J. Appl. Phys. 90, 232 (2001)

References

159

22. F.B. Xiong, X.Q. Lin, Z.D. Luo et al., J. Appl. Phys. 99, 064905 (2006) 23. S.B. Piepho, P.N. Schatz, Group Theory in Spectroscopy with Applications to Magnetic Circular Dichroism (Wiley, New York, 1983) 24. M.J. Weber, in Optical Properties of Ions in Crystals, ed. by H.M. Crosswhite, H.W. Moos. (Wiley, New York, 1967) 25. J.D. Axe, J. Chem. Phys. 39, 1154 (1963) 26. D.J. Newman, G. Balasubramanian, J. Phys. C 8, 37 (1975) 27. M.F. Reid, F.S. Richardson, J. Chem. Phys. 71, 5735 (1983) 28. M.F. Reid, F.S. Richardson, J. Phys. Chem. 88, 3579 (1984) 29. M.F. Reid, J.J. Dallara, F.S. Richardson, J. Chem. Phys. 79, 5743 (1983) 30. M.F. Reid, J. Chem. Phys. 87, 6388 (1987) 31. M.F. Reid, J. All. Com. 180, 93 (1992) 32. G.W. Burdick, C.K. Jayasankar, F.S. Richardson, M.F. Reid, Phys. Rev. B 50, 16309 (1994) 33. R.L. Stefan, H.U. Gudel, M.P. Hehlen, J.R. Quagliano, Phys. Rev. B 57, 15229 (1998) 34. Y.D. Huang, Z.D. Luo, J. Phys. Condens. Matter 5, 1581 (1993) 35. Z.D. Luo, Y.D. Huang, J. Phys. Condens. Matter 6, 3737 (1994) 36. X.Y. Chen, Z.D. Luo, J. Phys. Condens. Matter 10, 5147 (1998) 37. Y.D. Huang, Ph.D. Dissertation, University of Strathclyde, U.K., 1997 38. C.L. Görller-Warlrand, A. Fluyt, Ceulemans et al., J. Chem. Phys. 95, 3099 (1991) 39. W.T. Carmall, P.R. Field, K. Rajnak, J. Chem. Phys. 49, 4412 (1968) 40. B.F. Aull, H.P. Jenssen, IEEE J Quant. Elect. QE 18, 925 (1982) 41. D.S. Sumida, T.Y. Fan, Opt. Lett. 17, 1343 (1994) 42. B.R. Judd, J. Chem. Phys. 44, 839 (1966) 43. S.F. Mason, R.D. Peacock, B. Stewart, Chem. Phys. Lett. 29, 149 (1974) 44. P.A. Ryabochkina, E.V. Bolshakova, S.N. Ushakov et al., J. Lum. 132, 240 (2012) 45. P.A. Ryabochkina, S.A. Antoshkina, E.V. Bolshakova et al., J. Lum. 132, 1900 (2012) 46. P.A. Ryabochkina, S.A. Antoshkina, S.A. Klimin et al., J. Lum. 138, 32 (2013) 47. D.E. Henrie, R.L. Fellows, G.R. Choppin, Coord. Chem. Rev. 18, 199 (1976)

Chapter 6

Phonon and Spectral Line

The lattice vibration has many effects on spectroscopic properties of active ions in solids, including inducing of electric-dipole transition and vibronic-electronic transition, broadening of spectral line, shifting of spectral line position, introducing of non-radiative transition, and transforming of excited energy between ions. Therefore, studying the interaction of electron with lattice vibration is one of the most important problems in the physics of solid-state laser material. During the discussion of this chapter, the conception of phonon by quantization of lattice vibration will be introduced; the effects of phonon emission and absorption on the spectral line shape, spectral linewidth, and spectral line shifting will be discussed. In these discussions, the concentration of active ions is very low and the interaction between different active ions can be neglected, and the interaction of electronic states of active ions with the electronic band of the crystals is neglected too. The non-radiative transition inside rare earth ions introduced by electron-phonon interaction will be discussed in Chap. 8, while the phonon-assisted energy transfer will be discussed in Chap. 9.

6.1

Quantization of Lattice Vibration—Phonon

Theoretically, the starting point for studying lattice vibration is to solve the Schrödinger equation in quantum mechanics. Before the discussion, one important approximation should be assumed. It aims at the separation of the movement of electrons and the lattice vibration. As well known, the mass of the electron is much less than that of the nucleus. Even for hydrogen atom, the mass of the electron is only one part of 1840 of that of the nucleus. From classical point of view, the movement of atoms (ions) is much slower than that of the electrons. Therefore, in the same period of time, the ions have just moved for a very short distance, while the electrons have moved around the nucleus for many circles. It is reasonable to solve the problem of the electronic movement in ﬁxed positions of the ions and then © Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8_6

161

162

6 Phonon and Spectral Line

solve the problem of the lattice vibration in some kinds of average electronic ﬁeld. This is referred to as the adiabatic approximation. By the formulas of classical and quantum mechanics, before taking into account the electron–lattice interaction, the total energy of a system of n electrons with mass me and N lattice ions with mass ma is [1] E¼

n N mX 1X 1 X X e2 1 X X e2 Za Zb 2 þ ma R_ a þ r_ 2i þ 2 i¼1 2 a¼1 2 i6¼j j ri rj 2 a6¼b b Ra Rb

ð6:1Þ

Changing the classical variables into quantum mechanics operators, the partial differential operators Δi and Δa are expressed as Di ¼

@2 @2 @2 @2 @2 @2 þ þ ; Da ¼ þ þ @xi @yi @zi @Xa @Ya @Za

ð6:2Þ

The last two terms in (6.1) are interaction potential usually denoted by V(r, R) Vðr; RÞ ¼

1 X X e2 1 X X e2 Za Zb þ 2 i6¼j j ri rj 2 a6¼b b Ra Rb

ð6:3Þ

By using operator expression of (6.2) and potential expression of (6.3), the Hamiltonian of the system will be H¼

h2 X h2 X Da Di þ V ðr; RÞ 2me i 2 a ma

and then the Schrödinger equation is expressed as

h2 X h2 X Da Wðr; RÞ Di Wðr; RÞ þ V ðr; RÞWðr; RÞ ¼ EWðr; RÞ ma 2me i 2 a

ð6:4Þ

In adiabatic approximation, the movement of electron and the lattice system can be dealt with as two independent systems (their interaction will be introduced later). The zero-order wave function can be written as Wðr; RÞ ¼ Uðr; RÞuðRÞ

ð6:5Þ

where U(r, R) is an electronic wave function depending on R (the coordinate of the lattice ions) as a parameter and u(R) is lattice wave function. Substituting (6.5) into (6.4) and neglecting the dependency of the electronic wave function on the lattice coordinates, that is, the following so-called non-adiabatic term

6.1 Quantization of Lattice Vibration—Phonon

h2 X 1 ½uðRÞDa Uðr; RÞ þ 2ra uðRÞra Uðr; RÞ 2 a ma

163

ð6:6Þ

then the equation becomes

X h2 h2 X Uðr; RÞDa uðRÞ uð RÞ Di Uðr; RÞ þ V ðr; RÞUðr; RÞuðRÞ ma 2me 2 a i ¼ EUðr; RÞuðRÞ

Let

X h2 uðRÞ Di Uðr; RÞ þ V ðr; RÞUðr; RÞuðRÞ ¼ W ðRÞUðr; RÞuðRÞ 2me i

That is

h2 X Di Uðr; RÞ þ V ðr; RÞUðr; RÞ ¼ W ðRÞUðr; RÞ 2me i

ð6:7Þ

Equation (6.7) is in fact an electronic equation. In this way, the separation between electronic coordinates and those of the lattice ions is done. The related equation for the lattice ions is

h2 X Da uðRÞ þ W ðRÞuðRÞ ¼ EuðRÞ ma 2 a

ð6:8Þ

In the following, (6.8) will be solved when the lattice ions have only a small vibration around their equilibrium positions. In this discussion, the coordinates of the lattice ions should be labeled clearly. For example, the unit cell of the lattice ion is numbered by n, and the class of the ion in the cell is numbered by a (note that the meaning of n and a are different from those in (6.1)). The lattice potential can be expanded as a Taylor series near the equilibrium position. Except for the zero-order term, which is independent of the coordinates of the displacement, the ﬁrst-order term representing the force subject by the lattice points is equal to zero in the equilibrium. If the terms higher than the second order are temporarily neglected, then the potential can be expressed as W ðRÞ ¼

1X @2W ½Rnai Rnai ð0Þ½Rn0 a0 i0 Rn0 a0 i0 ð0Þ 2 nai @Rnai @Rn0 a0 i0 Rð0Þ n0 a0 i0

¼

1 2

P

nai n0 a0 i0

fii0 ðna; n0 a0 Þui ðnaÞui0 ðn0 a0 Þ

ð6:9Þ

164

6 Phonon and Spectral Line

where the second-order derivative should adopt the value at the equilibrium position. fii′(na, n′a′) refers to the force constant and is a real number. Their symmetric properties can be seen from the deﬁnition. fii0 ðna; n0 a0 Þ ¼ fi0 i ðn0 a0 ; naÞ where i denotes the coordinate components i = 1, 2, 3. The Hamiltonian of the lattice system can be written as a sum of kinetic energy and potential energy H¼

1X 1 X ma u_ 2i ðnaÞ þ fii0 ðna; n0 a0 Þui ðnaÞui0 ðn0 a0 Þ 2 nai 2 nai n0 a0 i0

ð6:10Þ

The above formula has the same form as that of the Hamiltonian of the harmonic oscillator 12 mv2 þ 12 mx2 u2 . It means that the lattice vibration consists of a series of harmonic oscillators. In the following, the method of second quantization is used to describe the lattice vibration. In the Hamiltonian (6.10), the second term on the right-hand side is the potential of lattice system obviously. Then the motion equation of the lattice can be written as Ma € ui ðnaÞ ¼

X @W ¼ fii0 ðna; n0 a0 Þui0 ðn0 a0 Þ @ui ðnaÞ 0 0 0 naj

ð6:11Þ

The solution of this equation can be written as follows, because the lattice vibration is periodicity in time. Its displacement can be expressed as 1 ui ðnaÞ ¼ pﬃﬃﬃﬃﬃﬃ qi ðnaÞ expðixtÞ ma

ð6:12Þ

Substituting the above formula into (6.11), then x2 qi ðnaÞ ¼

X

Dii0 ðna; n0 a0 Þqi0 ðn0 a0 Þ

ð6:13Þ

n0 a0 i0

where fii0 ðna; n0 a0 Þ Dii0 ðna; n0 a0 Þ ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ma ma0 If the crystal has N unit cells and each cell has r atoms, then (6.13) is a simultaneous equation with 3rN dimensions and there are 3rN solutions of x2

6.1 Quantization of Lattice Vibration—Phonon

165

(therefore have 3rN normal vibrational modes). By using the translation symmetry of the lattice, the function of q(na) can be written as qi ðnaÞ ¼ si ðaÞ expðik Rn Þ

ð6:14Þ

where k is a reciprocal vector. Equation (6.13) then becomes ( ) X X fii0 ðn0 n; aa0 Þ x s i ð aÞ ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ exp½ik ðRn Rn Þ si0 ða0 Þ ma ma0 a0 i0 n0 n 2

ð6:15Þ

The translation symmetry has been used to write down (6.15). In this case, fii′(na, n′a′) depends only on the relative position of the cell, that is fii′(na, n′a′) = fii′(n′−n,aa′). If Dii′(k,aa′) is used to represent the quantities inside the curly bracket in (6.15), then X x2 si ðaÞ ¼ Dii0 ðk; aa0 Þsi0 ða0 Þ ð6:16Þ a0 i 0

Equation (6.16) is a 3r-dimensional simultaneous equation. It has 3r solutions for each k vector x xi ðkÞ

ði ¼ 1; 2; . . .; 3rÞ

The number of k vectors is the cell number N of the crystal and so the number of total vibration mode will be 3Nr. It can be shown that because of the translation symmetry of the crystal, these 3Nr modes are N-fold degeneracy. Every frequency xi has a corresponding si which can be normalized to become ei(k,a) and simply expressed as si ðaÞ ¼ ei ðk; aÞ

ð6:17Þ

The basic characteristics of the lattice vibration are obtained by using a model with two kinds of ions in a cell, which can be found in many textbooks in solid-state physics (e.g. [2]). For the sake of brevity, the details will not be introduced while the main results will be mentioned. When there are two kinds of ions in the cell (r = 2), the lattice system has three acoustic modes and three optical modes. The character of the acoustic mode is that two kinds of ions vibrate in the same direction, while for the optical mode, the vibration directions of two ions with opposite sign of electric charge are opposite. The later vibrational mode will produce a net electric-dipole moment and so can interact with radiation ﬁeld. In general cases, there are three acoustic modes and 3r–3 optical modes. The displacement of the lattice ions can be expressed by (6.12), (6.14), and (6.17) as a linear combination of the displacements of all the harmonic vibrational modes [3]

166

6 Phonon and Spectral Line

1 X ð jÞ unai ðtÞ ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃ Qj ðk; tÞei ðk; aÞexpðik Rn Þ Nma jk

ð6:18Þ

where the time dependency of the displacement has been put into the combination coefﬁcients Qj(k,t), which are the so-called normal coordinates. It can be seen by the free electron theory that p1ﬃﬃNﬃ expðik Rn Þ is the wave function of free electron in the lattice and satisﬁes the following orthogonal relation [1]: X

exp½iðk k0 Þ Rn ¼ Ndkk0 ;K m

ð6:19Þ

n

where Km is the period vector in k space. The basis vectors can be chosen to make the solution ei(k,a) of (6.16) to satisfy the following relation X ai

ð jÞ

ðj0Þ

ei ðk; aÞei

ðk; aÞ ¼ djj0

ð6:20Þ

Owing to the fact that the displacement unai(t) of the lattice ions must be a real number, then by (6.18), one has ð jÞ

ei

ð jÞ

ðk; aÞ ¼ ei ðk; aÞ; Qj ðk; tÞ ¼ Qj ðk; tÞ

Substituting (6.18) into (6.10) and using (6.15) and (6.19), the Hamiltonian of the system can be expressed as H¼

i 1Xh _ Qj ðk; tÞQ_ j ðk; tÞ þ x2j ðkÞQj ðk; tÞQj ðk; tÞ 2 jk

ð6:21Þ

Then the Lagrange function becomes L¼

i 1Xh _ Qj ðk; tÞQ_ j ðk; tÞ x2j ðkÞQj ðk; tÞQj ðk; tÞ 2 jk

Obviously, the normal momentum Pj(k, t) which is conjugated to normal coordinate Qj(k, t) will be Pj ðk; tÞ ¼

@L @L ¼ Q_ j ðk; tÞ; Pj ðk; tÞ ¼ ¼ Q_ j ðk; tÞ _ _ @ Qj ðk; tÞ @ Qj ðk; tÞ

then (6.21) can be written as

6.1 Quantization of Lattice Vibration—Phonon

H¼

167

i 1Xh Pj ðk; tÞPj ðk; tÞ þ x2j ðkÞQj ðk; tÞQj ðk; tÞ 2 jk

ð6:22Þ

Equation (6.22) is exactly the Hamiltonian of a set of harmonic oscillators. The normal coordinates and normal momentum satisfy the commutative relation in quantum mechanics

Qj ðk; tÞ; Pj0 ðk0 ; tÞ ¼ ihdkk0 djj0

Qj ðk; tÞ; Qj0 ðk; tÞ ¼ 0

Pj ðk; tÞ; Pj0 ðk; tÞ ¼ 0 ð6:23Þ

If one introduces the following transformation

1=2 h i h bj ðkÞ þ bjþ ðkÞ ; 2xj ðkÞ i hxj ðkÞ 1=2 1 h bj ðkÞ bjþ ðkÞ Pj ðk; tÞ ¼ 2 i

Qj ðk; tÞ ¼

that is i 1=2 h bjþ ðkÞ ¼ 2hxj ðkÞ xj ðkÞQj ðk; tÞ iPj ðk; tÞ ; i 1=2 h xj ðkÞQj ðk; tÞ þ iPj ðk; tÞ bj ðkÞ ¼ 2hxj ðkÞ then the following commutative relations can be proofed by (6.23)

i h i h bj ðkÞ; bj ðk0 Þ ¼ bjþ ðkÞ; bjþ ðkÞ ¼ 0; bj ðkÞ; bjþ ðkÞ ¼ dkk0 djj0

ð6:24Þ

For example, the last commutative relation can be demonstrated as follows h i bj ðkÞ; bjþ ðk0 Þ ¼ bj ðkÞbjþ ðk0 Þ bjþ ðk0 Þbj ðkÞ ih io 1 nh xj ðkÞQj ðk; tÞ þ iPj ðk; tÞ xj0 ðk0 ÞQj ðk0 ; tÞ iPj ðk0 ; tÞ ¼ 2 hxj ðkÞ nh ih io xj0 ðk0 ÞQj ðk0 ; tÞ iPðk0 ; tÞ xj ðkÞQj ðk; tÞ þ iPj ðk; tÞ h io 1 n ixj ðkÞ Qj ðk; tÞ; Pj ðk0 ; tÞ ixj0 ðk0 Þ Qj ðk; tÞ; Pj ðk0 ; tÞ ¼ 2 hxj ðkÞ ¼

i ixj ðkÞ i hdkk0 djj0 ixj0 ðk0 Þ i hdkk0 djj0 ¼ dkk0 djj0 2 hxj ðkÞ

Equation (6.23) has been used in the above calculation. The Hamiltonian expressed by (6.22) becomes

168

H¼

6 Phonon and Spectral Line

X jk

X 1 þ hxj ðkÞ bjþ ðkÞbj ðkÞ þ ix2j ðkÞ Qj ðk; tÞPj ðk; tÞ Qj ðk; tÞPj ðk; tÞ 2 jk

The summation is over all the k vectors. However, every k vector has a corresponding vector of −k, and so the second term in the above equation is equal to zero. Therefore H¼

X

hxj ðkÞ

bjþ ðkÞbj ðkÞ þ

jk

1 2

ð6:25Þ

By using quantum number (phonon number in this situation) representation introduced ﬁrst by Dirac [4], the ground state is denoted by |0> and the state having n phonons is denoted by |n> , then it can be shown by (6.24) and (6.25) that qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ bj ðkÞnj ðkÞ ¼ nj ðkÞnj ðkÞ 1 ; bjþ ðkÞnj ðkÞ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ¼ nj ðkÞ þ 1nj ðkÞ þ 1 ; bjþ ðkÞbj ðkÞnj ðkÞ ¼ nj ðkÞnj ðkÞ ð6:26Þ Equation (6.26) shows that the effect of operator bj(k) is to eliminate one phonon from the state and so it is called annihilation operator. The effect of b+j (k) is to create one phonon and so it is called creation operator. |nj(k) > is the eigenstate of operator b+j (k)bj(k) with eigenvalue nj(k) and b+j (k)bj(k) is a phonon number operator. The commutative relation (6.24) is satisﬁed by the creation operator and the annihilation operator. Therefore, there is no any restriction on the phonon number of any phonon mode. Hence phonon is a Boson in statistical physics. In this way, (6.25) means that besides the zero energy, the lattice system consisted of 3Nr harmonic oscillators and each has energy hxi ðkÞ. The total energy in a certain state will be Eðn1 ; n2 ; n3 ; . . .n3Nr Þ ¼

3Nr X i¼1

ni þ

1 x i h 2

ð6:27Þ

where the harmonic oscillator is labeled by the index i and the summation is over all the 3Nr harmonic oscillators. It should be pointed out that in the above discussion the terms higher than the second order in the expansion of (6.9) have been neglected. This is the so-called harmonic approximation. By this approximation, there is no interaction between different normal modes. The terms higher than second order will introduce the interaction between different normal modes and so are the mechanisms to reach thermal equilibrium. The probability to ﬁnd the system in a state with energy E is proportional to exp(−E/kBT) in thermal equilibrium (kB is Boltzmann constant). Naturally, the average phonon number of certain phonon mode with frequency xi, can be expressed as

6.1 Quantization of Lattice Vibration—Phonon

169

P P hxi =kB T Þ ni ni expðEi =kB T Þ ni ni expðni ni ¼ P ¼ P hxi =kB T Þ ni expðEi =kB T Þ ni expð where Ei ¼ ni þ 12 hxi , and the common factor expð hxi =2kB T Þ in the numerator and denominator has been reduced. The above summation is over the phonon number of a certain phonon mode. Obviously, X

expðni hxi =kB T Þ ¼

ni

1 hxi =kB T Þ ½1 expð

On the other hand X

ni expðhxi ni =kB T Þ ¼ expðhxi =kB T Þ

n

¼ expðhxi =kT Þ ¼

P

expð hxi ni =kB T Þ d ½expðhxi =kB T Þ n o

d

d

ni

1 ½1expðhxi =kB T Þ

d ½expð hxi =kB T Þ expðhxi =kB T Þ

½1 expðhxi =kB T Þ2

Therefore ni ¼

1 expðhxi =kB T Þ 1

ð6:28Þ

The above formula is often used to discuss the spectroscopic problem related to lattice vibration. For every phonon mode, one can obtain a formula for average phonon number like (6.28). Now turn to the problem of phonon state density. Similar to the photon state density, they all involve the state number in k space. The periodicity of the lattice requires that kx, ky, and kz should be integer multiples of 2p/L. An allowed k value in the volume element (2p/L)3 of k space corresponds to a phonon state. The total volume of the k space is 4pk3/3 and so the total state number is (L/2p)3 4pk3/3. For the acoustic phonon k = x/m, where m is the velocity of sound, the total state number will be Nm = Vx3/6p2m3, and so the state density can be expressed as DðxÞ ¼

dNm Vx2 ¼ 2 3 dx 2p v

ð6:29Þ

It has a similar dependent relation on the frequency and wave velocity as that for the photon state density. However, they have a big difference in the orders of magnitude, because the velocity of the light is 3 1010 cm/s but that of the sound in the solid is about 5 105 cm/s and the frequency of the light is about 100–1000 times

170

6 Phonon and Spectral Line

that of the sound. On the other hand, the energy of photon is many orders of magnitude higher than that of the phonon. Therefore, at a comparable power density level, the phonon number can be a dozen order of magnitude larger than the photon number. For example, in a ruby crystal, when the power density of laser light reaches 1 W/cm2, the photon number per cm3 is only 108 order of the magnitude. However, for a solid with high hardness (Debye temperature about 1000 K), the phonon number per cm3 can be 1023 orders of magnitude. This is the reason why the lattice vibration has a strong effect on the spectroscopic properties of the solid materials.

6.2

Phonon Emission and Absorption in the Optical Transition

It can be seen from (6.7) that the potential energy of the lattice vibration is an important potential energy term in the electron Schrödinger equation. On the other hand, the phonon density is very high. Consequently, the local electronic states are strongly affected by the lattice vibration. The lifetime of the electrons in their initial state is much longer than the time to reach thermal equilibrium by their interaction with phonons, so that the electron and phonon systems are in a thermal equilibrium before the electron transition. At the moment of the transition to the ﬁnal state, the electron distribution of the initial and the ﬁnal states has a considerable difference but the conﬁguration of the lattice has no substantial change, because compared to the lattice vibration, the process of electron transition is a very rapid process. Therefore, at the moment the electron transits to its ﬁnal state, the electron system and phonon system are not in the thermal equilibrium. In this circumstance, the electron will release or absorb phonon to reach thermal equilibrium of electron-phonon system; this is so called lattice relaxation. By the language of quantum mechanics, the vibrational wave functions with different vibrational quantum number of initial state and those of the ﬁnal state are generally not orthogonal, because the potential functions introduced to the vibrational Schrödinger equation are different for these two states. In this case, the phonon number will be changed in the transition process (phonon emission or absorption). In the following discussion, we will use a single-frequency model supposing that the phonon modes interacting with the electronic system all have the same frequency and demonstrate by the method of Huang and Rhys [5]. Referring to the transition probability expressions in Chap. 4, taking into account the summation over ﬁnal states and average over initial states, if we are not concerned about the dependence of the frequency and reflective index, then the following line shape function can be introduced

6.2 Phonon Emission and Absorption in the Optical Transition

F ðE Þ ¼ Av i

X Wf M jWi i2 d E Ef Ei

171

ð6:30Þ

f

where for electric-dipole transition, M is the electric-dipole moment. In the case studied, the electrons interact with the phonon system and act as one part of a composite system, and so their wave functions are not as simple as those in Chap. 3, but should be (6.5). The phonon wave functions u(R) are designated by phonon number n. Therefore, the wave functions of the initial and the ﬁnal states of the composite system can be simply denoted by |in′ > and |fn> , respectively. Summation over the ﬁnal states and average over the initial states of (6.30) can then be explicitly expressed as F ðEÞ ¼ Av0 n

X

2 jhfnjM jin0 ij d E Efn Ein0

ð6:31Þ

n

where the energy eigenvalue Ekm (k = i or f, m = n or n′) is the sum of electron energy and those of the phonons. In the single-frequency model Ekm ¼ Eke þ

X s

ms þ

1 x h 2

ð6:32Þ

where s is the label of different phonon modes having the same frequency x which is used to replace the phonon labels of j and k. The electric-dipole moment M is a function of electronic coordinates only, but the electronic wave functions U(r, R) is not only a function of the electronic coordinates but also parameterized dependence on the lattice coordinates. Condon approximation will to deal with this be adopted problem, which assumes that the matrix element Uf ðr; RÞ M jUi ðr; RÞi ¼ Mfi is independent of the lattice coordinates. In the harmonic approximation the interaction between different phonons can be neglected and different phonon modes are independent of each other. Therefore, the wave function for the phonon system is a product of phonon wave functions of all the phonon modes. As a result, the line shape function representing the intensity of a spectral line is 2 X Y 2 F ðEÞ ¼ Mfi Av0 ufm uin0 i d E Efn Ein n

n

ð6:33Þ

s

In order to obtain the line shape function, the important point is to calculate the overlap integral . For this purpose, the effect of the electronic movement on the coordinates of lattice vibration should be taken into account. It is necessary to introduce the interaction Hamiltonian of the electrons with phonons as well as the ﬁrst-order approximation expression of the potential function W(R). The normal coordinate Q is generally used to replace the coordinate R and a linear term of the interaction potential of the electrons with phonons is assumed. If Nm = 3Nr represents the total numbers of the phonon mode, then the interaction Hamiltonian

172

6 Phonon and Spectral Line

expanded to the linear term of normal coordinates Qs (i.e. the aforementioned Qj(k,t)) will be 1 X vs ðr ÞQs Hep ¼ pﬃﬃﬃﬃﬃﬃ Nm s

ð6:34Þ

where vs(r) is the ﬁrst derivative of the potential with respect to the phonon coordinate. The effect of this interaction is to add the following potential to the system 1 X hUi ðr; QÞjHep jUi ðr; QÞi ¼ pﬃﬃﬃﬃﬃﬃ hUi ðr; QÞjvs jUi ðr; QÞiQs Nm s Let hUi ðr; QÞjvs jUi ðr; QÞi=x2 Dis It should be noted that Dis is not the differentiate operator Di used previously and its meaning can be clearly seen in (6.38). Since the interaction potential x2Q2s /2 not being calculated, the lattice vibrational potential produced by electronic movement can be written as W i ð Q Þ ¼ W i ð 0Þ þ

1X 2 2 1 X 2 x Qs þ pﬃﬃﬃﬃﬃﬃ x Dis Qs 2 s Nm s

ð6:35Þ

Substituting it into (6.8), the wave equation of the lattice vibration can be written as (

" #) X 1 @2 1 X 2 2 2 h 2 þ x Qs þ pﬃﬃﬃﬃﬃﬃ W i ð 0Þ þ x Dis Qs uin ðQÞ ¼ Ein uin ðQÞ 2 @Qs Nm s s ð6:36Þ

After the following coordinates transformation 1 Qis ¼ Qs þ pﬃﬃﬃﬃﬃﬃ Dis Nm a typical simple harmonic oscillator equation is obtained (

) X 1 @2 2 2 h 2 þ x Qis Wi þ uin ðQÞ ¼ Ein uin ðQÞ 2 @Qis s s

where the zero-point energy is

ð6:37Þ

6.2 Phonon Emission and Absorption in the Optical Transition

W i ¼ W i ð 0Þ þ

173

1 X1 2 2 x Dis Nm s 2

and the lattice vibrational wave functions can be written as uin ðQÞ ¼

Y s

uns

1 Qs þ pﬃﬃﬃﬃﬃﬃ Dis Nm

ð6:38Þ

Equation (6.38) shows that due to the lattice relaxation, the coordinates of the lattice vibrational wave function have different shifts for different electronic energy levels, and the overlap integrals are generally not equal to zero if n 6¼ n′. For the sake of convenience, a factor of the product can be calculated at ﬁrst. Z

1 1 un0s Qs þ pﬃﬃﬃﬃﬃﬃ Dis uns Qs þ pﬃﬃﬃﬃﬃﬃ Dfs dQs Nm Nm

ð6:39Þ

In order to do this calculation; it is better to shift the origin of the coordinates by introducing 1 Qis ¼ Qs þ pﬃﬃﬃﬃﬃﬃ Dis Nm Then 1 1 1 1 1 Qs þ pﬃﬃﬃﬃﬃﬃ Dfs ¼ Qs þ pﬃﬃﬃﬃﬃﬃ Dis þ pﬃﬃﬃﬃﬃﬃ Dfs pﬃﬃﬃﬃﬃﬃ Dis ¼ Qis þ pﬃﬃﬃﬃﬃﬃ Dsfi Nm Nm Nm Nm Nm where the symbol Δsﬁ = Δfs−Δis is introduced. To simplify the mathematics expression, symbol η is used to denote p1ﬃﬃNﬃ Dsfi , at the same time, the index s is m

omitted, then (6.39) becomes Z un0 ðQi Þun ðQi þ gÞdQi

ð6:40Þ

where un ðQi þ gÞ should be expanded into a Taylor series of η, then one has Z

Z

@ un0 ðQi Þun ðQi ÞdQi þ g un0 ðQi Þ u ðQi ÞdQi @Qi n Z 1 @2 þ g2 un0 ðQi Þ 2 un ðQi ÞdQi þ 2! @Qi Z 1 @k þ gk un0 ðQi Þ k un ðQi ÞdQi þ k! @Qi

ð6:41Þ

174

6 Phonon and Spectral Line

The next step in the calculation of (6.41) is to study the detailed expression of the wave function of harmonic oscillators. By the formula of lattice dynamics [6], we have u n ðQ i Þ ¼

x 1=4 ph

xQ2 1 1 i pﬃﬃﬃﬃﬃﬃﬃﬃﬃ e2 h Hn 2n n!

rﬃﬃﬃﬃ x Qi h

ð6:42Þ

From textbook of mathematical physics [7], the Hermitian polynomial the pﬃﬃﬃ Hn n xh Qi can be obtained by the expansion of the generating function N(t, n) as follows 1 X tn Hn ðnÞ Nðt; nÞ ¼ exp 2tn t2 ¼ n! n¼0

It is obvious that from the above formula, one can obtain @N @N ¼ 2tN; ¼ 2ðt nÞN @n @t Substituting the expanded formula of N (t, n) into above equations and comparing the coefﬁcients of the same tn/n! terms, the following useful recursion formulas are obtained 1 Hn0 ðnÞ ¼ 2nHn1 ðnÞ; nHn ðnÞ ¼ Hn þ 1 ðnÞ þ nHn1 ðnÞ 2

ð6:43Þ

The expression of the ﬁrst derivative of phonon wave function is easily obtained by (6.42) and (6.43) i

x 1=2 h @ 1=2 1=2 u ð Q Þ ¼ ð n Þ u ð Q Þ ð n þ 1 Þ u ð Q Þ i i i n n1 n þ 1 i 2h @Q

ð6:44Þ

Differentiating both sides of the above equation with respect to Qi once again, it can be seen that the second derivative of the phonon wave function includes the terms of un−2(Qi) and un(Qi). Reasoning by analogy, @ k un ðQi Þ[email protected] includes the term of un−k(Qi), and its coefﬁcient is

x k=2 2h

1=2 n! ðn kÞ!

ð6:45Þ

If k is an even number, it includes also the term of un(Qi). The general expression of its coefﬁcient is rather complicated. In the case of un(Qi) = u0(Qi), it can be shown that the coefﬁcient of the term of ηk in (6.41) is

6.2 Phonon Emission and Absorption in the Optical Transition

175

k=2 1 x k=2 1 2 2h ðk=2Þ!

ð6:46Þ

Let us consider the line shape factor at very low temperature. Obviously, in the initial electronic state, the lattice should be in zero-point vibrational state, that is, n′s = 0. When electrons transit from a high energy state to a low energy state (emit the photons), the phonon number of all the modes can be increased. If the total number of phonon increased is p, xr denotes the photon frequency and x expresses the phonon frequency. The conservation of the energy requires that the variation of the electronic energy should be equal to the photon energy plus the total energy of the phonons, that is, DEfi ¼ hxr þ phx or hxr ¼ DEfi p hx. Similarly, in the process of radiation absorption, hxr ¼ DEfi þ phx. Suppose p phonons generated in the transition process belong to any different g modes which have phonon number increase of ns1, ns2, …, nsg, respectively, while the phonon numbers of other modes have no any change. The relation ns1 + ns2 + + nsg = p should be satisﬁed (the maximum g is p, corresponding to the special situation of each mode has only one phonon increase). In the case studied, the initial state is n′s = 0, then only terms in (6.41) with k equal to or larger than n are different from zero, because the derivative of wave function un(Qi) with respect to Qi only consists of the terms with ul(Qi) (l > 0), when k < n. In this case, ul(Qi) (l > 0) orthogonal to u0(Qi) leads the integral of related terms in (6.41) equal to zero. Note in the expansion of (6.41), the high-order derivative terms include also the wave functions of lower vibrational quantum number; therefore, for a certain phonon number variation, the result of (6.41) consists of a series of terms with power of η from lower to higher. Owing to the fact that Nm is a very large number and so η is a very small quantity, therefore it is only necessary to consider the term having lowest power of η, that is, the term with the power k equal to the phonon number variation. Consequently, 2 Y uns ðQi Þuns ðQi þ gs Þ s !nsg 2 ns1 2 ns2 1 xg1 1 xg2 1 xg2g ¼ ns1 ! 2h ns2 ! 2h nsg ! 2 h ( " # ) 2 2 Y 1 xg2s 1 1 xg2s þ 1 þ 2 2h 2! 2 2h s

ð6:47Þ

where the ﬁrst g factors are coming from terms in expansion expression (6.41) in which the phonon number that increased for the ﬁrst mode is ns1, second mode is ns2, and so on. Of course, the total phonon number increasing is p. The expressions of these g factors corresponding to n′s = 0 and k equal to ns1, ns2, …, nsg, respectively, are calculated by using (6.41) and (6.44). Following these factors,

176

6 Phonon and Spectral Line

there is the square of a continued product, which comes from the contributions of the modes without phonon number variation in the transition. Each factor in this continued product corresponds to the contribution from one mode. In (6.41), all the terms with even powers of η (even-order derivative @ k un ðQi Þ[email protected] ) have a contribution to this factor. Therefore, each factor is a summation of a series terms and their coefﬁcients are expressed by (6.46). The square of this continued product becomes (

# )2 2 Y 1 xg2 2 1 xg2s 1 1 xg2s s þ 1 þ ¼ exp 2 2! 2 2 2 h 2 h 2 h s s ! X xg2 s ¼ exp 2h s

Y

"

Because the total mode number Nm is very large, to exclude g modes having h over phonon number variation will not actually alter the summation of the xg2s =2 all the vibrational modes, therefore the above summation should be over all the vibrational modes s. On the other hand, the line shape factor, as shown in (6.33), should be summed over all possible ﬁnal states. To include all kinds of ﬁnal state, ns1, ns2, …, nsg must be selected to be any of the Nm modes. Hence, each of the g factors in (6.47) should be summed over all the Nm modes. The order of these factors is of no signiﬁcance, and so the result should be divided by permutation number of p!/ns1!ns2!…nsg! of the p units with the same ns1, ns2, …, nsg units among them. It is obviously 2 !ns1 Y 1 X 2 u0 ðQis Þjuns ðQis þ gs Þ ¼ xgs =2h s ns1 ! s !ns2 !nsg 1 X 2 1 X 2 xgs =2 h xgs =2 h ns2 ! nsg ! s s ! X xg2 1 s p!=ns1 !ns2 !. . .nsg ! exp 2 h s ! !p X X xg2 2 s ¼ exp xgs =2 h =p! 2h s s

Therefore, the line shape function takes the following form p 2 S FðEÞ ¼ Mfi eS p! where the Huang–Rhys factor S is deﬁned as

ð6:48Þ

6.2 Phonon Emission and Absorption in the Optical Transition

177

1 X xDsfi Nm s 2 h

ð6:49Þ

S¼

X xg2 s

s

2h

2

¼

Another method to obtain (6.48) is from the differential expression of Hermitian polynomial Hn ðnÞ ¼ ð1Þn en

2

d n n2 e dnn

A differential expression of the harmonic oscillator wave function can be obtained as iÞ ¼ un ðQ

x 1=4 ð1Þn n2 d n 2 pﬃﬃﬃﬃﬃﬃﬃﬃﬃ e 2 n en n ph 2 n! dn

pﬃﬃﬃ i . Calculating the overlap integral using the above formula, the where n xh Q (6.48) can be obtained by the way adopted by Di Bartolo [8]. It should be pointed out that this single-mode and single-frequency approximation can be generalized to multi-mode and single-frequency situation according to the method described above. From (6.49), one has Shx ¼

X1 s

2

x2 g2s ¼

X1 s

2

x2 DQ2s

ð6:50Þ

It means that Shx corresponds to the total lattice relaxation energy generated by the shift of the origin of vibrational coordinates during the electronic transition. It can be seen by the curve of the line shape function versus the S factor that the peak of the spectrum is at the point S = 1 when S factor of the system is equal to 1, and the peak of the spectrum will be at the point S = k when S factor of the system is equal to k. It shows that the electrons have the maximum transition probability when the lattice relaxation energy is equal to the phonon energy absorbed or emitted in the transition. If it is not at very low temperature, there are also phonons excited in the initial electronic states, then n′s 6¼ 0. In the electronic transition, the phonon number of some vibrational modes is increased while those of the other modes can be decreased. The line shape function in this case can be calculated by assuming that there is only one phonon increased or decreased in each of the modes having phonon number variation and those modes with several phonons variation can be dealt with as each mode has one phonon variation. Obviously, when the initial phonon number is n′s, by using (6.44) to calculate expansion (6.41), for those modes with one phonon increased, by using (6.45) and let n = n′s + 1 and k = n′s, it can be shown that each g factor xg2i =2hði ¼ 1; 2; . . .; gÞ in (6.47) should be multiplied by n′s + 1; for those modes with one phonon decreased, n = n′s and

178

6 Phonon and Spectral Line

k = n′s − 1, the corresponding factor xg2 =2h in (6.47) should be multiplied by n′s; and for those modes without phonon number variation, that is n = n′s, calculated by (6.41) and (6.44), it can be shown that each factor of xg2s =2h in the continued product of (6.47) should be multiplied by 2n′s + 1. If the total phonon number increase is p, then the number of modes with one phonon increased is p + k and those with one phonon decreased is k, while k can be any integer corresponding to different distribution of the phonon number variation. The result, obviously, should be summed over all possible k. Therefore, referring to (6.48), the line shape function before statistical average takes the form 2 S 2n0 þ 1 X S n0s þ 1 p þ k Sn0s k Mij e ð s Þ ðp þ kÞ!k! k The initial phonon number should be statistical average according to Boltzmann distribution law; that is the phonon number n′s should be multiplied by the factor Pexpðns hx=kB T Þ . As shown earlier, it corresponds to replace n′s by expðn hx=k T Þ s

B

s

n ¼ 1=½expðhx=kB T Þ 1, and so the emission line shape function at temperature T is X ½ Sð 2 n þ 1Þp þ k ðS nÞ k FðE DEfi þ phxÞ ¼ Mfi eSð2n þ 1Þ ðp þ k Þ!k! k

ð6:51Þ

The shape of this function obviously depends on temperature. Figure 6.1 is the relation of the relative strength of the spectral line versus the number of phonon emitted at T = 0 K. When the electron–phonon coupling is very weak (e.g. in the case of trivalent rare earth ions in solid), the value of S is assumed to be nearly zero. The spectral line is a single peak structure, like that shown in Fig. 6.1a. For stronger electron–phonon coupling (for example in the case of trivalent iron group ions in solid), the spectral line has a multi-peak structure, like that shown in Fig. 6.1b and it (a)

(b) 0.16

Relative strength

Relative strength

5 4 3 S=0 2 1

0.14 S=7

0.12 0.10 0.08 0.06 0.04 0.02

0

0.00 0

1

2

3

Phonon number

4

0

2

4

6

8

10

12

14

16

Phonon number

Fig. 6.1 The relation of the relative strength of the spectral line versus the number of phonon emitted at low temperature limit: a S = 0; b S = 7

Fig. 6.2 The relation between relative strength of the spectral line and the number of phonon emitted and absorbed at room temperature for the system with Huang–Rhys factor S=3

Relative strength

6.2 Phonon Emission and Absorption in the Optical Transition

179

4 S=3 3 2 1 0 -4

-2

0

2

4

6

8

Phonon number

is broadened by the electron–phonon coupling. Therefore, it is generally impossible to observe the single spectral peaks corresponding to different phonon emitted or absorbed, which can be seen at very low temperature, because the broadening effect of the spectral line is enhanced rapidly as temperature rise. This will be discussed in detail later. At a higher temperature, the phonon number in initial electronic states is not equal to zero and there are phonons emitted and absorbed in the electronic transition. The relation between the relative strength of the spectral line and the number of phonon emitted and absorbed is shown in Fig. 6.2, for the case of S = 3 and phonon energy hx ¼ 250 cm1 at room temperature T = 300 K. Negative phonon number corresponds to phonon absorption. Note that in Figs. 6.1 and 6.2, the curves are the relative line strength without taking into account the effect of line broadening. Actually, the phonon always has a frequency distribution over a certain frequency range. As that discussed by K. Huang [9], if the contribution of the single phonon transition to line shape function Þd x , then that for the two-phonon transition will is eS r1 ðx in frequency range dx be 1 S Þd x e r2 ðx 2! Þ is the following convolution integral where r2 ðx Z r2 ð xÞ ¼

r1 ð x xs1 Þr1 ðxs1 Þdxs1

These relations can be generalized to multi-phonon situations. It can be shown that the contribution of the multi-phonon transition to line shape function in fre is quency range d x 1 S Þd x e rn ðx n! Therefore, the phonon side band corresponding to high-order phonon transition has a wider bandwidth, while the line corresponding to p = 0 has a higher relative intensity than that shown in Figs. 6.1 and 6.2. Generally, the part of the spectrum

180

6 Phonon and Spectral Line

corresponding to smaller p has a higher relative intensity. However, for the system with smaller S factor, all the peaks of the phonon side band still can be seen. On the other hand, for many strong electron–phonon coupling systems, the spectral peaks of the phonon side band corresponding to p > S cannot be seen even at a very low temperature. In Condon approximation, it can be shown that the integral area of spectral band, consisting of the zero phonon line and all the phonon side bands, is independent of the temperature [10]. The intensity of zero phonon line decreases, while the area of the other part of the phonon side band increases with the rising of temperature. The relation between the zero phonon line intensity and the temperature can be at high temperature. The larger the expressed as IðTÞ ¼ I0 exp½2SkB T=hx the more Huang–Rhys factor S and the lower the average phonon energy hx, rapidly weakened is the intensity of zero phonon line. At intermediate temperature region, this relation is a complex function but the tendency is still: the intensity of the zero phonon line decreases with the increase of temperature and this decrease is more signiﬁcant for the situation of larger S factor. In the case of laser material activated by trivalent rare earth ions, the electron–phonon interaction is very weak (S factor is very small) and so the intensity variation of the zero phonon line with the temperature is not obvious. However, the transition metal ion in the laser material have a much larger S factor and so the above variation is very signiﬁcant that one often fails to see the zero phonon line at room temperature. The “barycenter” of a multi-phonon emission spectrum was discussed by K. Huang [9] using the method of Fourier transformation and its result was s Ee ¼ Wfi Shx

ð6:52Þ

For absorption spectrum, it can be shown that s Ea ¼ Wfi þ Shx can be expressed as where the average phonon energy hx s ¼ hx

1 X h xs 2 i D ð hx s Þ S s 2h sfi

ð6:53Þ

and sfi sfi ¼ pDﬃﬃﬃﬃﬃﬃ D Nm

Obviously, (6.52) shows that the separation of the “barycenter” of the emission spectrum from the difference of electronic energy levels is equal to the phonon energy multiplied by S, the same as the situations in single-frequency mode (Figs. 6.1 and 6.2). By using (6.52), the Stokes shift can be deﬁned as

6.2 Phonon Emission and Absorption in the Optical Transition

s ES ¼ 2Shx

181

ð6:54Þ

An approximation method of effective phonon model with phonon frequency xeff (belonging to single-frequency approximation) is often used in the study of spectroscopic properties of solid laser materials. By this approximation, it can be shown that the square of full width at half maximum of the spectrum is [9] 2 W 2 ¼ 8ðln 2ÞS hxeff coth hxeff =2kB T

ð6:55Þ

The above formulas are very useful for the calculation of spectroscopic parameters.

6.3

Main Mechanisms of the Thermal Spectral Line Broadening and Shifting

The spectral linewidth mentioned in the previous section is generated by the optical transition accompanied by multi-phonon emission or absorption. This section will discuss the thermal broadening and shifting of the zero phonon line. This broadening and shifting will have a direct effect on the thermal stability and tuning range of laser materials. The frequency of the spectral line is determined by the relative position of the initial state and the ﬁnal state. The thermal shifting and broadening of the spectral line are the combined results of the thermal shifting and broadening of the initial and ﬁnal energy levels involved in the electronic transition. As temperature increases, the lattice expansion, the spin orbit coupling constant, the Slater parameter, and the static crystal ﬁeld parameter also change, which are one of the reasons for thermal broadening and shifting of the spectral line. On the other hand, the interaction between electron and lattice vibration will also change the position and width of the initial and ﬁnal energy levels. Generally speaking, the broadening and shifting caused by the previous action are relatively small. The peak position of the spectral line shifts with the temperature, and the increase of its width with the temperature are mainly caused by the interaction of the electron with phonon. Defects and stresses in crystals also produce broadening and shifting of spectral lines, but this mechanism is generally independent of temperature. Therefore, the effect of lattice vibration on the thermal broadening and shifting of the spectral lines should be studied in detail. The effect of the electron–phonon interaction mechanism on the spectral linewidth can be summarized into two aspects: ﬁrst, the electron transits to other energy levels, thus shortens the lifetime of the electronic energy level, and broadens the width of the electronic energy level; second, the phonon absorption and emission in different crystal ﬁeld energy levels in the same multiplet as well as the Raman scattering in the same crystal ﬁeld energy level will extend the width of the electronic energy level in the time period shorter than its lifetime. For the Raman

182

6 Phonon and Spectral Line

scattering of phonon, the frequency of emitted phonon can be lower or higher than the frequency of absorbed phonon. The ﬁrst kind of contribution to the linewidth can be calculated by 5:3 1012 DE cm1 ¼ sðsecÞ

ð6:56Þ

where s is the lifetime of the electronic energy level. Equation (6.56) is obtained by uncertainty relation DEDt ¼ h and the energy is expressed as the unit of wave number according to 1 erg = 5.035 1015 cm−1. This linewidth is called the natural linewidth in spectroscopy. Actually, this kind of effect is not the main contribution of the linewidth for zero phonon lines. One can see it clearly from the example of the pure electronic transition line R1 of the trivalent chromium in ruby. The lifetime of the excited state in this case is 3 ms at room temperature. Calculating by (6.56), the linewidth will be 2 10−9 cm−1. However, the linewidth observed was 10 cm−1 in fact. In strong electron–phonon coupling system such as transition-metal ion system, the normal vibrational frequencies for ground and excited states can be different due to different force constants. This will result in spectral thermal line broadening. The non-harmonic lattice vibrational also brings about the thermal broadening and sift of the phonon side band. This information can refer to the literature [10]. This book mainly concerns the weak electron–phonon coupling system such as trivalent rare earth ions in solid-state laser materials. In these materials only zero phonon lines have observable intensity. From the above analysis it can be seen that in these materials the main mechanism of energy level broadening is phonon absorption and emission as well as the Raman scattering, which does not change the lifetime of the electronic energy level. It is equivalent to that the electrons of the initial and ﬁnal states are oscillating with the frequency of single-phonon emission, absorption, or Raman scattering. This oscillation corresponds to an additional energy to the electronic system. The additional energy is equal to the probability of above processes multiplied by the Planck constant h. As to the spectral line thermal shifting, besides the crystal ﬁeld weakened by lattice thermal expansion, the phonon transition effect on the energy of electronic system, and the modulation of the Coulomb interaction between electrons and the spin–orbital coupling all have their contributions. Many theoretical models have been introduced to explain thermal broadening and shifting of spectral line. However, the model proposed by McCumber and Sturge [11] is highly regarded as an enormously influential work, which is concise and clear, and its main conclusions can be applied quite generally [12]. Therefore we will use this model in the discussion of line broadening and shifting, but introduce the modiﬁcation of mass difference of the host ions. It should be pointed out that all the different models published so far include a series of signiﬁcant simpliﬁcation of the real physical reality (e.g. to use long wavelength approximation of the lattice vibration and the Debye distribution of phonon frequency), and so can only be used to describe approximately the related phenomena.

6.3 Main Mechanisms of the Thermal Spectral Line Broadening and Shifting

183

The method other than the perturbation theoretical can also be used to study these problems, but the mathematical tool of many-body theory should be used [13]. It should be pointed out that the broadening and shifting of the spectral line are caused by the transitions between the neighboring crystal ﬁeld levels with separation from 100 to 102 cm−1. Generally, the energy of optical phonon has a minimum order of magnitude of about 103 cm−1, while the energy of acoustic phonon can be from 0 cm−1 to cut-off energy. Therefore, the same as the other authors, the phonon used in the following discussion is the acoustic phonon.

6.4

The Contribution of Single-Phonon Absorption (Emission) to the Spectral Linewidth

To calculate the transition probabilities of the single-phonon absorption and emission, one should, at ﬁrst, expand the energy of the electron–phonon interaction as a series of the strain. The strain can be expressed as a linear combination of phonon annihilation operator and creation operator as will be shown in the following. In an anisotropy crystal, the strain is a tensor obviously. However, in the study of thermal vibrational effect on the spectral linewidth, the direction problem can be neglected and so the displacement of the lattice can be expressed by a scalar quantity u. It is the quantity in (6.18), which does not include the basic vector ð jÞ ei ðk; aÞ (Many authors adopted this expression; for example, Di Bartolo [14].) uðRa Þ ¼

X h 1=2 eikRa bðkÞ þ eikRa b þ ðkÞ 2Mxk k

where M = Nm is used to denote the mass of the crystal and for the acoustic mode k ¼ xk =v. Therefore, one has X hxk 1=2 @u e ¼ i ½bðkÞ b þ ðkÞ 2 @Ra Ra ¼ 0 2Mv k However, the assumption that all the ions in the host crystal have the same mass is too simple and cannot account for the actual situation of the host crystal. In fact, the laser materials are made up of more than two kinds of ions having different mass. The mass difference in the host crystal should be taken into account as pointed out by the authors [15]. Considering a crystal consisting of N molecules, each is constituted of not only na ions of mass ma but also nb ions of mass mb. The number of ions in a molecule is n = na + nb. The mass of each molecule is m = (nama + nbmb). The total number of ions in the crystal is nN and the mass of the crystal is M = N(nama+nbmb). By using the above expression of the strain, the

184

6 Phonon and Spectral Line

expression of the strain for the case of all the host ions have the same mass of ma and that for the case of all the host ions have the same mass of mb can be written as follows ea ¼ i

X hxk 1=2

2v2 X hxk 1=2 ¼i 2v2 k k

1 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ½bðkÞ b þ ðkÞ; eb nNma ! 1 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ½bðkÞ b þ ðkÞ nNmb

The average strain becomes X hxk 1=2 1 e ¼ na ea þ nb eb ¼ iD ½bðkÞ b þ ðkÞ 2 n 2Mv k where " pﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃ2 #1=2 m na mb þ nb ma D¼ n3 m a m b If there are three kinds of host ion with different masses in one crystal, the factor D can be derived by the same process as " pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ2 #1=2 m na mb mc þ nb ma mc þ nc ma mb D¼ n3 ma mb mc where n ¼ na þ nb þ nc , m ¼ na ma þ nb mb þ nc mc . Generalize the above formula, and it can be obtained that for the situation of four kinds of host ion, one has " pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ2 #1=2 m na mb mc md þ nb ma mc md þ nc ma mb md þ nd ma mb mc D¼ n2 ma mb mc md Expanding the energy of the electron–phonon interaction in terms of the local strain, then Vep ¼ V1e þ V2e2 þ

ð6:57Þ

The Hamiltonian of single-phonon transition expressed by linear term of e in (6.57) will be

6.4 The Contribution of Single-Phonon Absorption (Emission) …

Hesp ¼ iV1 D

X hxk 1=2 2Mv2

k

½ bð kÞ b þ ð kÞ

185

ð6:58Þ

According to Fermi golden rule, the transition probability of single-phonon absorption or emission will be Z 2 2p f jHesp ji q Ef ¼ Ei dEf Wsp ¼ ð6:59Þ h For the phonon absorption, the initial state is |i,nk> while the ﬁnal state is |f,nk−1 > . The matrix element for the transition from energy level i to energy level f will be X hxk 1=2 pﬃﬃﬃﬃﬃ nk h f jHesp jii ¼ iDh f jV1 jii 2Mv2 k The total transition probability of single-phonon absorption is Z X 2p h f jHesp jii2 q Ef ¼ Ei dEf Wsp ¼ h Ee [ Ee f

ð6:60Þ

ð6:61Þ

i

The problem now is to determine the ﬁnal state density q(Ef = Ei); it can be written as q Ef ¼ Ei ¼ q Ef d Ef Ei where Ef and Ei are the ﬁnal and initial state energies of the electron–phonon system. The state density of the ﬁnal state is a product of the electronic state density and the phonon state density, therefore one has

h

i q Ef ¼ Ei dEf ¼ q Efe q Efp d Efe þ Efp Eie þ Eip dEfe dEfp The system absorbs a phonon transition to the ﬁnal state f, Efe iEie , meanwhile Efp hEip , therefore d

h

i 1

Efe þ Efp Eie þ Eip ¼ d xefi xk h

q Efp dEfp ¼ qðxk Þd ðxk Þ

186

6 Phonon and Spectral Line

Because both Efe and Eie are discrete electronic levels and the transition is the emission or absorption of a phonon having particular frequency x0, the energy conservation law must be observed, so

q Efe dEfe ¼ d xefi x0 dxefi

where xefi ¼ Efe Eie =h. By using the above formula of phonon state density and the Debye approximation considering that the acoustic mode consisting of two transverse vibrational mode of phonon velocity vt and one longitudinal vibrational mode of phonon velocity vl, it can be obtained that ( qðxk Þ ¼

Vx2k 2p2

þ

1 v3l

0

2 v3t

xk xD xk ixD

ð6:62Þ

where hxD ¼ kB TD , TD is referred to as Debye temperature. Substituting these results to (6.61) and integral over xefi and xk, considering that in the thermal equilibrium, the phonon number is n ¼

1 1 ¼ ehxk =kB T 1 ehx0 =kB T 1

then the transition probability of one phonon absorption takes the form a Wsp ¼

X ðx0 Þ3 D2 1 f [i

v5l

2pqh

þ

2 1 jh f jV1 jiij2 hx =k T v5t e 0 B 1

ð6:63Þ

where q = M/V. Similarly, it can be shown that for phonon emission e Wsp ¼

X ðx0 Þ3 D2 1 f hi

2pqh

v5l

þ

2 1 2 i 1 þ f j j i j h jV 1 v5t ehx0 =kT 1

ð6:64Þ

These kinds of phonon absorption and emission are reversible and it does not change the lifetime of electronic energy levels. According to the analysis given in the last section, a broadening of the initial state i resulting from the phonon a a e e absorption and emission will be DEsp ¼ Wsp h and DEsp ¼ Wsp h, respectively. −1 In the energy unit of wave number cm , 1erg = 5.035 1015 cm−1, then h ¼ 6:62620 1027 erg sec ¼ 3:3362917 1011 cm1 sec ¼ 1c, therefore a DEsp

1

cm

¼

X 1 ðx 0 Þ3 D 2 1 f [i

c 2pqh

2 1 þ 5 jh f jV1 jiij2 hx =k T vt e 0 B 1 v5l

ð6:65Þ

6.4 The Contribution of Single-Phonon Absorption (Emission) …

187

1 X 1 ðx0 Þ3 D2 1 2 1 2 e DEsp cm þ i 1 þ f ¼ ð6:66Þ j j i j h jV 1 c 2pqh v5t ehx0 =kB T 1 v5l f \i where bﬁ is usually used in the literature to denote the product of the physical quantities in the above formulas bfi ¼

1 ðx0 Þ3 D2 1 2 þ jh f jV1 jiij2 c 2pqh v5t v5l

Neglecting the difference between the velocity of transverse and longitude acoustic waves, the above formula can be written as bfi ¼

3 ðx 0 Þ3 D 2 jh f jV1 jiij2 c 2pqhv5

ð6:67Þ

Hence X bfi DEsp cm1 ¼ f [i

1 ehx0 =kB T

1

þ

X f \i

bif

1 ehx0 =kB T

1

þ

X

bif

ð6:68Þ

f \i

where the ﬁrst term is the contribution of the phonon absorption and the following two terms are those of the phonon emission. At low temperature, two 1= ehx0 =kB T 1 factors in the summations of expression (6.68) are much smaller than 1 and so the main contribution comes from the third term. In this case, when the ﬁnal state of emission or absorption is a higher crystal ﬁeld level of the ﬁnal multiplet, there are more channels to carry out the phonon spontaneous emission, that is the third term of (6.68) has a larger value. Therefore the width of low temperature emission spectral line at longer wavelength is wider than that at shorter wavelength, while the width of low temperature absorption spectral line at longer wavelength is narrower than that at shorter wavelength. The estimation of the magnitude of the thermal linewidth produced by this mechanism as well as the comparison with those by other mechanisms will be given later.

6.5

The Contribution of Phonon Raman Scattering to the Spectral Linewidth

The perturbation theory will be used to introduce the related formulas. Readers can refer to the paper published by Skinner and Hsu to know the method of non-perturbation theory [13]. Raman scattering is a second perturbation process. It involves second-order perturbation of the ﬁrst-order term of electron–phonon

188

6 Phonon and Spectral Line

interaction Hamiltonian (see (6.58)) and ﬁrst-order perturbation of the following second-order term Hedp ¼ V2

hD2 X pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ xk xl ðbðkÞ b þ ðkÞÞðbðlÞ b þ ðlÞÞ 2Mv2 kl

ð6:69Þ

Note that the mass difference factor D has been introduced in the above expression. Similar to (6.59), the transition probability of the Raman scattering can be calculated by 2p WR ¼ 2 h

Z

jh f jHR jiij2 q xf dxf

ð6:70Þ

In the following discussion, the electronic wave functions are labeled by Greek letter. Because the Raman scattering process of an electronic level is discussed, the initial and ﬁnal states are the different phonon states of the same electronic state denoted by a. According to second-order perturbation theory, the transition matrix element appeared in (6.70) can be expressed as h f jHR jii ¼ ha; nk 1; . . .nl þ 1jHR ja; nk . . .nl i X ha; nk 1; . . .nl þ 1jHesp jc; nk 1. . .nl ihc; nk 1. . .nl jHesp ja; nk . . .nl i ¼ Ea ðEc hxk Þ c6¼a þ

X ha; nk 1; . . .nl þ 1jHesp jc; nk ; . . .nl þ 1ihc; nk ; . . .nl þ 1jHesp ja; nk . . .nl i c6¼a

Ea ðEc þ hxl Þ

þ ha; nk 1; . . .nl þ 1jHedp ja; nk . . .nl i

ð6:71Þ Substituting the ﬁrst-order term of the electron–phonon interaction Hamiltonian (6.58) and that of the second-order term (6.70) into above equation, the following can be obtained " pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ( h xk xl D2 X jhajV1 jcij2 hnk 1; nl þ 1jb þ ðlÞbðkÞjnk ; nl i h f jHR jii ¼ 2Mv2 E E h x a c k c6¼a # jhajV1 jcij2 hnk 1; nl þ 1jb þ ðlÞbðkÞjnk ; nl i þ Ea Ec þ hxl þ hajV2 jaihnk 1; nl þ 1jðbðkÞb þ ðlÞ þ b þ ðlÞbðkÞÞjnk ; nl ig ð6:72Þ The next step is to substitute the matrix elements of phonon creation and annihilation operators obtained previously. Ea ðEc hxk Þ and Ea ðEc þ hx l Þ

6.5 The Contribution of Phonon Raman Scattering to the Spectral …

189

in the denominators of the terms in the above equation can be approximately replaced by Ea−Ec because hxl hxk Ea Ec (in this way, the errors introduced by those terms with Ea−Ec> 0 will partly be cancelled by those with Ea−Ec< 0). Hence the following formula resulted pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 xk xl nk ðnl þ 1ÞD h f jHR jii Mv2 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ¼ vm x k x l nk ð nl þ 1 Þ h

X jhajV1 jcij2 c6¼a

Ea Ec

! þ hajV2 jai

ð6:73Þ

where ! hD2 X jhajV1 jcij2 vm ¼ þ hajV2 jai Mv2 c6¼a Ea Ec

ð6:74Þ

For the Raman scattering involving emit and absorb phonons with the same frequency, the ﬁnal state density can be expressed as q xf dxf ¼ qðxk Þqðxl Þdðxl xk Þdxl dxk Unlike the previous section, where only certain phonon energy can match the interval of two electronic energy levels, the initial and ﬁnal states of the Raman scattering process are the same electronic energy level, and there is no limitation on the energy of the scattering phonon. By using Debye approximation, the integral of (6.70) should be from the phonon frequency 0 to xD. By means of the formula of phonon state density (6.62), supposing the transverse acoustic mode and the longitude mode have the same velocity and using the thermal equilibrium phonon number expression, (6.70) becomes 2p 9V 2 WR ¼ 2 v2m 4 6 4p v h

ZxD 0

x6k ehxk =kB T ðehxk =kB T 1Þ

2

dxk

ð6:75Þ

After the variable transformation x ¼ hxk =kB T, it can also be expressed as 7 7 TZD =T 9V 2 T x6 ex 2 kB TD dx WR ¼ 3 2 6 vm TD h 2p h v ð e x 1Þ 2

ð6:76Þ

0

Similar to the introduction of (6.65) and (6.66) from (6.63) and (6.64), the formula of linewidth as a function of temperature can be deduced

190

6 Phonon and Spectral Line

1

T ¼ a TD

7 TZD =T

x6 ex

dx aF ðT=TD Þ

ð6:77Þ

!2 1 9D4 kB TD 7 X jhajV1 jcij2 a ¼ þ hajV2 jai c 2p3 q2 v10 h Ea Ec c6¼a

ð6:78Þ

DEðT Þ cm

0

ð e x 1Þ 2

where

where a=TD7 is an adjustable parameter depending on the density of the crystal, the phonon velocity, and the electron–phonon coupling strength. The value of this parameter is proportional to D4; therefore the mass difference of the host ions has a much obvious effect on the thermal line broadening than that in the case of phonon emission and absorption mechanisms. The value of a is generally less than 300 cm−1 for rare earth ions and is different for different ones. The value reaches the maximum for Ce3+ ion and then decreases gradually down to Gd3+ ion reaching the minimum, but it will increase again gradually up to Yb3+ ion reaching the maximum. This variation tendency reflects the U shape variation tendency of electron-phonon interaction strength. Ellens [16–18] measured the value of a for nine rare earth ions Ce3+, Pr3+, Nd3+, Eu3+, Gd3+, Tb3+, Er3+, Tm3+, and Yb3+ in LiYF4 crystal. Their experimental results are in agreement with the above variation tendency. Hellwege [19] thought that it is due to the fact that the total spin quantum number S is the same for the rare earth ions in the corresponding positions of two sides of Gd3+ ion but he did not explain how the symmetry tendency of S results in the variation tendency of electron-phonon interaction strength. According to the phenomenon of J–O parameters, X4 and X6 in Y2O3 crystal for the ions in the lanthanum series are larger in the front and the end, while smaller in the middle. Krupke [20] considered that the variation tendency of electron-phonon interaction strength is the reflection of variation tendency of J–O parameters. However, in crystals LiYF4, LaF3, and YAlO3 the variation tendency of J–O parameters is different from that of Y2O3 crystal. Ellens and his coworkers [18] suggested the following two mechanisms: the ﬁrst is the lanthanide contraction. With the increase of atomic number, the electronic radius of the 4f electron decreases, which weakens the interaction with the surrounding coordination ions; and the second is the parameter r related to the 4f electrons shielded or screened by the 5 s and 5p electrons, which decreases gradually from Ce3+ ion (r = 1.1) to Yb3+ ion (r = 0.6). For the ions on the left of the Gd3+ ion, the reduction of the electronic radius plays a major role on the variation tendency of electron-phonon interaction strength, while the ions on the right of the Gd3+ ion, the decrease of the shielding parameters plays a major role on the variation tendency. As a result, the U shape variation tendency of electron-phonon interaction strength is created. Actually, one can explain this variation tendency from another point of view. The average energy level separation between the fn conﬁguration and the 4fn−15d conﬁguration is

6.5 The Contribution of Phonon Raman Scattering to the Spectral …

191

minimum for Ce3+ ion, then increases gradually and reaches its maximum at Gd3+ ion. For the right side of Gd3+ ions, this separation decreases gradually and reaches its minimum at Yb3+ ion (it can be seen in Fig. 1.5). The variation of 4fn–4fn−15d energy level separation results in the variation of the proportion of the component of 5d wave function, which has a stronger interaction with its ligands, in the 4f wave function. The proportion of the component of 5d wave function can certainly measure the strength of electron–phonon interaction. Therefore, the U shape variation tendency of the strength of electron–phonon interaction is a reflection of the U shape variation of 4fn–4fn−15d separation. For transition metal ions, the electron– phonon interaction is much stronger and a 300 cm1 . Remember that its detailed values are different for different crystals (see the examples in Sect. 6.7). Different values of (T/TD)7 multiplied by the integral value of (6.76) are shown in Appendix G. As an example, at very low temperature when TD/T = 20 (TD= 500 K, a ¼ 300 cm1 , ΔE only has T = 25 K), F(T/TD) takes 5.72 10−7, even if −4 −1 1.8 10 cm while when TD/T = 1.7 (TD = 500 K, T = 300 K) F(T/TD) has a value of 5.8 10−2 and ΔE will reach 17 cm−1 with the same a value. The contributions of the above-mentioned mechanisms change with temperature. At very low temperature, the single-phonon emission and absorption have the major contribution and that of Raman scattering can be neglected. At higher temperature, the main contribution comes from Raman scattering, which covers the entire phonon spectrum and is independent of the energy level separation of the light transition. It should be pointed out that the thermal line broadening produced by electron– phonon interaction belongs to the so-called homogenous broadening. In a crystal with considerable defects, the line broadening of the active ions is often dominated by inhomogeneous broadening. In this kind of crystal, different ions can be in different positions with different strains, different lattice distortions, and so different crystal ﬁeld potentials. The spectrum observed is actually a superposition of the different spectra produced by the ions in different positions. Owing to the random distributions of the strains, defects, and impurity ions, the inhomogeneous broadening spectral line has Gaussian line shape with the following line shape function (

) 2 ln 2 1=2 2ðx x0 Þ pﬃﬃﬃﬃﬃﬃﬃ 2 gðxÞ ¼ ln 2 exp Dx p Dx

ð6:79Þ

However, each homogenous broadening spectral line has Lorentz line shape and its line shape function is gðxÞ ¼

2 pDx

1þ

1 xx0 Dx=2

2

ð6:80Þ

In the general case, the spectral line has a Voigt line shape, which is a convolution integral of the Lorentz lines with a Gaussian frequency distribution. When

192

6 Phonon and Spectral Line

the width of the Gaussian distribution is zero (in case of an ideal crystal without inhomogeneous), the line shape becomes Lorentz. On the other hand, when the width of Lorentz line tends to zero, the spectral line takes the shape of Gaussian. This is the line shape at very low temperature, in which the effect of lattice vibration is very weak. At high temperature, the linewidth of the Lorentz components can be much larger than that of the Gaussian in the composite Voigt line and so the integral line shape is practically Lorentz. This is the reason why the spectral lines of the active ions at room temperature in a reasonable perfect crystal that can be described by Lorentz line shape. For the crystals including defects and impurity ions, based on a theoretical model, Orth [21] obtained the result: when the density of defect and/or impurity ion is low, the line shape of the spectral line is still Lorentz; while the density of defect and/or impurity ion is high, the line shape is Gaussian.

6.6

Calculation of the Thermal Shifting of Spectral Lines

To discuss thermal shifting of the spectral lines, it is natural to think that the thermal expansion is the main mechanism, because thermal expansion will weaken the crystal ﬁeld and shorten the energy level separations. Certainly, for the so-called “soft crystal” having large thermal expansion coefﬁcient, this mechanism has the major contribution. However, it is not true for the “hard crystal” like YAG. Actually, the calculation results according to the mechanism of thermal expansion cannot account for the experimental data of thermal shifting, and even obtain a negative result in some situations. Therefore, the electron–phonon interaction can be considered as the major mechanism of the thermal shifting of spectral lines. Many authors proposed a variety of different theoretical models to deal with this problem, but as pointed out before, most of these models have not been universally accepted. So we still use the McCumber and Sturg model [11] to calculate thermal shifting of the spectral lines. In order to realize the relation between thermal shifting of the spectral line and the temperature, it is enough to calculate the diagonal matrix elements of electron-phonon interaction Hamiltonian by the general method, that is, to calculate the increase of the electronic level energy generated by the electron-phonon interaction. The electron–phonon interaction energy is expanded in terms of the normal coordinates of lattice vibration to second-order term and expressed as the sum of a single-phonon Hamiltonian He−sp and a double-phonon Hamiltonian He−dp Hep ¼ Hesp þ Hedp where He−sp and He−dp have been introduced in (6.58) and (6.69). To calculate the diagonal matrix elements in second-order perturbation approximation, the double-phonon Hamiltonian (it is already a second-order quantity) and the single-phonon Hamiltonian should be calculated to zero-order and ﬁrst-order terms, respectively, that is

6.6 Calculation of the Thermal Shifting of Spectral Lines

193

X iHesp j jHesp i dEi ¼ þ iHedp i Ei Ej j

ð6:81Þ

In the initial, intermediate, and ﬁnal states, the electron–phonon wave functions of the system are expressed as hij ¼ hajhnk j; h jj ¼ hbjhnk þ 1j and hij ¼ hbjhnk 1j where a and b are used to denote the electronic wave functions of the initial and ﬁnal states, respectively. By substituting (6.58) and (6.69) into (6.81), the following expression can be obtained hD2 dEi ¼ 2Mv2 þ

(

X b;k

X

"

hajV1 jbihbjV1 jai hajV1 jbihbjV1 jai hnk jbk bkþ jnk i þ hnk jbkþ bk jnk i xk hxk hxk Ea Eb þ Ea Eb )

#

xk jhajV2 jjaihnk jbk bkþ þ bkþ bk jnk i

k

ð6:82Þ By using matrix elements of creation and annihilation operators, it becomes hD2 dEi ¼ 2Mv2 þ

(

X

X b;k

"

nk þ 1 n þ k xk jhajV1 jbij Ea Eb þ hxk Ea Eb hxk )

#

2

ð6:83Þ

xk hajV2 jaið1 þ 2nk Þ

k

The terms independent of the temperature should be subtracted, because what we are concerned is the thermal shifting of the spectral line. In this way, the shifting of the energy level i should be " # ( ) X hD2 X 1 1 2 þ þ 2hajV2 jai dEi ¼ xk n k jhajV1 jbij 2Mv2 k Ea Eb þ hxk Ea Eb hxk b6¼a

ð6:84Þ Two cases of Ei Ej hxD and Ei Ej hxD will be analyzed separately in the following. For the case of Ei Ej hxD , (6.84) can be reduced to dEi0 ¼ a

X k

x k nk

ð6:85Þ

194

6 Phonon and Spectral Line

where " # hD2 X jhajV1 jbij2 a¼ þ hajV2 jai Mv2 b6¼a Ea Eb

ð6:86Þ

In thermal equilibrium, the averaged phonon number is 1= ehxk =kB T 1 , and the phonon density is qðxk Þ ¼ 3Vx2k =2p2 m3 . In this case, the summation in (6.85) should be replaced by the following integral after using Debye model. 3V 2p2 v3

ZxD 0

TZD =T x3k dxk 3V kB T 4 x3 dx ¼ ex 1 ðehxk =kB T 1Þ 2p2 v3 h

ð6:87Þ

0

The thermal shifting in the unit of wave number can be expressed as

1

dE cm

T ¼a TD

4 TZD =T ex

x3 dx 1

ð6:88Þ

0

where a has the following relation with a expressed in (6.86) and h ¼ 1=ð2pcÞ , then one has # " 3D2 kB TD 4 X jhajV1 jbij2 a¼ 3 5 þ hajV2 jai 4p qv c h Ea Eb b6¼a

ð6:89Þ

For the case of Ei Ej hxD , the second-order term can be neglected, (6.84) can be similarly written as ZxD 2 Ea Eb x3k hD2 X 3V 2 h i dEi ¼ jhajV1 jbij P dxk 2 2Mv2 b6¼a 2p2 v3 Ea Eb ðhxk Þ2 ðehxk =kB T 1Þ 0 ¼

TZD =T 4 hD2 X 3V 1 x3 1 2 kB T P a b E E dx j h jV j i j 1 a b 2 2 2 3 x h Mv b6¼a 2p v e 1 Tab T 2 x2 ðkT Þ

¼

X 3x3ab D2 2p2 qv5 b6¼a

0

jhajV1 jbij2

T Tab

2

TZD =T

P 0

3

x 1 dx ex 1 Tab T 2 x2

ð6:90Þ where Tab ¼ ðEa Eb Þ=kB , xab ¼ 2pðEa Eb Þ=h. P means the principal value of the integral. By using a formula similar to (6.67), the above formula can be reduced and expressed in the unit of wave number

6.6 Calculation of the Thermal Shifting of Spectral Lines

dEi cm

1

TD =T X 1 T 2 Z x3 1 P dx ¼ b 2 ab 2c x1 2p T e ab Tab T x2 b6¼a

195

ð6:91Þ

0

bab ¼

3x3ab D2 2pqhv5

jhajV1 jbij2

The above calculation does not calculate separately the thermal shifting of the higher and the lower energy levels, it just ﬁnds the magnitude of the difference to give the sign of the spectral shifting. We cannot predict whether the thermal spectral line shifting is red or blue one. The experiments show that most of the thermal spectral line shiftings are red one [22]. Therefore, the phenomena of the thermal spectral line shifting should have a more comprehensive study. An important aspect of the research on thermal shifting that should be mentioned is the thermal shifting of the “barycenter” of the spectral terms induced by lattice vibration. The mechanism of this “barycenter” shifting can be the modulation of the spin–orbital coupling by lattice vibration mentioned by Kaminskii [22]. Another mechanism of thermal shifting of the “barycenter” was proposed by the author [23]. The decrease of the Coulomb interaction between electrons caused by the exchange of phonons generates a thermal shifting of the “barycenter” of the spectral term and 2S+1L was expressed as GT

2S þ 1 L ¼

gð2S þ 1 LÞS2q xq ehxq =kB T 1

where g(2S+1L) denotes the average pair number of the electron satisfying phonon exchange condition, xq is the frequency of the phonon and Sq is a parameter measuring the electron–phonon interaction strength.

4 TDR=T 3 x The values of TTD ex 1 dx can be found in the Appendix G. For example, 0

when TD/T = 1.2 (TD = 500 K, T = 417 K), it is 1.724 10−1, and when TD/T = 0.6 (TD = 500 K, T = 833 K), it is 4.405 10−1. At the end of this section, it should be pointed out that the mass difference of host ions certainly has important effects on the spectral line thermal broadening and shifting. It can be seen from the fact that D2 appears as a factor of the parameter a and D4 appears as a factor of the parameter a. It should also be mentioned that the thermal broadening and shifting of spectral lines are inversely proportional to v10 and v5, respectively, where v is the sound velocity of the crystal, owing to the fact that sound velocity of the crystal is inversely proportional to the product of crystal density q and compressibility j [24]. If the binding energy of crystal is almost the same, the compressibility of homogeneous solid is increased with mass difference of their ions [25]. It means the larger the D factor, the larger is the compressibility j. On the other hand, the mass of anion usually is smaller than that of the cation so

196

6 Phonon and Spectral Line

that the density of the materials with the same anion is increased with the D factor. For example Y3Al6O12: D2 = 1.35, q = 4.55 g/cm3; YAlO3: D2 = 1.44, q = 5.35 g/cm3; Y3Ga6O12: D2 = 1.55, q = 5.83 g/cm3; Gd3Ga6O12: D2 = 1.86, q = 7.05/cm3; Lu3Ga6O12: D2 = 1.95, q = 7.79 g/cm3. It demonstrates that the mass difference of the host ions affects the thermal broadening and shifting of spectral lines not only directly through the D factor but also indirectly through its variation of material density and compressibility. Therefore, the larger mass difference factor D always corresponds to the wider thermal broadening and larger shifting of the spectral lines. A detailed example will be shown in Sect. 6.7.

6.7

Examples for the Calculation of Thermal Spectral Line Broadening and Shifting

In order to have a perceptual knowledge about thermal broadening and shiftings of the spectral lines, the study of phonon effects on the fluorescence lines of Nd3+ ions in crystal Gd3Sc2Ga3O12 by Chen and Di Bartolo [26] will be introduced as an example. We discuss only four spectral lines corresponding to the transitions from crystal ﬁeld energy level R1 (11,439 cm−1) and R2 (11,500 cm−1) of multiplet 4F3/2 to the lowest energy level Y1 (1983 cm−1) and the highest energy level Y6 (2432 cm−1) of multiplet 4I11/2 (Fig. 6.3). Other experimental data can be directly referred to their paper [26]. On the thermal broadening of spectral lines, the total broadening of fluorescence lines was written as a sum of the following terms [26]

Fig. 6.3 Energy levels of 4 F3/2 and 4I11/2 multiplets of Nd3+ ion

R2 4

F3/2

R1

4

I11/2

Y6 Y5 Y4 Y3 Y2 Y1

6.7 Examples for the Calculation of Thermal Spectral Line …

197

X þ DE DT þ DE R b DEi cm1 ¼ DEistrain þ DEiM þ ij i i j\i

The ﬁrst term DEstrain is the broadening introduced by the defects and other i inhomogeneous in the crystals and is independent of the temperature. The second term DEiM is the broadening induced by multi-phonon emission and is essentially independent of the temperature. The third term corresponds to the last term of (6.68), which is the contribution of the spontaneous phonon emission and is also independent of temperature. DEiDT consisting of the ﬁrst two terms in (6.68) can be neglected at very low temperature. DEiR is the broadening introduced by phonon Raman scattering. The major contribution to linewidth at low temperature comes from phonon spontaneous emission, that is, the third term of (6.68). At temperature of 78 K, the spectral line corresponding to R1 ! Y1 transition has nearly a Lorentzian line shape (it shows that the crystal is rather perfect, and the influence of defects is small) and has a linewidth of 2.49 cm−1 smaller than that of any other spectral lines, because R1 and Y1 are the lowest levels at multiplets 4F3/2 and 4I11/2, respectively, and so there is no spontaneous phonon emission contribution to the linewidth. Fitting the experimental data of thermal line broadening to theoretical calculation results by taking into account or neglecting the effect of DEiDT , respectively, Chen and Di Bartolo [26] found that the contribution of DEiDT cannot be neglected at temperature 78 K; otherwise the Debye temperature TD obtained will be different from that obtained by the ﬁtting of thermal line shifts. For the R1 ! Y1 emission line, the phonon absorption Y1 ! Y2 and phonon absorption R1 ! R2 have contributed to the thermal line broadening while for the R2 ! Y1 emission line, the phonon absorption Y1 ! Y2 and phonon absorption R1 ! R2 as well as the spontaneous phonon emission R2 ! R1 have contributed to the thermal line broadening. Noting that bR1!R2 = bR2!R1, then the spectral line thermal broadening of the transitions R1 ! Y1 and R2 ! Y1, except the linewidth contribution of the spontaneous phonon emission R2 ! R1 for R2 ! Y1 emission line, can be expressed as DE cm1 ¼ DE0 þ bR1 !R2

1 expðDER2 !R1 =kB T Þ 1 1

T þa þ bY1 !Y2 expðDEY2 !Y1 =kB T Þ 1 TD

7 TZD =T 0

x6 ex ðex 1Þ2

dx

The last term in the above equation is the contribution of Raman scattering, where a is also a ﬁtting parameter like those of bY1!Y2, bR1!R2, ΔE0, and TD. The ﬁtting results are ΔE0 = 2.1 cm−1 for R1 ! Y1 emission line and ΔE0 = 2.5 cm−1 for R2 ! Y1 emission line. The reason for this difference has been stated previously, that is because the thermal line broadening of R2 ! Y1 emission line has more

198

6 Phonon and Spectral Line

contribution bR2!R1 that comes from the phonon spontaneous emission and it shows bR1!R2 = bR2!R1 = 0.4 cm−1. Other parameters ﬁtted are: bY1!Y2 = ¼ 34 cm1 , TD = 500 K and bY1!Y2 = 0.288 cm−1, a ¼ 49 cm1 , 0.158 cm−1, a TD= 500 K for R1 ! Y1 and R2 ! Y1 transitions, respectively (Fig. 6.4). The effect of temperature on the position of the lines R1 ! Y1, R2 ! Y1, R1 ! Y6, R2 ! Y6, and R1 ! Z5 (also known as X5, the highest energy level of 4 I9/2) was also studied by Chen and Di Bartolo [26]. All the measured lines shifted to the red (longer wavelength) except for the R1 ! Z5 line which shifted to the blue (shorter wavelength) with the increase of temperature. According to (6.88), the ﬁtting parameters are: R1 ! Y1 and R2 ! Y1: a = −61 cm−1, TD = 600 K; R1 ! Y6: a = −32 cm−1, TD = 760 K; R2 ! Y6: a = −26 cm−1, TD = 660 K. The ﬁtting curve for R1 ! Y1 transition is shown in Fig. 6.5. Fig. 6.4 The ﬁtting results of thermal broadening of emission spectral lines for transition R1 ! Y1 [26]

18

18

Linewidth ΔE(cm -1)

16

16

experimental Theoretical R1-->Y1 TD=500K

14 12

14 12

10

10

8

8

6

6

4

4

2 50

100

150

200

250

300

350

400

450

500

550

600

2 650

Temperature (K)

Fig. 6.5 The ﬁtting results of thermal line shifting of emission spectral lines for transitions R1 ! Y1 [26]

20

20

experimental theoretical R1-->Y1 TD=500K

Lineshift - δ(cm-1)

15

10

15

10

5

5

0

0

-5 50

-5 100 150 200 250 300 350 400 450 500 550 600 650

Temperature (K)

6.7 Examples for the Calculation of Thermal Spectral Line …

199

The thermal spectral line broadening and shifting have nearly the same orders of magnitude for the same rare earth ion in different materials or the different rare earth ions in the same material. The following are some other data for comparison. The ¼ 45 5 cm1 , ﬁtting parameters for 1.23% Er3+: YAlO3 [27] are: a −1 TD = 350 ± 30 K for thermal broadening; a = −10 ± 1 cm , TD = 300 ± 30 K for thermal shifting. The data obtained have no substantial difference for different doping concentration. The ﬁtting parameters for 1% Nd3+: CaWO4 [28] are: ¼ 70 cm1 0:5%, TD = 200 K ± 0.5% for thermal broadening, and for a ¼ 76 12 cm1 , TD = 200 ± 20 K for thermal broadNd3+:RbMnF3 [29] are: a ening; a = −30 ± 6 cm−1, TD = 500 ± 40 K for thermal shifting. One of the reasons for obtaining different Debye temperature for thermal broadening and thermal shifting is that the contribution of single phonon absorption and emission has not been taken into account. It must be pointed out that the thermal spectral line broadenings and shiftings are different for different energy level pairs of the same rare earth ion, or the same rare earth ion and the same energy level pair but in different materials. For example, for Nd3+: LLGG crystal [30] the width of spectral line R1 ! Y3 increases by 17.3 cm−1 when temperature rises from 10 to 300 K but the width of spectral line R1 ! Z5 only increases by 8.1 cm−1 for the same temperature increment. The thermal spectral line shiftings of this crystal between different energy level pairs have much difference. The spectral line of R1 ! Z5 blue shifts by 16 cm−1 but the spectral line of R1 ! Y3 red shifts by 3 cm−1 when temperature rises from 10 to 300 K. In the case of another garnet crystal Nd3+: CAZGAR [31] spectral line of R1 ! Z6 blue shifts by 2.3 cm−1 while the longer wavelength spectral line R1 ! Y1 red shift by 3.2 cm−1 in a temperature range of 10–300 K. Originally, the thermal spectral line shifting that results from electron–phonon interaction should be red shifting, but why some of the spectral lines have blue shifting? Actually, it should be noted that the lattice expands at higher temperature then the distance between the active ions and their ligands will be lengthened, and the crystal ﬁeld will be weakened, so in the above example the crystal ﬁeld splitting of multiplet 4I9/2 becomes smaller. The position of the energy level above the “barycenter” of the multiplet such as Z5 will be lower because the “barycenter” of the multiplet is not affected by the crystal ﬁeld interaction. Although the crystal ﬁeld thermal effect is generally relatively small, but for the highest crystal energy levels in the multiplets like Z5 and Y6, the quantity of energy level position change is considerable. The aforementioned spectral line R1 ! Z5 of Nd3+: GSGG crystal has a thermal blue shifting while all the spectral lines of Nd3+: YAG crystal reported by Kushida [32] have thermal red shifting except the spectral lines of R ! Z5 and R ! Y6 have thermal blue shifting. These are the embodiment of the above mechanism. Kushida [32] attempted to explain these phenomena by a pushing effect between multiplets 4I13/2 and 4I11/2 as well as that between multiplets 4 I11/2 and 4I9/2, but he neither proposed its physical mechanism nor explained if the higher multiplet has pushing effect to lower multiplet and whether the lower multiplet has the same pushing effect to the higher multiplet and how this effect

200

6 Phonon and Spectral Line

change the position of the “barycenter” of the multiplet. Therefore the pushing effect is difﬁcult to explain the phenomena of thermal blue shifting of the spectral line. The following examples illustrate the effect of mass difference of host ions on the spectral line thermal broadening of active ions. Take the thermal spectral line broadening of Nd3+ ion in garnet crystals LLGG and CAZGAR as examples [30, 31]. By using their R1 ! Z5 spectral line thermal broadening data TD and a and the expression of D factor given in Sect. 6.4, the following parameters are calculated: for LLGG crystal D=1.44, a=TD7 ¼ 2:5 1017 cm1 =K7 and for CAZGAR crystal D=1.22, a=TD7 ¼ 1:65 1018 cm1 =K7 . When temperature rises from 10 K to 300 K, the spectral line R1 ! X5 thermal broadenings of Nd3+: LLGG crystal and Nd3+: CAZGAR crystal are 8.1 and 4.5 cm−1, respectively. The situation is similar for the transition metal ions. By using TD and a data of R line in Cr3+: YAG and Cr3+: YGG [33], the calculated result for YAG crystal is D = 1.17, a=TD7 ¼ 1:53 1017 cm1 =K7 ; for YGG crystal it is D = 1.23, a=TD7 ¼ 8:77 1017 cm1 =K7 . When the temperature rises from 7 K to 240 K, the R line broadenings of Cr3+: YAG crystal and Cr3+: YGG crystal are 5.4 and 25 cm−1, respectively. Just as pointed out in Sect. 6.4, the spontaneous phonon emission constitutes the main contribution to the spectral line broadening at very low temperature. Therefore, the transition to higher energy states of ﬁnal multiplet will have larger spectral linewidth. This is a common phenomenon, not only demonstrated on the R1 ! Y1 and R2 ! Y1 spectral lines but also can be clearly seen in the following low temperature emission and absorption spectra: Fig. 6.6a is the emission spectrum of Pr3+: YAB excited to multiplet 1D2 measured at 10 K [34]. It can be seen that the spectral linewidth increases with wavelength. The emission lines with longer wavelength are those jumping to higher crystal ﬁeld energy levels of ground multiplet which have more spontaneous phonon emission channels. Figure 6.6b is absorption spectrum of NAB crystal that corresponds to the transition to multiplet

Fig. 6.6 a YAB: Pr3+ 1D2 ! 3H4 emission spectrum at 10 K; (a), (c), (d), (f) are transition to crystal energy levels in 0, 231, 332, 560 cm−13 of H4 [34]; b 4I9/2 ! 4F3/2 absorption spectrum of NAB at 10 K [35]

6.7 Examples for the Calculation of Thermal Spectral Line …

201

4

F3/2 measured at 10 K [35]. The absorption spectral line peak at shorter wavelength corresponds to the transition to a higher crystal ﬁeld energy level R2 of multiplet 4F3/2 which has the probability to emit phonon so that it has wider spectral linewidth compared to that of the absorption spectral line peak at longer wavelength which is the transition to the lowest crystal ﬁeld energy level R1 of multiplet 4F3/2 and the level is impossible to emit phonon. The spectral line thermal broadening of laser materials not only has practical meaning for usually laser application but also is an important subject of the study of coherent optical signal processing, storage and quantum information technology, because in these cases the spectral line thermal broadening appears as optical dephasing and decorrelation in time domain.

References 1. A.S. Davydov, Quantum Mechanics, 2nd edn. (Pergamon Press, Oxford, 1976) 2. C. Kittel, Introduction to Solid State Physics, 6th edn. (Wiley, New York, 1976) 3. W. Ludwig, in Phonons and Phonon Interactions, T.A. Bak (ed.), (W.A. Benjamin, INC, New York, Amsterdam, 1964) 4. P.A.M. Dirac, The Principles of Quantum Mechanics (Oxford, 1958) 5. K. Huang, A. Rhys, Proc. Roy. Soc. A 204, 406 (1950) 6. M. Born, K. Huang, Dynamics Theory of Crystal Lattice (Oxford, 1954) 7. W. Magnus, F. Oberhettinger, P.R. Soni, Formulas and Theorems for the Special Functions of Mathematical Physics (Springer, New York, 1966) 8. B. Di Bartolo, in Spectroscopy of Solid-State Laser-Type Materials, B. Di Bartolo (ed.), (Plenum Press, New York, 1987) 9. K. Huang, Progress in Physics 1, 31 (1981). (In Chinese) 10. K. Rebane, Impurity Spectra of Solid (Plenum Press, New York, 1970) 11. D.E. McCumber, M.D. Sturge, J. Appl. Phys. 34, 1682 (1963) 12. R.M. Macfarlane, J. Lum. 85, 181 (2000) 13. D. Hsu, J.L. Skinner, J. Chem. Phys. 81, 1604–5471 (1984); 83, 2097–2107 (1985) 14. B. Di Bartolo, Optical Interactions in Solids (Wiley, New York, 1968) 15. Z.D. Luo, Y.D. Huang, X.Y. Chen, J. Physics, Condens. Matter. 13, L447 (2001) 16. A. Ellens, H. Andres, M.L.H ter Heerdt et al., J. Lum., 66 and 67, 240 (1996) 17. A. Ellens, H. Andres, A. Meijerink et al., Phys. Rev B 55, 173 (1997) 18. A. Ellens, H. Andres, M.L.H ter Heerdt et al., Phys. Rev B 55, 180 (1997) 19. K.H. Hellwege, Ann. Phys. 40, 529 (1941) 20. W.F. Krupke, Phys. Rev. 145, 325 (1966) 21. D.L. Orth, R.J. Mshl, J.L. Skinner, J. Phys.: Condens. Matter 5, 2533 (1993) 22. A.A. Kaminskii, Laser Crystal Physics (Springer, New York, 1980) 23. Z.D. Luo, Sci. Bull. 17, 786 (1979). (in Chinese) 24. J, Callaway, Quantum Theory of the Solid State, 2nd edn (Academic Press, Inc., 1991) 25. H.G.F. Winkler, Struktur und Eigenschaften der Kristalle (Springer, Berlin, 1955) 26. X. Chen, B. Di Bartolo. J. Lumin. 54, 309 (1993) 27. C. Peistner, P. Albers, W. Luthy et al., Phys. Lett. A 137, 457 (1989) 28. R. Moncorge, D. Pacheco, B. Di Bartolo, Phys. Stat. Sol. (a) 43, K45 (1977) 29. J. Dunko, D. Pachcco, B. Di Bartolo, Phys. Stat. Sol. (a) 63, K31 (1981) 30. D.K. Sardar, R.M. Yow, F.S. Salinas, Opt. Mater. 18, 301 (2001) 31. D.K. Sardar, R.M. Yow, Opt. Mater. 10, 191 (1998)

202 32. 33. 34. 35.

6 Phonon and Spectral Line A. Kushida, Phys. Rev. 185, 500 (1969) A.P. Vink, A. Meijerink, J. Lumin. 87–89, 601 (2000) M.H. Bartl, K. Gatterer, E. Cavalli, et al., Spectrochimica Acta Part A 57, 1981 (2001) D. Jaque, O. Enguita, G.U. Caldino et al., J. Appl. Phys. 90, 561 (2001)

Chapter 7

Energy Levels and Spectroscopic Properties of Transition Metal Ions

The ruby crystal used by Maiman in 1960 to observe laser emission ﬁrst in the world is aluminum oxide crystal doped with trivalent chromium (Cr3+:Al2O3). Tunable laser crystals and laser materials for Q switch and mode-locked devices have been widely used in the ﬁeld of laser technology after 1970. Most of them are doped with transition metal group ions (only the ions of the ﬁrst transition group, i.e. the ions of iron group are discussed here), including titanium sapphire (Ti3+: Al2O3), trivalent chromium-doped lithium strontium aluminum fluoride (Cr3+: LiSrAlF6), and tetravalent chromium-doped magnesium olivine (Cr4+:Mg2SiO4) and yttrium aluminum garnet (Cr4+:Y3Al5O12). On the other hand, the crystals doped with bivalent iron group ions like V2+, Co2+, Ni2+, and Fe2+ also have laser emission. More than 10 years ago, tunable laser wavelength had been extended to 4.7 lm [1] (shown in Fig. 7.1). The basic theoretical knowledge of the energy level and spectroscopy characteristics for transition metal ions in crystals will be introduced in this chapter. The method of group chain scheme will be used to calculate matrix elements of crystal ﬁeld energy level splitting and transition probability. On the other hand, some related laser properties will be briefly mentioned. There are many excellent monographs [2–5] dealing with crystal ﬁeld theory of transition metal ions and a very extensive volume of literature on the iron group ions doped laser crystals, which will not be introduced in detail, so the readers can directly refer to. The character of the electronic structure of these ions is that they have an unﬁlled 3d shell, that is, their electronic conﬁgurations are 3dq, where the electron number q can vary from 1 to 9. The 3dq shells of these ions are not shielded by outer ﬁlled shells like those of rare earth ions; in this situation the crystal ﬁeld and lattice vibration have a strong effect on their electronic states and the transitions between these states. The crystal ﬁeld energy is comparable to the energy of Coulomb interaction between electrons but larger than that of the spin–orbit interaction. Therefore, in order to perform the theoretical calculation of energy levels, the crystal ﬁeld perturbation of d electron must be considered at ﬁrst, from high symmetry ﬁeld to lower symmetry ﬁeld step by step, then the spin–orbit coupling is © Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8_7

203

7 Energy Levels and Spectroscopic Properties of Transition …

204 Fig. 7.1 Overview of tunable solid-state lasers [1]

subsequently included. The discussion of Chap. 6 shows that, in this situation, there are larger shift between the zero points of conﬁguration coordinate curve of the excited state and that of the ground state; hence the emission and absorption spectra show the pattern of multi-phonon side band. Solid-state laser properties of transition metal ions will be discussed as examples. However, the knowledge of energy level structure and transition characteristics of the transition metal ions studied in this chapter can also be used to luminescent materials. It should be said that in order to accord with energy level symbols usually used in spectroscopy of transition metal ions, the Milliken’s symbols of group representation are adopted in this chapter except those used in 3jm factors.

7.1

Energy Levels and Spectral Properties of 3d1 Electron System

Supposing Ti3+ ions in crystal are at the center of a regular octahedron consisting of six anions with charge –Ze, let’s consider the crystal ﬁeld effect on the d electron. Obviously, the interaction potential of these anions with d electron can be, in point charge model, expressed as Vc ðrÞ ¼

6 X

Ze2 jRi rj

ð7:1Þ

i¼1

where r = (r, h, u) and Ri = (R, Hi, Ui) are the position vectors of the electron and the ligand i, respectively. The Schrödinger equation of the electron can be written as

7.1 Energy Levels and Spectral Properties of 3d1 Electron System

2 h =2m D þ U ðr Þ þ Vc ðrÞ uðrÞ ¼ EuðrÞ

205

ð7:2Þ

where U(r) is the interaction potential of the electron with central ﬁeld of the free ions which is independent of the angular variables, thus can be expressed as a function of scalar coordinate r. The perturbation method, to treat Vc(r) as a perturbation, should be used to solve (7.2). Crystal ﬁeld potential Vc(r) is generally expanded in terms of spherical harmonic functions in crystal ﬁeld theory. It takes the form of Vc ðrÞ ¼

1 X k X

r k Bkq CqðkÞ ðh; uÞ

ð7:3Þ

k¼0 m¼k

where CqðkÞ ðh; uÞ ¼ Bkq ¼

4p 2k þ 1

4p 2k þ 1

1=2

1=2 Ykq ðh; uÞ

6 Ze2 X Y ðH i ; U i Þ Rk þ 1 i¼1 km

ð7:4Þ

ð7:5Þ

Equation (7.3) is a general expression, when it is applied to speciﬁc case studied, then some restrictions should be added. First, according to Wigner–Eckart theorem and the triangle condition of the 3j symbol introduced in Chap. 2, it can be seen that in case of d electron where l = l′ = 2, the related matrix element hunlm jVc jun0 l0 m0 i is zero unless k 4. For the problem of crystal ﬁeld energy splitting, the wave functions involved belong to the same conﬁguration (i.e. the same parity) and so the crystal ﬁeld potential should have even parity, that is only the even k value in k 4 should be considered. Secondly, in the ﬁrst-order approximation, the active ion can be seen as in the center of regular octahedron composed by six negative ions with charge −Ze. As pointed out in Chap. 2, Vc is invariant under the operations of cubic group operations. Owing to the existence of the fourth-order symmetry axis, in the range of k 4, k can only be equal to 0 or 4 and q must also be 0, 4, and −4. If the term with k = 0 is omitted, which has only a parallel shift of all the levels, then the crystal ﬁeld potential will be ( ) 1=2 h i 7Ze2 4 5 ð4Þ ð4Þ ð4Þ Vc ¼ r C0 ðh; uÞ þ C4 ðh; uÞ þ C4 ðh; uÞ 14 2R5

ð7:6Þ

By using the language of group chain scheme introduced in Chap. 3, it means that when the irreducible representation of rotation group SO3 is reduced to the irreducible representation of cubic group, there is only the term of k = 4 that can have a component belonging to the identity representation. If the wave function of the

7 Energy Levels and Spectroscopic Properties of Transition …

206

3d electron expressed as u32m= R32(r)Y2m(h,u), then the matrix elements can be calculated as

u32; þ 2 jVc ju32; þ 2 ¼ u32;2 jVc ju32;2 ¼ Dq

u32; þ 1 jVc ju32; þ 1 ¼ u32;1 jVc ju32;1 ¼ 4Dq

u32;0 jVc ju32;0 ¼ 6Dq

u32; þ 2 jVc ju32;2 ¼ u32;2 jVc ju32; þ 2 ¼ 5Dq 4

Ze2 , < r4 > 3d is the fourth power of the electronic coordinates where Dq ¼ 6R 5 r 3d r averaged over 3d orbital. The calculation of the matrix elements can use (2.43a) of the Wigner–Eckart theorem and 3-j symbol introduced in Chap. 2. For example

7Ze2 4

2 4 2 22 4 u32; þ 2 jVc ju32; þ 2 ¼ r ð 1 Þ 2 C 2i h 3d 2R5 2 0 2 pﬃﬃﬃ 1=2 2

7Ze 4 5 2 1 Ze2 4

p ﬃﬃﬃﬃﬃ ¼ r ¼ r 3d Dq 3d 18 35 2R5 6R5 35 ð7:7Þ where 3-j symbol can be found from Rotenberg [6]; at the same time note that the 3j symbols vanish unless m1 + m2 + m3 = 0 and so for the calculation of above three matrix elements only the ﬁrst term of (7.6) should be considered. On the other hand, (2.53) is used to calculate h2C ð4Þ 2i. Therefore the following secular equation is obtained

E 0 þ Dq E

0

0

0

5Dq ¼0

0 E 0 4Dq E 0 0 0

0 0 E0 þ 6Dq E 0 0

0 0 0 E 0 4Dq E 0

5Dq

0

0

0

0 E þ Dq E

By exchanging the ﬁfth row with the second row and then exchanging the ﬁfth line with the second line, the secular equation changes to

E 0 þ Dq E

5Dq

0

0

0 ¼0

5Dq E 0 þ 4Dq E 0 0 0

0 0 E 0 þ 6Dq E 0 0

0 0 0 E 0 4Dq E 0

0

0

0

0

0 E Dq E

7.1 Energy Levels and Spectral Properties of 3d1 Electron System

207

This determinant equation is equivalent to a three-order one with only diagonal elements and a two-order one. It is easy to ﬁnd out that its solution can be divided into two groups, one has double degeneracy, the other has triplet degeneracy, that is (E) = E0+ 6Dq with double degeneracy and E(T2) = E0−4Dq with triplet degeneracy. The spin degeneracy has not been considered now. From Chap. 2 we know that the representation DL (L = 2) of the rotation group SO3 will be reduced to one irreducible representation C3(E) (two-dimension) and one irreducible representation C5(T2) (three-dimension) of group O (it can be found in Appendix B, there is 2!3⊕5 of the SO3!O irreducible representation reduction). Only the electronic states of the orbital and their degeneracy are considered here, so the spin degeneracy has not been included. The energy levels are denoted by the symbols of group irreducible representation as shown in Fig. 7.2. When active ions have the octahedral coordination symmetry, the energy levels of 2E and 2T2 are shown in Fig. 7.2, in which the energy of 2E is higher than that of the 2T2. However, if the active ions have tetrahedral or cubic coordination symmetry, the energy of the 2E is lower than that of the 2T2; besides their crystal ﬁeld splittings are smaller by a factor of 4/9 and 8/9, respectively. This is because in these three coordination symmetries, the Dq values have the following relation 9 9 DqðoctaheÞ ¼ DqðtetratÞ ¼ DqðcubicÞ 4 8

ð7:8Þ

In titanium sapphire (Ti3+:Al2O3), the positions occupied by Ti3+ ions have a small trigonal distortion, that is, they have the crystal ﬁeld components with point group symmetry C3, which further split the energy levels with symmetry of point group O. Since the crystal ﬁeld does not change the spin multiplicity, in the following discussion, the sign of the spin multiplicity is omitted for the symbols of all the energy levels. The irreducible representation C5(T2) of group O becomes reducible in group C3 and can be reduced to the sum of two irreducible representations A1⊕E (C1⊕(C2⊕3)) of group C3. Correspondingly, the energy level

2

2

D

E

2

John-Teller effect

E

A1 2

T2 2

Free ion

Cubic

Spin-orbit coupling

E

Trigonal

Fig. 7.2 Energy levels of d1 electron in cubic and trigonal ﬁelds

208

7 Energy Levels and Spectroscopic Properties of Transition …

E(C5) is split into two energy levels E(C1) and E(C2⊕3) (the C2 and C3 are one-dimensional irreducible representations and conjugate to each other, and together form a two-degree degenerate level). On the other hand, the irreducible representation E(C3) of group O corresponds to the irreducible representation E (C2⊕3) of group C3. It means that the energy level E(C3) of the system with symmetry O will not be further split in the trigonal crystal ﬁeld. Moreover, this double-electron state has no spin–orbit splitting, as discussed in the following. For a single electron, the spin–orbit interaction Hamiltonian is expressed as (1.2), where the operator of orbital angular momentum belongs to T1(C4) irreducible representation of the group O. If the orbital wave function belongs to G irreducible representation of group O, then the condition for a non-zero spin– orbit interaction matrix element is that the product G⊗T1(C4)⊗ G should include A1(C1) representation of group O. Therefore, the matrix element of the spin–orbit interaction between the energy levels with orbital wave functions belonging to T1(C4) and T2(C5) of group O is non-zero, because T2(C5)⊗T1(C4)⊗T2(C5) includes A1(C1) representation of group O. The ground electronic double-state E(E) is one of the energy levels split under trigonal crystal ﬁeld from energy level E(T2) belonging to irreducible representation T2 of group O (see Fig. 7.2). According to the formula given in Chap. 3, the matrix element of spin–orbit interaction of the wave function with irreducible representation E of C3 symmetry group can be expressed as the spin–orbit interaction matrix element of wave function with T2 irreducible representation of group O multiplied by corresponding 3jm factor. Therefore, the ground electronic double-state E (E) under C3 symmetry can be split by spin–orbit interaction into two electronic single levels. The higher electronic double-state E(E) is the energy levels split under trigonal crystal ﬁeld from energy level E(E) belonging to E irreducible representation of group O, and its wave function does not satisfy the condition E(C3)⊗T1(C4)⊗E(C3) that includes A1(C1) so that it cannot split by the spin–orbit interaction. However, some of the energy levels without spin–orbit splitting can be split by Jahn-Teller effect, that is the degeneracy will be removed by the electron–lattice vibration interaction. Similar to the analysis given by Sugano [3] for the E level with cubic symmetry, the Jahn-Teller splitting of E level with trigonal symmetry can be calculated. If one denotes two coordinates of normal modes by Q1 and Q2 belonging to irreducible representation E which have interaction with electron states, introducing the polar angle h and radius vector q, coordinates Q1 and Q2 can be expressed as Q1 ¼ q cos h; Q2 ¼ q sin h Therefore, after Jahn-Teller splitting the energy separation between these two levels will be

7.1 Energy Levels and Spectral Properties of 3d1 Electron System

209

DEJT ¼ 2Aq where A has the following relation with Q1 and Q2 A¼

1 EVEg ðrÞEi 2

E E

E E

E E

O C3

where VEg ðr Þ is the coefﬁcient of the ﬁrst-order term of the electron-phonon interaction energy expanding in terms of the normal coordinates, which belongs to the Eg representation. The 3jm factor [7] involved in the formula is

E E

E E

E E

O

C3

3 2

3 2

3 2

O

1 ¼ pﬃﬃﬃ 2 C3

In the case of titanium sapphire, the value obtained by experiment is DEJT = 1850 cm−1 [8]. The energy levels of Ti3+ in titanium sapphire have been shown in Fig. 7.2. It should be pointed out that the ﬁve electronic single-states split by crystal ﬁeld and spin–orbit interaction or Jahn-Teller effect still have Kramers degeneracy, which can only be removed by magnetic interactions. The absorption band of titanium sapphire is peaked at 490 nm corresponding to the transition from low-energy double-state E (E) to high-energy double-state E(E). The peak of the emission band is at 770 nm and the p polarized spectrum has higher intensity than that of the r polarized spectrum at 300 K. Its absorption and emission spectra are shown in Fig. 7.3. It is shown that the titanium sapphire used as tunable laser crystal has the following distinct advantages: First, the separation between the excited state and the ground state is proportional to crystal ﬁeld strength and so is strongly affected by crystal ﬁeld and lattice vibration. There are large Stokes shift between the excited Fig. 7.3 Absorption and emission spectra of titanium sapphire

Absorption

Emission

7 Energy Levels and Spectroscopic Properties of Transition …

210

and ground states, which leads to a very wide phonon side band; hence the titanium sapphire laser has a very wide tunable range from 650 to1060 nm. Secondly, the initial and ﬁnal states of the transition have the same spin multiplicity, thus the transition is spin allowed and so is strong. Correspondingly, the lifetime of the upper laser state is as short as 3.2 ls, thus it can only be efﬁciently pumped by laser sources. Thirdly, the aluminum oxide is a material with very high Debye temperature so that the electrons of Ti3+ ions have strong interaction with lattice vibration. In this way, the absorption and emission will be intensiﬁed. As a result, the pumping efﬁciency is higher than 25%. Fourthly, as shown in the energy level diagram, above the fluorescent level, there are no other excited states; hence the excited state absorption is non-existent. These are the prominent advantage of titanium sapphire over other tunable laser crystals. Other spectral properties of the titanium sapphire can be referred to the paper published by Moulton [9]. Ti: BeAl2O4 is also a trivalent titanium tunable laser crystal, and its spectral properties can be found in [10]. It should be pointed out that the disadvantage of Ti3+ laser materials is the valence instability of Ti3+ ions; they can change to Ti2+ or Ti4+ and will reduce the laser performance.

7.2

Energy Levels and Spectral Properties of 3d2 Electron System

Transition metal ions Cr4+, V3+, Ti2+, and Mn5+ have electronic shell 3d2; among these the Cr4+ ion is more stable. One can investigate the electronic states of d2 conﬁguration in crystals by two schemes. First, the weak ﬁeld scheme: It can be seen from Table 1.1 in Chap. 1 that the terms of the free ions with conﬁguration d2 are: spin single-state—1S, 1D, 1G and spin triple-state—3P, 3F. When the ions are sited in positions with symmetry lower than that of the rotation group SO3, then the free ion states 2S+1L belonging to irreducible representation DL of group SO3 will be split into crystal ﬁeld states belonging to irreducible representations of group O. The reduction of irreducible representation can be obtained by the theorem introduced in Chap. 2. One can refer to the reduction table in Appendix B to obtain the following results: 1

SðL ¼ 0Þ 1 A1 ; DðL ¼ 2Þ 1 E;1 T2 ;1 GðL ¼ 4Þ 1 A1 ;1 E;1 T1 ;1 T2 ;

3

PðL ¼ 1Þ 3 T1 ;3 FðL ¼ 3Þ 3 A2 ;3 T1 ;3 T2 .

Secondly, the strong ﬁeld scheme: As having been seen in the previous section, single electron in the cubic ﬁeld will have two energy levels E and T2. Two d electrons can be: both in E state; both in T2 state; or one in E state and the other in T2 state. After introducing the interactions between electrons and between the spin and orbital momentum, the ﬁnal electronic energy levels usually will be denoted by irreducible representation symbol with lowercase letters. Therefore, the states

7.2 Energy Levels and Spectral Properties of 3d2 Electron System

211

occupied by single electron are designated by letter e and t2. The electronic system studied can have the conﬁgurations of t22, e2, or t12e1. By the multiplication table of the irreducible representation of group O, the following can be obtained T2 ð5Þ T2 ð5Þ ¼ A1 ð1Þ Eð3Þ T1 ð4Þ T2 ð5Þ Eð3Þ Eð3Þ ¼ A1 ð1Þ A2 ð2Þ Eð3Þ T2 ð5Þ Eð3Þ ¼ T1 ð4Þ T2 ð5Þ The ﬁgures in the brackets of Muliken symbols are the subscripts i of Bethe symbol Ci. The corresponding relationship between the Muliken symbol and the Bethe symbol (and the subscript of Bethe symbol) is listed to facilitate the search for the relevant tables of this book. The following will be described in accordance with the Muliken symbols usually used in the literature of spectroscopy for iron group ions. The relations of two kind symbols for low symmetry group can be found in Appendix A. According to Pauli exclusion principle, two electrons in the states of T1 and T2 in conﬁguration t12e1 can have their spin either parallel (spin triple state) or antiparallel (spin single-state), which results in the states of 3T1 1T1, 3T2, and 1T2. The spin multiplicity of the conﬁgurations of t22 and e2 can be determined similarly. According to Pauli exclusion principle, the total electron wave functions should be antisymmetry. Thus, if the orbital wave function is symmetry, the spin wave function should be antisymmetry. Contrarily, if the orbital wave function is antisymmetry, the spin wave function should be symmetry. In order to determine the symmetry properties of orbital wave function, the symmetry properties of the irreducible representation reduced by direct product of group representations discussed in Chap. 2 should be utilized. The vector space of t22 is the direct product of two t2 vector spaces t2⊗t2. If the basic vector of one of these vector spaces is expressed by w(1,i) (ith basic vector of electron 1), the other is w(2,j) (jth basic vector of electron 2), then the basic vector of the direct product space will be w(1,i)w(2,j). This direct product space can be reduced to a sum of a series of subspaces with each subspace corresponding to one irreducible representation reduced from the direct product representation of T2⊗T2. The basic functions of these subspaces are the linear combinations of w(1,i)w(2,j). As to the symmetry properties of exchange electronic coordinates, the basic vector of the direct product space can be divided into: symmetry type w(1,i)w(2,j) + w(2,i)w(1,j) and antisymmetry type w(1,i)w(2,j)-w(2,i)w(1,j) (i6¼j). The subspaces formed by symmetric basic vectors correspond to one or several symmetric irreducible representations and those formed by antisymmetric basic vectors correspond to one or several antisymmetric irreducible representations. The character of the symmetric representation of the square direct product is denoted by [v2](G) and that of the antisymmetric representation is denoted by {v2}(G) (in the problem discussed, G is one of the symmetry operation of the cubic group O). Obviously, [v2](G) can be calculated as follows

7 Energy Levels and Spectroscopic Properties of Transition …

212

G½wð1; iÞwð2; jÞ þ wð2; iÞwð1; jÞ ¼

X

Gli Gmj ½wð1; lÞwð2; mÞ þ wð2; lÞwð1; mÞ

lm

The indexes l and m are only the symbols for summation; exchanging them will not alter the values of the sum. Therefore, the above expression can be changed into 1X Gli Gmj þ Gmi Glj ½wð1; lÞwð2; mÞ þ wð2; lÞwð1; mÞ 2 lm The character [v2](G) obviously is to multiply from the left of the wave function wð1; iÞwð2; jÞ þ wð2; iÞwð1; jÞ then let l = i, m = j and sum over i and j as shown in the following X 2 v ðGÞ ¼ ½wð1; iÞwð2; jÞ þ wð2; iÞwð1; jÞ G½wð1; iÞwð2; jÞ þ wð2; iÞwð1; jÞ ij

¼

1h i Gii Gjj þ Gij Gji ¼ vðGÞ2 þ v G2 2 2

X1 ij

ð7:9Þ because X i

Gii ¼

X j

Gjj ¼ vðGÞ;

X ij

Gij Gji ¼

X

G2jj ¼ v G2

j

Similarly, one can obtain 2 i 1h v ðGÞ ¼ vðGÞ2 v G2 2

ð7:10Þ

The characters of the symmetry and antisymmetry representations of the cubic group are listed in Table 7.1. According to the reduction formula of irreducible representation ((2.7) in Chap. 2) and the characters given in Table 7.1, it is possible to determine the symmetry and antisymmetry irreducible representations. By using the symmetry representation character shown in Table 7.1 [v2](T2) = v(A1) + v(E) + v(T2) and {v2}(T2) = v(T1). It shows that the direct product T2⊗T2 includes symmetry irreducible representations A1, E, and T2, and antisymmetry irreducible representation T1. The antisymmetry character of the total wave function requires that the symmetry orbital wave function should be coupled with antisymmetry spin wave function. Contrarily, the antisymmetry orbital wave function should be coupled with symmetry spin wave function. Consequently, t22 conﬁguration generates three-spin single states 1A1, 1E, and 1T2 as well as one-spin triple state 3T1. Similarly, e2 conﬁguration includes two-spin single states 1A1, 1E, and one-spin triple state 3A2. Obviously, the results obtained by the strong ﬁeld scheme are the same as those of the weak ﬁeld scheme.

7.2 Energy Levels and Spectral Properties of 3d2 Electron System Table 7.1 Symmetry and antisymmetry representations of T2⊗T2 of the cubic group O

213

O

E

8C3

3C2

6C4

6C2’

v(A1) v(A2) v(E) v(E2) v(T1) v(T2) v(T22) [v2](E) {v2}(E) [v2](T2) {v2}(T2)

1 1 2 2 3 3 3 3 1 6 3

1 1 −1 −1` 0 0 0 0 1 0 0

1 1 2 2 −1 −1 3 3 1 2 −1

1 −1 0 2 1 −1 −1 1 −1 0 1

1 −1 0 2 −1 1 3 1 −1 2 −1

By means of the term energy of the free ions given in Chap. 1, it is convenient to calculate energy levels of the ions in a crystal ﬁeld by the weak ﬁeld scheme. The vector space formed by the electronic wave function of the entire 3d2 conﬁguration can be reduced to several subspaces; each subspace has the same irreducible representation and spin multiplicity. Owing to the fact that the crystal ﬁeld Hamiltonian belongs to the identity representation of the point group of active ions and does not include spin variable, the crystal ﬁeld matrix elements between wave functions belonging to different subspaces are equal to zero. Therefore, the calculation of energy eigenvalue only needs to be performed in the same irreducible representation subspace. As a simple example, one can see the energy calculation of the levels belonging to A1 representation of cubic group O. Both the free ion terms 1 S and 1G generate level A1 in the cubic crystal ﬁeld. The electrostatic interaction energy between electrons has been given in Chap. 1, i.e.

d 2 ; 1 S; A1 H0 þ Hee d 2 ; 1 S; A1 ¼ A þ 14B þ 7C

2 1 d ; G; A1 H0 þ Hee d 2 ; 1 G; A1 ¼ A þ 4B þ 2C

The calculation of the matrix elements of the crystal ﬁeld Hamiltonian can utilize directly the 3jm factor of the group-chain SO3 O and (2.53) as well as the formulas similar to (3.18) and (3.19). The reduced matrix elements of tensor U(4) can be found from the published tables [11]. In the case of d electron in cubic ﬁeld, there is only one term in the crystal ﬁeld Hamiltonian Vc ¼ C04 b40

ð7:11Þ

By using tetragonal coordinate system, that is adopting the tetragonal symmetry axis as z-axis, it can be obtained in the electrostatic model that

7 Energy Levels and Spectroscopic Properties of Transition …

214

C04 ¼ 42ð3=7Þ1=2 Dq

ð7:12Þ

The energy of 3A2 level is equal to that of the spectral term 3F of the free ion, that is A-8B (shown in Chap. 1, Table 1.4) plus the following crystal ﬁeld energy

d 2 ; 3 F; 3 A2 Vc d 2 ; 3 F; 3 A2 E

3 4 3 SO3 2 D 2 3 ¼ d ; F U ð4Þ d 2 ; 3 F d C 4 d C04 2 1 2 O c pﬃﬃﬃ pﬃﬃﬃﬃﬃ pﬃﬃﬃ pﬃﬃﬃ 2 11 5 2 42 3 ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 pﬃﬃﬃ pﬃﬃﬃﬃﬃ pﬃﬃﬃ Dq ¼ 12Dq 3 11 7 5 35

ð7:13Þ

where 2jm symbol equals +1, therefore

d 2 ; 3 F; 3 A2 H0 þ Hee þ Vc d 2 ; 3 F; 3 A2 ¼ A 8B þ 12Dq

ð7:14Þ

Similarly, the energy of 3T2 is equal to the A-8B plus the following crystal ﬁeld energy

d 2 ; 3 F; 3 T2 c Vc d 2 ; 3 F; 3 T2 c E

3 4 3 SO3 5 5 1 5 OD 2 3 ¼ d ; F U ð4Þ d 2 ; 3 F d C4 d C04 5 1 5 O c c 1 c pﬃﬃﬃﬃﬃ pﬃﬃﬃ pﬃﬃﬃ 1 1 11 5 2 42 3 ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃ pﬃﬃﬃ pﬃﬃﬃﬃﬃ pﬃﬃﬃ Dq ¼ 2Dq 3 7 3 2 11 5 35 ð7:15Þ

In the above equation c represents the component of T2 irreducible representation. The products of 2jm symbol with 3jm symbol following it for three c components pﬃﬃﬃ all equal to þ 1= 3, therefore

d 2 ; 3 F; 3 T2 c H0 þ Hee þ Vc d 2 ; 3 F; 3 T2 c ¼ A 8B þ 2Dq

ð7:16Þ

In the strong ﬁeld scheme, the energy of 3A2 level is 20Dq and the energy of 3T2 level is 10Dq [5]. The energy difference of the two levels is also 10Dq. All the above matrix elements include a common term A, while it has only the effect to shift all the energy levels parallel. If we focus on the separation between different levels, the term A can be omitted. Substituting the detailed value of B and Dq into above secular determinant or matrix elements of Hamiltonian, the eigenvalues of all the energy levels discussed can be obtained. Drawing a curve of energy eigenvalue E/B versus the crystal ﬁeld strength Dq/B, the Tanabe-Sugano (T-S) energy level diagram shown in Fig. 7.4 can be obtained.

7.2 Energy Levels and Spectral Properties of 3d2 Electron System

215

Fig. 7.4 Tanabe-Sugano diagram of d2 electron conﬁguration in the octahedron position

This T-S energy level diagram is in fact similar to that of the d8 conﬁguration in the octahedron position. In the latter case, the ground state is 3A2 but not 3T1 and the third excited state with the same spin multiplicity belongs to 3T1. The relationship of the energy level of the transition metal ions in the octahedron position with that in the tetrahedron position is described below. The previous calculation shows that if the transition metal ions occupy the octahedron position, the crystal ﬁeld parameter in the group chain scheme can be expressed as the form of (7.12). The T-S energy level diagram given in many reference books is for this octahedron position. However, when the active ions are sited in tetrahedron position, (7.8) shows that the crystal ﬁeld parameter Dq is not only different in number but also opposite in sign to that for the octahedron position. Consequently, their energy level diagrams will be different. The following relation between the reduced matrix element of tensors U(k)(4 l + 2−q) and U(k)(q) was given by Nielson et al. [11] D E D E aSLU ðkÞ ð4l þ 2 qÞaSL0 ¼ ð1Þk aSLU ðkÞ ðqÞaSL0 Applying it to the case studied k = 4, the sign of reduced matrix elements of tensor U(4) for dq conﬁguration is the opposite of that for d10−q conﬁguration. Therefore, the dq conﬁguration in octahedron position has a similar T-S energy level diagram as d10−q conﬁguration in tetrahedron position, because the negative sign generated in crystal parameter is cancelled by the negative sign coming from reduced matrix elements of tensor U(4). This is the reason why the T-S energy level diagram for d8 conﬁguration in octahedron position is similar to that of d2 conﬁguration in tetrahedron position, if one concerns only the relative position of different energy levels. As typical examples of the energy levels and spectra of d2 electronic conﬁguration, the energy levels and spectra of Cr4+:Y2SiO5 and Cr4+:Mg2SiO4 will be

216

7 Energy Levels and Spectroscopic Properties of Transition …

analyzed. The former is a very good example for the study of the spectra of tetravalent chromium-doped crystals, because there is pure Cr4+ doping, where Cr4+ ions occupy deﬁnite C3v positions. The energy levels of crystal Cr4+:Y2SiO5 are shown in Fig. 7.5. Cr4+ ions in crystal Cr4+:Mg2SiO4 occupy Si positions of the SiO4 tetrahedron and have approximately the C3v symmetry [12]. Note that the axis a has a threefold symmetry. Now let’s turn to the discussion of the selection rule of absorption transitions. It can be seen from the character table of group C3v that the z component of the electric-dipole moment belongs to representation A1 of the group C3v and its x and y components belong to representation E. The allowed electric-dipole transitions should satisfy the requirement of hijerj f i 6¼ 0. In the language of group theory, the product of the irreducible representations of the initial and the ﬁnal states should include the irreducible representations of the electric-dipole moment. Note that the z axis should be the threefold axis of SiO4, that is the crystal axis a. The transition 3 A2!3A2 (3T1) shown in Fig. 7.5 has polarization of electric ﬁeld E parallel to axis a, because of the relations A2⊗A2 = A1 (the z component of the electric-dipole moment belongs to A1 representation). Similarly, the transition 3A2!3E (3T1) has polarization of electric ﬁeld E perpendicular to axis a, because of the relation A2⊗E = E. Strictly speaking, the position symmetry of Cr4+ ions in crystal Y2SiO5 is Cs, Therefore, the transition 3A1 (3T2)!3A2 forbidden in the C3v symmetry case is allowed in crystal Cr4+:Y2SiO5, which corresponds to a weak absorption at

Fig. 7.5 Energy level diagram of Cr4+:Y2SiO5

7.2 Energy Levels and Spectral Properties of 3d2 Electron System

217

wavelength of 882.6 nm. The weakness of this absorption line shows that the distortion of crystal ﬁeld to Cs symmetry is small. The polarized absorption spectrum of the Cr4+:Y2SiO5 crystal is shown in Fig. 7.6 and the fluorescence spectrum of this crystal is shown in Fig. 7.7. The laser properties of this crystal at the temperature of liquid nitrogen were studied by Chai et al. [13] Actually there is a laser emission even at temperature of 257 K. It is very interesting to note that pumped at different wavelengths, their laser and tunable performances have a big difference. Pumped by 1064 nm-laser, the emission peak is at 1270 nm and has linewidth of 10 nm. However, the emission peak is at 1225 nm and has linewidth of 23 nm when the pumping wavelength is 532 nm. Finally, pumped at 840 nm, the emission peak is still at 1225 nm while the linewidth changes to 30 nm. Chromium ions in crystal Mg2SiO4 may exist at the same time as trivalent and tetravalent states with trivalent chromium occupies the octahedron Mg position (having symmetry of Cs and Ci) and the tetravalent one occupies the tetrahedron Si position (having approximately C3v symmetry with Cs distortion component). These have been conﬁrmed by detailed structure data, electron paramagnetic resonance and electron nuclear double-resonance experiments [12, 14, 15].

Fig. 7.6 Polarized absorption spectrum of the Cr4+:Y2SiO5 crystal [13]

218

7 Energy Levels and Spectroscopic Properties of Transition …

Arbitrary unit

Fig. 7.7 Fluorescence spectrum of Cr4+:Y2SiO5 crystal [13]

However, as one of the tunable laser crystal, the Cr4+:Mg2SiO4 has a series of advantages, although the spectrum of this crystal is rather complicated. Particularly, its laser emission tunable wavelength range of 850–1400 nm covers the wavelength of 1300 nm, which is very important to the laser optical communication. It also covers the water absorption wavelength range, and by tuning the wavelength of the laser, the penetration depth in the human body can be controlled, hence is very useful in laser medical treatments. The Cr4+:Mg2SiO4 laser has become one of the important commercial laser systems at room temperature [16], and it is necessary to know more about its spectral properties. The ratio of the amount of Cr4+ ions to that of Cr3+ ions depends on the condition of crystal growth. For the crystals grown in reduction atmosphere, the ratio of the Cr4+ will be decreased and that of the Cr3+ will be increased. Therefore, in order to obtain crystal with larger amount of Cr4+, the crystal growth should be in standard condition. Their main transition wavelengths are listed in Table 7.2 [16]. Table 7.2 Main transitions and their central wavelengths of Cr4+:Mg2SiO4 crystal

Transition channel

Central wavelength (nm)

A2!3T2 3 A2!3T1(t2e) 3 A2!1E 3 A2!3T1(t22) 3 A2!1T2 3 T2!3A2

1092.9 648.1 629.9 373 348 1142.9

3

7.2 Energy Levels and Spectral Properties of 3d2 Electron System

219

The spectral and tunable laser properties of Cr4+ ions in garnet crystals especially in YAG crystal have been fully studied [17]. Wavelength of these lasers covers the wavelength range of minimum loss ﬁber communication and eye safe. Among these, Cr4+:YAG has realized 1309–1596 nm tunable laser emission at room temperature with peak emission cross-section of 1.7 10−19 cm2, while Cr4+: YSAG has realized 1446–1604 nm tunable laser emission at room temperature with peak emission cross-section of 1.5 10−19 cm2.

7.3

Energy Levels and Spectral Properties of 3d3 Electronic System

Now turn to the energy level structure and spectral properties of trivalent chromium, which have been studied ﬁrst and intensively among transition metal ions. Compared with 3d2 system, 3d3 system has more complicated energy level structure. However, using the group chain scheme, the crystal ﬁeld calculation will be very simple. Taking the upper laser state 4T2 and lower laser state 4A2 of the Cr3+ tunable laser crystal as examples, let us see how to use the method proposed to calculate energy eigenvalues of the crystal ﬁeld Hamiltonian. Both the states come from free ion’s spectral term 4F and there are only one 4A2 state and one 4T2 state in the conﬁguration 3d3, so it is only necessary to calculate the diagonal matrix elements for the calculation of crystal ﬁeld energy levels

d 3 ; 4 F; 4 T2 c Vc d 3 ; 4 F; 4 T2 c E

5 1 5 OD 3 4 3 4 3 SO3 5 ¼ d ; F U ð4Þ d 3 ; 4 F d C4 d C04 c c 1 c 5 1 5 O pﬃﬃﬃﬃﬃ pﬃﬃﬃ pﬃﬃﬃ 11 5 2 42 3 1 1 ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃ pﬃﬃﬃ pﬃﬃﬃﬃﬃ pﬃﬃﬃ Dq 3 7 3 2 11 5 35 ¼ 2Dq

ð7:17Þ It should be noted that for irreducible representation T2, its three c components that have the same crystal ﬁeld matrix elements corresponding to the calculated energy level is a threefold degenerate electronic orbital energy level. On the other hand,

7 Energy Levels and Spectroscopic Properties of Transition …

220

d 3 ; 4 F; 4 T1 c Vc d 3 ; 4 F; 4 T1 c E

3 4 3 SO3 4 4 1 1 OD 3 4 ¼ d ; F U ð4Þ d 3 ; 4 F d C4 d C04 4 1 4 O c c 1 c pﬃﬃﬃﬃﬃ pﬃﬃﬃ pﬃﬃﬃ 11 5 2 42 3 1 1 ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃ pﬃﬃﬃ pﬃﬃﬃﬃﬃ pﬃﬃﬃ Dq 3 7 2 11 5 35 ¼ 6Dq

ð7:18Þ

d 3 ; 4 F; 4 A2 Vc d 3 ; 4 F; 4 A2

3 4 3 SO3 3 4

4

3 4 ¼ d ; F U d ; F d C4 d C04 2 1 2 O pﬃﬃﬃﬃﬃ pﬃﬃﬃ pﬃﬃﬃ pﬃﬃﬃ 11 5 2 42 3 2 ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃ pﬃﬃﬃﬃﬃ pﬃﬃﬃ Dq 3 11 7 5 35 ¼ 12Dq

ð7:19Þ

4

A2 and 4T2 levels are both derived from the same free ion spectral term 4F, and the spectral term near it in energy is 4P, which can only introduce the energy level 4 T1 with different irreducible representation from those of 4A2 and 4T2 levels. The energy operator matrix elements between them is equal to zero. Therefore, the energy eigenvalues of 4A2 and 4T2 levels can be determined by the diagonal matrix element of the energy operator, then Eð4 T2 Þ Eð4 A2 Þ ¼ 10Dq

ð7:20Þ

By using strong coupling approximation, it can be shown [18] that E(4A2) = 3A −15B and E(4T2) = 10Dq + 3A−15B, then the separation between these two levels is the same as (7.20), which is a formula often used in the calculation of spectroscopic parameters of tunable laser crystals. Dq is a parameter to characterize the crystal ﬁeld strength of transition ions. The value of Dq increases with anions according to the order Cl− < F− 3d have not any substantial variation in the process of lattice vibration. It means that the crystal ﬁeld energy E depends on the ﬁfth power of R. Consider all the interactions including point charge Coulomb interaction, the general dependent relation of the crystal ﬁeld energy will take the following form: E ¼ ARn

ð7:32Þ

where A is a constant, n assumes the value of 5 in point-charge approximation and a value between 4.5 and 5 in general. By (7.32) it is obvious dE ¼ nE=R dR

ð7:33Þ

The energy variation dE in the process of electronic transition also satisﬁes the same relation ddE ¼ ndE=R dR

ð7:34Þ

On the other hand, by assuming a single-mode model as that adopted by the conﬁguration coordinate model, we discuss in fact the interaction of the electrons in the central active ion with a “breathing mode” vibration of six ligand ions, which has A1g symmetry. This local structure consists of six linear oscillators; each has an energy change of dE/6 during the electronic transition. If the variation of conﬁguration coordinates of any of these oscillators during the electronic transition is denoted by Dji, then the interaction force generated by the transition for each oscillator can be expressed as

234

7 Energy Levels and Spectroscopic Properties of Transition …

F¼

1 ddE 2 Dji ¼ Mx 6 dR

ð7:35Þ

where M refers to as the mass of the ligand ion. According to the deﬁnition of Huang–Rhys factor and the fact that there are six oscillators in the model discussed, noting that the mass of oscillator has been dealt with as a unit in the formula of S in Chap. 6, it is obvious 2ji =h S ¼ 3M xD

ð7:36Þ

Therefore, the following relation will be obtained by (7.34), (7.35), and (7.36) S¼

n2 ðdE Þ2 3 12hMR2 x

ð7:37aÞ

or 2 n2 h2 dE ¼ Shx 2 12MR hx

ð7:37bÞ

Equation (6.54) shows that the Stocks shift corresponding to the difference of the peak of the absorption spectrum Ea and that of the emission spectrum Ee is equal and dE in the above equation is the peak of the absorption to the double of Shx, spectrum Ea, then ¼ Ea hx

n R

h2 6M ðEa Ee Þ

1=2 ð7:38Þ

Associating with (6.55), the full-width at half-maximum of the emission line can be expressed as 1=2 cothð W ¼ ½4ðln 2ÞðEa Ee Þhx hx=2k B T Þ

ð7:39Þ

Equations (7.32)–(7.39) are really introduced by simple single-mode approximation, which is the same as that has been adopted in the performance investigation of tunable laser crystals. Therefore, one can use these formulas to describe performances of tunable laser crystals without considering whether they have real microcosmic meaning, but remembering that they are only phenomenological parameters. Actually, electron–phonon interaction in laser materials is indeed multi-mode and multi-frequency, and the phonon state density of different mode is always different. They are still phenomenological and even two or three modes are used to describe the spectral properties. Ducilos et al. [49] have shown that for Cr3+:Al2O3 at a pressure as high as 35 GPa, n in (7.32) increases with R. Therefore they have assumed that n/R is a

7.5 Estimation of Trivalent Chromium Ion Spectral …

235

constant within a certain range of pressure. For oxides and fluorides, it can be assumed that n/R = 2.25 108 cm−1. The mass of oxygen ion is MO = 2.7 10−23 g and that of fluorine ion is MF = 3.2 10−23 g, then the phonon energy of effective single mode for the transition between electronic levels 4 A2 and 4T2 can be expressed as, for oxides 2:25Ea ½0:3456=ðEa Ee Þ 1=2 hx

ð7:40Þ

2:25Ea ½0:2910=ðEa Ee Þ 1=2 hx

ð7:41Þ

for fluorides

By means of (7.39), (7.40), and (7.41), the effective phonon energy and width of the spectral line in single-mode approximation can be obtained by the data of the peak positions of the absorption and emission spectra. By using (6.54), (7.40), and (7.41), the effective phonon energy and Huang–Rhys factor can be calculated. Compared with the results obtained by other methods, it is evident that the approach proposed is suitable for the investigation of the performances of laser crystal. This comparison is shown in three tables followed. The calculated results and the comparison with the experimental data of the linewidth are given in Tables 7.7 and 7.8. The relative errors for oxide and fluoride crystals are all less than 10% in the 23 examples given, except for those cases in which disorders or second centers appear in the crystals. Comparing the effective phonon energy and Huang–Rhys factor calculated by the direct method proposed with those obtained by other methods published in the literature, it can be seen that the direct method proposed also lead to very good results, which are given in Table 7.9. It is simple to measure the width of the spectral line. By using the direct method proposed to calculate linewidth and comparing with the experimental result, it is possible to ﬁnd if there is disorder structure or multi-center in crystals. In this case, the calculated linewidth will be much smaller than the measured value obtained by the experiment. Certainly, to obtain a correct experimental data of linewidth, the response curve of the spectrometer should certainly be corrected.

Table 7.7 Comparison of calculated results with experimental data of emission linewidth for the transition 4T2!4A2 of Cr3+ ions in fluoride crystals Crystal

T (K)

Ea (cm−1)

Ee (cm−1)

W Cal. (cm−1)

W Exp. (cm−1)

Ref.

Error (%)

KZnF3 ScF3 LiSrAlF6 LiSrGaF6 Na3Ga2Li3F12

80 14 20 295 18

14858 14280 15676 15873 16069

12934 12028 12821 12054 13313

1482 1510 1679 2237 1685

1521 1495 1690 2438 1740

[50] [51] [52] [53] [54]

2.6 1.0 1.2 8.2 3.2

7 Energy Levels and Spectroscopic Properties of Transition …

236

Table 7.8 Comparison of calculated results with experimental data of emission linewidth for the transition 4T2!4A2 of Cr3+ ions in oxide crystals Crystal

T (K)

Ea (cm−1)

Al2(WO4)2 ZnWO4 ZnWO4 YAl3(BO3)4 La3Ga5SiO4

300 15229 300 13766 9 13500 300 16949 300 15748 300 15748 YGG 300 16293 GGG 300 15963 YSGG 300 16128 LGG 300 14794 GSGG 300 15631 177 15430 89 15430 GAGG 300 15600 100 15600 300 16000 Ca3Ga2Ge4O14 Sr3Ga2Ge4O14 300 16260 Sc2O3 14 15200 a There is disorder for the crystal ﬁeld

Ee (cm−1)

W Cal. (cm−1)

12157 10278 10145 13513 r:11395 p:11549 13691 13617 13332 11758 12993 13506 13624 13444 13717 10989 11905 11875 of chromium

2073 2117 1693 2215 2406 2370 1971 1886 2022 2051 1963 1606 1538 1817 1576 2560 2420 1792 ions, bthere

W ExP. (cm−1)

Ref.

Error (%)

2100 [24, 55] 1.3 2105 [36] 0.6 1588 [56] 6.6 2127 [57] 4.1 2127 [26] 1.3 2525 [26] 6.1 1900 [32] 1.5 1900 [32] 0.7 2100 [32] 3.7 2100 [32 2.3 2000 [32] 1.9 1558 [58, 59] 3.1 1429 [58, 59] 7.6 1732 [58, 59] 4.9 1514 [58, 59] 4.1 3645 [50] 29.7a 4085 [50] 40.8a 2329 [51] 23.0b is two chromium centers

Table 7.9 Comparison of the results of the method proposed with those obtained by other methods for effective phonon energy and Huang–Rhys factor of the transition 4T2!4A2 of Cr3+ ions in fluoride crystals Crystal

K2NaScF6 K2NaGaF6 Na3Ga2Li3F12 ScF3

T

Ea

Ee

(K)

(cm−1)

(cm−1)

295 295 18 14

15600 16000 16069 14280

13100 13600 13313 12028

Results of this method S hx (cm−1)

Results by other method S hx (cm−1)

Ref.

3.30 3.03 3.7 3.0

3.95 3.98 3.5 3.0

[60] [60] [54] [51]

379 396 372 367

380 378 400 380

There is another simple method to calculate effective phonon energy and Huang–Rhys factor if one has correct linewidth data. In the following, the calculation method without simpliﬁed supposition of (7.35) will be introduced. The detailed description of this method can be referred to [34]. The main basis of this method is (6.54) and (6.55), but it technically introduces a ratio c

7.5 Estimation of Trivalent Chromium Ion Spectral …

c¼

237

W2 DEs =2

ð7:42Þ

By means of (6.54) and (6.55), we have

hx c ¼ 8ðln2Þhxcoth 2kB T

ð7:43Þ

This method requires the experimental data of the peak positions of the absorption and emission spectra as well as the full-width at half-maximum of the emission line W. From the experimental data mentioned, c can be calculated by has a one-to-one corresponding (7.42). As shown in (7.43), the phonon energy hx It is easy to make a curve or to list a relation between c and phonon energy hx. table by this equation and then from the c value one can determine phonon energy although it is difﬁcult to express hx as an analytic function of c. Then S factor hx, and S factor obtained by these two can be found by (6.54). It has indicated that hx methods introduced are almost identical. The calculation in this section shows that for the strong electron–phonon system, the single-mode approximation is suitable to describe shape of spectral line including phonon side band, although it is a rough model. In view of the fact that the phonons have different frequencies, Huang Kun has proposed a statistical multi-phonon model [61]. According to this model, the author designed a method for measuring the phonon energy and Huang–Rhys factor by using measured spectral data [34]. However, from the practical point of view, the single-mode approximation is enough for the study of laser crystal. Of course, the single-phonon model has a lot of limitations. For example, when the spectral measurement can resolve zero-phonon line and a certain order of phonon side band, their intensity ratios cannot be always predicted by the single mode. When active ions situated in the positions with central symmetry, the electric-dipole transition within the same conﬁguration is forbidden but the lattice vibration breaks this central symmetry and introduces forced electric-dipole transition. In this case, the single phonon line but not the zero-phonon line is induced by electric-dipole transition, and so the zero-phonon line is much weaker. Further investigation shows that the intensity of electron–phonon coupling depends on the concentration of the active ions. Auzel [62] has reported the increase of Huang–Rhys S factor along with the concentration of the active ions. Physically, it can be interpreted as the range of electron interaction increases with the concentration of the active ion; it’s like the wave function of electrons with a larger range. When the concentrations of Ni2+ are 2 and 10%, the S factor will be 0.5 and 2.25, respectively, for Ni2+:MgF2 crystal.

238

7 Energy Levels and Spectroscopic Properties of Transition …

References 1. S. Kück, Appl. Phys. B 72, 515 (2001) 2. J.S. Grifﬁth, The Theory of Transition-Metal Ions (Cambridge University Press, Cambridge, 1961) 3. S. Sugano, Y. Tanabe, H. Kamimura, Multiplets of Transition-Metal Ions in Crystals (Academic Press, New York, 1970) 4. C.A. Morrison, Crystal Fields for Transition-Metal Ions in Laser Host Materials (Springer, Berlin, 1992) 5. B. Henderson, R.H. Bartram, Crystal-Field Engineering of Solid- State Laser Materials (Cambridge University Press, Cambridge, 2000) 6. M. Rotenberg, R. Bivins, N. Metropolis et al., The 3-j and 6-j Symbols (MIT Press, Massachusetts, 1959) 7. P.H. Butler, Pont Group Symmetry Application: Method and Tables (Plenum, New York, 1981) 8. E.D. Nelson, J.Y. Wong, A.L. Schawlow, Phys. Rev. 156, 298 (1967) 9. P.F. Moulton, in Laser Handbook, vol. 5, ed. by M. Bass, M.L. Stitch (North-Holland Publishers, Amsterdam, 1985), pp. P203–P289 10. A. Suginoto, Y. Segawa, P.H Kim., et al., J. Opt. Soc. Am. B, 6, 2334 (1989) 11. C.W. Nielson, G.F. Koster, Spectroscopic Coefﬁcients for the pn, dn, fn Conﬁgurations (MIT Press, Massachusetts, 1959) 12. R. Verdun, L.M Thomas, D.M. Andrauskas, et al., in ed. by M.L. Shand, H.P. Jenssen, OAS Proceedings on Tunable Solid State Lasers, vol. 5, (1989), p. 85 13. B.H.T. Chai, Y. Shimony, C. Deka, et al., in ed. by L.L. Chase, A.A. Pinto, OAS Proceedings on Advanced Solid State Lasers, vol. 13 (1992) 14. H. Rager, Phys. Chem. Miner. 1, 371 (1977) 15. L.H. Bershov, J.M. Gaite, S.S. Hafner, et al., Phys. Chem. Miner. 9, 95 (1983) 16. V. Petricevic, S.K. Gayen, R.R. Alfano, in ed. by M L. Shand, H.P. Jenssen, OAS Proceedings on Tunable Solid State Lasers, vol. 5, p. 77 (1989) 17. A. Sennaroglu, Prog. Quant. Elect. 26, 287 (2002) 18. B. Henderson, G.F. Imbusch, Optical Spectroscopy of Inorganic Solids (Clarendon Press, Oxford, 1989) 19. P.F. Moulton, Proc. IEEE 80, 348 (1992) 20. J.C. Walling, O.G. Peterson, H.P. Jenssen, et al., IEEE J. Quant. Elect. QE-16, 1302 (1980) 21. M.L. Shand, S.T. Lai, IEEE J. Quant. Elect. QE-20, 105 (1984) 22. P.T. Kenyon, L. Andrews, B. McCollum, et al., IEEE J. Quant. Elect. QE-18, 1189 (1982) 23. B. Struve, G.J. Huber, Appl. Phys. 57, 45 (1985) 24. Z.D. Luo, J.M. Chen, et al., Chin. Phys. 6, 991 (1986) 25. W. Kolbe, K. Petermann, G. Huber, IEEE J. Quant. Elect. QE-21, 1596 (1985) 26. S.T. Lai, B.H.T. Chai, M. Long, et al., IEEE J. Quant. Elect. QE-24, 1922 (1988) 27. S.A. Payne, L.L. Chase., H.W. Newkirk, et al., IEEE J. Quant. Elect. QE-24, 2243 (1988) 28. S.A Payne, L.L. Chase., L.K. Smith, et al., J. Appl. Phys. 66, 1051 (1988) 29. R. Scheps, Opt. Mater. 1, 1 (1992) 30. M.D. Perry, Laser Focus World 27, 69 (1991) 31. P. Beaud, M. Richardson, E.J. Miesak et al., Opt. Lett. 18, 1550 (1993) 32. B. Struve, G.J. Huber., Appl. Phys. B 36, 195 (1988) 33. Z.D. Luo, Y.D. Huang, J. Phys.: Condens. Matter 4, 9751 (1992) 34. Z.D. Luo, J.M. Chen, Chin. Phys. 11, 399 (1991) 35. C.J. Donnelly, S.M. Healy, T.J. Glynn et al., J. Lumin. 42, 119 (1988) 36. A.J. Wojtowicz, M. Grinberg, A. Lempicki, J. Lumin., 50, 231 (1991) 37. L.F. Johnson, H.J. Guggenheim, J. Appl. Phys. 38, 4837 (1967) 38. W. Knierim, A. Honold, U. Brauch et al., J. Opt. Soc. Am. B 3, 119 (1986)

References

239

39. L.F. Johnson, R.E. Dietz, H.J. Guggenheim, Phys. Rev. Lett. 11, 318 (1963); Phys. Rev. 149, 179 (1966) 40. P.F. Moulton, A. Mooradian, Appl. Phys. Lett. 35, 838 (1979) 41. B.C. Johnson, P.F. Moulton, A. Mooradian, Opt. Lett. 9, 116 (1984) 42. D. Welford, P.F. Moulton, Opt. Lett. 13, 975 (1988) 43. V. Petricevic, S.K. Gayen, R.R. Alfano, Appl. Opt. 27, 4162 (1988) 44. D.M. Rines, G.A. Rines, D. Welford, et al., in ed. by L.L. Chase, A.A. Pinto, OAS Proceedings on Advanced Solid State Lasers, vol. 13. p. 161 (1992) 45. W. Kunzel, U. Durr, Opt. Comm. 36, 383 (1981) 46. W. Kunzel, U. Durr, Appl. Phys. B 28, 233 (1982) 47. W. Koechner, Solid-State Laser Engineering, (Springer, Berlin, 1976) 48. Luo Zundu, Huang Yidong, J. Phys.: Condens. Matter 5, 9411 (1993) 49. S.J. Ducilos, Y.K. Vohra, A.L. Ruoff, Phys. Rev. B 41, 5372 (1990) 50. A.A. Kaminskii, A.V. Butashin, A.A. Demidovich et al., Phys. Status. Solidi. (a) 112, 197 (1989) 51. G.J. Huber, S.A. Payne, L.L. Chase et al., J. Lumin. 39, 259 (1988) 52. S.A. Payne, L.L. Chase, G.D. Whike, J. Lumin. 44, 167 (1989) 53. L.K. Smith, S.A. Payne, W.L Kway, et al., IEEE J. Quant. Elect. QE-28, 2612 (1992) 54. J.A. Caird, S.A. Payne, P.R. Stave, et al., IEEE J. Quant. Elect. QE-24, 1077 (1988) 55. K. Petermann, G.J. Huber, J. Lumin. 31–32, 71 (1984) 56. M. Yamaga, A. Marshall, K.P. O’Donnell et al., J. Lumin. 47, 65 (1990) 57. J.M. Chen, Z.D. Luo, A.D. Jiang, Chinese J. Lumin. 11, 104 (1990) 58. B. Henderson, A. Marshall, M. Yamaga, K.P. O’Donnell et al., J. Phys.: Solid State Phys. 21, 6187 (1988) 59. K.P. O’Donnell, A. Marshall, M. Yamaga, et al. J. Lumin. 1989, 42(365) (1990) 60. L.J. Andrews, A. Lempicki, B.C. McCollum et al., Phys. Rev. B 34, 2735 (1986) 61. K. Huang, J. Lumin. 31–32, 738 (1984) 62. F. Auzel, in Proceedings of the First International School on Excited States of Transition Elements ( World Scientiﬁc, Singapore, 1989)

Chapter 8

Non-radiative Transition Inside Ions

One of the important effects of lattice vibration on spectral properties of active ions is the emission or absorption of phonon between the electronic energy levels without the emission or absorption of photon. This is the so-called non-radiative transition. In this chapter, the non-radiative transition process discussed will not involve the energy transfer between ions which will be discussed in the next chapter. In solid-state laser materials, one of the non-radiative transition process is the transfer of an active ion energy to lattice vibration; thus its fluorescence efﬁciency is reduced, which can be expressed as gf ¼

Wr Wr þ Wnr

where Wnr refers to radiative transition probability and Wr denotes non-radiative transition probability. Obviously, a high non-radiative transition probability leads to low fluorescence efﬁciency. On the other hand, non-radiative transition is also a useful process for laser materials, because the active ions that transit from pump band to upper laser level and from lower laser level decay to ground state in a four-level system should rely on this process. There are extensive volume of papers and many monographs published dealing with this process since the 1950s, for example, the papers of Huang and Rhys [1], Perlin [2], Riseberg and Weber [3], Perlin and Kaminskii [4], Schuurmans and Dijk [5], Auzel [6], Hagston and Lowther [7], and Huang [8, 9] as well as monographs of Englman [10], Stoneham [11], and Fong [12]. Although many works in this area have been reported, the study of this high-order quantum process is still immature. We cannot give a detailed theoretical description on this process but can introduce some knowledge related to the spectroscopic properties of solid-state laser materials and focus on the study of weak electron–phonon coupling system such as rare earth ions in the materials. In principle, there is a process where the electron from a lower energy level transits to a higher energy level and absorbs energy from lattice system, but the © Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8_8

241

242

8 Non-radiative Transition Inside Ions

probability is very low especially when the energy separation between high and low energy levels is larger than that of a few phonons, so the probability can be neglected. In the language of thermodynamics, the process of energy transfer from electronic system with high order to lattice vibration system with low order is irreversible. The irreversibility is related to the increase of system entropy. In order to have a deep understanding about this problem, readers can refer to the book published by Fong [12], in which the relaxation processes including multi-phonon non-radiative process are dealt with by statistical theory. The book written by Englman [10] also discussed this problem. The process mentioned above is a multi-phonon one and will be dealt with by the same theoretical model as that adopted in Chap. 6, considering it as a lattice relaxation process excited by non-adiabatic interaction.

8.1

Introduction of Non-radiative Transition Matrix Elements

In the development process of non-radiative transition theory, three different methods have been adopted to calculate the matrix element of non-adiabatic operator, that is, Condon approximation, non-Condon approximation, and static coupling approximation. The calculation of some authors in earlier time has shown that the calculation result of non-Condon approximation is higher by 2–3 orders of magnitude than that of the Condon approximation. For the situation of single-frequency mode, the transition probabilities calculated by these two approximations differ by p2 times (p is the phonon number emitted in the transition). Thereafter, the calculation of static coupling approximation has also shown that its result is higher than that of the Condon approximation by several orders of magnitude. In 1980s, K. Huang [8, 9] analyzed different approximations in the calculation of non-radiative transition probability. P P By using only the non-diagonal 0 part of electron-phonon interaction HeL ¼ i6¼j j jih jjHeL jiihij while assuming a special adiabatic electronic wave function ui ð xÞ ¼ u0i ð xÞ þ

X i

Wi0

Wj0

h jjHeL jii u0 ð xÞ þ ðhijHeL jii h jjHeL j jiÞ j

a non-radiative transition matrix element the same as that of the static coupling theory was obtained [8]. Commutation rule of quantum mechanics had been used by the author [13] to transform the matrix elements of non-adiabatic operator in Condon approximation. In this way, a non-radiative transition matrix element the same as that of the static coupling theory also was obtained without assuming an explicit function expression of the electronic wave function at the beginning of discussion. This method will be described in the following.

8.1 Introduction of Non-radiative Transition Matrix Elements

243

The Hamiltonian of the electronic wave function can be expressed as follows He ¼ Te þ Vee þ Ven

ð8:1Þ

In the adiabatic approximation, the wave function of electron-phonon system can be expressed as w(r, R) = U(r, R)u(R), where U(r, R) is the electron wave function and u(R) is the phonon wave function. By using the Condon approximation, after expanding the electronic wave function to a power series of the amplitude R of lattice vibration, the terms of Rn with n 2 in the expansion expression can be neglected. Therefore, the ﬁrst term of the non-adiabatic operator of (6.6) is equal to zero. If Hnr denotes the non-adiabatic interaction, then its effect on the wave function can be written as Hnr Wðr; RÞ ¼

X h2 @ @ Uðr; RÞ uðRÞ @Ra Ma @Ra a

If one uses normal coordinates Q as that used in the literature [8, 9], then Hnr Wðr; QÞ ¼

X k

h2

@ Uðr; QÞ @Qk

@ uðQÞ @Qk

ð8:2Þ

where Wðr; QÞ ¼ Uðr; QÞuðQÞ, u(Q) is a continued product of vibrational wave functions corresponding to a series of normal vibrational modes. According to the golden rule in quantum mechanics, the transition probability can be expressed as Wnr ¼

X 2p 2 Av0 jhfmjHna jim0 ij d Eim0 Efm h m m

ð8:3Þ

The above formula has been summed over different ﬁnal vibrational states and averaged over different initial vibrational states. For the sake of simplicity, it is assumed that in the electronic initial state, the ions are populated in the zero vibrational state m′ = 0. If the ﬁnal state density complying with the law of energy conservation is q(E), then the non-radiative transition probability can be expressed as Wnr ¼

2p jhfmjHna ji0ij2 qðE Þ h

ð8:4Þ

It is necessary to further investigate the coordinate derivative of the electronic wave function before substituting the Hamiltonian of (8.2) into (8.4) and calculating the transition probability. Let

244

8 Non-radiative Transition Inside Ions

rQk Uðr; QÞ ¼

@ Uðr; QÞ @Qk

The electronic wave function U(r, Q) is an eigenfunction of He expressed by (8.1). The ﬁrst two terms of He involves only electronic coordinates and commute with rQk , therefore rQk ; He Ui ¼ rQk He Ui ðr; QÞ He rQk Ui ðr; QÞ ¼ rQk Ven Ui ðr; QÞ Ven rQk Ui ðr; QÞ ¼ ðrQk Ven ÞUi ðr; QÞ On the other hand He Uf ðr; QÞ ¼ Ef ðeÞUf ðr; QÞ; He Ui ðr; QÞ ¼ Ei ðeÞUi ðr; QÞ

ð8:5Þ

where Ef(e) and Ei(e) stand for the energy eigenvalues of the ﬁnal and the initial electronic states, respectively. Therefore

@

i ¼ f rQ Ven i f ½rQk ; He i ¼ Ei ðeÞ Ef ðeÞ f rQk i DEðeÞ f k @Qk and so

@ f @Q

k

@ i ¼ 1 f V en i DEðeÞ @Q

ð8:6Þ

k

where jii and hf j are the bra and ket of the initial and ﬁnal electronic wave functions, respectively and DE(e) = Ei(e) − Ef(e). The lattice wave functions satisfy the following equations HL uim0 ðQÞ ¼ Eim0 ð pÞuim0 ðQÞ; HL ufm ðQÞ ¼ Efm ð pÞufm ðQÞ

ð8:7Þ

where the lattice Hamiltonian is X 2 X 1 1 2 2 @ 2 2 h Pk þ x2k Q2k HL ¼ þ xk Qk 2 2 2 @Q k k k and Eim′(p) and Efm(p) are the eigenenergy of HL, that is, the energy of lattice system in the states im′ and fm. One can ﬁnd the following commutation relation in quantum mechanics [14] f ðPÞQ Qf ðPÞ ¼ ih

@ f ðP Þ @P

ð8:8Þ

8.1 Introduction of Non-radiative Transition Matrix Elements

If

P f ðPÞ TL ¼

k

245

P2k

2

Except TL, other terms in the lattice Hamiltonian HL commute with Q and so we have HL Qk Qk HL ¼ ih

@ @ f ¼ i hPk ¼ h2 @Pk @Qk

ð8:9Þ

Calculating the matrix element of operator (8.9) between initial and ﬁnal vibrational states and using (8.7), then

@

uim0 ðQÞ ¼ 1 DE ð pÞ ufm ðQÞjQk juim0 ðQÞ ufm ðQÞ ð8:10Þ 2 @Qk h where DE(p) = Efm(p) − Eim′(p) is the energy difference between ﬁnal and initial vibrational states. The d function in (8.3) requires that the process should keep the energy conservation, that is Ef ðeÞ þ Efm ð pÞ ¼ Ei ðeÞ þ Eim0 ð pÞ or DE ð pÞ ¼ DE ðeÞ Consequently, after substituting (8.6) and (8.10) into (8.2), one can obtain the following relation

X

Wfm ðr; QÞjHna jWim0 ðr; QÞ ¼ Wfm ðr; QÞrQk Ven Qk Wim0 ðr; QÞ ð8:11Þ k

where Wjn ðr; QÞ ¼ Uj ðr; QÞujn ðQÞ. Expanding Ven in terms of Qk, it can be obtained X @Ven X @ 2 Ven 0 Ven ¼ Ven þ Qk þ Q2k þ ð8:12Þ 2 @Q @Q k Q ¼0 k k k k Qk ¼0

Obviously, rQk Ven ¼ @Ven [email protected] jQk ¼0 , by (8.11) one has

+ X @Ven [email protected] jQk ¼0 Qk Wim0 ðr; QÞ Wfm ðr; QÞjHna jWim0 ðr; QÞ ¼ Wfm ðr; QÞ k

¼ Wfm ðr; QÞjHeL jWim0 ðr; QÞ

*

246

8 Non-radiative Transition Inside Ions

In the above matrix element, HeL ¼

P k

@Ven [email protected] jQk ¼0 Qk , it has the same expres-

sion as the HeL expression given by Kun Huang, in which @Ven [email protected] jQk ¼0 is equivalent to uk(x) in (3.2.1) of reference [9]. It is a function that depends only on the electronic coordinates. If the electronic wave function takes the zero approximation term in its expansion in terms of the vibrational coordinates, that is, it depends only on electronic coordinates, and then the result obtained is the same as that of the static coupling approximation

Uf ðrÞufin ðQÞjHeL ðQÞjUi ðrÞuim0 ðQÞ It shows that the simple way in the calculation of the non-radiative transition probability is to use commutation rule in quantum mechanics to transform the non-adiabatic operator at ﬁrst and then substitute the electronic wave function and electron–phonon interaction potential. In this procedure, it is impossible to underestimate the non-radiative transition probability, although the Condon approximation is adopted for the electronic wave functions. Peuker et al. [15] also showed that the non-radiative transition matrix element obtained by non-Condon approximation and static coupling approximation can also be obtained by Condon approximation.

8.2

Promoting Mode and Accepting Mode in Non-radiative Transition Process

A further expression for non-radiative transition probability can be obtained by (8.2) and (8.4) 2 2p X 2 k @ Wnr ¼ h Lfi ufm jui0 iG qðEÞ h k @Qk

ð8:13Þ

The concepts of accepting mode and promoting mode are introduced to describe different effects of the vibrational modes. The product of matrix elements Lkfi ¼

Uf ðr; Qk Þ@[email protected] jhUi ðr; Qk Þji and ufm [email protected][email protected] jui0 is not equal to zero in promoting mode and so it can stimulate the transition, which are labeled by index k. On the other hand, accepting mode cannot stimulate the transition but can receive energy in the non-radiative transition process. By the discussion in Chap. 6, because

Q of the lattice relaxation, the product of the overlap integral G ¼ k ufmk jui0k is non-zero. The factor G is called accepting mode factor and k is the index of accepting mode.

8.2 Promoting Mode and Accepting Mode in Non-radiative Transition Process

247

In (8.13), there is a transformation between normal coordinates Qk and lattice coordinates Rn

X @ i ¼ ð8:14Þ Lkf ¼ f Cnk hf jrRn jii @Qk n where Cnk is the transformation coefﬁcients between the matrix elements of lattice vibrational coordinates and those of normal coordinates. It should be noted that although (8.14) is a ﬁrst-order perturbation expression, the non-radiative transition probability is a small quantity of 2p-order Wnr ¼ O jHnr j2p This is due to the fact that, as pointed out by Englman [10], the wave functions have been “renormalized” by the lattice vibration and so G¼

Y ufnk ui0k i ¼ O jHnr jp1 k

Therefore, p phonon non-radiative transition is still a p-order quantum process. The vibrational wave function un of the nth excited state with phonon frequency xk (6.42) can be rewritten as un ¼

x 1=4 k

p h

1 1xk 2 pﬃﬃﬃﬃﬃﬃﬃﬃﬃ e2 h Qk Hn n 2 n!

rﬃﬃﬃﬃﬃﬃ xk Qk h

ð8:15Þ

By using (6.44), it is easy to show that in the condition of m = 1, Dk ! 0 (Sk ! 0),

/fm [email protected][email protected] j/i0 2 reaches its maximum value at xk/2 h. It shows that the promoting modes are those with Huang–Rhys factor Sk ! 0. However, Sk ! 0 means that the corresponding modes have a minimum value of @Ven [email protected] . The optical modes correspond to the vibrations in which the movement directions of opposite charge particles are opposite and the acoustic modes correspond to the vibrations in which the movement directions of opposite charge particles are the same. Obviously, the acoustic modes have the minimum variation of Ven and so the promoting modes should be acoustic modes. The non-radiative transition probability can be written as Wnr ¼ ph2

X 2 Lkfi xk G2 qðE Þ k

The summation is over all the promoting modes.

ð8:16Þ

248

8.3

8 Non-radiative Transition Inside Ions

Non-radiative Transition Probability for Weak Coupling Systems

By using overlap integral of lattice vibrational functions obtained in Chap. 6, it is easy to show that the accepting mode factor is G2 ¼ Sp1 eS =p1 !, where S is Huang-Rhys factor and p1 is the total phonon number that the accepting mode consumed, while the phonon number emitted in the non-radiative transition process is p = p1 + 1. If the frequencies of the promoting modes and the accepting modes are xk and xm, respectively, and the separation between two electronic energy level is DE, then p1 = (DE − hxk)/hxm. For multi-phonon non-radiative transition, p1 is a larger number and so by the Stirling approximation formula p1 ! ¼ pp11 ð2pp1 Þ1=2 expðp1 Þ, the following expression can be obtained "

# ph2 X k 2 S Wnr ¼ pﬃﬃﬃﬃﬃﬃ Lfi xk e qðE Þ expðp1 bÞ 2p k where

ð8:17Þ

p1 þ 1=2 DE hx k ln p1 ln S 1; p1 ¼ b¼ p1 hx m

Substituting the expression of b and p1 to (8.17), the expression known as exponential energy gap law of the non-radiative transition probability resulted as follows Wnr ¼ WexpðaDE Þ where

ð8:18Þ

"

# ph2 X k 2 xk S b a ¼ b=hxm ; W ¼ pﬃﬃﬃﬃﬃﬃ Lfi xk e qðE Þ exp xm; 2p k

b in the above formula is in fact a slow variation function of p1, and W and a are also not the constants. Therefore, (8.18) is only an approximate energy gap exponential relation of the transition probability. The relation between b and p1 can be tabulated as: S = 0.1, b(10)/b(2) = 1.71 2 3 P1 b 2.17 2.58 S = 0.2, b(10)/b(2) = 2.05 2 3 P1 b 1.48 1.89

4 2.86

5 3.07

6 3.2

7 3.39

8 3.51

9 3.62

10 3.72

4 2.17

5 2.38

6 2.5

7 2.76

8 2.82

9 2.93

10 3.03

8.3 Non-radiative Transition Probability for Weak Coupling Systems

249

It can be seen that only for the system with smaller value of S factor (weak coupling system), the assumption of constant b is reasonable. Therefore the exponential energy gap relation of non-radiative transition probability is only valid for the weak electron–phonon coupling system. Schuurmans et al. [5] modiﬁed the above relation to put all the variables depending on p1 into exponential function. Writing the total product of all the terms depending on p1 in (8.17) as exp½ðp1 1Þb0 then b0 ¼

2p1 þ 1 p1 p1 ln p1 ln S 2ð p1 1Þ p1 1 p1 1

ð8:19Þ

The detailed calculation shows that compared with the variation of b, b′ is a much slower function of p1 S = 0.1 2 p1 b′ 4.34 S = 0.2 2 p1 b′ 2.95

3 3.88

4 3.83

5 3.84

6 3.89

7 3.96

8 4.01

9 4.07

10 4.15

3 2.84

4 2.90

5 2.98

6 3.06

7 3.14

8 3.22

9 3.30

10 3.36

Note that b and b′ increase with p1. It means that the decrease of non-radiative transition probability is faster than that predicted by the exponential energy gap law. Suppose a0 ¼ b0 =hxm , then non-radiative transition probability has the following form Wnr ¼ W 0 exp½a0 ðDE hxk hx m Þ

ð8:20Þ

where "

ph2 X k 2 W ¼ pﬃﬃﬃﬃﬃﬃ Lfi xk eS qðEÞ 2p k

#

0

W′ is a quantity independent of p1 and DE, and a0 is substantially independent of DE. Therefore, (8.20) is a more accurate exponential relation of the non-radiative transition probability with the energy gap. It should be pointed out that the above formula has a bit difference from that given by Schuurmans et al. [5]. The effective energy gap in the above formula is DE minus one phonon energy of accepting mode and another of promoting mode instead of two phonon energies of accepting

250

8 Non-radiative Transition Inside Ions

modes. Generally, the phonon energy of accepting mode is different from that of promoting mode. However, as shown in (8.20), the high-energy acoustic phonons and the high-energy optical phonons both have greater contribution to the non-radiative transition, so long as Lkfi is non-zero. Equation (8.20) can be written in the form of (8.18), if one puts the factor of exp[a0 ðhxk þ hxm Þ] into W′. Nevertheless, the pre-exponential factor in (8.18) has a strong dependence on the host crystals. As pointed out by Schuurmans et al. [5], the pre-exponential factor in (8.18) can have a variation of 4–5 orders of magnitude for different host crystals or glasses doped with the same rare earth ions but the variation in the pre-exponential factor in (8.20) is within one order of magnitude. It should be pointed out that the Huang–Rhys factor S is dependent on the kinds of rare earth ions, although the difference of S factors is within a factor of two. Consequently, strictly speaking, the values of b′ and a′ for different kinds of rare earth ion in the same host are different. The above exponential energy gap law can be used to describe the transition probability of multi-phonon non-radiative process involving more than ﬁve phonons, although the demonstration is limited to the processes of 3–5 phonons. The reader can refer to the article published by Riserberg and Weber [3] to know more about this problem. It should be admitted that the multi-phonon non-radiative process is a complicated high-order quantum process and it is difﬁcult to describe all its characteristics by any one approximate theoretical method. In the description of the exponential energy gap law of non-radiative transition probability, the perturbation theory introduced by Hagston and Lowther [7] should be mentioned. According to their analysis, non-radiative transition resulted from the following electron–phonon interaction potential VeL ¼ V1 e þ V2 e2 þ Vn en þ

ð8:21Þ

where Vn ¼

@ n VeL @Qn

It should be noted that in this theory the zero-order electronic wave functions are the eigenfunctions of Hamiltonian that do not include VeL and the phonon wave functions are independent of the electronic states, that is, without lattice relaxation and non-adiabatic interaction. The contributions of p-order perturbation of ﬁrst-order term V1 and the ﬁrst-order perturbation of p-order term Vp to the probability of p phonon transition are compared [7]. Their results showed that the major contribution is due to the ﬁrst-order perturbation of p-order term and the transition probability takes the following form

8.3 Non-radiative Transition Probability for Weak Coupling Systems

Wnrp ¼

2p 2 f Vp i jhmjep jnij2 d Ei Ef phxeff h

251

ð8:22Þ

In this formula, hxeff is the effective phonon energy. Their calculation showed that the ratio of interaction matrix element of a p-phonon transition process to that of a (p − 1)-phonon transition process is varied in a small range, that is 2 aV b p 4 2 a Vp1 b In the following calculation this ratio is approximately assumed to be 3. Therefore, the ratio of transition probability of p-phonon process Wnrp to that of a (p − 1)-phonon transition process Wnrp1 can be approximately considered as a constant Rn ¼

Wnrp Wnrp1

2 aV b

hx D p e2 3 ¼ a Vp1 b 50qv5

ð8:23Þ

In the calculation of above formula, (6.29) for phonon state density (neglecting the difference between the velocities of transverse and longitude acoustic waves) and the strain expression of the linear combination of creation operator and annihilation operator have been used. The integral over phonon frequency is from 0 to Debye frequency xD. Obviously, the magnitude of Rn depends only on the variety of host materials. Consequently Wnrp ¼ Wnr0 Rn ¼ Wnr0 expðaDE Þ

ð8:24Þ

If one takes a ¼ ln R=hxeff , then a depends only on the type of host material. It must be pointed out that it is hard to see the approximate degree of the exponential law by this analysis; the problem is it is difﬁculty to estimate the error of transition probability introduced by assuming a constant ratio of 2 a V p b aVp1 b that is difﬁcult to be estimated. Using the density matrix method of statistical theory, Fong [12] introduced, in weak coupling condition, a formula for non-radiative transition probability as follows Wnr ¼ Aexp pcp

ð8:25Þ

where p = DE/hxk. The pre-exponential factor A is composed of the square of nÞ p matrix element [email protected][email protected] j f ij2 and the averaged phonon number factor ð1 þ while cp is a slow variation function of p cp ¼ ln

h io f 1 n f 1 f ð2 þ f Þ 2 ln ð f Þ 1 þ ð 1 þ f Þ ln þ ð8:26Þ =2 2p 2p p 2Lk g2k 4Lk g2k

252

8 Non-radiative Transition Inside Ions

where h i1=2 f ¼ ðp 3Þ þ ðp 1Þ2 þ 4 Similar to Huang–Rhys factor, Lkg2k is a quantity representing the strength of electron–phonon coupling. The strict energy gap exponential law requires that cp should be a constant. However, it can be seen from (8.26) and in the following table that cp is a slow variation function of p. Lkg2k = 0.04 p 3 c 1.68 Lkg2k = 0.02 p 3 c 2.14

4 2.27

5 2.80

6 3.02

7 3.29

8 3.51

9 3.69

10 3.85

15 4.44

4 2.79

5 3.25

6 3.60

7 3.88

8 4.11

9 4.31

10 4.48

15 5.09

Obviously, the result is the same as presented previously that the non-radiative transition probability increased faster than that predicted by the exponential law, when the energy gap narrows down. However, it has been pointed out by many review articles, for example Riseberg and Weber [3], that the exponential law is useful at least for the estimation of the orders of magnitude of non-radiative transition probability. Figure 8.1 is a typical example showing the relation of non-radiative transition probabilities versus energy gap for ﬁve laser crystals. The comparisons between experimental data and those of the calculated results given by Perlin and Kaminskii [4] for different rare earth ions in crystal YAP and YAG are shown in Fig. 8.2a, b. The following is some reference values for the parameters in (8.24) [16]. Host YAG YAP Y2O3 LiYF4 LaF3 SrF2 LaCl3

W0 (sec−1)

hxeff ðcm1 Þ

a (cm) 7

9.710 2.235108 5.0109 6.425109 2.7108 1.204108 3.5107 6.4107 6.6108 3.966109 3.1108 3.935108 1.51010 3.0081010

−3

3.110 3.510−3 4.610−3 4.6910−3 3.810−3 3.5310−3 3.810−3 3.610−3 5.610−3 6.4510−3 4.510−3 4.610−3 1.310−2 1.3710−2

700 700 550–600 600 430–550 600 400 560 350 305 360 350 260 250

Wnr (sec-1)

8.3 Non-radiative Transition Probability for Weak Coupling Systems

10

7

10

6

10

5

10

4

10

3

10

2

10

1

10

0

253

YAlO3 -1 (550-600cm )

LaCl 3 -1 (260cm )

Y2O3 -1 LaF3 (430-550cm ) -1 (350cm )

LaBr3 -1 (175cm ) 0

1000

2000 -1 ΔE (cm )

3000

4000

Fig. 8.1 Non-radiative transition probability versus energy gap for laser crystals of YAlO3, Y2O3, LaF3, LaCl3, and LaBr3 [3]

Fig. 8.2 a Non-radiative transition probabilities of a series of rare earth ions in crystal YAP at T ! 0 K; b non-radiative transition probabilities of a series of rare earth ions in crystal YAG at T!0K

254

8 Non-radiative Transition Inside Ions

The phonon energy of borate crystals or glasses reaches 1400 cm−1. Their non-radiative transition probabilities are much higher than those of other crystals and glasses. As an example, for YAl3(BO3)4 (YAB) crystal, W0 = 8.0 108 s−1, a = 2.110−3 cm, hxeff ¼ 1400 cm1 . These three parameters for four kinds of glasses are shown as follows [16]: W0 (sec−1) 5.41012 1.41012 3.4109 1.61010

Host Phosphate glass Silicate glass Germanate glass Fluoride glass

8.4

1200 h xeff (cm−1)

a (cm) 4.710−3 4.710−3 4.910−3 5.210−3

1100 900 500

Parallelism Between Non-radiative Transition Probability and Radiative Transition Probability

By using commutation formula equivalent to (8.8) f ðpÞr rf ðpÞ ¼ ih

@ f @p

p where f ðpÞ ¼ Te ¼ 2m , and the operator form of electronic momentum p, the following relation is obtained 2

Te r rTe ¼

h2 rr m e

ð8:27Þ

In the Hamiltonian He of (8.1), except Te, the other two terms are commuted with electronic coordinates. It is obvious from (8.27) that He

X i

rei

X i

rei He ¼

2 X h rrei m i

ð8:28Þ

and by using (8.5) and (8.28), the following formula resulted + + * * X X h2 f rei i ¼ rrei i f i mDEðeÞ i

ð8:29Þ

8.4 Parallelism Between Non-radiative Transition Probability …

255

rre and Te are differential operators and commute with each other. On the other hand, Vee has the following form X Vee ¼ V ðre re0 Þ e6¼e0

P P and commutes with e rre . Therefore, e rre commutes with the ﬁrst two terms in the expression of He. Similar to the introduction of (8.6), one has + + * * X X 1 f f rrei i ¼ rrei Ven i i DE ðeÞ i

ð8:30Þ

The interaction potential between any electron and any lattice ion can be expressed in the following general form Ven ¼ f ðrei Rn Þ

ð8:31Þ

The potential function in static electric model is the well-known Coulomb potential. By (8.31) rrei Ven ¼ rRn Ven Therefore, according to (8.6) in the form of lattice coordinate system and (8.30), we have + + * * X X ð8:32Þ f rrei i ¼ f r R n i i n By using (8.29) and (8.32), it can be shown that hfj

X n

rRn jii ¼

X X mDE ðeÞ mDE ðeÞ rei jii ¼ mei jii hfj hfj 2 2 h he i i

ð8:33Þ

where mei = erei is the dipole moment of electron i. The above formula can be written as hfj

X i

rRn jii ¼

mDEðeÞ M fi h2 e

ð8:34Þ

256

8 Non-radiative Transition Inside Ions

In the zero-order approximation it is assumed that the matrix element Mﬁ is independent of lattice coordinates. By (8.14) and (8.34), we obtain Lkfi ¼

X mDE n

h2 e

Cnk M fi

ð8:35Þ

Equation (8.35) shows that Lkfi is a linear combination of the dipole matrix element Mﬁ, therefore the relation between the non-radiative transition probability and the electric-dipole transition probability, which is proportional to the square of the Mﬁ, can be clearly obtained from (8.20) and (8.35). The ratio between these two transition probabilities will be given in the following. By means of (8.35), the pre-exponential factor in (8.20) can be related to radiative transition probability Wr [5] W 0 40

c3 Wr M1 DE

ð8:36Þ

where M1 is the mass of ligand ions of the rare earth ion. This relationship is sometimes called parallelism between the non-radiative and radiative transition probabilities. As early as the beginning of the 1980s, Ray and Chowdhury [17] had actually discussed this parallelism in a special problem of non-radiative transition excited by the ligands. They mentioned about one interesting situation that the rare earth ions are sited in the positions with central symmetry. In this situation the electric-dipole transition is forbidden and the above parallelism undoubtedly requires that the probability of non-radiative transition is also very small, thus ensuring that the related electronic states have a very long fluorescence lifetime. The energy transfer efﬁciency between Ho3+ ions and that between Ho3+ and Yb3+ or Sm3+ ions sited at central symmetry positions is as high as 99%. This is an indirect evidence of this parallelism. If the non-radiative transition probability is still high, it is impossible to provide the long-lived intermediate states to make an energy transfer with so high efﬁciency. This parallelism is also introduced in 1983 from another analysis by the author [18].

8.5 8.5.1

Temperature Dependence of Non-radiative Transition Probability in Weak Coupling Systems Experimental

Many luminescent materials can only emit at lower temperature but not at higher temperature. This is known as the thermal quenching of luminescence. The thermal quenching can be caused by the increase of the non-radiative transition probability

8.5 Temperature Dependence of Non-radiative Transition Probability …

257

of the electron in the active ion with the increase of temperature, and also can be caused by the increase of the electronic transition probability between the electronic state of active ion and the charge transfer state of the ligand after the temperature rises. Following this charge transfer, the electron will undergo a strong coupling non-radiative transition to another electronic state of active ion. The ﬁrst and the second kinds of thermal quenching involve the temperature dependence of non-radiative transition probability in weak coupling and strong coupling systems, respectively. The mechanism of the ﬁrst kind of thermal quenching will be addressed. Simply speaking, when temperature is raised, the electron–phonon interaction becomes stronger, thus the non-radiative transition probability Wnr is higher. For a deﬁnite luminescence system, the radiative transition probability Wr is independent of the temperature basically, therefore the fluorescence efﬁciency will become lower and even tend to zero when the temperature is raised. From the expression of overlapping integral of phonon wave function in Chap. 6, it can be seen that for rare earth ions, S 1. The overlapping integral of p − 1 accepting modes has the following relation G/

Sp1 ð1 þ nÞp1 ðp 1Þ!

The square mean of the matrix element ufm [email protected][email protected] jui0 of promoting mode includes a factor ð1 þ nÞ, therefore the non-radiative transition probability includes a factor ð1 þ nÞp . It can also be seen from (8.25) that the pre-exponential factor A includes a factor of ð1 þ nÞp . Obviously, the relation of the non-radiative transition probability with the temperature can be written as Wnr ðT Þ ¼ Wnr ð0Þð1 þ nÞ p

ð8:37Þ

where n ¼

1 expðhxeff =kT Þ 1

ð8:38Þ

This relation can be explained by the example of Nd3+:YAG system. The energy separation between 4F3/2 state and 4I15/2 state is about 5000 cm−1 and this crystal has effective phonon energy of about 700 cm−1, so the non-radiative transition is a 7-phonon process. According to (8.37), it is easy to obtain the following results: the non-radiative transition probability at 300 and 600 °C are three times and 11 times of that at the room temperature, respectively. At very high temperature, the

258

8 Non-radiative Transition Inside Ions

Fig. 8.3 Transition probability versus temperature for three different orders of multi-phonon process

90 80 70

(1+n)**p

60 p=7 50 40 30

5

20 3

10 0

0

100

200

300

400

500

T(K)

non-radiative transition probability is proportional to seven powers of the temperature. The thermal quenching is obvious. Figure 8.3 shows this relation for a series of different orders of multi-phonon process. The effective phonon energy hxeff is assumed as 250 cm−1.

8.6

Non-radiative Transition in Strong Coupling Systems

Strong electron-phonon coupling means Huang–Rhys factor S > 1. The transition metal group ions in materials belong to this case. The formulas introduced in previous sections with the assumption of S 1 are invalid in this situation. In order to obtain calculation formulas of the non-radiative transition probability, one can start with a phenomenological discussion by using conﬁguration coordinate curve. Because in the strong electron–phonon coupling case S > 1, the origins of the conﬁguration coordinates of potential curves for the excited state and that of the ground state have a considerable shift. Consequently, the two potential curves will have an intersect point (see Fig. 8.4). Suppose the energy difference between this intersect point and the zero-potential point of the excited state is DEe. When electronic energy reaches or exceeds DEe, the active ions will go from the excited state to the ground state. This is the most important non-radiative pathway in such a strong coupling system. The electrons populated in the excited state according to Boltzmann distribution law and the non-radiative transition probability can be expressed as Wnr ¼ Wnr0 expðDEe =kB T Þ

ð8:39Þ

8.6 Non-radiative Transition in Strong Coupling Systems

259

Fig. 8.4 Conﬁguration coordinate diagram for non-radiative transition

The process of having this form of transition probability expression is usually called a thermal activated process and DEe denotes the activation energy, which can be found in the following way. If the lowest energy point of the potential energy curve for the initial state i is at the conﬁguration coordinate Q = 0, assuming a single-phonon mode with phonon frequency , then the potential energy for the initial state can be written as Ei þ

1 hxi2 Q2 2

ð8:40Þ

The corresponding potential energy of the ﬁnal state f is Ef þ

1 hxi2 ðQ þ Dfi Þ2 2

ð8:41Þ

The above two energy curves intersect at the point with conﬁguration coordinates Q = Qc, then Qc ¼

Eif 12 hxi2 D2fi hxi2 Dfi

ð8:42Þ

260

8 Non-radiative Transition Inside Ions

Obviously, the activation energy DEe is 1 DEe ¼ hxi2 Q2c ¼ 2

2 Eif 12 hxi2 D2fi 2hxi2 D2fi

ð8:43Þ

According to the formula introduced in Chap. 6, in the case of single mode, we have 1 Shhxi ¼ hxi2 D2fi 2 Therefore, the activation energy can be expressed as

2 Eif Shhxi DEe ¼ 4Shhxi

ð8:44Þ

By the above simple discussion, the relation between the non-radiative transition probability and the energy gap as well as the temperature can be obtained, although it is impossible to know the detail about pre-exponential factor and in what condition this expression can be used. For a more sophisticated discussion, one should start with the general results given in the classical paper of Huang and Rhys [1]. When the phonon number in the initial state is non-zero, the overlap integral G consists of ﬁve terms: Gp+2, Gp+1, Gp, Gp−1, and Gp−2. Considering non-radiative transition between large energy gap in condition of larger Huang-Rhys factor, it can be assumed that the phonon-order in the above ﬁve terms are the same. Therefore Wnr ﬃ h2

X 2 1 1þ n p=2 h pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃi n þ Llfi Ip 2S nð n þ 1Þ exp½Sð1 þ 2nÞ 2 n l ð8:45Þ

Expanding the above Bessel function, then 1 X 2 X 1 ½Sð1 þ nÞk þ p l n þ ðS nÞk Wnr ¼ h Lfi exp½Sð1 þ 2nÞ k!ðk þ pÞ! 2 k¼0 l X 2 nð n þ 1Þ 1 ½Sð1 þ nÞp S2 n þ 1þ ¼ h2 Llfi þ exp½Sð1 þ 2nÞ p! pþ1 2 l 2

ð8:46Þ The relation of the non-radiative transition probability with the energy gap cannot be seen from this formula. The saddle point approximation will be used to introduce this relation in strong electron–phonon coupling situation. Generally, the non-radiative transition probability can be expressed as

8.6 Non-radiative Transition in Strong Coupling Systems

1 Wnr ¼ h

Zþ 1

f ðzÞegðzÞ dz

261

ð8:47Þ

1

where 1 X q f ðzÞ ¼ L Dfq þ Diq þ Difq cos zhxq þ icoth hxq hxq 2kB T sin z 2 q fi 1 X q 2 h coth hxq 2kB T cos z h xq þ Lfi hxq þ isin z 2 q xq

!2

ð8:48Þ and gðzÞ ¼ izDE q þ

X xk k

2h

D2ifk fcothðhxk =2kB T Þ½cosðzhxk Þ 1 þ isinðz hx k Þ g ð8:49Þ

where

DE q ¼

DE hxq DE þ hxq

where DE−q corresponds to the emission of a promoting phonon, while DE+q corresponds to the absorption of a promoting phonon. The right-hand side of (8.49) includes the factor of phonon frequency, which is obviously a large positive real number. Therefore, the right-hand side of (8.49) can be written as a large positive real number t multiplied by a function J(z), that is gðzÞ ¼ tJ ðzÞ Equation (8.47) is generally an integral of complex function and can be calculated approximately by saddle point method. It can be seen from the form of the function that (8.48) is a slowly varied function of z. By using saddle point method introduced by Irving and Mullineux [19] and taking into account that the probability is a positive number as well as the phase factor can be assumed a value of 1, the result of the integration is Wnr

1 2p 1=2 f ðz0 Þexp½gðz0 Þ h g00 ðz0 Þ

ð8:50Þ

where z0 is the so-called saddle point, and it satisﬁes the condition of the ﬁrst-order derivative with respect to z to be zero

262

8 Non-radiative Transition Inside Ions

g0 ð z 0 Þ ¼ 0

ð8:51Þ

The problem now is how to calculate saddle point z0 according to (8.51). By considering the case of strong electron–phonon coupling and expanding the cos(zhxk) and sin(zhxk) functions of (8.49) of z, the second term in the right-hand side can be written as Sð T Þ

E E X ð1Þn D X ð1Þn D ðhxÞ2n z2n þ iS ð hxÞ2n þ 1 z2n þ 1 T ð2nÞ! ð2n þ 1Þ! n1 n0

ð8:52Þ

where Sð T Þ ¼

X

Difk 2

k

x k cothðhxk =2kB0 T Þ 2h

i D E 1 X h 2 xk Difk hxk Þ2n ðhxÞ2n ¼ cothðhxk =2kB T Þ ð T Sð T Þ k 2h D

E 1 X h x i k ðhxÞ2n þ 1 ¼ D2ifk ð hxk Þ2n þ 1 S k 2h

ð8:53Þ

ð8:54Þ

ð8:55Þ

It can be shown [9] in high temperature strong coupling approximation, the terms with powers higher than z2 can be neglected, then the saddle point z0 calculated according to (8.51) leads to the following result DE q Shhxi D E z0 ¼ i SðT Þ ðhxÞ2 T

Obviously, at saddle point we have 92 8 DE < hhx qi S = D E i ðhxÞ2 z20 h : Scoth hhxi ; T 2kB T Therefore, when DE q hhxi S 1 hhxi Scoth 2k BT

ð8:56Þ

it is reasonable to neglect the terms higher than z2 in the expansion of (8.52). Inequality (8.56) corresponds to the criterion introduced by Lin et al. [20].

8.6 Non-radiative Transition in Strong Coupling Systems

263

At high temperature

therefore

kB T hxq

ð8:57Þ

coth hxq =2kB T 2kT= hxq

ð8:58Þ

Substituting it into (8.48) and (8.49) to obtain f(z0) and g(z0), and expanding f(z0) as a power series of T and keeping only linear term of T, then the results for f (z0) and g(z0) are 0

2 1 Lqfi X B C k T f ðz0 Þ @ 2 A B x q q

DE q Shhxi gðz0 Þ 4kB TShxi

ð8:59Þ

2 ð8:60Þ

In the introduction of (8.59) and (8.60), the terms with negative and zero powers of T are neglected, because T 1. According to (8.50), the non-radiative transition probability can be obtained 0 1 1=2 X Lq 2 fi C 1 p kT B Wnr expðDEe =kB T Þ @ 2 A h Shhxi x q q

ð8:61Þ

Transition probability can be written in this form, which means that the process is a thermal activation process with activation energy

2 DE q Shhxi DEe ¼ 4Shhxi

ð8:62Þ

Note that (8.61) has the same form as that of (8.39), while (8.62) is the same as (8.44). It means that the non-radiative transition in strong coupling system is a thermal activation process. However, it should be noted that the inequality (8.56) has to be satisﬁed. In multi-mode approximation, a similar formula can also be introduced. Freed and Jortner [21] introduced a formula for the calculation of the non-radiative transition probability; in this case Wnr ¼

rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ X q p C 0 xq coth hxq =2kB T expðDEe =kB T Þ ee 4ShhxikB T q

ð8:63Þ

264

8 Non-radiative Transition Inside Ions

where Cijq denotes the matrix element between electronic states i and j Cijq ¼ ihhij

@ j ji @Qq

ð8:64Þ

The summation in (8.63) should be over all the promoting mode q. The relation between effective temperature T* and the environment temperature T is T ¼

hhxi cothðhhxi=2kB T Þ 2kB

ð8:65Þ

where hxi denotes the averaged promoting mode frequency. At very high temperature, that is, T hhxi=2kB cothðhhxi=2kB T Þ ! 2kB T= hhxi then T T Niznan et al. [22] pointed out that this kind of Gaussian function relation between the non-radiative transition probability and the energy gap is only valid if the following condition is satisﬁed. DE=hhxi S

1 Scoth2 ðhhxi=2kB T Þ

ð8:66Þ

The meaning of high temperature and strong coupling can be seen from (8.58) and (8.56). Equation (8.56) shows that for different magnitude of energy gap, the requirement of strong coupling for Huang–Rhys factor is different. By the calculation of the Cr3+:Al2O3 system, this can be clearly seen. Assuming h = 250 cm−1, S = 7 [23], at a temperature higher than room temperature kT > 200 cm−1, (8.58) is roughly satisﬁed. For an energy gap of DE = 2500 cm−1, the left side of (8.56) is smaller than 0.18. The criterion for strong coupling is satisﬁed, but for a larger energy gap, for example DE = 5000 cm−1, the above criterion cannot be satisﬁed. Therefore, for the 4T2 ! 4A2 transition in ruby, the thermal activation relation cannot be satisﬁed at room temperature. Only at much higher temperature it is valid. However, the situations for the 4T2 ! 2E and 4T2 ! 2 T1 transitions are different. The experimental results obtained by Misu [24] showed the following relation at high temperature: Wnr ð4 T2 !2 T1 Þ ¼ 2:7 108 expðDEe =kT Þ; DEe ¼ 2200 cm1 Wnr ð4 T2 !2 EÞ ¼ 4:4 108 expðDEe =kT Þ; DEe ¼ 2600 cm1

8.6 Non-radiative Transition in Strong Coupling Systems

265

For the 2E ! 4A2 transition in ruby, because the potential energy curves of the two correlated electronic levels are basically parallel, the non-radiative transition between them cannot be described by the above strong coupling approximation.

8.7

Nonlinear Theory of Non-radiative Transition

The theory introduced previously is mainly based on the supposition that the expansion of the electron–phonon interaction Hamiltonian in terms of the strain keeping only the linear term is enough. This is the so-called linear theory of non-radiative transition. Perlin and Kaminskii [4] pointed out that this linear theory gives a too low transition probability for 3–6 multi-phonon non-radiative transition while by the nonlinear theory they obtained the results well compared with the experimental data. Orlovskii and Basiev et al. [25–28] applied nonlinear theory to the non-radiative transition of many laser crystals and obtained some valuable conclusions. Some of their conclusions on the relationship of the non-radiative transition rate with the structure and chemical composition of the host materials will be introduced in the following [28]. Their study shows that the non-radiative transition rate can be expressed as WNR ðJ ! J 0 Þ ¼

D 2 X 1 1 ð2J þ 1Þ1 ð2J 0 þ 1Þ Nk ð pÞ LSJ U ðkÞ L0 S0 J 0 i 137 k¼2;4;5 ð8:67Þ

2 p k k 2 Npc k ð pÞ ¼ g n =R0 ½ð2p þ 2k Þ!=ð2k þ 1Þ!p!ð2l þ 1Þ

l 0

l 0

k 0

2

Ze2s m hR20 ð8:68Þ

p Nex k ð pÞ ¼ g

l 1 Gs jSs j2 þ Gr jSr j2 þ Gp ck jSp j2 4ð2l þ 1Þ2p Ukp 137 0

l

k

0

0

2

Zc ðmR0 Þ2

ð8:69Þ g

h 8pcmMR20

ð8:70Þ

Equations (8.68) and (8.69) denote the contributions of the point charge Coulomb interaction and the exchange interaction to the non-radiative transition rates, respectively. In the above four formulas, p is the phonon number in non-radiative transition process, R0 denotes the separation between the active ion and its nearest neighbor anion and l = 3 for 4f electrons, m is the effective phonon frequency in the unit of wave number, n is the radius of rare earth ion, Z is the number of the anions

266

8 Non-radiative Transition Inside Ions

nearest to the RE ion, and M is the reduced mass of the anion and cation of host material. The contribution of Coulomb interaction to the non-radiative transition rate is 2 proportional to Z, e2 , and nk . On the other hand, it is inversely proportional to s

mp þ 1 , Mp, and R02k þ 2p þ 2 . The contribution of exchange interaction is composed of the overlap effect of 4f electronic wave function with the ligand wave function, the effect of ligand charge distribution on the Coulomb interaction, as well as the effect of charge transfer state. The non-radiative transition rate of exchange interaction is proportional to Z and the summation of the product G and S2, while inversely proportional þ2 , Mp, and m2p þ 2 . Crystal ﬁeld ﬁtting parameters G of fluoride and oxide to R2p 0 crystals are Gs = Gr = Gp ≅ 8–10. Lattice dynamics parameter g is affected greatly by the mass of lattice ions, and the orders of magnitude of g is in the range of 10−3–10−4 for fluoride and oxide crystals. The larger the reduced mass M of the lattice ions, the lower is the non-radiative transition rate WNR. The shorter the distance between the active ion and its nearest neighbor anion and the larger the radius of nearest neighbor anion leads to the higher the WNR. On the other hand, the higher the degree of electronic cloud overlapping, that is the larger covalent bond proportion, the higher is the WNR. Furthermore, by comparing the WNR expression given above and the expression of electric-dipole transition probability AR obtained by the J–O theory, it can be seen that both WNR and AR are proportional to the square of reduced matrix element of unit operator and it also demonstrates the parallelism between WNR and AR. The contribution of Coulomb interaction to the non-radiative transition rate depends largely on the radius of active ion. Some data of rare earth ions usually used in laser crystals are listed as follows (in atomic unit). Ion

2

n

4

n

6

n

Pr3+ Nd3+ Ho3+ Er3+ Tm3+

1.09 1.01 0.69 0.67 0.63

2.82 2.40 1.22 1.13 1.07

15.7 12.4 4.5 3.98 3.65

Nonlinear theory shows that the non-radiative transition rate WNR is different for the same active ion in different crystals as well as different active ions in the same crystal. In all the following transitions discussed, the contribution of k = 4 and k = 6 terms in (8.67) is much smaller than that of the k = 2 term because N4 and N6 are much smaller than N2 [28], so that it is enough only to compare the values of the reduced matrix element of U (2) for different transitions. The radius of Nd3+ ion is larger than that of Er3+ ion. The reduced matrix element U(2) for the 4G7/2 ! 4G5/2 + 2G8/2 transition of Nd3+ ion and that for the 4F5/2 ! 4F7/2 transition of Er3+ ion is nearly the

8.7 Nonlinear Theory of Non-radiative Transition

267

same. In LaF3 crystal both the transitions belong to a 4-phonon process but the non-radiative transition rate WNR of the former is about six times that of the latter. The radius of Pr3+ ion is larger than that of Ho3+ ion. The reduced matrix element U(2) for the 1G4 ! 3F4 transition of Pr3+ ion is nearly the same as that of the 5I5 ! 5I6 transition of Ho3+ ion. In YLF crystal both the transitions belong to a 5-phonon process but the non-radiative transition rate WNR of the former is about 2.6 times of the latter. The radius of Er3+ ion is a little larger than that of Tm3+ ion. The reduced matrix element of U(2) for the 3F5/2 ! 3F7/2 transition of Er3+ ion is equal to that for the 3F3 ! 3H4 transition of Tm3+ ion, but the non-radiative transition rate WNR of the former is about 1.5 times of the latter. The effect of the radius of active ion on the non-radiative transition rate is mainly due to the fact that Coulomb and exchange interactions are stronger for larger active ion radius. The effect of Coulomb interaction is reflected by the average square of nk in (8.68), while the effect of exchange interaction is reflected by the overlap parameters. If the lattice dynamics parameter g is larger, the combined effect of g and the radius n makes the difference of non-radiative transition rate WNR more obvious. For the LaF3 crystal, m = 400 cm−1, R0 = 2.5 Å, M = 2.2810−23g while for the YLF, m = 560 cm−1, R0 = 2.27 Å, M = 2.6010−23g. Calculating by (8.70), the g value of the former is larger than the latter by a ratio of 2.1, in addition that the radius of Nd3+ ion is larger than that of the Tm3+ ion. Therefore, for the same 4-phonon transition process, the WNR of the 4G7/2 ! 4G5/2 + 2G7/2 transition of Nd3+:LaF3 crystal is 4.5 times that of the 3H5 ! 3F4 transition of Tm3+:YLF crystal, although the ratio of the square reduced matrix element U(2) for the former to that of the latter is 6/9. The square reduced matrix element of U(2) for the 4G7/2 + 2K13/2 ! 4 G5/2 + 2G7/2 transition of Nd3+ ion is 0.0583 while that for the 4D3/2 ! 2P3/2 transition is 0.0118, that is, the former is 4.9 times of the latter. In Nd3+:YAG crystal the non-radiative transition rate of the former is 5.9 times that of the latter. The lattice dynamics parameter g is proportional to the mean square of lattice vibration amplitude; therefore if the melting point of the crystal is lower or the hardness of the crystal is lower, the lattice vibration amplitude will be larger at the same temperature, then the non-radiative transition rate of active ion in this crystal generally will be higher, when the other factors are similar. Non-radiative transition rate decreases with the increase of the distance between the active ion and its ligands. Following is the non-radiative transition rate WNR for the 3P0 ! 1D2 transition of Pr3+ ion in four different crystals. Comparing the Pr3+ ion substituting for La3+ ion with that substituting for Y3+ ion, the radius of La3+ ion larger than that of the Y3+ ion results in the distance between the Pr3+ ion and its nearest neighbor O2+ ion larger for the former than that for the latter. Therefore in the following table, the non-radiative transition rate of the ﬁrst crystal is lower than that of the second crystal, while the third crystal is lower than that of the fourth crystal.

268

8 Non-radiative Transition Inside Ions

Crystal

DE (cm−1)

hxmax ðcm1 Þ

n

WNR (s−1)

LaNbO4 YNbO4 Na5La(WO4)4 Na5Y(WO4)4

3500 3500 3740 3720

810 830 960 960

4.32 4.16 3.896 3.875

4.5104 2.2106 6.0104 1.0105

For the non-radiative transition process emitting phonon number p > 6, the non-radiative transition rate obtained by nonlinear theory is still lower than the experimental result; moreover, the deviation between the calculated values and the experimental data will increase with p.

8.8

Stimulated Non-radiative Transition

According to the aforementioned theory of non-radiative transition, by a simple calculation, it can be seen that in the four-level high power continuous laser, the stimulated radiative transition (SRT) probability between upper and lower laser levels is much higher than the decay rate from the lower laser level to the ground state. The continuous Nd3+:YAG laser can be used as an example to illustrate this problem. It is well known that the photon number in the laser cavity can be calculated by the following expression nk ¼

2Lc Pout ccout hmk

ð8:71Þ

where Pout is laser output power, Lc is the length of laser cavity, and cout is loss per pass due to the mirror transmission. The laser wavelength of Nd3+:YAG crystal is kk =1.064 lm (emission generated by the transition of R2 ! Y3, that is, from energy level R2 of multiplet 4F3/2 to energy level Y3 of multiplet 4I11/2) and the frequency of laser is mk 2.81014 s−1. Its multi-mode oscillation linewidth is in the range of 15–30 K GHz [29]. Suppose it is 20 K GHz, then Dmk 21010 s−1. When laser output power reaches 10 W 51023 cm−1s−1 (energy in the unit of wave number), and suppose the length of cavity is Lc = 20 cm, the loss per pass cout = 0.2 and that the photon number is nk 3.61011. Suppose the shape of laser spectral line is Lorenz type, then the relation of the spontaneous transition probability AR2Y3 with the stimulated emission cross-section rem is [30] AR2Y3 ¼

4p2 n2 Dmrem k2

ð8:72Þ

Using the data of stimulated emission cross-section rem = 6.5 10−19 cm2 for laser transition R2 ! Y3 [30], AR2Y3 1.5102 s−1 can be obtained. The SRT

8.8 Stimulated Non-radiative Transition

269

probability of R2 ! Y3 transition will be nkAR2Y3, and it reaches 5.4 1013 s−1. However, according to the experimental result [16], the non-radiative transition probability of 4I11/2 ! 4I9/2 at room temperature is 1010 s−1 orders of magnitude at most (taking account of the nonlinear mechanism, the theoretical calculation value can only reach 1.6 1010 s−1 [16]). It means that when the output power of Nd3+: YAG laser reaches P = 10 W, the SRT probability of 4F3/2 ! 4I11/2 transition is far outweighing the non-radiative transition probability of 4I11/2 ! 4I9/2. In this case, the particles in the low laser level cannot be removed in time, so that the population inversion of the upper and the lower laser levels cannot be maintained and the bottleneck effect is inevitable. However, as it is well known, the output power of continuous Nd3+:YAG laser has reached the scale of kilowatt nowadays, but no bottleneck effect appeared. Obviously, the experimental fact can only be explained by a new non-radiative transition mechanism excited by the laser itself. In the following it will be demonstrated that the mechanism proposed by the author [31, 34] referred to as stimulated non-radiative transition (SNT), can well explain the related phenomenon. The starting point to solve this problem is to deal with the photon–electron– phonon system as a whole and write the Hamiltonian of the system as H ¼ He þ Hr þ Hl þ Her þ Hel

ð8:73Þ

where He, Hr, and Hl express the Hamiltonians of electron, photon, and phonon, respectively, Her is the Hamiltonian of photon–electron interaction, and Hel is the Hamiltonian of electron–phonon interaction. As being shown in Chap. 4, in dipole approximation, Her can be written as Her ¼

e e X 2ph 1=2 ikr þ pA¼ e a ð kÞ p a þ aka ðtÞeikr ka ðtÞe mc m ka Vxk e

ð8:74Þ

Suppose there are N phonon modes Qi, so that Hel is 1 X @V Hel ¼ pﬃﬃﬃﬃ Qi N i @Qi

ð8:75Þ

The transition between electronic energy levels corresponds to the absorption or emission in the wavelength range of ultraviolet–visible–near infrared. Suppose the photon and the phonon has no direct interaction, so that the term to describe its interaction is not included in (8.73). If there are nk photons in the electromagnetic ﬁeld, the wave function of electron– photon system can be written as j/ik i ¼ jwi ijnk i

ð8:76Þ

where |w > is electronic wave function and |nk > is photon wave function. Phonon system can be regarded as slow system compared with photon-electron system.

270

8 Non-radiative Transition Inside Ions

Similar to the adiabatic approximation in lattice relaxation theory, the initial state wave function of photon-electron-phonon system can be expressed as jUikk i ¼ jwi ijnk ijuik i

ð8:77Þ

By the single-mode approximation of the radiation ﬁeld and phonon ﬁeld, the zero-order eigenvalue of initial photon–electron–phonon system is expressed as Eikk

1 1 ¼ Ei þ nk þ hxk þ nk þ hx k 2 2

ð8:78Þ

The perturbation of non-diagonal matrix elements of interaction Hamiltonian Her and Hel induce the radiative transition, non-radiative transition, and light scattering processes. SNT is a process induced by the following second-order perturbation matrix element of Her ð2Þ Mif

X hUikk jHer jUvk1 k i Uvk1 k jHer jUfk1 k1 ¼ Eikk Evk1 k þ id vk k

ð8:79Þ

1

In this process, the electron excited by the photon transits from the most probable phonon state k of the initial electronic state i to the same phonon state k of the intermediate electronic state m and stimulated by the photon transiting simultaneously to the ﬁnal phonon excited state k1 of ﬁnal electronic state f. In this process, the electronic system undergoes a non-radiative transition of i ! f, the phonon system absorbs the energy emitted by the electron, while the photon system completed a virtual process without energy variation. The initial electronic state i, the intermediate electronic state m, and ﬁnal the electronic state f discussed here are the crystal ﬁeld energy levels 4I11/2, 4F3/2, and 4I9/2 multiplets of Nd3+ ion, respectively. The energy of electron and phonon satisﬁes the following relations hxk p hx k DEif ¼ Ei Ef [ 0; nk1 [ nk ; Ei Ef ¼ ðnk1 nk Þ In (8.79) d is the linewidth of laser beam in the unit of energy. When the photon energy hxk satisﬁes the resonance condition Eikk Emk1 k ¼ Ei þ hxk Em ¼ 0, this process has practical physical meaning. In order to introduce expression of the transition probability, suppose the N phonon modes which interacted with electronic system have the same frequency xk and the radiation ﬁeld also has one mode xk, the initial photon wave function can be written as jni i ¼ jn1 ; n2 ; . . .; nk ; . . .i

ð8:80Þ

On the other hand, the photon wave functions of the intermediate and the ﬁnal states are

8.8 Stimulated Non-radiative Transition

271

jnm i ¼ jn1 ; n2 ; . . .; nk 1; . . .i;

nf ¼ jn1 ; n2 ; . . .; nk ; . . .i

ð8:81Þ

According to the golden rule of quantum mechanics, similar to the deducing method of Heitler [32], the transition probability of this process can be expressed as W SNT ¼

2p h

Z ð 2Þ 2 Mif q Ef dEf

ð8:82Þ

Considering that the ﬁnal state is an electronic discrete stationary state but a photon–phonon composed continuum, the product of ﬁnal state density q(Ef)dEf can be expressed as q Ef dEf ¼ qðEk ÞqðEk0 Þd Eif p hxk0 dEk dEk0 1 ¼ qðxk Þqðxk0 Þdðxk0 xk =pÞdxk dxk0 h In the above deduction, the following relations are used 1 xk ¼ Eif =h; xk ¼ xk =p d Eif phxk0 ¼ dðxk0 xk =pÞ h Substituting these expressions to (8.82) and integrating over xk′, the probability of SNT can be expressed as follows Z 2p ð2Þ 2 ð8:83Þ W SNT ¼ 2 qðxk Þ Mif qðxk Þdxk h In virtue of linewidth Dxk of the laser beam is very narrow, the above expression is approximately equal to W SNT

2p ð2Þ 2 M qðxk ÞDxk qðxk Þ h2 if

ð8:84Þ

The state density q(xk) of ﬁnal photon state can be calculated by (4.15) of Chap. 4, which is rewritten in the following qðxk Þ ¼

Vx2k dXk 8p3 c3

ð8:85Þ

The accepting mode of the non-radiative transition is optical mode, q(xk) is the state density of optical phonon mode, which is a quantity related to the crystal structure and the magnitude of wave vector k and has not a simple analytic expression. The matrix element of (8.79) can be expressed as

272

8 Non-radiative Transition Inside Ions

hUikk jHer jUmk1 k i ¼ hwi jhnk jHer jnk 1ijwm ihuik jumk i

hUmk1 k jHer Ufkk1 ¼ hwm jhnk 1jHer jnk iwf humk juf k1

ð8:86aÞ ð8:86bÞ

Integrating the above transition matrix elements over the photon wave function at ﬁrst and then referring to the (4.16) and (4.17) and the Poisson equation of quantum mechanics used in the derivation of (4.19) and (4.20), the transition matrix element for the photon-stimulated absorption process in electric dipole approximation can be obtained as hwi jHer jwm ihuik jumk1

2phxk nk ¼ Ve

1=2 * X + w i e r w huik jumk i j j m

ð8:87aÞ

For photon-stimulated emission the transition matrix element is 1=2 * X +

2p h x n k k w m e rj wf humk juf k1 hwm jHer wf humk juf k1 ¼ j Ve

ð8:87bÞ

For the special process considered here, only one intermediate state satisfy the condition of Eikk Emk1 k ¼ 0 and remember that the initial phonon state is the same as the phonon state of the intermediate electronic state, juik i ¼ jumk i, huik jumk i ¼ 1 and so the square of matrix element in (8.79) can be expressed as

ð2Þ

Mif

2

2 Mim2 Mmf2 huik juf k1 =d2

Because uk ¼

Y

uks

s

huik juf k 2 can be referred to as lattice relaxation factor flr having an expression 1 the same as (6.47) of Chap. 6.

2 Sp flr ¼ huik juf k1 ¼ eS p! where S is Huang–Rhys factor of the crystal, so that the probability of SNT is

8.8 Stimulated Non-radiative Transition

273

2p 2 2 M M qðxk Þqðxk ÞDxk flr =d2 h2 im mf * X +2 2phxk nk 2 Mim ¼ r w w i e j j m Ve * X +2 2phxk nk 2 Mmf ¼ r w wm e j j f Ve W SNT

By using the stimulated absorption transition probability from initial state to intermediate state WimSRT ¼

2p jMim j2 qðxk Þ h2

and the spontaneous emission transition probability from intermediate state to ﬁnal state is Amf ¼

2p 2 Mmf qðxk Þ=nk h2

Therefore, the SNT probability is expressed as

h2 Dxk qðxk Þ W flr rnk Amf Wimsrt 2pd2 qðxk Þ 2 h Dxk qðxk Þ h qðxk Þ r¼ ¼ flr f lr 2pd qðxk Þ 2pd2 qðxk Þ SNT

nk Amf WimSRT

ð8:88Þ

In the above expression d ¼ hDxk has been used. The Huang–Rhys factor S is generally in the order of magnitude 10−2–10−1 for rare earth ions in crystals, and in YAG crystal, it can supposed to be 0.05. At room temperature, the minimum energy separation between the crystal energy level Y3 of 4I11/2 and the crystal energy level X3 of 4I9/2 is about 2000 cm−1 [16] and the effective phonon energy of YAG crystal is about 700 cm−1. The phonon number in (8.80) can be taken as p = 3, therefore, flr = 2 10−5. On the other hand, by using Dmk 21010 s−1, d 0.7 cm−1 and h=2pd ¼ 1:2 1012 s, it can be obtained that r = 2.610−17(q(xk)/q(xk)) s. According to the ratio of fluorescence branch ratios of R2 ! Y3 transition to R2 ! X3 (Z3) transition being 0.125/0.054 and A(R2 ! Y3) 1.5102 s−1, it can be estimated that A(R2 ! X3) 65 s−1. Substituting it into (8.88), the following expression resulted

274

8 Non-radiative Transition Inside Ions

W SNT 4 I11=2 ! 4 I9=2 6 105 ðqðxk Þ=qðxk ÞÞW SRT ðR2 ! Y Þ

ð8:89Þ

The calculation of the density q(xk) of optical phonon mode for YAG crystal is a problem to be studied, however, owing to the fact that the phonon velocity is much less than that of the photon, without doubt the density q(xk) of optical phonon mode has more than 5 orders of magnitude higher than that of the photon mode density q(xk). Therefore, when laser power reaches 10 W, it can be seen that W SNT 4 I11=2 ! 4 I9=2 W SRT ðR2 ! Y3 Þ That is, the probability of SNT from the lower laser level to the ground state is much higher than that of SRT from upper laser level to lower laser level. For lasers with higher output power, the multiple of the SNT probability higher than that of the SRT will be increased, and the bottleneck effect will never happen.

References 1. K. Huang, A. Rhys, Proc. Roy. Soc. A204, 406 (1950) 2. Yu.E. Perlin, Uspekli ﬁz. Nauk 80, 553 (1963) 3. L.A. Riserberg, M.J. Wiber, in Progress in Optics, ed. by E. Wolf, vol. XIV (North- Holland Publ. Co., Amsterdam, 1976) 4. Yu.E. Perlin, A.A. Kaminskii, Phys. Stat. Sol. (B) 132, 11 (1985) 5. M.F.H. Schuumams, J.M.F. van Dijk, Phys. B 123, 131 (1984) 6. F. Auzel, in Advances in Nonradiative Processes in Solids, ed. by B. Di Bartolo (Plenum Press, New York, 1991) 7. W.E. Hagston, J.E. Lowther, Physica 70, 40 (1973) 8. H. Kun, Scientia Sinica, XXIV, 27 (1981) 9. Huang Kun, Phys. Prog. 1, 31 (1981). (in Chinese) 10. R. Englman, in Radiationless Decay of Ions and Molecules in Solids (North-Holland, 1979) 11. A.M. Stoneham, The Theory of Defects in Solids (Clarendon Press, Oxford, 1975) 12. F.K. Hong, Theory of Molecular Relaxation: Application in Chemistry and Biology (Wiley-Interscience, New York, 1975) 13. Z.D. Luo, Chin. J. Lumin. 20, 1 (1999) 14. L.D. Landau, E.M. Lifshitz, Quantum Mechanism (Pergamon Press, Oxford, 1958) 15. K. Peuker, R. Enderlein, A. Schenk, E. Gutsche, Phys. Stat. Sol. B 109, 599 (1982) 16. A. A. Kaminskii, Crystalline Lasers: Physical Processes and Operating Schemes (CRC Press, Boca Raton, 1996) 17. D.S. Ray, M. Chowdhury, Chem. Phys. 61, 157 (1981) 18. Z.D. Luo, Chem. Phys. Lett. 94, 498 (1983) 19. J. Irving, N. Mullineux, Mathematics in Physics and Engineering (Academic Press Inc., New York, 1959) 20. S.H. Lin, H.P. Lin, D. Knittel, J. Chem. Phys. 64, 441 (1975) 21. K.F. Freed, J. Jortner, J. Chem. Phys. 52, 6272 (1970) 22. B. Nitznan, S. Mukamel, J. Jortner, J. Chem. Phys. 63, 200 (1975) 23. B. Henderson, G.F. Imbusch, Optical Spectroscopy of Inorganic Solids (Clarendon Press, Oxford, 1989) 24. Misu, J. Phys. Soc. Japan, 19, 2260 (1964)

References 25. 26. 27. 28. 29. 30. 31.

32. 33. 34.

275

YuV Orlovskii, K.K. Pukhov, T.T. Basiev et al., Opt. Mater. 4, 583 (1995) T.T. Basiev, YuV Orlovskii, K.K. Pukhov et al., Laser Phys. 8, 1139 (1998) K.K. Pukhov, T.T. Basiev, Yu.V. Orlovskii, et al., J. Lumin. 76/77, 586 (1998) T.T. Basiev, Yu.V. Orlovskii, K.K. Pukhov et al., J. Lumin. 68, 241 (1996) J.E. Geusic, IEEE J. Quant. Elect. 2: Digest of Tech. Paper, in 1966 International Quantum Electronics Conference, Apr 1966 W. Koechner, in Solid-State Laser Engineering (Springer, 1976) Z.D. Luo, in Proceedings of the First International School on Excited States of Transition Elements, ed. by B. Jezowska-Trzebiatowska, J. Legendziewicz, W. Strek (World Scientiﬁc, Singapore, 1989) W. Heitler, The Quantum Theory of Radiation (Clarendon Press, Oxford, 1954) J. Calloway, Quantum Theory of the Solid State (Academic Press, New York, 1976) Z.D. Luo, Phys. Stat. Sol. b 133, K77 (1986)

Chapter 9

Energy Transfer and Migration Between Ions

In the previous discussion on the absorption and emission of light, all processes take place in a single active center. In fact, other centers in the medium contribution to the absorption and emission of a single active center. It involves the physical processes of energy transfer and migration, which are very important in the study of laser materials. After absorbing excitation energy, the electrons in luminescent center transit to excited states, then the excitation energy can be consumed usually by light emission or transferred to thermal energy of lattice vibration. However, part of the excitation energy can be transferred from one center to other centers. Basically, there are three kinds of centers in laser materials, that is, active center (activator), sensitized center (sensitizer), and quenching center. The activator is luminescent center in the materials. The sensitizer is deﬁned as the center used to absorb excitation energy then transfer it to the activator, whereas the quenching center only consumes the excitation energy being transferred to it. Certainly, ion, group, or molecule of host material can also act as a sensitizer to transfer absorbed excitation energy to activator. This is called as host sensitization. Usually, the energy exchange between sensitizers or activators is deﬁned as energy migration, while the energy exchange between sensitizer and activator is deﬁned as energy transfer. We will discuss these two processes but does not involve electric charge migration. The energy transfer and migration discussed are the results of electric multi-pole, magnetic dipole, or exchange interactions. As early as 1940s, Forster [1, 2] developed the theory of dipole-electric interaction and Dexter [3] further generalized it to include high-order multi-pole and exchange interactions in 1950s. Orbach [4], Miyakawa and Dexter [5] extended the theory to include phonon-assisted transfer. With the rapid development in the ﬁeld of laser and fluorescent materials, especially the development of powerful laser spectroscopy (time-resolved spectroscopy, selection excitation spectroscopy, fluorescence narrowing spectroscopy, and so on.), many micro processes including many ultrafast processes in the material can be observed in depth and concretely. All of these stimulate the research interest in the area of energy transfer and make it has a great progress. In this chapter, some basic © Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8_9

277

278

9

Energy Transfer and Migration Between Ions

theoretical knowledge of this ﬁeld closely related to the spectroscopic properties of solid-state laser material will be introduced. There is a very extensive volume of literature published, which the reader can directly refer to. Among these, the review articles written by Auzel [6–8], Blasse [9, 10], Yen [11], and Holstein [12] are worthy to be read to obtain a general idea about the development in this ﬁeld.

9.1

Theory of Resonant Energy Transfer

There are several types of energy transfer between active ions: Radiation reabsorption (the radiation trapping effect mentioned earlier), photoconductivity, exciton migration, and non-radiative resonance energy transfer. The following discussion is about non-radiative resonance energy transfer, in which the light transition is a virtual process. Only two-body interaction is to be dealt with, although there are three-body and even many-body interactions in fact. Phonon-assisted energy transfer and energy migration will be introduced later. Assume that in the initial state i, there is a sensitizer (S) in excited state while a nearby activator (A) is in ground state. In the ﬁnal state f, S goes down to ground state, while A goes up to excited state (as shown in Fig. 9.1). This process is introduced by a series of interactions between ions. One should ﬁrst examine their interaction Hamiltonian. Hamiltonian H of the system can be divided into two parts, H0 of the single ion and Hsa of the interaction between two ions, expressed as H ¼ H0 þ Hsa

ð9:1Þ

Hsa (excluding exchange interaction temporarily) is Hsa ¼

e2 ejRsa rs þ ra j

ð9:2Þ

where Rsa is the distance vector between two nuclei, rs and ra are the electronic coordinates of S and A, respectively. e is the dielectric constant of the material. Expanding (9.2) in terms of Rsa, then

Fig. 9.1 Schematic diagram for resonant energy transfer between ions

S

A

9.1 Theory of Resonant Energy Transfer

279

edd edq eqd eqq mdd Hsa ¼ Hsa þ Hsa þ Hsa þ Hsa þ Hsa þ

ð9:3Þ

where the ﬁrst term is the electric dipole–dipole interaction expressed as edd Hsa ¼

a 1 3 s s a m m m m R R sa sa ed ed ed eR3sa R2sa ed

ð9:4Þ

msed and maed denote the electric dipole of S and A, respectively. The other terms in (9.3) are the Hamiltonians of electric dipole–quadrupole, electric quadrupole– quadrupole, and magnetic dipole–dipole interactions. Hsa usually can be expanded as X e2 Hsa ¼ ð9:5Þ Cqðk11qk22 Þ Dðqk11 Þ ðrs ÞDðqk22 Þ ðra Þ k1 þ k2 þ 1 eR k k q q 1 2 1 2

Multi-pole moment in the above expression is DðkÞ q ðrÞ

X 4p 1=2 ¼ rmðkÞ Ykq ðhi ; ui Þ 2k þ 1 i

ð9:6Þ

It is summed over all the electrons in S or A and Cqðk11qk22 Þ ¼ ð1Þk1

4pð2k1 þ 2k2 Þ! 1=2 k1 q1 ð2k1 Þ!ð2k2 Þ!

k2 q2

k1 þ k2 q1 q2

Yk1 þ k2 q1 þ q2 ðh; uÞ ð9:7Þ

The ﬁrst term in (9.3), that is, the (9.4), corresponds to the case k1 = k2 = 1. The second term corresponds to k1 = 1, k2 = 2, the third term corresponds to k1 = 2, k2 = 1, the fourth term corresponds to k1 = 2, k2 = 2, and so on. The wave function of the initial state is |W(rs, ae; ra, ag)〉 and that for the ﬁnal state is |W(rs, ag; ra, ae)〉. a refers to the electronic states. Consequently, the probability of energy transfer becomes W¼

2 2p W rs ; ae ; ra ; ag jHsa jW rs ; ag ; ra ; ae q Ef d Ef Ei h

ð9:8Þ

A detail expression for the energy transfer probability of electric dipole–dipole interaction can be introduced as follows. Let’s focus on the energy transfer between one S and one A. By excluding the exchange interaction between these two ions, the zero-order wave function can be expressed as a product of the wave functions of these two ions, that is

280

9

Energy Transfer and Migration Between Ions

W rs ; ai ; ra ; aj ¼ Wðrs ; ai ÞW ra ; aj

ð9:9Þ

Owing to the fact that the direction of electric dipole is arbitrary in the space, substituting (9.4) into (9.8), the following scalar products should be averaged over c, c1, and c2, that is, the angles between ra and rs, rs and Rsa , and ra and Rsa , respectively msed maed ¼ msed maed cosc; msed Rsa ¼ msed Rsa cosc1 ; maed Rsa ¼ maed Rsa cos c2 It is easy to obtain 1 4p

Z

1 1 cos cdX ¼ ; 3 4p 2

Z

1 coscdX ¼ 0; 4p

Z sincdX ¼ 0

ð9:10Þ

The results for the average over c1 and c2 are the same. The average square of (9.4) consists of three terms and by using (9.10) it can be shown that the sum of the ﬁrst and the third term is equal to (4e4/3)|〈rs〉|2|〈ra〉|2. The calculation of the second term involves the relationship between three vectors and the angles c1, c2, and c. The scalar products of ra with rs, rs with Rsa and ra with Rsa can be calculated by using a spherical coordinate system with Rsa acting as a polar axis. In this way one has c = c1 − c2. The calculation result of this second term is −(2e4/3)|〈rs〉|2|〈ra〉|2. Therefore * + 4 s 2 2e m ma 3 ms Rsa ma Rsa ¼ jhrs ij2 jhra ij2 ed ed ed ed R2 3 sa

ð9:11Þ

av

where |〈rs〉|2 denotes the matrix element |〈W(rs, ae)|rs|W(rs, ae)〉|2, and similar for |〈ra〉|2. The transition matrix element multiplied by state density q(Ef) in (9.8) can be written as the transition matrix element multiplied by the product of line shape factor gs(E)Ga(E) and then integrate over the energy E, where Z Z gs ðEÞdE ¼ Ga ðEÞdE ¼ 1 For the sake of simplicity, the degeneracy of the energy levels has not been taken into account and by using (9.4) and (9.11), we obtained Wdd ¼

4p 1 3he2 R6sa

Z jehrs ij2 jehra ij2 gs ðEÞGa ðEÞdE

ð9:12Þ

If the probability As of S adopts the expression of (5.2a) and denote the factor 2 ½3n=ðn2 þ 2Þ as b, then jehrs ij2 ¼ 3hc3 bAs =4x3 n3 . On the other hand, the square of dipole matrix element can be expressed by oscillator strength of (5.18a) as |e〈ra〉|2 = 3he2bfa/2mnxs. Transform the variable x to wave number m by using

9.1 Theory of Resonant Energy Transfer

281

gðEÞ ¼ ngðmÞ=hc and xn ¼ 2pcm; substitute As ¼ gs =ssf . The energy transfer probability of the electric dipole–dipole interaction ﬁnally takes the form Wdd

1 3fa gs e2 2 ¼ 6 b Rsa 64p4 n3 ssf mc2

Z

ga ðmÞGs ðmÞ dm m4

ð9:13Þ

where e = n2 has been used. The factor b approximately equals to 1 and so will be omitted in the following formulas. Using mav to represent the average wave number in the overlap region of emission spectrum of S and absorption spectrum of A, then the transfer probability can be expressed approximately as Wdd

1:36 1016 cm fa gs Oin R6sa n3 ssf m4av

ð9:14Þ

where the diameter of the electron e2/mc2 = 2.82 10−13 cm has been substituted R and Oin ¼ ga ðmÞGs ðmÞdm is the overlap integral between emission spectrum of S and absorption spectrum of A. If one uses both the oscillator strengths of S and A, then (9.12) takes the form Wdd

1 3phe4 fa fs ¼ 6 6 2 2 Rsa n m x

Z gs ðEÞGa ðEÞdE

ð9:15Þ

Considering the difference of one factor (1/4pe0)2 in different unit system, the difference in the deﬁnition of oscillator strength used and the approximation of 3n/(n2 + 2) 1 adopted here, it can be seen that formula (9.15) is consistent with the formula (10.12) in the book of Henderson and Imbusch [13]. The conceptions of critical interaction distance and critical concentration have been used in the literature to deal with energy transfer between ions. When the separation between S and A equals to the critical distance, the energy transfer probability will be equal to the fluorescence decay rate 1/ssf of S. By (9.14), it is obvious that the critical interaction distance takes the following form Rc ¼ 2:27 103

fa gs Oin 1=6 cm n3m4

ð9:16Þ

The critical concentration Cc is deﬁned as a concentration in which there is an interaction ion in the sphere with the radius of critical interaction distance; obviously Cc ¼

4p 3 1 Rc 3

ð9:17Þ

By means of critical interaction distance, the energy transfer probability of dipole– dipole resonance can be written as

282

9

Wdd ¼

Energy Transfer and Migration Between Ions

R6C R6sa ssf

ð9:18Þ

The critical interaction distance and critical concentration can be roughly estimated for the energy transfer of rare earth ions. A typical value of 10−6 for the oscillator strength of rare earth ions can be assumed, and the wave number of the radiation is supposed to be 2 104 cm−1 and gs 1, n = 1.7. The overlap integral Oin is estimated to be 5 10−3 cm. Substituting all these data into (9.16) results in Rc 4.2 10−8 cm. By (9.17) one can obtain Cc = 3.2 1021 cm−3. It indicates that the energy is easy to be transferred by the interaction of ions. The expressions of energy transfer probability by high-order multi-pole interaction will not be introduced in detail here. The relations between them can be written as Wdq ¼ ðk=Rsa Þ2 ðfQ =fD ÞWdd

ð9:19Þ

Wqq ¼ ðk=Rsa Þ4 ðfQ =fD Þ2 Wdd

ð9:20Þ

where k is the wavelength of the transition and fD and fQ are the oscillator strengths of electric-dipole and electric-quadrupole transitions, respectively. From (9.5), the energy transfer probability by multi-pole interactions is closely related to the distance between two kinds of ions: Dipole-Dipole ð1=Rsa Þ6 Dipole-Quadrupole ð1=Rsa Þ8 Quadrupole-Quadrupole ð1=Rsa Þ10 Besides, energy transfer induced by the magnetic dipole–dipole interaction has similar distance dependence as that induced by the electric dipole–dipole interaction. For 3d electrons, the additional exchange interaction among them has to be taken into account. The energy transfer probability depends on both coordination number Z and wave function overlap integral S WEX /exp½2ZlnS

9.2

ð9:21Þ

Phonon-Assisted Energy Transfer Between Ions

The energy transfer related energy level separation between S and A in the material is not well matched in many cases. Therefore, there is an energy mismatch between the photon energy emitted by S and that absorbed by A. Thus, the overlap integral Oin in (9.14) is equal to zero generally. The energy transfer in this situation makes

9.2 Phonon-Assisted Energy Transfer Between Ions

(a)

phonon

283

(b) phonon

S

A

S

A

Fig. 9.2 Schematic diagram of phonon-assisted energy transfer, S: sensitizer, A: activator. a Energy mismatch DEsa compensated by phonon emission; b energy mismatch DEsa compensated by phonon absorption

using phonon as an intermediate. This process is called phonon-assisted energy transfer, and it is shown schematically in Fig. 9.2. In this kind of energy transfer process, the energy mismatch can be compensated by absorbing or emission one or two phonons, so as to maintain the energy conservation of the whole process. However, the multi-phonon-assisted energy transfer has a very low probability. As will be discussed later, there is also an exponential energy gap law here. Let’s ﬁrst introduce the expression of transfer probability for single-phonon-assisted energy transfer. It can also be calculated by the golden rule in quantum mechanics, that is W1p ¼

2p jMif j2 dðhxk DEsa Þ h

ð9:22Þ

where the matrix element Mif is a second-order matrix element because it involves multi-pole interaction between ions as well as electron–phonon interaction, and can be expressed as the product of the matrix elements of ion–ion interaction and that of electron–phonon interaction

X ha ; s; nk 1jHsa ja; s ; nk 1i a; s ; nk 1 Hep ðmÞ a; s ; nk Mif ¼ Es ðEs hxk Þ m¼s;a

ð9:23Þ X a ; s; nk 1 Hep ðmÞ a ; s; nk ha ; s; nk jHsa ja; s ; nk i þ Es Ea m¼s;a where a and s denote the ground states (a* and s* denote excited states) of activator (A) and sensitizer (S), respectively. As introduced previously, the ﬁrst-order electron–phonon interaction can be expressed in terms of the strain e as

284

9

Energy Transfer and Migration Between Ions

Hep ¼ V1 e In the above expression, strain tensor e has been averaged over the solid angle in the space. By using formula in Chap. 6, e can be expressed as linear combination of phonon creation and phonon annihilation operators and an angle averaged factor a is introduced, which has the order of magnitude 1. e¼i

X hxk a1=2 k

2Mv2

bk bkþ

ð9:24Þ

This expression has the similar form as that introduced in Sect. 6.5; the difference is that an angle factor a with order of magnitude 1 is introduced here. On the other hand, if we use the notations hujV1 jui ¼ f and hu jV1 ju i ¼ g to denote the matrix elements of V1 in low energy state u and high energy state u*, respectively, where u = a or s, then

a; s ; nk 1 Hep ðsÞ a; s ; nk ¼ gðsÞhnk 1jeðsÞjnk i

¼ gðsÞhnk 1jejnk i expð ik rs Þ a; s ; njk 1 Hep ðaÞ a; s ; njk ¼ f ðaÞhnk 1jeðaÞjnk i

¼ f ðaÞhnk 1jejnk i expð ik ra Þ a ; s; nk 1 Hep ðsÞ a ; s; nk ¼ f ðsÞhnk 1jeðsÞjnk i

ð9:25Þ

¼ f ðsÞhnk 1jejnk i expð ik rs Þ a ; s; nk 1 Hep ðaÞ a ; s; nk ¼ gðaÞhnk 1jeðaÞjnk i

¼ gðaÞhnk 1jejnk i expð ik ra Þ The relation of strain e with wave vector k and position vector r can be referred to Chap. 6. Owing to the fact that the ion–ion multi-pole interaction does not involve phonon coordinates and the phonon wave functions are normalized, we have ha ; s; nk 1jHsa ja; s ; nk 1i ¼ ha ; s; nk jHsa ja; s ; nk i ¼ ha ; sjHsa ja; s i If Jsa is used to represent the above matrix element, then it is easy to obtain Mif ¼ Jsa

hnk 1jejnk i expð ik ra Þ½ðf ðsÞ gðsÞÞexpð ik rsa Þ ðf ðaÞ gðaÞÞ DEsa ð9:26Þ

where rsa = rs − ra and DEsa is absolute value of energy difference between the electronic excited state of S and A. For the single-phonon process, we have DEsa = |Es − Ea| =hxk. In the introduction of formula (9.26), it should be noted that when Es > Ea, the electronic system will emit one phonon in the energy transfer

9.2 Phonon-Assisted Energy Transfer Between Ions

285

process, thus the phonon state becomes nk+ 1, and the energy difference in the denominator of the ﬁrst term of (9.23) is hxk ¼ DEsa ; when Es < Ea, the electronic system will absorb one phonon in the energy transfer process, thus the phonon state become nk − 1, and the energy difference in the denominator of the ﬁrst term of (9.23) is hxk ¼ DEsa . In the case of S and A are the same or similar kind of ion, f(a) − g(a) f(s) − g(s). By using (9.22), the single-phonon-assisted energy transfer probability takes the form W1p ¼

2 2p Jsa ðf gÞ2 X hxk DEsa Þ jhnk 1jejnk ij2 hðk; rsa Þdð 2 h DEsa k

ð9:27Þ

hðk; rsa Þ ¼ jexpðik rsa Þ 1j2 On the other hand, by using (9.24), for a particular phonon mode one has jhnk 1jejnk ij2 ¼

hxk a 2Mv2

nk þ 1 nk

ð9:28Þ

The summation over k in (9.27) can be changed to integral according to the following way Z X V 2 ð9:29Þ jhnk 1jejnk ij ¼ 3 jhnk 1jejnk ij2 4pk2 dk 8p k where 8pV 3 is the state density in k space, and it can be changed to an integral over xk by xk= km V 2p2 v3

Z jhnk 1jejnk ij2 x2k dxk

ð9:30Þ

The factor h(k, rsa) has different values in two different cases. When energy mismatch DEsa is large, krsa > 1. The wavelength of the phonon is in the same order of magnitude as the distance between S and A. In this case the space average of h(k, rsa) is about 2. By using the following relation dðhxk DEsa Þ ¼

dxk 1 dðxk DEsa =hÞ ¼ dðxk DEsa = hÞ h dE

the single-phonon-assisted energy transfer probability can be calculated according to (9.27) to obtain the result as follows

286

9

W1p ¼

Energy Transfer and Migration Between Ions

2 Jsa ðf gÞ2 DEsa a v5 6ph4 q

nk þ 1 nk

ð9:31Þ

where q denotes the density of the material. When energy mismatch DEsa is small, krsa 1, and the space average of h(k, rsa) is approximately (krsa)2/3. After the similar calculation, the following expression for single-phonon-assisted energy transfer probability can be obtained W1p ¼

2 3 2 Jsa ðf gÞ2 DEsa rsa a 6 v7 6ph q

nk þ 1 nk

ð9:32Þ

In thermal equilibrium, nk in (9.31) and (9.32) should be replaced by the following average value n ¼

1 expðDEsa =kB T Þ 1

ð9:33Þ

Two-phonon-assisted energy transfer probability can be introduced by third-order perturbation method in the similar way. For the case of small energy mismatch, two-phonon inelastic scattering may result in an efﬁcient energy transfer, and in this case DEsa ¼ hxk0 hxk . If energy mismatch is larger than the energy of one phonon, in the third-order perturbation, the absorption and emission of two phonons satisfy DEsa ¼ hxk0 þ hxk : The energy gap law of phonon-assisted energy transfer should be simply mentioned. It involves a system with strong electron phonon coupling. Although there is a certain amount of mismatch between the related energy gaps of S and A, but the overlapping integral of the phonon sideband of the emission spectrum for S and that of the absorption spectrum for A is not equal to zero. Miyakawa and Dexter [5] demonstrated by using generating function method that the relation of energy transfer probability for p-phonon-assisted process with that for the zero-phonon energy transfer process can be expressed as WðpÞ ¼ Wsa ð0Þ exp ðbDEÞ

ð9:34aÞ

Wsa(0) and b is expressed as R 2 2pJsa ga ðEÞGs ðEÞdE ðgs þ ga Þ e Wsa ð0Þ ¼ h

p b ¼ ðhxk Þ1 ln 1 ðgs þ ga Þðn þ 1Þ

ð9:34bÞ ð9:34cÞ

In the above expression, gs and ga are the coupling coefﬁcients of electron–phonon coupling (written as ga and gb in [5]). By using these expressions, the

9.2 Phonon-Assisted Energy Transfer Between Ions

287

temperature-dependent relation can be deduced. Substituting p = DEsa/hxk and (9.34c) into (9.34a), it can be seen that the p-phonon energy transfer probability is proportional to the following factor

expðhxk =kB T Þ ½n þ 1 ¼ expðhxk =kB T Þ 1

p

p

If one uses the average phonon energy hx to express the compensation of the energy gap mismatch, hx = DEsa/p. At low temperature expð hx=kB TÞ 1, expðhx=kB TÞ=ðexpðhx=kB TÞ 1Þ 1, then the energy transfer probability is independent of the temperature. However, at a higher temperature, the transfer probability will be increased. For the transfer processes involving 4–10 phonons, Yamada [14] ﬁtted the calculation values to the experimental data according to the above-mentioned factor and the result was satisfactory. For the transfer processes involving 1–2 phonons, Colins and Di Bartolo [15] observed that the transfer probability decreases with temperature. By taking into account the particle distribution in the initial and ﬁnal states, the abnormal temperature dependence can be well explained. It demonstrates, on the other hand, that (9.34a) is suitable only for the transfer processes involving large number of phonons. Auzel and Chen [16] pointed out that the phonon energy in energy transfer and phonon side band processes is actually lower than that in non-radiative transition process. They calculated this difference for trivalent erbium in glass ZBLAN and silicon glass. For trivalent erbium in glass ZBLAN, in the probability calculation of non-radiative transition, phonon energy of 580 cm−1 should be used while that of phonon side band or energy transfer, phonon energy can only be 325–350 cm−1. For trivalent erbium in silicon glass, the former is hx ¼ 1100 cm1 while for the 1 latter it is hx ¼ 500 cm .

9.3

Statistical Theory of Energy Transfer Between Ions

The distance between S and A is different in different locations of the media. To obtain a formula which can be practically used in the calculation of transfer probability, it should be based on statistical theory. A detailed procedure to do this is as follows: First, investigate the rate equation of particle number for a certain S– A distance to establish an expression of time-dependent particle number; then statistically average the particle number variation to ﬁnd out the average expression of the variation of particle number. Suppose S can be classiﬁed into several classes, in the case that same class S has the same A surrounding. By using (9.18), the k class S has the following expression of energy transfer probability

288

9

k Wdd ¼

Energy Transfer and Migration Between Ions

Na X R6c R6 s i¼1 ik sf

ð9:35Þ

The summation is over all the A, where Rik is the distance between the S of the k class and the A of the i class. Assuming no energy migration among S, the particle number of S in k class will satisfy the following rate equation: dNsk 1 ¼ ssf dt

1þ

Na X R6

!

c 6 R i¼1 ik

ð9:36Þ

Nsk

where the ﬁrst term accounts for the decay of S by spontaneous emission and the second term corresponds to the decay produced by energy transfer. Integrating (9.36), then (

" 1

Nsk ¼ Nsk ð0Þexp ðssf Þ t 1 þ

Na X

#) ðRc =Rik Þ

6

ð9:37Þ

i¼1

For the random distribution of A, the probability that the S belongs to the k class is Pk dk ¼

Na Y 4pR2 dRik ik

i¼1

V

sk is The statistical average of Nsk denoted by N Z sk ¼ Nsk Pk dk N

ð9:38Þ

ð9:39Þ

In the problem discussed, the condition (ssf)−1t(Rc/Rik)6 1 is always satisﬁed. In this situation, Forster [1] did the integration of (9.39) and obtained the following result h i sk ¼ Nsk ð0Þexp ðssf Þ1 t ðCa =Cc Þðp t=ssf Þ1=2 N

ð9:40Þ

where Ca denotes the concentration of A, and Cc is the critical concentration. On the basis of the above theory, Inokuti and Hirayama [17] assumed a random spatial distribution of A around S and which is not affected by the distribution of S. Without considering the energy migration between S, a general number decay expression of S in fluorescence level for multi-pole interactions (n = 6, 8, 10) was derived

9.3 Statistical Theory of Energy Transfer Between Ions

3 1 3=n Nsk ¼ Nsk ð0Þexp ðssf Þ t C 1 ðCa =Cc Þðt=ssf Þ n

289

ð9:41Þ

The time-variation of S fluorescence intensity, therefore, is 3 IðtÞ ¼ Ið0Þexp ðssf Þ1 t C 1 ðCa =Cc Þðt=ssf Þ3=n n

ð9:41aÞ

This expression is also written as t IðtÞ ¼ Ið0Þexp ct3=n ssf

ð9:41bÞ

3 3=n c ¼ C 1 ðCa =Cc Þssf n

ð9:41cÞ

where

In these expressions, n = 6 for dipole–dipole interaction, n = 8 for dipole–quadrupole interaction, and n = 10 for quadrupole–quadrupole interaction. The gamma functions in (9.41) are: Cð1 3=6Þ ¼ Cð1=2Þ ¼ p1=2 1:77; Cð1 3=8Þ ¼ Cð5=8Þ 1:43; Cð1 3=10Þ ¼ Cð7=10Þ 1:30: Note that (9.40) and (9.41) are obtained in the condition of no energy migration among S. The characteristic of this energy transfer pattern is: in the initial stage of the luminescence decay curve of S (i.e. t ssf), ln[I(t)/I(0)] is proportional to t3/s but with the increase of time, the number of non-excited A around excited S is decreased. Owing to the fact that the energy transfer probability between S and A is greatly decreased with the increase of distance between these two ions so that more S will decay by their luminescent emission and their luminescence decay curve will become approximately simple exponential decay curve. Here, simple exponential decay curve means that the exponent of exponential function only involves a linear term of time, while the non-simple exponential decay curve refers to the nonlinear term of time appearing in the exponent .That is to say, the total fluorescence decay curve is divided into two segments of the initial non-simple exponential decay and the subsequent approximately simple exponential decay. It should be pointed out that I-H model was obtained under the assumption of without energy migration between S; it is applicable for the case of low concentration of S and A.

290

9 0

10

-1

10

N/N(0)

Fig. 9.3 Schematic diagram of the decay of particle number of sensitizer for different types of multi-pole interaction under the assumption of Ca/C0 = 1. Abscissa is in the unit of the lifetime of S ion

Energy Transfer and Migration Between Ions

-2

10

n=10 n=8

-3

10

n=6

-4

10

0

1

2

3

4

5

6

t/t(f)

The decay rates for different interactions are different. The dipole–dipole interaction produces the highest decay rate, the dipole–quadrupole interaction has a lower decay rate, and the quadrupole–quadrupole interaction has the lowest decay rate. These relations are shown in Fig. 9.3 with exponential coordinate of particle number versus t/ssf.

9.4

Energy Migration Between Ions

When A and S are coexistent in the sample and the concentration of S is high enough, the excited energy can migrate among S before transfer to A. This is a multi-step process. The transfer of excitation energy can be seen as the migration of exciton among S and the trapping of the exciton at site of A will modify the decay rule of the excited state population of S. In this section, the main results of the related theory will be briefly introduced. Generally speaking, there are two kinds of method to deal with this problem, namely random walk theory and diffusion theory. First let us discuss the simplest case, in which the S-A interaction is equivalent to the S-S interaction and belong to the electric dipole–dipole interaction. During the energy transfer of S ! A, S can also emit photon directly. The energy transfer to A will be described as exciton random walk to the positions of A (trap). Suppose the propagating time of the exciton from one ion to another ion is th. The emission probability of S per second is 1/ss. On the other hand, the possibility of the exciton fall into the traps for walking to a new lattice position is Ca (the concentration of A). When the exciton walks to a new lattice position, the probability for falling into the traps per second will be Ca/th, so that the lifetime of the exciton in this walking process is th/Ca. Therefore, the number N0 of original exciton will be reduced to N0exp [−th/(th/Ca)] = N0exp (−Ca); in other words, the decay rate of the exciton

9.4 Energy Migration Between Ions

291

number by walking to a new lattice position is exp(−Ca). According to mathematical theory of random walk [18], the probability W(0, n) for the n-step random walk can be expressed as the product of the corresponding probability of random walk at successive steps Wð0; nÞ ¼ Wð0; 1ÞWð1; 2ÞWð2; 3Þ. . .Wðn 1; nÞ

ð9:42Þ

The mathematical theory of random walk in lattice has been studied by Montroll et al. [19] According to their result, the number of lattice positions visited by the exciton after its n-step random walk (n is a very large number) can be expressed as Snn (Sn = 0.66 for simple cubic lattice, Sn = 0.74 for face-centered cubic lattice, and Sn = 0.72 for body-centered cubic lattice). After n-step random walk the decay rate of the exciton will be ½expðCa ÞSn n ¼ expðnSn Ca Þ Supposing there are N0 excitons at t = 0, then after time t1 by the trapping effect, the exciton number will become N0 expðnSn Ca Þ

ð9:43Þ

where n = t1/th. On the other hand, after n-step walk, by the direct emission, the decay factor of exciton is obviously expðt1 =ss Þ

ð9:44Þ

The exciton number without both trapping and emission will be N0 expðnSn Ca Þexp½t1 =ss ¼ N0 exp½t1 ðSn Ca =th þ 1=ss Þ N0 exp t1 =s0s ð9:45Þ Therefore the fluorescence lifetime of S affected by both energy transfer and radiation transition will be s0s ¼

1 1=ss þ Ca Sn =th

ð9:46Þ

Suppose Wrw is the energy transfer probability generated by random walk; W0 and W denote the transition probabilities without A and the total transition probability of S in case the coexistence of A and S, respectively, then W ¼ W0 þ Wrw

ð9:47Þ

292

9

Energy Transfer and Migration Between Ions

Obviously Wrw ¼ Sn Ca =th

ð9:48Þ

By the formula introduced previously, the jumping time of exciton is the reciprocal of energy transfer th ¼ ss ðRss =Rc Þ6

ð9:49Þ

where Rc is the critical interaction distance deﬁned in (9.16) and Rss denotes the distance between S and its nearest neighbor S. It is easy to realize that (Rss/Rc)6 = (Cc/Cs)2, where Cs and Cc are the concentration and critical concentration of S. If the fluorescence intensities of S without and with the presence of A denoted by Is0 and Is, respectively, it can be proved that Is ¼ Is0 =ð1 þ ss Wrw Þ ¼ Is0 =½1 þ Sn Ca ðCs =Cc Þ2

ð9:50Þ

By using the conceptions of exciton jumping and average jumping time, Brushtein introduced another luminescence decay formula of S in the case of S-S energy migration probability is higher than S-A energy transfer probability, that is ass > asa. This is called hopping model [20] pﬃ t IðtÞ ¼ Ið0Þexp n t K 0 t ssf

ð9:51Þ

where K′ is energy transfer probability assisted by energy migration and the values of n and K′ by the electric-dipole interaction can be expressed as pﬃﬃﬃﬃﬃﬃ 4 n ¼ p3=2 Ca asa 3

ð9:52Þ

pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ K 0 ¼ pð2p=3Þ5=2 Ca Cs asa ass

ð9:53Þ

On the other hand, according to (9.14), by taking into account degeneracy ge of the excited level and degeneracy gg of the ground level of S, the energy transfer parameter asa and the energy migration parameter ass for the electric-dipole interaction can be expressed as add sa

1:36 10

16

fa gs gg Oin dd fs gs gg Oin 16 cm 3 ; a 1:36 10 cm 3 n ge m4 ss n ge m4 ð9:54Þ

These two parameters also denote as Csa and Css and can also be calculated by emission and absorption cross-section as follows

9.4 Energy Migration Between Ions

293

Z 3c gg ðaÞ rðsÞ asa Csa ¼ 4 02 em ðkÞrab ðkÞdk; 8p n ge Z 3c gg ðsÞ ass Css ¼ 4 02 rðsÞ em ðkÞrab ðkÞdk 8p n ge

ð9:55Þ

In the case of energy migration among S has high probability; one can also treat the energy migration process as diffusion process. Martin et al. [21] used diffusion model to study energy migration and energy transfer processes for random distribution of ion. The density q(R, t) of excited S satisfy the following equation " # NA @ 1 X qðR; tÞ ¼ Ds D Wsa Rs Raj qðR; tÞ @t ssf j¼1

ð9:56Þ

where Ds is a diffusion parameter which characterizes the migration processes among S, ssf is the lifetime of S and Wsa(Rs − Raj) is the energy transfer probability from S at position Rs to A at position Raj. The ﬁrst term in the right-hand side of this equation expresses the diffusion effect; it has not appeared in (9.36). By using Padé approximation to solve (9.56), we can obtain "

ðn3Þ=ðn2Þ # t 4pCA 3 ðnÞ 3=n 1 þ a1 x þ a2 x2 C 1 IðtÞ ¼ Ið0Þexp asa t ssf n 3 1 þ b1 x ð9:57Þ 2=n ðnÞ where x ¼ Ds asa t12=n and the expression of Ds as well as the values of a1 , a2 , and b1 , for dipole–dipole interaction n = 6, dipole–quadrupole interaction n = 8, and quadrupole–quadrupole interaction n = 10 respectively are shown as follows: n

Ds

6 8 10

a1

a2

Ds ¼

4=3 ð6Þ 3:376Cs ass

10.866

15.500

b1 8.743

Ds ¼

ð8Þ 2:924Cs2 ass

17.072

35.860

13.882

Ds ¼

8=3 ð10Þ 4:559Cs ass

24.524

67.909

20.290

Obviously, when Ds = 0, (9.57) is identical to (9.41) because in this case (9.56) is actually the same as (9.36). Yokota and Tanimoto [22] solved (9.56) before Martin for the special case of electric-dipole interaction and obtained the result of (9.57) for n = 6 "

3=4 # t 4pCa 1=2 ð6Þ 1=2 1 þ 10:87y þ 15:50y2 p IðtÞ ¼ Ið0Þexp asa t ð9:58Þ ssf 3 1 þ 8:743y

294

9

Energy Transfer and Migration Between Ions

1=3 y ¼ Ds að6Þ t2=3 sa Equations (9.57) and (9.58) are all referred to as Yokota–Tanimoto model (Y-H model) in the literature. In the above expressions, the diffusion parameter Ds is dependent on the S-S energy migration probability and the concentration of S. In the case of low S concentration Huber [23] obtained its expression for multi-pole interaction as follows n2 3 1 4 Ds ¼ ðn 5Þ1 pCs aðnÞ ss 2 3

ð9:59Þ

For dipole–dipole interaction, this diffusion parameter is 43 1 4 pCs að6Þ Ds ¼ ss 2 3

ð9:60Þ

After a long enough time t, the fluorescence decay of S will be asymptotically simple exponential and if S-S energy migration is dipole–dipole process then the decay rate s−1 follows the following equation 1 1 ¼ þ WsaðdiffÞ s ssf

ð9:61Þ

Accordant to the calculation of Huber [23] 1=4 1=4 3=4 WsaðdiffÞ ¼ 8:5Cs að6Þ D3=4 ¼ 21Cs Ca að6Þ add sa s sa ss

ð9:62Þ

It can be demonstrated that when ass asa the hopping model is suitable, while when ass asa diffusion model is suitable. The interaction between S increases with the temperature and is proportional to T 3 [24]. Therefore, the diffusion model can be used to describe the energy transfer at relatively low temperature, whereas at higher temperature the hopping model should be used. A typical example is presented in the following. Hegarty et al. [24] studied the energy transfer rule of Nd3+:PrF3. Nd3+ concentration in this sample is 5 at.%. The emission of Pr3+ is observed under pulse laser excitation. The investigation of logarithm relation between Wsa (WDA) and ð6Þ

ð6Þ

ð6Þ

ð6Þ

ass =asa aDD =aDA in the temperature range of 10–13 K showed that the slope of 3=4 ð6Þ is in agreement with the result obtained by diffusion model, but at the ass

temperature higher than 15 K, it should be described by exciton hopping model. This is shown in Fig. 9.4.

9.4 Energy Migration Between Ions

295

ð6Þ

ð6Þ

Fig. 9.4 The variation of exciton transfer versus temperature and the ratio of aDD =aDA in Nd3+: PrF3 [24]

In some cases, the following rate equations can be used to calculate the energy transfer probability by means of the data of fluorescence intensity and fluorescence lifetime dNs Ns dNa Na ¼ Ps 0 Kt Ns ; ¼ 0 þ Kt Ns dt dt ssf saf

ð9:63Þ

where Ns and Na are the particle numbers of S and A in excited state, while s0sf and s0af denote the lifetime of S and A, respectively. Kt is the transfer rate between S and A, while Ps is the exciting rate of S. Obviously, in the case of steady state (Ps is constant), the solutions of Ns and Na are Ns ¼

Ps s0sf Kt Ps s0sf s0af ; Na ¼ 0 1 þ Kt ssf 1 þ Kt s0sf

ð9:64Þ

while in the case of pulse excitation, the solutions are t NS ðtÞ ¼ NS ð0Þexp ð1 þ Kt ssf Þ ssf NA ðtÞ ¼

Kt NS ð0Þs0sf s0af 0 ssf s0af Kt s0sf s0af

t t exp 1 þ Kt s0sf 0 exp 0 ssf saf

ð9:65aÞ ð9:65bÞ

296

9

Energy Transfer and Migration Between Ions

The decay of fluorescence intensity with time written by (9.65a) will be t IðtÞ ¼ Ið0Þexp 0 Kt t ssf

ð9:65cÞ

This expression is the same as (9.51) by neglected n(t)1/2; however, the condition of obtaining (9.51) is ass > asa. Owing to the fact that n = 7.42Ca(asa)1/2 and K′ = 19.9CsCa(assasa)1/2, if Cs Ca the relation K′t n(t)1/2 is certainly satisﬁed. Therefore, when S-S energy migration probability is much higher than S-A energy transfer probability and the concentration of S is much higher than that of A, the decay of S fluorescence intensity after doping of A is still a simple exponential type; the only difference is the decay rate is increased. On the other hand, a conclusion can be drawn: the premise conditions of using the above rate equation to analyze energy transfer process are the S-S energy migration probability is much higher than that of the S-A energy transfer and the concentration of S is much higher than that of the A. The laser material of Yb3+ ions sensitize Tm3+ ions is one of the examples which satisfy this condition, because the energy migration between Yb3+ ions is a resonance process; what is more, the overlapping between the emission spectrum and the absorption spectrum of Yb3+ ion is great, while the energy transfer between Yb3+ ion and Tm3+ ion is a phonon-assisted process so that ass > asa. On the other hand, in this kind of laser material, in order to increase the pumping light absorption efﬁciency, the concentration of sensitized Yb3+ ion is much higher than that of the activated Tm3+ ion. Therefore, the above premise conditions for using rate equation to analyze energy transfer process are satisﬁed. Energy transfer rate Kt can also be obtained by fluorescence lifetime measurement. If the fluorescence lifetime of S is ssf with A in the sample, while the fluorescence lifetime of S is s0sf without A in the sample, then the transfer probability will be Kt ¼

s0sf ssf ssf s0sf

ð9:66Þ

By using this formula, it is only necessary to obtain the experimental data of fluorescence lifetime for S with and without A in the sample, respectively. On the other hand, one can use integrated fluorescence intensities Is and Ia of S and A when two kinds of ions coexist in the sample. It can be shown that in this case one has the following expression Ia Aa Na ma ssr Na ks ¼ ¼ Is As Ns ms sar Ns ka

ð9:67Þ

where Na and Ns are concentration, while As and Aa are spontaneously transition probabilities of S and A, respectively; meanwhile, ssr and sar are corresponding radiative lifetimes. By using measured integrated luminescence intensities Is and Ia, when two kinds of ions are present in the sample simultaneously and the solutions

9.4 Energy Migration Between Ions

297

of (9.64) and (9.67), the energy transfer rate in steady-state condition can be obtained as Kt ¼

sar Ia ka saf ssr Is ks

ð9:68Þ

To analyze the relation between the Yb3+ fluorescence lifetime and the concentration of Yb3+ and Tm3+ ions, one can also use the following simple model. To facilitate the discussion of the problem, the Yb3+ ion is denoted by S while the Tm3+ ion is denoted by A. First, let us discuss the effect of the presence of A on the number of S in excited state. Suppose the atomic percentage concentrations of S is Cs and that of A is Ca and S–S energy migration probability is Wss while S ! A energy transfer probability is Wsa. Under certain excitation conditions, the S ! A energy transfer rate is proportional not only to transfer probability Wsa but also to concentration Ca. Suppose the proportional constant is g, then by the fluorescence decay of S and S ! A energy transfer, the change rate of S particle in excited state will be dNS NS ¼ gCa Wsa NS dt ssf

ð9:69Þ

where ssf is fluorescence lifetime of S. In the calculation of the number decrease of excited state S caused by fluorescence decay, the effect of radiation trapping should be deducted. Suppose the reabsorption probability of S is Wreab, the number of excited state S generated by the reabsorption is proportional to the product of CsWreab and so can be written as g′CsWreab. Therefore, the rate equation of S should be dNS 1 0 ¼ þ gCa Wsa g Cs Wreab NS ssf dt

ð9:70Þ

Integrating the above equation, we obtain 1 0 þ gCa Wsa g Cs Wreab t NS ðtÞ ¼ NS ð0Þ exp ssf

ð9:71Þ

From the formula (9.13), the ratio of Wsa and Wss is expressed as 6 Wsa Rss Cs þ Ca 2 ¼s ¼s Wss Rsa Cs

ð9:72Þ

where Rss is the average separation between different S, Rsa is that between A and S, and the parameter s only depends on the spectral properties of A and S but independent of their concentrations. If Rsc represents the average separation of S at critical concentration Csc, then by using (9.18), Wss can be expressed as

298

9

Wss ¼ s1 sf

Rsc Rss

6

Energy Transfer and Migration Between Ions

¼ s1 sf

Cs Csc

2 ð9:73Þ

Therefore Wsa ¼

s Cs þ Ca 2 ssf Csc

ð9:74Þ

In addition, the probability of radiation trapping is proportional to the fluorescence emission probability of S and inversely proportional to the square of ions separation [25]; therefore it can be written as Wreab /

s1 sf

1 Rss

2

2=3 ¼ rs1 sf ðCs Þ

ð9:75Þ

Integrating the effects of the above three processes, the S number in excited state at time t is

i t h 2 NS ðtÞ ¼ NS ð0Þexp 1 þ sgCsc Ca ðCa þ Cs Þ2 g0 rCs5=3 ssf

ð9:76Þ

That is, after considering the fluorescence emission of S, the radiation trapping and the energy transfer to A, the fluorescence lifetime of S can be expressed as h i 2 Ca ðCa þ Cs Þ2 s0sf ¼ ssf = 1 g0 rCs5=3 þ sgCsc

ð9:77Þ

The second term in the denominator of the above expression takes into account the radiation trapping effect while the third term is the contribution of sensitizing effect on the fluorescence lifetime. If one discusses not the S ! A energy transfer but the concentration dependent fluorescent quenching of S, the same deduction method can be used. However, the above S ! A energy transfer should be replaced by A ! Q energy transfer (Q denotes the quenching center). To discuss the fluorescence lifetime of A varied with the concentration of A and Q, the above parameters r, g, and g′ should be replaced by r1, g1, and g1′, then 2 2 s0af ¼ saf = 1 r1 g01 Ca5=3 þ s1 g1 Cac Cq Cq þ Ca

ð9:78Þ

wheresaf is fluorescence lifetime of A, Cq is the atomic percentage concentrations of quenching center Q, and Cac is the critical concentration of A. The second term on the denominator of the above expression takes into account the radiation trapping effect, while the third term is the contribution of quenching effect on the fluorescence lifetime.

9.4 Energy Migration Between Ions

299

Equation (9.78) can be used to analyze the concentration dependent fluorescent quenching and radiation trapping effect of Yb3+: YAB crystal [26]. Fluorescence concentration quenching of Yb3+ ion in this crystal is due to the impurity ion in the crystal, because the purities of Yb2O3 and Y2O3 raw materials used for growing crystals were 99.99 and 99.999% respectively. The percent content of impurity ions in the crystal, especially that of the rare earth impurities, which are difﬁcult to separate in the raw material, can be seen as proportional to the percentage of Yb2O3 in the crystal. On the other hand, from the crystal growth point of view, it can be assumed that the point defects which may form the energy traps in the crystal are also related to the concentration of doped Yb3+ ion. At lower Yb3+ concentration (e.g. lower than 50%), the concentration of point defect can be seen as proportional to the Yb3+ concentration while at the Yb3+ concentration higher than 50%, the concentration of point defect can be seen as decreased with Yb3+ concentration, because the increase of Yb3+ concentration is equivalent to the reduction of impurity ion Y3+ from the perfect crystal of YbAB. If the atomic percentage concentration of Yb3+ ion is CYb then the atomic percentage of fluorescence quenching center can be assumed as aCYb for the Yb3+ concentration lower than 50%. In (9.78) let Ca = CYb and Cq = aCYb, then the following can be obtained 5=3 5=3 2 3 3 s0af ¼ saf = 1 r1 g01 CYb þ s1 g1 að1 þ aÞ2 Cac CYb saf = 1 ACYb þ BCYb ð9:79Þ 2 A ¼ r1 g01 ; B ¼ sg1 að1 þ aÞ2 Cac

The measured values of the fluorescence lifetime for Yb3+: YAB powder sample placed in index matching fluid with different Yb3+ concentrations are listed in Table 9.1. The experimental data can be ﬁtted to the (9.79) very well. The ﬁtting parameters are saf = 510 ls, A = 1.89 and B = 95.79. Figure 9.5 is the ﬁtting result Table 9.1 Yb: YAB crystal fluorescence lifetimes at different Yb3+ atomic percentage concentrations [26] CYb (%)

sbf (ls)

spf (ls)

sdf (ls)

sr (ls)

5.6 680 / / 600 6.5 960 557 513 606 17.3 910 449 480 652 29.2 237 141 490 620 40.7 194 122 509 616 65.5 20 23 541 575 75.0 77 26 520 613 100 17 23 535 672 sbf, spf, sdf, andsr are the Yb3+ fluorescence lifetime measured values in bulk sample, powder sample, and diluted powder sample, respectively and radiative lifetime calculated values of 2F5/2 multiplet. The data of sbf are taken from reference [27]

300

9

Energy Transfer and Migration Between Ions

Fig. 9.5 Room temperature fluorescence lifetime of Yb3+: YAB crystal in powder samples at 1038 nm under excitation at 930 nm versus Yb3+ concentration. The points represent the experimental data and the solid curve is the ﬁtting result from (9.79) [26]

of the relation of the fluorescence lifetimes at 1038 nm with the Yb3+ atomic percentage concentration for Yb3+: YAB crystal powder sample at room temperature. The above analysis of the effects of concentration dependent fluorescent quenching and radiation trapping is only ﬁtted to the data of powder sample placed in index matching fluid. However, due to the fact that the refractive index of the matching fluid still has some difference from that of the YAB crystal powder, the internal reflection is still existence, so that A 6¼ 0. Nevertheless, the particle size of the samples with different Yb3+ concentration is the same; the values of A for different sample are approximately the same, so the experimental data can be ﬁtted. The result obtained by this method can also easily explain the data of diluted powder sample in Table 9.1. All these powder samples are diluted by pure YAB powder to an average Yb3+ concentration 0.5%. Although the difference of the distribution of Yb3+ ions in the sample causing the difference in parameter r results in several times difference of parameter A, but because the Yb3+ concentration is 3 very low, F = 1 − AC5/3 Yb + BCYb and is always very close to 1 (A = 2.0, F = 0.9989; A = 20.0, F = 0.9959). This is the reason that the fluorescence lifetimes of all these diluted samples are about 510 ls. In Table 9.1, the fluorescence lifetime of bulk sample certainly cannot be explained by (9.79). One of the important reasons is in these samples, the defects, bubbles, and dislocations, which can cause the internal reflection of fluorescence emission, are different for different crystal grown batches, and even different for the different parts of the same piece of grown crystal. This complexity makes the theoretical model not correctly describe the contribution of radiation trapping effect on the fluorescence lifetime. However, it can be seen from this table that the fluorescence lifetime of bulk sample with low Yb3+ concentration is more signiﬁcantly longer than that of the powder sample in index matching fluid with same Yb3+ concentration. The reason for this phenomenon is that in low Yb3+ ion concentration bulk sample the

9.4 Energy Migration Between Ions

301

internal reflection radiation can maintain at a higher intensity for a longer time in spite of the weak reabsorption of radiation in a single pass. With the increasing of Yb3+ concentration, the fluorescence lifetime of diluted samples has a change from longer to shorter and then from shorter to longer. The reason for this change can be interpreted as: when the concentration of Yb3+ ion is lower than 50%, the increase of Yb3+ ion concentration corresponds to the increase of crystal defects; while when the concentration of Yb3+ ion is higher than 50%, the increase of Yb3+ ion concentration corresponds to the reduction of crystal defects as has been explained. The study of energy transfer always involves the calculation of fluorescence lifetime. It is necessary to discuss the problem of how to calculate this parameter correctly. It can be seen from the above discussion that in the case of isolated ions or energy migration probability between ions is higher than that of energy transfer probability, the fluorescence decay is described by a simple exponential function. However, in the general case of energy transfer between ions, such as that shown in (9.41), (9.51), and (9.58), in addition to a linear term of time, a nonlinear term of time appears in the exponent of the function of fluorescence intensity. In this case, the attenuation curve of the fluorescence intensity in the logarithmic coordinate is not a straight line so that the calculation method of fluorescence lifetime should be studied. Some one used the following formula to calculate this kind of non-simple fluorescence decay Z1 sf ¼

IðtÞdt=I0

ð9:80aÞ

0

It can be shown that this formula is applicable only to the case of simple fluorescence decay and can be demonstrated from the deﬁnition of fluorescence lifetime. Fluorescence lifetime is the time in which the fluorescent particle stays in the fluorescent level. Obviously, the particles transition at different moments has different lifetimes, so that only the average lifetime of the particle in the fluorescent level has physical meaning. If one divides the fluorescence process into inﬁnite small time intervals Dt, at moment t the particle number in the fluorescent level is N(t) and the transition probability for the downward transition is A, then the particle number downward transition from the moment t to the moment t + Dt will be N(t)ADt. The fraction of particle having lifetime t relative to the total particle number of fluorescent level is NðtÞADt=

t¼1 X t¼0

NðtÞADt

302

9

Energy Transfer and Migration Between Ions

Therefore, the average fluorescence lifetime is 0

2

!1 BtX

sf ¼ lim B [email protected]

t¼0

31

R1

R1

tIðtÞdt 6 NðtÞADt 7C 0 0 6 7 C t4t!1 ¼ R1 5A ¼ R1 P NðtÞAdt IðtÞdt NðtÞADt t¼0

tNðtÞAdt

0

ð9:80bÞ

0

This formula is the correct one for the fluorescence lifetime calculation. The calculation formula (9.80a) is practically the result of (9.80b) in a special case when the fluorescence decay satisfy the following equation IðtÞ ¼ I0 eAt ; where sf ¼ A1 According to (9.80a), the fluorescence lifetime will be Z1 sf ¼

Z1 IðtÞdt=I0 ¼

0

e

At

1

Z1

dt ¼ A

0

deAt ¼ A1 ¼ sf

0

Substitute this simple exponential expression of I(t) into the right side of (9.80b), then Z1

Z1 tIðtÞdt ¼ I0

0

te

At

Z1

dt ¼ I0 A

0

tde

At

1

¼ I0 A

0

Z1 ¼ sf

1

1 teAt 0

1

Z1

þ I0 A

eAt dt

0

IðtÞdt 0

that is, it agrees with (9.80b). However, if the fluorescence decay satisfy the following equation IðtÞ ¼ I0 eAtBt ðq\1Þ q

the results obtained by (9.80a) and (9.80b) are different. It means that in this case the lifetime obtained by (9.80a) is not consistent with the correct deﬁnition of fluorescence lifetime.

9.5 Characteristics of Concentration Dependent Fluorescence Quenching …

9.5

303

Characteristics of Concentration Dependent Fluorescence Quenching for Self-activated Laser Crystals

In this section we would like to take the self-activated laser crystals as an example to introduce the research result of the author to the relation of energy transfer probability with the chemical composition of the crystals. The so-called self-activated laser crystal is one kind of crystals in which the active ion (A) is the constituent of the crystal but not doped impurity. It is well known that for many laser crystals such as YAG and YAP, the concentration of A is usually a few percent in atomic percentage. For the crystals with higher concentration of A, the quenching effect has to be considered. A general viewpoint about the requirement for a crystal without quenching effect is as follows: the shortest separation between the positions which can be occupied by A should be longer than 60 nm. However, among the crystals satisfying this geometric condition, what is the relation between the quenching effect and the characteristics of the host crystals? Auzel [8] reported that for the weak quenching crystals, the crystal ﬁeld should be weak enough to satisfy the following inequality Nv ¼

X

!1=2 B2kq

1800 cm1

ð9:81Þ

k;q6¼0

The investigation of emission intensity and fluorescence lifetime has shown that the strength of quenching effect is proportional to the square of the concentration of A for the crystals like YAG and YAP, but it is proportional to the concentration of A for self-activated laser crystals [28]. Obviously, the fluorescence quenching in the crystals like YAG and YAP is generated by the electric dipole–dipole cross-relaxation process 4F3/2 + 4I9/2!4I15/2 + 4I15/2, because the probability of this process is inversely proportional to the six powers of the separation between A, as shown in (9.14); that is, proportional to the square of the concentration of A. R Auzel [29] discussed this problem by the overlap integral ga ðEÞGs ðEÞdE in the expression of resonant energy transfer probability of (9.12). In order to have a non-zero value of this integral, the energy released by the Nd3+ ions in excited state should be equal to the energy absorbed by the neighbor Nd3+ ions in the ground state. It requires that the related pair of energy levels satisfy the matching condition. It can be clearly seen in Fig. 9.6. Figure 9.6 shows that the resonant energy transfer condition is E1M = E2M. e1 is the separation between barycenters of 4I15/2 and 4I9/2 while e2 is the separation between barycenters of 4F3/2 and 4I15/2. The resonant energy transfer condition can be expressed as DE2 DE1 =2 þ DE3 =2 ¼ e1 e2

ð9:82Þ

304

9

Energy Transfer and Migration Between Ions

Fig. 9.6 Schematic diagram for the energy levels related to the concentration quenching effect of fluorescence level 4 F3/2 of Nd3+ ion

where DE1, DE2, and DE3 are crystal ﬁeld splitting of 4I9/2, 4I15/2, and 4F3/2, respectively. The following scalar crystal ﬁeld parameter is a very interesting quantity " Nv ¼

4p 2k þ 1

X k;q6¼0

#1=2 B2kq

"

X

#1=2 B2kq

ð9:83Þ

k;q6¼0

It was found experimentally [28] that no matter the Nd3+ ion sited in what kind of position, the crystal ﬁeld splitting of the above spectral terms approximately have the following relations DE1 0:23Nv ; DE2 0:27Nv ; DE3 0:026Nv

ð9:84Þ

Substituting the above relations to (9.82), it is easy to ﬁnd Nv ¼ ðe1 e2 Þ=0:168 Therefore, if the crystal ﬁeld is weak enough to satisfy the condition Nv < (e1 − e2)/0.168, then the resonant energy transfer condition cannot be satisﬁed. The fluorescence energy cannot transfer from multiplet 4F3/2 of one Nd3+ ion to multiplet 4I15/2 of another Nd3+ ion by cross-relaxation, and the fluorescent quenching will not occur. This is the reason why the strength of quenching effect of self-activated laser crystal is not proportional to the square of the concentration of A. It should be seen that apart from the above-mentioned cross-relaxation, the fluorescence quenching effect of Nd3+-doped laser crystal may also be the energy migration between 4F3/2 multiplet of different Nd3+ ions and ﬁnally fall into the “trap” of impurity ions or crystal defects that existed in the crystal. This is the

9.5 Characteristics of Concentration Dependent Fluorescence Quenching …

305

reason why the strength of quenching effect is proportional to the concentration of A in self-activated laser crystal, because the concentration of the “trap” is usually proportional to the concentration of doping ions. However, there is still no answer to the relation of quenching effect with chemical composition of crystals. The author [30] pointed out that the fluorescence quenching effect is closely related to the chemical characteristics of ligand anions or ligand anion groups by using a parameter R, or parameter L = 1/R = r−/(r+Dx) [31] to measure the strength of quenching effect, where r+ is the radius of the cation directly connected to the coordination anion, r− is the radius of the anion, and Dx is the difference of the electronegativity between cation and anion. Taking seven Nd3+-doped laser crystals as an example, the relation of parameter L with Nd3+ concentration of unit quenching ratio is listed in Table 9.2. If sr indicates the radiative lifetime of Nd3+ ion in the crystal, sf is its fluorescence lifetime. Quenching rate of fluorescence is deﬁned as Kq = (sr − sf)/sfsr. The quenching rate of fluorescence lifetime reduced to half of the radiation lifetime is obviously K1/2 = 1/sr. Quenching ratio is deﬁned as Rq = Kq/K1/2 = (sr − sf)/sf. It can be clearly seen that the crystals with larger L value have higher Nd3+ concentration of unit quenching ratio. NdAl3(BO3)4 crystal has a large value of L and so the quenching effect is very weak. It has been demonstrated by experiment that this crystal is a good material for microchip laser [32–36]. To study the relationship between the concentration quenching strength with the chemical composition of the crystals, the situation when the resonant energy transfer condition cannot be satisﬁed should also be discussed. The single-phonon-assisted energy transfer probability can be calculated by (9.31) and (9.32) for the cases of the energy mismatch is large and small, respectively. It can be seen from these formulas that the key quantities are @V @V f ¼ k k ; g ¼ k k @Q @Q and phonon velocity v. The probability of energy transfer is proportional to (f − g)2 and inversely proportional to v5 or v7. In order to have a weaker cross-relaxation, the magnitude of f and g should be small and the phonon velocity v should be high. It has been pointed out [30] that the weak crystal ﬁeld leads to a small magnitude of f and g as well as the difference between them. Consequently, it is important to investigate the chemical composition of Nd3+-doped laser crystals in which Nd3+ ions experience a weak crystal ﬁeld as well as a high phonon velocity. What are the relations of the parameter L with crystal ﬁeld strength and the velocity of phonon? If the radius r+ of the ligand directly connected to Nd3+ ion is smaller but r- of the cations is larger, and the difference of the electronegativity Dx between the cation and the anion is smaller, then the parameter L = r−/(r+Dx) will assume a larger value. In this case, the polarization effect of the cations on the ligand will be stronger. It means that the ligands of the Nd3+ ion will have a smaller effective charge. It is easy to realize that it corresponds to a weak crystal ﬁeld as well as a smaller variation of the crystal ﬁeld potential with the movement of normal

306

9

Energy Transfer and Migration Between Ions

Table 9.2 Relation of parameter L with Nd3+concentration of unit quenching ratio Rq Crystal

Space group

NdAl3(BO3)4 (NAB)

D73-R32 C62h-C2/c C62h-C2/c C52h-P2/c C64h-I41/a C53v-R3m D46h-63/mmc

LiNd(PO3)4 NaNd(PO3)4 NdP5O14 NaNd(WO4)4 K5Nd(MoO4)4 NdMgAl11O19

L = R−/R+Dx

Nd3+ number of unit quenching ratio (1021/cm3)

4.3

2.17

2.7

1.62

2.7

1.55

2.7

1.56

1.5

0.95

1.5

0.75

1.2

0.25

coordinates so that a smaller value of f − g. On the other hand, the phonon velocity is inversely proportional to the square root of the compressibility of material while the compressibility of the ionic crystal is decreased with the decrease of ion–ion spacing and the increase of electrovalence [37] (the increase of cation valence corresponds to its electronegativity closer to the electronegativity of anions [38]). Therefore, for the same oxide (the same r−), the smaller cation radius r+ and smaller electronegativity difference (a larger parameter L) corresponds to a weak crystal ﬁeld (a smaller f − g) and a smaller a compressibility (a higher phonon velocity) of the host material, that is, a lower phonon-assisted energy transfer probability as well as a lower cross-relaxation probability and therefore a weak fluorescence concentration quenching effect of Nd3+ ions. Of course, the concentration dependent fluorescence quenching is an effect conditioned by many factors; a qualitative parameter cannot be used to describe all the aspects. However, when we discuss the influence of the chemical composition on the effect of fluorescence quenching, parameter L is a useful qualitative parameter.

References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10.

T. Forster, Ann. Phys. 255 (1948) T. Forster, Z. Naturforsch. A4, 321 (1949) D.L. Dexter, J. Chem. Phys. 21, 836 (1953) R. Obach, in Optical Properties of Ions in Crystals, ed. by H.W. Moos, H.M. Crosswhite (Wiley-Interscience, New York, 1967) T. Miyakawa, D.L. Dexter, Phys. Rev. B 1, 2961 (1970) F. Auzel, in Luminescence of Inorganic Solids, ed. by B. DI Barstool (Plenum, New York, 1978) F. Auzel, in Radiationless Processes, ed. by B. Di Bartolo, V. Golberg (Plenum, New York, 1980) F. Auzel, in Spectroscopy of Solid-State Laser-Type Materials, ed. by B. Di Bartolo (Plenum, New York, 1987) G. Blasse, in Radiationless Processes, ed. by B. Di Bartolo, V. Golberg (Plenum, New York, 1980) G. Blasse, in Spectroscopy of Solid-State Laser-Type Materials, ed. by B. Di Bartolo (Plenum, New York, 1987)

References

307

11. W.M. Yen, in Spectroscopy of Solids Containing Rare Earth Ions, ed. by A.A. Kaplyanskii, R.M. Macfarlane (North-Holland, Amsterdam, 1987) 12. T. Holstein, S.K. Lyo, R. Orbach, in Laser Spectroscopy of Solids, ed. by W.M. Yen, P.M. Selzer (Springer, Berlin, 1981) 13. B. Henderson, G.F. Imbusch, Optical Spectroscopy of Inorganic Solids (Clarendon Press, Oxford, 1989) 14. M. Yamada, S. Shionoya, T. Kushida, J. Phys. Soc. Jpn. 32, 1577 (1972) 15. J.M. Colins, B. Di Bartolo, J. Lumin. 69, 335 (1996) 16. F. Auzel, Y.H. Chen, J. Lumin. 66&67, 224 (1996) 17. M. Inokuti, F. Hirayama, J. Chem. Phys. 43, 1978 (1965) 18. F. Spitzer, Principles of Random Walk (D. Van Nostrand, Princeton, 1964) 19. E.W. Montroll, J. Math. Phys. 6, 167 (1965) 20. A.I. Burshtein, Sov. Phys. JEIP 35, 882 (1972) 21. I.R. Martin, V.D. Rodriguez, U.R. Rodriguez-Mendoza et al., J. Chem. Phys. 111, 1191 (1999) 22. M. Yokota, O. Tanimoto, J. Phys. Soc. Jpn. 22, 779 (1967) 23. D.L. Huber, Phys. Rev. B 20, 2307 (1979) 24. J. Hegarty, D.L. Huber, W.M. Yen, Phys. Rev. B 23, 6271 (1981) 25. F. Auzel, in Spectroscopic Properties of Rare Earths in Optical Materials, ed. by G. Liu, B. Jacquier (Springer, Berlin, 2005), p. 267 26. J.S. Liao, Y.F. Lin, Y.J. Chen et al., J. Opt. Soc. Am. B 23, 2572 (2006) 27. P. Wang, J.M. Dawes, P. Dekker, et al., J. Opt. Soc. Am. B 16, 63 (1999) 28. A.A. Kaminskii, Laser Crystal (Springer, Berlin, 1980) 29. F. Auzel, Mat. Res. Bull. 14, 223 (1979) 30. Z.D. Luo, Commun. Fijian Inst. Res. Struct. Matter (1), 1 (1976) (in Chinese) 31. Z.D. Luo, A.D. Jiang, Y.C. Huang et al., Sci. China (Ser. A) 34, 762 (1991) 32. D. Jaque, O. Enquitra, S.J. Gacia, et al., App. Phys. Lett. 76, 2176 (2000) 33. D. Jaque, O. Enguita, U. Caldino, et al., J. App Phys. 90, 561 (2001) 34. Z.D. Luo, Y.D. Huang, M. Montes et al., App. Phys. Lett. 85, 715 (2004) 35. E. Bovero, Z.D. Luo, Y.D Huang., et. al. App. Phys. Lett. 87, 211108 (2005) 36. M. Montes, D. Jaque, Luo Zundu. Opt. Lett. 30, 397 (2005) 37. H.G.F. Winkler, Struktur und Eigenschaften der Kristalle (Springer, Berlin, 1955) 38. C.A. Coulson, Valence (Oxford University Press, London, 1961)

Chapter 10

Laser and Physical Properties of Materials

After the study of basis rules of radiative and non-radiative transition and main spectral properties of the materials, it is necessary to investigate the relationship between the laser performance and the physical properties of the materials and to realize the requirements of laser devices on the material properties. To this end, it is useful to give an outline of fundamentals of solid-state laser, although the detailed discussion is not in the scope of this book.

10.1

Brief Introduction of Solid-State Laser Principle

There are two types of energy level system of solid-state laser that have been generally used, that is, the so-called three-level system and four-level system. Figure 10.1 is a schematic diagram of their energy levels. In the three-level system, the energy levels of laser operation are the absorption band, the upper laser level, and the lower laser level. The active ions absorb the pump light and transit to absorption band then non-radiative decay to the upper laser level. The radiative transition between the upper laser level and the lower laser level emits the radiation at laser wavelength. In order to generate laser emission, the laser material must be placed in a laser resonator and the intensity of pump light should be strong enough to produce enough population inversion between the upper and the lower laser levels, so that the gain of the medium at laser wavelength is enough to compensate for its losses. The probability of the stimulated radiative transition is proportional to the photon number of the same resonator mode in the resonator. Therefore, the avalanche-like increase of the photon number will generate radiation with high intensity, high monochromaticity, high coherence, and high directionality, that is, the laser emission. The difference between the four-level system and the three-level system is in the lower laser level. Different from the three-level system, the low laser level of four-level system is not its ground state. Typical example of the three-level system is ruby Cr3+:Al2O3; its energy level and © Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8_10

309

310

10 Laser and Physical Properties of Materials

Fig. 10.1 Schematic diagram of three-level system and four-level system of laser

relaxation

pumping

relaxation

pumping

lasing

lasing

relaxation

Four−level system

Three−level system

spectral properties have been discussed in Chap. 7. On the other hand, there are many examples of four-level system. The neodymium-doped yttrium-aluminum garnet Nd3+:Y3Al5O12(Nd3+:YAG) is a typical crystal which has been widely used in laser technique. Whether the three-level systems or the four-level systems, the ﬁrst condition for the laser emission is the pumping should be strong enough to make the laser material become an optical gain medium. The early solid-state lasers usually used rare gas discharge lamps as pump sources (flash lamp is used in the pulse excitation while in the continuous excitation the arc lamp should be used). Laser material and straight tubular pumping lamp are usually placed in two focus lines of the elliptical cylindrical light condenser having inner surface coated with gold ﬁlm or silver ﬁlm of high reflectivity. Owing to the fact that the emission spectra of the pump light and the absorption spectra of the laser material cannot match well and the gathering efﬁciency of light is difﬁcult to reach 100%, the pumping efﬁciency is always too low. On the other hand, the unwanted radiation of pumping lamp always rise the temperature of the laser material. Figure 10.2 is a schematic diagram of a solid-state laser. The pump source used is a semiconductor laser (LD), which is an efﬁcient pumping method not producing too much heat and can keep the good performance of laser material at a lower temperature. The rear mirror in Fig. 10.2 is usually in the form of dielectric ﬁlm deposited directly on the surface of the laser material. It has high transmission at the

LD light condenser

rear mirror

laser crystal

Fig. 10.2 Schematic diagram of a solid-state laser pumped by LD

front

10.1

Brief Introduction of Solid-State Laser Principle

311

wavelength of pumping light but high reflectivity at the laser wavelength. The output mirror (front mirror) should have certain amount of transmission at the laser wavelength to output laser emission. If the reflectivity of the rear mirror and front mirror at the laser wavelength is R1 and R2, respectively, then the laser light with intensity I0 will become I0R1R2 = Ie−2(−1/2lnR1R2) after back and forth reflection between the rear mirror and the front mirror. By using loss coefﬁcient c′ = -ln (R1R2)1/2 the laser intensity can be expressed as I = I0e−c′. If R is written as R (R1R2)1/2, in the case of small output coupling -lnR 1–R, that is, the output loss c′ = 1–R. Besides the scattering loss of the optical resonator, there are the absorption and scattering of the impurities and defects that existed in the materials. All these losses can be represented by b. Therefore, the total loss is c ¼ 1 Rþb

ð10:1Þ

Photon lifetime in a laser cavity is a conception commonly used in laser science and technology, and it can be measured by the time the laser intensity in the cavity decay to e−1 of its original intensity. By the above discussion it is obvious that passing through the resonant cavity for one time, the laser light intensity I0 will be attenuated from I0 to I0e−c. After a period of time t, the distance traveled by the light is ct/n (n is refractive index of laser material). If the length of the laser material is L, then in the period of time t the laser light pass through the resonant cavity ct/nL times, so that the laser light decays into ctc I ¼ I0 ðec Þct=nL ¼ I0 exp nL

ð10:2Þ

Obviously, the photon lifetime in the laser cavity is sc ¼

nL cc

ð10:3Þ

The quality factor Qc of resonator is deﬁned as the 2p times of the cycle number in which the energy in the cavity is consumed, that is, Qc = 2pm0I/(dI/dt). By using (10.2) and (10.3), it is obvious that nL ¼ 2pm0 sc cc

ð10:4Þ

2pm0 nL cQc

ð10:5Þ

Qc ¼ 2pm0 then c¼

Under the excitation of pump source, the inversion concentration between the upper and the lower laser levels is DN and so the laser material becomes a gain medium with its gain coefﬁcient ag proportional to DN

312

10 Laser and Physical Properties of Materials

ag ðmÞ ¼ a0g ðmÞDN rem ðmÞDN

ð10:6Þ

where a0g ðmÞ is the gain coefﬁcient for each inversion particle, that is, the emission cross-section rem of the laser material and by (5.66) of Chap. 5, it is rem ðmÞ ¼

c2 c2 AgðmÞ ¼ gðmÞ 2 2 8pm n 8pm2 n2 sr

ð10:7Þ

The condition of laser generation is obviously the product of the gain coefﬁcient ag multiplied by the material length L must be equal to or greater than the loss coefﬁcient c. By using (10.3), (10.6), and (10.7), one can obtain c3 DNsc gð m Þ 1 8 p n3 m 2 s r

ð10:8Þ

Among the various parameters of the above formula, from the angle of pump intensity, what can be changed only is DN. When DN reaches a value which can satisfy (10.8), it is said that the laser oscillation threshold is achieved, then the number of inversion particle per unit volume is called the threshold inversion concentration DNth, that is DNth ¼ In virtue of

R

8 p n3 m 2 s r c 3 s c gð m Þ

ð10:9Þ

gðmÞdm ¼ 1, approximately one has g(m) = 1/Dm, therefore DNth ¼

8 p n3 m2 Dmsr sr sf ¼p ¼p c3 sc sc s c gf

ð10:10Þ

where p ¼ 8 p n3 m2 Dm=c3 gives the mode density,sr is the radiative lifetime,sf is the fluorescence lifetime, and gf is the fluorescence quantum efﬁciency. The threshold pump energy and pump power for three-level system and four-level system will be studied in the following. For three-level systems, because the lower laser level is ground state, the particle number per unit volume on the upper laser level must be more than half of the total particle concentration, that is Nu ¼ N1 =2 þ DN where N1 is the active ion concentration in the ground state. Owing to the fact that N1 is several orders of magnitude greater than DN, one can approximately adopt Nu N1/2 and N1 simply is the doping concentration of active ion. For a four-level system, the lower laser level is not the ground state, at general temperature, its particle concentration can be neglected compared with the total

10.1

Brief Introduction of Solid-State Laser Principle

313

particle concentration in the medium; therefore, the particle concentration difference between the upper and the lower laser levels is that pumped to the upper laser level Nu = DN. In the case of pulse pumping, if the bandwidth of the pump pulse is shorter than the fluorescence lifetime then the threshold energy eth required by unit volume of the laser material is equal to the photon energy of the pumping light multiplied by the particle concentration that must be pumped. Owing to the fact that the active ions in absorption band and fluorescent energy level have both downward radiative and non-radiative transitions, therefore, if the particle number involved in the radiative transition of the upper laser level is n, then particles of n=g should be pumped into the upper laser level. Here g is the total quantum efﬁciency. g ¼ g1 g2 ; g1 denotes the quantum efﬁciency of absorption band and g2 is the quantum efﬁciency of the upper laser level, that is, the fluorescence quantum efﬁciency. Because usually one has g1 1, generally the approximation g g2 gf can be adopted, therefore the threshold energy is expressed as Eth ¼ eth V ¼

N1 hxp V 2gf

Eth ¼ eth V ¼

DNth hxp V gf

three-level system

ð10:11Þ

four-level system

ð10:12Þ

Substitute the expression (10.10) of DNth into (10.12), the relationship between the threshold energy and the spectral parameters for four-level system can be obtained as Eth ¼

psf hxp V sc g2f

ð10:13Þ

In the case of continuous pumping, below the threshold, the particle energy in the upper laser level is only consumed by spontaneous radiative transition and non-radiative decay in the time interval of fluorescence lifetimesf, therefore the threshold pumping power Pth = Eth/sf can be expressed as following for three-level system and four-level system, respectively Pth ¼ Pth ¼

N1 hxp V 2gf sf

three-level system

DNth hxp V phxp V ¼ gf s f sc g2f

four-level system

ð10:14Þ ð10:15Þ

Most of the pump energy (power) in the three-level systems is consumed in exciting half of the active ions in ground state to the upper laser level. Only beyond this threshold the excitation energy can be converted into laser energy. Comparing with N1/2, DNth can be completely neglected; therefore, the laser threshold of the

314

10 Laser and Physical Properties of Materials

four-level systems is much lower than that of the three-level systems. Moreover, the four-level systems can operate continuously, but the three-level systems can only operate in the pulse mode. The expressions of laser energy, power, and efﬁciency of four-level system are derived as follows. Assuming the energy for exciting the active ions to the upper laser level is E, then after deduction the energy Eth consumed in the generation of threshold particles, energy E–Eth will be transferred into laser energy. However, the energy consumed in the non-radiative decay also should be taken off; that is, the laser energy obtained should be multiplied by the luminescent efﬁciency gf . Therefore EL ¼

psf hxp V E 1 Eth s c gf

ð10:16Þ

Similarly, it can be concluded that the laser power output in the case of continuous pumping is PL ¼

phxp V P 1 Pth s c gf

ð10:17Þ

Owing to the fact that reflectivity of the rear mirror and the front mirror at laser wavelength is R1 and R2, the output laser energy should be h i 1 R2 Eout ¼ EL ð1 R2 Þ 1 þ R1 R2 þ ðR1 R2 Þ2 þ ðR1 R2 Þ3 þ ¼ EL 1 R2

ð10:18Þ

where R (R1R2)1/2. Similarly, the output laser power is Pout ¼ PL

1 R2 1 R2

In order to have a higher laser output energy or power, obviously EL or PL has to be as high as possible. From the point of view of device design, it is necessary to reduce cavity loss and making R1 as close to 1 as possible, while in the case of high pumping energy and power, R2 has to be appropriately increased. On the other hand, Eth and Pth should be as low as possible for laser material. Section 10.2 will start from this point to discuss the quality factor of laser material. In recent years, a new pumping method has been adopted for some Nd3+ laser crystals, such as Nd3+:YVO4 and Nd3+:YAG; that is directly pump up the active ions to the upper laser level 4F3/2 of Nd3+ion [1, 2]. The main advantage is that it can reduce the heat generated during the operation of laser. This problem will be further analyzed in Sect. 10.4. It should be pointed out that because the energy level of absorption band is the upper laser level, the number of energy levels involved in laser operation is less than that of the original four-level system, whether it is a 1.06 nm laser or a 946 nm laser. However, from the angle of the population

10.1

Brief Introduction of Solid-State Laser Principle

315

inversion and the threshold calculation formula, the former is identical to the four-level system which has been analyzed above, but the latter must be analyzed and calculated by using the quasi three-level system. A typical example of a quasi three-level system is Yb3+ laser material. It has become a hot spot in the development and application study of solid laser materials after the development of semiconductor laser. Although this material has a higher threshold than that of the Nd3+ laser material but Yb3+ ion has simple energy level structure. Theoretically, there is no up-conversion and excited-state absorption and if there are no other rare earth impurities in the host, there will be no concentration quenching and its long fluorescent lifetime is beneﬁcial to energy storage. Moreover, the pump wavelength is close to the wavelength of laser emission, so that the heat loss of pump energy is very low. On the other hand, the broad emission and absorption spectra produced by the strong electron–phonon coupling between the Yb3+ ion and the medium are beneﬁcial to LD pumping, and the laser emission tuned in a wider wavelength range, which is conducive to the realization of ultrashort pulse laser output by mode-locked method to realize the laser output of ultrashort pulse. In recent years, the continuous laser power of Yb3+ laser has reached kilowatt level and its ultrashort pulse output to reach dozens femtosecond level is not difﬁcult. Their laser performance in many aspects has been reported in many literatures. Here it is not necessary to go into details. However, it should be pointed out that Yb3+ ion is a quasi three-level system. The high proportion distribution of particle in the lower laser level results in a high laser oscillation threshold; therefore, search for low threshold host material has become an important problem in material research. From the perspective of energy level structure, this requires a greater separation between the lower laser level (high crystal ﬁeld energy level of multiplet 2F7/2) and the ground state (lowest crystal ﬁeld energy level of multiplet 2F7/2); consequently, Yb3+ ion must be doped in the host material with strong crystal ﬁeld. The problem of how to ﬁnd the host material with strong crystal ﬁeld has been discussed by many authors from different angles. Here just want to point out that Nd3+ laser materials have a very rich data of crystal ﬁeld energy level, so one can use relationship between the total crystal ﬁeld splitting of the multiplet 4I9/2 of Nd3+ ion and the multiplet 2F7/2 of Yb3+ ion obtained by Auzel [3]: DE(2F7/2)1.6D(4I9/2) to ﬁnd the Yb3+ laser material with strong crystal ﬁeld from the Nd3+ laser material having strong crystal ﬁeld. In the Yb3+ ion laser system, the lower laser level is one crystal ﬁeld energy level of ground multiplet. There is also a certain absorption coefﬁcient (absorption cross-section) at the wavelength of laser emission. Obviously, laser gain cross-section should be deducted by the loss from the absorption at the same wavelength. If the particle number inversion ratio is f(f = DN/N0), the ratio of particle number remaining in the lower laser level to the particle number in the ground state is (N0–DN)/N0 = 1–f, then the gain cross-section for each inversion particle deducted by ground state absorption cross-section should be

316

10 Laser and Physical Properties of Materials

rg ðmÞ ¼ f rem ðmÞ ð1 f Þrab ðmÞ The inversion population DNth at laser oscillation threshold in this situation will be greater than that expressed in (10.10). The general method in this case is to calculate different rg values for different f numbers according to measured emission and absorption cross-sections and to investigate in what range of wavelength and what f value the inequality rg > 0 can be satisﬁed, as well as at what wavelength rg reach the maximum, from these data the wavelength of laser emission can be determined. Solid-state lasers emitting in the spectral range of 1.5 lm are very promising for eye-safe laser, range ﬁnding, ophthalmology, ﬁber-optic communication systems, and optical location. One of the effective ways to realize the laser emission of 1.5 lm band is using Yb3+ ion to sensitize Er3+ion. After Yb3+ ions efﬁciently absorb pumping energy at 967 nm and excited to multiplet 2F5/2, by the energy transfer of Yb3+!Er3+, Er3+ions are excited to their multiplet 4I11/2, then the upper laser level 4 I13/2 is populated by 4I11/2!4I13/2 non-radiative decay. Because Er3+ ion has many energy levels in the 4f conﬁguration, so that the existent excited-state absorption, up-conversion, and cross-relaxation as well as Er3+!Yb3+ back energy transfer processes will produce the deexcitation of 4I11/2 and 4I13/2 multiplets. Therefore, ideal 1.5 lm laser material must be the Yb3++ Er3+-doped crystals with short 4I11/2 fluorescence lifetime and higher thermal conductivity. This is the reason why the Yb3+ + Er3+:RAl3 (BO3)4(R = Y, Gd, Lu) crystals with high phonon energy have been realized as high efﬁciency 1.5 lm laser crystal [4–14]. The 1.5 lm continuous laser output with power up to 1 W and low noise laser of power 100 mW has been realized in this type of crystal. The nanosecond, picosecond, and femtosecond short pulse laser output are also realized by Q switch and mode lock method [15–18].

10.2

Quality Factor of Solid-State Laser Materials

It can be seen from previous discussion that to evaluate the performance of a laser material, it should be judged that when the cavity loss is minimum whether it has low threshold power Pth or low threshold energy Eth, and whether it can absorb more energy or power from pumping sources. Therefore, one should start with threshold optical power flux /th to investigate which material’s physical properties make pump threshold optical power flux /th smaller, The power absorbed by the laser material per unit volume should be equal to the power consumed at threshold DNth hxp =sf , that is /th rp N1 ¼ where rp is absorption cross-section, then

DNth hxp sf

10.2

Quality Factor of Solid-State Laser Materials

/th ¼

317

DNth hxp sf rp N1

By using (10.10), the following can be obtained /th ¼

DNth hxp p hx p ¼ sf rp N1 sc rp gf N1

ð10:19Þ

By (10.7) and the formula of mode density given above, the emission cross-section can transform into rem ¼

c2 n AgðmÞ ¼ cpsr 8 p m 2 n2

Then the mode density is expressed as p¼

n crem sr

In this way, the threshold optical power flux is /th ¼

hxp n csc rp N1 sf rem

ð10:20Þ

The second factor n/rpN1sfrem in the above formula only relates to the inherent properties of laser materials, and so the quality factor M of laser material can be deﬁned as M¼

rp N1 sf rem n

ð10:21Þ

Obviously, the laser material having large M value has a lower laser threshold. The laser technology generally uses the product sfrem to evaluate the laser threshold; for example, the comparison of related properties of ﬁve laser crystals was listed by Loutts [19], as shown in Table 10.1.

Table 10.1 Comparison of spectral properties of several laser crystals Crystal (cm2s)

Emission cross-section rem (cm2)

Fluorescence lifetime sf (s)

Product lose sfrem (cm2s)

Nd:BFAP Nd:SFAP Nd:YVO4 Nd:YAG Nd:YAB

>5 10−19 5.4 10−19 10.5 10−19 3.04 10−19 10 10−19

3.7 10−4 2.98 10−4 9.8 10−5 2.7 10−4 2.0 10−5

>1.85 10−22 1.61 10−22 1.03 10−22 8.3 10−23 2.0 10−23

318

10 Laser and Physical Properties of Materials

If the concentration N1 of doping ion and the absorption cross-section rp have not much difference, it is possible to use the above product to compare the performance of different laser materials. Some authors [20] used rpN1sfrem as quality factor of laser performance. Because most laser materials have little difference in refractive index, the quality factor without refractive index can also be used. To compare laser performance under the excitation of semiconductor laser, the absorption cross-section rp at pumping wavelength can also be replaced by the absorption peak area Ap at pumping wavelength, it is due to the fact that the emission wavelength of semiconductor laser will change with the temperature, so that the wider linewidth of absorption peak at pumping wavelength is to help the stability of laser output. Therefore, the quality factor of the laser performance of the material can be written as M¼

Ap N1 sf rem ; or M ¼ Ap N1 sf rem n

ð10:22Þ

Although the product sfrem of some laser materials is not very large, but their laser performances are still better than those of the materials with larger product of sfrem. For example, for the Nd3+:YAG crystal, the sfrem is 1.63 times that of the Nd3+:KGd (WO4)2 (Nd3+:KGW) crystal, but its Nd3+ ion concentration is only 1/3 of that of the Nd3+:KGW crystal. On the other hand, the pumping light absorption performance of the Nd3+:KGW crystal is better than that of the Nd3+:YAG crystal. The linewidth of absorption peak at 809 nm of the former is three times that of the latter, although the height of absorption peak of the latter is 1.1 times that of the former [21]. From these data it can be predicted that the laser performance of the Nd3+:KGW crystal is better than that of the Nd3+:YAG crystal. To conﬁrm this statement, many experiments [22–27] have shown that the laser performance of Nd3+:KGW crystal is better than that of the Nd3+:YAG crystal, whether it is pumped by LD or flash lamp and whether the laser output wavelength is 1067 or 1350 nm. Certainly, owing to the fact that Nd3+:YAG crystal has far superior thermal performance and so can keep the same performance in high energy or power level but the laser performance of Nd3+:KGW crystal will be deteriorated rapidly with the increase of power or energy and can only be applied to the range of medium and low power. Thermal–optical properties of laser crystals will be discussed in Sect. 10.4.

10.3

Relationship Between Laser Threshold and Chemical Composition of Host Materials

In recent years, the output power of semiconductor laser (LD) is increasing rapidly, they generate laser emission with many different wavelengths, and the price is dropping rapidly. It promotes the rapid development of LD pumped solid-state lasers and puts forward the new requirements of relevant laser materials.

10.3

Relationship Between Laser Threshold …

319

From the point of view of material science, undoubtedly, it is necessary to understand the special requirements of the structure and chemical composition of laser material. Nevertheless, each parameter of laser or spectral performance is related to the static spatial structure of the crystal as well as the lattice vibration and the electron motion of the crystal; therefore it is very difﬁcult to obtain a quantitative relation theoretically. A practical and feasible method is to analyze the relationship of the laser-related performance of the material with their atomic and bonding parameters, in order to build a bridge between the important parameters of laser performance and the chemical composition of laser materials. A qualitative empirical relationship of the laser threshold with the atomic parameters of host crystal which was obtained by the authors [28] will be described in this section. It can be seen from (10.20) that continuous laser threshold is inversely proportional to the product of stimulated emission cross-section rem and fluorescence lifetimesf. The relationship of the product remsf with crystal refractive index and fluorescence spectral linewidth will be analyzed in the following, to ﬁnd the relations of optical and spectral parameters with the atomic parameters of host crystal and then to discuss the possible effect of the chemical composition of host crystal on the threshold of laser oscillation. From (5.66) of Chap. 5 and the relationship between spontaneous emission probability A, fluorescence lifetime sf, and fluorescence quantum efﬁciency gq ; that is, A ¼ gq =sf , it can be shown that rem sf ¼

gq c 2 gð m Þ 8pm2 n2

Substituting the formula of Gauss or Lorentz line shape function g(m) given in Chap. 6, then rem sf /

gq 2 n Dm

ð10:23Þ

From this expression it can be seen that large remsf value is related to high fluorescence quantum efﬁciency and narrow emission linewidth as well as small refractive index of host material. In order to have high fluorescence quantum efﬁciency, electron–phonon interaction should not be strong and the effective phonon energy should not be high. On the other hand, the contribution to the emission linewidth comes from the effects of lattice vibration and the inhomogeneous of crystal ﬁeld. Except for the group consisting of the atoms with very small mass, such as the borate group BO3 having especially high vibrational frequency, the difference of phonon frequency for different oxide materials is within two times while the different fluorides have a slightly different but much lower phonon frequency. Weaker crystal ﬁeld will generally lead to weaker electron–phonon interaction and higher fluorescence quantum efﬁciency. If crystals have roughly the same integrity, it also corresponds to a narrower inhomogeneous line broadening. At the temperature of laser operation, the contribution to the thermal line

320

10 Laser and Physical Properties of Materials

broadening mainly comes from Raman process; its thermal linewidth can be expressed by (6.77) and (6.78) of Chap. 6. It can be seen that the thermal linewidth is proportional to the fourth power of the mass difference factor D. It is difﬁcult to ﬁnd out the quantitative relationship between the structure and the refractive index of material; however, if one can discover some qualitative relationship between refractive index and such as the parameters of ionic mass, ionic radius and electrical negativity, it will be helpful to the research of new materials. As is well known, the refractive index of material is the square root of the following dielectric tensor eik ¼ e0 dik þ a1 uik þ a2 ull dik

ð10:24Þ

where e0 is the dielectric constant without strain. The second and the third terms in the above equation are the dielectric tensors related to the strain of material, while uik is deﬁned as 1 @ui @uk uik ¼ þ 2 @Xk @Xi

ð10:25Þ

where ui and uk are different components of particle displacement vector. Refractive index can be expressed as the following expression if one does not concern its anisotropy e ¼ e0 þ a

@u @R R¼0

ð10:26Þ

The ﬁrst term in the above expression is the polarizability contribution of the original dipole of material which is proportional to original dipole moment. With the increase of the cationic radius r+ the polarizability of the cation increases and with the increase of atomic number in the same family of periodic table, the polarizability of cations also increases. (Note that with the increase of the atomic number in the same family of periodic table, the electrical negativity difference Dx between cation and anion is increased.) On the other hand, the polarizability of chemical bond is an increasing function of the difference Dx. Therefore, parameter G = Dxr+ can be used to measure the dielectric constant e0, that is e0 is an increasing function of G. The effect of the difference of host ion mass will be considered as follows. If the host material is composed of the ions with the same mass, then

@u i X ¼ pﬃﬃﬃﬃﬃ kQðkÞ @R R¼0 M k;

ð10:27Þ

where M = Nm is the total mass of host material, while N, k, R, and Q(k) are total particle number, phonon wave vector, coordinate, and canonical coordinate of lattice point, respectively. The material, in fact, is generally composed of two or

10.3

Relationship Between Laser Threshold …

321

more than two kinds of ions with different masses. If there are N molecule formula units in the material and each molecule formula unit has n = na+nb ions, in which na ions with mass of ma and nb ions with mass of mb while the total mass of the material is M = N (nama+nbmb). Referring to (10.27), the average strain of the material as that taken in Chap. 6 will be " # X @u i na nb pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ þ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ¼ kQðkÞ @R R¼0 n Nnma Nnmb k

ð10:28Þ

The above expression can also be written as

@u iD X ¼ pﬃﬃﬃﬃﬃ kQðkÞ @R R¼0 M k

ð10:29Þ

where D is the mass difference factor of host material given in Chap. 6. Obviously, the second term of the expression (10.26) of dielectric constant is proportional to D. In summary, the dielectric constant e0 increases with the parameter G, while the second term of (10.26) increases with the increase of parameter D. The dielectric constant e and the refractive index of the material with the same anion will be decreased with the increase of parameter P = r−/GD = r−/(r+DxD) = L/D (where L = r−/(r+Dx) is given in Chap. 9). The refractive index data of oxide compound shown in Fig. 10.3 demonstrate that the refractive index is a decreasing function of P. From the previous discussion, a conclusion can be drawn that a larger P value generally corresponds to a lower refractive index and a narrower fluorescence linewidth. Then by (10.23) it can be seen that it results in a larger product of fluorescence lifetime and emission cross-section. This is conﬁrmed by the data of 12 laser crystals doped with Nd3+ ion shown in Fig. 10.4. In the calculation of parameter P, the value of r−/G = r−/(r+Dx) (i.e. the parameter L) must take the

n

Fig. 10.3 Refractive index as a function of parameter P. The curve in the ﬁgure is a ﬁtting curve

2.7 Bi4Ti3O12 2.6 Bi12TiO20 Bi12SiO20 2.5 2.4 BaTiO3 2.3 La2Ti2O7 2.2 PbMoO4 BNN LN KN 2.1 YVO4 2.0 GGG YAP 1.9 CaWO4 YGG YAG 1.8 GCOB YAB 1.7 YCOB 1.6 BBO LBO 1.5 0.2 0.4 0.6 0.8 1.0 1.2 1.4 1.6 1.8 2.0 2.2 2.4 2.6 2.8 3.0 3.2 3.4

P

322

10 Laser and Physical Properties of Materials 11 YVO4

10 9

σeτf (X10-23cm2s)

Fig. 10.4 The product of sfrem as a function of the parameter P. The curve in the ﬁgure is a ﬁtting curve

8 7

GdVO4

6 YAG

GGG

5 4 GSGG

3 2 1 0.4

KGW

KYW YGG

KYM

YAP

Y2O3

NGW

0.5

0.6

0.7

0.8

0.9

1.0

1.1

1.2

P

average value of the simple molecule formula units contained; for example, in the Y3Al5O12 crystal, its molecular unit can be considered as a complex oxide molecular unit consisting of 3/2 Y2O3 unit and 5/2 Al2O3 unit, altogether four simple oxide molecular units, so the average of L is LðY3 Al5 O12 Þ ¼ ½1:5 LðY2 O3 Þ þ 2:5 LðAl2 O3 Þ 4

10.4

Thermo-Mechanical and Thermo-Optical Properties of Solid-State Laser Materials

It has been mentioned in previous section that in high power or high energy application, the laser performance of YAG crystal is better than that of the KGW crystal. This is because the laser performance of KGW crystal but not the YAG crystal is rapidly deteriorated when the temperature is increased. In order to ﬁnd out its reason, the effect of thermal properties of materials on the laser performance should be studied. In general, the going up of temperature will widen the fluorescence linewidth and shorten the fluorescence lifetime, and thus increase the laser threshold and decreases the laser output efﬁciency. On the other hand, the non-uniform temperature distribution in laser crystal will produce thermal stress, thermal birefringence, and thermal lens effects. First, see the heat produced in the laser operation. Take four-level system as an example; transition from absorption band to the upper laser level is a non-radiative decay process, and part of excited electronic energy is transferred to the heat of host material. There are radiative and non-radiative ways for the transition from the upper laser level to the lower laser level and the proportion of non-radiative decay is calculated by the following formula

10.4

Thermo-Mechanical and Thermo-Optical …

Wnr ¼ 1 gq Wr þ Wnr

323

ð10:30Þ

where Wnr, Wr, and gq are non-radiative decay rate, radiative transition rate, and fluorescence quantum efﬁciency, respectively. Obviously, the higher the fluorescence quantum efﬁciency, the less the amount of heat generated by non-radiative decay. The transition from the lower laser level to ground state is also a non-radiative decay process; the excited energy will all be changed to heat energy. If the pump frequency is xp (wavelengthkp), laser frequency is xl (wavelengthkl), fluorescence quantum efﬁciency is gq , neglecting the spontaneous emission light energy scattered out of the laser cavity, then the percentage of pump energy converted to the heat energy (thermal loading) is pt ¼

x p gq x l gq kp ¼1 xp kl

ð10:31Þ

This formula is only applicable to the operation level near threshold. When operation level much higher than the threshold, the radiative transition rate from the upper laser level to the lower laser level is much higher than the non-radiative decay rate between these two levels. The heat generated by non-radiative decay can be ignored. However, the volume of the pumping area in the laser material is often larger than that of the laser oscillation. In this case to calculate the overall thermal loading, the fluorescence quantum efﬁciency gq in (10.31) should be replaced by the ratio of the volume of laser oscillation to the volume of pump area. If these two volumes are well coincident, a value close to 1 can be adopted, even if its fluorescence quantum efﬁciency gq is low. The percentage of pump energy converted to heat energy by different pump methods can be estimated. For example, the Nd3+ ion activated crystal or glass pumped by 805 nm semiconductor laser. Suppose in (10.31) gq ¼ 90%, then for the laser emission at 1064 nm, it can be calculated that the heat energy generated is 32% of the pump energy. If the same laser material pumped by rare gas discharge lamp, assuming that the average pumping wavelength is 590 nm, then the similar calculation shows the heat energy generated is 50% of the pump energy. If directly pumped to the upper laser level 4F3/2 is adopted, and supposing the pumping wavelength is 880 nm, then the thermal loading is reduced to 25%. Obviously, the higher the fluorescence quantum efﬁciency and the closer the pump band to the upper laser level, the lower is the thermal loss. Moreover, the lower thermal load of laser material will reduce the limitation of laser output by thermal lens effect, thermal broadening of emission spectral line, and shortening of fluorescence lifetime. For example, the NAB crystal, pumped by laser at wavelength 750, 808 nm and directly pump to the upper laser level 4F3/2 at 882 nm, the slope efﬁciency of laser output are 34, 50, and 70%, respectively [29]. For the 946 nm laser operation of Nd3+:YAG crystal, the advantage of direct pump to the upper laser level is even greater. It has been mentioned that the pump wavelength is close to the laser wavelength for Yb3+-doped laser material, and so the thermal loss of pumping

324

10 Laser and Physical Properties of Materials

light is low. Yb3+:YAG crystal lasers at 1030 nm and diode-pumped at 943 nm, the theoretical thermal loading is pt = 0.09, its thermal loading is lower than half of the thermal loading of the directly pumped 1064 nm laser of Nd3+:YAG. The non-radiative center in laser material and the concentration quenching of active ion will consume the excitation energy and transfer the energy to the heat of host material. Moreover, because of the presence of unwanted impurity ions or other absorption centers in the materials, some of the laser energy can also be converted into heat; all these will further increase the thermal loading of laser material. Another way to generate heat in laser operation is the up-conversion of laser upper level. When pump power is low, the probability of up-conversion is very low and the effect of up-conversion on fluorescence quantum efﬁciency and heat production can be neglected, but at a high pumping level, this effect must be considered. Jacinto et al. [30] used experiment of thermal lens to study the effect of energy transfer-assisted up-conversion (ETU) process on the fluorescence quantum efﬁciency of NAB crystal and conﬁrmed that the effect of up-conversion on fluorescence quantum efﬁciency and thermal loading cannot be neglected at high pumping level. However, it should be pointed out that there are still some problems in the calculation of that paper and it should be reconsidered. For example, in their formula (7) the fluorescence quantum efﬁciency gq at high power pumping level was expressed as gq ¼

g0 1 þ bne

where g0 and bne are the fluorescence quantum efﬁciency at low power pumping level and the effect of up-conversion on this efﬁciency, respectively. However, as has been mentioned, at a high power laser operation level, because of the stimulated emission transition probability is proportional to laser intensity, so the actual quantum efﬁciency is much higher than the fluorescence quantum efﬁciency measured by spectroscopic measurements and also related to the pumping power level, but this fact has not been taken into account. On the other hand, a portion of the excitation energy carried away by the up-conversion process is changed to the light of other wavelengths but not the thermal energy. To correctly calculate gq , the spectra emitted by the up-conversion process must be measured. Of course, the effect of this process on the fluorescence quantum efﬁciency and the heat generation is really a problem that should be studied. Anyhow, the thermal problems in laser operation cannot be ignored. In addition to a considerable part of pump energy change into thermal energy, there is some radiation losses; that is the spontaneous emission loss outside divergence angle of laser emission and the diffraction losses of laser cavity. The proportional relation between the thermal power generated and the output laser power can be expressed as follows [31]

10.4

Thermo-Mechanical and Thermo-Optical …

PQ ¼ vq Pout ¼ pq V

325

ð10:32Þ

where pq is the thermal power production per unit volume. The typical value of vq is between 1 and 4. Thermal energy generated in the process of laser operation will rise the temperature of laser material. According to thermodynamic formula, the thermal energy generated and the rise of temperature per second can be expressed as the following expression @Q ¼ Cp [email protected]

ð10:33Þ

where Q, Cp, and q denote the thermal energy, the speciﬁc heat at constant pressure, and the density of a material, respectively. If there is a temperature gradient in x direction, according to the continuity equation of heat flow, the following equation can be obtained @Q ¼

@T pq V þ KAc @t @x

ð10:34Þ

In the right-hand side of the above equation, the ﬁrst term is the thermal power generated during the laser operation in the laser medium with volume V and sectional area Ac and the second term is the thermal power transferred into the volume V which is the product of the thermal conductivity K, the sectional area Ac, and the temperature gradient ∂T/∂x. Remembering that ∂V/∂x = Ac, deriving the formulas (10.33) and (10.34) with respect to x and equating the two expressions obtained, then the following partial differential equation is resulted @T vPout K @2T ¼ þ @t Cp q @x2 Cp qV

ð10:35Þ

In general, ∂2T/∂x2 should be replaced by spatial temperature gradient ∇ T = (∂2/∂x2 + ∂2/∂y2 + ∂2/∂z2)T, so the following equation is obtained 2

@T vPout ¼ þ jr2 T @t Cp qV

ð10:36Þ

where thermal diffusion coefﬁcient j is expressed as j¼

K Cp q

ð10:37Þ

Let’s discuss the steady temperature distribution in x direction of a slab-shape laser crystal. The sectional area of the crystal perpendicular to the direction x is Ac, the slab has a length l in z direction, width w in y direction, and thickness 2d in x direction, that is, the coordinates of x direction of the slab center, the upper

326

10 Laser and Physical Properties of Materials

interface, and the lower interface are 0, d, and -d, respectively. The upper and the lower sides of the slab are cooled by flowing cooling liquid or gas. The pump light uniform illuminates the slab along x direction from the upper and the lower sides. By solving differential (10.15) with boundary condition T = Tc for j xj [ d þ dl, the following temperature distribution in x direction of the laser slab can be obtained [31]

T ð xÞ ¼

8 x2 > T þ DT þ DT 1 > 2 c s 0 < d Tc þ DTs 1 > > : Tc

jxd j dl

x d d j xj d þ dl j xj [ d þ dl

ð10:38Þ

Between the slab surface and cooling medium, there is a temperature linear transition layer of thickness dl, which depends on surface parameters, coolant parameters, and flow condition. By using the above equations, in a continuous pumping case, it can be shown that the temperature difference between the slab surface and the cooling medium is DTs = vPout(dl)2/VK and the steady-state temperature increase at x = 0 is DT0 = vPoutd/4wKl. If the laser material in the cooling medium at temperature Tc is a cylinder with radius r0 and length l, it is cooled by a liquid flowing along the cylinder surface, then the equation of heat flow will be 2 @T vPout @ T 1 @T ¼ þj þ @t @r 2 r @r Cp qV

ð10:39Þ

Solving this equation, the temperature distribution in the laser material can be obtained [31] 8 2 > < Tc þ DTs þ DT0 1 rr2 0 T ðr Þ ¼ T þ DT 1 rr0 c s > dl : Tc

r r0 r0 r r0 þ dl r [ r0 þ dl

ð10:40Þ

The meaning of DTs is the same as the above and DT0 is the steady temperature increase at r = 0. This function is shown in Fig. 10.5. The temperature is highest at the center of the rod, then gradually decreased toward the edge of the rod; it is a parabolic-type function. In the calculation of formula (10.40), the positive temperature value is adopted for the two opposite direction of the diameter. Let r2 T ¼ DTs =dl2 in (10.36), then DTs ¼

vPout dl2 pr02 lK

ð10:41Þ

10.4

Thermo-Mechanical and Thermo-Optical …

327

Fig. 10.5 Temperature distribution in the laser rod

T( r )

Tc 0

r0

r

Substitute (10.40) into (10.36) and consider that r2 T ¼ @@rT2 þ (10.36) and (10.39), it can be shown that 2

DT0 ¼

vPout r02 vPout ¼ 4KV 4 p lK

1 @T r @r

obtained by

ð10:42Þ

In the case of general pulse pumping, by solving time-dependent thermal conduction equation, it can be shown that after switching the pump light, DT0(t) will decrease with time according to the following formula t DT0 ðtÞ ¼ DT0 ð0Þexp s0

ð10:43Þ

where s0 ¼

r02 4j

ð10:44Þ

Consider that @ 2 T @r 2 þ r 1 @[email protected] DTs =dl2 and @[email protected] ¼ @DTs [email protected]: It can be shown that after switching the pump light, that is, the ﬁrst term in the right-hand side of (10.35) equal to zero, DTs(t) will be decreased with time according to the following formula t DTs ðtÞ ¼ DTs ð0Þexp ss

ð10:45Þ

where ss ¼

dl2 j

ð10:46Þ

It can be seen that the temperature increase DT0 (0) and DTs (0) as well as their decay times s0 and ss are inversely proportional to thermal conductivity K. For the

328

10 Laser and Physical Properties of Materials

solid-state laser materials,s0 andss are generally of the order of second. Obviously, for the high energy or high power laser applications, the laser materials should have high thermal conductivity. The period Dtp of pulsed laser pumping is generally shorter than 5 ms, that is, Dtp < wp The temperature distribution in the laser material can be expressed as [32] 8 2 r0 r2 pt Pin jab ejab z < ln w2p þ 1 w2p ; r wp T ðr; zÞ T ðr0 ; zÞ ¼ 2 4pK ð1 ejab l Þ : ln r02 ; r [ wp r

ð10:49Þ

10.4

Thermo-Mechanical and Thermo-Optical …

329

The temperature distribution along the radius is shown in Fig. 10.6. The thermo-optic effects on the laser properties of materials should be discussed next. First, the quantitative description of thermal stress and its physical effects must be made; this involves the concepts of stress and strain in physics. If the plane with normal direction x of an object is subjected to the action of force along direction x, then the stress of the plane per unit area is referred to as rxx and it will result in the elongation of the object in the x direction. The strain exx is deﬁned as normalized length variation dl/l. According to Hooke’s law, the stress rxx is proportional to the strain exx, that is rxx ¼ EY exx or exx ¼

rxx EY

ð10:50Þ

The proportion constant EY in the formula is the Young’s modulus. This stress will lengthen the object in the direction x, while shorten the object in the transverse direction y. The transverse strain exy is deﬁned as normalized length variation -dw/w, and the relation between exy and exx is exy ¼ mPo

rxx EY

ð10:51Þ

where mPo is the Poisson’s ratio with a value usually between 0.3 and 0.25 (mPo = 0.28 for Nd3+:YAG, mPo = 0.25 for ruby, mPo = 0.33 for Nd3+:YLF, and mPo = 0.28 for Yb3+:YAB). Another important concept is shear stress: force in the

Fig. 10.6 Radial temperature distribution of laser rod pumped by optical ﬁber-coupled semiconductor laser

330

10 Laser and Physical Properties of Materials

y direction applied to the yz plane will cause a shear stress rxy, which has the following relation with shear strain cxy cxy ¼

rxy GR

ð10:52Þ

where GR is called shear modulus of elasticity and has a relation with Young’s modulus EY and Poisson’s ratio mPo as follows GR ¼

EY 2ð1 þ mPo Þ

ð10:53Þ

The material has a maximum limit stress, and exceeding this limit the material will produce thermal stress damage. In the case of continuous wave pumping, the maximum limit stress occurs at the rod surface produced by temperature distribution in a cylindrical laser rod. As shown in Fig. 10.5, it is [31] rmax

pﬃﬃﬃ 2 avEY Pout ¼ 8p K ð1 mPo Þl

ð10:54Þ

Most of the parameters in the above formula have been described, while a is the coefﬁcient of thermal expansion. By (10.54), the maximum laser power output allowed before thermal stress damage of the laser rod can be obtained [31] 8p lRM Pmax ¼ pﬃﬃﬃ 2 vq

ð10:55Þ

where RM = rtK (1-mPo)/aEY is a measure of the thermal shock resistance of materials and is referred to as thermal shock resistance parameter. The reference value of the thermal shock resistance parameter RM for several kinds of laser materials are: [33] RM(glass) = 1, RM(GSGG) = 6.5, RM(YAG) = 7.9 and RM(Al2O3) = 100, in the unit of W cm−1. Obviously, in order to increase the laser output power, the materials with higher heat shock resistance RM and smaller heat production parameter vq should be selected and the length l of laser rod better to be longer. Actually, due to the thermo-optic effect, the laser output power cannot reach the above maximum value. This is mainly because of that after temperature rising, spectral linewidth becomes wider and fluorescence lifetime becomes shorter. According to (10.21), laser material quality factor will be decreased and laser threshold will be elevated. On the other hand, it can be seen from (10.40), the temperature of the central region of laser rod is higher than that of its edge; therefore thermal expansion will also being larger in the central region and entire laser rod is changed into a convex lens. In the simple isotropic cases discussed, refractive index change with temperature can be expressed as

10.4

Thermo-Mechanical and Thermo-Optical …

DnðT Þ ¼

331

dn ðT T 0 Þ dT

Referring to (10.40), the refractive index at the radius r can be expressed as nðr Þ ¼ nð0Þ þ

2 dn dn r ½T ðr Þ T ð0Þ ¼ nð0Þ DT0 dT dT r0

ð10:56Þ

If the temperature coefﬁcient of refractive index is positive (e.g. in YAG crystal), the refractive index increases with the increase of temperature; therefore the refractive index of central region of the rod is higher than that of the rod edge. This will create a convex thermal lens effect. Following is an analysis of this problem. Suppose that the optical path variation of the light passing the laser rod includes the optical path change dnTl via temperature variation, the optical path change dnPl via photoelastic effect, and the optical path change ndl via thermal expansion. Because these three kinds of focusing effect are different in calculation, the focal length fT via temperature variation, the focal length fP via photoelastic effect, and the focal length fa via thermal expansion should be calculated separately, and then the total focal length fth by thermal lensing will be 1 1 1 1 ¼ þ þ fth fT fP fa

ð10:57Þ

First to calculate dnl, according to (10.56), at the edge of laser rod r = r0 the variation of refractive index is 2 dn r nðr ÞT nð0ÞT ¼ DT0 dT r0

ð10:58aÞ

It can be seen from the above equation that the refractive index in this laser rod shows a quadratic variation with radius r; therefore this laser rod is equivalent to a spherical lens. However, the focal length of a lens-like medium with length l, radius r, and refractive index n0 can be expressed as follows [33] f r 2 =2l½nðr Þ nð0Þ

ð10:59Þ

Comparing the equation of (10.59) with (10.58a) and using (10.42) of DT0, it can be shown that pr 2 K fT ¼ 1 dn 0 2 dT vPout dnP via photoelastic effect can be expressed as [33]

ð10:60aÞ

332

10 Laser and Physical Properties of Materials

1 nðr ÞP nð0ÞP ¼ n30 aCr;/ vPout r 2 =pr02 Kl 2

ð10:58bÞ

where a and Cr,/ are the thermal expansion coefﬁcient and the photoelastic coefﬁcient of laser rod, respectively. Cr,/ has two values, one for the radial component and one for the tangential component of polarized light. By using (10.59) and (10.58b), the focal length fP via photoelastic effect can be expressed as fP ¼

pr02 K n30 aCr;/ vPout

ð10:60bÞ

On the other hand, due to thermal expansion, the laser rod change to a biconvex lens, the focal length f of lens can be usually expressed as [34] f ¼

1 ðn0 1Þð1=R1 1=R2 Þ

ð10:61Þ

where R1 and R2 are the radius of the front and the rear end face curvature. For the biconvex lens-like laser rod produced by thermal expansion, R2 = −R1 = −R and R−1 = −d2l(r)/dr2, by using (10.40), the length l(r) of laser rod varying with respect to r is expressed as lðr Þ ¼ al½T ðr Þ T ð0Þ ¼ alDT0 r 2 =r02 The curvature of end face will be equal to R1 ¼ 2alDT0 =r02 Therefore, the focal length fa via thermal expansion can be obtained as follows fa ¼

1 r02 pr02 K ¼ ¼ 2ðn0 1ÞR1 4ðn0 1ÞalDT0 ðn0 1ÞavPout

ð10:60cÞ

In introducing the above equation, (10.42) has been used. Then by using (10.60a, 10.60b, 10.60c) and (10.57), the total focal length fth of thermal lensing can be expressed as follows fth ¼ 1 dn 2 dT

pr02 K þ aðn0 1Þ þ an30 Cr;/ vPout

ð10:62Þ

Equation (10.62) is applicable for side pumping laser; this equation is in good agreement with the experiment of side-pumped Nd3+:YAG rod laser [35]. The following expression of the focal length of thermal lens for the laser diode end pumping is derived by Innocenzi [36]. A Gaussian pump beam incident into the crystal was assumed as follows

10.4

Thermo-Mechanical and Thermo-Optical …

333

I ðr; zÞ ¼ I0 exp 2r 2 =w2p exp jp z

ð10:63Þ

where jp is the absorption coefﬁcient and wp is the (1/e2) Gaussian radius of pump beam. With vPout, the thermal power generated in laser operation, the effective focal length for entire laser rod can be expressed as Kpw2p 1 fth ¼ vPout ðdn=dT Þ 1 exp jp l

! ð10:62bÞ

The thermal lens effect of laser material will decrease laser output and laser beam quality, especially the TEM00 mode output. In the design of laser devices, some measures can be taken to reduce the influence of thermal lens effect [37–39]. In the case of crystal, the thermal stress causes the refractive index change with temperature by photoelastic effect. The anisotropy of refractive index is described by optical indicatrix in crystal optics. The second-order optical indicatrix tensor N can be expressed as [40] N ¼ PE

ð10:64Þ

where P is the photoelastic tensor; generally, it is a fourth-order tensor and E is a second-order stress tensor. For different crystal systems, the above tensors have different forms (the symmetry of the crystal results in the vanishing of some components of tensor [40]). The thermal conduction equation of anisotropic crystals will also be anisotropic. When discussing the lens effect, it is necessary to calculate the effect for different crystal orientations, respectively. In addition, the thermal effect of crystal can also cause thermal birefringence [40] and it affects the polarization output of laser. These involved in the design of laser device and can refer to the literatures and books of laser device. It is necessary to talk about some microscopic relations of the thermal properties before the end of this section. Because of laser material is insulator (except for the semiconductor laser material not discussed in this book), its main mechanism of thermal conduction is phonon conduction, and the microscopic process of thermal resistance is derived by the anharmonic interaction of lattice vibration. It can be demonstrated that the thermal conductivity is proportional to the cubic of Debye temperature TD and inverse proportional to absolute temperature T and the square of Grüneisen constant cG [41] K/

TD3 Tc2G

ð10:65Þ

Therefore, the material with a higher maximum phonon energy will have a higher thermal conductivity, if it has the same or almost the same anharmonic,

334

10 Laser and Physical Properties of Materials

because hxmax kTD . On the other hand, the thermal conductivity can be expressed as 1 K ¼ Cv vlp 3

ð10:66Þ

where Cv, v, and lp are the speciﬁc heat, the phonon velocity, and the phonon mean free path of the material, respectively. Considering the Debye temperature and phonon velocity and remembering that the phonon velocity is inversely proportional to the square root of compressibility of materials mentioned in Chap. 9, it can also be seen that the more compact the material structure, the higher is the thermal conductivity. It is also true for the same anisotropic crystal, the thermal conductivity in the direction with compact structure is higher than that in the direction with looser structure; especially for the material with laminated structure, the thermal conductivity along the direction of the layer is signiﬁcantly higher than that in the direction perpendicular to the layer. On the other hand, thermal expansion of the crystal also is one of the anharmonic effects and the coefﬁcient a of thermal expansion can be expressed as [42, 43] a¼

cG Cv k

ð10:67Þ

The thermal expansion coefﬁcient is proportional to Grüneisen constant cG and inversely proportional to the compressibility k of crystal. It is also closely related to the structure of the material. The more compact the structure, the higher the binding energy, the smaller the coefﬁcient of thermal expansion. Because the compressibility k is often different in different directions; in the same anisotropic crystal, there is little difference in Grüneisen constants in different directions. Therefore, the difference in the coefﬁcient of thermal expansion in different directions often comes from the different compressibility. The compressibility is increased with the increase of the distance between ions, therefore in the direction of greater lattice constant; the coefﬁcient of thermal expansion is often relatively smaller. For example, the lattice constants of YVO4 crystal are: a = b=7.12Å, c = 6.29 Å, its thermal expansion coefﬁcients are: aa= 4.410−6/K and ac= 1110−6/K;the Nd3+: KGW crystal has lattice constants: a = 8.10Å, b = 10.43Å and c = 7.60 Å, its thermal expansion coefﬁcients are: aa= 4.010−6/K,ab= 1.610−6/K and ac= 8.5 10−6/K; another example of Yb3+:YAB crystal has lattice constants: a = b=9.295Å and c = 7.243Å, then its thermal expansion coefﬁcients are: aa= 1.410−6/ K,ac= 8.110−6/K. At very low temperature, the anharmonic interaction of lattice vibrations can be neglected, so the thermal conductivity of the materials is very high. The phonon mean free path lp is also related to the order degree of the material. The order degree of a material can be seen from two aspects: ﬁrst is whether the mass of lattice ions is uniform; if the masses of lattice ions are equal or approximately equal, then the phonon mean free path reaches its maximum. The larger the difference of the mass of lattice ion, the lower the lattice order, the shorter the mean free path lp and the

10.4

Thermo-Mechanical and Thermo-Optical …

335

lower the thermal conductivity K of the crystal. An obvious example is the comparison of the thermal conductivity of yttrium aluminum garnet with that of the ruby. The density of yttrium aluminum garnet (Y3Al5O12) is 4.55 g/cm3 but the density of ruby (Al2O3) is only 3.98 g/cm3. However, the thermal conductivity of the yttrium aluminum garnet is 11 W/mK which is lower than half of the thermal conductivity 28 W/mK of the ruby. One of the important reasons is the masses of aluminum ion and oxygen ion are very different from that of the yttrium ions while the ion mass difference is much smaller in ruby. The second factor that affects the order of a material is the defect in the material. A material with fewer defects will have higher order degree and so longer phonon mean free path and higher thermal conductivity, while a material with more defects only has shorter phonon mean free path and lower thermal conductivity. Especially when the temperature is not high, the main mechanism of phonon scattering is not the anharmonic lattice vibration but the phonon scattering by the impurities or defects, so that there is a great difference in the thermal conductivity of the material with and without impurities or defects. When active ions enter into the crystal lattice, due to the mass difference between the active ion and the host ion as well as the other defects introduced by the doping of the active ion, the mean free phonon path will be greatly reduced, so that the thermal conductivity is reduced appreciably. This can be seen by the comparison of thermal conductivity temperature dependence of pure YAG crystal and 0.5 at.% Nd3+:YAG crystal, shown in Fig. 10.7. The thermal properties of YAG, YAP, and other laser crystals are studied in detail by Aggarwal et al. [45]. Table 10.2 lists the data measured at temperature 300 K (the temperature coefﬁcient of refractive index is measured at 1.06 lm), where Yb3+:YAB data are quoted from Nikogosyan’s book [46]. These data are not complete; some of these values are not consistent with those published in the literatures. Actually, due to the different doping concentration of active ion in the crystal, different measurement wavelength and temperature, different crystal integrity and optical homogeneity, as well as different measurement methods, the

Fig. 10.7 Comparison of thermal conductivity temperature dependence of pure and 0.5 at.% Nd3+:YAG crystals [44]

336

10 Laser and Physical Properties of Materials

Table 10.2 Comparison of thermal performance parameters of several laser materials Crystal

Expansion coefﬁcient a (10−6K−1)

Temp. derivative of refractive index dn/dT (10−6K−1)

Conductivity K (Wm−1K−1)

YAG Al2O3 YAlO3

6.14 4.4(⊥c), 6.8(//c) 2.32(a axis), 8.0 8(b axis) 8.7(c axis) 14.31 (a axis), 10.05 (c axis) 13.6 (a axis), 10.8 (c axis) 1.9

7.8 12.8 (E⊥c), 11.8 (E//c) 7.7(E-a axis), 11.7(E-b axis) 8.3(E-c axis) −4.6 (E-a axis), −6.6 (E-c axis)

11.2 28 11.7(a axis), 10.0 (b axis) 13.3 (c axis) 5.3 (a axis), 7.2 (c axis)

−3.6 (E-a axis), −6.0 (E-c axis)

5.0 (a axis), 6.3 (c axis) 2.6

YLF LuLF KGWb axis KYWb axis Yb:YAB

3.0

2.7

8.1(c axis), 4(⊥c axis) (Yb 1 at.%)

4.7 (Yb 5.6 at.%)

results obtained by different authors often to be different. However, some data published in the literature also do not conform to the principles of crystal physics. For example, the thermal expansion coefﬁcient is a second-order symmetric tensor which is an isotropic physical quantity in the cubic YAG crystal, while there are reports of different thermal expansion coefﬁcients in different directions (e.g. the data quoted in the literature [33]). Certainly, the non-uniform distribution of Nd3+ ions in the crystal or other inhomogeneity in the crystal growth process can lead to the deviation of the measured data. Aggarwal et al. [45] obtained a series of the temperature function of thermal conductivity, thermal expansion coefﬁcient, and the temperature coefﬁcient of refractive index for laser crystals. For example, the relationship between expansion coefﬁcient and temperature is að T Þ ¼ M 0 þ M 1 T þ M 2 T 2 þ M 3 T 3 The parameters for YAG crystal are M0 = −1.8496, M1 = 4.36810−2, M2 = −5.684410−5, M3 = 0. The relationship between the temperature coefﬁcient of refractive index and temperature is dn ðT Þ ¼ P0 þ P1 T þ P2 T 2 þ P3 T 3 dT The parameters for YAG P2 = −4.560510−5, P3 = 0.

crystal

are

P0 = -3.946,

P1 = 5.29410−2,

10.4

Thermo-Mechanical and Thermo-Optical …

337

It is necessary to mention another important physical property of materials, that is, the hardness of materials. The end surface of laser materials is required to be processed into a surface with a high degree of parallelism and ﬁneness; it requires the material to have a high hardness and therefore a high binding energy. In short, starting from the requirements of laser device, a laser material must have a high thermal conductivity K, a high thermal diffusion coefﬁcient j, a high hardness H, a high tensile strength, and a high thermal shock resistance Rm. On the other hand, it is necessary to have a small coefﬁcient of thermal expansion a and a small refractive index temperature coefﬁcient. The thermal resistance and thermal expansion of an insulator are all resulted from the anharmonic effect of lattice vibration. The thermal conductivity decreases with the increase of the mass difference of the lattice ions while temperature coefﬁcient of refractive index is proportional to the coefﬁcient of thermal expansion a. The requirements of a small thermal expansion coefﬁcient, a high thermal conductivity, and a small refractive index temperature coefﬁcient are consistent. Because of these performance requirements, an ionic crystal with a higher binding energy, a higher melting point, and a smaller mass difference of the lattice ions should be adopted as a laser host material.

10.5

Laser Damage and Nonlinear Optical Properties

Many laser crystals have both laser emission and various nonlinear optical properties. This section mainly introduces the relationship between the nonlinear optical properties and laser damage of these crystals, but the nonlinear optical properties of laser crystals and their applications in laser operations such as self-frequency doubling, self-frequency mixing, and self-Raman lasers will be described in next chapter. In high power or high energy laser operation, the nonlinear optical properties of a laser material can result in laser beam distortion, self-focusing, self-defocusing, [47, 48] and material damage. When laser intensity is very high, the nonlinear effect of dielectric polarization cannot be ignored and the dielectric coefﬁcient of the material can be written as e ¼ e0 þ e2 E 2

ð10:68Þ

The corresponding refractive index has the following relation n ¼ n0 þ n2 E 2

ð10:69Þ

where E is the electric ﬁeld intensity of light ﬁeld. When laser power is very high, the intensity of E is high enough, and then the second term of the above equation will produce a nonlinear effect. It should be noted that the intensity of laser beam often is the strongest at the central part (near the axis). If n2 is positive, the effect of

338

10 Laser and Physical Properties of Materials

nonlinear term makes the refractive index of the material near the central of laser beam cross-section higher than that of its marginal part. The result of this nonlinear effect is that the laser beam just like is focused by a series of converging lens. If n2 is negative, the effect of nonlinear term makes the refractive index of the material near the central of beam cross-section lower than that of the marginal part, then the result is that the laser beam just like is defocused by a series of divergent lens. The difference of the refractive index of different points on the cross section of laser beam caused by the nonlinear effect also produces a phase difference between the different points in the cross-section of laser beam; thus the wavefront distortion is produced and the linewidth of the laser beam is increased. The strong lasers can also generate two-photon absorption, stimulated Raman scattering, stimulated Brillouin scattering, and other nonlinear optical processes. All these effects will bring about the loss of laser power or energy. Therefore, the materials with weak nonlinear optical effect should be selected as the laser host materials of high power or high energy laser; for example, the crystal with central symmetry or low refractive index (by the Miller rule, if the linear polarization is small, then the nonlinear polarization is also small [49]). It is impossible to give a detailed description to a large number of nonlinear optical effects, but only choose self-focusing effect for further discussion, because it is directly related to the laser damage of the material. The self-focusing of laser beam and its threshold can be described by a simple model. The main idea of this model is: when the refractive index n0 + n2E2 inside the laser beam higher than refractive index n0 outside the laser beam, total internal reflection will occur at the boundary of laser beam. This total internal reflection will cancel out the beam divergence due to diffraction and with the increase of the laser power the laser beam will be further converged to a smaller and smaller beam width. As shown in Fig. 10.8, the divergence angle of laser beam due to diffraction is d1, and the incidence angle of total internal reflection at the boundary of the beam is d2. Obviously, d1 and d2 are supplementary, that is sin2 d1 þ sin2 d2 ¼ sin2 d1 þ cos2 d2 ¼ 1 If the beam width of a laser beam is D then the ideal divergence angle generated by the diffraction has the following relation sind1 1:22k=n0 D

ð10:70Þ

n0

Fig. 10.8 Schematic diagram of laser beam self-focusing

2 δ2 n0 +n2 E

δ1

10.5

Laser Damage and Nonlinear Optical Properties

339

According to refraction law and the refractive index of internal and external laser beam given above, it is concluded that the total internal reflection of a laser beam on the boundary must satisfy the following relation sind2 ¼ n0 =ðn0 þ n2 E 2 Þ

ð10:71Þ

The complementarily of d1 and d2 become ð1:22k=n0 DÞ2 þ ½n0 = ðn0 þ n2 E 2 Þ2 ¼ 1

ð10:72Þ

The second term of the above equation can be approximately calculated as follows n20 =ðn0 þ n2 E 2 Þ2 ¼ 1=ð1 þ E2 n2 =n0 Þ2 ð1 E 2 n2 =n0 Þ2 1 2E2 n2 =n0 ð10:73Þ then the following equation is established ð1:22k=n0 DÞ2 þ 1 2E 2 n2 =n0 ¼ 1

ð10:74Þ

Namely, when the electric ﬁeld intensity of a laser beam is equal to E2 = (1.22k)2/ (2n0n2D2), the laser beam began to focus. Therefore the threshold electric ﬁeld intensity of self-focusing is E2 (1.22k)2/(2n0n2D2). Because the sectional area of a laser beam is pD2/4, the intensity of a laser beam is n0cE2/8p, so that the threshold power of self-focusing is PTH ¼ ð1:22kÞ2 c=64n2

ð10:75Þ

It can be seen that this threshold power is proportional to the square of laser wavelength and inversely proportional to nonlinear refractive index. One can also approximately calculate the self-focusing threshold of a laser beam from Maxwell equation of classical electrodynamics [46]. This aspect of narrative can also refer to textbook published by Yariv [50] or monograph published by Akhmanov [51]. The appearance of self-focusing makes the diameter of a laser beam decrease and optical power density increase rapidly; therefore many physical processes introduced by strong laser including stimulated Raman scattering, stimulated Brillouin scattering, high-order harmonic generation, and a series of element excitation processes will take place. After absorbing strong laser energy, high temperature thermal effects such as the emission of electron, ion, or, molecule and the formation of plasma of a medium can be produced. Therefore, the laser beam self-focusing is closely related to the laser damage of a medium. The relationship between the self-focusing of laser beam and the damage of a material will be simply discussed in the following.

340

10 Laser and Physical Properties of Materials

It is generally believed that laser damage is caused by the following three kinds of mechanism: ﬁrst is the local fracture of a material caused by high-intensity ultrasonic phonon generated by stimulated Brillouin scattering; second is the defects or impurities in a material absorbing the laser energy then the local temperature rise up to tens of thousands degrees and thus the damage is caused by the explosion of heat shock wave or micro plasma; the third is that under extremely high laser power, the electric ﬁeld intensity of laser radiation is close to or even higher than that of the atom itself, then the nonlinear effect has become very strong that the multi-photon absorption excites electrons in some atoms into the conduction band or even ionization. The resulting electrons accelerated by high-intensity laser ﬁeld will generate the phenomenon of electron avalanche, similar to the dielectric breakdown under strong static electric ﬁeld. No matter what kinds of mechanism, laser damage can occur only at sufﬁciently high laser power density. When laser beam is incident into an optical material, the power density of the laser may not reach the threshold of laser damage, but after going through a distance of the medium, the self-focusing effect will increase the power density of laser beam which entirely possible to reach or exceed the damage threshold. The material with positive temperature coefﬁcient of refractive index (dn/dT > 0) may produce thermal lens effect due to the absorption of laser light by impurities and defects appeared. This is the reason of laser damage threshold on the incident surface is higher than that of the exit surface for some crystals and glasses. One direct example of the relation of the damage threshold of laser self-focusing with laser wavelength is that after frequency doubling by using KDP or other nonlinear optical crystal the damage threshold is lower than that by using laser beam without frequency doubling. When the second harmonic laser of power 105 W focuses into ruby or sapphire crystal, some 1 cm long, 10 lm diameter ﬁlaments and a long string of cracks along the path of the light can be observed. However, the same power of laser without frequency doubling focus into the same materials cannot observe this phenomenon. As mentioned above, the damage threshold of laser self-focusing is proportional to the square of laser wavelength; obviously after frequency doubling, the damage threshold of laser self-focusing will be decreased four times, and this can explain the observed phenomenon. Of course, not all the laser damage of different materials results from beam self-focusing. By using laser pulse of single longitudinal mode and TEM00 transverse mode at wavelength 1064 nm with width of 9.9 ns, Do and Smith [52] observed the laser damage threshold of undoped and Nd3+, Cr4+, Yb4+-doped YAG crystals and ceramics. The relevant parameters of YAG crystal were used to calculate damage threshold by laser self-focusing and damage threshold by stimulated Brillouin scattering. The results are higher than the actual observed damage threshold; while the multi-photon ionization and avalanche ionization induced by the light electric ﬁeld heating electrons of conduction band can successfully illustrate the experimental data of single-pulse excitation. As for the damage threshold of continuous multiple pulse excitation lower than that of the single excitation, they considered that the cumulative damage may be due to the distribution of electrons to low

10.5

Laser Damage and Nonlinear Optical Properties

Table 10.3 The property requirements of solid-state laser material

341

Host material 1. Suitable size can be prepared easily and economically 2. Stable and durable during laser operation 3. Have chemical stability under light radiation, heating and mechanical processing 4. Better thermal properties: (1) high thermal conductivity, (2) high thermal diffusion coefﬁcient (3) small thermal expansion coefﬁcient 5. Better mechanical properties: (1) High stress rupture limit and high tensile strength (2) Small stress optical coefﬁcients (3) High laser damage threshold (for the material used in high energy and high power laser) (4) high hardness 6. Better optical quality: (1) Minimum packages, defects, and other scattering centers (2) Minimum absorption at laser and pump wavelength (3) Small refractive index temperature coefﬁcient Active ion 1. Valence and radius of active ion can match that of the substituted host ion 2. Can be well-distributed in the host material 3. High ground state (but no excited state) absorption at pumping wavelength and minimum ground state or excited state absorption at laser wavelength 4. Small quantum defect to make high efﬁciency population of metastable level and reduce thermal loading 5. Having an appropriate metastable state lifetime to make full use of all the pump energy 6. Can generate radiation at laser wavelength with high quantum efﬁciency 7. Emission line with linewidth and intensity both meet the requirements of laser device. 8. Have suitable ion–ion interaction to achieve the maximum pumping absorption and minimal quenching

energy and long life self-trapping exciton states; their ionization is easier than that of the valence electrons. Briefly, in order to satisfy the requirements of laser application, laser materials must have the appropriate mechanical, thermal, and optical properties. The property requirements of solid-state laser material are listed in Table 10.3 for reference.

342

10 Laser and Physical Properties of Materials

References 1. V. Lupei, N. Pavel, T. Taira, Opt Comm. 201, 431 (2002) 2. V. Lupei, N. Pavel, T. Taira, Appl. Phys. Lett. 2002(81), 2677 (2002) 3. F. Auzel, in 2000 Proceeding of the 2nd International Symposium On Laser, Scintillator and Nonlinear Optical Materials (Lyon, 2000), pp. 28–31 4. N.A. Tolstik, V.E. Kisel, N.V. Kuleshov et al., Appl. Phys. B 97, 357 (2009) 5. Y.J. Chen, Y.F. Lin, J.H. Huang et al., Opt. Express 18, 1370 (2010) 6. Y.J. Chen, Y.F. Lin, J.H. Huang et al., Opt. Express 21, 18919 (2013) 7. K.N. Gorbachenyo, V.E. kisel, A.S. Yasukevich, et al., Opt. Lett. 38, 2446 (2013) 8. Y.J. Chen, Y.F. Lin, J.H. Huang et al., Opt. Lett. 40, 4927 (2015) 9. Y.J. Chen, Y.F. Lin, J.H. Huang et al., Opt. Express 23, 72401 (2015) 10. Y.J. Chen, Y.F. Lin, J.H. Huang et al., Opt. Express 2017(25), 17128 (2017) 11. J.H. Huang, Y.J. Chen, H. Wang et al., Opt. Express 2017(25), 24001 (2017) 12. J. Huang, Y. Chen, Y. Lin et al., Opt. Lett. 43, 1643 (2018) 13. Y.J. Chen, Y.F. Lin, J.H. Huang et al., Opt. Express 26, 419 (2018) 14. Y.J. Chen, Y.F. Lin, Z.M. Yang et al., OSA Contin. 2, 142 (2019) 15. N.A. Tolstik, S.V. Kurilchik, V.E. Kisel et al., Opt. Lett. 32, 3233 (2007) 16. Y. Li, J. Feng, P. Li et al., Opt. Express 21, 6082 (2013) 17. Y. Chen, Y. Lin, Y. Zou et al., Opt. Express 22, 13969 (2014) 18. A.A. Lagalsky, V.E. Kisel, A.E. Jroshin et al., Opt. Lett. 33, 83 (2008) 19. G.B. Loutts, C. Bonner, C. Meegoda et al., Appl. Phys. Lett. 71, 303 (1997) 20. F. Auzel, in ed. by B. Di Bartolo, Spectroscopy of Solid-State Laser-Type Materials. (Plenum Press, New York, 1987) 21. V. Kushawaha, A. Banerjee, L. Major, Appl. Phys. B 56, 239 (1993) 22. Y. Chen, L. Major, V. Kushawaha, Appl. Opt. 35, 3203 (1996) 23. O. Musset, J.P. Boquillon, Appl. Phys. B 64, 503 (1997) 24. O. Musset, J.P. Boquillon, Appl. Phys. B 65, 13 (1997) 25. V. Kushawaha, Y. Yan, Y. Chen, Appl. Phys. B 62, 533 (1996) 26. Z.D. Luo, X.Y. Chen, C.Y. Tu, et al., Chin. Phys. Lett. 17, 888 (2000) 27. X. Mateos, P. Loiko, J.M. Serres et al., IEEE. J. Quant. Elect. 53, 1 (2017) 28. Z.D. Luo, Y.D. Huang, Opt. Comm. 206, 159 (2002) 29. Z.D. Luo, Y.D. Huang, M. Montes, D. Jaque, Appl. Phys. Lett. 85, 715 (2004) 30. C. Jacinto, T. Catunda, D. Jaque et al., Phys. Rev. B 72, 235111 (2005) 31. A. Penzkofer, Prog. Quantum Electron. 12, 291 (1988) 32. Y.F. Chen, T.M. Huang et al., IEEE. IEEE J. Quantum Electron. 33, 1424 (1997) 33. W. Koechner, Solid-State Laser Engineering, 6th edn. (Springer Verlag, Berlin, 1996) 34. M. Born, E. Wolf, principle of Optics, 5th edn. (Pergamon Press, Oxford, 1975) 35. X.B. Wang, X.J. Xu, X. Li, et al., Appl. Opt. 46, 5237 (2007) 36. M.E. Innocenzi, H.T. Yura, C.L. Fincher, Appl. Phys. lett. 56, 1831 (1990) 37. J.D. Foster, L.M. Osterink, J. Appl. Phys. 61, 3656 (1970) 38. T. Chin, R.C. Morris, O. Kafri, et al., in Technical Digest of the Conference on Lasers and Electro- Optics CLEO’86. (California, San Francisco, 1986), p. 212 39. I. Moshe, S. Jackel, R. Lallouz et al., Proc. SPIE 1997(3110), 238 (1997) 40. J.F. Nye, Physical Properties of Crystals, their Representation by Tensors and Matrices (Clarendon Press, Oxford, 1957) 41. G. Leibfried, E. Schloemann, Nachr Ak Wiss Gottingen. Math. Phys. 11a, 71 (1954) 42. P.G. Klemens, in Solid State Physics, vol. 7, eds. Seitz, Turnbull, (Academic Press, New York, 1958) 43. C. Kittel, Introduction to Physics, 5th edn. (Wiley, New York, 1976) 44. B.S. Wang, H.H. Jiang et al., Eur. Phys. 39, 23 (2007) 45. R.L. Aggarwal, D.J. Ripin, et al., J. Appl. phys. 98, 103514 (2005)

References

343

46. D.N. Nikogosyan, Nonlinear Optical Crystals-A Complete Survey (Springer Science + Business Media, New York, 2005) 47. R. Menzel, Photonics—Linear and Nonlinear Interactions of Laser Light and Matter (Springer, Berlin, 2001) 48. Z.D. Luo, Optoelectronic Technology (Internal publication of the Fujian Institute of the Research on the Structure of Mater), First Issue 27, (1973) (in Chinese) 49. Y.R. Shen, The Principles of Nonlinear Optics. (Wiley, 1984) 50. A. Yariv, Quantum Electronics, 3rd edn. (Wiley, 1989) 51. S.A. Akhmanov, R.V. Khokhlov, A.P. Sukhorukov, Laser Handbook, vol. 2 (North–Holland Publishing Company, Amsterdam, 1972), p. P1151 52. B. Do, A. Smith, Appl. Opt. 48, 3512 (2009)

Chapter 11

Nonlinear Optical Properties of Laser Crystals and Their Applications

As mentioned above, many laser crystals have nonlinear optical properties and so can double, mixing, or transform the frequency of laser beam by second harmonic (SH) and stimulated Raman scattering (SRS) effects. With the development of laser technology, the study on these effects and their applications has become increasingly extensive and in-depth because of its important signiﬁcance in technology. More laser applications require the devices to be more portable, more compact, and easier to be adjusted and used. To meet these requirements is the key to expand laser application, because small and portable devices are easy to be used in more occasions. To concentrate the generation and modulation function of laser beam in the same crystal, no doubt that it will bring the beneﬁts of small, lightweight, easy to be adjusted and used. This requires that a crystal has both the performances of laser generation and the modulation of spatial and temporal characteristics. In this chapter, we ﬁrst discuss the combination of laser emission with frequency doubling and mixing, then the combination of laser emission with SRS effect. The emphasis will be placed on the physical principle rather than technical aspect, a relatively simple model is adopted, and so only the most influential factors are considered while some problems that must be considered in practical application are neglected. As it is well known, blue and green lasers are an urgent need in information technology and many other laser applications. At the start of the study, it is found that to directly generate the laser emission at such wavelengths is more difﬁcult than to generate near-infrared laser emission and then to double or mix the frequency of fundamental laser emission. Technically, blue and green laser beams are generally produced by an infra laser beam generated by one laser crystal, then through frequency doubling, mixing, or optical parametric oscillation by another nonlinear crystal. If the second-order nonlinear optical coefﬁcient of the laser crystal is large enough, then can the laser beam with double frequency be obtained by the frequency doubling effect of the laser crystal itself, that is, generating the so-called self-frequency doubling (SFD) laser beam? The answer is afﬁrmative. Johnson [1] in 1969 and Dmitriev [2] in 1979 published, respectively, their laser SFD results by using Tm3+ and Nd3+ ion activated LiNbO3 crystal. Of course, the SFD efﬁciency © Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8_11

345

346

11

Nonlinear Optical Properties of Laser Crystals …

of this crystal was still very low. Dorozhkin [3] in 1981 ﬁrst did the SFD experiment of Nd3+:YAl3(BO3)4 (NYAB) crystals. Because the concentration of Nd3+ ion was too high, the self-absorption at the wavelength 0.53 lm was serious, so he only obtained the SFD laser at 0.66 lm generated by the frequency doubling of fundamental laser at 1.32 lm. Lu et al. [4] in 1986 grew this crystal with a Nd3+ ion concentration lower than 20% atomic ratios and realized the 0.53 lm SFD laser output pumped by pulsed dye laser, but the doubling efﬁciency is still low. The author [5, 6] pointed out that the Nd3+ ion concentration in laser crystal influences not only fundamental laser output level and luminescence concentration quenching effect but also nonlinear optical coefﬁcients, and all aspects of the effect must be taken into account to determine the optimum Nd3+ concentration in NYAB crystal. Both suitable Nd3+ concentration and suitable crystal growth method were adopted and the 1.06 ! 0.53 lm frequency conversion of NYAB crystal pumped by an incoherent light source—a common pulse xenon lamp—was realized in 1988 [5, 6]. Since then, the SFD laser crystal attracted the attention of many scientists, and a lot of research work has been carried out on crystal spectral properties, energy level structure, laser experiment, and the application of diode pumping of NYAB and NGAB (Nd3+:GdAl3(BO3)4) crystals [7–24]. Later is the work of Bartschke [24] who obtained the green laser output of 225 mW by using an NYAB crystal pumped by 1.6 W LD laser and at the same time obtained the green laser output of 450 mW by using the same crystal pumped by 2.2 W Ti3+:sapphire laser. It is shown that the SFD laser has practical application in laser technology. The SFD and self sum-frequency mixing (SSFM) properties of the Nd3+ and Yb3+ ions-activated MgO-LiNbO3, GdCOB (Ca4GdO(BO3)3), YdCOB (Ca4YO (BO3)3), and YAB crystals were also studied by many authors [25–42]. 1.1 W green laser output was obtained from Yb3+:YAB crystal, and its light–light efﬁciency reached 10% [40]. Moreover, a 510–545 nm green/yellow wide tuning laser was obtained in Yb3+: YAB crystal [41]. GdCOB and YCOB crystals have smaller walk-off angle and large crystal can be grown by Czochralski method in a relatively short period of time. Among them, the performance of Yb3+:YCOB is better than Nd3+:YCOB, while Nd3+GCOB is better than Yb3+:GCOB. A 1.35 W green laser output was obtained by the SFD of Nd3+:GdCOB crystal with maximum optical conversion efﬁciency of 17% [42] and it has application prospect of laser display, and so on. On the other hand, Capmany et al. [43, 44] used quasi-phase matching method to achieve SFD and SSFM laser output in the non-periodic polarization Nd3+:LiNbO3 crystal. This quasi-phase matching method can not only make use of the larger nonlinear optical coefﬁcient d33 in LiNbO3 crystal from the consideration of nonlinear optical conversion efﬁciency, but also take advantage of stronger fundamental polarization luminescence in a crystal from the angle of the fundamental laser generation. In this chapter, NYAB crystal will be taken as an example to introduce the relationship between fundamental laser emission and frequency doubling (mixing) laser generation in a nonlinear laser crystal, the effect of active ion doping on the nonlinear coefﬁcients of laser crystal, the selection of the optimum concentration of active ion, as well as how to efﬁciently generate self-doubling (mixing) laser and its

11

Nonlinear Optical Properties of Laser Crystals …

347

relationship with crystal structure and general physical properties of crystal. In the end, the basic knowledge about the composite effect of laser and stimulated Raman scattering (self Raman frequency shift) is introduced.

11.1

Second-Order Nonlinear Optical Effect of Crystal

In general, nonlinear optical effects include frequency doubling, frequency mixing, optical parametric process, stimulated Raman scattering, stimulated Brillouin scattering, and so on. The following is a discussion starting from second-order nonlinear optical effect, especially frequency doubling effect and by using Maxwell equation of electromagnetic wave. By the electrodynamics, in a dielectric medium (speciﬁc conductance r = 0, electric current i = 0), the magnetic and electric ﬁeld vectors of electromagnetic wave satisfy the following equations rH ¼

1 @D c @t

rE¼

1 @H c @t

D ¼ Eþ4pP

ð11:1Þ ð11:2Þ ð11:3Þ

If we only consider linear and second-order nonlinear polarization, polarization intensity P can be expressed as P ¼ vð1Þ E þ vð2Þ EE

ð11:4Þ

The second-order polarization susceptibility v(2) in (11.4) is a second-order tensor, and one component of P can be expressed as ð2Þ

Pi ¼ vð1Þ Ei þ vijk Ej Ek

ð11:5Þ

Because there is no free charge in the medium, ∇E = 0. By calculating the curl of both sides of (11.2) and using formula ∇ ∇ E = ∇∇E−∇2E and (11.1), the following can be obtained r2 E ¼

1 @2D c2 @t2

ð11:6Þ

Discussing only the propagation of light waves along the z direction and assuming a plane wave approximation can be used, the electric ﬁeld is constant in the x and y direction, and so the electric ﬁeld intensity is taken as the following form

348

11 ðxm Þ

El

Nonlinear Optical Properties of Laser Crystals …

1 ðz; tÞ ¼ Eml ðzÞexp½iðxm t km zÞ þ c:c 2

ð11:7Þ

where m in the above formula is the label of the frequency of different interaction laser beams (m can be 1, 2, 3) and l denotes the different electric ﬁeld components of a laser beam (l can be i, j, k). In the calculation of (11.6), a slow-varying amplitude approximation should be used; that is, assuming that the variation of the light wave amplitude with z is small enough, the following inequality is satisﬁed d 2 Em ðzÞ=dz2 \\km dEm ðzÞ=dz The second-order derivative of Eml(z) with respect to z can be ignored, then ðx Þ r2 E1i 1 ðz; tÞ can be expressed as ðx Þ r2 E1i 1 ðz; tÞ

dE1i ðzÞ 1 2 þ k1 E1i ðzÞ exp½iðx1 t k1 zÞ þ c:c ik1 dz 2

ð11:8Þ

On the other hand, by using e ¼ 1 þ 4pvð1Þ ¼ n2 and k ¼ nx=c, the right-hand side of (11.6) becomes

1 2p ð2Þ k12 E1i ðzÞexp½iðx1 t k1 zÞ 2 x21 vijk E3j E2k expfi½x1 t ðk3 k2 Þzg þ c:c 2 c ð11:9Þ It has been assumed that x1 = x3−x2 in the above equation. Let (11.8) is equal to (11.9) and eliminating the same terms on both sides of the equation obtained, the following equation can be obtained dE1i ðzÞ 2px1 ð2Þ ¼ i v E3j E2k exp½iðk3 k2 k1 Þz dz n1 c ijk

ð11:10Þ

Similarly, the following two equations can also be obtained dE2k ðzÞ 2px2 ð2Þ ¼ i v E E3j exp½iðk3 k2 k1 Þz dz n2 c kij 1i dE3j ðzÞ 2px3 ð2Þ ¼ þi v E E exp½iðk3 k2 k1 Þz dz n3 c jik 1i 2k

ð11:11Þ ð11:12Þ

Remembering that light intensity is equal to the speed of light multiplied by its energy density c ce 2 cn 2 E ¼ E I¼ q¼ n 8pn 8p

11.1

Second-Order Nonlinear Optical Effect of Crystal

349

By using three equations of (11.10) to (11.12), it is clear that each laser beam is suitable for the following form of equation dI ðx; zÞ cn dEðx; zÞ dE ðx; zÞ ¼ E ðx; zÞ þ Eðx; zÞ dz 8p dz dz Consider the situation that the laser beams 1, 2, 3 only have one electric ﬁeld component and are not equal to zero. After determining the crystal orientation, the (2) actual effect of tensor v(2) ijk can be represented by tensor veff . The function relation (2) (2) between veff and vijk which depends on the symmetry of the crystal and the phase matching condition will not be discussed here. By using the relation between the complex amplitude phases quoted from YR Shen’s book [45] in the case without incident light of frequency x3, the following equation can be obtained by (11.10) dI ðx1 Þ 4px1 ¼ dz c

rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2p ð2Þ veff I ðx1 ÞI ðx2 ÞI ðx3 Þcos½ðk3 k2 k1 Þz ð11:13Þ cn1 n2 n3

Similarly rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2p ð2Þ veff I ðx1 ÞI ðx2 ÞI ðx3 Þcos½ðk3 k2 k1 Þz ð11:14Þ cn1 n2 n3 rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ dI ðx3 Þ 4px3 2p ð2Þ ¼ þ veff I ðx1 ÞI ðx2 ÞI ðx3 Þcos½ðk3 k2 k1 Þz ð11:15Þ dz cn1 n2 n3 c dI ðx2 Þ 4px2 ¼ dz c

When x3 = x1 + x2 it is obvious that dI ðx3 Þ dI ðx1 Þ dI ðx2 Þ þ þ ¼0 dz dz dz

ð11:16Þ

It means that in the process of a laser beam of frequency x1 interacts with a laser beam of frequency x2 to produce a laser beam of frequency x3, the total energy is conserved. From the previous analysis, one can see clearly that the energy of laser beams with different frequencies can be converted to each other due to the existence of nonlinear polarization. Now take a look at some of the characteristics of the second harmonic generation and the condition to achieve phase matching. For the frequency doubling process x1 = x2 = x, x3 = 2x; in this case the second-order polarization susceptibilities in (2) (2) (2) (11.10) to (11.12) have the relation v(2) jik = vijk = vkij = veff ; therefore (11.12) including phase factor can be written as dE3j ðzÞ 2px ¼ i v E1i E2k expðiDkzÞ dz n3 c eff

ð11:17Þ

350

11

Nonlinear Optical Properties of Laser Crystals …

where Dk = k3−k2−k1. Suppose there is no second harmonic input, that is, E3j(0) = 0 and the length of crystal is L. Under the small signal approximation, the efﬁciency of the double frequency conversion is very low, and the electric ﬁeld intensity of the fundamental laser beam can be considered to be independent of z. Integrating (11.17) in this condition, the laser ﬁeld at the output end of the crystal is obtained E3j ðLÞ ¼ i

2px eiDkL 1 veff E1i E2k n3 c iDk

Therefore 2 2 2 E3j ðLÞ2 ¼ 4p x v2 E2 E2 L2 sin ðDkL=2Þ eff 1j 2k 2 2 n3 c ðDkL=2Þ2

Attention, in the case of frequency doubling, I2I(x3) = I(2x), I1I(x1) = I(x2) = I(x), while in (11.17) and the above equation, the refractive index n3 is denoted by n2 and the refractive index at the fundamental wavelength is expressed as n1, thus the second harmonic conversion efﬁciency can be obtained I2 1 sin2 ðDkL=2Þ ¼ 32 p3 x2 v2eff L2 3 2 I1 I1 c n2 n1 ðDkL=2Þ2

ð11:18Þ

It can be seen that the second harmonic conversion efﬁciency is proportional to the intensity and the frequency square of the fundamental laser, the square of second-order nonlinear optical coefﬁcient, and the square of crystal length. The factor sin2(DkL/2)/(DkL/2)2 is determined by a phase matching condition. In the case of phase matching Dk = 0, this factor reaches its maximum value. When calculating the second harmonic intensity, the total loss of the fundamental wave is the sum of (11.13) and (11.14), which is two times that of the (11.13). A is used to express the product of the following series of parameters ð2Þ A ¼ ð8 px1 =cn1 Þveff ð2 p=cn2 Þ1=2 ¼ 16 p2 m1 =cn1 veff ð2 p=cn2 Þ1=2 Therefore the coupling equation can be written as (

pﬃﬃﬃﬃ dI1 dz ¼ AI1pﬃﬃﬃﬃI2 ðj1 þ c1 ÞI1 dI2 dz ¼ AI1 I2 ðj2 þ c2 ÞI2

ð11:19Þ

The prerequisite Dk = k3 − k2 − k1 = 0 for the generation of second harmonic wave has been taken into account and at the same time, the absorption coefﬁcient j1,j2 and the loss coefﬁcient c1, c2 are added to take into account the absorption of fundamental and double frequency laser beams and the other losses.

11.1

Second-Order Nonlinear Optical Effect of Crystal

351

Different ways to achieve Dk = 0 is by corresponding to different types of phase matching. One can take the negative uniaxial crystal as an example to explain how to realize the type I and the type II phase matching. Wave vector k is the momentum of photon and Dk = 0 is k3 = k2 + k1. The equality on both sides of this vector equation means the consistency of the momentum in number and direction, so phase matching is the conservation of momentum in nonlinear optical process. If this condition is satisﬁed, the second harmonic generation in fundamental wave propagation process will strengthen each other and form a stronger second harmonic laser beam. The wave vector is nx/c in quantity and for the frequency doubling process, the condition of phase matching k2 = 2k1 is n2 ðx2 Þx2 ¼ 2n1 ðx1 Þx1 Substituting x2 = 2x1 then nð2x1 Þ ¼ nðx1 Þ

ð11:20Þ

In the case of light propagating in a normal dispersion medium, the higher the frequency, the higher the refractive index, the above conditions cannot be satisﬁed. However, when there is birefraction phenomenon in the crystal, the refractive index of ordinary light (o light) is not equal to that of the extraordinary light (e light). If the fundamental light is o (or e) light while the second harmonic light is e (or o) light, then (11.20) can be satisﬁed. The way to realize the phase matching is to select a particular direction of the crystal so that (11.20) can be satisﬁed; it is called angle phase matching. In some of the nonlinear optical crystals, the temperature coefﬁcient of the refractive index for ordinary light is different from that of the extraordinary light and so phase matching can be achieved by changing the temperature; it is called temperature phase matching. Some speciﬁc problems of angle phase matching will be explained as follows. For a negative uniaxial crystal (no > ne), if one chooses fundamental light as o light and second harmonic light as e light, the refractive index of high-frequency second harmonic light can be equal to that of the low-frequency fundamental light. This matching method is referred to as ooe type matching method. Obviously, for a positive uniaxial crystal, because ne > no, one can only choose eeo matching method to satisfy the phase matching condition. It can be seen that, whether it is ooe or eeo matching method, the polarization directions of two fundamental light are parallel, so it is called a parallel phase matching or a type-I phase matching. Of course, one can still choose two fundamental waves as o light and e light, respectively, and the frequency doubling light in a negative uniaxial crystal as e light (oee type phase matching) and in an uniaxial positive crystal as o light (oeo type phase matching). In these two cases the polarization directions of two fundamental lights are all perpendicular to each other, so these phase matching are called orthogonal phase matching or type-II phase matching. According to the phase matching conditions, the optimal angle of different types of phase matching can be deduced. The calculation formulas will be simply listed in

352

11

Nonlinear Optical Properties of Laser Crystals …

the following. The phase matching angle for type-I phase matching of a negative uniaxial crystals is ð hm Þ I ¼

" 2 2 #1=2 ne2 2 no2 no1 sin 2 2 no1 no ne 1

2

ð11:21Þ

2

The phase matching angle for type-II phase matching of a negative uniaxial crystals is 8 2 .

91=2 2 < 2no2 þ no1 1= ne1 ðhm Þ II 1 ð hm Þ o e 2 II ¼ sin : ; n2 n2 1

ð11:22Þ

The right side of (11.22) includes the unknown quantity, so one can use iterative method to work out the phase matching angle. For type-I and type-II phase matching of a positive uniaxial crystal, the corresponding phase matching angle formulas can be obtained as follows " ðhm ÞIþ ¼

sin

1

2 #1=2 1 no1 no2 2 1 no1 ne1

" #1=2 o o o 2 n n 1 2n 1 2 1 ðhm ÞIIþ ¼ sin1 o e 2 n1 n1 1

ð11:23Þ

ð11:24Þ

The angle hm in (11.21) to (11.24) is the angle between the wave vector of optical wave and the optical axis of crystal. It must be noted that when the direction of wave vector (direction of light power flow) and the direction of the optical axis of a uniaxial crystal is not equal to 90°, the traveling direction of the fundamental laser beam and that of the second harmonic laser beam will not completely coincide but is taken off a small angle d called walk-off angle. For type-I phase matching of a negative uniaxial crystal, d satisﬁes the following equation [46] 0 2 h e 2 0 2 i n tand ¼ 1 n2 n2 sinð2hm Þ 2

ð11:25Þ

As the light continues to travel in a crystal, the overlapping between fundamental laser beam and second harmonic laser beam becomes smaller and the frequency doubling efﬁciency decreases, which greatly limits the crystal size that can be used. It can be seen from (11.25) that d = 0 when hm = 90° and the unfavorable factor caused by walk-off angle disappears. Usually the phase matching of hm = 90° is called non-critical phase matching while the phase matching of hm 6¼ 90° is called critical phase matching. It can be seen from (11.21) that for the type-I phase

11.1

Second-Order Nonlinear Optical Effect of Crystal

353

matching of a negative uniaxial crystal, when no1 = ne2, hm = 90°. Technically, the crystals with no1 close to ne2 and d(no1−ne2)/dT6¼0 is generally chosen to realize non-critical phase matching by using the method of temperature regulation. In addition to the above-mentioned laser power, frequency doubling coefﬁcient, and crystal length, the other factors that affect the efﬁciency of frequency doubling should be taken into account. First is the allow angle breadth Dhm; beyond it the frequency doubling efﬁciency is less than 50% of its maximum value, and can be obtained from the formula [46] 0:66k1 no1 Dhm ¼ o L n2 ne2 sin2hm

ð11:26Þ

where k1 is the wavelength of fundamental laser beam and L is the length of crystal. The frequency doubling efﬁciency will decrease when the wavelength of fundamental laser deviates from the wavelength of phase matching. If the wavelength deviation is dk and the frequency doubling efﬁciency reduced to half of its maximum value, then the laser spectral linewidth Dk = 2dk and Dk can be expressed as [46] 0:44k1 i Dk ¼ [email protected] @ne ðhÞ L @k11 12 @k2 2

ð11:27Þ

Obviously, the smaller the divergence angle, the better the monochromaticity of a laser beam and the higher the efﬁciency of second harmonic generation; therefore one can also use spectral brightness to simultaneously describe the monochromaticity, directionality, and the power of a laser beam, that is, the power of laser beam per unit solid angle and unit wavelength interval. The spectral brightness can be improved by using a mode selection method of transverse mode and longitudinal mode. In addition, the change of crystal working temperature will cause the change of the refractive index of a crystal, which deviates from the phase matching point. Therefore, depending on the refractive index temperature coefﬁcient of various crystals, each nonlinear optical crystal has a permissible frequency doubling temperature range DT [46] DT ¼

0:44k1 Ld ne2 no1 dT

ð11:28Þ

The temperature change which affects the phase matching mainly comes from the change of environment temperature, but the light absorption of a crystal may also produce the temperature change. Particularly for a SFD laser crystal, because the doping of active ion, the total thermal effect or non-uniform thermal effect caused by the non-uniform absorption of pump light will reduce the efﬁciency of frequency doubling. This will be further discussed in the following. Similarly, the optical inhomogeneity in a crystal will also make parts of the region passing through by the

354

11

Nonlinear Optical Properties of Laser Crystals …

laser beam does not satisfy the phase matching condition, thereby reducing the total conversion efﬁciency of frequency doubling. A series of second harmonic laser parameters mentioned above are related to the refractive indexes of o-light and e-light for fundamental and second harmonic wave, while these refractive indexes also related to the active ion concentration of a crystal. The dispersion relations of the refractive index of two typical SFD laser crystals are listed below. NYAB: The Nd3+ concentration is 5.6 at%, in the temperature range of 293 K < T < 473 K and wavelength range of 0.4 lm < k < 0.7 lm. The dispersion relation is (the temperature T is in unit of Kelvin and the wavelength k is in unit of lm) [19] n2o ¼ 1 þ n2e ¼ 1 þ

172:4727 ð0:10985 þ 7:7

107 T

2:38 109 T 2 Þ2 k2

161:08069 ð0:10669 þ 1:3 106 T 3:2 109 T 2 Þ2 k2

Yb3+:YAB: The Yb3+ concentration is 8 at%. The dispersion relation at room temperature is (the wavelength k is in unit of lm) [47] n2o ¼ 3:1762 þ 0:0013= k2 0:1480 0:0971k2 n2e ¼ 2:8632 þ 0:0090= k2 0:0937 0:0083k2 Phase matching angle, walk-off angle, and other parameters can be calculated by (11.21) to (11.28), while the refractive indexes and phase matching parameters of a series of nonlinear optical crystals, including the frequency doubling crystal, can also be found in related manuals and books [48–50].

11.2

Relationship Between Fundamental and Second Harmonic Waves in SFD Laser Crystal

In principle, the SFD laser can be summed up in one sentence: the stimulated radiation emitted by the active ions forms a fundamental laser beam in an optical resonator, then a second harmonic laser beam is generated by the second-order nonlinear optical effect of the crystal, ﬁnally the second harmonic laser beam output by the output mirror of a laser resonator. However, it cannot be understood as a simple addition of laser effect and second harmonic effect. On the one hand, the efﬁciency of second harmonic conversion is proportional to the intensity of fundamental laser, and the increase of the intensity of fundamental laser is undoubtedly beneﬁcial to the increase of the intensity of second harmonic laser. On the other

11.2

Relationship Between Fundamental and Second Harmonic …

355

hand, the conversion between fundamental laser and second harmonic lasers is not only mutually promoted but also restricted to each other. This is owing to the fact: ﬁrst, the doping of ions into the host crystal has certain effect on the nonlinear optical coefﬁcient of the crystal; secondly, a fundamental laser beam transformed into a second harmonic laser beam will form an important loss of the fundamental laser oscillation, that is, the generation of second harmonic laser has a restrictive function on the generation of fundamental laser; thirdly, the second harmonic laser absorbed by the active ion will weaken the intensity of second harmonic laser; fourthly, in the Nd3+ ion-doped crystal, second harmonic laser has a pumping effect on the active ions. The speciﬁc details of the above four aspects must be analyzed separately and then use a model to sum up the four kinds of effect and study the interaction between them. First, the effect of the doping of active ion on the second-order nonlinear optical susceptibility of host crystal should be studied. Taking NYAB crystal as an example, the Y3+ ion in the crystal is substituted by doping Nd3+ ion. The radius of Nd3+ ion is slightly larger than that of the Y3+ ion (the Goldschmidt radius of Nd3+ ion is 0.115 nm and that of the Y3+ ion is 0.106 nm). The competition between increase effect and decrease effect on nonlinear optical susceptibility by the doping of Nd3+ ion determines the optimal concentration of Nd3+ ion. The nonlinear optical susceptibility of NYAB crystal can be seen as the summation of the nonlinear optical susceptibility of all the BO3 groups in the crystal, while the nonlinear optical susceptibility of BO3 group mainly comes from the contribution of p electron in the group. In NYAB crystal, there is one type of BO3 group (type I group) in which the O2+ ion (O2+ (1)) only is directly adjacent to Al3+ ion. The other type of BO3 group (type II group) has two O2+ (O2+ (2)) ions occupying, respectively, the vertices of two triangular cones in which the Y3+ ion is situated at the center. The p electron distribution of the BO3 group of type II will be affected by the substitution of Nd3+ ion. When Nd3+ ion concentration is low, one Nd3+ ion replaces the Y3+ ion in one of the triangular cone, then the surrounding environment symmetry of BO3 group is reduced, and the nonlinear optical susceptibility of this type of group is increased. The local space symmetry distortion of the crystal in the case of low Nd3+ ion concentration is less important and has not obvious influence on the summation of nonlinear optical susceptibility of different BO3 groups in the crystal; therefore, the overall nonlinear optical susceptibility of the crystal will increase with the increase of Nd3+ ion concentration. However, when Nd3+ ion concentration increased to a certain level, the total variation of local space symmetry caused by the Nd3+ doping is obvious and is detrimental to the summation of nonlinear optical susceptibility of different BO3 groups in the crystal. At the same time, when Nd3+ ion concentration increases to reach a certain level, there will be more BO3 groups that have two Y3+ ions substituted by Nd3+ ions and so the number of low environment symmetry BO3 group will be lower than that of the low Nd3+ ion concentration case. Hence, the number of BO3 group with higher nonlinear optical susceptibility will be decreased with the increase of Nd3+ ion concentration, at the same time the local space group symmetry distortion will decrease the summing result of nonlinear optical susceptibility of different BO3 groups. Consequently, when Nd3+ ion concentration exceeds

356

Nonlinear Optical Properties of Laser Crystals …

11

a certain level (optimum concentration), the nonlinear optical susceptibility of NYAB crystal will be decreased with the increase of Nd3+ ion concentration. The test of frequency doubling effect of NYAB powder sample with different Nd3+ ion concentration basically reflects the competition of these two opposite effects. The nonlinear coupling equations of the SFD process are discussed in detail below. First, study the term of second harmonic conversion in (11.19). In accordance with the condition of equal gain and loss under steady state, one has pﬃﬃﬃﬃ AI1 I2 ¼ ðc2 þ j2 ÞI2 where j2 is the absorption coefﬁcient of second harmonic laser in crystal, c2 is the total loss including the output loss, the diffraction loss, and the walk out angle loss of second harmonic laser, in which the output loss is the main loss. One has the following expression for the intensity of second harmonic laser. I2 ¼

A c 2 þ j2

2 I12

ð11:29Þ

pﬃﬃﬃﬃ Let h = A2/(c2 + j2) then AI 1 I2 ¼ hI12 . By (11.19), if one ignores the small fundamental wave absorption and other small loss, the following equation resulted (

dI1 dz dI2 dz

¼ hI12 ¼ hI12 ðj2 þ c2 ÞI2

ð11:30Þ

The effect of Nd3+ concentration on the intensity of second harmonic laser beam is included in the second equation. If the contribution of pumping intensity to fundamental laser intensity is taken into account in (11.30), a nonlinear-coupled equation set can be obtained, which includes the generation of fundamental laser and the transformation of fundamental laser into second harmonic laser. When the relationship between parameter A and Nd3+ concentration is obtained, then this equation can sum up the three aspects of the effects mentioned, which can be used to study the relation among several laser and nonlinear optics parameters. The pumping effect of the second harmonic wave is reflected in the inversion of particle number, which will be taken into account in the rate equation of population inversion in the next section. It can be seen from (10.6) of Chap. 10 that the fundamental laser gain coefﬁcient ag = rem DN, because DN is proportional to the product of the pump absorption rate ap and the fluorescence lifetimesf of laser level, and so ag/apremsf. Look at the relation of pump absorption rate with Nd3+ ion concentration. By means of absorption spectra measurement, the absorption coefﬁcient at wavelength 0.804 lm when Nd3+ ion concentration is 1%, j0.804 (1%Nd) = 1.44 cm−1 for NYAB crystal can be obtained, then the pump absorption rate of this crystal is proportional to the following factor

11.2

Relationship Between Fundamental and Second Harmonic …

357

ap / 1 ej0:804 ð1%cc ÞN ð% Þtp The concentration of Nd3+ ion N (%) is in the unit of atomic percentage (it will be simply expressed as % in the following), and tp is the crystal thickness of pump light penetration. The relation of the utilization rate of pumping light with Nd3+ ion concentration can be seen in Fig. 1 in reference [6]: when pumped with LD at wavelength 0.804 lm, if the crystal length is 0.5 cm, the concentration of Nd3+ ion is 8%, then the pump light utilization rate can reach 99.7%. It means that on further increase, the Nd3+ doping concentration has no practical beneﬁt to the improvement of pump efﬁciency. On the other hand, the fluorescence quenching effect of Nd3+ ion in a YAB crystal is very weak, which belongs to one kind of self-active laser crystal. The concentration quenching rate KQ of this kind of crystal is proportional to the concentration of active ion KQ ¼ Cg N ¼

1 1 sf sr

ð11:31Þ

According to the experimental data of NYAB, the following relation can be obtained [6]

1 sf ¼ 3:3 104 N ð%Þ þ 1:66 102 ls

ð11:32Þ

Because one has the relation ag/apremsf and emission cross-section rem is essentially independent of Nd3+ concentration, so that gain coefﬁcient G can be expressed as i

1 h G ¼ Cg 3:3 104 N ð%Þ þ 1:66 102 1 ej0:804 ð1%ÞN ð%Þtp ð11:33Þ where Cg is a constant independent of Nd3+ concentration and pump light penetration thickness tp is in the unit of cm. It can be seen from Fig. 11.1 that regardless of the pump light penetration thickness, tp is 0.3 or 0.5 cm, under the conditions of Nd3+ concentration > ¼ WN1 ðWN1 Þth DN < dt hx 1 > dI cr I I > : 1 ¼ em 1 DN 1 dt n1 sc

ð11:35Þ

In the above ﬁrst equation, the total change rate of particle inversion number is equal to the increase rate of particle inversion number generated by pump light and minus the change rate of inversion number necessary to reach the threshold of laser oscillation and the change rate of inversion particle number produced by laser generation. Where DN ¼ N2 ðg2 =g1 ÞN1 ; W ¼ gB21 dðxÞp is the pumping rate, WN1

360

11

Nonlinear Optical Properties of Laser Crystals …

indicates the contribution of the pumping to population inversion density, g is the efﬁciency of pumping, and B21 expresses Einstein coefﬁcient in (5.53a) of Chap. 5. How to express energy density d(x)p as a function of light intensity will be discussed below. The second term (WN1)th indicates the pumping rate at the laser threshold, which includes the pumping rate necessary to overcome the losses of spontaneous emission and fundamental laser light. The ﬁrst term on the right hand side of the second equation of (11.35) is the contribution of stimulated radiation to laser intensity. In general laser rate equation this term should be divided by a factor of 1 + I1/Is, due to the fact that the saturation intensity of the fundamental laser in the experiments discussed is Is = hc/kremsf 104 W/cm2, but the intensity of fundamental laser light discussed satisfy I1 < < Is, so this factor can be omitted. The second term is the loss of the fundamental laser intensity in resonant cavity. Where rem,sc, I1, x1, and n1 are the emission cross-section, the resonant cavity lifetime, the intensity, the frequency, and the refractive index of fundamental laser, respectively. In order to write down the rate equation set of fundamental laser generation and its second harmonic conversion, one should obviously combine equations of (11.30) and (11.35) in some way. First, one should rewrite (11.30) into time differential form, namely to use formula dI/dt = dI/dz dz/dt to transform (11.30), where dz/dt is the speed of light in the medium, then the following equation set of the fundamental and second harmonic laser intensities in the case of steady output can be obtained 8 dI1 c 2 > > < dt ¼ n hI1 1 ð11:36Þ > dI c c > : 2 ¼ hI12 ðj2 þ c2 Þ I2 n2 n2 dt In the calculation of population inversion rate, for the total change rate of particle inversion number, in addition to those expressed in (11.35), the increase rate of particle inversion number generated by second harmonic wave should be considered. Combining (11.35) and (11.36) while taking into account that the second harmonic laser has pumping effect on active ion with pumping rate W2, that is, W2N1 and the pumping rate of pump source is W0, the following rate equation set for the fundamental laser of SFD laser crystal can be obtained 8 dDN rem I1 > > ¼ ðW0 þ W2 ÞN1 ðW0 N1 Þth DN < dt hx 1 ð11:37Þ > dI c I c > : 1 ¼ rem DNI1 1 h I12 n1 n1 dt sc Note, here DN is the population inversion density between the upper and the lower laser levels. Because the lower laser level is not ground state, the particle number density is very low, and it can be ignored, the particle number density of upper laser level is approximately equal to the population inversion density between the upper and the lower laser levels. N1 is the particle density of ground state, that is, the active ion density of the crystal. Under the steady-state one has the following equation set

11.3

Nonlinear Optical Coupling Equation of SFD Laser

8 r I > < ðW0 þ W2 ÞN1 ðW0 N1 Þth em 1 DN ¼ 0 hx 1 n > : rem DNI1 1 I1 hI12 ¼ 0 csc

361

ð11:38Þ

W2N1, which involves the variable I2, can be neglected in solving the ﬁrst-order approximate solution. The following equation can be obtained by the ﬁrst equation of (11.38)

rem DNI1 ¼ W0 N1 ðW0 N1 Þth hx 1 A quadratic equation of I1 with the following solution can be obtained

I1 ¼

csn1c

r ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2

n1 þ þ 4h W0 N1 ðW0 N1 Þth hx1 csc 2h

ð11:39Þ

Because the light intensity must be positive, the negative solution has been given up. The problem of how to use the second equation set of (11.36) to calculate SFD laser intensity will be discussed in the following. Pump energy density d(xp) can be expressed as I xp d xp ¼ c np

ð11:40Þ

In the problem discussed, the particle number of the upper laser level is much smaller than that of the ground state. The approximate assumption in Chap. 5 for the derivation of (5.11a) is valid. By using equations of (5.11a) and (5.53b), it is obvious that B12 gðxÞ ¼

cjðxÞ hxnN1

ð11:41Þ

For the pumping laser with narrow linewidth, one has I(xp) = I0d(x−xp), then the contribution of pumping laser to the variation rate of the particle number of the upper laser level can be obtained Z W0 N1 ¼ gN1

B12 gðxÞd xp dx ¼ g

Z

gj c I0 d x x p j xp dx ¼ p I0 hxnp hx p c np ð11:42Þ

where jp j(xp) and g is the pumping efﬁciency. For a certain volume of laser crystal, the intensity of pump light in different position is not the same, for example for diode laser end pumping, the pumping intensity is strongest on the incident surface of pumping light, deep into the interior of the crystal the pumping intensity

362

11

Nonlinear Optical Properties of Laser Crystals …

is exponential decay. The average pumping rate per unit volume should be an integral divided by the volume of the pumping region in the crystal. When the length of a crystal is L, assuming that the intensity distribution of pump laser on the cross section of the crystal is uniform then the average pumping rate per unit volume is R

W0 N1 dv ¼ V

RL g jp I0 ejp l dl 0

¼

hxp L

ð1 ejp L Þ gI0 hxp L

ð11:43Þ

The pump band is very close to the upper laser level, then the probability of non-radiative transition from pump band to the upper laser level is much higher than those of the radiative or non-radiative transitions from pump band to other lower energy levels and so g 1 can be assumed. Similarly, the pumping effect of the double frequency laser on the crystal can be written as W2 N 1 ¼

j2 I2 hx2

ð11:44Þ

The pump rate of pump source at the threshold can be expressed as follows ðW0 N1 Þth ¼

jp Ith hxp

ð11:45Þ

where Ith is the threshold pump intensity, that is, the threshold pump power per unit area. It is also the threshold power flux discussed in Chap. 10 and can be expressed as Ith /th ¼

hxp np csc rp N1 sf rem

ð11:46Þ

where rp is the absorption cross-section of the crystal at pump light wavelength and rem is the emission cross-section of the crystal at fundamental laser wavelength, therefore ðW0 N1 Þth ¼

np csc sf rem

ð11:47Þ

If laser output mirror has reflectivity R at pump light wavelength, then the corresponding pumping contribution of the reflected light should be added. By using the second equation of (11.39) and (11.29), as well as (11.47), the ﬁrst-order approximate solution of SFD laser intensity can be obtained

11.3

Nonlinear Optical Coupling Equation of SFD Laser

ð1 Þ

I2 ¼

363

"sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ #2 ﬃ 2 np h x1 n1 ð1 ejp L Þð1 þ Rejp L Þ I0 x1 n1 pﬃﬃﬃ þ pﬃﬃﬃ L xp csc sf rem 2csc h 2csc h ðN1 r2 þ c2 Þ

ð11:48Þ The second-order approximate solution of SFD laser intensity is obtained by adding the pumping effect of the SFD laser obtained in the ﬁrst-order approximation.

ð2Þ

I2 ¼

"sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ #2 2 np hx 1 n1 ð1 ejp L Þð1 þ Rejp L Þ I0 x1 n1 ð1Þ pﬃﬃﬃ þ pﬃﬃﬃ þ 0:5N1 r2 I2 x0 csc sf rem L 2csc h 2csc h ðN1 r2 þ c2 Þ

ð11:49Þ After n−1 iterations, the following is obtained

ðnÞ

I2 ¼

ﬃ "sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ #2 2 np h x1 n1 ð1 ejp L Þð1 þ Rejp L Þ I0 x1 n1 ðn1Þ pﬃﬃﬃ þ pﬃﬃﬃ þ 0:5Nr2 I2 L x0 csc sf rem 2csc h 2csc h ðN1 r2 þ c2 Þ

ð11:50Þ According to (11.39) and (11.44), W2 N1 hx1 ¼ N1 r2 I2 hx1 = hx2 ¼ 0:5N1 r2 I2 representing the pumping effect of second harmonic laser has been added to (11.48) to (11.50). After several iterations, the convergence of double frequency laser intensity can be obtained. The intensity of output SFD laser is equal to the above laser intensity multiplied by the transmission of output mirror. As mentioned in the previous section, the doping of a small amount of Nd3+ ion increases the nonlinear coefﬁcient of NYAB crystal. According to the experimental data in terms of nonlinear optical coefﬁcient measurement of a series of crystal powder samples, it can be assumed in the simulation calculation that −9 2 v(2) eff (Np) = 6.1207 10 (1 + Np/30−Np/900)esu, as is shown in Fig. 11.3. For NYAB crystal, the refractive index n1 = 1.755, n2 = 1.708 and in the case x1 = 1.77 1015 s−1, x2 = 3.54 1015 s−1, for type I (ooe) phase matching, an expression of A = 5.73 10−8 (1 + Np/30−N2p/900) can be obtained by the formula shown before the introduction of (11.19), where the Nd3+ concentration Np is in the unit of atomic percentage while the product of active ion number N1 per unit volume and absorption cross-section rp can be replaced by the product of Np and the absorption coefﬁcient jp(1%) of Nd3+ ion at unit atomic percentage concentration, as shown in Sect. 11.2. jp = N1rp Npjp(1%) and j2 = N1r2 Npj2(1%). According to the data given, for the semiconductor laser pumping at wavelength 0.804 lm, j0.804(1%) = 1.44 cm−1 and j2(1%) = 0.27 cm−1, so that jp = 1.44Np (cm−1) and j2 = 0.27Np (cm−1).

364

11

Fig. 11.3 The relationship between nonlinear optical 3+ coefﬁcient v(2) eff (Np) and Nd atomic percentage concentration Np

Nonlinear Optical Properties of Laser Crystals …

1.3

1.2 χ(2)eff(Νp) 1.1

1

0

20

10

30

Np

Suppose the surfaces of a NYAB crystal with length L = 0.5 cm has 100% transmittance for the pump light, while the rear mirror and output mirror of the resonator with length Lc have reflectivity 85 and 15%, respectively, at the wavelength of second harmonic laser, the cavity loss coefﬁcient per centimeter is c2 = −ln (0.15 0.85)/2Lc(Lc/L) = 1.03/2L. By including other losses, c2 = 1.25/L can be assumed, therefore h

i2 5:73 108 1 þ Np =30 Np2 =900 A2 ¼ h¼ j2 þ c2 0:27Np þ 1:25=L If the crystal is placed in a resonant cavity consisting of a rear mirror M1 and an output mirror M2, the cavity length is Lc = 50 mm. The reflectivities of the rear mirror and the output mirror are all 99.75% at the wavelength of fundamental laser and the reflectivity of output mirror at the wavelength of pumping light is 70%. The single pass loss of the fundamental wave in the cavity mirrors is very low. By taking into account the other loss, it can be assumed that a round-trip loss in the cavity is 2%, that is, cc = 0.02, then the photon lifetime in the cavity can be calculated bysc = 2[Lc + (n1−1) L]/(ccc). In the calculation of SHG intensity of NYAB crystal, according to (11.48) to (11.50), the parameters are: fluorescence lifetime sf = (3.3 10−4 Np + 1.66 10−2)−1 ls [6], emission cross-section at the wavelength of fundamental laser rem = 4.5 10−19 cm2 [12], and the refractive index at pumping wavelength n0 = 1.77. If the length of the NYAB crystal is 0.5 cm, the power of the pump laser is 400 mW and pumping light after focusing is a cylindrical beam with diameter 100 nm. In this case the curve of SFD efﬁciency for different Nd3+ concentration obtained is shown in Fig. 11.4. The maximum efﬁciency of the SFD conversion of NYAB crystal published by Japanese authors [12] was 17.5%, which is much lower than 29% shown in Fig. 11.4. This is understandable, because the above calculation does not consider the walk-off angle effect and the fact that the diameter of pump light cannot maintain 100 nm in the whole crystal.

11.3

Nonlinear Optical Coupling Equation of SFD Laser

365

Fig. 11.4 Relation of SFD efﬁciency with atomic percentage concentration Np of Nd3+ ion

Thus, even if one takes into account of the factor that the nonlinear optical coefﬁcient is increased with the increase of Nd3+ concentration, the optimum concentration of Nd3+ ion is still in the range of 2–4%. Further calculations show that the optimal Nd3+ concentration does not change with the pump power, but is related to the length of the crystal, higher Nd3+ concentration is more suitable for shorter crystals. The intensity of thermal effect by the increase of Nd3+ concentration and the effect of phase mismatch produced by the inhomogeneous of refractive index on the conversion efﬁciency have not been taken into account in this calculation . Considering the effect of phase mismatch, the lower Nd3+ concentration is appropriate. It also can be seen by the calculation that with the increase of pump power, the efﬁciency of frequency doubling will be increased. For the 1 W power pumping (other conditions unchanged), if the above various influence effects do not calculate, the maximum theoretical efﬁciency up to 33.4% can be obtained. It can be seen by this calculation that the loss of fundamental wave (mainly the loss of mirror) in the laser cavity has a great effect on the output of SFD laser. The above calculation result is obtained in the case of cc = 0.02. If cc = 0.04 is adopted then pumped by the same power the maximum theoretical conversion efﬁciency is only 26.4%. With the increase of crystal length, in order to obtain a best SFD efﬁciency, the lower Nd3+ concentration should be adopted. On the other hand, taking into account the effect of walk-off angle on the efﬁciency of second harmonic generation and with the increase of crystal length, to assume the beam width of pump laser remains 100 nm in the whole crystal the error will be bigger, and it can be seen that selecting the Nd3+ concentration of 4% and the crystal length of 0.3 cm are more appropriate. After calculating the effects of the spatial distribution of the pumping, fundamental and second harmonic laser beams, as well as the walk-off angle, the results in good agreement with the experimental observation values can be obtained. This information can be obtained by referring to the literatures [54–57].

366

11

11.4

Nonlinear Optical Properties of Laser Crystals …

Self Sum-Frequency Mixing Effect in Nonlinear Laser Crystal

Blue laser is an important light source in the ﬁeld of optical information storage, lithography, laser printing, underwater laser communication, laser display, and laser medical treatment. By using the self sum-frequency mixing (SSFM) effect of nonlinear laser crystal to generate blue laser has the advantages of integration, easy adjustment, and high beam quality. The NYAB and Nd3+:GdCOB crystals ﬁrst achieve the blue laser output by this kind of SSFM effect. The principle of SSFM laser generation will be described below. A simple rate equation model is introduced ﬁrst, which does not consider the spatial distribution of laser beam and the effect of walk-off angle. The aim is to let the reader have a simple and clear understanding of the physical process of SSFM. In the problem to be studied the pump beam besides acting as an excitation source of the fundamental laser (frequencyx1) will also mix with the fundamental laser by SSFM effect to produce a laser beam of frequency x2 = x1 + xp, here, xp is the frequency of pump beam. The corresponding wave vectors satisfy the phase matching relation k2 = k1 + kp. Referring to Sect. 11.1, nonlinear optical coupling equations can be written as sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ dI xp 4pxp 2p ð2Þ ¼ veff I xp I ðx1 ÞI ðx2 Þexp i k2 k1 kp z cnp n1 n2 c dz ð11:51Þ dI ðx1 Þ 4px1 ¼ dz c

sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2p ð2Þ veff I xp I ðx1 ÞI ðx2 Þexp i k2 k1 kp z cnp n1 n2 ð11:52Þ

dI ðx2 Þ 4px2 ¼ þ dz c

sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2p ð2Þ veff I xp I ðx1 ÞI ðx2 Þexp i k2 k1 kp z cnp n1 n2 ð11:53Þ

By using a symbol B to represent 4p(2p/cnpn1n2)1/2v(2) eff and let I1 I(x1), I2 I(x2). Because I0 is used to denote the pump beam intensity on the incident face, Ip I(xp) will be used to represent the pump beam intensity in the crystal (which has a relation with the incident laser intensity I0 illustrated in the following), then the rate equations satisfying the phase matching condition can be written as dIp xp pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ¼ B Ip I1 I2 dz c

ð11:54Þ

11.4

Self Sum-Frequency Mixing Effect in Nonlinear Laser Crystal

367

dI1 x1 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ¼ B Ip I1 I2 dz c

ð11:55Þ

dI2 x2 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ¼ þ B Ip I1 I2 dz c

ð11:56Þ

In steady state, the loss per unit crystal length caused by the generation of second harmonic laser is equal to the gain expressed by (11.56), therefore

1=2 c2 I2 ¼ ðx2 =cÞ B Ip I1 I2 I2 ¼

x2 B 2 Ip I1 cc2

ð11:57Þ ð11:58Þ

The above rate equations become dIp xp x2 B2 ¼ 2 Ip I1 dz c c2

ð11:59Þ

dI1 x1 x2 B2 ¼ 2 Ip I1 dz c c2

ð11:60Þ

dI2 x2 B2 ¼ þ 22 Ip I1 dz c c2

ð11:61Þ

By (11.59) it can be seen that in addition to the original absorption loss jp of the crystal, pump beam also subjected to a loss j resulted from frequency mixing conversion. Taking the incident point of pump beam as zero, the pump beam intensity at the position z can be expressed as Ip ¼ I0 eðjp þ jÞz

ð11:62Þ

x x

where j ¼ cp2 c 2 B2 I1 . Combining the laser rate equations for a four-level system in 2 steady state, the nonlinear optical coupling equations can be written. The corresponding equation of (11.38) for the fundamental laser is 8 > >

> : rDNI1 I1 B Ip I1 ¼ 0 n1 sc cc2 n1 W0 N1 ðW0 N1 Þth

ð11:63Þ

Intensity I1 can be obtained by the above equation after averaging the pump beam intensity of (11.62) by the same way as (11.43) and taking into account the effect of output mirror reflectivity R on the pump beam; at the same time, the expressions of W0N1 and (W0N1)th take the similar forms of (11.42) and (11.47), respectively.

368

11

Nonlinear Optical Properties of Laser Crystals …

The fundamental laser intensity I1 by multiple trips in the cavity will arrive at the following steady value

c W0 N1 ðW0 N1 Þth hx1 h i I1 ¼ ð jp þ jÞ L 2 n1 x1 x2 B I0 1 e þ s cc2 jp þ j L c h ih i np hx1 c 1 eðjp þ jÞL 1 þ Reðjp þ jÞL I0 x1 jp =xp sc sf rem h i ¼ ð jp þ jÞ L 2 Ln1 x1 x2 B I0 1 e þ sc cc2 jp þ j

ð11:64Þ

The fundamental laser intensity I1 should be solved by iterative method. By assuming j = 0 in (11.64) to calculate the ﬁrst-order approximation of I1, and then using this ﬁrst-order approximation of I1 to calculate the second-order approximation of I1, after several iterations, the results of I1 and j can be obtained. By the integral of equation (11.61), the intensity of the frequency mixing light inside the cavity can be obtained i !2 h ð jp þ jÞ L I 1 e 0 x2 B I2 ¼ 1=2 jp þ j cc2 h ih i np hx 1 c 1 eðjp þ jÞL 1 þ Reðjp þ jÞL I0 x1 jp =xp sc sf rem h i ð jp þ jÞ L 2 Ln1 x1 x2 B I0 1 e þ sc cc2 jp þ j

ð11:65Þ

According to the above formula, the relationship between the efﬁciency of SSFM and Nd3+ concentration can be estimated. Assuming that the intensity of SSFM laser output is TI2 = 0.85I2 and g ¼ 0:85I2 =I0 , the photon cavity lifetime sc of the fundamental laser can be calculated by the value in Sect. 11.3 and the loss coefﬁcient is estimated to be c2 = 1.5/L. When pump power and crystal length is 500 mW and 0.5 cm, respectively, and the reflectivity of output mirror at pump wavelength is R = 0.7, according to the above formula the calculated efﬁciency of blue laser is shown in Fig. 11.5. Obviously, this efﬁciency is much lower than that of the SFD green laser Fig. 11.5 Relation between efﬁciency of SSFM and Nd3+ atomic percentage concentration Np

11.4

Self Sum-Frequency Mixing Effect in Nonlinear Laser Crystal

369

in the same condition. One of the important reasons is: as a component of SSFM process, the loss of the pumping light is very high. The above calculation also ignores the two influence factors, that is, the effect of walk-off angle and pump beam is impossible to be focused into a very ﬁne beam in the whole length of the crystal. Taking into account these factors, the efﬁciency of SSFM will be much lower. Mougel et al. [22] used GCOB crystals to obtain SSFM laser beam. The efﬁciency was only 0.2%. Although the above calculation shows that the SSFM efﬁciency will increase with the increase of crystal length, it is not good to use a longer crystal after considering the effect of walk-off angle and other loss factors. In addition, higher SSFM efﬁciency can be achieved only when the Nd3+ ion concentration is about 1%. Considering the real space distribution of all the light beams and the effect of walk-off angle, a result near to the experimental observation value can be obtained. The following is a brief introduction of how to use the expression published by Boyd and Kleinman [55] and correct their formula of efﬁciency-decreasing factor to calculate the laser output power of SSFM, and discuss the relationship of SSFM efﬁciency with crystal length and Nd3+ ion concentration [56] (symbols of physical quantity used are the same as reference [56]). In the case discussed, a nonlinear laser crystal with length L is placed as close as possible to the input mirror in a plano-concave resonator with reflectances R1 and R2 at fundamental wavelength for the input and output mirrors, respectively. The light is propagated along the crystal length direction z. The pump beam is focused at the entrance face of the crystal. With this design a maximum mode overlap among the pump, the fundamental and the SSFM lasers inside the cavity can be obtained within crystal length L. The pump beam is a focused Gaussian beam of TEM00 mode and the fundamental and the SSFM lasers are also Gaussian beams. The beam waists of pump beam and fundamental laser are wp0 and wc0, respectively. The spot sizes are assumed to propagate according to the following expression ! k21 z2 2 2 wp ðzÞ ¼ wp0 1 þ 2 4 2 ð11:66Þ p wp0 n1 w2c ðzÞ

¼

w2c0

k2 z 2 1 þ 2 24 2 p wc0 n2

ð11:67Þ

where k1 andk2 are the wavelengths of the pump beam and fundamental laser, respectively, and n1 and n2 are the corresponding refractive indexes. Let the intensity of the pump, the fundamental, and the SSFM lasers vary with coordinate z and radial coordinate r according to the following expression I ðr; zÞ ¼ PðzÞf ðr; zÞ f ðr; zÞ ¼

2 exp 2r 2 =w2 ðzÞ 2 pw ðzÞ

ð11:68Þ ð11:69Þ

370

11

Nonlinear Optical Properties of Laser Crystals …

where P(z) is the power of the wave as a function of z and f(r, z) is the normalized beam proﬁle for the TEM00 mode. The pump power Pp(z) as a function can be expressed as PðzÞ ¼ Pp0 exp ap z

ð11:70Þ

In the above expression Pp0 is the pump power incident upon the crystal, ap is the absorption coefﬁcient at the pump wavelength. The rate equation of the fundamental laser is dIc ¼ dt

g0 ðr; zÞ ac I c 1 þ 2Ic =Is

ð11:71Þ

where ac is the distributed loss per unit length in the crystal and Is denotes the saturation intensity of fundamental laser, Is ¼ hc=k2 re sf , the small signal gain coefﬁcient with spatial distribution g0(r,z) is expressed as g0 ðr; zÞ ¼

2re sf ap k1 Pp0 2 2 exp a z 2r =w ð z Þ p p phcw2p ðzÞ

ð11:72Þ

where re, sf, are the emission cross-section of fundamental wave and the lifetime of upper laser level, respectively. After calculation, the circulating fundamental power Pc in the cavity can be expressed as Pc ¼

p w2c Is 2G Pp0 1 2dL ln R þ 2KPp0 4q

ð11:73Þ

where d is the internal loss of the crystal, which originates from the crystal defect, scattering, diffraction, and so on. K is deﬁned by the following expression K¼

2x20 v2eff pe0 c3 n20 n3

Lk0 exp ap L=2

"

# 1 f2 ð 1 c2 Þ 0 h ðr; b; j; n; lÞ 1 þ cf

where parameters c, f and efﬁciency-decreasing factor h′(r, b, j, n, l) can be found in (11.80) and (11.81). Taking into account the reflection factors that are due to the absence of antireflection coatings on the surfaces of the crystal, the effective reflectance of the two cavity mirrors with reflectances R1 and R2 is R = [r1/2 + (R1R2)1/2]2[1 + (rR1R2)1/2]−2(r = (n2 − 1)2/(n2 + 1)2), and the factors G and q were expressed as

11.4

Self Sum-Frequency Mixing Effect in Nonlinear Laser Crystal

2re sf k1 1 exp ap L

G¼ 2p þ w 2c phc w q ¼ 1 0:92

2p w

371

ð11:74Þ

ð11:75Þ

2c 2p þ w w

2p and w 2c are the mean beam spot size for the pump and fundamental lasers where w RL 2 ¼ w

w2 ðzÞdz

0

ð11:76Þ

L

The next is to introduce the expression of P3, the power of the frequency mixing laser in resonant cavity, by a heuristic approach of Boyd and Kleinman [55] P3 ¼

2x20 v2eff Pp0 Pc pe0 c3 n20 n3

" 0

Lk0 expða LÞ

# 1 f2 ð 1 c2 Þ hðr; b; j; n; lÞ ð11:77Þ 1 þ cf

where the parameters r, b, j, n, and l represent phase mismatch, double refraction, absorption, strength of focusing, and focal position, respectively. The subscripts 1, 2, 3 of the physical quantities correspond to the pumping wave, the fundamental wave, and the frequency mixing wave. Here the parameters c, f, x0, and n0 is introduced to let x1 = x0(1 − c), x2 = x0(1 + c), n1 = n0(1 − f), and n2 = n0(1 + f), where c = (x2 − x1)/(x2 + x1) and f = (n2 − n1)/(n2 + n1). The phase matching condition n3x3 = n1x1 + n2x2 must be satisﬁed, so that n3 = n0(1 + cf) and k0 = (k1 + k2)/2. The efﬁciency-decreasing factor h(r,b,j,n,l) introduced by Boyd and Kleinman is hðr; b; j; n; lÞ ¼

0

expðla LÞ 4n

Z

nðZ 1 þ lÞ

nð1lÞ

dsds0

h i exp jðs þ s0 Þ þ irðs s0 Þ b2 ðs s0 Þ2 ð1 þ isÞð1 is0 Þ

ð11:78Þ The above formula is applicable to the case of the source beams with the same confocal parameters (such as the case of frequency doubling). In this case the confocal parameters are b = k(w0)2, r = bDk/2 (Dk is the phase mismatch), n = L/b, l = (L − 2f)/L (f is the focal position of the pump beam in the crystal, when pump beam is focused on the input surface f = 0, l = 1), j = ab/2, a = (a1 + a2 − a3)/2, a′ = (a1 + a2 + a3)/2, b = qk1w01/2 (q is the walk-off angle of the frequency mixing beam generated by the birefringence of crystal). In the case of SFM with arbitrary confocal parameters (or beam waists) of pump and fundamental laser beams, the expression of efﬁciency-decreasing factor must be extended to the case of source beam with arbitrary waist (w10, w20) or confocal

372

11

Nonlinear Optical Properties of Laser Crystals …

parameters b1 = k1(w01)2 and b2 = k2(w02)2. Introducing a so-called ﬁctitious beam and let its wave vector k0, confocal parameter b0, and beam waist w0 satisfy the following expression k0 ¼ ðk1 þ k2 Þ=2; b0 ¼ ðk1 b1 þ k2 b2 Þ=2; w20 ¼ 2 k12 w210 þ k22 w220 =ðk1 þ k2 Þ2 ð11:79Þ The frequency and refractive index of the ﬁctitious beam are deﬁned as x0 ¼ x1 =ð1 cÞ ¼ x2 =ð1 þ cÞ;

n0 ¼ n1 =ð1 fÞ ¼ n2 =ð1 þ fÞ

ð11:80Þ

Introducing b1 = b1/b0 and b2 = b2/b0 then the efﬁciency-decreasing factor h′(r, b, j, n, l) can be expressed as expðlaLÞ h ðr; b; j; n; lÞ ¼ 4nb1 b2 0

Z

nðZ 1 þ lÞ

0

dsds nð1lÞ

h i ð1 þ isÞð1 is0 Þ exp jðs þ s0 Þ þ irðs s0 Þ b2 ðs s0 Þ2 ð1 þ is=b1 Þð1 is0 =b1 Þð1 þ is=b2 Þð1 is0 =b2 Þ

ð11:81Þ When the two beams with the same confocal parameter are involved in the mixing, then b1 = b2, so that b1 = b2 = 1. Obviously (11.81) is the same as (11.78), that is, (11.78) is the expression of (11.81) in the special case. If the efﬁciency-decreasing factor h(r,b,j,n,l) is replaced by h′(r,b,j,n,l) and consider that the output mirror has a transmittance T at the frequency mixing wavelength, the absorption coefﬁcients of the crystal on the fundamental and frequency mixing beams can be neglected, then a = a′ = ap/2; therefore the output power of frequency mixing wave will be Ps ¼ P3 T ¼ Pp0 Pc T

2w20 v2eff pe0 c3 n20 n3

Lk0 exp ap L=2

"

# 1 f2 ð 1 c2 Þ 0 h ðr; b; j; n; lÞ 1 þ cf ð11:82Þ

It can be seen from (11.73) to (11.82) that the laser power output of the SSFM is a complicate function of crystal length, doping ion concentration, pump beam waist, fundamental cavity mode size, walk-off angle, phase mismatch, effective nonlinear coefﬁcient, pump beam absorption coefﬁcient, pump power, and internal loss. The relationship of the output power (efﬁciency) of NYAB crystal with several parameters is shown in Figs. 11.6, 11.7, 11.8.

11.4

Self Sum-Frequency Mixing Effect in Nonlinear Laser Crystal

373

Fig. 11.6 Typical curves of the self-frequency mixing laser output of NYAB crystal as functions of a Nd3+ concentration for different crystal lengths; b crystal length for different Nd3+ concentrations [56]

Fig. 11.7 Dependences of the self-frequency mixing laser output on the walk-off angle. Dotted curves, output at the walk-off angle of q = 2.4° for NYAB crystal [56]

Fig. 11.8 Self-frequency mixing laser output of NYAB crystal as functions of a different pump beam waists in simulating a Ti sapphire pump and b at a ﬁxed pump waist wp0 = 60 lm in simulating a LD pump, N = 5.5 at% and L = 1.7 mm for the NYAB crystal. The absorbed pump power is 200 m [56]

374

11

Nonlinear Optical Properties of Laser Crystals …

Fig. 11.9 Output power of SFD of NYAB crystal versus Nd3+ concentration for the different crystal length under direct and indirect pumping [54]

As mentioned in Chap. 10, the thermal load of the fundamental laser operation of current Nd3+ ion-doped laser crystals can be reduced by pumping directly into the upper laser level 4F3/2. This method can also be used in the operation of SFD and SSFM; the problem of small pumping absorption coefﬁcient can be solved by appropriate increase in the active ion concentration to maintain sufﬁciently high absorption efﬁciency. Especially for the SSFM, according to the above calculation, it can be seen that direct pumping to the upper laser level, being another component in the mixing process, the pump laser beam can have higher intensity, although owing to the weaker 4I9/2 ! 4F3/2 absorption, the fundamental laser intensity may be lower for certain concentration of activate ion. By appropriate choice of the active ion concentration, the new pumping method can still achieve high enough conversion efﬁciency. On the other hand, by using direct pumping method the thermal load is smaller and the temperature rise of the crystal will be lower and so bring about the improvement of the actual output efﬁciency. Figure 11.9 is a comparison of the theoretical results of SFD output power of NYAB crystal for the direct pumping and the indirect pumping.

11.5

Stimulated Raman Scattering Effect of Laser Crystal

The laser crystal with strong enough third-order nonlinear optical effect is possible to transform a fundamental laser beam into a series of Raman laser emission lines at different wavelengths by stimulated Raman scattering (SRS) effect and have been realized in Nd3+:KGW [57] and Nd3+:Gd2(MoO4)3 [58] crystals. SRS process has no phase matching requirement as those in the second-order nonlinear optical

11.5

Stimulated Raman Scattering Effect of Laser Crystal

375

processes of frequency doubling, mixing, or optical parametric oscillation; thereby has no instability caused by temperature, angle, and wavelength variations, which shows that it has advantages in producing a series of special laser wavelength. The main properties of this effect and its relationship with crystal structure characteristics will be briefly introduced in this section. It is well known that Raman scattering is a non-elastic interaction between light and optical lattice vibration (or photon and optical phonon). Photon can emit one or several phonons (Stokes scattering) or absorb one or several phonons (anti-Stokes scattering) in Raman scattering. Raman scattering cross-section is usually calculated by perturbation theory of quantum mechanics while the semi-classical theory is used to discuss some features of this effect. The dipole moment of a medium can be expressed as l = lI + lP, where lI is the dipole moment induced by external electric ﬁeld and lP is its intrinsic dipole moment. These two kinds of polarization can be changed by lattice vibration. lI is generally expressed as lI = aE (for simplicity the scalar form is written). The lattice vibration will cause the variation of induced polarization of a medium and it can be expanded with respect to vibration coordinate u in ﬁrst-order approximation as a ¼ a0 þ ð@[email protected]Þ0 u þ . . . On the other hand, the intrinsic dipole moment of the medium can also be changed by the lattice vibration, which can be expanded respect to coordinates u in the same approximation as lp ¼ l0p þ @lp [email protected] 0 u so that

l ¼ l0p þ aE ¼ l0p þ a0 E þ @lp [email protected] 0 u þ ð@[email protected]Þ0 uE

It is well known that the energy operator of dipole moment interacting with the electric ﬁeld E of external radiation ﬁeld is Hi ¼ l E Using the scalar form, it can be directly written as Hi ¼ l0p E a0 E 2 ð@lP [email protected]Þ0 uE ð@[email protected]Þ0 uE2

ð11:83Þ

The third and fourth terms of the above equation are the interaction energy of lattice vibration with external electric ﬁeld. Written in operator form, the electric ﬁeld E of the photon can be expressed as (4.5b) in Chap. 4, that is a linear combination of photon creation and annihilation operators and can be simply expressed as X

þ E¼ ð11:84Þ c1 ðkaÞaka þ c2 ðkaÞaka ka

376

11

Nonlinear Optical Properties of Laser Crystals …

On the other hand, the displacement u of lattice vibration can also be expressed as a formula in Chap. 6 in the form of linear combination of phonon creation and annihilation operators written as i Xh c1 ðqjÞbqj þ c2 ðqjÞbqjþ u¼ ð11:85Þ qj

The letters k and q are used to represent the wave vector of a photon and a phonon, respectively. The transition matrix element of the interaction of photon with phonon is hijHi jf i. Only the third and the fourth terms of (11.83) are involved in the change of photon and phonon states. E The third term involves the D þ matrix element ic1 ðkaÞc2 ðqjÞaka bqj f corresponding to absorb a photon and emit a phonon. The phonon frequency is in the infrared range, so it is called infrared absorption. The fourth term involves matrix element D E ic1 ðkaÞc2 ðk0 a0 Þc2 ðqjÞaka akþ0 a bqjþ f corresponding to absorb a photon of mode ka (frequencyxk) and emit a photon of mode k′a′ (frequency x′k′) at the same time emit a phonon of mode qj (frequencyxq), where xk > x′k′. It is Stokes Raman scattering. Equation (11.83) alsoincludes another form of matrix elements, that is D E 0 0 þ 0 ic1 ðkaÞc2 ðk a Þc1 ðqjÞaka ak a bqj f corresponding to absorb a photon of mode k′a′ (frequencyx′k′), emit a photon of mode ka (frequency xk), and at the same time absorb a phonon of mode qj (frequencyxq); it is the inverse process of Stokes scattering and is called anti-Stokes scattering. Referring to (4.2), the calculation of the matrix element of photon creation and annihilation operator shows that the probability of positive process is proportional to [p(xk′) + 1]p(xk)(∂a/∂u)20 while the probability of inverse process is proportional to [p(xk) + 1]p(xk′)(∂a/∂u)20, where p(xk) and p(xk′) are the photon numbers of incident light and scatter light, respectively. In the general Raman scattering process, because of p(xk′) < < p(xk), the probability of the inverse process is much lower than that of the positive process. In this spontaneous Raman scattering process the medium has no ampliﬁcation effect on the scattering light of frequency xk′. It can be shown [59] that the third-order nonlinear optical coefﬁcient of a medium is the negative imaginary part of the refraction index of Raman scattered light. When the medium has a larger v3, it will have a sufﬁciently large ampliﬁcation effect on the Raman scattering light; therefore under a strong pumping, the gain of the Raman scattering light is enough to overcome its loss and can generate a stimulated Raman emission. The important difference of the SRS with the spontaneous Raman scattering is the scattering light of SRS is a coherent light and the intensity of scattered light increases exponentially with its distance through a medium. In addition, because the gain factor of stimulated scattering is proportional to the incident light intensity in the unit solid angle, if the gain medium is placed inside a cavity it has the so-called “cleanup effect” which makes the light beam quality of the scattering light better than that of the incident light. Therefore, the poor pump light quality can be converted to Gaussian laser beam output of the Raman laser. A detail discussion on these important nonlinear optical effects can be referred to the literatures [60] and [61].

11.5

Stimulated Raman Scattering Effect of Laser Crystal

377

Raman lasers utilize the SRS effect of the materials to shift the laser frequency to a series of Stokes and anti-Stokes laser lines. In order to make the Raman laser have a higher efﬁciency, it is necessary to have a higher total Raman gain G. It can be proved that the light intensity Is(l) of the ﬁrst Stokes Raman scattering has the following relation with the length l of the Raman medium the light passed Is ðlÞ ¼ Is ð0Þ exp gR Ip l

ð11:86Þ

where Ip is the pump intensity and gR is the Raman gain coefﬁcient. The total Raman gain G of the medium obviously is G ¼ gR Il

ð11:87Þ

Raman gain coefﬁcient gR can also be expressed as gR / qn ð@[email protected]Þ=m3s Dms

ð11:88Þ

In the above expression qn is the phonon density, (∂r/∂X) is called the differential scattering cross-section of Raman scattering (from previous derivation, it is shown that this cross-section is proportional to (∂a/∂u)20) and ms is the frequency of Raman scattering light with linewidth Dms. Therefore, the requirement of Raman laser on its working material is: the Raman linewidth should be narrow, the differential cross-section should be high. Of course, the material must be transparent in the spectral region of Raman emission. From this basic requirement, we can study the relationship of SRS performance with the structure and the chemical composition of materials. Raman line broadening is induced by the anharmonic interaction of a crystal, in which one phonon decays into two other phonons. One can easily imagine that Raman spectral linewidth will be narrow for the materials with weak anharmonic interaction. It is well known that the thermal conductivity and the thermal expansion properties of a crystal are involved with the anharmonic interaction. Therefore, the requirement for narrow Raman linewidth to the materials is consistent with that of the high thermal conductivity and small thermal expansion. In other words, materials with high thermal conductivity and small thermal expansion have narrow Raman line. It is easy to imagine that the width of Raman line is proportional to the coefﬁcient of linear expansion aL and inversely proportional to speciﬁc heat Cv and compressibility Kc Dms / aL =Kc Vc

ð11:89Þ

On the other hand, the high gain coefﬁcient requires the materials have high values of polarizability a and high values of ∂a/∂u. Two cases can satisfy these requirements. First case is a has a relatively high value and also has a great variation with the vibration; second case is a has not as high as the ﬁrst case but has a greater variation with the vibration.

378

11

Nonlinear Optical Properties of Laser Crystals …

The crystals consist of molecule groups having the so-called “breathing vibrational mode” which belong to irreducible representation A1g having a maximum polarizability variation ∂a/∂u, also have a lowest-lying energy level of charge transfer to act as an intermediate state to generate a high value of polarizability tensor, because the value of polarizability tensor is inversely proportional to the square of energy interval between initial state and intermediate state. Therefore, the tungstate, molybdate, vanadate, and nitrate have both high values of a and ∂a/∂u, thus have a high Raman scattering gain. The second case is like the crystals such as diamond. They have the advantage of the covalent crystal and have a higher value of ∂a/∂u than that of the ionic crystals although without low-lying charge transfer level of molecular group to act as intermediate state to result in a high value of polarizability. In addition, as will be mentioned below, the very narrow Raman spectral linewidth of diamond makes it have a very high Raman gain coefﬁcient. The data of Raman gain coefﬁcient, Raman linewidth, and Raman frequency shift of some typical materials are given in Table 11.1. Stankov and Marowsky [57] used Nd3+:KGW crystal pumped by flash lamp and electro-optic Q switched to obtain 1067 nm fundamental wave laser, then by the self SRS effect directly produce a ﬁrst Stokes Raman line at 1180.8 nm, a second Stokes line at 1321.5 nm, and a ﬁrst anti-Stokes Raman line at 973.5 nm. By the frequency doubling and mixing effects of nonlinear optical crystal LiIO3, laser emissions of 355.6, 367, 378, 393, 408, 423, 440, 533.5, 560, 590, 620, and 660 nm, altogether 12 different wavelengths of ultraviolet and visible light were obtained. Chang [65] demonstrated a continuous-wave self-Raman laser with high Table 11.1 Relevant data of several materials with high gain coefﬁcient of Raman scattering Molecular formula

Gain coefﬁcient (cm/GW)

Linewidth (cm−1)

Raman shift (cm−1)

PbWO4 [62] 8.4 (532 nm) 900 5.0 (1064 nm) 2.7 921 SrWO4 [63] 8.5 (1064 nm) 1.6 926 BaWO4 [63] 30 (532 nm, estimated value) 940 La2(WO4)3 [66] 6 (1064 nm) 5.9 901.5 KGd(WO4)2 [61] 5.7 (1064 nm) 886 SrMoO4 [64] 3.1 768 Li3Ba2Gd3(MoO4)8 [61] 4.7 (1064 nm) 4.5 (1064 nm) 0.732). Then, because of the much higher ionicity between the rare earth cation and the fluorine anion and much weaker polymerized network in the HMF glasses compared with oxide glasses, the regularity of the site occupied by the rare earth ion in the HMF glasses is much higher than that in the oxide glasses, and increases as the rare earth ion radius decreases. For example, Tm3+ ions in silica-based glasses possess one distinct type of site with a broad distribution of bond lengths or angles (low regularities), whereas in ZBLAN glass they are found to possess more than one distinct type of sites with a narrow distribution of bond lengths and angles (high regularities). Owing to the role of rare earth fluorides (ReF3) as intermediate element in these glasses, they are able to be both in and out of network positions. This implies that rare earth ions in HMF glasses are more evenly distributed. This behavior is in distinct contrast with oxide glasses, in which rare earth ions play only the glass modiﬁer role. Further, the multi-component nature of these HMF glasses allows the rare earth ion–ion separation characteristic to be more remarkable than that in the common silica-based oxide glasses. The fact that fluorescence quenching of Er3+ in the ZBLAN glass occurs at higher Er3+-doping level than in the oxide glasses is in accord with the prediction by the crystal chemistry model. Similarly, it can be predicted that the rare earth concentration-dependent fluorescence quenching effect is also less in fluorophosphate glasses, because the rare earth is also an intermediate element in this glass. Clearly, the crystal chemistry model for the local structure of rare earth ions in glasses can well describe and predict the spectral properties of the active ions, including the concentration-dependent fluorescence quenching effect.

12.2

Apparent Crystal Field Hamiltonian for Rare Earth Ions in Non-crystal Host

The rare earth-doped non-crystal and polycrystal play more important role in the photoelectronic area. Besides the popular oxide and fluoride glasses, the rare earth-doped sulﬁde glass can also be prepared as bulk, ﬁber, and ﬁlm devices and

392

12

Apparent Crystal Field Model of Laser Glass and Its Application

become scholarly interests due to its low phonon energy, high refractivity, and transparent in infrared. The Er3+ and Pr3+-doped ﬁber ampliﬁers are the key element in optical ﬁber communications. Different from that in the crystals, local environment of rare earth ions in the above hosts are variant. Local structures around rare earth ions in non-crystal materials can be investigated using, for example EXAFS, neutron or X-ray scattering, and fluorescence line narrowing (FLN) laser spectroscopy. Unlike the case of crystal, except the method of FLN, only the average result, that is, the average number of coordination around rare earth ion, the average distance between the rare earth ion and the ligands, and the “average” local symmetry are obtained. The method of FLN still cannot determine the local structures exactly. Consequently, the direct relation between the point symmetry of the site occupied by a rare earth ion and its energy level splitting cannot be built through crystal ﬁeld Hamiltonian like in crystals. Strictly, a rare earth ion cannot occupy a position with point symmetry higher than C1 in non-crystal host. It means that radiative transition polarized in any direction is permitted without retraction coming from point group symmetry selection rule. Furthermore, the lack of long-range correlation between sites prevents the use of polarization behavior as a criterion to identify a given transition. Nevertheless, certain features common to the entire set of spectra indicate that some degree of local order persists in the immediate environment of the emitting ion, which has been proved in the above analysis of glass structure. Conventionally, the analysis of crystal ﬁeld levels for rare earth ions in non-crystal host by means of the crystal ﬁeld theory is generally focused on the Eu3+ ions with small J number on the basis of the model proposed by Brecher and Riseberg [5]. In this model, the C2v point group is adopted to describe the “average” local symmetry, that is, the “average” crystal ﬁeld Hamiltonian. The major reasons for adoption of the C2v are as follows. First, it is the highest symmetry in which full splitting of the 7 F1 and 7 F2 levels is allowed. Secondly, it is a subgroup of almost all the point groups with higher symmetry in which rare earth ions are normally found, enabling application of the standard technique of descending symmetries. And ﬁnally, it is the lowest symmetry for which simple crystal ﬁeld calculations can be routinely performed at that time. This model can explain the crystal ﬁeld splitting of Eu3+ ions in glasses very well. Although the model was proposed for Eu3+ ions in silicate glasses, it has subsequently been applied to the analysis of rare earth ions in many kinds of non-crystal hosts [12–14]. To explain the model clearly, Brecher and Riseberg assumed the geometrical structure of the coordination around Eu3+ ions in silicate and fluoride glasses [5, 15]. However, experimental results have shown that the ligand environments, that is, the point symmetries, around the rare earth ions in non-crystal hosts are variant and do not support the assumption of single local environment. Consequently, the physical basis of choosing C2v to describe the crystal ﬁeld of rare earth ions in glasses is not very sound. Moreover, the model only allows four transitions between 5 D0 and 7F2 multiplets for Eu3+ ions, but the whole ﬁve transitions have been observed in spectral experiments. Many spectral experiments have also revealed that all the transitions between crystal ﬁeld levels are allowed for rare earth ions in

12.2

Apparent Crystal Field Hamiltonian for Rare Earth Ions in Non-crystal Host

393

non-crystal hosts as in crystals with low symmetry, although the structure of energy levels has the character of high point symmetry [16, 17]. This also cannot be explained by the above model. To relate the spectral properties of rare earth ions and the effect of ligand ions in non-crystal materials more close to the reality, it is necessary to establish a simple and practical crystal ﬁeld model with sound physical basis from the real ligand conditions around the rare earth ions in non-crystal hosts. The model is expected to describe the spectral properties and the average results of energy level splitting, and called apparent crystal ﬁeld model. Owing to the fact that the crystal ﬁeld is variable in non-crystal host, the group chain scheme introduced in Chap. 3 may be a simple and effective way for this purpose. The group–subgroup relation of the 32 point groups (imbeddings of the crystallographic point groups [18]) is shown in Fig. 12.3. The distortion from high to low symmetries step by step is displayed clearly in the ﬁgure. With the high point symmetries descending to low ones, the representations of group O3 or SO3 reduce to their subgroups. The eigenfunctions of crystal ﬁeld levels and the crystal ﬁeld Hamiltonian Hcf are expressed by a series of the irreducible representations of the group chain from group to subgroup step by step. Suppose that the active ions occupy the positions having the symmetry of point group G, then the Hcf is invariant under the action of any elements of G, that is, it transforms as the scalar irreducible representation. As an example, for the condition of G = D4, considering the group chain to be SO3 O D4 ; Hcf , Hcf can be expressed as Hcf ¼

X

Clk bkl ¼ C32 b23 þ C14 b41 þ C34 b43 þ C16 b61 þ C36 b63

ð12:1Þ

k;l

The parameters in this expression are deﬁned in Chap. 3. When the symmetry of environment descent to its subgroup G1, the terms in HcfG1 should belong to identical representation of G1. Furthermore, the group–subgroup branching rule tells us that the identical representation of G is still identical representation of G1 when symmetry goes down from G to G1. Therefore, all the terms Fig. 12.3 Group–subgroup relation of the 32 point groups [18]

Oh D 4h

Th

O

C 4h D 4 D 2d C 4v D2h S4 C4 Ci

Td T

D 6h D6

C 6h C 6v D 3d D 3h

D 2 C 2h C 2v C 6 C 3i D 3 C 3v C 3h C2

Cs C1

C3

394

12

Apparent Crystal Field Model of Laser Glass and Its Application

in HcfG will appear in HcfG1 such as can be seen from Table 3.17. The terms of Hcf with point group of higher symmetry, for example, O, will appear in most of the Hcf with different point groups of lower symmetry. The lower symmetry position is actually some kind of distortion from high symmetry position and the distortion potential is always smaller than the high symmetry potential. For rare earth ions in a glass, the terms of Hcf of rare earth ions in higher symmetry positions will appear “repeatedly” in most of the Hcf of rare earth ions in different lower symmetry positions and then take a more important part than other terms belonging only to the particularly lower symmetry position in the effective Hcf. Contrary to the choice of C2v which is a subgroup of almost all the higher symmetry point groups [5], we consider a high symmetry point group with many subgroups of lower symmetry to describe the apparent crystal ﬁeld of rare earth ions in glasses. The corresponding crystal ﬁeld Hamiltonian is called the apparent crystal ﬁeld Hamiltonian Hcfa . For a given rotation group G, its isomorphic groups and its corresponding rotation-inversion direct product group Gi = G Ci have the same mathematical expression of Hcf [19]. We ﬁrst choose O, including Td and Oh, which have the same expression of Hcf, as the high-point symmetry group (see Fig. 12.3). The point symmetry D6 (or C6v, D3h, D6h) is not considered because positions with symmetry of 6-fold rotation axis are rarely observed for active ions in crystal [20] and so in glasses. In the group chain scheme, the Hcf of O point symmetry HcfO has only two terms, one for k = 4 and the other for k = 6, which will express the major terms of the corresponding rank of Hcf for rare earth ions in glass Hcfa . The term of k = 2 only appears in crystal ﬁeld with symmetry of group D4 (including C4v, D2d, and D4h), D3 (including C3v and D3d) and lower symmetry groups, so there are two possible choices for this term. After these considerations, the Hcfa may be written in a “simpliﬁed” group chain [21, 22] SO3 O D4 as Hcfa ðD4 Þ ¼ C32 b23 þ C14 b41 þ C16 b61

ð12:2Þ

Hcfa ðD3 Þ ¼ C52 b25 þ C14 b41 þ C16 b61

ð12:3Þ

or SO3 O D3 as

In these equations, the terms C14 b41 and C16 b61 belong to the HcfO and still exist in the Hcf of its subgroup D4 and D3. The other terms of k = 4 and 6 in D4 and D3, which do not belong to identical representation of point group O, can be neglected because these components of crystal ﬁeld are perturbation of crystal ﬁeld of symmetry O. As a result, in the expressions of Hcfa , only three crystal ﬁeld parameters C32 (or C52 ), C14 , and C16 , one for each k, will be ﬁtted by the values of crystal ﬁeld splitting data. From (9.3.7) in [18], it can be easily shown that the relationship between the crystal ﬁeld parameters of the conventional JM scheme Bkq and the group chain scheme Clk are:

12.2

Apparent Crystal Field Hamiltonian for Rare Earth Ions in Non-crystal Host

395

For D4 point symmetry: rﬃﬃﬃ rﬃﬃﬃ rﬃﬃﬃ rﬃﬃﬃ 7 5 1 5 7 4 B40 þ B44 ; ¼ B44 ; C3 ¼ B40 3 6 2 3 6 rﬃﬃﬃ pﬃﬃﬃ 7 1 1 7 1 B64 ; C36 ¼ C16 ¼ pﬃﬃﬃ B60 þ B60 þ B64 2 2 2 2 2 2

C32

B20 ; C14

1 ¼ 2

ð12:4Þ

and the relationship for D3 point symmetry has been shown in (3.31). As having introduced above, the crystal ﬁeld theory has been widely used to analyze the energy level splitting of rare earth ions in crystals. However, a quantitative comparison of crystal ﬁeld strengths for rare earth ions in different materials cannot be made directly from the crystal ﬁeld parameters. Therefore, as having mentioned in Chap. 9, the concept of scalar crystal ﬁeld strength was introduced by Auzel [23, 24]. The relation between the scalar strength Nv and the crystal ﬁeld parameters is " #1=2 " #1=2 X 4p 2 X 4p 2 k Nv ¼ ¼ Bkq Cl 2k þ 1 2k þ 1 k;q k;l

ð12:5Þ

The strength of crystal ﬁeld for rare earth ions in crystals and glasses can be analyzed by means of the parameter Nv. Whatever the symmetry, the strengths of crystal ﬁeld for rare earth ions between different crystals, furthermore, between crystal and non-crystal can be analyzed and compared quantiﬁcationally [13, 14, 23–25]. Subsequently, Leavitt [26] proposed the invariants of quadratic rotation as "

1 X 2 sk ¼ Bkq 2k þ 1 q

#1=2

"

1 X k 2 ¼ Cl 2k þ 1 l

#1=2 ð12:6Þ

Obviously, these invariants express the contributions of components k = 2, 4, and 6 to the whole strength of crystal ﬁeld. The relationship between the invariants and the scalar strength is " Nv ¼ 4p

X

#1=2 ðsk Þ

2

ð12:7Þ

k¼2;4;6

Auzel and Malta [24] related the invariant sk with the maximum splitting of multiplet DE, that is, the gap between the highest and lowest crystal ﬁeld levels in multiplet 2S+1LJ, as

396

12

ðDEÞ2 ¼

Apparent Crystal Field Model of Laser Glass and Its Application

E 2 D X

D E

2 12g2a

2

½SLJ U ðkÞ ½SLJ f C ðkÞ f ðsk Þ gðga þ 2Þðga þ 1Þ k¼2;4;6 ð12:8Þ

where g = (2J + 1), ga is the effective degeneracy of the multiplet: ga = g/2 if J is a half-integer. Furthermore, for the multiplets with J 3 and the difference of

½SLJ U ðkÞ ½SLJ 2 for different k less than a factor of 10, the maximum splitting of multiplet and the scalar strength of crystal ﬁeld can be related by

3g2a DE ¼ p gðga þ 2Þðga þ 1Þ

# 1=2 " Y D E

D E 1=3 ðkÞ

Nv

½SLJ U ½SLJ

f C ðkÞ f

k¼2;4;6

ð12:9Þ As an example, for the common active ion Nd3+ in solid-state laser materials, the scalar strength of crystal ﬁeld can be estimated from the maximum splitting of 4I9/2 multiplet in various hosts. In Chap. 9, the analysis of self-activated Nd3+ laser crystal on the basis of the scalar strength of crystal ﬁeld introduced by Auzel has been mentioned. The relation between the splitting of the 4I9/2 multiplet and the scalar strength of crystal ﬁeld for Nd3+ in a series of crystal and non-crystal materials is shown in Fig. 12.4. The relation obeys (12.9). Besides applications in the analysis of spectra and energy levels, the scalar strength of crystal ﬁeld can be related with other properties. For example, though there isn’t a general theory of melting points of solids (Tm), it may be related with Nv by [27] Tm 0:48 Nv þ 300

ð12:10Þ

where the intercept (300 °C) corresponds to the B00 term not contained in Nv. The parameter Nv is also related with the hardness and cohesive energy of crystals [27]. The authors and Auzel compared the strengths of crystal ﬁeld for different rare earth ions in a host by means of Nv [28, 29]. From Fig. 12.5, it can be found that there is a linear relationship between the scalar strength of Nd3+ and Er3+ in different crystals. An empirical relation between the crystal ﬁeld strengths of Nd3+ ions with electron conﬁguration 4f 3 and rare earth ions with 4fq has been proposed by Auzel [29]. NV ð4f q Þ ¼ NV 4f 3 0:034ðq 3ÞNV 4f 3 Therefore, from the crystal ﬁeld strength of one rare earth ion in a host, the crystal ﬁeld strength of other rare earth ions in the host can be estimated. This is more beneﬁcial to the Yb3+-doped materials. It is obvious that the scalar crystal

12.2

Apparent Crystal Field Hamiltonian for Rare Earth Ions in Non-crystal Host

397

1-NdP5O14, 2-LiNd(PO3)4, 3-Na2Nd2Pb6(PO4)Cl2, 4-Na5Nd(WO4)4, 5-Na(La,Nd)(WO4)2, 6-K5Nd(WO4)4, 7-K5Nd(MoO4)4, 8-NdAl3(BO3)4, 9-Na18Nd(BO3)7, 10-NdCl3, 11-(Nd,La)Ta7O19, 12-LiNdNbO4, 13tellurite glass, 14-Nd2O2S, 15-CaF2, 16-YAlO3(La,Nd), 17-Y3Al5O12(La,Nd), 18-Ba2MgGe2O7, 19NdNb5O14, 20-silicate flint glass, 21-Gd1.7Nd0.3(MoO4)3, 22-Li(Y,Nd)F4, 23-(Nd,La)F3, 24-Nd(C2H5ZO4)3, 25-Ca5(PO4)3F, 26-KY3F10, 27-Nd2S3, 28-YVO4, 29-PbMoO4, 30-LiNbO3, 31-phosphate glass, 32KY(MoO4)2, 33-CaAl4O7, 34-La2O3, 35-LaOF, 36-CaWO4, 37-NdCl3 in ice

Fig. 12.4 Maximum splitting of multiplet 4 I9=2 Nd3 þ versus Nv for different host materials [27]

ﬁeld strength has important application in the analysis of rare earth ion-doped laser materials. In the apparent crystal ﬁeld model mentioned above, there is only one term for each k in the expressions of Hcfa in (12.2) and (12.3). Therefore, for rare earth ions in non-crystal host, the invariant of quadratic rotation in (12.8) can be substituted directly by the crystal ﬁeld parameter

X ½SLJ U ðkÞ ½SLJ 2 f C ðkÞ f 2 2 12g2a Clk ðDE Þ ¼ gðga þ 2Þðga þ 1Þ k¼2;4;6 2k þ 1 2

ð12:11Þ In the conventional analysis of spectra and crystal ﬁeld for rare earth ions in crystals, the crystal ﬁeld parameters are related with the crystal ﬁeld splittings of multiplets through the crystal ﬁeld Hamiltonian. The parameters can be obtained by calculating the eigenvalues of perturbation matrix and ﬁtting with the values of splittings recorded in low temperature spectral experiments. Now, on the basis of

398

12

Apparent Crystal Field Model of Laser Glass and Its Application 19

3500

15 Bi4Ge3O12

N v of Er 3+ (cm-1 )

3000 2500

11 13

17CaF2

14

LiYF4 CsCdBr3

2000 1500

5 3

1000 1

500 0

0

1000

6

Y2O3

20Y3Sc2Al3O12 Y3Al5O12 21 18Y3Ga5O12

Cs2NaRCl6 16YAlO3

9

CaWO4 12 NaLa(MoO4)2 YVO4 LaF3 10 LiRP4O12 YPO4 7LuPO4

8

4R(C2H5SO4)3°¡ 9H2O ThGeO4

LaCl3 LaBr3 2

2000

3000 3+

4000

5000

-1

Nv of Nd (cm ) 1-LaCl3, 2-LaBr3, 3-ThGeO4, 4-R(C2H5SO4)3⋅9H2O, 5-YPO4, 6-LiRP4O12, 7-LuPO4, 8-YVO4, 9La(MoO4)2, 10-LaF3, 11-CsCdBr3, 12-CaWO4, 13-LiYF4, 14-Cs2NaRCl16, 15 -Bi4Ge3O12, 16-YAlO3, 17CaF2, 18-Y3Ga5O12, 19-Y2O3, 20-Y3Sc2Al3O12, 21-Y3Al5O12

Fig. 12.5 Crystal ﬁeld strength of Nd3+ and Er3+ ions in different crystals

the apparent crystal ﬁeld model, the crystal ﬁeld parameters for rare earth ions in non-crystal hosts can be related with the maximum splittings of multiplets by (12.11) and the absolute values of the parameters can be obtained simply by linear ﬁtting process. The calculation is simple and the result is explicit; furthermore, the requirement of spectral experiment is not excessive. As mentioned above, the large inhomogeneous spectral line widths of rare earth ions in non-crystal hosts cause a lot of trouble to identiﬁcation of the spectral lines, which related to the transitions between crystal ﬁeld levels; so it is very difﬁcult to determine all the splittings in a multiplet. Especially, for the rare earth ions having important application in solid-state laser materials, such as Er3+ and Nd3+, the determination is more difﬁcult due to the large J value of the multiplets related to laser operation and so the large number of crystal ﬁeld levels. By means of the apparent crystal ﬁeld model, the crystal ﬁeld parameters for rare earth ions in non-crystal hosts can be calculated from only the maximum splittings but not every splittings in the multiplets. It means that the parameters may be obtained after the width of spectral band corresponding to the transitions between multiplets is measured at low temperature. Then, the crystal ﬁeld parameters can be used to analyze the properties of spectra and laser of non-crystal materials. Conventionally, the disorder of non-crystal materials causes a lot of trouble to the analysis of crystal ﬁeld and spectra of rare earth ions doped inside. Quite the contrary, on the basis of the apparent crystal ﬁeld model, the disorder makes the calculation and analysis simpler than those in crystals. Auzel adopted a higher icosahedral symmetry further to describe the apparent crystal ﬁeld of non-crystal

12.2

Apparent Crystal Field Hamiltonian for Rare Earth Ions in Non-crystal Host

399

and make the calculation more simple [30]. It can also be used to analyze the spectral characteristics of rare earth ion in glasses but cannot deal with the subtle crystal ﬁeld splittings of a multiplet.

12.3

Crystal Field Level Analysis for Er3+ Ions in Three Typical Glasses

Silicate, germanate, and ZBLAN glasses are three kinds of host materials widely used in solid-state laser. Especially, the ZBLAN is the medium of the Er3+-doped ﬁber ampliﬁer, which is one of the key elements in the DWDM technique of optical communications. In the following, the crystal ﬁeld splittings of Er3+ ions in the three glasses are systematically analyzed on the basis of the apparent crystal ﬁeld model [21, 22]. The samples used in the measurement of spectra, that is, silicate, germanate, and ZBLAN glasses of formulas SiO2–Na2O, GeO2–BaO–K2O, and ZrF4–BaF2–LaF3– AlF3–NaF, respectively, were cooled to 13 K. Absorption spectra of Er3+ ions were recorded in a range from 400 to 1600 nm corresponding to the transitions from 4 I15=2 ! 2 G9=2 to 4 I15=2 ! 4 I13=2 . A 488 nm Ar+ ion laser was used to excite Er3+ ions to their 4F7=2 multiplet. Fluorescence spectra corresponding to the 4 S3=2 ! 4 I15=2 ; 4 S3=2 ! 4 I13=2 , 4 F9=2 ! 4 I15=2 ; 4 I11=2 ! 4 I15=2 , and 4 I13=2 ! 4 I15=2 transitions were measured. The absorption and emission spectra recorded at 13 K were resolved into different components with Voigt-type proﬁle. This proﬁle was chosen because the linewidth may contain homogeneous and inhomogeneous broadenings with Lorenzian and Gaussian proﬁles, respectively. The central position, FWHM, and area of each separated spectral line were determined. At 13 K, the higher levels in multiplets have much lower populations and the spectra are predominated by the transitions from the lowest levels in multiplets. As an example, Fig. 12.6 shows the ﬁtted Voigt components in the emission spectral bands of the transition from 4 S3=2 to 4 I15=2 for Er3+ ions in the silicate, germanate, and ZBLAN. The spectral lines corresponding to transitions from the lower crystal ﬁeld level (level 1 in the ﬁgure) in 4 S3=2 to all the crystal ﬁeld levels (levels 1–8 in the ﬁgure) in 4 S15=2 are pointed out. Previous studies on Eu3+ ions in glasses have shown that, due to the low-point symmetries of the sites occupied by rare earth ions, the multiplets of the ions split thoroughly [7, 15]. For Er3+ ions, the J multiplet splits into (2J + 1)/2 crystal ﬁeld levels after taking into account the Kramers degeneracy. Owing to the large inhomogeneous width, some of the spectral lines mix in one Voigt proﬁle and make the number of observable lines, corresponding to the transitions between some couples of multiplets, less than the number of expected spectral lines. In view of this, the FWHM, the area under spectral line corresponding to the intensity of transition, and the expected number of spectral lines are considered. For a line with

400

12

Fig. 12.6 Voigt proﬁle ﬁt to the emission spectra of 4 S3=2 ! 4 I15=2 transitions of Er3+ at 13 K. a Silicate, b germanate, and c ZBLAN

Apparent Crystal Field Model of Laser Glass and Its Application

(a)

1 7+8

1 4+5 1 2+3

1 6

(b)

1 1

1 7+8 1 4+5 1 6

1 3 1 1+2 1 4+5

(c)

1 7+8

1 3 1 2 1 1

1 6

17500

17750

18000

18250

18500

18750

extremely large values of FWHM and area, more than one transition can be reasonably involved in the line. Some of the mixing lines will be separated after all the related experimental spectra are resolved. Finally, the central positions and widths of the crystal ﬁeld levels for Er3+ ions in silicate, germanate, and ZBLAN glasses obtained from the above resolving are listed in Table 12.1. The uncertainty on the crystal ﬁeld level positions determined from the experimental spectra is 12 cm−1 for all the three glasses. When two levels are overlapped together, another choice is also given in the table and signed by “*”: we assume that the two levels have the same shape and that their central positions are separated by a distance as large as possible before they can be separated by the procedure mentioned above, then we have (Rayleigh criterion) w ¼ 0:7ðw1 þ w2 Þ; w1 ¼ w2 so that

12.3

Crystal Field Level Analysis for Er3+ Ions in Three Typical Glasses

Table 12.1 Positions and widths of crystal ﬁeld levels of Er3+ ions in silicate, germanate and ZBLAN glasses from experimental spectra at 13 K (cm−1).

Manifold

Position

401 Width

* 4

I15=2

4

I13=2

4

I11=2

4

I9=2

4

F9=2

4

S3=2

2

H11=2

0 23 50 70 139 295 414 414 6498 6503 6540 6559 6582 6760 6820 10,205 10,223 10,240 10,240 p 10,338( ) p 10,338( ) 12,384 12,438 12,543 12,614 12,614 15,203 15,232 15,348 15,392 15,494 18,291 18,348 19,129 19,161 19,210 19,268 19,301 19,323

p 386( ) p 443( )

p 10,228( ) p 10,252( ) 10,321 10,355

p 12,601( ) p 12,627( )

* 0.5 11 15 38 45 147 133 23 24 24 26 47 81 68 13 18 54 p 79( ) 79 49 98 60

p 95( ) p 95( )

p 39( ) p 39( ) 56 56

p 43( ) p 43( )

28 39 58 55 60 35 99 24 44 36 52 20 24 (continued)

402 Table 12.1 (continued)

12

Apparent Crystal Field Model of Laser Glass and Its Application Manifold

Position

Width *

4

F7=2

4

F5=2

4

F3=2

2

G9=2

20,456 20,522 20,572 20,613 22,145 22,145 22,265 22,509 22,610 24,440 24,516 24,555 24,606 24,642

p 22,136( ) p 22,154( )

* 30 55 32 99 44

p 31( ) p 31( )

52 61 75 64 61 49 40 38

(b) 4

4

4

4

I15=2

I13=2

I11=2

I9=2

0 35 63 95 95 274 377 457 6488 6500 6530 6564 6595 p 6754( ) p 6754( ) 10,202 10,224 10,224 10,224 10,330 10,330 12,386 12,432 12,542 p 12,615( ) p 12,615( )

p 82( ) p 108( )

6719 6788

18 29 21 60 161 135 94 5 20 10 8 40 p 160( )

p 43( ) p 43( )

114 114

7 65 p 10,316( ) p 10,343( )

12,605 12,625

64 102 32 80 p 47( )

p 46( ) p 46( )

34 34 (continued)

12.3

Crystal Field Level Analysis for Er3+ Ions in Three Typical Glasses

Table 12.1 (continued)

Manifold

Position

403 Width

* 4

F9=2

4

S3=2

2

H11=2

4

F7=2

4

F5=2

4

F3=2

2

G9=2

15,183 15,219 15,337 15,382 15,480 18,262 18,329 19,108 19,145 19,186 19,255 19,280 19,309 20,425 20,498 20,549 20,586 22,119 22,119 22,242 22,496 22,594 24,427 24,509 24,549 24,593 24,629

p 22,108( ) p 22,129( )

* 12 28 48 31 54 35 43 36 14 18 47 0 6 31 48 14 100 48

p 34( ) p 34( )

25 72 54 107 25 25 17 38

(c) 4

4

I15=2

I13=2

0 47 111 154 194 226 p 308( ) p 308( ) 6542 6569 6603 6631

275 341

40 54 51 30 57 82 p 154( )

110 110

29 32 18 33 (continued)

404 Table 12.1 (continued)

12

Apparent Crystal Field Model of Laser Glass and Its Application Manifold

Position

Width *

6696

4

I11=2

4

I9=2

4

F9=2

4

S3=2

2

H11=2

4

F7=2

4

F5=2

4

F3=2

2

G9=2

6696 6780 10,228 10,289 10,289 10,289 10,289 10,289 12,413 12,472 12,538 p 12,617( ) p 12,617( ) 15,271 15,301 15,361 15,398 15,449 18,429 18,525 19,160 19,203 19,235 19,267 p 19,309( ) p 19,309( ) 20,541 20,586 20,643 20,643 22,244 22,273 22,273 22,571 22,664 24,545 24,582 24,631 24,689 24,689

p

6677( ) p 6715( ) p 10,267( ) p 10,285( ) p 10,289( ) p 10,293( ) p 10,311( )

12,604 12,630

19,300 19,318 p 20,619( ) p 20,667( ) p 22,264( ) p 22,282( )

p 24,679( ) p 24,699( )

*

87 81 20 59

4 35 40 p 61( ) 26 44 47 8 62 11 46 18 3 0 0 p 42( ) 20 18 114 24 44 30 69 0 18 17 47

p 62( ) p 62( ) p 30( ) p 30( ) p 30( ) p 30( ) p 30( )

44 44

30 30 p 81( ) p 81( ) p 31( ) p 31( )

p 34( ) p 34( )

12.3

Crystal Field Level Analysis for Er3+ Ions in Three Typical Glasses

405

w ¼ 1:4 w1 where w is the total width determined by spectral line while w1 and w2 are, respectively, the widths of the two single levels. As a result, the central positions of the two levels are xc1 ¼ xc 0:3w1 ; xc2 ¼ xc þ 0:3w2 where xc is the central position of the mixing level, while xc1 and xc2 are the central positions of the two levels, respectively. After the apparent crystal ﬁeld analysis presented in the following, p one of these two data for overlapping levels will be chosen and signed by “( )” in Table 12.1. To relate the crystal ﬁeld splitting of Er3+ ions with the apparent crystal ﬁeld, the parameters Clk were ﬁrst estimated through ﬁtting the crystal ﬁeld splittings listed in Table 12.1 directly by the apparent crystal ﬁeld Hamiltonian expressed in (12.2) or (12.3) in the conventional way [31]. Simultaneously, (12.11) for the scalar crystal ﬁeld strength could also be used to derive the absolute values of parameters Clk by ﬁtting the experimental values of DE obtained from Table 12.1 by a least-squares ﬁtting procedure. Then, the signs of the values were determined by comparing the crystal ﬁeld splittings calculated from the parameters Clk by (12.2) or (12.3) and the experimental data. In the calculations, the intermediate coupling wavefunctions given by Weber [32] and the values of reduced matrix elements aSL U ðkÞ aSL provided in [33] were used to obtain the values of ½SLJ U ðkÞ ½SLJ ; and the J-mixing was not taken into account. To verify the assumption on Hcfa , a series of Hamiltonian Hcf from point symmetry O (including Td and Oh), D4 (including C4v, D2d, and D4h), D3 (including C3v and D3d), to D2 (including C2v and D2h), which contain all the possible crystal ﬁeld parameters, were also adopted to ﬁt the crystal ﬁeld splittings of Er3+ ions in the three glasses. The root-mean-square (RMS) deviations of all the calculations are shown in Fig. 12.7a, b, and c, respectively, for Er3+ ions in silicate, germanate, and ZBLAN. Because some of the crystal ﬁeld levels cannot be resolved in the experiment, different possible choices of level structure should be considered and the ranges of the RMS deviations are represented by error bars in Fig. 12.7. On the x-axis, the various point symmetries used in the analysis are distributed: the positive direction represents the distortion along the chain of O D4 D2, and the negative direction represents the distortion along the chain of O D3. The apparent crystal

12

Fig. 12.7 RMS deviations between the experimental crystal ﬁeld splittings and those calculated by crystal ﬁeld Hamiltonian of O, D4, D3, D2 point symmetries and the apparent crystal ﬁeld model proposed for non-crystal, Hcfa ðD4 Þ and Hcfa ðD3 Þ . a Silicate, b germanate, and c ZBLAN. The ranges of RMS, for all possible choices of level structure, are shown as error bars

Apparent Crystal Field Model of Laser Glass and Its Application 40 35

fitted by CF Hamiltonian fitted by scalar CF strength

(a)

30 25 20 15 40 35 RMS (cm-1)

406

(b)

30 25 20 15 40 35

(c)

30 25 20 15 10

D3

G(D3)

G(D4)

D4 O

D2

ﬁeld Hamiltonians are represented by Hcfa ðD4 Þ and Hcfa ðD3 Þ , locating in the group chains O D4 D2 and O D3, respectively. For the convenience of presentation, the distance between the representations of the different symmetries has arbitrarily been chosen as the difference of the numbers of crystal ﬁeld parameters included in the ﬁtting process, for example, there are two crystal ﬁeld parameters for O point symmetry and ﬁve for D4, so the distance between them is 3 units. For the silicate and germanate glasses, although there is only one more adjustable parameter, C32 , in Hcfa ðD4 Þ than in HcfO , the RMS deviations shown in Fig. 12.7a, b have remarkably smaller values in the Hcfa ðD4 Þ . Moreover, Hcfa ðD4 Þ , HcfD4 , and HcfD2 have similar values of RMS although the numbers of adjustable parameters in the Hamiltonian are 3, 5, and 9, respectively. On the other hand, the values of RMS show that Hcfa ðD4 Þ is much better than Hcfa ðD3 Þ for expressing the apparent crystal ﬁeld Hamiltonian of Er3+ ions in the oxide glasses. As a whole, the RMS deviations have smaller values in the direction O D4 D2 than in O D3, especially when the number of ﬁtting parameters is considered. From Fig. 12.7a, b, it can be concluded that the Er3+ ions in the oxide glasses occupy preferentially the positions with point symmetry of D4, D2d, C4v, D4h and their subgroups, that is, the positions with the 4and twofold rotation axes rather the threefold rotation axis. Figure 12.7a, b also

12.3

Crystal Field Level Analysis for Er3+ Ions in Three Typical Glasses

407

show that the parameters Clk could be obtained through ﬁtting the maximum splittings of multiplets by (12.11). Then all crystal ﬁeld splittings could be calculated by (12.2) from the parameters. The RMS deviations between the calculated and experimental data of crystal ﬁeld splitting are almost the same as those of ﬁtting all the crystal ﬁeld splittings in the conventional way by (12.2). Moreover, the Clk obtained by these two different procedures are listed in Table 12.2 and have very similar values. Consequently, the crystal ﬁeld splittings of Er3+ ions in the oxide glasses calculated by Hcfa ðD4 Þ in which the parameters Clk were obtained from the scalar crystal ﬁeld strength analysis (12.11) are listed and compared with the data obtained from the low temperature spectra in Table 12.3. After the analysis, the positions of the levels appearing mixed in spectral experiments were determined (see the levels signed “(√)” in Table 12.1). For the ZBLAN glass, Fig. 12.7c demonstrates that, different from the oxide glasses, the RMS deviations have similar values in both directions of the group chains O D4 D2 and O D3; especially, the deviations do not decrease remarkably from HcfO to apparent glass Hamiltonian Hcfa ðD4 Þ or Hcfa ðD3 Þ . Therefore, it can be supposed that Er3+ ions in the ZBLAN glass can equally occupy positions with any kind of point symmetries, that is, symmetries distorted not only from D4, D4h and their isomorphic groups but also from D3, D3d and their isomorphic groups. Comparing the experimental data for crystal ﬁeld splittings and the data calculated by Hcfa , the parameters Clk in Hcfa could be obtained through ﬁtting the maximum splittings of multiplet by (12.11) or ﬁtting all of the crystal ﬁeld splittings in conventional way by (12.2) or (12.3). The RMS deviations are different for these two ways (see Fig. 12.7c), and the Clk got by these two different procedures are listed in Table 12.4. In the oxide glasses, the values of Clk got by these two different procedures are very similar (see Table 12.2); however, in the ZBLAN glass, the values are different. The above results show that the symmetry of the apparent crystal ﬁeld for the ZBLAN glass is higher than that for the oxide glasses, so the crystal ﬁeld cannot be expressed by Hcfa ðD4 Þ or Hcfa ðD3 Þ alone. The crystal ﬁeld splittings calculated by Hcfa ðD4 Þ and Hcfa ðD3 Þ with parameters Clk obtained from the scalar crystal ﬁeld strength analysis (12.11) are listed and compared with the experimental data in Table 12.5. In this table, the average values of the crystal ﬁeld splittings calculated by Hcfa ðD4 Þ and Hcfa ðD3 Þ are also given out. Table 12.2 Parameters Clk and Nv of Er3+ ions in silicate and germanate glasses (cm−1) Silicate Fitting DE

Fitting crystal ﬁeld level

Germanate Fitting DE

Fitting crystal ﬁeld level

C32

683.3

672.2

706.2

669.1

C14

2477.7

2535.6

2274.5

2290.5

C16

−95.2

−96.1

−471.5

−506.6

Nv

3123

3182

2948

2949

408

12

Apparent Crystal Field Model of Laser Glass and Its Application

Table 12.3 Comparison of experimental and calculated crystal ﬁeld splittings of Er3+ ions in silicate and germanate glasses (cm−1) Multiplet 4

I15=2

4

I13=2

4

I11=2

4

I9=2

4

F9=2

4

S3=2

2

H11=2

Silicate Exp.

Cal.

Germanate Exp.

−175.7 −152.3 −125.8 −105.9 −36.6 119.2 210.1 266.9 −110.9 −105.9 −68.8 −49.8 −26.8 151.1 211.1 −58.9 −41.0 −35.6 −12.4 74.0 74.0 −134.6 −80.6 24.4 82.5 108.3 −131.1 −101.7 14.3 58.3 160.3 −28.3 28.3 −103.0 −71.0 −22.0 36.0 69.0 91.0

−181.6 −151.7 −129.9 −65.3 −10.2 83.3 222.3 233.1 −133.6 −117.0 −76.5 −26.9 35.1 150.2 168.6 −76.0 −58.9 −25.4 −6.6 73.9 93.1 −106.6 −98.9 47.0 62.1 96.3 −118.5 −82.6 10.4 34.2 156.5 −37.9 37.9 −90.3 −80.4 −41.5 57.5 63.9 90.9

−174.7 −139.3 −111.6 −92.3 −66.7 99.7 202.5 282.5 −109.5 −97.5 −67.9 −34.1 −2.7 155.8 155.8 −53.9 −31.3 −31.3 −31.3 60.2 87.6 −132.0 −86.0 24.0 97.0 97.0 −137.2 −101.2 16.8 61.8 159.8 −33.4 33.4 −105.8 −68.8 −27.8 41.2 66.2 95.2

Cal. −168.6 −149.6 −128.5 −57.2 −45.8 84.1 223.6 241.9 −121.3 −117.5 −66.6 −29.7 24.8 154.0 156.3 −74.2 −54.3 −21.6 −11.8 75.6 86.4 −112.3 −103.6 29.7 88.5 97.7 −107.9 −73.9 −4.2 28.9 157.1 −39.1 39.1 −91.6 −82.0 −18.0 50.1 56.2 85.3 (continued)

12.3

Crystal Field Level Analysis for Er3+ Ions in Three Typical Glasses

409

Table 12.3 (continued) Multiplet 4

F7=2

4

F5=2

4

F3=2

2

G9=2

Silicate Exp. −84.8 −18.8 31.3 72.3 −49.4 −30.6 80.0 −50.5 50.5 −111.8 −35.8 3.2 54.2 90.2

RMS dev.

Cal. −90.6 −32.5 52.3 70.8 −42.9 −1.0 43.8 −55.4 55.4 −94.6 −81.2 36.6 46.5 92.7 21.9

Germanate Exp. −89.7 −16.4 34.6 71.6 −51.4 −30.8 82.2 −49 49 −114.4 −32.4 7.6 51.6 87.6

Cal. −99.9 −21.7 40.7 80.8 −42.0 0.6 41.4 −57.2 57.2 −99.4 −84.1 23.0 66.1 94.6 19.3

Table 12.4 Parameters Clk and Nv of Er3+ ions in ZBLAN glass (cm−1) Fitting DE

Fitting crystal ﬁeld level by Hcfglass ðD4 Þ

Fitting crystal ﬁeld level by Hcfglass ðD3 Þ

Cl2

503.8

509.6

583.5

C14 C16

1597.6

1376.6

1295.8

−367.0

−482.9

−497.9

Nv

2081

1877

1855

The RMS deviations of 21.3 cm−1 for Hcfa ðD4 Þ and 21.6 cm−1 for Hcfa ðD3 Þ decreasing to 18.9 cm−1 for the average result shows that, in the analysis of apparent crystal ﬁeld in ZBLAN glass, the combination of Hcfa ðD4 Þ and Hcfa ðD3 Þ may be a suitable way. The values of the scalar crystal ﬁeld strength parameter Nv calculated by (12.5) are listed in Tables 12.2 and 12.4. For Er3+ ions in the oxide glasses, silicate and germanate, the values are around 3000 cm−1; while in the ZBLAN glass, the values are only around 2000 cm−1. It shows that the ﬁrst neighbor anions take a crucial part in the crystal ﬁeld strength and the crystal ﬁeld for the oxide is generally much stronger than that for the fluoride. In the conventional way, a “pure” and low-point symmetry was tried to describe the average environment of rare earth ions in glasses. On the basis of the fact that the disordered structure of glass leads to site-to-site variations at the rare earth ion sites, an apparent crystal ﬁeld Hamiltonian for the rare earth ions has been introduced by means of the group chain scheme. Although this is a simple model and only three parameters Clk of the Hamiltonian are considered, it has been used to

410

12

Table 12.5 Comparison of experimental and calculated crystal ﬁeld splittings of Er3+ ions in ZBLAN glass (cm−1)

Apparent Crystal Field Model of Laser Glass and Its Application Multiplet 4

I15=2

4

I13=2

4

I11=2

4

I9=2

4

I9=2

4

S3=2

2

H11=2

Exp. −168.3 −121.6 −57.2 −14.3 25.2 57.3 139.5 139.5 −103.0 −76.0 −42.4 −14.4 31.9 69.3 134.6 −51.1 −11.8 6.2 10.2 14.2 32.2 −118.4 −59.4 6.6 85.6 85.6 −85.0 −55.0 5.0 42.0 93.0 −47.8 47.8 −87.2 −44.2 −12.2 19.8 61.8 61.8

Cal. Hcfglass ðD4 Þ

Hcfglass ðD3 Þ

Average

−119.1 −109.6 −89.5 −40.9 −34.0 60.4 158.6 174.1 −85.1 −83.7 −46.5 −21.7 17.0 110.0 110.0 −52.6 −38.1 −15.0 −8.9 54.0 60.8 −80.3 −74.1 16.1 65.7 72.6 −75.7 −51.8 −4.2 20.1 111.7 −27.9 27.9 −65.2 −58.5 −10.8 35.0 39.3 60.1

−150.1 −113.1 −54.1 −49.6 −34.6 116.0 138.6 146.9 −120.0 −64.4 −35.4 −29.3 80.7 82.2 86.2 −72.4 −30.4 −15.8 36.4 38.2 44.1 −82.2 −72.8 17.8 67.9 69.3 −90.9 −57.0 15.4 46.5 86.0 −27.9 27.9 −63.1 −60.3 −11.3 34.9 39.1 60.7

−134.6 −111.4 −71.8 −45.3 −34.3 88.2 148.6 160.5 −102.6 −74.1 −40.9 −25.5 48.8 96.1 98.1 −62.5 −34.3 −15.4 13.7 46.1 52.4 −81.3 −73.4 17.0 66.8 70.9 −83.3 −54.4 5.6 33.3 98.9 −27.9 27.9 −64.1 −59.4 −11.0 35.0 39.2 60.4 (continued)

12.3

Crystal Field Level Analysis for Er3+ Ions in Three Typical Glasses

Table 12.5 (continued)

Multiplet 4

F7=2

4

F5=2

4

F3=2

2

G9=2

RMS dev.

Exp. −62.3 −17.3 15.4 64.2 −19.3 0.3 19.1 −46.5 46.5 −82.2 −45.2 3.8 51.7 71.9

411

Cal. Hcfglass ðD4 Þ

Hcfglass ðD3 Þ

−71.8 −14.6 28.0 58.4 −29.8 0.5 29.2 −40.8 40.8 −71.1 −60.1 12.5 49.5 69.2 21.3

−58.7 −16.7 −1.0 76.4 −17.1 −17.0 34.1 −40.8 40.8 −74.5 −58.9 17.4 55.7 60.3 21.6

Average −65.3 −15.6 13.5 67.4 −23.4 −8.2 31.6 −40.8 40.8 −72.8 −59.5 14.9 52.6 64.7 18.9

explain the spectral properties of rare earth ions in non-crystal materials in a rather realistic way. The ﬁtting results have shown that the Hamiltonian Hcfa ðD4 Þ is more suitable than a Hcf ðD3 Þ for describing the apparent crystal ﬁeld of Er3+ ions in the silicate and germanate oxide glasses. This means that the Er3+ ions in the oxide glasses could not equally occupy positions with any kind of point symmetries. This conclusion is in agreement with those mentioned in Sect. 12.1, that is, rare earth ions can only play a role as network modiﬁer in oxide glasses but cannot joint the network of host, and the Er3+ ions in oxide glasses can only have coordination number 6 [11]. Because of the strong ionic nature of the fluoride glasses, the rare earth fluorides play a role as an intermediate element in the glasses. They are able to be both in and out of network positions. On the other hand, all rare earth ions in the fluoride glasses are capable of having 7–9-coordinated sites owing to the smaller radius of F− ion [11]. As a result, the rare earth ions in fluoride glasses possess more than one distinct type of sites. This implies that rare earth ions in fluoride glasses may be more evenly distributed. As an apparent result, the Hamiltonian for fluoride glass may have “higher” point symmetry than for oxide glass. By means of the group chain scheme, the apparent crystal ﬁeld Hamiltonian has the characteristic of high-point symmetry close to the O point group. The cubic crystal ﬁeld terms (C14 and C16 ) give the major contribution to the crystal ﬁeld strength when the term from the low symmetry (C32 or C52 ) allows the complete removal of degeneracy. Such a consideration explains why transitions between crystal ﬁeld levels of rare earth ions are allowed in glasses as in crystal with

412

12

Apparent Crystal Field Model of Laser Glass and Its Application

low-point symmetry, but at the same time the structure of levels displays the feature of high-point symmetry [34]. In conclusion, on the basis of the apparent crystal ﬁeld model the crystal ﬁeld splittings of Er3+-doped glasses, which have important applications in the area of photoelectronics, can be analyzed quite completely and systematically. Obviously, this is a simple method for analyzing energy level splitting of rare earth ions in disordered hosts. The values of the splittings are essential for predicting properties of spectra and laser of rare earth-doped glasses [35–38].

References 1. F. Gan, Optical and Spectral Properties of Glass (in Chinese) (Shanghai Scientiﬁc & Technical Publishers, Shanghai, 1992) 2. F. Gan, Photonic Glasses and Their Applications (in Chinese) (Shanghai Scientiﬁc & Technical Publishers, Shanghai, 2011) 3. M.J. Weber, Laser excited fluorescence spectroscopy in glass, in Laser Spectroscopy of Solids, ed. by W.M. Yen, P.M. Selzer (Springer, New York, 1981), pp. P189–P239 4. H. Scholze, Glass: Nature, Structure, and Properties (Springer, New York, 1991) 5. C. Brecher, L.A. Riseberg, Phys. Rev. B 13, 81 (1976) 6. G. Lei, J.E. Anderson, M.I. Buchwald et al., Phys. Rev. B 57, 7673 (1998) 7. W.H. Zachariasen, J. Am. Chem. Soc. 54, 3841 (1932) 8. C.N. Greaves, J. Non-Cryst. Solids 71, 203 (1985) 9. C. Huang, A.N. Cormack, J. Chem. Phys. 93, 8180 (1990) 10. C. Huang, A.N. Cormack, J. Chem. Phys. 95, 3634 (1990) 11. J. Wang, W.S. Brecklesby, J.R. Lincoln et al., J. Non-Cryst. Solids 163, 261 (1993) 12. T.F. Belliveau, D.J. Simkin, J. Non-Cryst. Solids 110, 127 (1989) 13. M.J. Lochhead, K.L. Bray, Phys. Rev. B 52, 15763 (1995) 14. G. Pucker, K. Gatterer, H.P. Fritzer et al., Phys. Rev. B 53, 6225 (1996) 15. C. Brecher, L.A. Riseberg, Phys. Rev. B 21, 2607 (1980) 16. C.C. Robinson, J.T. Fournier, J. Phys. Chem. Solids 31, 895 (1970) 17. J.T. Fournier, R.H. Bartram, J. Phys. Chem. Solids 31, 2615 (1970) 18. P.H. Butler, Point Group Symmetry Application: Method and Tables (Plenum, New York, 1981) 19. C.A. Morrison, R.P. Leavitt, Spectroscopic properties of triply ionized lanthanides in transparent host crystals, in Handbook on the Physics and Chemistry of Rare Earths, ed. by K. A. Gschneidner, Jr., L. Eyring (North-Holland Publishing Company, Amsterdam, 1982), pp. 461–692 20. A.A. Kaminskii, Laser Crystals-Their Physics and Properties (Springer, London, 1990) 21. Y.D. Huang, M. Mortier, F. Auzel, Opt. Mater. 15, 243 (2001) 22. Y.D. Huang, M. Mortier, F. Auzel, Opt. Mater. 17, 501 (2001) 23. F. Auzel, Mater. Res. Bull. 14, 223 (1979) 24. F. Auzel, O.L. Malta, J. Phys. (Paris) 44, 201 (1983) 25. F. Auzel, J. Chavignon, D. Meichenin et al., J. Non-Cryst. Solids 161, 109 (1993) 26. R.P. Leavitt, J. Chem. Phys. 77, 1661 (1982) 27. F. Auzel, Materials for ionic solid state lasers, in Spectroscopy of Solid-State Laser-Type Materials, ed. by B. Di Bartolo (Plenum Press, London, 1987), pp. P293–P341 28. Y. Huang, Z. Luo, Y. Chen et al., J. Chin. Rare Earth Soc. (in Chinese) 19, 614 (2001) 29. F. Auzel, Opt. Mater. 19, 89 (2002) 30. F. Auzel, Mol. Phys. 102, 1113 (2004)

References

413

31. Z. D. Luo, Y. D. Huang, J. Phys.: Condens. Matter 6, 3737 (1994) 32. M.J. Weber, Phys. Rev. 157, 262 (1967) 33. C.W. Neilson, G.F. Koster, Spectroscopic Coefﬁcients for pn, dn and fn Conﬁgurations (MIT, Massachusetts, 1974) 34. L. Bigot, A.M. Jurdyc, B. Jacquier et al., Phys. Rev. B 66, 214204 (2002) 35. M. Gorjan, M. Marincek, M. Copic, J. Opt. Soc. Am. B 27, 2784 (2010) 36. A. Malouf, O. Henderson-Sapir, M. Gorjan et al., IEEE J. Quantum Electron. 52, 1600412 (2016) 37. F. Maes, V. Fortin, M. Bernier et al., IEEE J. Quantum Electron. 53, 1600208 (2017) 38. J. Li, H. Luo, Y. Liu et al., IEEE J. Sel. Topics Quantum Electron. 20, 0900414 (2014)

Appendix A Character Tables for Point-Symmetry Group

In this appendix the tables of irreducible representation character are given by using three different representation labels adopted by Milliken, Bethe, and Butler for the convenient of comparison. The spatial basis functions are only given for the usage in this book.

Note The ﬁrst and the second column on the left are the Milliken symbols correspond to the point groups of the ﬁrst and the second row respectively, the following tables where the Milliken symbols of two groups being different are also so arranged

© Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8

415

416

Appendix A: Character Tables for Point-Symmetry Group

Note x = e−ip/3, x3 = −1, here C2 and C3 are deﬁned as those of Butler, which are different from Koster et al deﬁned in “Properties of the thirty-two point groups”, there are similar differences in the following tables

Appendix A: Character Tables for Point-Symmetry Group

417

418

Appendix A: Character Tables for Point-Symmetry Group

Note The Milliken symbols of point groups C6v and D6 are as shown above; the Milliken symbol of point group D3h are: C1 ! A01 , C2 ! A02 , C3 ! A001 , C4 ! A002 , C5 ! E″, C6 ! E′

Appendix A: Character Tables for Point-Symmetry Group

419

Appendix B Correlation Table of Group–Subgroup

In the following tables, the orbital angular momentum quantum number will be used to label the irreducible representation of SO3 group, but the subscripts of Bethe symbols are used to label those of point groups. When more than one irreducible representation of subgroup corresponds to one irreducible representation, right subscripts are used to distinguish. Sign of + and − in front of the symbols of irreducible representation of subgroup means that corresponding 2jm factor equal to +1 and −1, respectively. For the point group having central symmetry the symbol with superscript + represents even irreducible representation and the symbol with superscript − represents odd irreducible representation.

© Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8

421

422

Appendix B: Correlation Table of Group–Subgroup

Appendix B: Correlation Table of Group–Subgroup

423

Appendix C Multiplication Tables for Some Point Groups

In the following tables, the subscripts of Bethe’s symbol are used to represent irreducible representation, and the direct summations of irreducible representation are denoted by the symbol ⊕. Point group C2 and Cs

Point group C3

Point group C4

Point group D2

S4

C2v

1 1

1 1

2 2 1

3 3 4 2

4 4 3 1 2

1 1

2 2 3

3 3 1 2

4 4 6 5 2

5 5 4 6 1 3

6 6 5 4 3 2 1

2 2 1

3 3 4 2

4 4 3 1 2

5 5 7 8 6 3

6 6 8 5 7 1 4

7 7 5 6 8 4 2 3

1 1

2 2 1

3 3 4 1

4 4 3 2 1

Subscript i of

i

1 2 3 4

5 5 5 5 5

1 2 3 4

Subscript i of

i

1 2 3 4 5 6

8 8 6 7 5 2 3 1 4

Subscript i of

i

1 2 3 4 5 6 7 8

Subscript i of

i

1 2 3 4 5

© Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8

425

426

Point group D3

Point group D4

Appendix C: Multiplication Tables for Some Point Groups

C3v

C4v D2d

Point group T

Point group O

1 1

1 1

Td

1 1

2 2 1

2 2 3

3 3 3 1 2 3

1 1

2 2 1

2 2 1

3 3 4 1

3 3 1 2

3 3 3 1 2 3 4 1

4 4 3 2 1

4 4 4 5 6 2 3

5 5 5 5 5

1 2 3 4

4 4 4 4 1 2 3 3 4 5

4 4 5

5 5 6 4 3 2

6 6 5 4 3 1 2

i

1 2 3 4 5 6

6 6 6 7 7

7 7 7 6 6

Subscript i of

6 6 7 5 5 6 7 2 4 3 4

7 7 5 6 5 6 7 3 4 1 4 2 4

7 7 6

8 8 8

6 6 7

4 5

4 5

8

1 3 4 5

2 3 4 5 1 3 4 5

6 8 7 8 1 4

8 7 6 2 1

8 8 5 4

i

1 2 3 4 5 6 7

6 7 6 7 1 2 5 3 4 5 1 2 5

5 5 6 7 6 7 1 4

5 5 4

Subscript i of

Subscript i of

i

1 2 3 4 5 6 7

Subscript i of

1 2

6 7 8

3

6 7 8 8 6 7 8 8 3 4 5 3 4 5 1 2 3 4 4 5 5

4 5 6 7 8

i

Appendix D Squared Reduced-Matrix Elements of Unit Operator for J ! J′ Transition in Rare Earth Ions

Squared reduced-matrix elements of unit operator for J ! J′ transitions in rare earth 2 ions expressed as 4f n ½aSLJ U ðkÞ 4f n ½a0 S0 L0 J 0 commonly used in laser materials are given in this appendix, which the intermediate coupling has been taken into 2 account and the following relation is assumed 4f n ½aSLJ U ðkÞ 4f n ½a0 S0 L0 J 0 ¼ jh4f n ½a0 S0 L0 J 0 U ðkÞ 4f n ½aSLJij2 . These data are cited from the book published by A.A. Kaminskii: “Laser Crystals, their Physics and Properties. Heidelberg: Springer-Verlag, 1981” and “Crystalline Lasers: Physical Processes and Operating Schemes. Boca Raton: CRC Press, 1996”. Pr3+: 2S+1 3

H5

3

H6 F2

3

3

F3

3

F4

LJ

2S′+1 3

H4 3 H5 3 H4 3 H6 3 H5 3 H4 3 F2 3 H6 3 H5 3 H4 3 F3 3 F2 3 H6 3 H5 3 H4

L′J′

EJJ′ (cm−1) 2050 2200 4250 700 2900 4950 1380 2100 4300 6350 450 1850 2550 4750 6800

k=2

k=4

k=6

0.1096 0.1080 0.0002 0 0 0.5079 0.0212 0 0.6285 0.0658 0.0262 0.0015 0.6330 0.0368 0.0162

0.2035 0.2328 0.0322 0.0167 0.2978 0.4048 0.0508 0.3182 0.3468 0.3487 0.0735 0.0027 0.6805 0.3371 0.0528

0.6106 0.6421 0.1407 0.3040 0.6597 0.1196 0 0.9460 0 0.7002 0.013 0.0948 0.5165 0.5278 0.4901

(continued) © Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8

427

Appendix D: Squared Reduced-Matrix Elements …

428 (continued) 2S+1 1

G4

1

D2

3

P0

3

P1

1

I6 P2

3

1

S0

LJ

2S′+1 3

F4 3 F3 3 F2 3 H6 3 H5 3 H4 1 G4 3 F4 3 F3 3 F2 3 H6 3 H5 3 H4 1 D2 1 G4 3 F4 3 F3 3 F2 3 H6 3 H5 3 H4 3 P0 1 D2 1 G4 3 F4 3 F3 3 F2 3 H6 3 H5 3 H4 3 H4 1 I6 3 P1 3 P0 1 D2 1 G4 3 F4 3 F3 3 F2 3 H6 3 H5 3 H4 3 H4

L′J′

EJJ′ (cm−1)

k=2

k=4

k=6

3050 3500 4900 5600 7800 9850 6950 10,000 14,950 16,300 17,000 21,250 16,800 3900 10,800 13,850 14,350 15,700 16,400 18,600 20,650 600 4500 11,400 14,450 14,950 16,300 17,000 19,200 21,250 21,250 1250 1250 1850 5700 12,650 15,700 16,150 17,550 18,250 20,450 22,500 46,750

0.0683 0.0026 0.0002 0.1927 0.0307 0.0019 0.3865 0.5144 0 0 0.0036 0.0081 0.0200 0.0134 0 0 0 0.2943 0 0 0 0 0.0749 0 0 0.5714 0.2698 0 0 0 0.0081 0 0.4232 0.1929 0.0011 0.5640 0.5233 0.2584 0.0323 0 0 6 10−5 0

0.1203 0.0031 0.0138 0.1905 0.0715 0.0044 0.0493 0.0004 0.0009 0.0050 0.0132 0.0447 0.0165 0 0.0425 0.1213 0 0 0 0 0.1713 0 0 0.0605 0.2852 0.1964 0 0 0.2857 0.1721 0.0447 0.0257 0 0 0.0718 0.0341 0.1170 0.3082 0.3001 0.5010 0.1888 0.0362 0.0064

0.2844 0.0452 0.0032 0.1865 0.3344 0.0119 0.0844 0.0147 0.0025 0.0301 0.0046 0.0203 0.0493 0 0 0 0 0 0.0726 0 0 0 0 0 0 0 0 0.1246 0.0893 0 0.0203 0.1405 0 0 0 0.0184 0.0072 0 0 0.0544 0.1316 0.1373 0

Appendix D: Squared Reduced-Matrix Elements …

429

Nd3+: 2S+1

LJ

4

I11/2 4 I13/2 4

I15/2

4

F3/2

4

F5/2

2

H(2)9/2

4

F7/2

4

S3/2

2S′+1 4

L′J′

I9/2 4 I11/2 4 I9/2 4 I13/2 4 I11/2 4 I9/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2

EJJ′ (cm−1)

k=2

k=4

k=6

1850 2000 3850 2100 4100 5950 5400 7500 9500 11,350 1000 6400 8500 10,500 12,350 100 1100 6500 8600 10,600 12,450 1050 1150 2150 7550 9650 11,650 13,500 – 1050 1150 2150 7550 9650 11,650 13,500

0.0195 0.0256 0.0001 0.0196 0 0 0 0 0 0 0.0795 0 0 0 0.0010 0.0065 0 0 0.0387 0.0028 0.0092 0.0059 0.0674 0.0066 0 0 0.0006 0.0010 0 0 0 0.0004 0 0 0 0

0.1073 0.1353 0.0136 0.1189 0.0109 0.0001 0 0 0.1136 0.2293 0.0523 0 0.1805 0.1681 0.2371 0.0315 0.0144 0.2120 0.0061 0.0004 0.0080 0.0342 0.0547 0.0792 0.1545 0.3282 0.2373 0.0423 0.0004 0.0044 0.0006 0 0 0 0 0.0027

1.1653 1.2379 0.4558 1.4511 0.4184 0.0453 0.0288 0.2085 0.4104 0.0548 0 0.2309 0.4025 0.0364 0.3972 0.0050 0.0217 0.0765 0.1155 0.0246 0.1155 0.0036 0.0902 0 0.6209 0.0001 0.3094 0.4246 0 0.0002 0 0 0.3302 0.3307 0.2033 0.2352 (continued)

Appendix D: Squared Reduced-Matrix Elements …

430 (continued) 2S+1

LJ

4

F9/2

2

H(2)11/2

4

G5/2

2

G(1)7/2

2S′+1 4

L′J′

S3/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2 4 F9/2 4 S3/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2 2 H(2)11/2 4 F9/2 4 S3/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2 4 G5/2 2 H(2)11/2 4 F9/2 4 S3/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2

EJJ′ (cm−1)

k=2

k=4

k=6

1150 1150 2200 2300 3300 8700 10,800 12,800 14,650 1150 2300 2300 3350 3450 4450 9850 11,950 13,950 15,800 1400 2550 3700 3700 4750 4850 5850 11,250 13,350 15,350 17,200 – 1400 2550 3700 3700 4750 4850 5850 11,250 13,350 13,530 17,200

0 0.1473 0.0486 0.0109 0 0 0.0035 0.0001 0.0009 0.0892 0 0.0950 0.0676 0 0 0.1311 0.0045 0.0043 0.0001 0 0.0025 0.0009 0.0339 0.0010 0.2681 0.4830 0 0 0 0.8979 0.0002 0.0066 0.0264 0.0008 0.0389 0.0076 0.2683 0.0817 0 0 0.4416 0.0757

0.0026 0.0076 0.0026 0.0504 0.0048 0.0050 0.2188 0.0345 0.0092 0.0248 0.0568 0.0929 0.0039 0.0029 0.0002 0.0695 0.0172 0.0093 0.0027 0.0003 0.0064 0.1771 0.0612 0.0138 0.1292 0.0444 0 0.0349 0.2892 0.4093 0.1493 0 0.0520 0.0834 0.1018 0.0302 0.0069 0.0449 0.0017 0.1025 0.1844 0.1848

00013 0.1040 0.0056 0.1082 0.1137 0.4668 0.5165 0.3678 0.0417 0.0910 0.0017 0.0760 0.2229 0.0236 0.0081 0 0.0028 0.0063 0.0104 0.0146 0.1338 0 01267 0.0017 0 0 0.0968 0.0472 0.0104 0.0359 0.0874 0.3467 0.2705 0 0.1636 0.1822 0.0825 0 0.1048 0.0383 0.0484 0.0314 (continued)

Appendix D: Squared Reduced-Matrix Elements …

431

(continued) 2S+1

LJ

2

K13/2

4

G7/2

4

G9/2

2S′+1 2

L′J′

G(1)7/2 4 G5/2 2 H(2)11/2 4 F9/2 4 S3/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2 2 K13/2 2 G(1)7/2 4 G5/2 2 H(2)11/2 4 F9/2 4 S3/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2 4 G7/2 2 K13/2 2 G(1)7/2 4 G5/2 2 H(2)11/2 4 F9/2 4 S3/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2

EJJ′ (cm−1)

k=2

k=4

k=6

1550 1550 2950 4100 5250 5250 6300 6400 7400 12,800 14,900 16,900 18,750 250 1800 1800 3200 4350 5500 5500 6550 6650 7650 13,050 15,150 17,150 19,000 450 700 2250 2250 3650 4800 5950 5950 7000 7100 8100 13,500 15,600 17,600 19,450

0 0 0.0014 0.0437 0 0.1407 0.1201 0 0 0 0.0034 0.0002 0.0069 0 0.0575 0 0.0016 0.0006 0.0021 0.1641 0.0518 0.2359 0.0983 0 0 0.5314 0.0550 0.0401 0.0195 0.0195 0 0.0025 0.1298 0 0.5747 0.0381 0.1987 0 0 0.9950 0.1447 0.0046

0.6615 0.0019 0.0043 0.0042 0 0.0653 0.0061 0.0028 0 0.0010 0.0002 0 0.0002 0.5688 0.0005 0.2246 0.0208 0.0089 0.1929 0.0671 0.0503 0.0015 0.0584 0.0270 0.2296 0.0959 0.1571 0.1400 0.0402 0.2246 0.10676 0.0327 0.1604 0.2010 0 0.0485 0.1060 0.0610 0.1580 0.3890 0.3577 0.0609

0.0013 0.0081 0.4823 0.2821 0.0007 0.0091 1.1455 0.0049 0.0073 0.0068 0.0025 0.0171 0.0312 0.0014 0.0377 0.0053 0.1166 0.0074 0 0.0031 0.3898 0.1124 0 0.0027 0.0576 0.0120 0.0553 0.1343 0.1080 0.0053 0.2531 0.2089 0.0272 0.0009 0.0894 0.0909 0.0016 0.1492 0.2346 0.0123 0.0552 0.0406 (continued)

Appendix D: Squared Reduced-Matrix Elements …

432 (continued) 2S+1

LJ

2

K15/2

2

G(1)9/2

2S′+1 4

L′J′

G9/2 4 G7/2 2 K13/2 2 G(1)7/2 4 G5/2 2 H(2)11/2 4 F9/2 4 S3/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2 2 K15/2 4 G9/2 4 G7/2 2 K13/2 2 G(1)7/2 4 G5/2 2 H(2)11/2 4 F9/2 4 S3/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2

EJJ′ (cm−1)

k=2

k=4

k=6

1450 1900 2150 3700 3700 5100 6250 7400 7400 8450 8550 9550 14,950 17,050 19,050 20,900 150 1600 2050 2300 3850 3850 5250 6400 7550 7550 8600 8700 9700 15,100 17,200 19,200 21,050

0 0 0.0068 0 0 0.1511 0 0 0 0 0 0 0.0112 0.0004 0.0020 0 0 0.0018 0.0147 0.0147 0.0050 0.0001 0.0562 0.1026 0 0.1218 0.0015 0.0416 0 0 0.2854 0.0238 0.0010

0.1135 0.0200 0.4290 0.0354 0 0.0014 0.0003 0 0 0.4724 0 0 0.0002 0.0003 0.0003 0.0052 0.9742 0.0351 0.0578 0.0888 0.0631 0.0282 0.0344 0.0088 0.0800 0.0127 0.0009 0.0353 0.0190 0.1424 0.0275 0.0434 0.0148

0.0228 0.0025 0.0221 0.0128 0.0053 1.5109 0.2020 0.0028 0.0084 0.4238 0.0050 0.0097 0.0243 0.0186 0.0034 0.0143 0.0182 0.1866 0.0231 0.0543 0.0298 0.0308 0.5917 0.3021 0 0.0453 0.1452 0.0057 0.0265 0.0044 0.0727 0.0452 0.0139 (continued)

Appendix D: Squared Reduced-Matrix Elements …

433

(continued) 2S+1

LJ

2

D(1)3/2

4

G11/2

2S′+1 2

L′J′

G(1)9/2 2 K15/2 4 G9/2 4 G7/2 2 K13/2 2 G(1)7/2 4 G5/2 2 H(2)11/2 4 F9/2 4 S3/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2 2 D(1)3/2 2 G(1)9/2 2 K15/2 4 G9/2 4 G7/2 2 K13/2 2 G(1)7/2 4 G5/2 2 H(2)11/2 4 F9/2 4 S3/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2

EJJ′ (cm−1)

k=2

k=4

k=6

100 250 1700 2150 2400 3950 3950 5350 6500 7650 7550 8750 8800 9800 15,200 17,300 19,300 21,150 300 400 550 2000 2450 2700 4250 4250 5650 6800 7950 7950 9000 9100 10,100 15,500 17,600 19,600 21,450

0 0 0 0.0216 0 0.0087 0.0003 0 0 0.0068 0.0018 0 0.0041 0.0046 0 0 0.0238 0 0 0.0997 0.0094 0.0444 0.0028 0.0002 0.0107 0 0.0010 0.9477 0 0.1736 0.1747 0 0 1.5282 0.1282 00044 0

0.0089 0 0.0029 0.0477 0 0.0839 0.0038 0.1148 0.0003 0 0.0003 0.0255 0. 0. 0 0.0016 0.0434 0.0189 0.0312 0.0104 0.0168 0.5128 0.0283 0.0084 0.1266 0.0091 0.0843 0.2103 0.3242 0.1640 0 0.0618 0.0015 0.8891 0.3502 0.0645 0.0053

0.0311 0.3531 0.0262 0 0.0788 0 0 0.1804 0.0156 0 0 0.0960 0 0 0.0081 0.0325 0.0452 0.0002 0.0003 0.3721 0.0919 0.1365 0.3827 0.0232 0.0040 0.0930 0.0111 0.0398 0.0005 0.1418 0.0033 0.1959 0.0995 0.1600 0.1608 0.0563 0.0080 (continued)

Appendix D: Squared Reduced-Matrix Elements …

434 (continued) 2S+1

LJ

2

P1/2

2

D(1)5/2

2S′+1 4

L′J′

G11/2 2 D(1)3/2 2 G(1)9/2 2 K15/2 4 G9/2 4 G7/2 2 K13/2 2 G(1)7/2 4 G5/2 2 H(2)11/2 4 F9/2 4 S3/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2 2 P1/2 4 G11/2 2 D(1)3/2 2 G(1)9/2 2 K15/2 4 G9/2 4 G7/2 2 K13/2 2 G(1)7/2 4 G5/2 2 H(2)11/2 4 F9/2 4 S3/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2

EJJ′ (cm−1)

k=2

k=4

k=6

1500 1850 1950 2100 3550 4000 4250 5800 5800 7200 8350 9500 9500 10,550 10,650 11,650 17,050 19,150 21,150 23,000 750 2300 2600 2700 2850 4300 4750 5000 6550 6550 7950 9100 10,250 10,250 11,300 11,400 12,400 17,800 19,900 21,900 23,750

0 0.0349 0 0 0 0 0 0 0.0327 0 0 0.0167 0 0 0.0093 0.0128 0 0 0 0 0.0300 0 0.2011 0.0383 0 0.0002 0.0004 0 0.0089 0.0016 0 0.0006 0.0096 0.0003 0.0125 0.0011 0.0015 0 0 0 0

0 0 0.0002 0 0.0010 0.0029 0 0.0096 0 0 0.0034 0 0.0183 0.0874 0 0 0 0 0 0.0367 0 0.0345 0.0030 0.1987 0 0.0055 0.0552 0.0040 0.0681 0.0007 0.2650 0.0094 0 0.0188 0.2248 0.0005 0.0015 0 0.0052 0 0.0002

0.0001 0 0 0 0 0 0.1761 0 0 0.1628 0 0 0.1418 0 0 0 0 0 0.0003 0 0 0.0008 0 0.0186 0.4977 0.0052 0.0671 0.1766 0.1674 0 0.0152 0.0114 0 0.0061 0.0736 0 0 0.0003 0.0170 0.0025 0.0021 (continued)

Appendix D: Squared Reduced-Matrix Elements …

435

(continued) 2S+1

LJ

2

P3/2

4

D3/2

2S′+1 2

L′J′

D(1)5/2 2 P1/2 4 G11/2 2 D(1)3/2 2 G(1)9/2 2 K15/2 4 G9/2 4 G7/2 2 K13/2 2 G(1)7/2 4 G5/2 2 H(2)11/2 4 F9/2 4 S3/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2 4 I15/2 4 I13/2 4 I11/2 4 I9/2 2 P3/2 2 D(1)5/2 2 P1/2 4 G11/2 2 D(1)3/2 2 G(1)9/2 2 K15/2 4 G9/2 4 G7/2 2 K13/2 2 G(1)7/2 4 G5/2 2 H(2)11/2 4 F9/2 4 S3/2 4 F7/2 2 H(2)9/2 4 F5/2 4 F3/2

EJJ′ (cm−1)

k=2

k=4

k=6

2350 3100 4650 4950 5050 5200 6650 7100 7350 7850 7850 10,300 11,450 12,600 12,600 13,650 13,750 14,750 20,150 22,250 24,250 26,100 2100 4450 5200 6750 7050 7150 7300 8750 9200 9450 11,000 11,000 12,400 13,550 14,700 14,700 15,750 15,850 16,850

0.0050 0.0026 0 0.0058 0 0 0 0.0045 0 0.0001 0.0066 0 0 0.0073 0.0009 0 0.0023 0.0031 0 0 0 0 0.0118 0.0268 0.1086 0 0 0 0 0 0.1363 0 0.2824 0.1786 0 0 0.2297 0.2326 0 0.0595 0.1430

0.0001 0 0.0031 0 0.0910 0 0.0602 0.0086 0 0 0 0.0031 0.0596 0 0.0003 0.0130 0.0044 0 0 0 0.0172 0.0014 0. 0.0072 0 0.0039 0 0 0 0.0002 0.0125 0 0.0173 0.0007 0.0427 0.2023 0 0.0657 0.0209 0.2095 0

0 0 0.0001 0 0.1466 0.0043 0.0590 0 0.2481 0 0 0.0125 0.0539 0 0 0.0732 0 0 0.0029 0.0090 0.0008 0.0008 0 0 0 0.2047 0 0.0346 0.0014 0.0904 0 0.0024 0 0 0.0135 0.0007 0 0 0.0033 0 0 (continued)

Appendix D: Squared Reduced-Matrix Elements …

436 (continued) 2S+1

EJJ′ (cm−1)

k=2

k=4

k=6

4

22,250

0

0

0.0091

4

24,350 26,350 28,200 28,350 28,500 28,750 29,150 29,850 30,400 30,600 32,450 33,350 33,800 34,350 38,350 39,800 47,550

0 0 0 0.0001 0.0049 0 0 0.0001 0 0 0.0001 0 0.0001 0.0007 0.0021 0 0

0 0.2942 0.1959 0.0567 0.0146 0.2584 0.0248 0.0013 0.0036 0.0010 0.0085 0.0112 0.0001 0.0006 0.0033 0.0004 0.0015

0.0245 0.0084 0.0169 0.0275 0.0034 0 0.0097 0.0017 0.0080 0.0013 0 0.0011 0.0002 0.0034 0 0.0007 0.0001

2S′+1

LJ

L′J′

I15/2

I13/2 I11/2 4 I9/2 4 I9/2 4 I9/2 4 I9/2 4 I9/2 4 I9/2 4 I9/2 4 I9/2 4 I9/2 4 I9/2 4 I9/2 4 I9/2 4 I9/2 4 I9/2 4 I9/2 4

4

D5/2 I11/2 4 D1/2 2 L15/2 2 I13/2 4 D7/2 2 L17/2 2 H(1)9/2 2 D(2)3/2 2 H(1)11/2 2 D(2)5/2 2 F(2)5/2 2 F(2)7/2 2 G(2)9/2 2

Sm3+ 2S+1

LJ

6

H7/2 6 H9/2 6

H11/2

6

H13/2

6

F1/2

2S′+1 6

L′J′

H5/2 6 H7/2 6 H5/2 6 H9/2 6 H7/2 6 H5/2 6 H11/2 6 H9/2 6 H7/2 6 H5/2 6 H13/2 6 H11/2 6 H9/2 6 H7/2 6 H5/2

EJJ′ (cm−1) 1100 1200 2300 1300 2500 3600 1500 2800 4000 5100 1100 2600 3900 5100 6200

k=2

k=4

k=6

0.2085 0.2983 0.0221 0.3451 0.0336 0 0.3412 0.0280 0 0 0 0 0 0 0.1947

0.1986 0.1652 0.1340 0.2226 0.1760 0.0262 0.3450 0.1696 0.0276 0.0011 0 0 0.1485 0.1395 0

0.0822 0.0104 0.3117 5 10−5 0.2588 0.2678 0.1129 0.3968 0.2768 0.0605 0.1026 0.3343 0 0 0 (continued)

Appendix D: Squared Reduced-Matrix Elements …

437

(continued) 2S+1

LJ

6

F3/2

6

H15/2

6

F5/2

6

F7/2

6

F9/2

2S′+1 6

L′J′

F1/2 6 H13/2 6 H11/2 6 H9/2 6 H7/2 6 H5/2 6 F3/2 6 F1/2 6 H13/2 6 H11/2 6 H9/2 6 H7/2 6 H5/2 6 H15/2 6 F3/2 6 F1/2 6 H13/2 6 H11/2 6 H9/2 6 H7/2 6 H5/2 6 F5/2 6 H15/2 6 F3/2 6 F1/2 6 H13/2 6 H11/2 6 H9/2 6 H7/2 6 H5/2 6 F7/2 6 F5/2 6 H15/2 6 F3/2 6 F1/2 6 H13/2 6 H11/2 6 H9/2 6 H7/2 6 H5/2

EJJ′ (cm−1) 300 1400 2900 4200 5400 6500 300 600 1700 3200 4500 5700 6800 400 700 1000 2100 3600 4900 6100 7200 1000 1400 1700 2000 3100 4600 5900 7100 8200 1000 2000 2400 2700 3000 4100 5600 6900 8100 9200

k=2

k=4

k=6

0.0182 0 0 0 0.2443 0.1427 0 0 0.2371 0.0148 0 0 0 0 0.0239 0.0125 0 0 0.3358 0.1980 0.0365 0.0393 0 0.0133 0 0 0.4617 0.2140 0.0391 0.0044 0.0520 0.0130 0 0 0 0.7048 0.2264 0.0377 0.0032 9 10−5

0 0 0.2100 0.1183 0.1164 0.1356 0 0 0.4010 0.1133 0.0104 0.0006 0 0 0.0250 0 0.2014 0.2319 0.1046 0.0538 0.2704 0.0049 0.1104 0.0076 0.0227 0.4062 0.0370 0.1243 0.2824 0.1151 0.0041 0.0335 0.5734 0.0286 0.0060 0.0293 0.3614 0.3323 0.1269 0.0190

0 0.4017 0.0279 0.3742 0 0 0.0600 0 0.6819 0.4900 0.1907 0.0394 0.0031 0.3316 0 0 0.2866 0.2035 0.0398 0.4172 0 0.0054 0.6524 0 0 5 10−5 0.3017 0.2447 8 10−5 0.3984 0.0419 0.0347 0.7566 0.0128 0 0.4178 0.0092 0.1687 0.4513 0.3557 (continued)

Appendix D: Squared Reduced-Matrix Elements …

438 (continued) 2S+1

LJ

6

F11/2

EJJ′ (cm−1)

k=2

k=4

k=6

F9/2 6 F7/2 6 F5/2 6 H15/2 6 F3/2 6 F1/2 6 H13/2 6 H11/2 6 H9/2 6 H7/2 6 H5/2

1400 2400 3400 3800 4100 4400 5500 7000 8300 9500 10,600

0.0532 0.0065 0 1.0105 0 0 0.1581 0.0190 0.0014 4 10−5 0

0.0676 0.0456 0.0188 0.7661 0.0030 0 0.5983 0.2577 0.0674 0.0102 0.0006

0.0189 0.0325 0.0500 0.3489 0.0499 0.0313 0.7011 0.7461 0.5189 0.2322 0.0527

2S′+1

EJJ′ (cm−1)

2S′+1

L′J′

6

Eu3+: 2S+1 7

F1 7 F2 7

F3

7

F4

7

F5

7

F6

LJ

7

F0 7 F1 7 F0 7 F2 7 F1 7 F0 7 F3 7 F2 7 F1 7 F0 7 F4 7 F3 7 F2 7 F1 7 F0 7 F5 7 F4 7 F3 7 F2 7 F1 7 F0

L′J′

400 600 1000 900 1500 1900 1000 1900 2500 2900 1000 2000 2900 3500 3900 1100 2100 3100 4000 4600 5000

k=2

k=4

k=6

0 0.0518 0.1372 0.1852 0.2087 0 0.3833 0.2207 0 0 0.5611 0.1737 0 0 0 0.5212 0.0846 0 0 0 0

0 0 0 0.2121 0.1266 0 0.1337 0.0066 0.1731 0.1382 0.0131 0.2522 0.3150 0.1190 0 0.6455 0.5150 0.2306 0.0476 0 0

0 0 0 0 0 0 0.1554 0.0317 0 0 0.4430 0.3817 0.2088 0.0544 0 0.1217 0.2719 0.4120 0.4696 0.3765 0.1442 (continued)

Appendix D: Squared Reduced-Matrix Elements …

439

(continued) 2S+1 5

D0

5

D1

5

D2

5

D3

LJ

2S′+1 7

F6 7 F5 7 F4 7 F3 7 F2 7 F1 7 F0 5 D0 7 F6 7 F5 7 F4 7 F3 7 F2 7 F1 7 F0 5 D1 5 D0 7 F6 7 F5 7 F4 7 F3 7 F2 7 F1 7 F0 5 D2 5 D1 5 D0 7 F6 7 F5 7 F4 7 F3 7 F2 7 F1 7 F0

L′J′

EJJ′ (cm−1)

k=2

k=4

k=6

12,300 13,400 14,400 15,400 16,300 16,900 17,300 1700 14,000 15,100 16,100 17,100 18,000 18,600 19,000 2500 4200 16,500 17,600 18,600 19,600 20,500 21,100 21,500 2400 4900 6600 18,900 20,000 21,000 22,000 22,900 23,500 23,900

0 0 0 0 0.0035 0 0 0 0 0 0 0.0042 0.0009 0.0028 0 0.0105 0.0112 0 0 0.0024 0.0023 0.0018 0.0002 0.0009 0.0300 0.0136 0 0 0.0002 0.0036 0.0009 0.0003 0.0005 0

0 0 0.0030 0 0 0 0 0 0 0.0009 0.0031 0.0024 0 0 0 0 0 2 10−5 0.0018 0.0002 0.0026 0.0015 0 0 0.0172 0.0074 0 7 10−5 0.0014 0.0004 0.0004 0.0021 0.0012 0

0.0005 0 0 0 0 0 0 0 0.0006 5 10−5 0 0 0 0 0 0 0 0.0002 2 10−5 0.0001 0 0 0 0 0 0 0 2 10−5 2 10−6 0.0002 0.0002 0 0 0

Appendix D: Squared Reduced-Matrix Elements …

440

Tb3+: 2S+1 7

F5 7 F4 7

F3

7

F2

7

F1

7

F0

5

D4

5

D3

LJ

2S′+1 7

F6 7 F5 7 F6 7 F4 7 F5 7 F6 7 F3 7 F4 7 F5 7 F6 7 F2 7 F3 7 F4 7 F5 7 F6 7 F1 7 F2 7 F3 7 F4 7 F5 7 F6 7 F0 7 F1 7 F2 7 F3 7 F4 7 F5 7 F6 5 D4 7 F0 7 F1 7 F2 7 F3 7 F4 7 F5 7 F6

L′J′

EJJ′ (cm−1)

k=2

k=4

k=6

2100 1400 3500 900 2300 4400 700 1600 3000 5100 500 1200 2100 3500 5600 200 700 1400 2300 3700 5800 14,700 14,900 15,400 16,100 17,000 18,400 20,500 6300 21,000 21,200 21,700 22,400 23,300 24,700 26,800

0.5122 0.5415 0.0868 0.3474 0.1621 0 0.1685 0.2211 0 0 0.0512 0.1928 0 0 0 0 0.1388 0 0 0 0 0 0 0.0016 0.0137 0.0003 0.0139 0.0007 0.0501 0 0.0017 0.0016 0.0005 0.0073 0.0008 0

0.6426 0.0122 0.5140 0.1288 0.2358 0.2142 0.1936 0.0060 0.3129 0.0479 0 0.1204 0.1707 0.1175 0 0 0 0 0.1386 0 0 0.0022 0.0025 0.0004 0.0010 0.0019 0.0010 0.0013 0.0274 0 0.0030 0.0030 0.0111 0.0002 0.0028 0.0006

0.1181 0.4360 0.2667 0.1450 0.3512 0.3804 0 0.0326 0.2077 0.4676 0 0 0 0.0544 0.3738 0 0 0 0 0 0.1440 0 0 8 10−5 0.0007 0.0015 0.0026 0.0011 0.0063 0 0 0 0.0002 0.0003 0.0016 0.0014

Appendix D: Squared Reduced-Matrix Elements …

441

Dy3+: 2S+1

LJ

6

H13/2 6 H11/2 6

H9/2

6

F11/2

6

H7/2

6

F9/2

6

H5/2

6

F7/2

2S′+1 6

L′J′

H15/2 6 H13/2 6 H15/2 6 H11/2 6 H13/2 6 H15/2 6 H9/2 6 H11/2 6 H13/2 6 H15/2 6 F11/2 6 H9/2 6 H11/2 6 H13/2 6 H15/2 6 H7/2 6 F11/2 6 H9/2 6 H11/2 6 H13/2 6 H15/2 6 F9/2 6 H7/2 6 F11/2 6 H9/2 6 H11/2 6 H13/2 6 H15/2 6 H5/2 6 F9/2 6 H7/2 6 F11/2 6 H9/2 6 H11/2 6 H13/2 6 H15/2

EJJ′ (cm−1)

k=2

k=4

k=6

3400 2250 5650 1900 4150 7550 – 1900 4150 7550 1350 1350 3250 5500 8900 – 1350 1350 3250 5500 8900 1100 1100 2450 2450 4350 6600 10,000 800 1900 1900 3250 3250 5150 7400 10,800

0.2286 0.2464 0.0673 0.3280 0.0276 0 0.0039 0.0022 0.2274 0.8749 0.0006 0.2974 0.0309 0 0 0.0025 0.0138 0.0356 0.2382 0.6199 0 6 10−5 0.2047 0 0.0228 0 0 0 0.0031 0.0450 0.0430 0.0333 0.2182 0.4029 0 0

0.3879 0.4412 0.0409 0.1702 0.1647 0.0157 0.1009 0.1907 0.4342 0.8360 0.0256 0.1574 0.1466 0.0265 0.0007 0.1193 0.0162 0.3155 0.3663 0.0246 0.5628 0.0180 0.1871 0.0023 0.1319 0.0225 0.0010 0 0.1256 0.0049 0.2747 0.0272 0.1272 0.0527 0.4138 0.1167

0.6525 0.0359 0.5891 0.0077 0.3766 0.2003 0.4608 0.7845 0.7254 0.1909 0.1374 0.0095 0.3047 0.2709 0.0415 0.4088 0.0151 0.1816 0.0121 0.3811 0.6747 0.3172 0.0784 0.0183 0.2970 0.2812 0.0606 0.0032 0.3907 0.0481 0 0.0792 0.2475 0.2756 0 0.6619 (continued)

Appendix D: Squared Reduced-Matrix Elements …

442 (continued) 2S+1

LJ

6

F5/2

6

F3/2

6

F1/2

2S′+1

L′J′

6

F7/2 6 H5/2 6 F9/2 6 H7/2 6 F11/2 6 H9/2 6 H11/2 6 H13/2 6 H15/2 6 F5/2 6 F7/2 6 H5/2 6 F9/2 6 H7/2 6 F11/2 6 H9/2 6 H11/2 6 H13/2 6 H15/2 6 F3/2 6 F5/2 6 F7/2 6 H5/2 6 F9/2 6 H7/2 6 F11/2 6 H9/2 6 H11/2 6 H13/2 6 H15/2

EJJ′ (cm−1)

k=2

k=4

k=6

1400 2200 3300 3300 4650 4650 6550 8800 12,200 800 2200 3000 4100 4100 5450 5450 7350 9600 13,000 400 1200 2600 3400 4500 4500 5850 5850 7750 10,000 13,400

0.0395 0.0353 0.0133 0.1940 0 0.3313 0 0 0 0.0222 0.0148 0.1318 0 0.0430 0 0 0 0 0 0.0152 0.0113 0 0.1902 0 0 0 0 0 0 0

0.0061 0.2690 0.0307 0.0542 0.0455 0.1045 0.1953 0.1998 0 0.0273 0.0071 0.1279 0.0312 0.2747 0.0164 0.1228 0.1852 0 0 0 0 0.0260 0 0.0072 0.1330 0 0.1460 0 0 0

0.0077 0 0.0288 0.3982 0.0834 0.0425 0.1690 0.2747 0.3385 0 0 0 0.0092 0 0.0302 0.3315 0.0340 0.3776 0.0606 0 0 0 0 0 0 0.0048 0 0.3336 0.0991 0

Ho3+: 2S′+1

EJJ′ (cm−1)

k=2

k=4

k=6

5

5

5050

0.0249

0.1344

1.5210

5

5

3400

0.0319

0.1336

0.9308

5

8550

0.0083

0.0383

0.6917

5

2250

0.0438

0.1705

0.5729

5

6050

0.0027

0.0226

0.8887

5

11,150

0

0.0098

0.0936

2S+1

I7 I6

LJ

L′J′

I8 I7 I8

5

I5

I6 I7 I8

(continued)

Appendix D: Squared Reduced-Matrix Elements …

443

(continued) 2S+1 5

I4

LJ

2S′+1

EJJ′ (cm−1)

k=2

k=4

k=6

5

2050

0.0313

0.1238

0.9100

5

4600

0.0022

0.0281

0.6640

5

8100

0

0.0033

0.1568

L′J′

I5 I6 I7

5

13,150

0

0

0.0077

5

2250

0.0001

0.0059

0.0039

5

4300

0.0068

0.0271

0.1649

5

6850

0.0102

0.1213

0.4995

5

10,350

0.0177

0.3298

0.4340

5

15,400

0

0.4277

0.5685

5

3000

0

0.0110

0.0036

5

5250

0.0014

0.0262

0.2795

5

7300

0

0.0043

0.1062

5

9850

0

0.0206

0.1540

5

13,350

0

0

0.4096

I8

5

F5

I4 I5 I6 I7 I8

5

S2

F5 I4 I5 I6 I7

5

18,450

0

0

0.2270

5

–

0.0002

0.0147

0.0052

5

3000

0.1944

0.0923

0.0080

5

5250

0.0001

0.0234

0.2587

5

7300

0.0018

0.1314

0.4655

5

9850

0.0012

0.2580

0.1697

5

13,350

0

0.1988

0.0324

I8

5

F4

S2 F5 I4 I5 I6 I7

5

18,450

0

0.2402

0.7079

5

2100

0.0971

0.0289

0.0957

5

2100

0.0061

0.0009

0

5

5100

0.0388

0.0820

0.0873

5

7350

0.0003

0.0980

0.3964

5

9400

0

0.2154

0.0173

5

11,950

0

0.0904

0.2170

5

15,450

0

0.2483

0.2275

5

20,550

0

0

0.3464

5

450

0.0459

0.0002

0

5

2550

0.0067

0.0268

0.0270

5

2550

0.0016

0.0028

0

5

5600

0

0.0082

0.1172

5

7950

0.0004

0.1810

0.0273

5

9850

0

0.0427

0.3125

5

12,450

0

0.1287

0.1532

5

15,590

0

0

0.1760

5

21,000

0

0

0.1918

I8

5

F3

F4 S2 F5 I4 I5 I6 I7 I8

5

F2

F3 F4 S2 F5 I4 I5 I6 I7 I8

(continued)

Appendix D: Squared Reduced-Matrix Elements …

444 (continued) 2S+1 3

K8

LJ

2S′+1

EJJ′ (cm−1)

k=2

k=4

k=6

5

250

0

0

0.0005

5

750

0

0

0.0062

5

2850

0

0.0079

0.0004

5

2850

0

0

0.0002

5

5850

0

0.0263

0.0195

5

8100

0

0.0045

0.0012

5

10,150

0

0.0004

0.0041

5

12,700

0.0059

0.0041

0.0138

5

16,200

0.0019

0.0046

0.0406

5

21,250

0.0209

0.03,294

0.1579

3

850

0.0005

0.0027

0.2616

5

1150

0

0.0257

0.1144

5

1600

0

0.0666

0.1595

5

3700

0.2551

0.2392

0.1347

5

3700

0

0.3250

0.0031

5

6700

1.1528

0.3576

0.0329

5

8950

0.0005

0.0013

2 10−5

5

11,000

0.0165

0.0307

0.0133

5

13,500

0.0093

0.0837

0.1094

5

17,050

0.1523

0.04,374

0.2588

5

22,150

1.5180

0.8548

0.1416

5

–

0

0

0.0530

3

850

0

0

0

5

1150

0.0496

0

0

5

1600

0.0080

0.0604

0

5

3700

0

0.0470

0

5

3700

0.0096

0

0

5

6700

0

3 10−5

0.1139

5

8950

0

0.1442

0

5

11,000

0

0.14042

0.1710

5

13,550

0

0

0.2398

5

17,050

0

0

0.0570

5

22,150

0

0

0

5

1750

0

0.0078

0.0574

5

1750

0.0617

0.2595

00.617

3

2650

0

0.0093

0.0007

5

2900

0

0.1292

0.0022

5

3500

0.1927

0.1029

00.319

5

5450

0.2984

0.0216

0.1446

5

5450

0

0.1292

0.0018

5

8500

0.3540

0.0426

0.1198

5

10,750

10−5

0.0100

0.0427

5

12,750

0.0036

0.0689

0.0598

5

15,350

0.1374

0.1857

0.0806

5

18,850

0.6185

0.0308

0.1090

5

23,900

0

0.0548

0.1610

L′J′

F2 F3 F4 S2 F5 I4 I5 I6 I7 I8

5

G6

K8 F2 F3 F4 S2 F5 I4 I5 I6 I7 I8

5

F1

G6 K8 F2 F3 F4 S2 F5 I4 I5 I6 I7 I8

5

G5

F1 G6 K8 F2 F3 F4 S2 F5 I4 I5 I6 I7 I8

(continued)

Appendix D: Squared Reduced-Matrix Elements …

445

(continued) 2S+1

LJ

5

G4

2S′+1

EJJ′ (cm−1)

k=2

k=4

5

1900

0.0082

01650

0.0224

5

3700

0

00564

0

5

3700

0.0042

02045

0.2885

3

4550

0

00800

0.0017

5

4800

0.2149

00002

0.0732

5

5300

0.2233

00215

0.0489

5

7400

0.4086

01102

0.0214

5

7400

0.0246

02293

0.0097

5

10,400

0.0298

00141

0.2246

5

12,600

0.0154

01093

0.0545

5

14,700

0.2268

02775

0.0322

5

17,250

0.7156

00246

0.0009

5

20,750

0

02990

0.0653

5

25,800

0

0.0346

0.0348

5

250

0

0.0139

0.0042

5

2150

0.0163

00059

0.2302

5

3900

0

0

0.0018

5

3900

7 10−5

0.0002

0.1060

3

4800

0.0877

7 10−5

0.1252

5

5050

0

0

0.0104

5

5500

0

0.0074

0.0041

5

7600

0

0.0153

0.0089

5

7600

0

0

0.0260

5

10,650

0.0015

0.0113

0.0141

5

12,900

0

0.0007

0.0069

5

14,900

0.0068

0.0042

0.0312

5

17,500

0.0011

0.0058

0.0716

5

20,950

0.0056

0.0062

0.0050

5

26,050

0.0058

0.0046

0.0338

L′J′

G5 F1 G6 K8 F2 F3 F4 S2 F5 I4 I5 I6 I7 I8

3

K7

G4 G5 F1 G6 K8 F2 F3 F4 S2 F5 I4 I5 I6 I7 I8

k=6

Er3+: 2S+1

LJ

4

I13/2 4 I11/2 4

I9/2

4

F9/2

2S′+1 4

L′J′

I15/2 4 I13/2 4 I15/2 4 I11/2 4 I13/2 4 I15/2 4 I9/2

EJJ′ (cm−1)

k=2

k=4

k=6

6500 3600 10,100 2150 5750 12,250 2900

0.0195 0.0331 0.0282 0.0030 0.0004 0 0.1279

0.1173 0.1708 0.0003 0.0674 0.0106 0.1732 0.0059

1.4316 1.0864 0.3953 0.1271 0.7162 0.0099 0.0281 (continued)

Appendix D: Squared Reduced-Matrix Elements …

446 (continued) 2S+1

LJ

4

F9/2

4

S3/2

2

H(2)11/2

4

F7/2

4

F5/2

4

F3/2

2S′+1 4

L′J′

I11/2 4 I13/2 4 I15/2 4 F9/2 4 I9/2 4 I11/2 4 I13/2 4 I15/2 4 S3/2 4 F9/2 4 I9/2 4 I11/2 4 I13/2 4 I15/2 2 H(2)11/2 4 S3/2 4 F9/2 4 I9/2 4 I11/2 4 I13/2 4 I15/2 4 F7/2 2 H(2)11/2 4 S3/2 4 F9/2 4 I9/2 4 I11/2 4 I13/2 4 I15/2 4 F5/2 4 F7/2 2 H(2)11/2 4 S3/2 4 F9/2 4 I9/2 4 I11/2 4 I13/2 4 I15/2

EJJ′ (cm−1)

k=2

k=4

k=6

5050 8650 15,150 3200 6100 8250 11,850 18,350 800 4000 6900 9050 12,650 19,150 1150 1950 5150 8050 10,200 13,800 20,300 1650 2800 3600 6800 9700 11,850 15,450 21,950 350 2000 3150 3950 7150 10,050 12,200 15,800 22,300

0.0704 0.0101 0 0 0 0 0 0 0 0.3629 0.2077 0.0357 0.0230 0.7125 0.1229 0.0001 0.0121 0.0163 0.0035 0 0 0.0765 0 0.0082 0.0004 0.0107 0 0 0 0.0618 0.0026 0 0.0260 0 0 0 0 0

0.0112 0.1533 0.5354 0.0003 0.0788 0.0042 0 0 0.1988 0.0224 0.0662 0.1382 0.0611 0.4123 0.0153 0.0058 0.0342 0.0954 0.2648 0.3371 0.1468 0.0503 0.0586 0.0040 0.2415 0.0576 0.0979 0.1783 0 0.0350 0.0584 0.0005 0 0.0040 0.2299 0.0927 0 0

1.2839 0.0714 0.4619 0.0264 0.2542 0.0739 0.3462 0.2211 0.0101 0.0022 0.2858 0.0371 0.0527 0.0925 0.4017 0 0. 0.4277 0.1515 0.0001 0.6266 0.1015 0.1825 0 0.3575 0.0102 0.0028 0.3429 0.2233 0 0 0.0030 0 0.0595 0.0558 0.4861 0.0345 0.1272 (continued)

Appendix D: Squared Reduced-Matrix Elements …

447

(continued) 2S+1

LJ

2

G(1)9/2

4

G11/2

4

G9/2

2S′+1 4

L′J′

F3/2 4 F5/2 4 F7/2 2 H(2)11/2 4 S3/2 4 F9/2 4 I9/2 4 I11/2 4 I13/2 4 I15/2 2 G(1)9/2 4 F3/2 4 F5/2 4 F7/2 2 H(2)11/2 4 S3/2 4 F9/2 4 I9/2 4 I11/2 4 I13/2 4 I15/2 4 G11/2 2 G(1)9/2 4 F3/2 4 F5/2 4 F7/2 2 H(2)11/2 4 S3/2 4 F9/2 4 I9/2 4 I11/2 4 I13/2 4 I15/2

EJJ′ (cm−1)

k=2

k=4

k=6

2100 2450 4100 5250 6050 9250 12,150 14,300 17,900 24,400 2000 4100 4450 6100 7250 8050 11,250 14,150 16,300 19,900 26,400 950 2950 5050 5400 7050 8200 9000 12,200 15,100 17,250 20,850 27,350

0 0.0124 0.1058 0.0308 0 0.0055 0.0147 0.0428 0.0780 0 0.2906 0 0 0.0877 0.0004 0 0.4252 0.0716 0.0003 0.1013 0.9181 0.0005 0.0269 0 0.1630 0.6062 0.0218 0 0.2201 0.0051 0.0894 1.0908 0

0.0208 0.0259 0.0488 0.1828 0.0019 0.0314 0.0062 0.0824 0.1194 0.0190 0.1170 0.0234 0.0378 0.1287 0.1539 0.1302 0.0368 0.0131 0.0496 0.2651 0.5261 0.2021 0 0.1750 00824 0.0088 0.3274 0.1551 0.3121 0.0042 0.1524 0.3520 0.2415

0.0087 0.0063 0.0240 0.0671 0.0025 0.0369 0.0043 0.1128 0.3535 0.2255 0.1328 0.0923 0.0815 0.0159 0.0494 0.0044 0.0122 0.0235 0.0134 0.2594 0.1171 0.1639 0.0452 0.1089 0.0028 0.1243 0.1496 0.0100 0.3765 0.0027 0.0144 0.0160 0.1234 (continued)

Appendix D: Squared Reduced-Matrix Elements …

448 (continued) 2S+1

LJ

2

K15/2

2

G(1)7/2

2

P3/2

2S′+1 4

L′J′

G9/2 4 G11/2 2 G(1)9/2 4 F3/2 4 F5/2 4 F7/2 2 H(2)11/2 4 S3/2 4 F9/2 4 I9/2 4 I11/2 4 I13/2 4 I15/2 2 K15/2 4 G9/2 4 G11/2 2 G(1)9/2 4 F3/2 4 F5/2 4 F7/2 2 H(2)11/2 4 S3/2 4 F9/2 4 I9/2 4 I11/2 4 I13/2 4 I15/2 2 G(1)7/2 2 K15/2 4 G9/2 4 G11/2 2 G(1)9/2 4 F3/2 4 F5/2 4 F7/2 2 H(2)11/2 4 S3/2 4 F9/2 4 I9/2 4 I11/2 4 I13/2 4 I15/2

EJJ′ (cm−1)

k=2

k=4

k=6

350 1300 3300 5400 5750 7400 8550 9350 12,550 15,450 17,600 21,200 27,700 150 500 1450 3450 5550 5900 7550 8700 9500 12,700 15,600 17,750 21,350 27,850 3700 3850 4200 5150 7150 9250 9600 11,250 12,400 13,200 16,400 19,300 21,450 25,050 31,550

0 0.0965 0 0 0 0 0.0977 0 0 0 0.0468 0.0001 0.0219 0 0.0041 0.0150 0.0145 0.0941 0.3716 0.1239 0.0019 0.0445 0.0003 0.1586 0.4934 0 0 0.0125 0 0 0 0 0.0123 0.0173 0.0211 0 0.0813 0 0 0 0 0

0.0114 0.0595 0.7106 0 0 0.0001 0.0001 0 0.0776 0.2221 0.0018 0.0016 0.0041 0.1154 0.1891 0.0604 0.0056 0.0314 0.0023 0.0424 0.0344 0.1594 0.0078 0.3607 0.2708 0.1009 0.0174 0.0004 0 0.0125 0.0266 0.2083 0 0.0433 0.0076 0.0168 0 0.0464 0.0461 0.0995 0 0

0.0598 0.0706 0.0708 0.0001 0.0461 0.0002 1.1458 0.0032 0.0125 0.1003 0.2488 0.0361 0.0758 0.0026 0.1582 0.0193 0.0205 0 0.0378 0.0071 0.2672 0 0.0128 0.2204 0.1674 0.0512 0.1163 0 0.0268 0.0053 0.0107 0.2591 0 0 0 0.0263 0 0.0060 0.0041 0.0400 0.1478 0.0172 (continued)

Appendix D: Squared Reduced-Matrix Elements …

449

(continued) 2S+1

LJ

2

K13/2 4 G5/2 2 P1/2 4 G7/2 2 D(1)5/2 2 H(2)9/2 4 D5/2 4 D7/2 2 I11/2 2 L17/2 4 D3/2 2 D(1)3/2 2 I13/2 4 D1/2 2 H(1)9/2 2 L15/2 2 D(2)5/2

EJJ′ (cm−1)

k=2

k=4

k=6

I15/2 4 I15/2 4 I15/2 4 I15/2 4 I15/2 4 I15/2 4 I15/2 4 I15/2 4 I15/2 4 I15/2 4 I15/2 4 I15/2 4 I15/2 4 I15/2 4 I15/2 4 I15/2 4 I15/2

33,000 33,300 33,350 33,900 34,700 36,450 38,450 39,050 40,900 41,600 42,150 42,850 43,600 46,950 47,750 47,750 48,900

0.0032 0 0 0 0 0 0 0 0.0002 0.0047 0 0 0.0055 0 0 0.0002 0

0.0029 0 0 0.0334 0 0.0500 0 0.8919 0.0285 0.0663 0 0 0.0171 0 0.0038 0.0027 0

0.0152 0.0026 0 0.0028 0.0227 0.0001 0.0267 0.0291 0.0034 0.0328 0.0126 0.0002 0.0050 0 0.0001 0.0021 0.0096

2S′+1

EJJ′ (cm−1)

k=2

k=4

k=6

5600 2500 8100 4450 6950 12,550 1800 6250 8750 14,350 650 2450 6900 9400 15,000

0.249 0.011 0.107 0.089 0.129 0.527 0.002 0.629 0.081 0 0.004 0.311 0 0.287 0

0.118 0.48 0.231 0.125 0.133 0.718 0.0005 0.347 0.344 0.316 0.075 0.056 0.29 0.163 0.0005

0.608 0.004 0.638 0.905 0.213 0.228 0.167 0 0.264 0.841 0 0.044 0.583 0.074 0.258 (continued)

2S′+1

L′J′

4

Tm3+: 2S+1

LJ

3

H4 (3F4) 3 H5 3

F4 (3H4)

3

F3

3

F2

3

L′J′

H6 3 H4 (3F4) 3 H6 3 H5 3 H4 (3F4) 3 H6 3 F4 (3H4) 3 H5 3 H4 (3F4) 3 H6 3 F3 3 F4 (3H4) 3 H5 3 H4 (3F4) 3 H6

Appendix D: Squared Reduced-Matrix Elements …

450 (continued) 2S+1 1

G4

1

D2

3

P0

1

I6

3

P1

LJ

2S′+1 3

L′J′

F2 3 F3 3 F4 (3H4) 3 H5 3 H4 (3F4) 3 H6 1 G4 3 F2 3 F3 3 F4 (3H4) 3 H5 3 H4 (3F4) 3 H6 1 D2 1 G4 3 F2 3 F3 3 F4 (3H4) 3 H5 3 H4 (3F4) 3 H6 3 P0 1 D2 1 G4 3 F2 3 F3 3 F4 (3H4) 3 H5 3 H4 (3F4) 3 H6 1 I6 3 P0 1 D2 1 G4 3 F2 3 F3 3 F4 (3H4) 3 H5 3 H4 (3F4) 3 H6

EJJ′ (cm−1)

k=2

k=4

k=6

6100 6700 8500 12,950 15,500 21,050 6750 12,850 13,450 15,250 19,700 22,250 27,800 6900 13,650 19,700 20,350 22,150 26,600 29,100 34,700 1400 8300 15,050 21,100 21,750 23,550 28,000 30,500 36,100 – 1400 8300 15,050 21,100 21,750 23,550 28,000 30,500 36,100

0.0060 0.0105 0.0034 0.0738 0.1583 0.0481 0.1905 0.0647 0.1607 0.5631 0 0.1240 0 0.0253 0 0.3543 0 0 0 0 0 0 0 0.2128 0 0 0.0622 0.0010 0.0669 0.0107 0 0 0.4444 0 0.1370 0.5714 0 0 0 0

0.0717 0.0733 0.0194 0.0059 0.0042 0.0752 0.1722 0.3055 0.0680 0.0935 0.0011 0.0116 0.3079 0 0.0525 0 0 0.2715 0 0.0204 0 0 0.0520 1.2488 0.0410 0.0028 0.5013 0.0021 0.3112 0.0392 0 0 0 0.0050 0 0.1964 0.1074 0.2857 0.4055 0

0.0417 0.3056 0.0718 0.5423 0.3783 0.0119 0.0009 0 0 0.0225 0.0185 0.2266 0.0926 0 0 0 0 0 0 0 0.0757 0.0190 0.8448 0.6302 0.3545 0.0074 0.3921 0.0056 0.0992 0.0136 0.0011 0 0 0 0 0 0 0.0893 0 0.1239 (continued)

Appendix D: Squared Reduced-Matrix Elements …

451

(continued) 2S+1 3

P2

LJ

2S′+1 3

L′J′

P1 1 I6 3 P0 1 D2 1 G4 3 F2 3 F3 3 F4 (3H4) 3 H5 3 H4 (3F4) 3 H6

EJJ′ (cm−1)

k=2

k=4

k=6

1800 1800 3200 10,100 16,850 22,900 23,550 25,350 29,800 32,300 37,900

0.1822 0 0.1247 0.0004 0.5964 0.0045 0.1445 0.1359 0 0.2811 0

0 0.0981 0 0.1560 0.0009 0.0433 0.2343 0.0858 0.1979 0.0096 0.2713

0 0.6808 0 0 0.1055 0 0 2 10−5 0.1895 0.0064 0.0228

Appendix E 3jm Factors for Some Group Chains

For the convenience of the table list, the symbol of point group irreducible representation adopted the subscript of Bathe symbol (i.e. C1 ) 1, C2 ) 2, C3 ) 3, …). The irreducible representations of group G and its subgroup H denoted by ki and li, respectively, then the 3jm factor of group chain G H expressed as follows k1 l1

k2 l2

k3 l3 s a1

a2

a3

where ai denotes the multiple decomposition of irreducible representation, s denotes the multiple coupling of subgroup H. As an example, some of the 3jm factors of SO3 O group chain will be used to illustrate the meaning of the following table. In the table of group chain SO3 O it can be found the black numbers 3 5/2 3/2 which characterize the irreducible representations of SO3 group and below this line there is a line of 4 7

8

0 000 þ

pﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃ þ 3= 2:7

It means that

3 5=2 4 7

3=2 8

pﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ¼ þ 3= 2 7

0 ~

In this 3jm factor the irreducible representations of O group are 1, 12, 32 of Butler symbol and C4, C7, C8 of Bethe while the symbol in this book is simply 4, 7, 8. The multiple coupling of subgroup is s = 0 and the multiple decomposition of irreducible representation a1 = 0, a2 = 0, a3 = 0 and the sign change brought by the column permutation are given after the multiple decomposition symbol, the column permutation + and − express that the column exchange the sign of the 3jm factor does not change and change, respectively. Particular attention should be paid to the © Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8

453

454

Appendix E: 3jm Factors for Some Group Chains

points between the numbers of the numerical value of the 3jm factor. It expresses the meaning of multiplication, rather than the decimal point. The next two lines are 3 5

5=2 8

3=2 8 0

3 5

5=2 8

3=2 8 0

0 0þ

0

3 C5

5=2 C8

3=2 C8

3 C5

5=2 C8

3=2 C8

SO3 0O

5 ¼ pﬃﬃﬃﬃﬃ 2 21

with 0

0

0

SO3 1O

1 ¼ pﬃﬃﬃﬃﬃ 2 21

For the situation of absence of multiple coupling of subgroup or multiple decomposition of irreducible representation, the corresponding marks will not appear in the table. The 3jm factor has two kinds of symmetry, that is, the column permutation symmetry and the complex conjugate symmetry. After two column permutation operation, the value of 3jm factor remains unchanged; for example, the 3jm factor of D2 C2 group chain

5 4

5 1 3 1

D2

1 ¼ pﬃﬃﬃ 2 C2

After column permutation one have

5 4

1 5 1 3

¼

1 1

5 3

5 4

¼

5 3

5 4

1 1

1 ¼ pﬃﬃﬃ 2

If the complex conjugate will bring changes of the sign of 3jm factor then an asterisk will be added to the upper right corner of it, as an example

5 5 4 3

1 1

¼

1 5 pﬃﬃﬃ ¼ 3 2

5 1 4 1

This result is the same as the results of the permutation. For the 3jm factor of D3 C3 group chain

6

3

6 6

3 3

6

2

1 1 pﬃﬃﬃ ¼ pﬃﬃﬃ 5 6 2 4 2 2 4 5 3 4 i i ¼ pﬃﬃﬃ ¼ pﬃﬃﬃ ¼ 4 6 3 5 2 2 4

¼ þ

5 3

4

¼

Appendix E: 3jm Factors for Some Group Chains

2

455

Some of the 3jm Factor of SO3

3/2 3/2

8

8

1

0 100+

3

8

8

0 000+

2

5

8

8

1

0 110+

5

8

8

0 000+

3

5

8

8

4

0 000-

5

8

8

1 000-

9/2 9/2

0

2

8

4

0 100-

8

4

0 110-

0 0

6

3

0 000-

1 5 11

8

8

4

1 000-

6

3

0 100-

4 7 5 3.11

8

8

4

1 100-

8

6

5

0 000-

8

8

4

1 110-

3.11

8

6

5

0 100-

8

8

3

0 000+

8

8

3

0 000+

4 2.3 5 5.11

8

8

3

0 100+

0

2 7 3 3.5.11.13

8

8

O Group Chain

5.11.13

0

8

8

2

4

4

11.13

1

11.13

0 2.3

11.13

0

8

8

3

0 100+

2.7 5 5.11

8

8

3

0 110+

8.2 2 3 3.11.13

8

8

3

0 110+

8 2 5 3.5.11

8

8

5

0 000+

2.3 5 11.13

8

8

5

0 000+

9 5 5.11

8

8

5

0 100+

4 7 5 3.11.13

8

8

5

0 100+

4 7 5 3.5.11

8

8

5

0 110+

4 13 3.5 11

2.3 5 5.11

8

8

5

1 000-

8

8

5

1 100-

8

8

5

1 110-

6 1

9/2

9/2

6

6

0 000+

1

8

8

0 000+

4 2.3 5 5.11.13

1

8

8

0 010+

3 7 5 2.5.11.13

2.5.11.13

1

8

8

0 011+

3.5.11.13

4

6

6

0 000-

4

8

6

0 000+

4

8

6

0 010+

8

8

5

0 110+

8

8

5

1 000-

8

8

5

1 100-

8

8

5 4

9/2 9/2

1 110-

0 2 7

3.5.11

0

6

6

1

0 000+

6

6

4

0 000-

8

6

4

0 000+

8

6

4

0 100+

8

6

3

0 000-

4

8

6

3

0 100-

2 7 3 3.5.11.13

7 2.7 3 3.5.11.13

0 3 7 2 2

5.11.13

8

6

5

0 000-

19

8

6

5

0 100-

2 2.7 3 5.11.13

8

8

1

0 000+

5

8

6

2.3.5.11.13

3.7

5.11.13

0 010-

3

2 2.3 5 11.13

5

8

6

0 100-

5

8

6

0 110-

5 5

8 8

8 8

0 000+ 0 010+

2.5.7.13

2 2.13 5 7.11

0 5

3.7.13

0 7

3.11.13

0 8

3.5.11.13

8.4 2 5 3.5.11.13

0 2.3.7 5 11.13 3.7 5 2.11.13

0

4

8

8

0 000-

4

8

8

0 010-

4

8

8

0 011-

0

4 4

8 8

8 8

1 000-

0

4 3

8 8

8 6

0 000-

2.7 5 11.13

3

8

6

0 010-

8 2 5 3.11.13 8 3.7 5 5.11.13

3

1 0101 011-

3

8

8

0 000+

3

8

8

0 010+

3

8

8

0 011+

5

8

6

0 000-

3 3

5.11.13

5.11.13

0

11 5 5.13 8.2 7 5 3.5.11.13 2

3.5.13

456

Appendix E: 3jm Factors for Some Group Chains

Appendix E: 3jm Factors for Some Group Chains

457

Appendix F Clebsch-Gordan Coefﬁcients of the Cubic Point Group with Trigonal Bases

© Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8

459

460

Appendix F: Clebsch-Gordan Coefﬁcients of the Cubic Point Group …

Appendix F: Clebsch-Gordan Coefﬁcients of the Cubic Point Group …

461

Appendix G Integral Numerical Value Associated with the Thermal Effect of the Spectra

T TD

T D/ T

0.0

0

7 Z

TD =T

x6 ex ð e x 1Þ 2

0

dx

0.1

0.2

0.3

0.4

0.5

0.6

0.7

0.8

0.9

19988.1 10−3

4988.1 10−3

2210.3 10−3

1238.1 10−3

788.2 10−3

543.8 10−3

396.4 10−3

300.8 10−3

235.3 10−3

1

188.5 10−3

153.9 10−3

127.6 10−3

107.1 10−3

90.98 10−3

77.95 10−3

67.31 10−3

58.52 10−3

51.18 10−3

44.99 10−3

2

39.73 10−3

35.23 10−3

31.35 10−3

27.99 10−3

25.06 10−3

22.49 10−3

20.24 10−3

18.25 10−3

16.48 10−3

14.92 10−3

3

13.52 10−3

12.28 10−3

11.16 10−3

10.16 10−3

9.26 10−3

8.44 10−3

7.71 10−3

7.05 10−3

6.44 10−3

5.90 10−3

4

5.40 10−3

4.95 10−3

4.54 10−3

4.17 10−3

3.83 10−3

3.52 10−3

3.24 10−3

2.98 10−3

2.74 10−3

2.53 10−3

5

2.33 10−3

2.15 10−3

1.98 10−3

1.83 10−3

1.69 10−3

1.56 10−3

1.44 10−3

1.33 10−3

1.23 10−3

1.14 10−3

6

1.05 10−3

9.77 10−4

9.05 10−4

8.38 10−4

7.77 10−4

7.20 10−4

6.68 10−4

6.19 10−4

5.75 10−4

5.34 10−4

7

4.96 10−4

4.60 10−4

4.28 10−4

3.98 10−4

3.70 10−4

3.45 10−4

3.21 10−4

2.98 10−4

2.78 10−4

2.59 10−4

8

2.41 10−4

2.25 10−4

2.10 10−4

1.96 10−4

1.83 10−4

1.71 10−4

1.59 10−4

1.49 10−4

1.39 10−4

1.30 10−4

(continued)

© Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8

463

Appendix G: Integral Numerical Value Associated …

464 (continued) T D/ T

0.0

0.1

0.2

0.3

0.4

0.5

0.6

0.7

0.8

0.9

9

1.22 10−4

1.14 10−4

1.07 10−4

1.00 10−4

9.37 10−5

8.79 10−5

8.24 10−5

7.73 10−5

7.25 10−5

6.80 10−5

10

6.39 10−5

6.00 10−5

5.63 10−5

5.30 10−5

4.98 10−5

4.68 10−5

4.41 10−5

4.15 10−5

3.90 10−5

3.68 10−5

11

3.47 10−5

3.27 10−5

3.08 10−5

2.91 10−5

2.74 10−5

2.59 10−5

2.44 10−5

2.31 10−5

2.18 10−5

2.06 10−5

12

1.95 10−5

1.84 10−5

1.75 10−5

1.65 10−5

1.56 10−5

1.48 10−5

1.40 10−5

1.33 10−5

1.26 10−5

1.19 10−5

13

1.13 10−5

1.08 10−5

1.03 10−5

9.73 10−6

9.25 10−6

8.79 10−6

8.36 10−6

7.95 10−6

7.56 10−6

7.20 10−6

14

6.85 10−6

6.52 10−6

6.21 10−6

5.92 10−6

5.64 10−6

5.37 10−6

5.12 10−6

4.89 10−6

4.67 10−6

4.46 10−6

15

4.25 10−6

4.06 10−6

3.88 10−6

3.71 10−6

3.55 10−6

3.39 10−6

3.24 10−6

3.10 10−6

2.97 10−6

2.84 10−6

16

2.72 10−6

2.60 10−6

2.49 10−6

2.39 10−6

2.29 10−6

2.19 10−6

2.10 10−6

2.02 10−6

1.93 10−6

1.86 10−6

17

1.78 10−6

1.71 10−6

1.64 10−6

1.58 10−6

1.51 10−6

1.46 10−6

1.40 10−6

1.34 10−6

1.29 10−6

1.24 10−6

18

1.20 10−6

1.15 10−6

1.11 10−6

1.06 10−6

1.03 10−6

9.87 10−7

9.50 10−7

9.15 10−7

8.82 10−7

8.50 10−7

19

8.19 10−7

7.90 10−7

7.61 10−7

7.34 10−7

7.08 10−7

6.83 10−7

6.59 10−7

6.36 10−7

6.14 10−7

5.93 10−7

20

5.72 10−7

5.52 10−7

5.34 10−7

5.16 10−7

4.98 10−7

4.81 10−7

4.65 10−7

4.50 10−7

4.35 10−7

4.20 10−7

T 10 TD

4 Z

5

0

TD =T

x3 dx ex 1

0.0

22480.5 7352.1 3150.8 1514.4 783.9 431.0 250.0 152.3 97.0 64.3 44.2 31.3 22.6 16.7 12.8

TD/T

0 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15

321000 19610.5 6703.8 2915.9 1413.8 736.6 407.2 237.4 145.4 93.0 61.8 42.6 30.3 21.9 16.3 12.4

0.1

154499 17244.3 6124.1 2701.9 1320.6 692.4 385.0 225.6 139.0 89.1 59.4 41.1 29.4 21.2 15.8 12.0

0.2 99110.5 15265.4 56068.4 2505.8 1234.4 651.1 364.2 211.4 132.7 85.3 57.1 39.7 28.4 20.6 15.4 11.7

0.3 71498.7 13590.3 5140.7 2326.0 1154.7 612.8 344.6 204.0 126.5 81.9 55.0 38.3 27.5 20.0 15.0 11.3

0.4 54997.5 12157.5 4722.0 2160.9 1080.8 577.2 326.1 194.0 120.9 78.6 53.2 37.0 26.6 19.5 14.6 11.1

0.5 44051.3 10922.3 4343.5 2009.5 1012.3 543.8 308.9 184.6 115.6 75.4 51.1 35.7 25.7 18.9 14.2 10.8

0.6 36279.0 9848.7 4005.4 1870.0 948.6 512.6 292.8 175.9 110.6 72.5 49.2 34.5 24.8 18.4 13.8 10.6

0.7 30489.9 8909.3 3690.4 1741.8 889.7 483.5 277.6 167.6 105.8 69.6 47.4 33.4 24.1 17.8 13.5 10.3

0.8

26022.7 8083.1 3407.9 1623.3 835.6 456.0 263.4 159.7 101.3 66.9 45.7 32.2 23.4 17.3 13.1 10.1

0.9

Appendix G: Integral Numerical Value Associated … 465

Index

Symbols 3-j symbol, 57–59, 63, 64, 67, 72, 138, 144, 145, 205, 206 6-j symbol, 58–60, 66, 138, 139 9-j symbol, 59, 60 Al2O3, 203, 207, 222, 228, 234, 264, 309, 322, 330, 335, 336, 386 BeAl2O4, 210, 223 Be2Al2(SiO3)6, 223 BaWO4, 378 CsCaF3, 226 Ca3Ga2Ge4O14, 236 Ca4GdO(BO3)3 (GdCOB), 346 Ca4YO(BO3)3 (YCOB), 346 Gd3Ga5O12, 142, 223 Gd2(MoO4)3, 374 Gd3Sc2Ga3O12, 196, 223 GdVO4, 378, 381 K2NaScF6, 236 K2NaGaF6, 236 KGd (WO4)2 (KGW), 158 KZnF3, 223, 227, 235 La3Lu2Ga3O12, 223 La2(WO4)3, 378 La3Ga5SiO4, 236 LiCaAlF6, 223, 224 LiSrAlF6, 203, 223, 224, 235 MgF2, 223, 226, 227, 237 Mg2SiO4, 203, 215–218 NdAl3(BO3)4 (NAB), 28, 88, 305 Na3Ga2Li3F12, 235, 236 PbWO4, 378–381

RAl3(BO3)4(R=Y, Gd, Lu ), 316 ScF3, 235, 236 Sc2O3, 236 Sr3Ga2Ge4O14, 236 SrMoO4, 378 SrWO4, 378 YAl3(BO3)4 (YAB), 91, 254 Y3Al5O12 (YAG), 20, 42, 158, 196 Y3Ga5O12 (YGG), 142, 196 Y3Sc2Ga3O12 (YSGG), 223 Y2SiO5, 215–218 YVO4, 98, 117–119, 314, 317, 334, 378, 381, 382 ZnWO4, 223, 236 A Absorption band, 209, 222, 309, 313, 314, 322 Absorption coefﬁcient, 103, 125, 128, 129, 132–134, 136, 315, 328, 333 Absorption cross section, 103, 129, 136, 151, 292, 315, 316, 318, 362, 363 Active ion, 1, 48, 52, 54, 69–73, 90, 91, 103, 114–118, 161, 191, 192, 199, 200, 205, 207, 213, 215, 222, 225, 233, 237, 241, 257, 258, 265–267, 278, 303, 309, 312–314, 324, 335, 341, 346, 353–355, 357, 359, 360, 363, 374, 385, 391, 393, 394 Angular momentum quantum number, 5, 6, 9, 15, 17, 54, 64, 89, 91, 115, 208 Apparent crystal ﬁeld, 393, 394, 397–399, 405–407, 409, 411, 412

© Science Press and Springer Nature Singapore Pte Ltd. 2020 Z. Luo and Y. Huang, Physics of Solid-State Laser Materials, Springer Series in Materials Science 289, https://doi.org/10.1007/978-981-32-9668-8

467

468 B Boltzmann distribution, 138, 145, 153, 155, 258 Bond angle, 386 C Character of Irreducible representation, 37, 115 Character table, 39, 40, 49, 50, 84, 121, 122, 216 Charge transfer, 257, 266, 378 Clebsch-Gordan coefﬁcient (C-G coefﬁcient), 41, 63, 230, 231 Cohesive energy, 396 Concentration quenching, 298–300, 303–306, 315, 324, 346, 357 Condon approximation, 171, 180, 242, 243, 246 Conﬁguration coordinate, 204, 233, 258, 259 Continuous group, 9, 12, 15, 46, 47 Coordination number, 158, 282, 387, 388, 390, 411 Crystal ﬁeld, 12, 13, 15, 19, 54, 57, 66, 69–73, 75–81, 88–93, 95, 98–100, 114, 116–118, 121, 122, 136–140, 144, 145, 147, 152, 153, 157, 158, 181–183, 187, 191, 192, 196, 199–201, 270, 315, 319 parameter, 66, 70, 72, 73, 77–80, 91, 93, 94, 98–100, 181, 215, 227, 232, 233, 266, 304, 394, 395, 397, 398, 405, 406 quantum number, 81–90, 119 splitting, 70, 72, 199, 207, 304, 315, 392, 394, 399, 405–408, 410, 412 strength, 117, 140, 209, 214, 220–223, 226, 232, 305, 389, 395, 396, 398, 409, 411

Index Electric quadrupole transition, 112, 113, 115, 116, 122, 156, 282 Electron phonon interaction, 181, 209, 234, 246, 250, 257, 265, 269 Emission cross section, 129, 136, 151–153, 155, 219, 222, 223, 268, 312, 317, 319, 321, 357, 360, 362, 364, 370 Energy migration, 277, 278, 288–290, 292–294, 296, 297, 301, 304 Excited state absorption, 210, 226, 341 F Fluorescence branching ratio, 142, 155 concentration quenching, 299, 300, 303–306 lifetime, 155, 222–227, 256, 291, 296–303, 305, 312, 313, 316, 317, 319, 321–323, 330, 356, 364 quantum efﬁciency, 155, 312, 313, 319, 323, 324 quenching, 299, 303, 305, 357, 387, 391 Fluoride glass, 254, 388, 391, 392, 411 Four-level system, 222, 241, 309, 310, 312–315, 322, 359, 367 G Gaussian line shape, 191 Germanate glass, 254, 406–408 Glass former, 386, 387, 391 Glass modiﬁer, 386, 387, 391 Ground state absorption, 145, 315 Group chain, 12, 16, 90–92, 98, 386, 393, 394, 406, 407, 409, 411

D Debye distribution, 182 Debye temperature, 170, 186, 197, 199, 210, 333, 334 Degenerate, 8, 92, 122, 127, 137, 208, 219 Dipole-dipole interaction, 289, 290, 293, 294 Dipole moment, 111, 113, 115–119, 136, 165, 171, 216, 229, 230, 255, 320, 375 Disorder, 235, 236, 385, 387, 389, 398

H Hardness, 170, 267, 337, 341, 396 Harmonic oscillator, 164, 167, 168, 172, 174, 177 Homogeneous broadening, 399 Hopping mode, 292, 294 Huang–Rhys factor, 176, 180, 225, 226, 232, 234–237, 247, 250, 252, 258, 260, 264, 272, 273 Hypersensitive transition, 156–158

E Einstein coefﬁcient, 146, 360 Electric dipole-dipole interaction, 279, 281, 282, 290 Electric dipole transition, 69, 130–132, 136–139, 147, 149, 150, 156, 161, 171, 216, 228, 229, 237, 256, 266

I I-H model, 289 Inhomogeneity, 336, 353, 390 Inhomogeneous broadening, 191, 385, 399 Intermediate coupling, 9, 16, 17, 25, 72, 73, 116, 405 Invariant of quadratic rotation, 397

Index Ionic radius, 320, 388 Irreducible representation, 12, 27, 37–41, 46, 47, 49–52, 54–57, 61, 63, 64, 70, 72, 81–92, 95, 96, 99, 116–119, 121, 122, 144, 205, 207, 208, 210–214, 216, 219, 220, 378, 393 Irreducible representation tensor, 61, 62, 64 J Jahn-Teller effect, 208, 209 J-O parameter, 111 L Lanthanide contraction, 20, 190, 388 Laser gain coefﬁcient, 356–358 Laser glass, 385 Laser threshold, 222, 313, 317, 319, 322, 330, 360 Lattice vibration, 42, 70, 103, 114, 157, 161, 162, 164, 165, 169–172, 181, 182, 192, 195, 203, 208–210, 222, 225, 233, 237, 241, 243, 247, 267, 277, 319, 333–335, 337, 375, 376 Ligand ion, 233, 234, 256, 388, 389, 393 Line broadening, 179, 181, 182, 190, 191, 196, 197, 199, 200, 319, 320, 377 Line shape function, 170, 171, 176–179, 191, 233, 319 Line shift, 161, 181, 195, 197–199 Linewidth, 161, 181–183, 187, 189, 192, 197, 200, 201, 217, 222, 224, 233, 235, 236, 268, 270, 271, 318, 319, 321, 322, 330, 338, 341, 361, 377, 378, 382 Local environment, 388–390, 392 region, 386 structure, 233, 388, 389, 391, 392 symmetry, 31, 355, 392 Lorentzian line shape, 197 Lower laser level, 241, 269, 309, 311–313, 315, 322, 323, 360 L-S coupling, 10, 11, 16, 121 M Magnetic dipole-dipole interaction, 279, 282 Magnetic dipole transition, 112, 113, 116, 120–122, 131, 139, 140, 146, 147, 149, 150 Mass difference factor, 188, 196, 320, 321 Melting point, 267, 337, 396 Mode density, 274, 312, 317 Multi-phonon transition, 179 Multiplet, 88, 89, 91, 92, 96, 98, 121, 122, 138, 140, 141, 144, 147, 151–155, 181, 187,

469 196, 197, 199–201, 268, 270, 299, 304, 315, 316, 385, 392, 395–399, 407, 410 N Nearest ligand, 386 Network former, 386 Network modiﬁer, 386, 411 Non-crystal, 391–393, 395–398, 406, 411 Nonlinear crystal, 345 Nonlinear optical coefﬁcient, 345, 346, 350, 355, 359, 363, 365, 376, 379 Nonlinear polarization, 338, 347, 349 Nonradiative transition, 161, 222, 241–243, 246–250, 252–254, 256–260, 263–271, 287, 309, 313, 362 O Oscillator strength, 103, 125, 130–132, 147, 149, 150, 158, 280–282 Oxide glass, 386, 388–391, 406, 407, 409, 411 P Parity, 5, 8, 72, 81, 91, 93, 114–117, 136, 137, 139, 140, 147, 157, 205, 229, 230 Phase-matching angle, 352, 354 Phonon, 114, 152, 161, 168–172, 174–192, 194–201, 210, 221–223, 225, 226, 232, 234–237, 241, 242, 247–251, 257–261, 265, 267–274, 277, 283–287, 296, 305, 306, 315, 316, 319, 320, 333–335, 340, 375–377, 392 Phonon-assisted energy transfer, 161, 278, 282, 283, 285, 286, 305, 306 Photon lifetime, 311, 364 Point group, 9, 41–43, 48–50, 52, 63, 64, 70, 72, 75, 77–79, 81, 82, 84–86, 88–94, 96, 98, 100, 114, 115, 118, 119, 121, 122, 144, 145, 147, 157, 158, 207, 213, 226, 230, 392–394, 411 Polarization, 69, 88, 90, 103–105, 109–111, 118, 119, 121, 122, 126, 134–137, 139, 141, 142, 145, 149, 150, 152, 157, 216, 223, 229, 305, 333, 337, 338, 346, 347, 349, 351, 375, 381, 392 Population inversion, 269, 309, 315, 356, 359, 360 Q Quality factor, 311, 314, 316–318, 330 Quantum efﬁciency, 136, 313, 341 Quasi-three-level system, 155 Quenching rate, 305 Quenching ratio, 305, 306

470 R Radiation trapping effect, 278, 298–300 Radiative lifetime, 135, 136, 141, 152, 155, 223, 296, 299, 305, 312 Radiative transition, 103, 222, 309, 313, 323, 392 Radius ratio, 388, 389 Raman gain coefﬁcient, 377, 378, 380, 381 Raman scattering, 181, 182, 187–189, 191, 197, 338, 339, 345, 347, 375–379 Random network, 386–390 Rate equation, 287, 288, 295–297, 356, 359, 360, 366, 367, 370 Resonant energy transfer, 278, 303–305 S Scalar crystal ﬁeld parameter, 304 Scalar crystal ﬁeld strength, 395, 397, 405, 407, 409 Second Harmonic Generation (SHG), 349, 351, 353, 365 Selection rule, 103, 113, 115–122, 139, 141, 147, 156, 216, 392 Self-activated, 303–305, 396 Self Frequency Doubling (SFD), 337, 345, 346, 353, 354, 356, 359–365, 368, 374 Self frequency mixing, 337 Self Raman scattering, 347 Short-range order, 386 Silicate glass, 390, 392, 401 Slope efﬁciency, 323, 381, 382 Space group, 41–43, 306, 355, 379 Spectral brand, 180, 398, 399 line, 114, 118, 119, 161, 171, 178, 179, 181–183, 187, 191–193, 195–201, 235, 237, 268, 319, 323, 330, 377–379, 385, 387, 388, 398, 399, 405 term, 9–13, 15–17, 20, 29, 47, 54, 55, 195, 214, 219–221, 227, 304 Spin-orbital interaction, 5–7, 9, 10, 12, 13, 16, 20, 26, 27 Spin-orbit coupling constant, 9 Splitting, 6, 9, 11, 13, 48, 55, 57, 70, 72, 77–79, 203, 205, 208, 392, 393, 395–398, 407, 412 Spontaneous emission, 103, 108, 109, 111, 112, 125–127, 135, 146, 147, 187, 197, 198, 273, 288, 319, 323, 324, 360 Stimulated emission, 108, 113, 125–127, 145, 146, 223, 268, 272, 319, 324 Stimulated non-radiative, 268, 269

Index Stimulated radiative transition, 103, 268, 309 Strain, 183, 184, 191, 251, 265, 283, 284, 320, 321, 329, 330 Strong coupling, 220, 257, 258, 262–265 Symmetry operation, 34, 36, 42, 48, 56, 75, 76, 87, 211 T Thermal birefringence, 322, 328, 333, 382 broadening, 181, 182, 195–201, 323 conductivity, 316, 325, 327, 328, 333–337, 341, 377, 382 diffusion coefﬁcient, 325, 337, 341 equilibrium, 168, 170, 186, 189, 194, 286 expansion coefﬁcient, 192, 332, 334, 336, 337, 341, 382 loading, 323, 324, 328, 341 lens effect, 322, 323, 328, 331, 333, 340, 381 linewidth, 320 shift, 181, 182, 192–195, 199 stress, 322, 328–330, 333 Three-level system, 155, 222, 309, 310, 312–315 Threshold, 223, 312–317, 319, 323, 338–341, 358, 359, 362, 380 Transition probability, 63, 107, 109–111, 114, 121, 125, 127, 138, 139, 141, 147, 153, 155, 156, 170, 177, 185, 186, 188, 203, 225, 229, 241, 243, 248–252, 254, 291, 301, 324 U Up-conversion, 145, 315, 316, 324 Upper laser level, 223, 227, 241, 274, 309, 312–314, 316, 322, 323, 360–362, 370, 374 W Weak coupling, 6, 222, 248, 249, 251, 257 Wigner-Eckart theorem (W-E theorem), 62, 63 Y Yokota–Tanimoto model (Y–H model), 294, 374 Z ZBLAN glass, 388, 391, 399, 400, 407, 409, 410